Introduction to Computational Plasticity
This page intentionally left blank
Introduction to Computational Plasticit...

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

Introduction to Computational Plasticity

This page intentionally left blank

Introduction to Computational Plasticity FIONN DUNNE AND NIK PETRINIC Department of Engineering Science Oxford University, UK

1

3

Great Clarendon Street, Oxford ox2 6dp Oxford University Press is a department of the University of Oxford. It furthers the University’s objective of excellence in research, scholarship, and education by publishing worldwide in Oxford New York Auckland Cape Town Dar es Salaam Hong Kong Karachi Kuala Lumpur Madrid Melbourne Mexico City Nairobi New Delhi Shanghai Taipei Toronto With ofﬁces in Argentina Austria Brazil Chile Czech Republic France Greece Guatemala Hungary Italy Japan Poland Portugal Singapore South Korea Switzerland Thailand Turkey Ukraine Vietnam Oxford is a registered trade mark of Oxford University Press in the UK and in certain other countries Published in the United States by Oxford University Press Inc., New York © Oxford University Press, 2005 The moral rights of the authors have been asserted Database right Oxford University Press (maker) First published 2005 Reprinted 2006 (with corrections) All rights reserved. No part of this publication may be reproduced, stored in a retrieval system, or transmitted, in any form or by any means, without the prior permission in writing of Oxford University Press, or as expressly permitted by law, or under terms agreed with the appropriate reprographics rights organization. Enquiries concerning reproduction outside the scope of the above should be sent to the Rights Department, Oxford University Press, at the address above You must not circulate this book in any other binding or cover and you must impose the same condition on any acquirer British Library Cataloguing in Publication Data (Data available) Library of Congress Cataloging in Publication Data (Data available) Typeset by Newgen Imaging Systems (P) Ltd., Chennai, India Printed in Great Britain on acid-free paper by Biddles Ltd, King’s Lynn ISBN 0-19-856826-6 (Hbk)

978-0-19-856826-1

3 5 7 9 10 8 6 4 2

To Hannah and Roberta, with love

This page intentionally left blank

Preface

The intention of this book is to bridge the gap between undergraduate texts in engineering plasticity and the many excellent books in computational plasticity aimed at more senior graduate students, researchers, and practising engineers working in solid mechanics. The book is in two parts. The ﬁrst introduces microplasticity and covers continuum plasticity, the kinematics of large deformations and continuum mechanics, the ﬁnite element method, implicit and explicit integration of plasticity constitutive equations, and the implementation of the constitutive equations, and the associated material Jacobian, into ﬁnite element software. In particular, the implementation into the commercial code ABAQUS is addressed (and to help, we provide a range of ABAQUS material model UMATs), together, importantly, with the tests necessary to verify the implementation. Our intention, wherever possible, is to develop a good physical feel for the plasticity models and equations described by considering, at every stage, the simpliﬁcation of the equations to uniaxial conditions. In addition, we hope to provide a reasonably physical understanding of some of the large deformation quantities (such as the continuum spin) and concepts (such as objectivity) which are often unfamiliar to many undergraduate engineering students who demand more than just a mathematical description. The second part of the book introduces a range of plasticity models including those for superplasticity, porous plasticity, creep, cyclic plasticity, and thermo-mechanical fatigue (TMF). We also describe a number of practical applications of the plasticity models introduced to demonstrate the reasonable maturity of continuum plasticity in engineering practice. We hope, above all, that this book will help all those—undergraduates, graduates, researchers, and practising engineers—who need to move on from knowledge of undergraduate plasticity to modern practice in computational plasticity. Our aims have been to encourage development of understanding, and ease of passage to the more advanced texts on computational plasticity. September 2004

F. P. E. D. and N. P.

This page intentionally left blank

Contents Acknowledgements

xii

Notation

xiii

Part I. Microplasticity and continuum plasticity 1. 1.1 1.2 1.3 1.4

2. 2.1 2.2 2.3 2.4 2.5 2.6 2.7

3. 3.1 3.2 3.3 3.4 3.5

Microplasticity Introduction Crystal slip Critical resolved shear stress Dislocations Further reading Continuum plasticity Introduction Some preliminaries Yield criterion Isotropic hardening Kinematic hardening Combined isotropic and kinematic hardening Viscoplasticity and creep Further reading Kinematics of large deformations and continuum mechanics Introduction The deformation gradient Measures of strain Interpretation of strain measures Polar decomposition

3 3 5 7 8 10 11 11 11 17 23 27 36 38 45 47 47 48 49 52 57

x

Contents

3.6 3.7 3.8 3.9

Velocity gradient, rate of deformation, and continuum spin Elastic–plastic coupling Objective stress rates Summary Further reading

60 66 69 81 82

4.

The ﬁnite element method for static and dynamic plasticity

83

Introduction Hamilton’s principle Introduction to the ﬁnite element method Finite element equilibrium equations Integration of momentum balance and equilibrium equations Further reading

83 84 96 100 136 142

4.1 4.2 4.3 4.4 4.5

5. 5.1 5.2 5.3 5.4 5.5 5.6

6. 6.1 6.2 6.3 6.4 6.5 6.6

Implicit and explicit integration of von Mises plasticity Introduction Implicit and explicit integration of constitutive equations Material Jacobian Kinematic hardening Implicit integration in viscoplasticity Incrementally objective integration for large deformations Further reading Implementation of plasticity models into ﬁnite element code Introduction Elasticity implementation Veriﬁcation of implementations Isotropic hardening plasticity implementation Large deformation implementations Elasto-viscoplasticity implementation

143 143 143 150 154 161 167 168 169 169 170 171 172 176 180

Part II. Plasticity models 7. 7.1 7.2

Superplasticity Introduction Some properties of superplastic alloys

185 185 185

Contents

7.3 7.4

8.

Constitutive equations for superplasticity Multiaxial constitutive equations and applications References Porous plasticity

8.1 8.2

Introduction Finite element implementation of the porous material constitutive equations Application to consolidation of Ti–MMCs References

8.3

9.

Creep in an aero-engine combustor material

9.1 9.2 9.3

Introduction Physically based constitutive equations Multiaxial implementation into ABAQUS References Appendix 9.1

xi

189 192 197 199 199 201 205 207 209 209 209 212 217 218

10. Cyclic plasticity, creep, and TMF

219

10.1 Introduction 10.2 Constitutive equations for cyclic plasticity 10.3 Constitutive equations for C263 undergoing TMF References

219 219 222 227

Appendix A: Elements of tensor algebra

229

Differentiation The chain rule Rotation

231 232 233

Appendix B: Fortran coding available via the OUP website

235

Index

239

Acknowledgements

The authors would like to express their sincere gratitude to Esteban Busso for reading a draft and providing many helpful comments and suggestions, to Paul Buckley for the provision of the ﬁgures in Chapter 1, and to Jinguo Lin for permission to use Figures 7.9–7.14. The authors acknowledge, with gratitude, permission granted to reproduce the following ﬁgures: Figures 7.9–7.14: Elsevier Ltd, Oxford, UK. Figures 8.1–8.6: Institute of Materials Communications Ltd, London, UK. Figures 9.1–9.4, 10.1–10.3: Elsevier Ltd, Oxford, UK.

Notation

• Regular italic typeface (v, σ, . . .): scalars, scalar functions. • Bold italic typeface (P , v, A, σ , . . .): points, vectors, tensors, vector and tensor functions. • Helvetica bold italic typeface (C, c, I, . . .): fourth order tensors.

Operations f (·) det[·] Tr[·] ln(·) [·] ∂ [·] ∂x ∇(·) = grad[·] div[·] = tr[∇(·)] x·y x⊗y σ :ε √ |u| = √u · u |A| = A : A

function of (·) determinant of [·] trace of [·] logarithm of (·) increment of [·] partial derivative of [·] with respect to x gradient of [·] divergence of [·] scalar product of vectors dyadic product of vectors double contraction of tensors norm of vector norm of tensor

Some commonly used notation C D E E ε

fourth-order tensor of material constants rate of deformation tensor Lagrangian strain tensor Young’s modulus strain tensor

xiv

F f ρ I J K M ν P P R R σ t t u u˙ u¨ W

Notation

deformation gradient force vector ﬁeld density second-order identity tensor Jacobian stiffness matrix mass matrix Poisson’s ratio material particle material point ∈ Rn rotation tensor real set Cauchy stress tensor time surface traction vector displacement vector ﬁeld velocity vector ﬁeld acceleration vector ﬁeld work

Part I. Microplasticity and continuum plasticity

This page intentionally left blank

1. Microplasticity

1.1

Introduction

This chapter brieﬂy introduces the origins of yield and plastic ﬂow, and in particular, attempts to explain the usual assumptions in simple continuum plasticity of isotropy, incompressibility, and independence of hydrostatic stress. While short, we introduce grains, crystal slip, slip systems, resolved shear stress, and dislocations; the minimum knowledge of microplasticity for users of continuum plasticity. The origin of plasticity in crystalline materials is crystal slip. Metals are usually polycrystalline; that is, made up of many crystals in which atoms are stacked in a regular array. A typical micrograph for a polycrystalline nickel-base superalloy is shown in Fig. 1.1 in which the ‘crystal’ or grain boundaries can be seen. The grain size is about 100 µm. The grain boundaries demarcate regions of different crystallographic orientation. If we represent the crystallographic structure of a tiny region of a single grain by planes of atoms, as shown in Fig. 1.2(a), we can then visualize plastic deformation taking place as shown in Fig. 1.2(a) and (b); this is crystallographic slip. Unlike elastic deformation, involving only the stretching of interatomic bonds, slip requires the breaking and re-forming of interatomic bonds and the motion of one plane of atoms relative to another. After shearing the crystal from conﬁguration 1.2(a) to conﬁguration 1.2(b), the structure is unchanged except at the extremities of the crystal. A number of very important phenomena in macroscopic plasticity become apparent from just two Figs 1.1 and 1.2: (1) plastic slip does not lead to volume change; this is the incompressibility condition of plasticity; (2) plastic slip is a shearing process; hydrostatic stress, at the macrolevel, can often be assumed not to inﬂuence slip; (3) in a polycrystal, plastic yielding is often an isotropic process. As we will see later, the incompressibility condition is very important in macroscale plasticity and manifests itself at the heart of constitutive equations for plasticity.

4

Microplasticity

100 mm

Fig. 1.1 Micrograph of polycrystal nickel-base alloy C263. (a)

τ

τ

(b)

τ

τ

Fig. 1.2 Schematic representation of the crystallographic structure within a single grain undergoing slip.

However, not all plastic deformation processes are incompressible. A porous metal, for example, under compressive load may undergo plastic deformation during which the pores reduce in size. Consequently, there is a change of volume and a dependence on hydrostatic stress. However, the volume change does not originate from the plastic slip process itself, but from the pore closure. The fact that plastic slip is a shearing process gives more information about the nature of yielding; in principle, it tells us that plastic deformation is independent of hydrostatic stress (pressure). For non-porous metals, this is one of the cornerstones of yield criteria. The von Mises criterion, for example, is one in which the initiation of macroscale yield is quite independent of hydrostatic stress. If we take a sample of the theoretical material shown schematically in Fig. 1.2(a) and submerge it to an ever deeper depth in an imaginary sea of water, the hydrostatic stress becomes ever larger but causes no more than the atoms in the theoretical material to come closer together. It will never in itself be able to generate the shearing necessary for crystallographic slip. Figure 1.1 shows a micrograph of a polycrystal. If we assume that there is no preferred crystallographic orientation, but that the orientation changes randomly from one

Crystal slip

(a)

5

(b)

Fig. 1.3 (a) Photograph of a single zinc crystal and (b) a schematic diagram representing single slip in a single crystal.

grain to the next, and if our sample of material contains a sufﬁciently large number of grains, we can get a reasonable physical feel that macroscale yielding of the material will be isotropic. This is a further cornerstone of the von Mises yield criterion.

1.2

Crystal slip

The evidence for crystal slip being the origin of plasticity comes from mechanical tests carried out on single crystals of metals. The single crystal of zinc shown in Fig. 1.3(a) is a few millimetres in width and has been loaded beyond yield in tension. The planes that can be seen are those on which slip has occurred resulting from many hundreds of dislocations running through the crystal and emerging at the edge. Each dislocation contributes just one Burger’s vector of relative displacement, but with many such dislocations, the displacements become large. Figure 1.3(b) shows schematically what is happening in Fig. 1.3(a). The ends of the test sample have not been constrained in the lateral directions. It can be seen that single slip in this case leads to the horizontal displacement of one end relative to the other. Had this test been carried out in a conventional uniaxial testing machine, the lateral motion would have been prevented. In order to retain compatibility, then, with the imposed axial displacement, the slip planes would have to rotate towards the loading direction. The uniaxial loading therefore leads not only to crystallographic slip, but also to rotation of the crystallographic lattice.

1.2.1

Slip systems: slip directions and slip normals

Observations on single crystals show that slip tends to occur preferentially on certain crystal planes and in certain speciﬁc crystal directions. The combination of a slip

6

Microplasticity

(111)

–

[110]

¯ in an fcc lattice. Fig. 1.4 The particular slip system (111)[110] (112)

(101)

(123)

–

(111)

Fig. 1.5 Slip systems in bcc materials.

plane and a slip direction is called a slip system. These tend to be the most densely packed planes and the directions in which the atoms are packed closest together. This is explained in terms of dislocations. In face centred cubic (fcc) materials, the most densely packed planes are the diagonal planes of the unit cell. In fact the crystal is ‘close-packed’ in these planes; the observed slip systems are shown in Fig. 1.4. ¯ The full family of slip systems in such crystals may be written as 110{111}. There are 12 such systems in an fcc crystal (four planes each with three directions). In body centre cubic (bcc) crystals, there are several planes that are of similar density of packing, and hence there are several families of planes on which slip occurs. However, there is no ambiguity about the slip direction, since the atoms are closest ¯ direction and those equivalent to it. The slip systems observed in bcc along the [111] crystals are shown in Fig. 1.5. Thus, there are three families of slip systems operative: ¯ 111{101};

¯ 111{112};

¯ 111{123}.

Table 1.1 shows the slip systems found in single crystals of some of the important fcc and bcc pure metals together with the resolved shear stress required to cause slip—the critical resolved shear stress (CRSS).

Critical resolved shear stress

7

Table 1.1 Slip systems and CRSS for some pure metals. Metal

Structure

Slip systems

CRSS (MPa)

Cu Al Ni

fcc fcc fcc

¯ 110{111} ¯ 110{111} ¯ 110{111}

0.64 0.40 5.8

α-Fe Mo Ta

bcc bcc bcc

¯ ¯ ¯ 111{101}, 111{112}, 111{123} ¯ 111{101} ¯ ¯ ¯ 111{101}, 111{112}, 111{123}

32 50 50

t Slip plane normal

n s f

l

s Slip direction

Fig. 1.6 A single crystal containing slip plane with normal n, slip direction s, and loaded in direction t.

1.3

Critical resolved shear stress

Suppose a single crystal in the shape of a rod is tested in tension. The axis of the rod is parallel to unit vector t. The crystal has an active slip plane, normal in direction of unit vector n. It has an active slip direction parallel to unit vector s, as shown in Fig. 1.6. When the applied tensile stress is σ , the shear stress acting on the slip plane and in the slip direction is τ which may be found as follows: if the cross-sectional area of the rod is A, the force in the slip direction is Aσ cos λ and it acts on an area A/cos φ of the slip plane. Hence the resolved shear stress is τ = σ cos φ cos λ = σ (t · n)(t · s).

(1.1)

Slip will take place on the slip system, that is, the crystal will yield, when τ reaches the CRSS. This is known as Schmid’s law. The data shown in Fig. 1.7 were obtained from tensile tests on cadmium single crystals which are hexagonal close packed (hcp). The measured yield stress depends upon the angle between the tensile loading direction and the basal plane. The minimum stress to cause yield occurs when the tensile axis is 45◦ to this plane, that is, when the shear stress is maximized. Schmid’s law provides a good explanation for the observed behaviour.

8

Microplasticity 7 Data Schmid’s law

Yield stress (MPa)

6 5 4 3 2 1 0 0

30 60 90 Angle between tensile axis and basal plane

Fig. 1.7 The dependence of yield stress on the angle between the tensile axis and basal plane in an hcp cadmium single crystal.

b

Fig. 1.8 An edge dislocation.

1.4

Dislocations

The theoretical shear strength of a crystal, calculated assuming that the shear is homogeneous (the entire crystal shears simultaneously on one plane), is given by G . τth = 2π The expected shear strength is therefore very large; many orders of magnitude greater than the CRSS values are shown in Table 1.1. The assumption of homogeneous shear is, of course, wrong and plastic deformation in crystals normally occurs by the movement of the line defects known as dislocations, that are usually present in large numbers. The glide of a dislocation involves only very local rearrangements of atoms close to it, and requires a stress much lower than τth , thereby explaining the low observed values of CRSS. Each dislocation is associated with a unit of slip displacement given by the Burgers vector b. Since the dislocation is a line defect, there are two extreme cases. Figure 1.8 shows a schematic representation of an edge dislocation. In this case the Burgers vector b is perpendicular to the line of the dislocation, and the dislocation corresponds to the edge of a missing half-plane of atoms. Thus b and

Dislocations

9

b

Fig. 1.9 A screw dislocation.

the dislocation line deﬁne a plane: a speciﬁc slip plane. If l is a unit vector parallel to the dislocation line, then s=

b |b|

and

n=

b×l . |b|

(1.2)

Figure 1.9 shows a schematic representation of a screw dislocation. This is the other extreme case where the Burger’s vector is parallel to the dislocation line. The dislocation itself corresponds to a line of scissors-like shearing of the crystal. It follows from the fact that b is parallel to l, that, although the slip direction s is deﬁned, the slip plane n is not. Hence, a screw dislocation can cause slip on any slip plane containing l. Dislocations are therefore vital in understanding yield and plastic ﬂow. We have said nothing about the important role of dislocations in strain hardening and softening. Nor have we discussed the effect of temperature on diffusivity which inﬂuences or controls many plastic deformation mechanisms including thermally activated dislocation climb leading to recovery, vacancy core and boundary diffusion, and grain boundary sliding. All of these subjects can be found in existing materials text books, some of which are listed below. Our aim has been to include sufﬁcient material on microplasticity to ensure that the physical bases of at least some of the assumptions made in macrolevel continuum plasticity are understood. There have been many developments over the last 25 years in physically based microplasticity modelling, including the development of time-independent and ratedependent crystal plasticity. Here, for a given crystallographic lattice (e.g. fcc), using ﬁnite element techniques, the resolved shear stresses on all slip systems can be determined to ﬁnd the active slip systems. Within either a time-independent or rate-dependent formulation, the slip on each active system can be determined from which the overall total deformation can be found. Such models are being used successfully for the plastic and creep deformation of single crystal materials which ﬁnd application in aero-engines. The modelling of single crystal components has become

10

Microplasticity

possible with the development of high-performance computing. More recently, using ﬁnite element techniques, polycrystal plasticity models have been developed. Here, the understanding of microplasticity discussed above is also employed and again, as in single crystal plasticity, the active slip systems can be identiﬁed and the corresponding slips determined to give the overall deformation within a given grain. This is now done for all the grains in the polycrystal, which all have their own measured or speciﬁed crystallographic orientations, subject to the requirements of equilibrium and compatibility which are imposed within the ﬁnite element method. In order to do this, it is necessary to generate many ﬁnite elements within each grain. It is clear that for large numbers of grains, such polycrystal plasticity modelling becomes untenable. The consequence is that while desirable, it is not (for the foreseeable future) going to be feasible to carry out polycrystal plasticity modelling at the engineering component level. Currently, and for many years to come, the plastic deformation occurring in both the processing to produce engineering components, and occurring under in-service conditions at localized regions of a component, will continue to be modelled using continuum-level plasticity. This is particularly so in engineering industry where pressures of time and cost demand rapid analyses. We will now, therefore, leave microplasticity and address, in the remainder of the book, continuum-level plasticity.

Further reading Dieter, G.E. (1988). Mechanical Metallurgy. McGraw-Hill Book Co., London. Meyers, M.A., Armstrong, R.W., and Kirchner, H.O.K. (1999). Mechanics and Materials. Fundamentals and Linkages. John Wiley & Sons Inc., New York.

2. Continuum plasticity

2.1

Introduction

This chapter introduces the fundamentals of time-independent and rate-dependent continuum, or phenomenological plasticity: multiaxial yield, normality hypothesis, consistency condition, isotropic and kinematic hardening, and simple constitutive equations for viscoplasticity and creep. We assume throughout the chapter that we are dealing with small strain problems in the absence of large rigid body rotations. The kinematics of large deformations are left until the following chapter.

2.2 2.2.1

Some preliminaries Strain decomposition

Figure 2.1 shows the idealized stress–strain behaviour which might be obtained from a purely uniaxial tensile test. Plasticity commences at a uniaxial stress of σy , after which the material strain hardens. It is called hardening because the stress is increasing relative to perfect plastic behaviour, also shown in the ﬁgure. If, at a strain of ε, the loading were to be reversed, the material would cease to deform plastically (at least in the absence of time-dependent effects) and would show a linearly decreasing stress with strain such that the gradient of this part of the stress–strain curve would Linear strain hardening

s

sy s

E E

«p

Perfect plasticity

«e

«

Fig. 2.1 The classical decomposition of strain into elastic and plastic parts.

12

Continuum plasticity

again be the Young’s modulus, E, shown in Fig. 2.1. Once a stress of zero is achieved (provided the material remains elastic on full reversal of the load), the strain remaining in the test specimen is the plastic strain, εp . The recovered strain, εe , is the elastic strain and it can be seen that the total strain, ε, is the sum of the two ε = εe + εp .

(2.1)

This is called the classical additive decomposition of strain. It is also apparent from Fig. 2.1 that the stress achieved at a strain of ε is given by σ = Eε e = E(ε − εp ).

(2.2)

In many practical situations, particularly in materials processing operations such as forging or superplastic forming, for example, the strains achieved can be very large indeed, and of order 1–4. Compare the magnitude of this strain with that of typical elastic strains of order 0.001 (the 0.1% proof strain) which are generated in metals, even in forming processes (you can estimate this from the measured forces to give a stress, and the elastic strains are of order σ/E). In such circumstances, it is entirely reasonable to make the assumption that ε e ≈ 0 so that εp ≈ ε. 2.2.2

Incompressibility condition

We saw in Chapter 1 that plastic deformation satisﬁes the incompressibility condition; that is, the deformation takes place without volume change. The consequence of this is that the sum of the plastic strain rate components is zero: p

p

p

ε˙ X + ε˙ Y + ε˙ Z = 0.

(2.3)

This is easily veriﬁed by considering a cube of material, with dimensions shown in Fig. 2.2, which undergoes purely plastic, uniform deformation (or simply argue that the strains are very large so that the elastic components are negligibly small). Constancy of volume requires xyz = x0 y0 z0 . Differentiating both sides with respect to time, and dividing by xyz gives y˙ z˙ x˙ + + = 0. (2.4) x y z The strains are deﬁned by x εX = ln x0 and similarly for εY and εZ , and the strain rate in the Y -direction is therefore 1 ˙ ε˙ Y = y. y Equation (2.4) is therefore the incompressibility condition given in Equation (2.3).

Some preliminaries

y

13

y0 z0

Y Z

z

x x0 X

Fig. 2.2 An element of material undergoing plastic, incompressible, elongation in the Y -direction.

2.2.3

Effective stress and plastic strain rate

Identifying the yield condition for uniaxial, monotonically increasing load is straightforward: If σ < σy then the material is elastic, If σ ≥ σy then the material has yielded. It is not quite so straightforward for a multiaxial stress state; that is, one in which more than one direct stress exists. A whole range of multiaxial yield criteria exist. The most commonly used in engineering practice, particularly for computational analysis, is that of von Mises (to which we will return later), which relies on the knowledge of an effective stress, sometimes called (von Mises) equivalent stress. In terms of principal stresses, the effective stress is deﬁned as 1 σe = √ [(σ1 − σ2 )2 + (σ2 − σ3 )2 + (σ3 − σ1 )2 ]1/2 , (2.5) 2 or in terms of direct and shear stresses, 1/2 3 2 2 2 2 2 2 (σ + σ22 + σ33 + 2σ12 + 2σ23 + 2σ31 ) , (2.6) σe = 2 11 where we use the numerical subscripts 1, 2, and 3 in an equivalent way to X, Y , and Z to indicate direction. σe is, of course, a scalar quantity and its origin lies in the postulate that yielding occurs when a critical elastic shear energy is achieved. Mohr’s circle tells us that in a given plane, the maximum shear stress is τ = (σ1 − σ2 )/2 so that with γ = τ/G, the elastic shear energy per unit volume is τ γ /2 = τ 2 /2G = (σ1 − σ2 )2 /8G. The origin of the terms in Equation (2.5) then becomes apparent. An effective plastic strain rate, p, ˙ is deﬁned, similarly, as √ 2 p p p p p p p˙ = (2.7) [(˙ε1 − ε˙ 2 )2 + (˙ε2 − ε˙ 3 )2 + (˙ε3 − ε˙ 1 )2 ]1/2 . 3

14

Continuum plasticity

Writing the stress and plastic strain rate tensors (dropping the plastic strain rate components) as ⎛ ⎞ ⎛ σ11 σ12 σ13 ε˙ 11 ε˙ 12 σ = ⎝σ21 σ22 σ23 ⎠ and ε˙ = ⎝ε˙ 21 ε˙ 22 ε˙ 31 ε˙ 32 σ31 σ32 σ33 then the effective stress and plastic strain rate may be written as 1/2 3

σe = σ :σ 2 1/2 2 p p 1/2 2 ε˙ : ε˙ ε˙ : ε˙ p˙ = ≈ 3 3

superscript p on the ⎞ ε˙ 13 ε˙ 23 ⎠ ε˙ 33

(2.8)

(2.9)

in which σ is the deviatoric stress given by σ = σ −

1 Tr(σ )I , 3

(2.10)

for example 1

σ11 = σ11 − (σ11 + σ22 + σ33 ) 3 1 2 = σ11 − (σ22 + σ33 ) 3 3 and

= σ12 − 0 ≡ σ12 . σ12

The deviatoric stress can be seen to be the difference between the stress and the mean stress, σm = 13 (σ11 + σ22 + σ33 ); the latter is often called the hydrostatic stress. The symbol ‘:’ in Equations (2.9) is called the double contracted product, or double dot product, of two second-order tensors, which will be deﬁned a little later in the chapter. The equations in (2.9) for the effective stress and plastic strain rates are a useful and compact way of writing the equations given in (2.5) and (2.7), respectively. The coefﬁcients in Equations (2.5) and (2.7) (and equivalently in Equations (2.9)) are chosen to ensure that under purely uniaxial loading, the effective stress σe is identical to the uniaxial stress and the effective plastic strain rate, p, ˙ is identical to the uniaxial plastic strain rate. Let us look at this in detail for the case in which a test specimen is loaded uniaxially upto large plastic strain (so that ε e ε p , and ε ≈ ε p ) under an applied stress σ11 , shown schematically in Fig. 2.3. We will now use Equation (2.9) to determine the effective stress and plastic strain rate.

Some preliminaries

15

s

1 2 s 3

Fig. 2.3 Uniaxial loading of a schematic test piece.

In these circumstances, σ11 = σ, σ22 = σ33 = 0, and all the shear components are zero. The incompressibility condition leads to the requirement that ε˙ 11 + ε˙ 22 + ε˙ 33 = 0.

(2.11)

Because of symmetry, ε˙ 22 = ε˙ 33 so that incompressibility gives ε˙ 22 = ε˙ 33 = − 21 ε˙ 11 = − 21 ε˙ . The deviatoric stress components can be determined using Equation (2.10) as 1

σ11 = σ11 − (σ11 + σ22 + σ33 ) 3 2 = σ11 3 1

σ22 = σ22 − (σ11 + σ22 + σ33 ) 3 1 = − σ11 . 3 Similarly, 1

σ33 = − σ11 3 and

σ12 = σ23 = σ33 =0

so that the deviatoric stress tensor becomes, for uniaxial loading, ⎞ ⎛2 0 0 3 σ11 σ = ⎝ 0 0 ⎠. − 13 σ11 1 0 0 − 3 σ11

(2.12)

We can now use Equation (2.9) to determine the effective stress for this trivial case, but we ﬁrst need to ﬁnd the contracted tensor product, σ : σ . This is deﬁned, for two

16

Continuum plasticity

second-order tensors, A and B, by A:B=

n n

Aij Bij .

(2.13)

i=1 j =1

That is, multiply component by component and sum the terms to give a scalar quantity. σ : σ is therefore given by 4 2 1 2 1 2 6 2 2 + σ11 + σ11 = σ11 ≡ σ2 σ : σ = σ11 9 9 9 9 3 and so

σe =

3

σ : σ

2

1/2

=

32 2 σ 23

1/2 ≡ σ.

For a uniaxial stress state, therefore, σe ≡ σ . Let us follow the same procedure for the effective plastic strain rate. With the incompressibility condition and symmetry conditions discussed above the plastic strain rate tensor becomes ⎛ ⎞ ⎛ ⎞ ε˙ 11 ε˙ 0 0 0 0 ε˙ = ⎝ 0 − 21 ε˙ 11 0 ⎠ = ⎝0 − 21 ε˙ 0 ⎠ 1 0 0 − 2 ε˙ 11 0 0 − 21 ε˙ so that 1/2 2 2 1 2 1 2 1/2 2 ε˙ : ε˙ ε˙ + ε˙ + ε˙ = p˙ = 3 3 4 4 1/2 23 2 ε˙ = = ε˙ . 32

For uniaxial loading, therefore, p˙ = ε˙ . Note that the plastic strain rates appearing in Equation (2.9) are not given as deviatoric quantities, that is, ε . This is because the plastic strain rate components are, in themselves, deviatoric due to the incom of plastic pressibility condition. For example, consider the deviatoric component ε˙ 11 strain rate. 1

ε˙ 11 = ε˙ 11 − (˙ε11 + ε˙ 22 + ε˙ 33 ). 3 Because of the incompressibility condition, therefore,

ε˙ 11 ≡ ε˙ 11 .

Yield criterion

2.3

17

Yield criterion

Only the von Mises yield criterion is considered here. There are many others including that of Tresca and the Gurson model for porous materials. In Chapter 1, we saw that there were several general requirements for yield in isotropic, non-porous materials. Let f be a yield function such that f = 0 is our yield criterion. Then: 1. Yield is independent of the hydrostatic stress. Since f is independent of σm , it must be expressible in terms of the deviatoric stresses σi (i = 1, . . . , 3) alone. 2. Yield in polycrystalline metals can be taken to be isotropic (provided we are concerned with yield in a volume of material containing many grains) and must therefore be independent of the labelling of the axes. Thus f must be a symmetric function of σi (i = 1, . . . , 3). 3. Yield stresses measured in compression have the same magnitude as yield stresses measured in tension. Thus f must be an even function of σi (i = 1, . . . , 3). The von Mises yield function is deﬁned by f = σe − σy =

3

σ : σ

2

1/2 − σy

(2.14)

and, with reference to Equation (2.5), it can be seen that it satisﬁes the three requirements given above. The yield criterion is given by f < 0: Elastic deformation f = 0: Plastic deformation.

(2.15)

The second stress invariant, J2 , is deﬁned as J2 = ( 21 σ : σ )1/2 and it is for this reason that plastic ﬂow based on the von Mises yield criterion is often referred to as J2 plasticity. Geometrically, Equation (2.14) corresponds to a cylinder in threedimensional principal stress space with axis lying along the line σ1 = σ2 = σ3 . It is apparent from this that hydrostatic stress has no effect on yield according to the von Mises criterion. Even inﬁnite, but equal, principal stresses σ1 , σ2 , and σ3 will never cause yield, since σe remains zero (see Equation (2.5)) and f < 0. Let us consider the yield function in two-dimensional principal stress space by putting σ3 = 0 and so imposing conditions of plane stress. Geometrically, this corresponds to ﬁnding the intersection between the von Mises cylinder and the plane σ3 = 0.

18

Continuum plasticity

d«p2 Load point

d«p

s2 sy

d«p1 Tangent to yield surface

Yield surface ( f = 0)

sy

sy

sy

s1

Elastic region

Fig. 2.4 The von Mises yield surface for conditions of plane stress, showing the increment in plastic strain, dε p , in a direction normal to the tangent to the surface.

From Equations (2.14) and (2.5), 1/2 3 f = σe − σy = σ :σ − σy 2 1 = √ [(σ1 − σ2 )2 + (σ2 − σ3 )2 + (σ3 − σ1 )2 ]1/2 − σy , 2 which for plane stress, at yield, becomes 1 f = √ [(σ1 − σ2 )2 + σ22 + σ12 ]1/2 − σy = 0 2

(2.16)

so σ12 − σ1 σ2 + σ22 = σy2 , which is the equation of an ellipse. The yield criterion is shown, for plane stress, in Fig. 2.4. Naturally, when σ1 = 0, σ2 = σy at yield and similarly for the other points where the ellipse intersects the lines σ1 = 0 and σ2 = 0. 2.3.1

The normality hypothesis of plasticity

We have now looked at the conditions necessary to initiate yielding. The question then is what happens after that if loading continues? After yield comes plastic ﬂow and the normality hypothesis of plasticity enables us to determine the ‘direction’ of ﬂow. For what is termed associated ﬂow, the hypothesis states that the increment in the plastic strain tensor is in a direction (i.e. relative to the principal stress directions) which is normal to the tangent to the yield surface at the load point. This is shown schematically in Fig. 2.4, but may be written in terms of the yield function, f , as dεp = dλ

∂f ∂σ

or

ε˙ p = λ˙

∂f . ∂σ

(2.17)

Yield criterion

19

In these expressions, the direction of the plastic strain increment (or equivalently, plastic strain rate) is given by ∂f /∂σ while the magnitude is determined, for the plastic strain rate, by λ˙ . This is called the plastic multiplier which we shall return to later. In order to look at this in more detail, and to make understanding easier, let us write the plastic strain rate and stress tensors in vector form (using what is known as Voigt notation, which we shall address in greater depth in Chapter 4). We will continue to consider principal components only, for the time being. Then for plane stress, σ σ= 1 . σ2 Note that the vector representation of the stress, σ, is not italicized. This is the convention to be adopted throughout the book for stress and strain: an italicized bold σ and ε indicates a tensor, a non-italicized bold symbol a vector, or Voigt notation. The yield function f , written in terms of principal stresses is, from Equation (2.16) 1 f = √ [(σ1 − σ2 )2 + σ22 + σ12 ]1/2 − σy = 0, 2 and we can then determine the direction of plastic ﬂow from Equation (2.17) as ⎞ ⎛ ∂f

1 2 (σ1 − σ1 σ2 + σ22 )−1/2 (2σ1 − σ2 ) ⎜ ∂σ1 ⎟ ∂f 2 ⎟ , = grad(f ) = ⎜ ⎝ ∂f ⎠ = 1 2 2 −1/2 (2σ − σ ) ∂σ 2 1 2 (σ1 − σ1 σ2 + σ2 ) ∂σ2 − σ 2σ 1 2 which has direction −σ + 2σ . This is normal to the yield surface at all points 1

2

(e.g. choose σ1 = σ2 = α, say, and the direction of the normal is clearly along the line σ1 = σ2 ). Let us now derive the plastic strain increment using the normality hypothesis with the von Mises yield criterion given in Equation (2.14), but using the other expression for effective stress for three-dimensions given in Equation (2.5). We p will look at just one component, namely dε1 , to see the general pattern emerge. From Equation (2.17), the ﬁrst component of direction of plastic ﬂow is given by ∂f 1 1 = √ [(σ1 − σ2 )2 + (σ2 − σ3 )2 + (σ3 − σ1 )2 ]−1/2 [2(σ1 − σ2 ) − 2(σ3 − σ1 )] ∂σ1 2 2 (3/2)[σ1 − (1/3)(σ1 + σ2 + σ3 )] = σe so ∂f 3 σ1

= ∂σ1 2 σe

20

Continuum plasticity

remembering the deﬁnition of deviatoric stress given in Equation (2.10). Similar results are obtained for the other components so that Equation (2.17) may be rewritten, for the von Mises yield criterion, as dεp = dλ

3 σ

∂f = dλ ∂σ 2 σe

(2.18)

in which the stress and strain are now written as tensor quantities. Let us now look at the meaning of the plastic multiplier (at least, that is, for a von Mises material). We can use the expression for effective plastic strain rate in Equation (2.9) to write a similar expression for the increment in effective plastic strain as 1/2 2 p p dp = dε : dε . (2.19) 3 If we substitute Equation (2.18) into (2.19) we obtain 2 3 σ 3 σ 1/2 ((3/2)σ : σ )1/2 dp = dλ : dλ = dλ 3 2 σe 2 σe σe so that with Equation (2.9) we obtain

and similarly,

dp = dλ

(2.20)

p˙ = λ˙ .

(2.21)

So, for a von Mises material, the plastic multiplier, dλ, turns out simply to be the increment in effective plastic strain. We can then rewrite the ﬂow rule in Equation (2.18) as σ

3 dε p = dp . (2.22) 2 σe In order for Equation (2.22) to be useful to us, we need to be able to calculate the increment in effective plastic strain, dp, or equivalently, the plastic multiplier, so that with prescribed loading, we can then calculate the increment in plastic strain components. We will address this next. 2.3.2

Consistency condition

Let us consider the case of uniaxial, tensile loading, for which the stress path taken relative to the yield surface is shown in Fig. 2.5. Starting from zero stress, σ2 then increases while the material deforms elastically until the load point (i.e. the point in stress space corresponding to the current loading) meets the yield surface at σ2 = σy . At this point, the material behaves plastically,

Yield criterion

Load point

21

s2 s2 sy

sy

sy

sy

«2

s1

sy Yield surface ( f = 0)

Fig. 2.5 The von Mises yield surface for plane stress and the corresponding stress–strain curve obtained for uniaxial straining in the 2-direction.

with no hardening, as shown in the resulting stress–strain curve in Fig. 2.5. With further plastic deformation, the load point remains on the yield surface and the stress remains constant and equal to σ y . The requirement for the load point to remain on the yield surface during plastic deformation (at least, that is, for time-independent plasticity—we will look at viscoplasticity later) is called the consistency condition, and it is this that enables us to determine the plastic multiplier, or equivalently for a von Mises material, the increment in effective plastic strain. The yield function given in Equation (2.14) includes a dependence on the stress components and the yield stress, σy . We will see later, when considering hardening, that the yield stress can increase (and sometimes decrease), and does so often as a function of effective plastic strain, p. It is therefore convenient to write the yield function as f (σ, p) = σe − σy = σe (σ ) − σy (p) = 0. (2.23) The consistency condition is written, for an incremental change in stress and effective plastic strain f (σ + dσ, p + dp) = 0. (2.24) We can expand this as f (σ + dσ, p + dp) = f (σ, p) +

∂f ∂f : dσ + dp. ∂σ ∂p

(2.25)

Note that all terms in the equation are scalar. Let us work in principal stress space only. The advantage of this is simplicity; the disadvantage is that we ignore the complicating features of dealing with tensor versus engineering strain components. However, this will be dealt with in Chapters 4–6. We will therefore store stress and strain principal components as vectors, in Voigt notation, as discussed above. The product

22

Continuum plasticity

∂f /∂σ : dσ then becomes the scalar (dot) product, (∂f/∂σ)·dσ of two vectors (this is only true in principal stress space, as we shall see later) which gives a scalar. Combining Equations (2.23)–(2.25) gives ∂f ∂f dp = 0. · dσ + ∂p ∂σ

(2.26)

We can use Hooke’s law in incremental form to relate the stress and elastic strains, written as column vectors, by dσ = C dεe = C(dε − dεp )

(2.27)

in which C is the elastic stiffness matrix. We will use the most general form for the plastic strain increment, given in Equation (2.17), for now, but simplify for the case of the von Mises yield criterion later. Substituting (2.17) into (2.27) gives ∂f dσ = C dε − dλ (2.28) ∂σ and (2.28) into (2.26)

∂f ∂f ∂f + dp = 0. · C dε − dλ ∂σ ∂p ∂σ

(2.29)

We can obtain the most general form for dp, that is, without assuming a von Mises material for the time being, by using Equations (2.17) and (2.19) to give 1/2 2 p 2 2 ∂f ∂f ∂f 1/2 ∂f 1/2 p dp = = = dε : dε dλ : dλ dλ · dλ 3 3 ∂σ ∂σ 3 ∂σ ∂σ (2.30) for principal stress space, in which the contracted tensor product simpliﬁes to the scalar product. Substituting (2.30) into (2.29) and rearranging gives the plastic multiplier dλ dλ =

(∂f /∂σ) · C dε (∂f /∂σ) · C(∂f /∂σ) − (∂f /∂p)((2/3)(∂f /∂σ) · (∂f /∂σ))1/2

.

(2.31)

The stress increment can then be determined by substituting (2.31) into (2.28) to give ∂f (∂f /∂σ) · C dε dσ = C dε − ∂σ (∂f/∂σ) · C(∂f/∂σ) − (∂f/∂p)((2/3)(∂f/∂σ) · (∂f/∂σ))1/2 (∂f/∂σ) · C ∂f dε = C−C ∂σ (∂f/∂σ) · C(∂f/∂σ) − (∂f/∂p)((2/3)(∂f/∂σ) · (∂f/∂σ))1/2 (2.32)

Isotropic hardening

23

or dσ = C ep dε.

(2.33)

C ep is called the tangential stiffness matrix. In the absence of plastic deformation, dλ = 0, and in this case, C ep ≡ C, the elastic stiffness matrix. In the case of plastic deformation, with knowledge of the total strain increment, the stress increment can be obtained from Equation (2.32). Before looking at the plastic multiplier in more detail, to gain better physical insight, we will ﬁrst introduce isotropic hardening.

2.4

Isotropic hardening

Many metals, when deformed plastically, harden; that is, the stress required to cause further plastic deformation increases, often as a function of accumulated plastic strain, p, which can be written as p = dp = p˙ dt, (2.34) where p˙ and dp are given in (2.9) and (2.19), respectively. A uniaxial stress–strain curve with non-linear hardening is shown in Fig. 2.6 together with schematic representations of the initial and subsequent yield surfaces. In this instance, the subsequent yield surface is shown expanded compared with the original. When the expansion is uniform in all directions in stress space, the hardening is referred to as isotropic. Let us just consider what happens in going from elastic behaviour to plastic, hardening behaviour in Fig. 2.6. Loading is in the 2-direction, so the load point moves in the σ2 direction from zero until it meets the initial yield surface at σ2 = σy . Yield occurs at this point. In order s2

s2

sy

sy

sy

sy sy

Saturation Hardening «2

s1 sy

Initial yield surface

r

Yield Subsequent, expanded yield surfaces after plastic deformation

Fig. 2.6 Isotropic hardening, in which the yield surface expands with plastic deformation, and the corresponding uniaxial stress–strain curve.

24

Continuum plasticity

for hardening to take place, and for the load point to stay on the yield surface (the consistency condition requires this), the yield surface must expand as σ2 increases, shown in Fig. 2.6. The amount of expansion is often taken to be a function of accumulated plastic strain, p, and for this case, the yield function becomes that given in (2.23), f (σ, p) = σe − σy (p) = 0,

(2.35)

where σy (p) might be of the form σy (p) = σy0 + r(p)

(2.36)

in which σy0 is the initial yield stress and r(p) is called the isotropic hardening function. There are many forms used for r(p) but a common one is r˙ (p) = b(Q − r)p˙

or

dr(p) = b(Q − r) dp

(2.37)

in which b and Q are material constants, which gives an exponential shape to the uniaxial stress–strain curve which saturates with increasing plastic strain, since integrating (2.37) with initial condition r(0) = 0, gives r(p) = Q(1 − e−bp ).

(2.38)

Q is the saturated value of r so that the peak stress achieved with this kind of hardening, from Equation (2.36), is therefore (σy0 +Q). The constant b determines the rate at which saturation is achieved. Figure 2.6 shows an example of the uniaxial stress–strain behaviour predicted using this kind of isotropic hardening function. Let us now consider a slightly simpler form of isotropic hardening and determine the plastic multiplier in Equation (2.31) and hence the stress increments in (2.32). 2.4.1

Linear isotropic hardening

We write the linear isotropic hardening function as dr(p) = h dp

(2.39)

in which h is a constant. With this hardening, we expect the uniaxial stress–strain curve to look like that shown in Fig. 2.7. For uniaxial conditions, dp = dεp , and referring to Figs 2.6 and 2.7, the stress increase due to isotropic hardening is just dr, so using Equation (2.39) we may write dσ h and, of course, the increment in elastic strain is just dεp =

dεe =

dσ E

Isotropic hardening

Gradient = E s

(

1–

E E+h

25

)

r sy «p

sy «

Fig. 2.7 Stress–strain curve for linear strain hardening with dr = h dεp .

so that the total strain is dσ dσ + = dσ dε = E h giving

E+h , Eh

E dσ = E 1 − E+h

dε.

The plastic multiplier has been derived, in Equation (2.31), in terms of the total strain increment. This is the most appropriate form when considering the development of computational techniques, including the ﬁnite element method in which, often, the total strain increments are provided, step by step, and it is then necessary to calculate the corresponding stress increments. However, in order to obtain better physical insight into the process, it is more appropriate (and simpler) to write the plastic multiplier in terms of a known stress increment. In this section, we will obtain the plastic multiplier in terms of the stress increment so that we can then examine the equations for a simple uniaxial problem using the von Mises yield criterion in Section 2.4.2. Now, returning to the plastic multiplier and combining Equations (2.26) and (2.30), we obtain ∂f ∂f ∂f 2 ∂f ∂f ∂f dp = · dσ + dλ · = 0. (2.40) · dσ + ∂p ∂σ ∂p 3 ∂σ ∂σ ∂σ Rearranging (2.40) gives the plastic multiplier, but now in terms of the stress increment, dσ , as −(∂f/∂σ) · dσ . (2.41) dλ = (∂f/∂p)((2/3)(∂f/∂σ) · (∂f/∂σ)) 2.4.2

Uniaxial loading with linear isotropic hardening

Let us consider purely uniaxial loading, in the 1-direction, for a material that yields according to the von Mises criterion. In other words, we will apply a stress σ1 in the

26

Continuum plasticity

1-direction, and all other stresses are zero. For simplicity, we will continue to work in principal stress space and represent the stresses in Voigt notation; that is, the stress is written in vector form as ⎡ ⎤ σ1 σ = ⎣σ2 ⎦ . σ3 We will now determine the plastic multiplier using Equation (2.41). We will consider the denominator ﬁrst. With the hardening function given in (2.39), the yield function becomes f (σ, p) = σe (σ ) − σy (p) = σe (σ ) − σy0 − r(p) = 0 (2.42) from which we can obtain

∂r ∂f =− = −h. (2.43) ∂p ∂p For the von Mises yield criterion, ∂f/∂σ can be obtained using Equation (2.18), with the deviatoric stress components taken from (2.12), as ⎡ 2 ⎤ ⎡ ⎤ σ1 1 ∂f 3 σ

3 1 ⎢ 31 ⎥ ⎢ 1 ⎥ − = = ⎣− 3 σ1 ⎦ = ⎣ 2 ⎦ ∂σ 2 σe 2 σ1 − 21 − 1 σ1 3

so that ∂f ∂p

2 ∂f ∂f · 3 ∂σ ∂σ

⎤ ⎡ ⎤⎞1/2 1 1 ⎜ 2 ⎢− 1 ⎥ ⎢− 1 ⎥⎟ = −h ⎝ ⎣ 2 ⎦ · ⎣ 2 ⎦⎠ = −h. 3 − 21 − 21 ⎛ ⎡

The numerator can be determined as follows: ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ 1 1 dσ1 dσ1 ∂f ⎢− 1 ⎥ ⎣ ⎦ ⎢− 1 ⎥ ⎣ ⎦ = dσ1 · dσ = − ⎣ 2 ⎦ · dσ2 = − ⎣ 2 ⎦ · 0 − ∂σ 1 1 0 dσ 3 −2 −2

(2.44)

(2.45)

and substituting (2.44) and (2.45) into (2.41) gives the plastic multiplier as dλ =

dσ1 . h

(2.46)

For a von Mises material, under uniaxial loading, therefore, p

dλ = dp = dε1 =

dσ1 . h

(2.47)

This is telling us that the increment in stress for unit increase in plastic strain is h. This arises because we chose linear hardening with gradient h. We know, of course,

Kinematic hardening

27

that because we are considering uniaxial loading and the incompressibility condition applies, the other plastic strain increments must be 1 p 1 dσ1 p p dε2 = dε3 = − dε1 = − . (2.48) 2 2 h We can, of course, obtain the other plastic strain components formally from Equation (2.17) as ⎡ ⎤ 1 dσ1 ⎢ 1 ⎥ ∂f p dε = dλ (2.49) = ⎣− 2 ⎦ ∂σ h 1 −2 in agreement with (2.48). The total strain increment in the loading direction is given by dσ1 dσ1 + . (2.50) E h Rearranging (2.50), and omitting the subscript 1 to indicate the uniaxial loading direction, gives E dσ = E 1 − dε, (2.51) E+h which is what we obtained earlier for linear strain hardening shown in Fig. 2.7. Equation (2.51) shows the linear hardening obtained, under uniaxial loading, for the isotropic hardening model chosen in Equation (2.39). If we choose perfect plasticity, that is, with no hardening (h = 0), Equation (2.51) gives a stress increment of zero. The plastic multiplier can, using (2.51) and (2.46), be rewritten as p

dε1 = dε1e + dε1 =

dλ =

2.5

E dε1 . E+h

(2.52)

Kinematic hardening

In the case of monotonically increasing loading, it is often reasonable to assume that any hardening that occurs is isotropic. For the case of reversed loading, however, this is often not appropriate. Consider a material which hardens isotropically, shown schematically in Fig. 2.8. At a strain of εi , corresponding to load point (1) shown in the ﬁgure, the load is reversed so that the material behaves elastically (the stress is now lower than the yield stress) and linear stress–strain behaviour results up until load point (2). At this point, the load point is again on the expanded yield surface, and any further increase in load results in plastic deformation. Figure 2.8(b) shows that isotropic hardening leads to a very large elastic region, on reversed loading, which is often not what would be seen in experiments. In fact, a much smaller elastic region

28

Continuum plasticity (a)

(b) s2

Load point (1)

s2

sy

sy E

sy

sy

«i

s1

«2

E sy

Initial yield surface

Subsequent, expanded yield surface

Load point (2)

Fig. 2.8 Reversed loading with isotropic hardening showing (a) the yield surface and (b) the resulting stress–strain curve. (b)

(a) Load point (1)

s2

s2

sy

sy

E E

|x| sy

sy

s1

«2

sy Initial yield surface

Subsequent, translated yield surface

Load point (2)

Fig. 2.9 Kinematic hardening showing (a) the translation, |x| of the yield surface with plastic strain, and (b) the resulting stress–strain curve with shifted yield stress in compression—the Bauschinger effect.

is expected and this results from what is often called the Bauschinger effect, and kinematic hardening. In kinematic hardening, the yield surface translates in stress space, rather than expanding. This is shown in Fig. 2.9. In Fig. 2.9(a), the stress increases until the yield stress, σy , is achieved. With continued loading, the material deforms plastically and the yield surface translates. When load point (1) is achieved, the load is reversed so that the material deforms elastically until point (2) is achieved when the load point is again in contact with the yield surface. The elastic region is much smaller than that for isotropic hardening shown in Fig. 2.8(b). In fact, for the kinematic hardening in Fig. 2.9, the elastic region

Kinematic hardening

29

is of size 2σy whereas for the isotropic hardening, it is 2(σy + r). In the case of plastic ﬂow with kinematic hardening, note that the consistency condition still holds; the load point must always lie on the yield surface during plastic ﬂow. In addition, normality still holds; the increment in plastic strain has direction normal to the tangent to the yield surface at the load point. The yield function describing the yield surface must now also depend on the location of the surface in stress space. Consider the initial yield surface shown in Fig. 2.9. Under applied loading and plastic deformation, the surface translates to the new location shown such that the initial centre point has been translated by |x|. We now need to determine the stresses relative to the new yield surface centre to check for yield. In the absence of kinematic hardening, the yield function written in terms of tensor stresses is 1/2 3

f = σe − σy = − σy . σ :σ 2 With kinematic hardening, however, it is 1/2 3

f = (σ − x ) : (σ − x ) − σy (2.53) 2 in which x is the kinematic hardening variable and is often called a back stress. Because it is a variable deﬁned in stress space, it has the same components as stress, and we can write it as a tensor, or, using Voigt notation, as a vector. In order to understand Equation (2.53), let us consider purely uniaxial loading with linear kinematic hardening. 2.5.1

Kinematic hardening under uniaxial loading

We will take the increment in kinematic hardening to be proportional to the increment in plastic strain, hence 2 2 dx = c dεp or equivalently, x˙ = cε˙ p (2.54) 3 3 in which c is a material constant, and the coefﬁcient of 23 will be discussed below. This is called Prager linear hardening. Equation (2.54) has the similarity with isotropic hardening, that the hardening variable depends linearly on the plastic strain. The major difference is that isotropic hardening is described by a scalar variable, r, whereas for kinematic hardening, the hardening variable (or back stress) is a tensor, just as for stress. Because of the incompressibility condition, we know that the plastic strain increment is a deviatoric quantity, that is 1 dε p = dεp − Tr(dεp ) ≡ dεp . (2.55) 3

30

Continuum plasticity

From Equation (2.54), dx is therefore also a deviatoric quantity so that for uniaxial loading in the 1-direction, we may write ⎞ ⎛ ⎞ ⎛ 0 0 x11 x11 0 0 ⎜ 1 0 ⎟ x = x = ⎝ 0 x22 0 ⎠ = ⎝ 0 − 2 x11 (2.56) ⎠. 1 0 0 x33 0 0 − 2 x11 The magnitude or norm of x is deﬁned by x = |x| = (x : x)1/2 ⎡⎛ 0 x11 ⎢⎜ 0 − 1 x = ⎣⎝ 2 11 0 0 1 2 2 = x11 + x11 + 4

(2.57) ⎞ ⎛

0 x11 ⎟ ⎜ 0 −1x ⎠:⎝ 2 11 − 21 x11 0 0 1/2 3 1 2 x = x11 4 11 2 0 0

0 0

⎞⎤1/2 ⎟⎥ ⎠⎦

− 21 x11 (2.58)

so the uniaxial component of x, that is x11 , is 23 times the magnitude of x. Bear in mind that under uniaxial loading, the effective stress is identical to the uniaxial applied stress, and the effective plastic strain increment is identical to the uniaxial plastic strain increment. Note also that like the plastic strain, uniaxial loading leads to the development of not only the uniaxial component of x, but also the other direct components as well. This is because x depends directly on the plastic strain, given in its evolution equation in (2.54). Consider now the components of dx, for uniaxial loading, in Equation (2.54). ⎛ ⎛ p ⎞ ⎞ 0 0 dε11 dx11 0 0 2 ⎜ ⎜ p − 21 dε11 0 ⎟ 0 ⎟ − 21 dx11 dx = ⎝ 0 ⎠ = c⎝ 0 ⎠ 3 1 1 p 0 0 − 2 dx11 0 0 − 2 dε11 so that 2 2 p c dε11 ≡ c dp. (2.59) 3 3 It is often simpler, and in particular, for uniaxial loading, to write the equations in terms of the magnitude of x rather than the loading direction component. Combining Equations (2.59) and (2.58), therefore, gives dx11 =

p

dx = c dε11 ≡ c dp, which is why the coefﬁcient of

2 3

appears in Equation (2.55).

(2.60)

Kinematic hardening

31

We may now determine the terms necessary for the yield function in Equation (2.53) for uniaxial loading as ⎛2 ⎞ 0 0 3 σ11 − x11 ⎜ ⎟ σ − x = ⎝ (2.61) 0 − 21 23 σ11 − x11 0 ⎠ 1 2 0 0 − 2 3 σ11 − x11 which can be written in terms of the magnitude, x, of the back stress as ⎞ ⎛ 0 0 σ11 − x 2⎜ ⎟ 0 − 21 (σ11 − x) σ − x = ⎝ 0 ⎠ 3 1 0 0 − 2 (σ11 − x) so that

⎛

0 (σ11 − x) 4⎜ 1

0 − 2 (σ11 − x) (σ − x ) : (σ − x ) = ⎝ 9 0 0 ⎛ 0 (σ11 − x) ⎜ 1 0 − 2 (σ11 − x) :⎝ 0

0

0 0

⎟ ⎠

− 21 (σ11 − x) ⎞ 0 ⎟ 0 ⎠ − 21 (σ11 − x)

4 1 1 = (σ11 − x)2 + (σ11 − x)2 + (σ11 − x)2 9 9 9 2 = (σ11 − x)2 3 so that

⎞

1/2 3

f = (σ − x ) : (σ − x ) − σy = |σ11 − x| − σy = 0. (2.62) 2 Because we are considering here only uniaxial loading, σ 11 is just the uniaxial stress, σ , so Equation (2.62) can be written f = |σ − x| − σy = 0.

(2.63)

The physical interpretation of Equation (2.63) can be seen in Fig. 2.9. Plastic deformation leads to the translation of the yield surface in stress space. Under uniaxial conditions, therefore, further yield occurs if |σ − x| is equal to the yield stress, σy . There are many forms of kinematic hardening available. What often distinguishes them is how the direction of translation of the yield surface is chosen, and the rate of its evolution as a function of the plastic strain. We shall now look at what is often called Armstrong–Frederick, or Chaboche non-linear kinematic hardening.

32

Continuum plasticity

2.5.2

Non-linear kinematic hardening

In its multiaxial form, the increment, dx, in the back stress is given by dx =

2 c dεp − γ x dp 3

(2.64)

2 p cε˙ − γ xp˙ 3

(2.65)

or equivalently, x˙ =

in which γ is a further material constant. In its uniaxial form, for monotonically increasing plastic strain, Equation (2.64) may be written in terms of the magnitude, x, as dx = c dεp − γ x dεp , which can be integrated, taking x to be 0 at εp = 0, to give x=

c p (1 − e−γ ε ). γ

(2.66)

The resulting form of the stress–strain curve, for this non-linear kinematic hardening, is shown together with the translated yield surface, in Fig. 2.10. As the plastic strain increases, so the back stress, x, in Equation (2.66) saturates to the value c/γ giving a maximum saturated stress of σy + c/γ . The constant γ is the time constant and determines the rate of saturation of stress. c/γ determines the magnitude. We will now examine the ﬂow rule for kinematic hardening. Saturated stress

s2

s2 x

sy

E sy

c/g

sy

sy

s1

sy «2

sy Initial yield surface

Subsequent, translated yield surface

Fig. 2.10 Non-linear kinematic hardening and the resulting non-linear hardening stress–strain curve which saturates at stress c/γ .

Kinematic hardening

2.5.3

33

Flow rule with kinematic hardening

We will use the normality hypothesis in Equation (2.17) together with the yield function in (2.53) to determine the ﬂow rule for plastic deformation with kinematic hardening. First, let us write the yield function, f , as 1/2 3

f = − σy (σ − x ) : (σ − x ) 2 = J (σ − x ) − σy .

(2.67)

The normality hypothesis then gives dεp = dλ

3 σ − x

∂f . = dλ ∂σ 2 J (σ − x )

(2.68)

We now need to use the consistency condition to determine the plastic multiplier. First, let us use Equation (2.68) just to show that 1/2 2 p [(3/2)(σ − x ) : (σ − x )]1/2 dp = dε : dεp = dλ (2.69) = dλ 3 J (σ − x ) for the case of kinematic hardening with a von Mises yield criterion. The yield function depends upon the stress, σ , and the back stress, x, which are both tensor quantities. However, for simplicity, we shall now work in principal stress space again, and use Voigt notation. The consistency condition becomes ∂f ∂f · dσ + · dx = 0, (2.70) ∂σ ∂x which, when combined with Hooke’s law in (2.27), the normality hypothesis in (2.17), and Equation (2.69) gives ∂f ∂f ∂f 2 p · C dε − dλ + · c dε − γ x dλ ∂σ ∂σ ∂x 3 ∂f ∂f 2 ∂f ∂f · C dε − dλ + · c dλ − γ x dλ = 0 = ∂σ ∂σ ∂x 3 ∂σ so that dλ =

(∂f/∂σ) · C dε (∂f/∂σ) · C(∂f/∂σ) + γ (∂f/∂x) · x − (2/3)c(∂f /∂x) · (∂f /∂σ )

(2.71)

and the plastic strain increment is dεp =

∂f (∂f/∂σ) · C dε (∂f/∂σ) · C(∂f/∂σ) + γ (∂f/∂x) · x − (2/3)c(∂f/∂x) · (∂f/∂σ) ∂σ (2.72)

34

Continuum plasticity

and so the stress increment can be obtained from Equation (2.27). We will simplify this to the case of uniaxial loading to interpret the terms in Section 2.5.4, but ﬁrst, we will start by obtaining the plastic multiplier in terms of stress rather than strain increments. Starting from the consistency condition in (2.70) gives ∂f ∂f ∂f ∂f 2 (2.73) · dσ + · dx = · dσ + · c dεp − γ x dp = 0. ∂σ ∂x ∂σ ∂x 3 From the yield function in (2.67), ∂f/∂x = −(∂f /∂σ ) and dp = dλ and with (2.68), (2.73) becomes ∂f ∂f 2 ∂f · dσ − · c dλ − γ x dλ = 0 ∂σ ∂σ 3 ∂σ so that −(∂f/∂σ) · dσ dλ = . (2.74) γ (∂f/∂σ) · x − (2/3)c(∂f/∂σ) · (∂f/∂σ) We will examine this for uniaxial loading in a von Mises material in the following section. 2.5.4

Simple uniaxial loading

For uniaxial loading, we can determine the terms in the denominator of Equation (2.74) as follows: ⎡

⎡ ⎤ ⎡ ⎤ ⎤ ⎡ ⎤ 1 1 1 x1 ∂f 2 ∂f ∂f ⎢− 1 ⎥ ⎣ ⎦ 2 ⎢− 1 ⎥ ⎢− 1 ⎥ γ · = γ ⎣ 2 ⎦ · x2 − c ⎣ 2 ⎦ · ⎣ 2 ⎦ . ·x− c 3 ∂σ ∂σ 3 ∂σ x3 − 21 − 21 − 21

(2.75)

We know that x is a deviatoric quantity so that for uniaxial loading in the 1-direction, 1 x2 = x3 = − x1 2 so that Equation (2.75) becomes just 23 γ x1 − c. Now, we can write x1 = 23 x so that this becomes γ x − c. The numerator in (2.74) is, as before, just −dσ1 so that the plastic multiplier for uniaxial loading is just dσ1 dλ = . (2.76) c − γx In a similar manner to that for the isotropic hardening example, we can obtain the uniaxial stress increment as E dσ = E 1 − dε. (2.77) E + c − γx

Kinematic hardening

35

Let us look at this in a little more detail. If the material behaviour is purely elastic, then the plastic multiplier is zero and the right-hand term in the bracket is zero so that (2.77) simply reduces to dσ = E dε. If we have elastic, perfectly plastic behaviour, that is, no strain hardening, then c = γ = 0 and then (2.77) tells us that during plastic deformation, the increment in stress is zero. If the material undergoes linear kinematic hardening, that is, γ = 0, the stress–strain relation during plasticity becomes E dσ = E 1 − dε (2.78) E+c which is linear during plastic deformation since c is constant. This equation for linear kinematic hardening and that for linear isotropic hardening in Equation (2.51) can be seen to be near identical. The two types of hardening are in fact the same for monotonically increasing loading (provided c = h) and only differ under uniaxial conditions on a load reversal when the Bauschinger effect becomes important. If, ﬁnally, the material undergoes non-linear kinematic hardening, the back stress, x, increases according to its evolution equation, (2.64), so that the stress increment progressively decreases until saturation is achieved at which point, no further stress increase occurs. This can be seen by substituting the equation for x, given in (2.66), into (2.77) to give E dσ = E 1 − dε E + c − γx E E =E 1− dε = E 1 − dε. p p E + c − γ [(c/γ )(1 − e−γ ε )] E + ce−γ ε As the plastic strain increases, so the exponential term diminishes until ultimately, the material becomes perfectly plastic with dσ = 0. Before ﬁnishing this section, Equation (2.77) demonstrates quite nicely the incremental nature of plasticity. Let us consider ﬁrst the case of elasticity only. Equation (2.77) gives dσ = E dε, e where dε = dε . Integrating this equation is clearly possible such that at any particular value of elastic strain, the stress can be calculated. This is simply not possible for the case of plasticity, for which all we can do (normally) is consider increments in stress resulting from an increment in strain. This follows from Equation (2.77) since x itself depends upon strain, so that the increment in stress varies from step to step. The increment in stress, and indeed plastic strain, often depend then, in plasticity, on the history of prior deformation. Plasticity must, in general, therefore, be considered to be an incremental process.

36

Continuum plasticity Expanded yield surface (isotropic hardening) after many cycles s2

s2 B

sy

sy

A

«2

sy s1

sy

C sy

D

Plasticity recommences

Initial yield surface Translated yield surface (kinematic hardening)

Expanded hysteresis loop resulting from isotropic hardening

Strain

Fig. 2.11 Combined kinematic and isotropic hardening.

Time

Fig. 2.12 Strain imposed resulting in cyclic plasticity shown in Fig. 2.11.

2.6

Combined isotropic and kinematic hardening

We will consider, ﬁnally, materials which harden both kinematically and isotropically. This is particularly appropriate for applications to cyclic plasticity where within an individual cycle, kinematic hardening is the dominant hardening process such that the Bauschinger effect can be represented, but over (normally) quite large numbers of cycles, the material also hardens isotropically such that the peak tension and compression stresses in a given cycle increase from one cycle to the next until saturation is achieved. Such a process is represented schematically in Fig. 2.11. Starting from the point of zero stress and strain, the material is subjected to the strain shown in Fig. 2.12. The stress increases until yield is achieved at point A, and the material kinematically hardens leading to the translation of the yield surface, as shown in Fig. 2.11. Once the peak strain is achieved, the strain reversal occurs so that the material becomes elastic

Combined isotropic and kinematic hardening

37

at point B. Elastic deformation continues until the load point reaches the yield surface again at point C where plasticity recommences until the next strain reversal at point D. The yield surface is translated again because of the kinematic hardening. The stress– strain loop BCDB produced in this way is called a hysteresis loop. If, in addition to the kinematic hardening, the material also isotropically hardens, then superimposed upon the translation of the yield surface is a progressive expansion, shown by the broken line hysteresis loop in Fig. 2.11. This process, by which the peak stress and strain in a hysteresis loop increase, due to isotropic hardening, is often called cyclic hardening, as it often occurs from cycle to cycle over many cycles. Kinematic hardening, on the other hand, occurs within each cycle. We will consider the case of non-linear kinematic and isotropic hardening, given by Equations (2.64) and (2.37), respectively. In order to determine the plastic multiplier, we will use the consistency condition as before. The yield function, for combined kinematic and isotropic hardening, depends on the stress, back stress, and accumulated plastic strain as follows f = J (σ − x ) − r(p) − σy

(2.79)

so that the consistency condition becomes ∂f ∂f ∂f · dx + dp = 0. · dσ + ∂x ∂p ∂σ

(2.80)

Substituting for dσ and dx from Equations (2.27) and (2.64) and writing ∂f /∂p = −(∂r/∂p) from (2.79), together with (2.37) gives ∂f ∂f 2 p p (2.81) · C(dε − dε ) + · c dε − γ x dp − b(Q − r(p)) dp = 0. ∂σ ∂x 3 Following the procedure for isotropic and kinematic hardening, (2.81) can be rearranged to give the plastic multiplier. Assuming von Mises behaviour, dp = dλ, and substituting for dε p from (2.17), gives the plastic multiplier as dλ =

(∂f/∂σ)· C dε . (∂f/∂σ)· C(∂f/∂σ)− γ (∂f/∂σ)· x +(2/3)c(∂f/∂σ)· (∂f/∂σ)+b(Q − r(p)) (2.82)

In a similar manner as before, we can determine the plastic multiplier in terms of the increment of stress, rather than strain, as follows. Equation (2.80) is written as 2 ∂f ∂f · c dεp − γ x dp − b(Q − r(p)) dp = 0 · dσ + ∂x 3 ∂σ

38

Continuum plasticity

so that the plastic multiplier becomes dλ =

(∂f/∂σ) · dσ . (2/3)c(∂f/∂σ) · (∂f/∂σ) − γ (∂f/∂σ) · x + b(Q − r(p))

(2.83)

As in previous examples, we can reduce this to the form for uniaxial loading of a von Mises material and obtain for the uniaxial stress increment E dε. (2.84) dσ = E 1 − E + c − γ x + b(Q − r(p))

2.7

Viscoplasticity and creep

So far, we have considered time-independent plasticity only; that is, the stress–strain behaviour has been assumed to be independent of the rate of loading, whether strain or stress controlled. The plasticity of materials which do exhibit rate effects is called viscoplasticity. We shall see that the same formalism for viscoplasticity is also appropriate for creep—the time dependent, irreversible deformation of a material under load. The usual convention for terminology is that viscoplasticity describes rate-dependent plasticity in which crystallographic slip is the dominant deformation process, though likely enhanced by thermally-activated processes such as diffusion-activated dislocation climb. Creep is normally used to describe low strain rate, time-dependent irreversible deformation which is either diffusion controlled, or inﬂuenced by diffusion, though there may well be crystallographic slip still occurring. In viscoplasticity, the elastic–plastic strain decomposition still holds, and yield is determined as for time-independent plasticity with a yield function. In addition, the plastic ﬂow rule is obtained as before using the normality hypothesis of plasticity, and once yielding has occurred, the material may harden isotropically or kinematically. An important difference occurs, however, in that the consistency condition is no longer formally applied so that the load point may now lie outside of the yield surface. As a result, some viscoplasticity models are referred to as over-stress models. We shall start by addressing uniaxial loading in the 1-direction, as before, for conditions of plane stress. Figure 2.13 shows schematically the material’s stress–strain response and the corresponding yield surface which we assume to expand due to linear isotropic hardening. At load point (1) shown on the yield surface in Fig. 2.13(a) and at the corresponding point on the uniaxial stress–strain curve in Fig. 2.13(b), for the case of time-independent plasticity, the stress achieved is the yield stress, σy , together with the contribution from the linear isotropic hardening, r(p) so that σ = σy + r(p).

Viscoplasticity and creep

39

(b)

(a) Load point (1)

s2

s2

sy

sy

sv r (p)

E sy

sy

s1

sy «2

sy Initial yield surface

Subsequent, expanded yield surface

Fig. 2.13 (a) The von Mises yield surface in plane stress for viscoplasticity with linear isotropic hardening, with viscous (over-stress) stress σv , and (b), the corresponding stress strain curve.

The resulting stress–strain curve is that shown by the broken line in Fig. 2.13(b). However, for the case of viscoplasticity, the stress is augmented by the viscous stress, σ v , also shown schematically in Fig. 2.13(b) by the solid line. There are many types of equations used to represent the viscous stress, but they often contain a dependence on the effective plastic strain rate (which for uniaxial conditions is identical to the uniaxial plastic strain rate), p. ˙ This, of course, is how the strain rate dependence of the plasticity is introduced. Let us consider the commonly used power law function σv = Kp˙ m

(2.85)

in which K and m are material constants. The constant m is called the material’s strain rate sensitivity. From Fig. 2.13(b), the stress–strain curve which includes the rate-dependence of stress is therefore σ = σy + r(p) + σv = σy + r(p) + Kp˙ m .

(2.86)

In viscoplasticity, the uniaxial stress depends on the yield stress, the hardening of the yield stress, and the plastic strain rate. The stress response is, therefore, strain rate dependent. For this reason, viscoplasticity is sometimes referred to as time-dependent plasticity or rate-dependent plasticity. Let us consider the uniaxial behaviour described by Equation (2.86) in a little more detail, but to simplify, let us assume perfect plasticity so that there is no isotropic hardening and r(p) = 0. In this case, the equation becomes σ = σy + Kp˙ m .

(2.87)

40

Continuum plasticity

(b)

(a)

s3 Stress

Strain

«• 3 «2

s2 s1

•

«1

sy

•

Plastic strain, p

Time

Fig. 2.14 (a) Applied strain and (b) the resulting rate-dependent stress response.

If we apply strain controlled loading to the uniaxial sample, as shown in Fig. 2.14(a), at a range of different strain rates as shown, the stress response (for given σy , K, and m) as a function of the plastic strain is shown in Fig. 2.14(b). The strain rate dependence of stress is clear and for the three strain rates applied, the corresponding stresses are given by Equation (2.87). Once yield is achieved, for uniaxial perfect plasticity, since dσ = 0, dp = dε, or equivalently, p˙ = ε˙ so that the stresses are σ1 = σy + K ε˙ 1m , σ2 = σy + K ε˙ 2m , σ3 =

(2.88)

σy + K ε˙ 3m .

Many materials exhibit strain rate-dependent plasticity, but unlike the stress–strain curves in Fig. 2.14, would also show isotropic or kinematic hardening. Let us return to the case of isotropic hardening given in Equation (2.86). We can rearrange the equation to give σ − r − σy 1/m p˙ = . (2.89) K If in addition to isotropic hardening, kinematic hardening also occurs, Equation (2.89) becomes σ − x − r − σy 1/m p˙ = . (2.90) K Equations (2.89) and (2.90) are constitutive equations relating uniaxial plastic strain rate to uniaxial stress, and which depend upon internal variables; the isotropic hardening, r, and the kinematic hardening, x. For a von Mises material, the uniaxial stress is identical to the effective stress and similarly for the effective plastic strain rate. Equation (2.90) can therefore be written J (σ − x ) − r − σy 1/m p˙ = . (2.91) K

Viscoplasticity and creep

41

In viscoplasticity, we need a constitutive equation, such as (2.91), which relates the effective plastic strain rate to the stress and internal hardening variables. This replaces the consistency condition in time-independent plasticity, which forces the load point to stay on the yield surface during plastic deformation. In viscoplasticity, the load point may lie outside the yield surface because of the viscous or over-stress. In addition to the viscoplastic constitutive equation, as before, we make use of the normality hypothesis and the elastic constitutive equation; namely Hooke’s law. For viscoplasticity, we write the normality hypothesis, from Equation (2.17), as ε˙ p = λ˙

∂f . ∂σ

(2.92)

The yield function is, from Section 2.6, f = J (σ − x ) − r(p) − σy so that

(2.93)

∂f 3 σ − x

= ∂σ 2 J (σ − x )

and

3 σ − x

λ˙ . (2.94) 2 J (σ − x ) We showed in Section 2.5.3 that for a von Mises material, dp = dλ, or equivalently p˙ = λ˙ so that (2.94) becomes ε˙ p =

ε˙ p =

σ − x

3 p˙ . 2 J (σ − x )

(2.95)

We may now combine the constitutive equation given in (2.91) with (2.95) to give the plastic ﬂow rule for viscoplasticity with isotropic and kinematic hardening as 1/m 3 J (σ − x ) − r − σy σ − x

p ε˙ = . (2.96) K 2 J (σ − x ) To complete the model, we need the evolution equations for the isotropic and kinematic hardening variables r and x, and the rate form of Hooke’s law. From Section 2.4, Equation (2.37) and Section 2.5.2, Equation (2.65), the hardening rates are given by r˙ (p) = b(Q − r)p, ˙

(2.97)

2 p cε˙ − γ x p˙ (2.98) 3 and we will now write Hooke’s law in terms of tensor rather than vector strain terms as x˙ =

σ˙ = 2G˙εe + λ Tr(˙εe )I ,

(2.99)

42

Continuum plasticity

where ε˙ e = ε˙ − ε˙ p

(2.100)

and in which G is the shear modulus, λ the Lame constant given by λ=

Eν (1 − 2ν)(1 + ν)

and I is the identity tensor given by ⎛

1 I = ⎝0 0

⎞ 0 0⎠ . 1

0 1 0

Equations (2.96)–(2.100) form the complete elastic–viscoplastic model. At a given time, t, with knowledge of the current total strain rate, ε˙ and the hardening variables r and x, together with the stress, σ , these equations enable the stresses at the end of a given step forward in time to be determined. We will address this in a later chapter, but for now, let us examine the equations for a simple problem of uniform, uniaxial, and axisymmetric upsetting. 2.7.1

Uniform, uniaxial, and axisymmetric compression

Upsetting is the name given to the open-die forging of cylindrical billets of material. We will consider the uniaxial compression of a cylinder between two platens such that the frictional effects on the contacting surfaces are negligible so that the cylinder remains under uniform, uniaxial compression. The process is shown schematically in Fig. 2.15.

z Undeformed material Platens Deformed material

u r

Fig. 2.15 Frictionless, uniaxial compression representing open-die forging.

Viscoplasticity and creep

43

We will consider constant strain rate-controlled loading and write the plastic strain rates as ⎞ ⎛ p p ε˙ rr ε˙ rz 0 ⎟ ⎜ p p ⎟. ε˙ p = ⎜ (2.101) ε ˙ 0 ε ˙ zz rz ⎠ ⎝ p 0 0 ε˙ θ θ Because we are assuming friction to be negligible, the shear terms are zero. The boundary conditions give us that σrr = σθ θ = σrz = 0 so that the stress and deviatoric stress tensors for the problem become ⎛ 1 ⎞ ⎞ ⎛ 0 0 − 3 σzz 0 0 0 ⎜ ⎟ 2 σ = ⎝ 0 σ = ⎝0 σzz 0⎠ , 0 ⎠. 3 σzz 0 0 0 0 0 − 13 σzz

(2.102)

We will now use Equation (2.96) to determine the plastic strain rate components for the problem. Under this loading, J (σ − x ) = σzz − x (2.103) and from Section 2.5.1,

⎛

− 21 (σzz − x) 0 2

⎝ σ −x = 0 σzz − x 3 0 0

⎞

0 0 − 21 (σzz

⎠ − x)

so that (2.96) becomes ⎞ ⎛ p p ε˙ rr ε˙ rz 0 ⎟ 3 |σzz − x| − r − σy 1/m ⎜ p p ⎟= ⎜ε˙ rz ε˙ zz 0 ⎠ 2 ⎝ K p 0 0 ε˙ θθ ⎛ 1 0 − (σzz − x) 2⎜ 2 1 × 0 σzz − x ⎝ |σzz − x| 3 0 0 which reduces to ⎛ p ⎞ p ⎛ ε˙ rr ε˙ rz 0 1/m − 21 ⎜ p ⎟ |σzz − x| − r − σy ⎜ p ⎜ε˙ rz ε˙ zz 0 ⎟ ⎝ 0 ⎝ ⎠= K p 0 0 0 ε˙ θ θ

(2.104)

0 1 0

⎞

0

⎟ ⎠

0 − 21 (σzz − x)

0

⎞

⎟ 0 ⎠. − 21

(2.105)

44

Continuum plasticity

We may now look at individual components of the plastic strain rate. We see that |σzz − x| − r − σy 1/m p ε˙ zz = (2.106) K which is, of course, just what we would get for purely uniaxial loading, and Equation (2.105) also shows that 1 p 1 |σzz − x| − r − σy 1/m p p ε˙ rr = ε˙ θ θ = − ε˙ zz = − 2 K 2 demonstrating that the incompressibility condition of plasticity is satisﬁed. 2.7.2

Power-law creep

Let us look at one further case in which we assume there to be neither isotropic nor kinematic hardening. Equation (2.96) then becomes, for the plastic strain rate, 1/m σ

3 J (σ ) − σy p (2.107) ε˙ = K J (σ ) 2 and J (σ ) = σe so the equation reduces further to 3 σe − σy 1/m σ

p ε˙ = . 2 K σe

(2.108)

Often in creep problems, where the time-dependent deformation is not dependent upon yield, creep deformation is assumed to occur with the application of a non-zero stress. For creep problems, therefore, Equation (2.108) is often written σ

3 σe 1/m σ

3 3 ε˙ c = = A(σe )n = Aσen−1 σ

(2.109) 2 K σe 2 σe 2 which is the multiaxial form of Norton’s creep law, where A and n are material constants. For uniaxial loading, it reduces to 2 3 Aσen−1 σ = Aσ n . 2 3 For completeness, we can write out Equation (2.109) in full component form as ⎛

⎛ c c c ⎞

⎞ σxx σxy ε˙ xx ε˙ xy ε˙ xz σxz ⎜ c c c ⎟ = 3 Aσ n−1 ⎜σ

⎟ ε˙ yz σyz (2.110) ⎠ ⎝ yx σyy ⎠ ⎝ε˙ yx ε˙ yy e 2 c c c

ε˙ zx ε˙ zy ε˙ zz σzx σzy σzz ε˙ c =

in which the stress and strain rate tensors are symmetric.

Further reading

2.7.3

45

Potential and yield function equivalence

In the last example, we saw how the plastic strain rate, based on the normality hypothesis together with an appropriate constitutive equation for plastic strain rate, was determined for viscoplasticity, but then reduced to Norton’s law for creep deformation. Because creep processes may occur independently of plastic yielding, it is not appropriate to use a yield surface, in the conventional sense discussed earlier. Instead, a potential function is deﬁned from which creep strain rates are determined. We will deﬁne a potential, φ, such that ε˙ 0 σ0 σe n+1 φ= (2.111) n + 1 σ0 in which ε˙ 0 and σ˙ 0 are material constants with units of strain rate and stress, respectively. The potential function, φ, therefore has units of Joules per second per unit volume. It therefore represents an energy per second per unit volume. The plastic (creep) strain rate is determined from ∂φ ∂σ

(2.112)

3 ε˙ 0 σ0 n−1 3 σ σ = Aσen−1 σ , 2 σ0n+1 e 2

(2.113)

ε˙ c = giving ε˙ c =

which is identical to Equation (2.109). The potential function, φ, in creep plays a similar role to the yield function in plasticity. In fact, often the yield function is considered to be a potential function. The surfaces in stress space represented by φ are often called equipotential surfaces; the energy per second per unit volume is the same at each point on the potential surface, just as the value of σe takes the same value on every point of a yield surface in plasticity.

Further reading Dieter, G.E. (1988). Mechanical Metallurgy. McGraw-Hill Book Co., London. Hill, R. (1998). The Mathematical Theory of Plasticity. OUP (Oxford Classics Series). (ﬁrst published in 1950). Khan, A.S. and Huang, S. (1995). Continuum Theory of Plasticity. John Wiley & Sons Inc, New York. Lemaitre, J. and Chaboche, J.-L. (1990). Mechanics of Solid Materials. CUP, Cambridge, UK. Lubarda, V.A. (2002). Elastoplasticity Theory. CRC Press, Florida, USA.

This page intentionally left blank

3. Kinematics of large deformations and continuum mechanics

3.1

Introduction

The strains, be they elastic or plastic, which most engineering components undergo in service are usually small, that is, 200%). This is three orders of magnitude larger than the strain needed to cause yield. In manufacturing processes, another very important feature is material rotation. Deformation processing leading to large plastic strains often also leads to large rigid body rotations. The bending of a circular plate, to large deformation, is an example which shows the rigid body rotation. Figure 3.1 shows the result of applying a large downward displacement at the centre of an initially horizontal, simply supported circular disc. Only one half of the disc section is shown. While the displacements and rigid body rotations can be very large, the strains remain quite small.

×

×

Fig. 3.1 Simulated large elastic–plastic deformation of an initially horizontal, simply supported circular plate. Only one half of the plate section is shown.

48

Large deformations and continuum mechanics

Towards the outer edge of the disc, where it is supported, the ﬁnite element simulation shows that the strains generated are quite small, but that because of the disc bending, the rigid body rotations are very large. Generally, deformation comprises of stretch, rigid body rotation, and translation. The stretch provides the shape change. The rigid body rotation neither contributes to shape change nor to internal stress. Because a translation does not lead to a change in stress state, we will not address it in detail here. In this chapter, we will give an introduction to measures of large deformation, rigid body rotation, elastic–plastic coupling in large deformation, stress rates, and what is called material objectivity, or frame indifference. Later chapters dealing with the implementation of plasticity models into ﬁnite element code will rely on the material covered here and in Chapter 2.

3.2

The deformation gradient

In order to look at deformation, let us consider a small lump of imaginary material which is yet to be loaded so that it is in the undeformed (or initial ) conﬁguration (or state). This is shown schematically as state A in Fig. 3.2. We will now apply a load to the material in state A so that it deforms to that shown in state B, the deformed or current conﬁguration. We will assume that the material undergoes combined stretch (i.e. relative elongations with respect to the three orthogonal axes), rigid body rotation, and translation. We will measure all quantities relative to the global XYZ axes, often known as the material coordinate system. Consider an inﬁnitesimal line, PQ, or vector, dX, embedded in the material in the undeformed conﬁguration. The position of point P is given by vector X, relative to the material reference frame. The line PQ undergoes deformation from state A to the deformed

Deformed (current) configuration, state B

Z Q9 dx O

x Q dX X

P9 u

X

P Y

Undeformed (original) configuration, state A

Fig. 3.2 An element of material in the reference or undeformed conﬁguration undergoing deformation to the deformed or current conﬁguration.

Measures of strain

49

conﬁguration in state B. In doing so, point P has been translated by u to point P . Relative to the material reference frame, point P is given by vector x where x = X + u.

(3.1)

The inﬁnitesimal vector dX is transformed to its deformed state, dx, by the deformation gradient, F , where dx = F dX. We can write this in component form as ⎛ ⎞ ⎛ Fxx dx ⎝dy ⎠ = ⎝Fyx dz Fzx

Fxy Fyy Fzy

⎛ ∂x

⎞ ⎛ ⎞ ⎜ ∂X dX Fxz ⎜ ⎜ ∂y ⎠ ⎝ dY ⎠ = ⎜ Fyz ⎜ ∂X dZ Fzz ⎝ ∂z ∂X

(3.2) ∂x ∂Y ∂y ∂Y ∂z ∂Y

∂x ⎞ ∂Z ⎟ ⎛dX ⎞ ⎟ ∂y ⎟ ⎝ ⎠ ⎟ dY ∂Z ⎟ dZ ⎠ ∂z ∂Z

(3.3)

or F =

∂x . ∂X

(3.4)

The deformation gradient, F , provides a complete description of deformation (excluding translations) which includes stretch as well as rigid body rotation. Rigid body rotation does not contribute to shape or size change, or internal stress. In solving problems, it is necessary to separate out the stretch from the rigid body rotation contained within F . In the following sections, we will see examples of stretch, rigid body rotation, and their combination, and how they are described by the deformation gradient.

3.3

Measures of strain

Let us consider the length, ds, of the line dx in the deformed conﬁguration. We may write ds 2 = dx · dx = (F dX) · (F dX) = dXT F TF dX T ∂x T ∂x = dX dX = dXT C dX ∂X ∂X so that C = F TF .

(3.5)

C is called the (left) Cauchy–Green tensor. Consider also the length, dS, of the element, dX, in the undeformed state: dS 2 = dXT dX.

(3.6)

50

Large deformations and continuum mechanics

Now dx = F dX so

dX = F −1 dx.

Substituting into Equation (3.6) gives dS 2 = (F −1 dx)T F −1 dx = dx T (F −1 )TF −1 dx = dx T B −1 dx, where

B −1 = (F −1 )TF −1

(3.7)

and B is called the (right) Cauchy–Green tensor. Both B and C are in fact measures of stretch as we will now see. A measure of the stretch is given by the difference in lengths of the lines PQ and

P Q in Fig. 3.2 in the undeformed and deformed conﬁgurations, respectively. We can write (3.8) ds 2 − dS 2 = dx · dx − dx · B −1 dx = dx · (I − B −1 ) dx in which I is the identity tensor. It can be seen, therefore, that B is related to the change in length of the line; in other words, a measure of stretch. It is independent of rigid body rotation because the orientations of the lines in the undeformed and deformed conﬁgurations are irrelevant. If ds and dS are the same length, then there is no stretch and ds 2 − dS 2 = 0. From Equation (3.8), this means that B=I

(3.9)

and there is no stretch, so that in this instance, the deformation gradient contains only rigid body rotation. The Cauchy–Green tensor, B, could itself be used as a measure of strain, since it is independent of rigid body rotation, but depends upon the stretch. This is an important criterion for any strain measure in large deformation analysis in which rigid body rotation occurs. A strain which depends upon rigid body rotation would not be appropriate since it would give a different measure of the strain depending upon orientation. However, the Cauchy–Green tensor given in (3.9) contains nonzero components even though the stretch is zero. An alternative and more appropriate strain measure called the Almansi strain was introduced: 1 e = (I − B −1 ) (3.10) 2 so that for zero stretch, e = 0.

Measures of strain

51

This strain measure behaves more like familiar strains, such as engineering strain, since for zero stretch, it gives us strain components of zero. A further measure of strain is the logarithmic, or true strain deﬁned as 1 ε = − ln B −1 , (3.11) 2 which we shall consider in more detail later. In determining the change of length of the line OP, we could have chosen the original conﬁguration to work in as follows: ds 2 − dS 2 = dx T dx − dX T dX = (F dX)T F dX − dXT dX = dXF TF dX − dXT dX = dXT (F TF − I ) dX = dXT (C − I ) dX = dXT (2E) dX, where

1 1 (C − I ) = (F TF − I ). (3.12) 2 2 E is called the large strain or the Green–Lagrange strain tensor. We can make this look a little more familiar, perhaps, by combining Equations (3.4) for F and (3.1) for x ∂x ∂(u + X) ∂u F = = = +I ∂X ∂X ∂X and then substituting into (3.12) to give

T 1 T ∂u 1 ∂u E = (F F − I ) = +I +I −I 2 2 ∂X ∂X

∂u T ∂u T ∂u 1 ∂u + . (3.13) + = 2 ∂X ∂X ∂X ∂X E=

If we ignore the second-order term, this reduces to 1 ∂u ∂u T E= . + 2 ∂X ∂X

(3.14)

We will examine this and other strains for simple uniaxial loading in Section 3.4. Before doing so, let us examine the symmetry of the strain quantities presented above. The symmetric part of a tensor, A, is given by 1 (A + AT ) (3.15) 2 and the antisymmetric or skew symmetric (or sometimes simply skew) part of A by sym(A) =

asym(A) =

1 (A − AT ). 2

(3.16)

52

Large deformations and continuum mechanics

To be pedantic, let us write out the symmetric and antisymmetric parts of the 2 × 2 matrix A given by a11 a12 A= a21 a22 in which a12 = a21 . ⎛ a12 + a21 ⎞ a11 2 ⎠ sym(A) = ⎝ a12 + a21 a22 2 and ⎛ a12 − a21 ⎞ 0 2 ⎠. asym(A) = ⎝ a12 − a21 − 0 2 Clearly, sym(A) is symmetric and the leading diagonal of an antisymmetric tensor always contains zeros. Let us now consider the quantity F TF which appears above in a number of strain quantities: 1 sym(F TF ) = [F TF + (F TF )T ] = F TF 2 and 1 asym(F TF ) = [F TF − (F TF )T ] = 0. 2 We see, therefore, that F TF is a symmetric tensor so that, in fact, the quantities B −1 , C, ε, and E are all themselves symmetric. In general, F will not necessarily be symmetric. If it is, the deformation it represents is made only up of stretch.

3.4

Interpretation of strain measures

Let us determine the deformation gradient for the simple case of a uniaxial rod which is subjected, ﬁrst to purely rigid body rotation and then to uniaxial stretch and then consider some of the measures of deformation and strain introduced in Section 3.3. 3.4.1

Rigid body rotation only

Figure 3.3 shows a rod lying along the Y -axis which undergoes a clockwise rotation about the Z-axis of angle θ . There is no stretch imposed, so the deformation gradient is simply the rotation matrix, R, given by ⎞ ⎛ cos θ − sin θ 0 (3.17) F = R = ⎝ sin θ cos θ 0⎠ . 0 0 1

Interpretation of strain measures

Y, y

y

53

u Y x

X, x

X

Fig. 3.3 A rod undergoing rigid body rotation through angle θ.

The uppercase letters in Fig. 3.3, XY, refer to the material reference frame directions. Also shown in the ﬁgure is a coordinate system which rotates with the deforming material (in this case, the rotating rod). We will generally use lowercase letters, xy, to indicate the reference frame which rotates with the material. This is called the co-rotational reference frame. We can now determine the Cauchy–Green tensor, B −1 , and the strain quantities. From Equation (3.7), ⎞ ⎞⎛ ⎛ cos θ sin θ 0 cos θ − sin θ 0 B −1 = (F −1 )TF −1 = ⎝ sin θ cos θ 0⎠ ⎝− sin θ cos θ 0⎠ 0 0 1 0 0 1 ⎞ ⎛ 1 0 0 ⎝ = 0 1 0⎠ . 0 0 1 The tensor B −1 is found to be the identity tensor for rigid body rotation because there is no stretch. Measures of deformation that are appropriate for large deformations with rigid body rotation must have this property: that they depend upon the stretch but are independent of the rigid body rotation. The Almansi strain, from (3.10), is 1 e = (I − B −1 ) = 0 2 and the true strain, (3.11), is given by 1 ε = ln B −1 = 0. 2 Similarly, the Green strain is 1 E = (F TF − I ) = 0. 2 We see that the three strain measures give zero for the case of rigid body rotation. Before moving away from rotation, it is important to note that a rotation tensor, such as R, is always orthogonal, that is, RR T = I

(3.18)

54

Large deformations and continuum mechanics

Deformed rod after stretch

Undeformed rod

Y, y

l

l0

Z, z

X, x

r r0

Fig. 3.4 A rod undergoing pure stretch in the absence of rigid body rotation.

so that

R T = R −1 .

We will make much use of this property in the subsequent sections. 3.4.2

Uniaxial stretch

Let us now consider uniaxial stretch of the circular rod in the Y -direction. This is shown schematically in Fig. 3.4. Note that because there is no rotation in this case, the co-rotational reference frame is directionally coincident with the material reference frame. For the uniaxial stretch shown, the stretch ratios, λ, are λx =

r , r0

λy =

l , l0

λz =

r . r0

(3.19)

Let us consider the case of large strain such that the elastic strains can be ignored. For large plastic deformation, the incompressibility condition written in terms of stretches is λx λy λz = 1 (3.20) so that

and therefore

1 λx = λz ≡ λy

−1/2 l λx = λz = . (3.21) l0 Considering the stretch along the Y -axis, any point, Y , lying on the undeformed rod becomes the point y = λy Y on the deformed rod. The deformation can therefore be represented by x = λx X, y = λy Y, z = λz Z

Interpretation of strain measures

so that

∂x = λx , ∂X

∂y = λy , ∂Y

55

∂z = λz ∂Z

and

∂x ∂x = = 0 etc. ∂Y ∂Z The deformation gradient can then be determined using Equation (3.3), ⎛ ⎞ ∂x ∂x ∂x ⎜ ∂X ∂Y ∂Z ⎟ ⎛ ⎞ ⎜ ⎟ λx 0 0 ⎜ ⎟ ∂x ∂y ∂y ∂y ⎟ ⎝ =⎜ = 0 λy 0 ⎠ F = ⎜ ∂X ⎜ ∂X ∂Y ∂Z ⎟ ⎟ 0 0 λz ⎝ ∂z ∂z ∂z ⎠ ∂X ∂Y ∂Z and with (3.19) and (3.21) ⎞ ⎛ −1/2 l 0 0 ⎟ ⎜ l ⎟ ⎜ 0 ⎟ ⎜ l ⎟. 0 0 F =⎜ ⎟ ⎜ l0 ⎟ ⎜ −1/2 ⎠ ⎝ l 0 0 l0 We ﬁrst notice that F is symmetric so that FT = F and therefore represents stretch only. Let us examine the various deformation and strain tensors. The inverse of F is ⎛ 1/2 ⎞ l 0 0 ⎟ ⎜ ⎜ l0 ⎟ ⎜ ⎟ −1 l ⎜ ⎟ F −1 = ⎜ 0 0 ⎟ ⎜ ⎟ l0 ⎜ 1/2 ⎟ ⎝ ⎠ l 0 0 l0 so the Cauchy–Green tensor is given by ⎛ ⎞ l 0 0⎟ ⎜ l0 ⎜ ⎟ −2 ⎜ ⎟ l −1 −1 T −1 −1 −1 B = (F ) F = F F = ⎜ 0⎟ ⎜0 ⎟. l0 ⎜ ⎟ ⎝ l⎠ 0 0 l0

56

Large deformations and continuum mechanics

The true plastic strain is, therefore, ⎞ ⎛ ⎛ ⎞ l 1 l 0 0 − ln 0 0 ⎟ ⎜ l0 ⎟ 2 l0 ⎜ −2 ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ 1 1 l l ⎟ ⎜ ⎟=⎜ ε = − ln B −1 = − ln ⎜ 0 ln 0 ⎟. 0 0 ⎟ ⎜ ⎟ 2 2 ⎜ l0 l0 ⎟ ⎜ ⎝ 1 l⎠ ⎝ l⎠ 0 0 − ln 0 0 2 l0 l0 (3.22) We see that the true strain components are εxx = εzz = − 21 ln(l/l0 ) = − 21 εyy and εyy = ln(l/l0 ), as we would expect for uniaxial plasticity conditions. Before leaving the true strain, note that we needed to take the logarithm of the Cauchy–Green tensor which we did by operating on the leading diagonal alone. We were able to do this in this case because the leading diagonal terms happen, in this simple case, to be the principal parts of the tensor (i.e. the eigenvalues). In general, in order to carry out an operation, p, on tensor A having a linearly independent set of eigenvectors, we need to diagonalize the tensor and operate on the principal values. In practice, this means transforming the tensor into its principal coordinates, by ﬁnding the eigenvalues and eigenvectors of A, operating on it and transforming it back. If the modal matrix (i.e. the matrix containing the eigenvectors of A) is written as M, and the diagonal matrix (i.e. the matrix containing the ˆ then A can be written eigenvalues of A along the leading diagonal) as A, ˆ −1 A = M AM so that we operate on A to give p(A) as follows −1 ˆ p(A) = Mp(A)M ,

(3.23)

where the operation p is carried out only on the leading diagonal terms. For example, −1 ˆ ln(A) = M ln(A)M .

In Equation (3.22), the modal matrix of B −1 in this case is just the identity matrix and −1 its diagonal matrix Bˆ is the same as B −1 so that ln(B −1 ) = M ln(Bˆ

−1

)M −1 = I ln(B −1 )I −1 = ln(B −1 ).

Let us ﬁnally determine the Green strain ﬁrst from (3.12) and second directly from the displacements using (3.14).

Polar decomposition

Using (3.12), we need ⎛ 2 r 0 ⎜ ⎜ r0 2 ⎜ l ⎜ F TF = ⎜ 0 ⎜ l0 ⎜ ⎝ 0 0

⎞

⎛ 2r ⎟ 1 + ⎟ ⎜ r0 ⎟ ⎜ ⎟ ⎜ 0 0 ⎟≈⎜ ⎟ ⎜ 2 ⎟ ⎝ r ⎠ 0 r0 0

57

⎞ 0

0

2l 1+ l0 1+

0

⎟ ⎟ ⎟ 0 ⎟ ⎟ 2r ⎠ r0

if we write r = r0 + r and assume that the strains are small, so that ⎤ ⎛ ⎡⎛ ⎞ ⎞ 2r r 1 + 0 0 0 0 ⎢⎜ ⎟ ⎛1 0 0⎞⎥ ⎜ r0 ⎟ r0 ⎥ ⎜ ⎢ ⎜ ⎟ ⎟ 1 ⎢⎜ l 2l ⎥ ⎜ ⎟ ⎝ ⎟ ⎠ = − E = ⎢⎜ 0 0 0 1+ 0 0 1 0 ⎥ ⎜ ⎟ ⎟. ⎥ ⎜ ⎟ ⎟ 2 ⎢⎜ l0 l0 0 0 1 ⎦ ⎝ ⎣⎝ r ⎠ 2r ⎠ 0 0 0 0 1+ r0 r0 We see that the components of the Green strain are therefore approximately the engineering strain components. If we now start from (3.14) in which we have also neglected second-order terms, we need the displacements, u, which are given by ux = (r − r0 ) so that

⎛

r ⎜ r0 ⎜ ∂u ⎜ =⎜ 0 ∂X ⎜ ⎝ 0

Y uy = (l − l0 ) , l0

X , r0

l l0 0

0 ⎟ ⎟ ⎟ 0 ⎟ ⎟ r ⎠ r0

Z r0

⎛

⎞ 0

uz = (r − r0 )

and

r ⎜

⎜ r0 ∂u T 1 ∂u ⎜ =⎜ 0 + E= ⎜ 2 ∂X ∂X ⎝ 0

⎞ 0 l l0 0

0 ⎟ ⎟ ⎟ 0 ⎟ ⎟ r ⎠ r0

as before. We have looked at a number of examples in which stretch and rigid body rotation have taken place exclusively. We will now look at how to separate them in cases where they occur simultaneously, using the polar decomposition theorem.

3.5

Polar decomposition

Recall that the deformation at any material point can be considered to comprise three parts: (1) rigid body translation (which we do not need to consider here); (2) rigid body rotation; (3) stretch.

58

Large deformations and continuum mechanics

The polar decomposition theorem states that any non-singular, second-order tensor can be decomposed uniquely into the product of an orthogonal tensor (a rotation), and a symmetric tensor (stretch). The deformation gradient is a non-singular, second-order tensor and can therefore be written as F = RU = VR, (3.24) where R is an orthogonal (R TR = I ) rotation tensor, and U and V are symmetric (U = U T ) stretch tensors. Using the polar decomposition theorem, we can now examine in more detail the right and left Cauchy–Green deformation tensors. From Equation (3.7), B −1 = (F −1 )TF −1 = [(VR)−1 ]T (VR)−1 = (R −1 V −1 )T R −1 V −1 = (V −1 )T (R −1 )T R −1 V −1 = (V −1 )T V −1 since R is orthogonal

B −1 = V −1 V −1 = (V −1 )2 ,

where the squaring operation is carried out on the diagonalized form of V −1 . This conﬁrms, therefore, that B is a measure of deformation that depends on stretch only, and is independent of the rigid body rotation, R. Similarly, for C, C = F TF = (RU )TRU = U T R TRU = U TU = U2

since R is orthogonal since U is symmetric.

The true strain rate can now be written in terms of V since 1 1 (3.25) ε = − ln B −1 = − ln(V −1 )2 = ln V , 2 2 which is also independent of the rigid body rotation and dependent on the stretch alone. Let us have a look at a problem in which both stretch and rigid body rotation occur together: the problem of simple shear. 3.5.1

Simple shear

Figure 3.5 shows schematically the simple shear by δ, in two dimensions, of a unit square. We can represent the deformation, which transforms a point (X, Y ) in the undeformed conﬁguration to (x, y) in the deformed conﬁguration, by x = X + δY,

y=Y

Polar decomposition

Y, y

59

Deformed square

d 1 Undeformed square 1

X, x

Fig. 3.5 A unit square undergoing simple shear.

so that

∂x ∂x = 1, = δ, ∂X ∂Y The deformation gradient is, therefore, 1 F = 0

∂y = 0, ∂X

∂y = 1. ∂Y

δ . 1

We can then determine the Cauchy–Green tensor, C, from 1 0 1 δ 1 δ T C=F F = . = δ 1 0 1 δ 1 + δ2

(3.26)

Note the symmetry of this deformation tensor. We can use the polar decomposition theorem to separate out the stretch and rigid body rotation contained in the deformation gradient. Let us set cos ϕ sin ϕ Uxx Uxy R= (3.27) U= − sin ϕ cos ϕ Uyx Uyy so that

F = RU

gives

1 0

δ cos ϕ = 1 − sin ϕ

sin ϕ cos ϕ

Uxx Uyx

Uxy . Uyy

(3.28)

Solving for the stretches in terms of δ and ϕ gives cos ϕ sin ϕ U= sin ϕ cos ϕ + δ sin ϕ and substituting back into (3.28) gives δ sin ϕ = √ 2 2 + δ2

and

so that R=√

1 22 + δ 2

2 cos ϕ = √ 2 2 + δ2

2 −δ

δ 2

(3.29)

60

Large deformations and continuum mechanics

and U=√

1

2 δ

δ . 2 + δ2

(3.30) 22 + δ 2 Comparing Equations (3.30) and (3.26), and with a little algebra conﬁrms that C = U 2 . U is the symmetric stretch and Equation (3.29) shows that the rigid body rotation is non-zero. It is useful to examine why this is. It may not be obvious that the deformation corresponding to simple shear shown in Fig. 3.5 leads to a rigid body rotation. Let us ﬁrst determine the Green–Lagrange strain for this deformation. Using Equation (3.12), 1 T 1 1 1 0 δ 1 δ 1 0 E = (F F − I ) = (C − I ) = − = . δ 1 + δ2 0 1 2 2 2 δ δ2 2 (3.31) From Equation (3.29), or from the components of strain in Equation (3.31), we see that the principal stretch directions rotate as the simple shear proceeds. That is, the ‘material axes’ rotate relative to the direction of the applied deformation. The polar decomposition theorem is fundamental to large deformation kinematics and we shall return to it in subsequent sections.

3.6

Velocity gradient, rate of deformation, and continuum spin

We have so far considered stretch, rigid body rotation, measures of strain, and the polar decomposition theorem which enables us to separate out stretch and rotation. All the quantities considered have been independent of time. However, many plasticity formulations (viscoplasticity is an obvious case) are developed in terms of rate quantities and it is necessary, therefore, to consider how the quantities already discussed can be put in rate form. Often, in fact, even rate-independent plasticity models are written in rate form for implementation into ﬁnite element code. This is easy to understand given that plasticity is an incremental process; rather than deal with increments in plastic strain, it is often more convenient to work with the equivalent quantity, plastic strain rate. Consider a spatially varying velocity ﬁeld, that is, one for which the material point velocities vary spatially. The increment in velocity, dv, occurring over an incremental change in position, dx, in the deformed conﬁguration, may be written as ∂v dx. ∂x The velocity gradient describes the spatial rate of change of the velocity and is given by dv =

L=

∂v . ∂x

(3.32)

Velocity gradient, rate of deformation, and continuum spin

61

Consider the time rate of change of the deformation gradient: ∂ ∂x ∂v ∂v ∂x ˙ F = = = = LF ∂t ∂X ∂X ∂x ∂X or ˙ −1 . L = FF

(3.33)

The velocity gradient, therefore, maps the deformation gradient onto the rate of change of the deformation gradient. The velocity gradient can be decomposed into symmetric (stretch related) and antisymmetric (rotation related) parts: L = sym(L) + asym(L), where sym(L) =

1 (L + LT ) 2

(3.34)

and 1 (L − LT ). (3.35) 2 The symmetric part is called the rate of deformation, D, and the antisymmetric part the continuum spin, W , so that asym(L) =

L = D + W,

(3.36)

where the rate of deformation D=

1 (L + LT ) 2

(3.37)

1 (L − LT ). 2

(3.38)

and the continuum spin is given by W =

We shall now examine both quantities, the rate of deformation and the continuum spin, for some simple examples, including uniaxial stretch and purely rigid body rotation in order to gain a physical feel for these quantities. 3.6.1

Rigid body rotation and continuum spin

We have previously looked at the rigid body rotation of a uniaxial rod. Figure 3.3 shows this schematically. We will now look not only at the rigid body rotation, but also the rate at which it occurs. Consider the rotation of the rod shown in Fig. 3.3,

62

Large deformations and continuum mechanics

at time t making an angle θ with the Y -axis, with no stretch, rotating at constant rate ˙ The deformation gradient at any instant is given by θ. ⎞ ⎛ cos θ − sin θ 0 (3.39) F = ⎝ sin θ cos θ 0⎠ 0 0 1 so that the rate of change of deformation gradient is ⎛ − sin θ − cos θ F˙ = θ˙ ⎝ cos θ − sin θ 0 0

⎞ 0 0⎠ . 0

(3.40)

In order to determine the velocity gradient, we need the inverse of F which we can obtain from (3.39) as ⎞ ⎛ cos θ sin θ 0 F −1 (= F T in this case) = ⎝− sin θ cos θ 0⎠ . 0 0 1 We may then determine the velocity gradient using Equation (3.33) as ⎞ ⎛ ⎞⎛ ⎛ 0 cos θ sin θ 0 − sin θ − cos θ 0 ˙ −1 = θ˙ ⎝ cos θ L = FF − sin θ 0⎠ ⎝− sin θ cos θ 0⎠ = θ˙ ⎝1 0 0 0 1 0 0 0 The transpose of L is

⎛

0 LT = θ˙ ⎝−1 0 so that the deformation gradient is given by

1 0 0 ⎛

0 1 D = (L + LT ) = θ˙ ⎝0 2 0

⎞ 0 0⎠ . 0

⎞ 0 0⎠ 0 0 0 0

⎞ 0 0⎠ = 0 0

and the continuum spin is

⎛ 0 1 W = (L − LT ) = θ˙ ⎝1 2 0

−1 0 0

−1 0 0

⎞ 0 0⎠ . 0

(3.41)

That is, there is no stretch rate contributing to the velocity gradient so that the rate of deformation is zero, but rigid body rotation occurs so that the continuum spin is non-zero. Let us now examine the signiﬁcance of the continuum spin for the case of rigid body rotation of the uniaxial rod without stretch.

Velocity gradient, rate of deformation, and continuum spin

˙ given by Consider the rate of rotation, R, ⎛ − sin θ − cos θ ˙ ⎝ ˙ R = θ cos θ − sin θ 0 0 Next, consider the product of W and R ⎞⎛ ⎛ cos θ − sin θ 0 −1 0 ⎠ ⎝ ⎝ ˙ WR = θ 1 0 0 sin θ cos θ 0 0 0 0 0

⎞ 0 0⎠ . 0

⎞ ⎛ − sin θ 0 ⎠ ⎝ ˙ 0 = θ cos θ 0 1

63

(3.42)

− cos θ − sin θ 0

⎞ 0 0⎠ . 0

That is, for this particular case of rigid body rotation only, we see that ˙ = WR R

(3.43)

˙ Remembering that R is orthogonal so so that W is the tensor that maps R onto R. T −1 that R = R , W can be written for this simple case as ˙ T. W = RR

(3.44)

The spin is not itself, therefore, a rate of rotation, but it is closely related to it. Let us use the polar decomposition theorem to examine the continuum spin in a little more detail and more generally, and introduce the angular velocity tensor. 3.6.2

Angular velocity tensor

From Equation (3.38), the continuum spin is given by 1 (L − LT ) 2 so substituting for the velocity gradient from (3.33) gives W =

1 ˙ −1 ˙ −1 − (F −1 )TF˙ T ). ˙ −1 )T ) = 1 (FF (FF − (FF 2 2 If we now substitute for F using the polar decomposition theorem in (3.24), after a little algebra we obtain W =

1 ˙ T ˙ T + R(U˙ U −1 − (U˙ U −1 )T )R T ]. [RR − R R 2 We will simplify this further by considering the product W =

RR T = I , which we can differentiate with respect to time to give ˙ T + RR ˙T =0 RR

(3.45)

64

Large deformations and continuum mechanics

so that

˙ T = −R R ˙ T = −(RR ˙ T )T . RR

(3.46)

˙ T is antisymmetric, since any tensor Z for which Z = −Z T We see, therefore, that RR is antisymmetric because 1 1 (Z + Z T ) = (Z − Z) = 0. 2 2 Substituting (3.46) into (3.45) gives sym(Z) =

˙ T + 1 R(U˙ U −1 − (U˙ U −1 )T )R T W = RR 2

(3.47)

or 1 (3.48) W = Ω + R(U˙ U −1 − (U˙ U −1 )T )R T = + R asym(U˙ U −1 )R T 2 ˙ T is called the angular velocity tensor which depends only on the in which Ω = RR rigid body rotation and its rate of change and is independent of the stretch. If we consider a deformation comprising of rigid body rotation only, as we did in Section 3.6.1, or if the stretch is negligibly small, then Equation (3.48) simply reduces to ˙ T W = Ω = RR

(3.49)

as we saw in Equation (3.44). In general, the angular velocity tensor and continuum spin are not the same; Equation (3.48) shows that they differ depending on the stretch, U . Both W and Ω are important when considering objective stress rates, as we shall see in Section 3.8. We will look at one further simple example in which we examine in particular the rate of deformation and the continuum spin; that of uniaxial stretch with no rigid body rotation. 3.6.3

Uniaxial stretch

We considered the uniaxial elongation of a rod lying along the Y -direction earlier (see Fig. 3.4) for which we obtained the deformation gradient, assuming purely plastic deformation and the incompressibility condition, in terms of the current, l, and original, l0 , rod lengths as ⎛ −1/2 ⎞ l 0 0 ⎜ l ⎟ ⎜ 0 ⎟ ⎜ ⎟ l ⎜ ⎟. F =⎜ 0 0 ⎟ l0 ⎜ ⎟ −1/2 ⎠ ⎝ l 0 0 l0

Velocity gradient, rate of deformation, and continuum spin

65

We will now determine the rate of deformation and continuum spin for the case of uniaxial stretch. Differentiating the deformation gradient gives ⎛ ⎞ 1 l −3/2 1 ˙ l 0 0 ⎜− ⎟ ⎜ 2 l0 ⎟ l0 ⎜ ⎟ ˙ l ⎜ ⎟ F˙ = ⎜ ⎟ 0 0 ⎜ ⎟ l0 −3/2 ˙ ⎟ ⎜ ⎝ l⎠ 1 l 0 0 − 2 l0 l0 and

F −1

⎛ 1/2 l ⎜ ⎜ l0 ⎜ ⎜ =⎜ 0 ⎜ ⎜ ⎝ 0

⎞ 0 −1 l l0 0

⎟ ⎟ ⎟ ⎟ 0 ⎟ ⎟ 1/2 ⎟ ⎠ l 0

l0

so that the velocity gradient is ⎛ ⎞ 1 l −1 l˙ 0 0 ⎜− ⎟ l0 ⎜ 2 l0 ⎟ ⎜ ⎟ ˙ l −1 l ⎜ ⎟ −1 ˙ L = FF = ⎜ ⎟= 0 0 ⎜ ⎟ l0 l0 ⎜ −1 ˙ ⎟ ⎝ 1 l l⎠ 0 0 − 2 l0 l0

⎛ 1 ⎜− 2 l˙ ⎜ ⎜0 l⎜ ⎝ 0

0 1 0

⎞ 0 ⎟ ⎟ 0 ⎟ ⎟. 1⎠ − 2

This is a symmetric quantity and therefore equal to the rate of deformation. In addition, its antisymmetric part is zero so that the continuum spin is zero. Formally, ⎞ ⎛ 1 −2 0 0 ˙ 1 l D = (L + LT ) = ⎝ 0 1 0 ⎠ , 2 l (3.50) 0 0 − 21 1 W = (L − LT ) = 0. 2 There is, therefore, no rigid body rotation occurring; just stretch. Let us look at the rate of deformation for this case of uniaxial stretch. For uniaxial stretch in the Y -direction, the true plastic strain components are given by εyy = ln

l , l0

1 εxx = εzz = − εyy 2

66

Large deformations and continuum mechanics

so that the strain rates are l˙ 1 l˙ ε˙ xx = ε˙ zz = − and ε˙ xy = ε˙ yz = ε˙ zx = 0. ε˙ yy = , l 2l Examination of the components of the deformation gradient in (3.50) shows, therefore, that D, for this case, can be rewritten ⎛ ⎞ ε˙ xx 0 0 D = ⎝ 0 ε˙ yy 0 ⎠ . (3.51) 0 0 ε˙ zz For uniaxial stretch, therefore, in the absence of a rigid body rotation, it can be seen that the rate of deformation is identical to the true strain rate. This is not generally the case; it happens to be so for this example because there is no rigid body rotation. However, the example gives us a reasonable feel for what kind of measure the rate of deformation is. We now return to the consideration of elastic–plastic material behaviour under large deformation conditions. We will consider cases in which the elastic strains, while not negligible, can always be assumed to be small compared with the plastic strains.

3.7

Elastic–plastic coupling

Consider now an imaginary lump of material in the undeformed conﬁguration, shown in Fig. 3.6. The material contains a line vector, dX. As before, after deformation F

Initial configuration

Current configuration

Z dX

dx x

X x

O

Fe Fp X dp Y

Intermediate, stress-free, configuration

Fig. 3.6 Schematic diagram showing an element of a material in the initial and current conﬁgurations and in the intermediate, stress-free, conﬁguration.

Elastic–plastic coupling

67

to the deformed or current conﬁguration, the line vector is transformed to dx. The transformation mapping of dX to dx is, of course, the deformation gradient, F . We now introduce what is called the intermediate conﬁguration. In transforming from the initial to deformed conﬁguration, the line vector dX has undergone elastic and plastic deformation. The intermediate conﬁguration is that in which line vector dx has been unloaded to a stress-free state; this is an imaginary state corresponding to one in which dX in the undeformed conﬁguration has undergone purely plastic deformation to become dp in the intermediate conﬁguration. The transformation mapping of dX to dp is the plastic deformation gradient so that dp = F p dX and the plastic deformation gradient is deﬁned as ∂p . (3.52) ∂X In the current conﬁguration dp is deformed into dx by the elastic deformation so that Fp =

dx = F e dp and the elastic deformation gradient is deﬁned as Fe =

∂x . ∂p

(3.53)

We may then write dx = F e dp = F eF p dX so that F = F eF p .

(3.54)

This is the classical multiplicative decomposition of the deformation gradient into elastic and plastic parts, due to Erastus Lee. Note that for general inhomogeneous plastic deformation, unloading a body will not generally lead to uniform zero stress; rather a residual stress ﬁeld exists. Considering a ﬁnite number of material points within a continuum, at each point an unstressed conﬁguration can be obtained, but F p and F e are, strictly, no longer pointwise continuous. Within the context of a ﬁnite element analysis, however, in which a discretization is necessary and the discontinuity of stress and strain resulting from the discretization is the norm, this is not a problem. In addition, note that the intermediate conﬁguration described by p is, in general, not uniquely determined since an arbitrary rigid body rotation can be superimposed on it, still leaving it unstressed. In Equation (3.54), both the elastic and plastic deformation gradients may contain both stretch and rigid body rotation.

68

Large deformations and continuum mechanics

However, in order to overcome the uniqueness problem, often, by convention, all the rigid body rotation is lumped into the plastic deformation gradient, F p , such that the elastic deformation gradient, F e , includes stretch only (no rigid body rotation). As a result, F e is written Fe = Ve

(symmetric stretch)

and so F p = V pR in which R is the equivalent total rigid body rotation. With this convention, let us now look at the velocity gradient and address the decomposition of the elastic and plastic rates of deformation. 3.7.1

Velocity gradient and elastic and plastic rates of deformation

We will now determine the velocity gradient in terms of the elastic and plastic deformation gradient decomposition given in (3.54). The velocity gradient is given by ∂ p e (F eF p )(F eF p )−1 = (F eF˙ + F˙ F p )F p−1F e−1 ∂t e p e p = F˙ F e−1 + F eF˙ F p−1F e−1 = V˙ V e−1 + V e F˙ F p−1 V e−1 .

˙ −1 = L = FF

Now, e Le = V˙ V e−1 = D e + W e p Lp = F˙ F p−1 = D p + W p

so L = Le + V e Lp V e−1 = D e + W e + V e D p V e−1 + V e W p V e−1 .

(3.55)

Now, D = sym(L)

W = asym(L).

Therefore, using Equation (3.55), D = D e + sym(V e D p V e−1 ) + sym(V e W p V e−1 )

(3.56)

W = W e + asym(V e D p V e−1 ) + asym(V e W p V e−1 ).

(3.57)

and In general, therefore, we see from (3.56) the result that the elastic and plastic rates of deformation are not additively decomposed, that is, D = D e + D p .

Objective stress rates

69

This is unlike the additive decomposition of elastic and plastic strain rates for the case of small deformation theory, given in Equation (2.1). However, if the elastic strains are small, then V e = V e−1 ≈ I . Also, sym(D P ) = D P , sym(W P ) = 0, since rate of deformation and spin are symmetric and antisymmetric, respectively. Hence, for small elastic stretches (V e ≈ I ), from Equations (3.56) and (3.57), D = De + DP

(3.58)

W = W e + W P.

(3.59)

and

This is an important and well-known result and we will shortly see that Equation (3.58) is often used in the implementation of plasticity models into ﬁnite element code. The plastic rate of deformation, D p , like the plastic strain rate in small strain theory, is speciﬁed by a constitutive equation. Often, in ﬁnite element implementations, the total rate of deformation, D, is known such that if D p is speciﬁed by a constitutive equation, then D e can be determined using (3.58) so that the stress rate may be determined using Hooke’s law. Once we know the stress rate, we can integrate over time to determine stress. This brings us to the ﬁnal step in our brief examination of continuum mechanics. We need to address stress rate and how to determine it in a material undergoing rigid body rotation with respect to a ﬁxed coordinate system. We will do this in Section 3.8, and then summarize the most important steps required in going from knowledge of deformation to determination of stress, before introducing ﬁnite element methods in Chapter 4.

3.8

Objective stress rates

The primary focus of this section is stress rate, but before looking at this, we need to look at what is called material objectivity. We will start not by considering stress rate, but by something more familiar; transformation of stress.

3.8.1

Principle of material objectivity or frame indifference

Consider the transformation of the stress tensor, σ , which undergoes a rotation through θ relative to the (XYZ) coordinate system. The stress transformation equations, or Mohr’s circle, tell us that the transformed stresses, σ , with respect to the

70

Large deformations and continuum mechanics

Reference plane ∆F n ∆A

u

s∆ A τ∆ A

Body

Fig. 3.7 Schematic diagram showing a body cut by a plane with normal n generating an area of intersection of A, subjected to resultant force F .

(XYZ) coordinate system become

σXX = σXX cos2 θ + 2σXY sin θ cos θ + σY Y sin2 θ

σY Y = σXX sin2 θ − 2σXY sin θ cos θ + σY Y cos2 θ

σXY

= (σY Y − σXX ) sin θ cos θ + σXY

(cos2 θ

(3.60)

− sin θ). 2

The last of the three equations enables us to determine the direction of the principal axes, relative to the applied stress direction, and of course, the principal stresses.

= 0 so that It does this because along the principal directions, σXY tan 2θ =

σXY . σXX − σY Y

(3.61)

We will look at an alternative way of dealing with stress (and indeed, other tensor quantities such as strain) transformation. In order to do this, we need to introduce the stress vector or surface traction. 3.8.1.1 The stress vector or traction. Figure 3.7 shows a lump of material, making up a body which has been cut by a plane with normal direction n, with an inﬁnitesimal area of intersection, A. Under uniform stress state, the resultant force acting on the area A is F . The stress vector acting on the area A is deﬁned by F t= . (3.62) A A→0 By deﬁnition, t is a vector quantity with normal, σ , and shear, τ , components, as shown in Fig. 3.7. We will now look at how the stress vector, t, on a particular plane with normal n is related to the stress tensor, σ . Consider the three orthogonal planes shown in Fig. 3.8(a) and the resulting plane ABC, reproduced in Fig. 3.8(b).

Objective stress rates (a)

y B sxy

tx sxz

szz

szy

tz

(b) s

szx

B

t

sxx n

z

71

A syy syz

syx

C

x

τ

A C

ty

Fig. 3.8 Schematic diagram showing (a) the stress vectors acting on three orthogonal planes with components in the x-, y-, and z-directions shown and (b) the resultant stress vector acting on plane ABC which has normal n, with components n = [nx ny nz ]T .

On each of the orthogonal planes in Fig. 3.8(a), a stress vector acts. For example, on plane ‘x’, that is, the plane orthogonal to the x-direction, the stress vector is t x . The stress vectors acting on the three orthogonal planes have components given by ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ σzx σxx σyx ⎣ ⎦ ⎣ ⎣ ⎦ t x = σxy , t x = σzy ⎦ . (3.63) t y = σyy , σzz σyz σxz The convention is that on plane ‘x’, the stress components are labelled σxx in the x-direction, σxy in the y-direction, and so on. If the area of plane ABC is A, then the areas of the three orthogonal planes are given by ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ 0 0 1 Ax = ⎣0⎦ · An = Anx , Ay = ⎣1⎦ · An = Any , Az = ⎣0⎦ · An = Anz . 0 1 0 (3.64a) By consideration of equilibrium, the resultant force on plane ABC must be balanced by the forces on the three orthogonal planes so that ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ σxx σyx σzx ⎦ ⎦ ⎣ ⎣ ⎣ tA = t x Ax + t y Ay + t z Az = σxy Anx + σyy Any + σzy ⎦ Anz . (3.64b) σxz σyz σzz Therefore ⎡

⎤ ⎡ ⎤ ⎡ ⎤ ⎛ σxx σyx σzx σxx ⎣ ⎦ ⎦ ⎦ ⎣ ⎣ ⎝ t = σxy nx + σyy ny + σzy nz = σyx σxz σyz σzz σzx

σxy σyy σzy

⎞⎡ ⎤ nx σxz ⎠ ⎣ σyz ny ⎦ σzz nz

(3.65)

72

Large deformations and continuum mechanics

remembering that for reasons of moment, or rotational equilibrium, the stress tensor is symmetric so that σxy = σyx etc. Equation (3.65) can be written in a simple way as t = σ n.

(3.66)

3.8.1.2 Transformation of stress. Let us now return to the problem of transformation of stress. Consider the stress vector, t, acting on a surface with normal n. At the point of interest, the stress is fully described by the tensor σ . Under some rotation, R, the stress vector t is transformed to t acting on a plane with normal n , and similarly, the stress σ is transformed to σ such that t = σn

and

t = σ n .

Under rotation, R, the vectors t and n transform according to t = Rt which give Combining these gives but

and

t = Rσ n and

n = Rn n = R T n .

t = RσR T n

t = σ n

so that ﬁnally

σ = RσR T . (3.67) We see, therefore, that unlike a vector, the stress tensor, σ , transforms according to Equation (3.67). To see what this means in detail, let us consider the two-dimensional transformation giving Equations (3.60). The rotation matrix, R, corresponding to the rotation of θ is cos θ − sin θ R= sin θ cos θ so that cos θ sin θ cos θ − sin θ σxx σxy

σ = . − sin θ cos θ sin θ cos θ σxy σyy Multiplying these equations will give Equation (3.60). The stress transformation equations, or Mohr’s circle representation, are beautifully and succinctly summarized, therefore, in Equation (3.67). This equation also tells us how other tensor quantities (such as strain, for example) transform. More formally, a tensor, A, is said to be frame indifferent or objective if it rotates according to the following: A = QAQT .

(3.68)

Comparing Equation (3.67) with (3.68) shows that the Cauchy stress tensor is objective. Let us consider a simple example to understand what is meant by objective.

Objective stress rates

3.8.2

73

Stressed rod under rotation: co-rotational stress

Consider a rod initially lying parallel to the Y -axis, of cross-sectional area A, under constant, axial, force P , shown schematically in Fig. 3.9(a). In this conﬁguration, with respect to the XY coordinate system, the stresses in the rod are: P , σXY = 0. A A co-rotational (xy) coordinate system has been introduced which rotates with the rod. The stresses in the rod relative to the co-rotational (xy) coordinate system initially are, similarly, P σxx = 0, σyy = , σxy = 0. A The rod undergoes a rotation of θ as shown in Fig. 3.9(b), relative to the (XY ) coordinate system. With respect to the co-rotational system, the rod is subjected to an unchanging stress in the y-direction of P/A; all other stress components remain zero. The stresses σXX = 0,

(a) Y P/A

σY Y =

s XX = 0 s Y Y = P/A s XY = 0

s XX ≠ 0 s YY ≠ 0 s XY ≠ 0

(b) Y u P/A

y

x y x

P/A

P/A

X

X

(c) Y

s X X = P/A s YY = 0 s XY = 0 x P/A

y

P/A

X

Fig. 3.9 A rod of cross-sectional area A undergoing rigid body rotation while subjected to axial force P (a) in the initial conﬁguration, (b) having rotated through angle θ, and (c) after rotating through 90◦ showing the changing stresses with respect to the material (XY) reference frame.

74

Large deformations and continuum mechanics

in the rod, however, when measured with respect to the material (XY) reference frame can be seen to change. For example, when the rod has rotated through 90◦ as shown in Fig. 3.9(c), it lies parallel to the X-axis so that now, the stresses with respect to the material (XY) reference frame are P σXY = 0. , σY Y = 0, A They are, therefore, completely different to what they were in the initial state shown in Fig. 3.9(a). However, the stresses relative to the co-rotational system are as before; that is, P σxx = 0, σxy = 0. σyy = , A The stresses relative to the co-rotational coordinate system, which we shall designate by σ , are related to those relative to the material (XY ) coordinate system, which we shall designate by σ , by σ = RσR T (3.69) σXX =

in which R is just the rotation matrix. σ is called an objective or co-rotational stress because with respect to the co-rotational reference frame (and indeed, the material undergoing the rotation), its stress state has not changed; it has simply rotated. Note that the co-rotational stress, given in Equation (3.69) follows the requirement of objectivity given in Equations (3.67) and (3.68). The objective stress, therefore, results from the constitutive response of the material; it is independent of orientation and derives from the material response rather than the rigid body rotation. Before addressing stress rate and its objectivity, we will ﬁrst look at the objectivity, or otherwise, of a number of other important quantities in large deformation kinematics. 3.8.3

Objectivity of deformation gradient, velocity gradient, and rate of deformation

Consider the deformation gradient F . dx = F dX.

(3.70)

After a transformation, Q, the quantities in Equation (3.70) become dx , F , and dX

so that dx = F dX . (3.71) Now,

dx = Q dx = QF dX

and dX remains unchanged under deformation, by deﬁnition, so that dX = dX.

Objective stress rates

75

Therefore, from Equation (3.71), F = QF .

(3.72)

F is, therefore, in fact objective and behaves like a vector because it is what is called a two point tensor, that is, only one of its two indices is in the spatial coordinate, x. We will now look at the objectivity of the velocity gradient, the rate of deformation, and the continuum spin. Differentiating Equation (3.72) gives

˙ + QF˙ F˙ = QF

so that

˙ + QF˙ )F −1 Q−1 = QQ ˙ T + QFF ˙ −1 QT L = F˙ F −1 = (QF

and

˙ T + QLQT . L = QQ

(3.73)

Comparing with the requirement for objectivity in Equation (3.68), therefore, shows that the velocity gradient is not objective. The transformed velocity gradient, L , from Equation (3.73) can be written L =

1 1 ˙ −1 . Q(L + LT )QT + Q(L − LT )QT +QQ 2 2 Symmetric

(3.74)

Antisymmetric

˙ T is antisymmetric. Therefore, from (3.74), From Equation (3.46) we see that QQ D = sym(L ) = and

1 Q(L + LT )QT = QDQT 2

˙ −1 . W = asym(L ) = QWQT + QQ

(3.75)

Therefore, the deformation rate, D, is objective, but the continuum spin, W , is not. It is useful to ask whether this is important or not. In Sections 3.8.1 and 3.8.2, we examined the objectivity of the Cauchy stress and found that it is indeed objective. The Cauchy stress is, therefore, a quantity for which the properties are independent of the reference frame. This is very important in the development of constitutive equations. An equation which relates elastic strain to stress, for example, must be independent of the reference frame in which the relationship is used; in other words, the constitutive equation must provide information about the material response which is independent of rigid body rotation. The same holds for constitutive equations relating rate of plastic deformation (which we have just shown to be objective) to Cauchy stress (also objective), or the constitutive equation relating stress rate to elastic rate of deformation. In fact, plasticity

76

Large deformations and continuum mechanics

problems, especially within the context of ﬁnite element implementations, are often formulated in rate form. It is therefore necessary for us to address stress rate and, in particular, to examine whether stress rate is objective or otherwise. It turns out that there are many measures of objective stress rate, and we will focus on one in particular; the Jaumann stress rate.

3.8.4

Jaumann stress rate

We will examine, ﬁrst, a rather contrived problem in order to get a physical feel for the meaning of the Jaumann stress rate. We will then look more generally at the objectivity of this stress rate, and ﬁnish by looking at a simple example. Consider again a rod under axial stress σ , shown in Fig. 3.10(a). The stress tensor, with respect to the material axes is σt . During a time increment of t, the rod undergoes a rigid body rotation such that at time t + t, the rod lies as shown in Fig. 3.10(b) in which the co-rotational reference axes (xy) now coincide with the material reference axes (XY ).

(a) Y

(b) Y

∆u

0 0 0 sRt+ ∆t = 0 s 0 0 0 0

s

s y

x y

x s s

Time = t Time = t + ∆t

X

X s + ∆s

(c) Y

y

0 st + ∆t = 0 0

0 s + ∆s 0

0 0 0

x s + ∆s Time = t + ∆t X

Fig. 3.10 A rod under axial stress, σ , undergoing rigid body rotation (a) at a time t, (b) at a time t + t having gone through incremental rotation R (corresponding to angle θ about the Z-direction) and (c) at the same time t + t but having also undergone stress increment σ .

Objective stress rates

77

The stress tensor σ with respect to the co-rotational reference frame is ⎞ ⎛ 0 0 0 σ t = ⎝0 σ 0⎠ , 0 0 0 which is obtained from

σt = Rσt R T ,

(3.76)

where R is the incremental rigid body rotation. Following the rigid body rotation, the rod is subjected to an additional axial stress, σ , shown in Fig. 3.10(c), so that the ﬁnal stress tensor, with respect to the co-rotational frame (and the material frame since they are coincident at time t + t) is ⎞ ⎛ 0 0 0

σt+t = ⎝0 σ + σ 0⎠ . 0 0 0 The Cauchy stress increment with respect to the co-rotational frame may be written approximately, using Equation (2.99), as σ = [2GD e + λTr(D e )I ]t,

(3.77)

where we have used the rate of elastic deformation in place of the elastic strain rate. The stress increment results, therefore, purely from the material’s constitutive response and is co-rotational. We may then write the co-rotational stress tensor at time t + t as the sum of (3.76) and (3.77) to give

σt+t ≡ σt+t = Rσt R T + [2GD e + λTr(D e )I ]t.

(3.78)

In order to investigate this further, let us consider the case in which the incremental rigid body rotation, R, is small. We may then approximate the rotation matrix as R = exp[ˆr ] ≈ I + ˆr in which ˆr is the associated antisymmetric tensor which is approximately given by Wt (a full explanation for this can be found, e.g., in Belytschko et al., 2000). Substituting into (3.78) then gives σt+t = (I + Wt)σt (I + Wt)T + [2GD e + λTr(D e )I ]t = σt + σt W Tt + W σt t + W σt W Tt 2 + [2GD e + λTr(D e )I ]t so that σt+t − σt = σt W T + W σt + σt W σt t + [2GD e + λTr(D e )I ]. t

78

Large deformations and continuum mechanics

Now, both σt and σt+t are given with respect to the material reference frame so that taking the limit, and letting t → 0, gives us the material stress rate, σ˙ as σ˙ = σt W T + W σt + 2GD e + λTr(D e )I and as W is antisymmetric (we saw earlier that this means W T = −W ), we obtain σ˙ = W σt − σt W + 2GD e + λTr(D e )I . We can rewrite this as

∇

σ˙ = σ +W σt − σt W , where

∇

σ = 2GD e + λTr(D e )I .

(3.79) (3.80) (3.81)

∇

σ in Equations (3.80) and (3.81) is called the Jaumann stress rate and it is the stress rate that results purely from the constitutive response of the material and not from rigid body rotation. It is, therefore, as we shall see in Section 3.8.4.1, an objective stress rate. We may therefore use it in constitutive equations such as (3.81) in which both the Jaumann stress rate and the elastic rate of deformation are objective quantities. The material stress rate, σ˙ however, does depend upon rigid body rotation. σ˙ is the Cauchy stress rate with respect to the material reference frame; that is, in Figs 3.9 and 3.10, σ˙ gives the stress rate with respect to the material (XY ) axes. In ﬁnite element simulations, we are ordinarily interested in the stresses with respect to the material axes. Equation (3.80) is therefore important in that it enables us to determine the required stresses from knowledge of the material’s constitutive response given by the Jaumann stress rate in (3.81). It is useful to remember that the stresses, σt , in Equation (3.80), are also given with respect to the material reference frame. 3.8.4.1 Objectivity of Jaumann stress rate. Let us now show that the Jaumann stress rate is objective. We saw earlier that a quantity A is said to be objective if it transforms according to (3.68), that is A = QAQT and that the Cauchy stress transforms in this way (σ = QσQT ). Differentiating the stress with respect to time gives T T ˙ ˙ T ) = QσQ ˙ ˙ T. ˙ T + σQ ˙ T + QσQ σ˙ = QσQ + Q(σQ + QσQ

(3.82)

We see from Equation (3.82) that the material rate of Cauchy stress is not objective (even though the stress itself is) since it does not transform according to (3.68). We saw in Section 3.8.3, Equation (3.75) that ˙ −1 . W = QWQT + QQ

Objective stress rates

79

Rearranging and remembering that Q is orthogonal gives

so that since both W and gives

W

˙ = W Q − QW Q

(3.83)

˙ T = −QT W + WQT Q

(3.84)

are antisymmetric. Substituting (3.83) and (3.84) into (3.82)

˙ T + Qσ WQT − QσQT W σ˙ = W QσQT − QW σQT + QσQ so that

σ˙ = Q(σ W − W σ + σ˙ )QT + W QσQT − QσQT W .

(3.85)

Substituting for QσQT = σ into (3.85) gives σ W − W σ + σ˙ = Q(σ W − W σ + σ˙ )QT .

(3.86) ∇

Equation (3.86) therefore shows that the Jaumann stress rate, σ , satisﬁes the requirement for objectivity in Equation (3.68), where ∇

σ = σ˙ + σ W − W σ .

(3.87)

There are objective stress rates other than that of Jaumann. Details of these may be found in many of the more advanced text books on continuum mechanics, and in particular, that of Belytschko et al. (2000). 3.8.4.2 Example of Jaumann stress rate for a rotating rod. We will conclude Section 3.8.4 with a simple example of a rotating rod under constant, uniaxial stress. We refer back to Fig. 3.9(b) which shows the rotating bar at an instant at which it makes an angle θ with the vertical. It is subject to a constant, uniaxial stress of P/A at all times. This, of course, gives a constant co-rotational stress (with respect to co-rotational xy-axes) of ⎞ ⎛ 0 0 σ = ⎝ (3.88) P ⎠. 0 A The stresses with respect to the material (XY ) axes, however, change with the rotation, as shown in Fig. 3.9(a)–(c). This means that there is a rate associated with each stress component which also changes with the rotation. We will now determine the stresses in the rod with respect to the material axes as it rotates. We will do this in two ways; ﬁrst, we will set up the problem in rate form and integrate to obtain the stresses and second, use the standard method for transformation of stress using Equation (3.67) (or equivalently, Mohr’s circle).

80

Large deformations and continuum mechanics ∇

We may obtain the objective, or co-rotational stress rate, σ , simply by differentiating (3.88) with respect to time. As the co-rotational stress is always constant, its derivative is zero, so ⎞ ⎛ 0 0 ∂ ⎝ ∇ σ = P ⎠ = 0. ∂t 0 A The stress rate with respect to the original conﬁguration, σ˙ , is given by rearranging (3.87) ∇

σ˙ = σ − σ W + W σ = W σ − σ W .

(3.89)

If there is no rotation, then W = 0 and (3.89) tells us that the stress rates with respect to the material axes are also zero. However, the rod is rotating, with constant angular speed θ˙ . We showed for this case, Equation (3.41), that this results in a continuum spin given by 0 −1 W = θ˙ . (3.90) 1 0 The stresses with respect to the material axes may be written σXX σXY σ = . σXY σY Y

(3.91)

Substituting (3.90) and (3.91) into (3.89) gives σ − σ −2σ XY XX Y Y σ˙ = θ˙ . σXX − σY Y 2σXY That is

dσXX dσY Y = −2θ˙ σXY ≡ − dt dt

and

(3.92)

dσXY = θ˙ (σXX − σY Y ). (3.93) dt Equation (3.92) gives σXX = −σY Y +k where k is just a constant. The initial conditions are σXX (0) = 0, σY Y (0) = P/A, σXY (0) = 0 so that k = P/A. Differentiating (3.93) and substituting into (3.92) and using k = P/A gives d2 σXX P = +4θ˙ 2 σXX = 2θ˙ 2 . A dt 2 This has general solution σXX = A sin 2θ + B cos 2θ +

P , 2A

Summary

81

˙ so that with the initial conditions, the full solution is where θ = θt, P P P σXX = sin2 θ, (3.94) σY Y = cos2 θ, σXY = sin θ cos θ. A A A We see, therefore, that the stresses with respect to the material reference frame change correctly with angle θ . For example, when θ = 0, σXX = 0, σY Y = P/A, σXY = 0, and when θ = π/2, σXX = P/A, σY Y = 0, σXY = 0. Finally, we will determine the same stresses using the stress transformation equation in (3.67). That is, σ = RσR T ↑ ↑ (x, y) (X, Y ) reference reference so that the stresses in the material (XY ) reference are given by ⎛ ⎞ 0 0 P cos θ sin θ ⎝ cos θ − sin θ sin2 θ σ = = P⎠ − sin θ cos θ sin θ cos θ A sin θ cos θ 0 A which just gives the expressions in Equation (3.94).

3.9

sin θ cos θ , cos2 θ

Summary

Before leaving the kinematics of large deformations, we will summarize some of the important steps required in going from knowledge of deformation through to the determination of stresses for an elastic–plastic material undergoing large deformations. This is often required in the implementation of plasticity models into ﬁnite element code so it is something we shall return to later. We assume that any deformation taking place is such that the stretches due to elasticity are small compared with those for plasticity so that the additive decomposition of rate of deformation given in Equation (3.58) holds. We also assume full knowledge of the deformation gradient, F and its rate, F˙ . The steps required in determining stresses are then as follows. 1. Determine the velocity gradient ˙ −1 . L = FF 2. Determine the rates of deformation and continuum spin 1 D = sym(L) = (L + LT ), 2 1 W = asym(L) = (L − LT ). 2

82

Large deformations and continuum mechanics

3. The rate of plastic deformation is speciﬁed by a constitutive equation. For example, from Chapter 2, for combined isotropic and kinematic hardening with power law dependence of effective plastic strain rate on stress, we have in the current conﬁguration 1/m σ − x

3 J (σ − x ) − r − σy p D = . 2 K J (σ − x ) 4. Determine the rate of elastic deformation De = D − Dp. 5. Determine the Jaumann stress rate using the tensor form of Hooke’s law, Equation (3.81), from the rate of elastic deformation ∇

σ = 2GD e + λTr(D e )I . 6. Determine the material rate of stress using (3.80) ∇

σ˙ = σ +W σ − σ W . 7. Use a numerical technique to obtain the stresses with respect to the material reference frame by integrating σ˙ . We will address all of these steps in some detail in later chapters.

Further reading Belytschko, T., Liu, W.L., and Moran, B. (2000). Non-linear Finite Elements for Continua and Structures. John Wiley & Sons Inc, New York. Khan, A.S. and Huang, S. (1995). Continuum Theory of Plasticity. John Wiley & Sons Inc, New York. Lubarda, V.A. (2002). Elastoplasticity Theory. CRC Press, Florida, USA. Simo, J.C. and Hughes, T.J.R. (1997). Computational Inelasticity. Springer-Verlag, Berlin.

4. The ﬁnite element method for static and dynamic plasticity

4.1

Introduction

There are few practical problems in plasticity which can be solved analytically. This is usually because of irregular geometry and/or complicated boundary and loading conditions. Computational mechanics, and in particular, the ﬁnite element method, enables the approximate solution of these types of problems. The important requirements of equilibrium, and compatibility, together with a material’s constitutive response, enable solutions to be obtained subject to the satisfaction of initial and boundary conditions. Satisfying the requirements of equilibrium, compatibility, constitutive equations, and boundary conditions is essential for the solution of any solid mechanics problem. Within the ﬁnite element method, the body under consideration is discretized into a ﬁnite number of elements and nodes, with the latter each having a speciﬁed number of degrees of freedom. The ﬁnite element model representing the body therefore contains a ﬁnite number of degrees of freedom and the implication is that the requirement for equilibrium cannot be satisﬁed exactly at every point in the continuum (in what is called the strong sense). Instead, within the ﬁnite element technique, a weak formulation of equilibrium is used in which global equilibrium for the body as a whole is imposed even though this does not necessarily ensure pointwise equilibrium. Further details of strong and weak formulations are available in texts that are more specialized. A weak formulation can be obtained by consideration of the principle of virtual work, which appears in many text books, but here, we shall use Hamilton’s principle. The advantage, as we shall see, is that the equilibrium equations of motion can be obtained in a fully uniﬁed manner, for both quasi-static and dynamic problems, and that the boundary conditions for the problem are also obtained. We shall use Hamilton’s principle to obtain the equations of motion (and boundary conditions) for a number of well known discrete and continuous systems. In this way, we aim to develop a good physical feel for what the principle is doing before addressing more complicated ﬁnite element applications.

84

Finite element method

We introduce Hamilton’s principle in Section 4.2. A reasonable knowledge of vector calculus is useful, but the important results are not impenetrable without it! Unfamiliar readers may like to skip on to the introduction to the ﬁnite element method in Section 4.3. Here, in keeping with the aims of this book, we address ﬁrst a simple one-dimensional rod element subjected to elastic deformation alone and then very brieﬂy look at element assemblage and some other ﬁnite element types. We then return to elastic–plastic problems and address plasticity in a one-dimensional rod element.

4.2

Hamilton’s principle

Hamilton’s principle, which results from conservation of energy, is one of the most general principles of mechanics. It provides a means for ﬁnding the equilibrium equations (equations of motion) of a dynamical system by determining the stationary value of a scalar integral. The principle states that the variation of the kinetic and potential energy plus the variation of the work done by non-conservative (external) forces acting during any time interval t1 to t2 must be zero. We will shortly see what is meant by variation, and of course, non-conservative implies forces that cannot be described by the change in a potential energy function (as can strain energy, for example), which are not already included in the potential energy term. Let the total kinetic energy of the system be T , the potential energy of the system be U , and the work done by non-conservative forces be W . The Lagrangian, L, is deﬁned as L=T −U +W (4.1) and the J-integral is deﬁned as t2 J = L dt = t1

t2

t1

(T − U + W ) dt.

(4.2)

Hamilton’s principle states that the ﬁrst variation (denoted by δ) of J is zero thus t2 t2 δL dt = δ(T − U + Wnc ) dt = 0. (4.3) δJ = t1

t1

In other words, the motion of a system between speciﬁed, realizable initial, and ﬁnal conditions at times t1 to t2 is such that the average value of L relative to any dynamical path compatible with the physical constraints has a stationary value. An illustration of such a motion is given in Fig. 4.1 for a single degree of freedom system (SDOF). Generally, the kinetic energy, potential energy, and work of non-conservative forces depend on some function (e.g. displacement, temperature, etc.) of time y(t) which

Hamilton’s principle

x

85

Two dynamical paths compatible with constraints (the difference between trajectories is dx)

dx

x(t ) x(t ) t1

t2

t

Fig. 4.1 Two dynamical paths subjected to having the same state at times t1 and t2 .

can be expressed as follows J =

t2

t1

L dt =

t2

t1

L(y, y , t) dt

(4.4)

in which y is just y˙ = dy/dt. Hamilton’s principle tells us that the dynamical path, y(t), is that which leads to a stationary value of J . Let us now look at how Equation (4.4), called a functional, may be minimized by use of the calculus of variations. Let y = y(t) be the actual minimizing curve (as distinct from any admissible curve) and let Y (t) = y(t) + εη(t) (4.5) be the family of comparison curves, where η(t) is an arbitrary function subjected to the constraint that η(t1 ) = η(t2 ) = 0 (4.6) and ε is an arbitrary parameter. The corresponding J integral is t2 L(Y, Y , t) dt J¯(ε) = t1

and its variation with respect to ε is t2 ∂L ∂Y

∂L ∂Y ∂ ¯ J (ε) = + dt. ∂ε ∂Y ∂ε ∂Y ∂ε t1

(4.7)

(4.8)

For ε = 0, and using (4.5), this variation yields by integrating by parts, as t2 t2 t2 ∂L

∂L t2 ∂L ∂L d ∂L ∂ ¯ J (0) = η + η dt = η dt + η − η dt

∂ε ∂y ∂y ∂y dt ∂y

t1 t1 ∂y t1 t1 t2 d ∂L ∂L ∂L t2 − η dt + η , = ∂y dt ∂y

∂y t1 t1

86

Finite element method

which for η(t1 ) = η(t2 ) = 0 yields t2 ∂ ¯ d ∂L ∂L J (0) = − η dt. ∂ε ∂y dt ∂y

t1

(4.9)

Therefore, the necessary condition for minimization of J is ∂ ¯ ∂ ¯ J (0) = J (ε) = 0. ∂ε ∂ε Hence,

t2

t1

(4.10)

∂L d ∂L η dt = 0. − ∂y dt ∂y

Since η is arbitrary, it follows that ∂L d ∂L − = 0, ∂y dt ∂y

(4.11)

which is known as Euler–Lagrange equation and which must be satisﬁed for J to have a minimum. If the function y(t) is replaced by y + δy where δy is the variation of y such that δy(t1 ) = δy(t2 ) = 0,

(4.12)

then it follows using Taylor’s theorem that t2 ∂L ∂L

J (y + δy) = J (y) + δy + (δy) dt ∂y ∂y t1 t2 2 ∂ L 2 ∂ 2L ∂ 2 L 2 1

δy + 2 δy(δy) + 2 (δy ) dt + 2! t1 ∂y∂y

∂y 2 ∂y 3 t2 ∂ 1 ∂ δy + δy L(y, y , t) dt + · · · + (4.13) 3! t1 ∂y ∂y since ∂F ∂F ∂F +s +t ∂x ∂y ∂z 2 ∂ ∂ ∂ 1 r +s +t F (x, y, z) + · · · . + 2! ∂x ∂y ∂z

F (x + r, y + s, z + t) ≈ F (x, y, z) + r

The quantity

δJ =

t2

t1

∂L ∂L

δy + (δy) dt ∂y ∂y

(4.14)

Hamilton’s principle

87

is called the ﬁrst variation while ∂ 2L ∂ 2 L 2 1 t2 ∂ 2 L 2

2 δy + 2 δy(δy) + 2 (δy ) dt δ J = ∂y∂y

2! t1 ∂y 2 ∂y is the second variation of J . If the ﬁrst variation is equal to zero for a particular function y(t) of the admissible class, the functional J (y) is said to have a stationary value for that particular function y. Before returning to equilibrium equations, let us look at one simple example to help understand the process of ﬁnding a stationary value. 4.2.1

Stationary value: minimizing the distance between two points

Figure 4.2 shows two points (x1 , y1 ) and (x2 , y2 ) which are joined by an inﬁnite number of possible paths, y(x). Only one is shown in the ﬁgure! Here note that y(x) is a function only of position, x, and not time. Our aim is to use the above approach to determine that path which minimizes the distance between the two points. An element of length dl lies on the path shown, and its length can be written as 2 dy 2 2 2 2 dl = dx + dy = dx 1 + dx such that

dl = (1 + y 2 )1/2 dx

and ﬁnally, we obtain the functional, or J integral as x2 J =l= (1 + y 2 )1/2 dx.

(4.15)

x1

Equation (4.15) is the functional which we wish to minimize to obtain the shortest path. We will use two approaches to do this. The ﬁrst is by obtaining directly the y

(x2, y2)

y (x) dl

dy dx

(x1, y1)

x1

x2

x

Fig. 4.2 A particular path, y(x), between two points, (x1 , y1 ) and (x2 , y2 ), and an element, dl, lying on the path.

88

Finite element method

stationary value of (4.15) and the second is to do the same by using the Euler–Lagrange Equation (4.11). The ﬁrst variation of (4.15) is given by x2 x2 1

2 1/2 (1 + y ) dx = (1 + y 2 )−1/2 δ(y 2 ) dx δJ = δ x1 x1 2 x2 = (1 + y 2 )−1/2 y δy dx. x1

Now,

dy d = (δy) δy = δ dx dx so x2 d δJ = (1 + y 2 )−1/2 y (δy) dx. dx x1 Integrating by parts gives x2 d ((1 + y 2 )−1/2 y ) δy dx δJ = [y (1 + y 2 )−1/2 δy]xx21 − dx x1 and since δy(x1 ) = δy(x2 ) = 0, and for a stationary value, we obtain x2 d ((1 + y 2 )−1/2 y ) δy dx = 0. δJ = − x1 dx Since δy is arbitrary, we obtain the differential equation d ((1 + y 2 )−1/2 y ) = 0, (4.16) dx which (unsurprisingly) has the solution y = Ax + B in which A and B are constants of integration. We see, therefore, that the process of ﬁnding the ﬁrst variation (or equivalently, the stationary value) of J , results in ﬁnding the function y(x) which minimizes the functional, J . To ﬁnish off, let us do the same thing but now using the Euler–Lagrange Equation (4.11). The functional, J , is a function of y, y , and x and from Equation (4.15) may be written as x2 J = L(y, y , x) dx,

where

L(y, y , x)

=

(1 + y 2 )1/2

x1

so the Euler–Lagrange equation becomes ∂L d ∂L − = 0. ∂y dx ∂y

(4.17)

Now, ∂L ∂L 1 = 0 and = (1 + y 2 )−1/2 2y

∂y ∂y 2 and substituting into (4.17) just gives us the differential Equation (4.16) which has the solution as before.

Hamilton’s principle

4.2.2

89

Equilibrium equations

Let us now return to Hamilton’s principle to see how it can be used to obtain equilibrium equations. For a solid elastic body, in the absence of body forces, the components of the Lagrangian can be expressed as follows: 1 T = ρ u˙ · u˙ dV , 2 1 σ : ε dV , (4.18) U= 2 t · u dA W = ∂

in which u and u˙ are the displacement and velocity vectors, ρ the density, t the stress vector, or traction, σ and ε the stress and strain tensors respectively, and ∂ and are domains of area, A and volume, V , respectively. Substituting for the stress vector, t, from Equation (3.66), and making use of the divergence theorem gives W = σ n · u dA = div [σ u] dV . (4.19) ∂

The J integral is, therefore t2 (T − U + W ) dt J = t1 t2

=

t1

1 1 ρ u˙ · u˙ dV − σ : ε dV + div [σ u] dV dt. 2 2

Taking the ﬁrst variation of J gives t2 δJ = δ(T − U + W ) dt t1 t2

1 1 2ρ u˙ · δ u˙ dV − (σ : δε + δσ : ε) dV + div [σ δu] dV dt = 2 2 t1 t2 ∂ ρ u˙ · δu dV − σ : δε dV + div [σ δu] dV dt = 0 = ∂t t1

and noting that div [σ δu] = div [σ ] · δu + σ : ∇δu and ∇δu = δε and integrating by parts gives t2 δJ = − ρ u¨ · δu dV + div σ δu dV dt t1 t2

=

t1

− ρ u¨ dV + div σ dV · δu dt = 0

90

Finite element method

so that

(−ρ u¨ + div σ ) · δu dV = 0

(4.20)

and since δu is arbitrary, −ρ u¨ + div σ = 0. These are the well-known equilibrium equations of stress analysis. If we consider quasi-static conditions, ρ u¨ = 0, and expand div σ , we obtain the more familiar expressions ⎡ ⎤ ∂σxy ∂σxx ∂σxz + + ⎢ ∂x ∂y ∂z ⎥ ⎢ ⎥ ⎢ ∂σ ∂σyy ∂σyz ⎥ ⎢ yx ⎥ + + div σ = ⎢ ⎥ = 0. ⎢ ∂x ∂y ∂y ⎥ ⎢ ⎥ ⎣ ∂σzx ∂σzy ∂σzz ⎦ + + ∂x ∂y ∂z Hamilton’s principle has therefore given us the very general form of the equilibrium equations of stress analysis. In addition, Equation (4.20) can be seen to be a statement ! of the principle of virtual work. The term (−ρ u¨ + div σ ) dV is just the residual force, r, so that the expression in (4.20) is simply δW = r · δu = 0. That is, in the course of an arbitrary, inﬁnitesimal virtual displacement, δu, from a position of equilibrium, the work done is zero. Hamilton’s principle has therefore provided us with the condition for equilibrium and, in doing so, a statement of the principle of virtual work. Before moving on to its application to ﬁnite elements, let us consider a few more examples, one for a discrete system, and two further continuous systems, in which we shall employ Hamilton’s principle to obtain the momentum balance equations for a number of simple problems. 4.2.3

Further examples of Hamilton’s principle

4.2.3.1 Discrete spring–mass problem. Consider the SDOF spring–mass system shown in Fig. 4.3. We will use Hamilton’s principle to derive the equation of motion for the mass, m. k

m

x(t )

Fig. 4.3 Simple SDOF mass and spring system.

Hamilton’s principle

91

We may write expressions for the kinetic and potential energies of the system as 1 1 T = mx˙ 2 . U = kx 2 , 2 2 The J integral may then be written, in the absence of external forces, as t2 t2 1 2 1 2 J = mx˙ − kx dt. (T − U ) dt = 2 2 t1 t1 Taking the ﬁrst variation gives t2 d 1 t2 mx˙ (δx) − kx δx dt (2mx˙ δ x˙ − 2kx δx) dt = δJ = 2 t1 dt t1 and integrating by parts, we get δJ =

[mx˙ δx]tt21

−

t2 t1

(mx¨ δx + kx δx) dt

and since δx(t1 ) = δx(t2 ) = 0, and δx is arbitrary, t2 δJ = − (mx¨ + kx) δx dt = 0 so mx¨ + kx = 0. t1

Hamilton’s principle has given us the governing equation of motion, or equilibrium equation, for the well known mass–spring problem. 4.2.3.2 Transverse vibration of a continuous beam. We shall next consider a continuous system and use Hamilton’s principle to obtain the equations of motion for it. Figure 4.4(a) shows an elastic beam undergoing bending with deﬂection, y. The bending moment variation with angle, φ, is shown in Fig. 4.4(b) assuming elastic behaviour. (b) M

(a) y

y

f+

−f −x dU =

f x

df

1 M df 2 f

Fig. 4.4 (a) An elastic beam in bending undergoing deﬂection y and rotation φ and (b) the linear variation of bending moment M with rotation φ leading to stored elastic strain energy U .

92

Finite element method

The elastic strain energy stored in an element of length dx of the beam is 1 1 ∂φ dU = M dφ ≈ M dx 2 2 ∂x and ∂y φ= ∂x so that 1 ∂ 2y dU = M 2 dx. 2 ∂x For an elastic beam, the bending moment is related to the deﬂection, y, by ∂ 2y , ∂x 2 where E is Young’s modulus and I is the second moment of area. Thus, 2 2 1 ∂ y dU = EI dx 2 ∂x 2 and ﬁnally, the potential energy for a beam of length L is 2 2 1 L ∂ y U= EI dx. 2 0 ∂x 2 The kinetic energy, in an element of length dx, of the beam, is 2 1 ∂y dT = ρA dx 2 ∂t in which A is the beam’s cross-sectional area. Hence the total system energy is 2 1 L ∂y T = ρA dx. ∂t 2 0 The work done by external forces, F (x, t) per unit length, is given by L F (x, t)y dx. W = M = EI

(4.21)

kinetic (4.22)

(4.23)

0

Consider the simply supported beam undergoing transverse vibration shown in Fig. 4.5. We apply Hamilton’s principle in the usual way. The J integral is t2 L dt J = t1

1 = 2

t2

t1

"

L 0

∂y ρA ∂t

2

L

dx − 0

EI

∂ 2y ∂x 2

2

L

dx + 0

# F (x, t)y dx dt.

Hamilton’s principle

93

F (x, t)

dx

Fig. 4.5 A simply supported beam with distributed load F (x, t) in transverse vibration.

We take the ﬁrst variation of J to give the stationary value and equate to zero t2 δJ = δL dt = 0. t1

Let us take the variation term by term. The contribution from the work done by external forces is obtained by substituting from (4.23) to give t2 L t2 δW dt = F (x, t) δy dx dt. t1

t1

0

The kinetic energy term, substituting for (4.22), is L 2 t2 ∂y 1 t2 δT dt = ρAδ dx dt 2 t1 ∂t 0 t1 L 1 t2 ∂y ∂y = δ dx dt ρA 2 2 t1 ∂t ∂t 0 t2 L ∂y ∂y = δ dx dt ρA ∂t ∂t 0 t1 t2 L ∂y ∂ = ρA δy dx dt 0 ∂t ∂t t1 # t2 t2 L " ∂y ∂ 2y δy − δy 2 dt dx = ρA ∂t ∂t 0 t1 t1 but δy(t1 ) = δy(t2 ) = 0 thus

t2

t1

δT dt = −ρA 0

L t2 t1

δy

∂ 2y dt dx. ∂t 2

94

Finite element method

The elastic strain energy term is, using (4.21),

t2 t1

1 δU dt = 2

= EI

t2

δ

t1

t2

t1

L

EI

∂ 2y ∂x 2

∂ 2y

∂2

0 L 0

∂x 2 ∂x 2

2

dx dt =

t2

t1

L 0

2 EI ∂ 2 y ∂ y 2 2δ dx dt 2 ∂x ∂x 2

δy dx dt

# ∂ 3y ∂ δy dx dt = EI − 3 0 ∂x ∂x t1 0 # L L 4 L 3 t2 " 2 ∂ y ∂ y ∂ ∂ y δy + δy dx dt. δy − = EI 4 ∂x 2 ∂x ∂x 3 0 ∂x t1 0 0

t2

"

∂ 2y ∂ δy ∂x 2 ∂x

L

L

Finally, summing the terms,

∂ 4y ∂ 2y δJ = − EI 4 + ρA 2 δy dx dt ∂x ∂t 0 t1 L # L 3 t2 L t2 " 2 ∂ y ∂ y ∂ δy F (x, t) δy dx dt dt + δy + − EI ∂x 2 ∂x ∂x 3 0 t1 t1 0 0 t2 L ∂ 4y ∂ 2y = − EI 4 + ρA 2 − F δy dx dt ∂x ∂t 0 t1 " L # L 3 t2 2 ∂ y ∂ y ∂ δy dt = 0. (4.24) δy − + EI ∂x 2 ∂x ∂x 3 t1 0 0

t2

L

For δJ to be zero the integrands between 0 and L must be zero and since δy is arbitrary it follows that the individual terms in (4.24) must also vanish so that (assuming uniform, constant transverse loading, F ), EI

∂ 4y ∂ 2y + ρA =F ∂x 4 ∂t 2

and in addition, the boundary conditions are ∂ 2y ∂ δy = 0 for x = 0 and x = L, ∂x 2 ∂x ∂ 3y δy = 0 for x = 0 and x = L, ∂x 3

(4.25)

Hamilton’s principle

95

which means either

∂ 2y =0 ∂x 2

∂ δy = 0 ∂x

or

for x = 0 and x = L

and

(4.26)

either

∂ 3y =0 ∂x 3

δy = 0

or

for x = 0 and x = L.

Equation (4.25) is the equilibrium equation for the vibrating beam problem. However, note that Hamilton’s principle has also given us the boundary conditions for the problem in Equations (4.26). We shall ﬁnish by looking at one further example. 4.2.3.3 Transverse vibration of a beam with axial loading. We shall now consider the previous problem but with the addition of an externally applied axial force, P , as shown in Fig. 4.6. The axial force does work as the beam shortens due to transverse displacement (here, we are ignoring axial displacement which results from the axial strain due to the force, P ). An element of the beam, ds, shortens by $ ds − dx = dx 2 + dy 2 − dx = =

⎧% ⎨ ⎩

1+

dy dx

2

%

1+

⎫ ⎬

dy dx

1 − 1 dx ≈ ⎭ 2

2 dx − dx ∂y ∂x

2 dx.

The work done by the axial force per differential length 1 dWP = P 2

∂y ∂x

2 dx.

F (x, t ) P

P

dy

ds

dx

dx

Fig. 4.6 Simply supported beam subjected to axial force P while undergoing transverse vibration.

96

Finite element method

The ﬁrst variation of the work done by external forces then becomes 2 t2 L t2 ∂y 1 F (x, t) δy + δP dx dt δW dt = 2 ∂x 0 t1 t1 t2 L ∂y ∂ δy dx dt F (x, t) δy + P = ∂x ∂x 0 t1 L # t2 L " ∂y ∂ 2y δy F (x, t) δy − P 2 δy dx + P dt. = ∂x ∂x 0 t1 0 Thus, for uniform transverse loading F (x, t) = F , the equilibrium equation becomes ∂ 2y ∂ 2y ∂ 4y + P + ρA =F ∂x 4 ∂x 2 ∂t 2 and the boundary conditions are EI

∂ 2y ∂ δy = 0 for x = 0 and x = L, ∂x 2 ∂x ∂ 3y ∂ 2y EI 3 + P 2 = 0 for x = 0 and x = L, ∂x ∂x which means either

∂ 2y =0 ∂x 2

either

EI

or

∂ δy = 0 ∂x

for x = 0 and x = L

and

4.3

∂ 2y ∂ 3y + P =0 ∂x 3 ∂x 2

or

δy = 0

for x = 0 and x = L.

Introduction to the ﬁnite element method

In this section, we will make use of Hamilton’s principle to obtain ﬁnite element equilibrium equations which we shall then apply to some simple, uniaxial problems, before considering some further ﬁnite elements, and their application in statics and dynamics. We shall start with an introduction to the ﬁnite element method. Figure 4.7 shows a representation of an undeformed body when the value of time is zero, which has been discretized into a ﬁnite number of tetrahedral ﬁnite elements which approximate the initial geometry of the body. A particular, single ﬁnite element is shown which has nodes at points P1 , P2 , P3 , and P4 in the undeformed conﬁguration. On the application of a load (which may be mechanical or thermal, for example), the body deforms (and undergoes

Introduction to the ﬁnite element method

97

Z, z F

Time = t Y, y p3 Time = 0

F

P3

X, x

P2

P4

p2

p4 p1

P1

Fig. 4.7 Schematic diagram showing the ﬁnite element discretization of a body with three-dimensional tetrahedral elements.

transformation ) to that shown in the current conﬁguration at time t. The nodes of the single element, after deformation, are now located at p1 , p2 , p3 , and p4 . For simplicity, let us suppose that the quantity we are interested in determining is temperature, chosen because it is a scalar variable. The basis of the ﬁnite element method is to assign nodes to the elements and to assume that we can determine shape functions to enable interpolation to give the value of the temperature at any point within the element in terms of the nodal values of temperature. The tetrahedral element shown in the ﬁgure has four nodes. If the temperatures at the four nodes are θ1 , θ2 , θ3 , and θ4 respectively, then the temperature anywhere within the element is given by n Ni θi , (4.27) θ = N1 θ1 + N2 θ2 + N3 θ3 + N4 θ4 = i=1

where Ni are called shape (or interpolation) functions. Let us consider in isolation the element shown in Fig. 4.7 in the deformed conﬁguration. The element is shown in Fig. 4.8(a) with respect to the current conﬁguration, and in (b) with respect to a local element reference frame (ξ1 , ξ2 , ξ3 ). A transformation is clearly needed to map the element from the local reference frame to the current conﬁguration, and similarly, from the local reference frame to the original conﬁguration, and we shall address this later. The shape functions for this element, in terms of the local variables, are N1 (ξ1 , ξ2 , ξ3 ) = 1 − ξ1 − ξ2 − ξ3 , N2 (ξ1 , ξ2 , ξ3 ) = ξ1 , N3 (ξ1 , ξ2 , ξ3 ) = ξ2 , N4 (ξ1 , ξ2 , ξ3 ) = ξ3 .

98

Finite element method (a)

(b)

j3

x3

4 4 1 1 2

2

3 x2

x1

3 j2

j1

Fig. 4.8 Four-noded tetrahedral element shown with respect to (a) the current conﬁguration and (b) the local element reference frame.

An important feature of the shape functions in the ﬁnite element method is that they generally take a value of unity at their own node and are zero at all others; at node 1, for example, ξ1 = ξ2 = ξ3 = 0, so N1 = 1. They generally sum to unity: N1 + N2 + N3 + N4 = 1; there are however, some special elements for which this is not the case. With knowledge of position (ξ1 , ξ2 , ξ3 ) within an element, the shape functions can be used together with Equation (4.27) to determine the value of the temperature at any point within the element, given the nodal temperatures. The shape functions may be used in a similar way for any variable of interest, but often, the ﬁnite element equilibrium equations are set up with displacement as the basic quantity for which solutions are obtained. Such an approach is often referred to, therefore, as the displacementbased ﬁnite element method. We will look at a further, very simple ﬁnite element in order to examine the displacement-based approach. Figure 4.9 shows a uniform bar under axial force P which has been discretized with a number of uniaxial truss elements. Each element has two nodes and is of length L. Each node has just one degree of freedom; namely axial displacement, u. The bar lies along the x-direction in the current conﬁguration. The shape functions are N1 (ξ ) = 1 − ξ,

N2 (ξ ) = ξ,

(4.28)

where ξ = x/L and 0 ≤ ξ ≤ 1, and the element displacements are given by u(ξ ) = N1 u1 + N2 u2 . This is often written in vector form as u(ξ ) = N uI = [N1

u1 . N2 ] u2

(4.29)

Introduction to the ﬁnite element method

99

P x

P

u2

L

x u1 N2 1

N1 1

N1(j) = 1– j

1

j N2(j) = j

1

j

Fig. 4.9 A uniform bar discretized using uniaxial truss elements with shape functions shown.

Because we know the displacement everywhere within the element, we can determine the small strain, which, for this simple, uniaxial displacement is just ∂N1 ∂ξ ∂u ∂N1 ∂N2 u1 ε= = = ∂ξ ∂x ∂x ∂x ∂x u2 u1 1 . = [−1 1] L u2

∂N2 ∂ξ ∂ξ ∂x

u

1

u2 (4.30)

The derivatives of the type ∂ξ /∂x relate the current conﬁguration to the local element reference frame and, in effect, provide the mapping of the element from the current conﬁguration to the local element reference frame. In this case, because ξ = x/L, the mapping is trivial and the derivatives ∂ξ /∂x are easily obtained. We will see how to do this for more general cases a little later. The matrix of spatial derivatives of the shape functions, given in Equation (4.30), is often referred to as the B matrix where for this particular element, B=

1 [−1 L

1].

(4.31)

It can be seen from (4.30) that the strain is constant everywhere within the element; it is an example (as is the four-noded tetrahedran above) of a constant strain element. In order to progress with the analysis of the loaded bar, we need to obtain the equations of motion or equilibrium. We shall do this in a general way using Hamilton’s principle, and then return to the loaded bar and to uniaxial truss elements.

100

Finite element method

4.4

Finite element equilibrium equations

4.4.1

Some preliminaries: tensor and Voigt notation, tensorial versus engineering strain

Tensorial notation is very elegant when it comes to theoretical derivations. However, for the purposes of developing numerical algorithms for implementation into computer programs, it is often more practical to work with arrays thus representing second-order tensor (strain, stress) as one-dimensional arrays and constitutive tensors (the elasticity tensor) as two-dimensional arrays. Symmetry of stress and strain tensors is used to obtain the following (memory saving) notation (Voigt notation): ⎡ ⎤ σxx ⎢ ⎥ ⎢σyy ⎥ ⎡ ⎤ ⎢ ⎥ σxx σxy σxz ⎢σ ⎥ ⎢ ⎥ ⎢ zz ⎥ σ = ⎣σxy σyy σyz ⎦ → σ = ⎢ ⎥ , (4.32) ⎢σxy ⎥ ⎢ ⎥ σxz σyz σzz ⎢σ ⎥ ⎣ yz ⎦ σxz ⎡ ⎤ ⎡ ⎤ εxx εxx ⎢ε ⎥ ⎢ ⎥ ⎢ yy ⎥ ⎢ εyy ⎥ ⎡ ⎤ ⎢ ⎥ ⎢ ⎥ εxx εxy εxz ⎢ εzz ⎥ ⎢ ε ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ zz ⎥ ε = ⎣εxy εyy εyz ⎦ → ε = ⎢ ⎥ = ⎢ (4.33) ⎥. ⎢γxy ⎥ ⎢2εxy ⎥ ⎢ ⎥ ⎢ ⎥ εxz εyz εzz ⎢γyz ⎥ ⎢2ε ⎥ ⎣ ⎦ ⎣ yz ⎦ γzx 2εzx Note that in vector, or Voigt notation, the shear strain components are stored as engineering shears, that is, twice the tensor shears. This sometimes causes confusion, so let us clarify by recalling Hooke’s law. Writing stress and elastic strain as column vectors, Hooke’s law in three dimensions becomes ⎤ ⎡ ⎤⎡ ⎡ ⎤ λ + 2µ λ λ 0 0 0 εxx σxx ⎥ ⎢ ⎥⎢ ⎢ ⎥ ⎢ λ ⎢ εyy ⎥ λ + 2µ λ 0 0 0⎥ ⎢σyy ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎥⎢ ⎢ ⎥ ⎢ ⎥ ⎢ λ λ λ + 2µ 0 0 0 ⎥ ⎢ εzz ⎥ ⎢ σzz ⎥ ⎥ ⎢ ⎢ ⎥ ⎥, ⎥⎢ σ = ⎢ ⎥ = Cε = ⎢ (4.34) ⎥ ⎢ ⎥ ⎢ γ 0 0 0 µ 0 0 ⎢σxy ⎥ xy ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎥⎢ ⎢ ⎥ ⎢ 0 ⎥ ⎢ γyz ⎥ ⎢ σyz ⎥ 0 0 0 µ 0 ⎥ ⎢ ⎥⎢ ⎣ ⎦ ⎦ ⎣ ⎦⎣ γ 0 0 0 0 0 µ xz σxz

Finite element equilibrium equations

101

where λ = Eν/(1 + ν)(1 − 2ν) and µ = G = E/2(1 + ν) are the Lame constants. Let us take one of the shear terms, for example, σxy = µγxy ≡

E γxy . 2(1 + ν)

We will now obtain the same shear stress, this time using the relation, given in Equation (2.99), that is, ⎛ ⎞ σxx σxy σxz ⎜ ⎟ ⎟ σ =⎜ ⎝σxy σyy σyz ⎠ = 2Gε + λTr(ε)I σxz σyz σzz ⎞ ⎛ ⎛ 1 εxx εxy εxz ⎟ ⎜ ⎜ ⎟ ⎜ = 2G ⎜ ⎝εxy εyy εyz ⎠ + λ(εxx + εyy + εzz ) ⎝0 εxz εyz εzz 0

(4.35) stress–strain tensor

0

0

⎞

1

⎟ 0⎟ ⎠.

0

1

The shear stress is, therefore, σxy = 2Gεxy ≡

E εxy . (1 + ν)

(4.36)

Comparison of (4.35) and (4.36) shows that we must have γxy = 2εxy and similarly for the other shear strains. A more elegant explanation of this is as follows. Let us consider the case of pure elastic shear, as described by the stress and strain tensors ⎛ ⎞ ⎛ ⎞ 0 σxy σxz 0 εxy εxz ⎜ ⎟ ⎜ ⎟ ⎟ σ =⎜ ε=⎜ 0 σyz ⎟ ⎝σxy ⎠, ⎝εxy 0 εyz ⎠ . σxz σyz 0 εxz εyz 0 The elastic strain energy per unit volume is given by the tensor product ⎛ ⎞ ⎛ ⎞ 0 σxy σxz 0 εxy εxz ⎟ ⎜ ⎟ 1⎜ 1 σ :ε= ⎜ :⎜ σxy 0 σyz ⎟ εxy 0 εyz ⎟ ⎝ ⎠ ⎝ ⎠ = (σxy εxy + σyz εyz + σxz εxz ) 2 2 σxz σyz 0 εxz εyz 0 and substituting for the shear stresses using (4.36) and similar expressions gives E 1 2 2 (ε 2 + εyz + εxz ). σ :ε= 1 + ν xy 2

(4.37)

102

Finite element method

We can also calculate the strain energy using engineering shear strain as 1 (τxy γxy + τyz γyz + τxz γxz ) 2 E 1 2 2 2 2 2 (γ 2 + γyz + γyz + γxz )= + γxz ). = G(γxy 4(1 + ν) xy 2

(4.38)

Comparison of (4.37) and (4.38), given that the three shear strains are independent, gives γxy = 2εxy as before, and similarly for the other shear strains. The strain tensor is, of course, an objective quantity; that is, one that satisﬁes the criteria for objectivity discussed in Chapter 3, and this means a quantity whose properties remain unchanged under rotation. We must therefore use the tensorial shear strain components (as opposed to the engineering shear) when rotating a strain. It might be of interest to note that it is for this reason that Mohr’s circle for strain is drawn in terms of γxy /2(= εxy ) rather than γxy . We write the dot product of two ﬁrst-order tensors, or vectors, as uT · v = ui vi = v T · u = vi ui =

n i=1 n

ui vi , vi ui

i=1

so that v T · u = uT · v. If, therefore, we calculate the product of the stress vector, for example, then from (4.32), σT · σ = (σxx

σyy

σzz

σxy

σyz

σxz ) · (σxx

σyy

σzz

σxy

σyz

σxz )T

2 2 2 2 2 2 = σxx + σyy + σzz + σxy + σyz + σxz .

It is important to note that this does not give the same result as the equivalent product of the stress tensor, which is 2 2 2 2 2 2 + σyy + σzz + 2(σxy + σyz + σxz ). σ : σ = σxx

It is therefore necessary to take care when using the vector (Voigt) notation for stress and strain in carrying out calculations. So, for example, the norm of σ , written |σ | is 2 2 2 2 2 2 1/2 + σyy + σzz + 2(σxy + σyz + σxz )] |σ | = (σ : σ )1/2 = [σxx

Finite element equilibrium equations

but if we work from the stress written as a column vector, then |σ | = σT Sσ, which includes the following scaling matrix ⎡ 1 0 0 ⎢ ⎢0 1 0 ⎢ ⎢ ⎢0 0 1 S=⎢ ⎢0 0 0 ⎢ ⎢ ⎢0 0 0 ⎣ 0 0 0

0

0

0

0

0

0

2

0

0

2

0

0

0

⎤

⎥ 0⎥ ⎥ ⎥ 0⎥ ⎥. 0⎥ ⎥ ⎥ 0⎥ ⎦ 2

The following are further examples of possible dangers in using Voigt notation: 1. Second invariant of deviatoric stress in tensorial notation 1 J2 = σ : σ

2 and its correct expression in Voigt notation 1 J2 = σ T Sσ . 2 2. Gradient of J2 invariant in tensorial notation ∂J2 = σ

∂σ

and its correct expression in Voigt notation ∂J2 = Sσ . ∂σ

3. Strain norm in tensorial notation √ |ε| = ε : ε and its correct expression in Voigt notation |ε| = εT S −1 ε, ⎡

where

S −1

1

⎢ ⎢0 ⎢ ⎢ ⎢0 =⎢ ⎢0 ⎢ ⎢ ⎢0 ⎣ 0

0

⎤

0

0

0

0

1

0

0

0

0

1

0

0

0

0

1 2

0

0

0

0

1 2

⎥ 0⎥ ⎥ ⎥ 0⎥ ⎥. 0⎥ ⎥ ⎥ 0⎥ ⎦

0

0

0

0

1 2

103

104

4.4.2

Finite element method

Finite element equations using Hamilton’s principle

For the purposes of obtaining the ﬁnite element equilibrium equations, we shall conﬁne ourselves initially to small elastic deformation problems so that we will not need to worry about the kinematics of large deformations. We will address large deformations later. The components of the Lagrangian for a general body subject to tractions t are given in Equations (4.18) using tensorial notation. We shall write them, here, using Voigt notation for a particular (the ‘m’th) ﬁnite element as follows 1 Tm = ρ u˙ T u˙ dV , 2 1 εT σ dV , (4.39) Um = 2 uT t dA, Wm = ∂

in which all non-scalar quantities are represented as column vectors and in particular, the stress and strain vectors are given by Equations (4.32) and (4.33), respectively ˙ and similarly for and the engineering shear strains are used. Note that u˙ T u˙ ≡ u˙ · u, other vector quantities. For completeness, the displacement and traction vectors are given by ⎡ ⎤ ⎡ ⎤ ux tx ⎢ ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ u=⎢ ⎣uy ⎦ and t = ⎣ty ⎦ . uz tz Hooke’s law, from Equation (4.34), is written as σ = Cεe .

(4.40)

The displacement within the particular ﬁnite element may be written in terms of the nodal displacements, uI , as we did in (4.29) so that u = N uI

(4.41)

and the strains can be written, in general, in terms of the nodal displacements and the B matrix, as we did for the truss element in Equation (4.30), ε = BuI .

(4.42)

For the uniaxial truss element, ε becomes just the unaxial, scalar, strain ε, but for other element types (in two and three dimensions), the other strain components are needed. We shall see an example of this later.

Finite element equilibrium equations

105

In applying Hamilton’s principle, we shall start from the Lagrangian, Lm , for the single element 1 1 Lm = Tm − Um + Wm = Tm = ρ u˙ T u˙ dV − εT σ dV + uT t dA 2 2 ∂ and substituting Equations (4.40)–(4.42) gives 1 T 1 T T T T Lm = u˙ I ρN N dV u˙ I − uI B CB dV uI + uI N T t dA. 2 2 ∂ If we deﬁne element mass and stiffness matrices as ρN T N dV m=

(4.43)

and k=

and the vector of nodal forces as

B T CB dV

(4.44)

N T t dA,

(4.45)

f =

∂

then the Lagrangian becomes Lm =

1 T 1 u˙ I mu˙ I − uTI kuI + uTI f . 2 2

The J integral is, therefore t2 J = Lm dt = t1

t2

t1

1 T 1 T T u˙ mu˙ I − uI kuI + uI f dt 2 I 2

and applying Hamilton’s principle gives t2 1 1 T T T δJ = δ(u˙ I mu˙ I ) − δ(uI kuI ) + δ(uI f ) dt 2 2 t1 t2 δuTI (−mu¨ I − kuI + f ) dt = 0. = t1

Since δuI is an arbitrary displacement, this gives for the equilibrium equation, for a single ﬁnite element mu¨ I + kuI = f . (4.46) Equation (4.46) is the ﬁnite element equilibrium equation, or equation of motion, written in terms of nodal displacements, uI . In the absence of inertia forces, it reduces to the standard, quasi-static equation kuI = f .

(4.47)

106

Finite element method

Some authors differentiate between momentum balance equations and equilibrium equations; those that are derived which include inertia (dynamic) effects—for example, that given in (4.46)—are often referred to as momentum balance equations, and those which do not include inertia effects (for quasi-static problems), are simply called equilibrium equations. In most cases in what follows, we shall simply refer to both types as equilibrium equations. In Section 4.4.2.1, we shall determine the mass and stiffness matrices for a truss element and examine a single-element problem. 4.4.2.1 Single truss element problem. Consider the uniform bar with crosssectional area A, made of material with density ρ, and Young’s modulus E, shown in Fig. 4.10(a). This is discretized with a single, uniaxial truss element shown in Fig. 4.10(b). The shape functions are those given in (4.28), N1 (ξ ) = 1 − ξ,

N2 (ξ ) = ξ

so that N = [1 − ξ

ξ ].

From above, (4.31), the B matrix is B=

1 [−1 L

1].

The mass matrix can then be determined from (4.43) as L 1−ξ T m= ρN N dV = ρ [1 − ξ x=0 ξ

ξ ]A dx.

This integral is currently given with respect to the deformed conﬁguration, x, so it needs to be transformed to the local element reference frame, ξ . While trivial in this case, since ξ = x/L, in general we would need to obtain the Jacobian, mapping dV (or equivalently, dx) in the current conﬁguration to dV (or, dξ ) in the element reference

r, E, A P

r, E, A

1 L

x2 u2

x1 u1

(b)

(a)

2

L

Fig. 4.10 (a) A uniform bar under axial force, P , and (b) its discretization using a single truss element.

Finite element equilibrium equations

frame, as we shall see later. For now, however, 1 L 1 − ξ 1−ξ ρ [1 − ξ ξ ]A dx = ρ [1 − ξ m= x=0 ξ =0 ξ ξ 1 (1 − ξ )2 ξ(1 − ξ ) dξ = ρAL 0 ξ(1 − ξ ) ξ2 so

m = ρAL The stiffness matrix is, using (4.44) B T CB dV = k=

=

1

ξ =0

E L2

L

x=0

1 −1

−1 1

1 3 1 6

1 6 1 3

.

1 1 −1 E [−1 L 1 L

107

ξ ]AL dξ

(4.48)

1]A dx

AL dξ,

where in this simple uniaxial case, the elasticity matrix C is simply Young’s modulus, E, so

EA 1 −1 (4.49) k= L −1 1 and the nodal force vector, (4.45), for this problem is simply F1 f = P

(4.50)

in which P is just the prescribed force at node 2 and F1 the currently unknown reaction at node 1, and no integration over ξ is necessary. Note that because t is a traction (stress vector), t dA is the force acting on the area dA at nodes 1 and 2. The integration of dA at the two ends therefore just gives A and is independent of ξ , so that tA at node 2 is P and that at node 1 is F1 , both of which act in a direction parallel to t; that is, the x-direction. The equilibrium Equation (4.46) therefore gives 1 1

u¨ 1 F1 EA 1 −1 u1 6 3 + = ρAL . (4.51) 1 1 L −1 1 u ¨ u P 2 2 6 3 Let us assume inertia forces are negligible and that this is, therefore, a quasi-static problem so that we may eliminate the inertia term from (4.51) to give

F1 EA 1 −1 u1 = . L −1 1 u2 P

108

Finite element method

With the boundary condition that u1 = 0, these equations can be solved to give the expected result that PL u2 = , F1 = −P EA and using u = N uI , that 0 PL =ξ . u2 = [1 − ξ ξ ] EA u2 where 0 ≤ ξ ≤ 1. Despite using just a single element, these results are exact. This is only because, in this particular problem, we have been using a constant strain element to discretize what is, in any case, a constant strain problem. In the following section, we shall give a more general description of the ﬁnite element method which includes the kinematics of large deformations and recognizes that the displacement of the nodes can become large; the problem then becomes geometrically non-linear. In addition, we need to give a fuller description of the mapping process between the current (and original) conﬁguration and the local element reference frame. We will then look at several further examples. 4.4.3

General ﬁnite element approach

We will now return to the body in the initial and current conﬁgurations shown in Fig. 4.7. We will formulate the ﬁnite element equations with respect to the current, or deformed, conﬁguration. When carried out incrementally, this is usually called an updated Lagrangian formulation. An alternative is to set up the equations with respect to the original conﬁguration, in which case, it is called a total Lagrangian formulation. The initial position of the material particle P within the element shown can be speciﬁed as follows X(ξ , t) ≈

NNODE

NI (ξ )XI (t),

(4.52)

I =1

where NNODE denotes the number of ﬁnite element nodes, NI (ξ ) represents, as before, the element shape functions and X I indicates the initial positions of the ﬁnite element nodal points P I , which are given in terms of the local element reference, (ξ1 , ξ2 , ξ3 ) shown in Fig. 4.8. Assuming that the material particle P remains attached to the same ﬁnite elements during the motion, the current positions of the material particles at the time t are speciﬁed by x(ξ , t) ≈

NNODE I =1

NI (ξ )x I (t)

(4.53)

Finite element equilibrium equations

109

where x I (t) denotes the current positions of the ﬁnite element nodal points pI . In the example in Section 4.4.2.1, the displacements were assumed to be small and there were no rigid body rotations. X(ξ , t) and x(ξ , t) were therefore identical and in addition, because the element considered was one-dimensional, ξ in Equations (4.52) and (4.53) was simply the scalar ξ . For two-dimensional elements, for example, two local reference frame independent variables are needed, (ξ1 , ξ2 ), to specify position. For the previous truss element example, x(ξ , t) becomes x(ξ, t) ≈

2

NI (ξ )xI (t) = (1 − ξ )x1 (t) + ξ x2 (t).

(4.54)

I =1

Equation (4.54), and for the general case (4.53), therefore, maps any point within an element, speciﬁed by ξ with respect to the local element reference system, onto the corresponding position in the current conﬁguration. The displacement and the velocity ﬁelds within each ﬁnite element are approximated as follows u(ξ , t) ≈

NNODE

NI (ξ )uI (t),

(4.55)

NI (ξ )v I (t).

(4.56)

I =1

v(ξ , t) ≈

NNODE I =1

In Equations (4.52)–(4.55), the same shape functions are used for interpolating position and displacement. Elements for which this holds true are called isoparametric. The deformation gradient tensor is obtained by differentiating Equation (4.53) with respect to the initial conﬁguration as follows F (ξ , t) ≈

NNODE

x I (t) ⊗ ∇X NI (ξ , t),

(4.57)

I =1

∂NI (ξ ) ∂NI ∂NI ∂NI = (4.58) ∇ X NI (ξ , t) = ∂X(t) ∂X ∂Y ∂Z are the derivatives of the shape functions NI . The gradient term, ∇, and the dyadic product, ⊗, are explained in Appendix A. The derivative can be rewritten as follows ∂NI (ξ ) ∂NI (ξ ) ∂ξ ∂NI (ξ ) ∂X(t) −1 ∇X NI (ξ , t) = . (4.59) = = ∂X(t) ∂ξ ∂X(t) ∂ξ ∂ξ where

It is normally not possible to determine ∂ξ /∂X in Equation (4.59) directly since Equation (4.52) speciﬁes X in terms of ξ . It is therefore necessary to determine ∂X/∂ξ instead and obtain the inverse. The derivative ∂X/∂ξ is called the Jacobian and relates

110

Finite element method

inﬁnitesimal quantities in the material conﬁguration to those in the local element coordinate system. We shall see this in several examples later. Using Equation (4.52), ∂X ∂NI (ξ ) = XI (t), ∂ξ ∂ξ

(4.60)

where the members of ∂X/∂ξ are given by NNODE ∂NI ∂Xi . = XiI ∂ξj ∂ξj

(4.61)

I =1

The small strain tensor can be approximated NNODE 1 1 [∇u + (∇u)T ] ≈ [uI (t) ⊗ ∇X NI (ξ ) + ∇X NI (ξ ) ⊗ uI (t)]. 2 2 I =1 (4.62) The velocity gradient is obtained as the spatial derivative of the velocity in Equation (4.56) as NNODE L(ξ , t) ≈ v I (t) ⊗ ∇x NI (ξ , t)

ε(ξ , t) =

I =1

and the rate of deformation tensor is obtained by using D = (1/2)(L + LT ) as follows D(ξ , t) ≈

NNODE 1 (v I (t) ⊗ ∇x NI (ξ , t) + ∇x NI (ξ , t) ⊗ v I (t)), 2

(4.63)

I =1

where

∂NI (ξ ) (4.64) ∂x(t) are the spatial derivatives with respect to the current conﬁguration, and are obtained from the shape functions as ∂NI (ξ ) ∂NI (ξ ) ∂ξ ∂NI (ξ ) ∂x(t) −1 , (4.65) = = ∇x NI (ξ , t) = ∂x(t) ∂ξ ∂x(t) ∂ξ ∂ξ ∇x NI (ξ , t) =

where members of the Jacobian, ∂x/∂ξ , are given by NNODE ∂NI ∂xi = xiI . ∂ξj ∂ξj

(4.66)

I =1

We return now to the equilibrium Equation (4.20), obtained from Hamilton’s principle, but write the increment in virtual work per unit volume and per unit time as ¨ · δv dV = 0, (div[σ ] − ρ u) (4.67) δW =

Finite element equilibrium equations

111

where δv is an arbitrary virtual velocity in the current conﬁguration. By noting that div[σ · δv] = div[σ ] · δv + σ : ∇δv,

(4.68)

n · σ δv = δv · t

that ∇δv = δL and that because σ is symmetric, it can be shown (with a little algebra) that σ : δL = σ : δD, substituting into (4.67) with the application of the divergence theorem gives δW = ρ u¨ · δv dV + σ : δD dV − t · δv dA = 0. (4.69)

∂

The second term in the right-hand side of (4.69) is the internal work per unit volume per second. A stress quantity is called work conjugate to the strain if their double contracted tensor product yields work. The co-rotational Cauchy, or true, stress is work conjugate to the rate of deformation. The spatial virtual work equation, (4.69), which describes the dynamic equilibrium of the element can be rewritten in terms of the ﬁnite element discretization as follows

NNODE

NNODE δW ≈ NI u¨ I NI δv I dV ρ

I =1

+

−

1 (δv I ⊗ ∇ x NI + ∇ x NI ⊗ δv I ) dV 2 I =1 NNODE

t· NI δv I dA.

σ :

∂

I =1

NNODE

(4.70)

I =1

As σ is a symmetric tensor, this reduces to

NNODE

NNODE ρ NI u¨ I NI δv I dV δW ≈

I =1

+

σ :

I =1

NNODE

δv I ⊗ ∇x NI dV −

I =1

∂

t·

NNODE

NI δv I dA

I =1

and as the nodal virtual velocities are independent of the integration, this may be rewritten to give NNODE δW ≈ δv I · NIT ρ u¨ I [N1 , N2 , . . . , NNNODE ] dV I =1

+

NNODE I =1

δv I ·

σ ∇x NI dV −

NNODE I =1

δv I ·

NI t dA.

(4.71)

112

Finite element method

The virtual work equation can ﬁnally be written in vector form as dW ≈

NNODE

dv I · (f Iinert + f Iint − f Iext )

(4.72)

I =1

by introducing expressions for the equivalent element nodal force vectors as follows f Iinert = NIT ρ u¨I [N1 , N2 , . . . , NNNODE ] dV , (4.73) int σ ∇ x NI dV , (4.74) fI = ext NI t dA, (4.75) fI = ∂

where f Iinert , f Iint , and f Iext represent the inertial, the internal, and the external element nodal forces, respectively. Since the discretized rate of virtual work, Equation (4.72) must be satisﬁed for all cases of the arbitrary virtual velocities, the element equation can be rewritten f Iinert + f Iint − f Iext = 0.

(4.76)

The nodal forces can be further assembled into global vectors (column matrices) by summing over all elements to give ⎡ ⎡ ⎤ ⎤ ⎡ ext ⎤ f 1inert f 1int f1 ⎢ inert ⎥ ⎢ int ⎥ ⎢ ext ⎥ ⎢f 2 ⎥ ⎢f 2 ⎥ ⎢f 2 ⎥ ⎢ ⎢ ⎥ ⎥ inert int ext ⎢ F = ⎢ . ⎥, (4.77) F = ⎢ . ⎥, F =⎢ . ⎥ ⎥, ⎢ .. ⎥ ⎢ .. ⎥ ⎣ .. ⎦ ⎣ ⎣ ⎦ ⎦ f ninert

f nint

f next

where n is the total number of points used in the discretization. Finally, the ﬁnite element discretization can be expressed by the set of non-linear equilibrium equations as follows: Finert (u) + Fint (u) − Fext (u) = 0 (4.78) for the set (column matrix) of nodal displacements ⎡ ⎤ u1 (t) ⎢u (t)⎥ ⎢ 2 ⎥ ⎥ u=⎢ ⎢ .. ⎥ ⎣ . ⎦ un (t) at time t.

(4.79)

Finite element equilibrium equations

113

We can rewrite Equation (4.76) in a more familiar way by considering the internal work term and writing it in terms of Voigt notation. We will assume small strain elasticity for simplicity. Returning to Equation (4.69), the internal work term originates from I δW = σ : δD dV

and may be written using Voigt notation as σ : δD dV = δDT σ dV , δW I =

(4.80)

where DT = (Dxx

Dyy

Dzz

2Dxy

2Dyz

2Dzx )

in which the off-diagonal terms (shear terms) are doubled to satisfy work conjugacy as speciﬁed in (4.80). The rate of deformation is given in terms of nodal velocities in (4.63) by D=

NNODE 1 (v I ⊗ ∇x NI + ∇x NI ⊗ v I ). 2 I =1

After some algebra, this can be written in Voigt notation as ⎡ ∂N

⎤

I

0

⎢ ∂x ⎢ ⎡ ⎤ ⎢ Dxx ⎢ 0 ⎢ ⎢ ⎥ ⎢ ⎢ Dyy ⎥ ⎢ ⎢ ⎥ ⎢ ⎢ ⎥ NNODE ⎢ 0 NNODE ⎢ Dzz ⎥ ⎢ ⎢ ⎥ ⎢ D=⎢ B I · vI = ⎥= ⎢ ∂NI ⎢2Dxy ⎥ I =1 I =1 ⎢ ⎢ ⎥ ⎢ ∂y ⎢ ⎥ ⎢ ⎢2Dyz ⎥ ⎢ ⎣ ⎦ ⎢ ⎢ 0 2Dzx ⎢ ⎢ ⎣ ∂N

∂NI ∂y 0 ∂NI ∂x ∂NI ∂z

I

0

∂z

0

⎥ ⎥ ⎥ 0 ⎥ ⎥ ⎥ ⎥ ∂NI ⎥ ⎡vxI ⎤ ⎥ ⎢ ⎥ ∂z ⎥ ⎥ ⎢vyI ⎥ ⎥⎣ ⎦ 0 ⎥ ⎥ vzI ⎥ ⎥ ∂NI ⎥ ⎥ ∂y ⎥ ⎥ ∂NI ⎦ ∂x

(4.81)

so that from (4.80) the internal energy term becomes δW I =

δDT σ dV =

NNODE

I =1

T B I dv I

σ dV .

(4.82)

114

Finite element method

If we assume purely elastic small deformation, then from (4.34), we may write

T NNODE I B I dv I Cε dV δW =

=

I =1

NNODE

T B I δv I

C

NNODE

I =1

B J uJ

dV

J =1

⎞

⎛

so that

NNODE

δW I = δv TI ⎝

I,J =1

B TI CB J dV ⎠ uJ

(4.83)

since we may also write the small strains in terms of the nodal displacements as ⎡ ∂N ⎤ I 0 0 ⎢ ∂x ⎥ ⎢ ⎥ ⎤ ⎡ ⎢ ⎥ ∂N I εxx ⎢ 0 0 ⎥ ⎢ ⎥ ⎥ ⎢ ∂y ⎢ ⎥ ⎢ εyy ⎥ ⎢ ⎥⎡ ⎤ ⎥ ⎢ ∂N ⎢ ⎥ uxI I ⎥ NNODE ⎢ ⎢ ⎥ 0 0 NNODE ⎢ εzz ⎥ ⎢ ⎢ ⎥ ∂z ⎥ ⎥ ⎢ ⎢ ⎥ ⎢uyI ⎥. B I · uI = ε=⎢ ⎥= ⎢ ⎥ ⎣ ⎦ ∂N ∂N ⎢2εxy ⎥ I I I =1 I =1 ⎢ ⎥ ⎢ 0 ⎥ ⎢ ⎥ ⎥ ⎢ ∂x ⎢ ∂y ⎥ uzI ⎢2εyz ⎥ ⎢ ⎥ ⎦ ⎣ ⎢ ∂NI ∂NI ⎥ ⎢ 0 ⎥ 2εzx ⎢ ∂z ∂y ⎥ ⎢ ⎥ ⎣ ∂N ∂NI ⎦ I 0 ∂z ∂x Equation (4.83) can be written as δW I = δv TI kuI , where k=

NNODE I,J =1

B TI CB J dV .

(4.84)

When combined with (4.71) and considering an arbitrary virtual velocity, δv, gives mu¨ + ku = f

(4.85)

ku = f .

(4.86)

and for quasi-static problems, This equation, in general, is non-linear if the problem considered is geometrically non-linear. This is because the stiffness matrix, k, depends upon the B matrix which

Finite element equilibrium equations

115

contains the derivatives of the shape functions with respect to the spatial coordinates. In a geometrically non-linear problem, the spatial coordinates change so that the stiffness matrix also changes. For geometrically non-linear problems, Equation (4.86) therefore has to be solved incrementally, and at each increment, the stiffness matrix must be updated. In the following sections, we look at a number of small deformation (geometrically linear) examples including a two-element axial vibration problem in which element assembly is addressed, a single-element and two-element bending problem in which beam elements are introduced, and a single square element static elastic problem in which linear four-noded (quad) elements are introduced. 4.4.3.1 Axial vibration of a beam using two truss elements. The uniform bar shown in Fig. 4.11(a) undergoes axial vibration. It is discretized using two truss elements shown in Fig. 4.11(b). The truss element formulation, relative to the local element reference frame, is shown in Fig. 4.12. (a)

2 A ∂ u2 dx ∂t

, E, A

dx

P

P + ∂P dx ∂x

L

(b)

x1 u1

1

1 , E, A

x2

x3

u2

u3

2 , E, A

2

L/2

3

L/2

Fig. 4.11 A uniform bar undergoing axial vibration (a) shown schematically and (b) its discretization using two truss elements.

l=1 1

2

0

1

j

Fig. 4.12 Linear truss element formulation shown relative to the local element reference frame, ξ .

116

Finite element method

The shape functions are N1 = 1 − ξ,

N2 = ξ

and in this problem, the two elements are identical so that their mass and stiffness matrices, respectively, are the same. Also, because this is a problem in which the displacements are inﬁnitesimal, the current and original conﬁgurations are taken to be the same. We shall determine the mass and stiffness matrices for a single element, and then consider their assemblage. The mass matrix given by (4.43) with respect to the spatial (which in this case coincides with the material) coordinate system is m=

ρN N dV = T

L/2

X=0

ρN T NA dX

but of course, the shape functions are given with respect to the local element reference frame. Therefore, we write m=

L/2

X=0

= ρA

ρN N A dX = T

1

ξ =0

1

ξ =0

1−ξ [1 − ξ ξ

ρN T NA det(J ) dξ

ξ ] det(J ) dξ

(4.87)

in which J is the Jacobian, mapping the spatial coordinate system onto the local element reference frame. In this one-dimensional problem, the determinant of the Jacobian is just ∂X ∂ X1 ∂N1 ∂N2 X1 det(J ) = = , = [N1 N2 ] X2 ∂ξ X2 ∂ξ ∂ξ ∂ξ which is of the general form given in Equation (4.60). Using the shape functions, we obtain L L L X1 det(J ) = [−1 1] = = = |[−X1 + X2 ]| = 0 + X2 2 2 2 so that the element mass matrix becomes

1 2 ξ − ξ2 ρAL 1 1 − 2ξ + ξ ρAL 3 m= dξ = 1 2 2 ξ =0 ξ − ξ2 ξ2 6

1 6 1 3

.

(4.88)

Finite element equilibrium equations

Let us write the mass matrix for elements 1 and 2 as 2 1 1 m11 m111 m112 ρAL 3 6 = = , m m1 = 2 1 1 2 m121 m122 m221 6 3 then the global mass matrix is given by ⎤ ⎡1 ⎡ 1 m112 0 m11 3 L ⎢1 ⎥ ⎢ 1 1 2 2 M = ⎣m21 m22 + m11 m12 ⎦ = ρA ⎣ 6 2 0 m221 m222 0

1 6 2 3 1 6

0

m212 m222

⎤

1⎥ 6⎦ 1 3

ρAL = 2 ⎡

=

1 6 ⎢1 ρAL ⎣ 12

0

1

1 12 1 3 1 12

117

1 6 1 3

3 1 6

0

,

⎤

1⎥ 12 ⎦ . 1 6

(4.89) The element stiffness matrix is given by (4.44) in terms of the spatial coordinates by L T B CB dV = B T CBA dX. k=

X=0

Introducing again the Jacobian in (4.87), the integral can be written with respect to the local element reference frame by 1 1 L T k= B CBA det(J ) dξ = B T CBA dξ . 2 ξ =0 ξ =0 Because the truss elements are one-dimensional, the elasticity matrix, C, becomes just the scalar Young’s modulus, E, so EAL 1 k= B T B dξ . 2 ξ =0 The B matrix contains the derivatives of the shape functions with respect to the spatial coordinates. We are assuming small displacements, however, and that the problem remains geometrically linear so that the spatial and material coordinates remain the same. Hence, ∂N1 ∂ξ ∂N2 ∂ξ ∂N1 ∂N2 ∂N1 ∂N2 B= ≡ = . ∂ξ ∂X ∂ξ ∂X ∂x ∂x ∂X ∂X In general, ∂ξ /∂X cannot be determined directly, since we ordinarily know X in terms of ξ . In its most general form, the relationship is given by (4.52), and for the truss element in this problem, this is X X = [N1 N2 ] 1 . X2 We have already determined the Jacobian derivative, in (4.87), and note that this is the inverse of ∂ξ /∂X. That is, therefore, −1 ∂ξ ∂X −1 L 2 −1 = =J = = . ∂ξ 2 L ∂X

118

Finite element method

In general, therefore, the derivatives needed for the B matrix are obtained from the inverse of the Jacobian. The B matrix is, therefore, ∂N1 ∂ξ ∂N2 ∂ξ 2 2 2 B= = [−1 1] = −1 × 1× ∂ξ ∂X ∂ξ ∂X L L L so that the element stiffness matrix becomes 2 EAL 1 2 2EA 1 −1 k= [−1 1] dξ = 1 2 L −1 ξ =0 L

−1 . 1

(4.90)

As for the mass matrices, we write the stiffness matrices for the two elements as 1 2 2 1 k11 k12 k11 k12 2EA 1 −1 2EA 1 −1 = = , k2 = k1 = 1 1 2 2 L −1 1 L −1 1 k21 k22 k21 k22 so that the global stiffness matrix become ⎡ ⎤ 1 1 ⎡ k11 k12 0 1 ⎢ 1 ⎥ 2EA 1 + k2 2 ⎥= ⎣−1 K=⎢ k k k 22 11 12 ⎦ ⎣ 21 L 0 2 2 0 k21 k22

−1 2 −1

⎤ ⎡ 0 2 EA ⎣−2 −1⎦ = L 1 0

−2 4 −2

⎤ 0 −2⎦ . 2

(4.91) The ﬁnite element equilibrium equation, given in (4.46) and (4.85) then becomes Mu¨ + Ku = 0 so

⎡

1 6 ⎢1 ⎢ ρAL ⎣ 12

0

⎤

⎡ ⎤ ⎡ u ¨ 2 1 ⎥ EA ⎣ 1 ⎥⎣ ⎦ −2 ¨2 + 12 ⎦ u L 0 u ¨ 3 1

1 12 1 3 1 12

0

−2 4 −2

⎤⎡ ⎤ ⎡ ⎤ u1 0 0 ⎦ ⎣ ⎦ ⎣ −2 u2 = 0⎦ . 0 2 u3

6

With the boundary condition u1 = 0, this reduces to 1 1 EA 4 −2 u2 u¨ 2 0 3 12 ρAL + = . 1 1 0 u¨ 3 u3 L −2 2 12

6

4.4.3.2 Cantilever beam in bending using a single element. The problem geometry and ﬁnite element discretization are shown in Figs 4.13 and 4.14. The Hermitian shape functions in the element local coordinate system (note that dx = L dξ ) are obtained as follows: N = a0 + a1 ξ + a2 ξ 2 + a3 ξ 3 .

Finite element equilibrium equations

119

r, E, A, I

L

Fig. 4.13 Cantilever beam of uniform section with second moment of area I .

v2

v1 u1

1

u1

r, E, A, I

1 x

2

L

Fig. 4.14 Single beam element discretization of a cantilever. The element has four degrees of freedom; two translational and two rotational.

First degree of freedom (y1 ) ⎫ dN1 ⎪ = 0⎪ ⎬ 1 dξ ⇒ N1 = 1−3ξ 2 +2ξ 3 . ⎪ dN1 ⎭ = 0⎪ ξ = 1, N1 = 0, 0 dξ

ξ = 0, N1 = 1,

1

j

1

j

Second degree of freedom (θ1 ) ⎫ dN2 ⎪ = 1⎪ ξ = 0, N2 = 0, ⎬ dξ ⇒ N2 = ξ −2ξ 2 +ξ 3 . ⎪ dN2 ⎭ = 0⎪ ξ = 1, N2 = 0, dξ

1 0

Third degree of freedom (y2 ) ξ = 0,

N3 = 0,

ξ = 1,

N3 = 1,

⎫ dN3 ⎪ = 0⎪ ⎬ dξ ⇒ N3 = 3ξ 2 −2ξ 3 . ⎪ dN3 ⎭ = 0⎪ dξ

1 0

1

j

120

Finite element method

Fourth degree of freedom (θ2 ) ξ = 0,

N4 = 0,

ξ = 1,

N4 = 0,

⎫ dN4 ⎪ = 0⎪ ⎬ dξ ⇒ N4 = −ξ 2 +ξ 3 . ⎪ dN4 ⎭ = 1⎪ dξ

1 0

1

j

We shall now apply Hamilton’s principle in order to obtain the ﬁnite element equilibrium equations. For a beam in bending, we may write the kinetic, T , and potential (strain), U , energies as 2 2 2 1 L 1 L ∂v ∂ v T = ρA dx, U= EI dx. 2 0 ∂t 2 0 ∂x 2 The ﬁnite element discretization is given by v(x, t) = N1 (ξ )v1 (t) + N2 (ξ )θ1 (t) + N3 (ξ )v2 (t) + N4 (ξ )θ2 (t) ∂v2 ∂v1 + N3 (ξ )v2 (t) + N4 (ξ ) ∂ξ ∂ξ ∂v1 ∂v2 + N3 (ξ )v2 (t) + N4 (ξ )L , = N1 (ξ )v1 (t) + N2 (ξ )L ∂x ∂x = N1 (ξ )v1 (t) + N2 (ξ )

which we shall write as v = Nu = [N1 (ξ )

N2 (ξ )

N3 (ξ )

N4 (ξ )] v1

∂v1 ∂x

v2

∂v2 ∂x

T .

The derivatives in the strain energy term are given by 1 ∂ 2v 1 ∂ 2 N1 ∂ 2 N2 ∂v1 ∂ 2 N3 ∂ 2 N4 ∂v2 ∂ 2v + = 2 2 = 2 v1 + L v2 + L ∂x 2 L ∂ξ L ∂ξ 2 ∂ξ 2 ∂x ∂ξ 2 ∂ξ 2 ∂x ⎤ ⎡ v1 ⎥ ⎢ ⎢ ∂v1 ⎥ ⎥ ⎢ ⎢ ∂x ⎥ 1 ∂ 2 N1 ∂ 2 N2 ∂ 2 N3 ∂ 2 N4 ⎥ = Bu. = 2 L L ⎢ ⎥ ⎢ L ∂ξ 2 ∂ξ 2 ∂ξ 2 ∂ξ 2 ⎢ v2 ⎥ ⎥ ⎢ ⎣ ∂v2 ⎦ ∂x The element kinetic and strain energies are given by L 1 L 1 T T T ˙ (N u) ˙ dx = u˙ T = ρA(N u) ρAN N dx u˙ 2 2 0 0

Finite element equilibrium equations

and

121

T 2 ∂ N ∂ 2N u u dx EI ∂ξ 2 ∂ξ 2 0 2 T 2 L ∂ N ∂ N 1 T dx u EI = u 2 2 ∂ξ ∂ξ 2 0 L 1 T T = u EI B B dx u. 2 0

1 U= 2

L

The element Lagrangian, L, is L=T −U = where

1 T 1 u˙ mu˙ − uT ku, 2 2

L

m=

(4.92)

ρAN T N dx

(4.93)

EI B T B dx.

(4.94)

0

and

k=

L

0

Integrating the Lagrangian with respect to time, and taking the ﬁrst variation gives mu¨ + ku = 0. The element mass matrix is ⎡ e ⎤ m11 me12 me13 me14 ⎢ e ⎥ e e e ⎥ ⎢m L m m m 22 23 24 ⎥ ⎢ 21 m=⎢ ρAN T N dx = ⎥ ⎢me me me me ⎥ 0 32 33 34 ⎦ ⎣ 31 me41 me42 me43 me44 ⎡ ⎤ 1 − 3ξ 2 + 2ξ 3 ⎥ 1⎢ ⎢(ξ − 2ξ 2 + ξ 3 )L⎥ ⎢ ⎥ = ρA ⎢ ⎥ 2 3 ⎢ ⎥ 0 − 2ξ 3ξ ⎣ ⎦ 2 3 (−ξ + ξ )L × 1 − 3ξ 2 + 2ξ 3 (ξ − 2ξ 2 + ξ 3 )L 3ξ 2 − 2ξ 3 ⎤ ⎡ 156 22L 54 −13L ρAL ⎢ 13L −3L2 ⎥ 4L2 ⎥. ⎢ 22L = 13L 156 −22L⎦ 420 ⎣ 54 −13L −3L2 −22L 4L2

. (−ξ 2 + ξ 3 )L L dξ

122

Finite element method

The element stiffness matrix is given by ⎡ e ⎤ e e e k13 k14 k11 k12 ⎢ e ⎥ e e e ⎥ ⎢k L ⎢ 21 k22 k23 k24 ⎥ k=⎢ = EI B T B dx ⎥ ⎢k e k e k e k e ⎥ 0 34 ⎦ 32 33 ⎣ 31 e e e e k41 k42 k43 k44 ⎡ ⎤ −6 + 12ξ ⎢ ⎥ 1 ⎥ 1 ⎢ 1 ⎢(−4 + 6ξ )L⎥ = ⎢ ⎥ EI 2 2 L 0 L ⎢ 6 − 12ξ ⎥ ⎣ ⎦ (−2 + 6ξ )L × [−6 + 12ξ (−4 + 6ξ )L 6 − 12ξ ⎤ ⎡ 12 6L −12 6L EI ⎢ 6L 4L2 −6L 2L2 ⎥ ⎥. = 3 ⎢ L ⎣−12 −6L 12 −6L⎦ 6L 2L2 −6L 4L2

(−2 + 6ξ )L]L dξ

The ﬁnite element equilibrium equation becomes ⎡ ⎤ ⎤ y¨1 156 22L 54 −13L ⎢ ⎥ 2 ⎢ θ¨ ⎥ ρAL ⎢ 13L −3L2 ⎥ 22L 4L ⎥ ⎢ 1⎥ ⎢ ⎥ 13L 156 −22L⎦ ⎢ 420 ⎣ 54 ⎣y¨2 ⎦ 2 2 −13L −3L −22L 4L θ¨2 ⎡ ⎤⎡ ⎤ ⎡ ⎤ 12 6L −12 6L y1 0 2 2 ⎢ ⎥ ⎢ ⎥ ⎢ EI 6L 4L −6L 2L ⎥ ⎢ θ1 ⎥ ⎢0⎥ ⎥. = + 3 ⎢ L ⎣−12 −6L 12 −6L⎦ ⎣y2 ⎦ ⎣0⎦ 0 6L 2L2 −6L 4L2 θ2 ⎡

With the boundary conditions v1 = 0 and θ1 = 0 at x = 0, the problem reduces to one with two degrees of freedom ρAL 156 −22L x¨2 EI 12 −6L x2 0 + 3 = . 2 2 ¨ −22L 4L −6L 4L 0 θ θ 420 L 3 3 4.4.3.3 Free transverse vibration of a propped cantilever using two beam elements. A uniform, propped cantilever beam is shown in Fig. 4.15 and its ﬁnite element discretization using two beam elements in Fig. 4.16.

Finite element equilibrium equations

123

r, E, A, I

L

Fig. 4.15 A uniform propped cantilever beam.

u1

1

y3

y2

y1 1 r, E, A, I

u2

2

u3

2 r, E, A, I

3

L /2

L /2

Fig. 4.16 Finite element discretization of a propped cantilever beam. The two beam elements are identical.

The element mass matrix (valid for both elements) is ⎡ 156

⎢ ⎢ ⎢ L ⎢ ⎢ 22 2 ρA(L/2) ⎢ ⎢ me = ⎢ 420 ⎢ ⎢ 54 ⎢ ⎢ ⎣ L −13 2

L 2 2 L 4 2 L 13 2 2 L −3 2

⎤ L 2 ⎥ 2 ⎥ L ⎥ ⎥ −3 ⎥ 2 ⎥ ⎥ L ⎥ ⎥ −22 ⎥ 2 ⎥ 2 ⎥ ⎦ L 4 2 −13

54

22

13

L 2

156 −22

L 2

and the stiffness matrix (valid for both elements) is ⎡ 12

⎢ ⎢ ⎢ ⎢ ⎢ 6L EI ⎢ ⎢ ke = (L/2)3 ⎢ ⎢−12 ⎢ ⎢ ⎢ ⎣ L 6 2

L 2 2 L 4 2 L −6 2 2 L 2 2 6

−12 −6

L 2

12 −6

L 2

⎤ L 2 ⎥ 2 ⎥ L ⎥ ⎥ 2 ⎥ 2 ⎥ ⎥. L ⎥ −6 ⎥ ⎥ 2 ⎥ 2 ⎥ L ⎦ 4 2 6

124

Finite element method

With the boundary conditions, we may write for the ﬁrst element ⎡

X

⎢ ⎡ ⎤ ⎡ ⎤ ⎢X y1 0 ⎢ ⎢ ⎢ θ1 ⎥ ⎢ 0 ⎥ EI ⎢ ⎥ = ⎢ ⎥ → k1 = u=⎢ ⎢ ⎣y2 ⎦ ⎣y2 ⎦ (L/2)3 ⎢X ⎢ ⎢ θ2 θ2 ⎣ X

X

X

X

X

X

12 −6

X

X

⎤

⎥ ⎥ ⎥ ⎥ L ⎥ −6 ⎥ 2 ⎥ ⎥ 2 ⎥ L ⎦ 4 2 X

L 2

and for element 2 that ⎡ ⎢ 12 ⎢ ⎡ ⎤ ⎡ ⎤ ⎢ y2 y2 ⎢ L ⎢6 ⎢θ2 ⎥ ⎢θ2 ⎥ EI ⎢ 2 ⎥ = ⎢ ⎥ → k2 = u=⎢ ⎢ ⎣y3 ⎦ ⎣ 0 ⎦ (L/2)3 ⎢ ⎢X ⎢ θ3 θ3 ⎢ ⎣ L 6 2

L 2 2 L 4 2 6

X 2 L 2 2

X X X X

⎤ L 2 ⎥ 2 ⎥ ⎥ L ⎥ ⎥ 2 2 ⎥ ⎥. ⎥ X ⎥ ⎥ 2 ⎥ L ⎦ 4 2 6

We proceed in a similar way for the mass matrix and obtain the ﬁnite element equilibrium equation Mu¨ + Ku = 0 to be ⎤ 13 ⎡ 156 0 − L ⎡ ⎤ ⎢ 4 ⎥ 172 ⎥ y¨2 ⎢ ⎥ ⎢ ⎥ EI ⎢ ρAL ⎢ 3 ⎢θ¨2 ⎥ + ⎢ ⎢ 0 L2 − L2 ⎥ ⎣ ⎦ L3 ⎣ 0 420 ⎢ 8 ⎥ ⎥ ⎢ ⎣ 13 24L 1 2 ⎦ θ¨3 3 L − L − L2 2 4 8 ⎡

0 16L2 4L2

⎤⎡ ⎤ ⎡ ⎤ y2 0 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢θ2 ⎥ = ⎢0⎥ . 4L2 ⎥ ⎦⎣ ⎦ ⎣ ⎦ 2 8L θ3 0

24L

4.4.3.4 Static analysis of a single square element. We will examine one further example before moving on; a single, two-dimensional, four-noded, isoparametric element subjected to a static force. We take the material behaviour to be elastic, and assume conditions of plane strain. The problem is shown schematically in Fig. 4.17, together with the elastic constants.

Finite element equilibrium equations

125

Geometry a = 1 mm 1

4

2

3

Material data E = 210 N / mm2 n = 0.25

a

Loading F = 10 N F

a

Discretization data (nodal coordinates) n1(0, 1), n2(0, 0), n3(1, 0), n4(1, 1)

45°

Fig. 4.17 Schematic diagram of a single, four-noded element subjected to force F directed at 45◦ to the vertical.

The shape functions for this element are as follows: Element local coordinate system 1 N1 (ξ, η) = (1 − ξ )(1 − η), h 4 1 4 3 N2 (ξ, η) = (1 + ξ )(1 − η), 1 4 1 N3 (ξ, η) = (1 + ξ )(1 + η), –1 1 4 j –1 1 N4 (ξ, η) = (1 − ξ )(1 + η). 1 2 4 We will ﬁnd that we need to carry out integrations (in order to obtain the stiffness matrix) of the shape functions. Previously, we have been able to do the integrations analytically. Here, we will need to use a numerical technique. Often, in order to simplify the process, the integration is carried out with respect to a particular point in the element; this point is known as an integration point. The integration will be performed numerically using a single integration point at P (ξ, η) = P (0, 0). Integrals over the element domain of the type I= f (ξ, η) dV

are expressed in the element local coordinate system by use of the Jacobian, J , as 1 1 I= f (ξ, η) det[J ] dξ dη, (4.95) −1 −1

where the Jacobian for a two-dimensional problem is given by ⎡ ∂X ∂X ⎤ ⎢ ∂ξ ∂η ⎥ ⎥ J =⎢ ⎣ ∂Y ∂Y ⎦ . ∂ξ

∂η

(4.96)

126

Finite element method

The integral in (4.95) will be approximated using Gauss quadrature (details may be found in any of the more specialized books on ﬁnite elements) by I≈

1

1

−1 −1

det[J ] dξ dη f (ξ, η).

The shape function derivatives at the integration point P (ξ, η) = P (0, 0) are obtained from ∂N ∂N ∂ξ ∂N ∂X −1 (4.97) = = ∂X ∂ξ ∂X ∂ξ ∂ξ and the shape function derivatives with respect to element local coordinates are given by ⎤ ∂N1 (0, 0) ∂N1 (0, 0) ⎥ ⎢ ∂ξ ∂η ⎥ ⎢ ⎡ ⎥ ⎢ (−1)(1 − η)|(0,0) ⎢ ∂N2 (0, 0) ∂N2 (0, 0) ⎥ ⎥ ⎢ ⎢ ⎥ 1 ⎢ (1)(1 − η)|(0,0) ∂ξ ∂η ∂N (0, 0) ⎢ ⎥= ⎢ =⎢ ⎥ 4 ⎢ (1)(1 + η)| ⎢ ∂N (0, 0) (0, 0) ∂N ∂ξ 3 3 (0,0) ⎥ ⎢ ⎣ ⎥ ⎢ ∂ξ ∂η ⎥ ⎢ (−1)(1 + η)|(0,0) ⎥ ⎢ ⎣ ∂N4 (0, 0) ∂N4 (0, 0) ⎦ ∂ξ ∂η ⎡ ⎤ −1 −1 ⎢ ⎥ 1 −1⎥ 1⎢ ⎥. = ⎢ 4⎢ 1⎥ ⎣1 ⎦ −1 1 ⎡

(1 − ξ )(−1)|(0,0)

⎤

⎥ (1 + ξ )(−1)|(0,0) ⎥ ⎥ (1 + ξ )(1)|(0,0) ⎥ ⎦ (1 − ξ )(1)|(0,0)

In order to determine the Jacobian matrix ∂X/∂ξ , let us ﬁrst write down the relationship between element and nodal positions; that is, X = N1 X1 + N2 X2 + N3 X3 + N4 X4 , Y = N1 Y1 + N2 Y2 + N3 Y3 + N4 Y4 . We see, therefore, that ∂N1 ∂NI ∂N2 ∂N3 ∂N4 ∂X = X1 + X2 + X3 + X4 = XI ∂ξ ∂ξ ∂ξ ∂ξ ∂ξ ∂ξ

Finite element equilibrium equations

127

and similarly for other terms. The Jacobian matrix, therefore, from (4.96) is ⎡ ∂X ∂X ⎤ ⎡ ∂N ∂NI ⎤ I XI XI ⎢ ∂ξ ⎢ ∂η ⎥ ∂η ⎥ ∂ξ ⎥=⎢ ⎥ J =⎢ ⎣ ∂Y ∂Y ⎦ ⎣ ∂NI ∂NI ⎦ YI YI ∂ξ ∂η ∂ξ ∂η ⎤ ⎡ ∂N1 ∂N1 ⎢ ∂ξ ∂η ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ ∂N2 ∂N2 ⎥ ⎥ ⎢ ∂ξ ∂η ⎥ X1 X2 X3 X4 ⎢ ⎥. ⎢ = ⎥ Y1 Y2 Y3 Y4 ⎢ ∂N ∂N 3 3 ⎥ ⎢ ⎥ ⎢ ∂η ⎥ ⎢ ∂ξ ⎥ ⎢ ⎣ ∂N4 ∂N4 ⎦ ∂η ∂ξ This can be written in the general form given in Equation (4.61) as J =X

∂N . ∂ξ

With the shape functions given above, evaluated at the integration point, and the nodal coordinates, the Jacobian becomes ⎡ ⎤ −1 −1 ⎥ ∂X ∂N X1 X2 X3 X4 1 ⎢ ⎢ 1 −1⎥ =X = ⎣ 1⎦ Y1 Y2 Y3 Y4 4 1 ∂ξ ∂ξ −1 1 1 −X1 + X2 + X3 − X4 −X1 − X2 + X3 + X4 = −Y1 − Y2 + Y3 + Y4 4 −Y1 + Y2 + Y3 − Y4 1 −0 + 0 + 1 − 1 −0 − 0 + 1 + 1 = 4 −1 + 0 + 0 − 1 −1 − 0 + 0 + 1 1 0 2 0 0.5 = . = −0.5 0 4 −2 0 The determinant of the Jacobian is ∂X 0 det[J ] = det = det −0.5 ∂ξ and its inverse is

∂X ∂ξ

−1

0 = 2

0.5 = 0.25 0

−2 . 0

128

Finite element method

Finally, the shape function derivatives with respect to the spatial (here, equivalent to the material) coordinates are ⎡ ⎤ −1 −1 −1 ∂N 1⎢ ∂N ∂X 1 −1⎥ 0 −2 ⎢ ⎥ = ⎣ = 1⎦ 2 0 ∂X ∂ξ ∂ξ 4 1 −1 1 ⎡ ⎤ ⎡ ⎤ −1 −1 −1 −1 ⎢ 1 −1⎥ 0 −0.5 1⎢ 1 −1⎥ 0 −2 ⎢ ⎥ ⎢ ⎥ =⎣ = ⎣ 1⎦ 2 0 1 1 ⎦ 0.5 0 4 1 −1 1 −1 1 ⎡ ⎤ −0.5 0.5 ⎢−0.5 −0.5⎥ ⎥ =⎢ ⎣ 0.5 −0.5⎦ . 0.5

0.5

The B matrix can now be obtained (for plane strain) from (4.81) ⎡ ⎤ ∂NI (0, 0) 0 ⎢ ⎥ ∂x ⎢ ⎥ ⎢ ∂NI (0, 0) ⎥ ⎢ ⎥ 0 BI = ⎢ ⎥, ∂y ⎢ ⎥ ⎢ ⎥ ⎣ ∂NI (0, 0) ∂NI (0, 0) ⎦ 0 0.5 −0.5

−0.5 0 −0.5

0 −0.5 −0.5

The elasticity matrix for plane strain is ⎡ λ + 2µ λ C=⎣ λ λ + 2µ 0 0

0.5 0 0 −0.5 −0.5 0.5 ⎤ 0 0⎦ , µ

νE = 84 N/mm2 , (1 + ν)(1 − 2ν) E = 84 N/mm2 , µ=G= 2(1 + ν) ⎤ ⎡ 252 84 0 C = ⎣ 84 252 0 ⎦ N/mm2 . 0 0 84 λ=

-------

−0.5 B=⎣ 0 0.5

∂x -------

∂y -------

⎡

0.5 0 0.5

⎤ 0 0.5⎦ . 0.5

Finite element equilibrium equations

129

The stiffness matrix can then be determined by using the approximate integration formula given above as k=

B CB dV = T

V

0

1 1

B CB dx dy = T

0

1

−1 −1

-------

≈ [B(0, 0)]T CB(0, 0) det[J (0, 0)].2.2 ⎤ ⎡ −0.5 0 0.5 ⎢ 0 0.5 −0.5⎥ ⎥ ⎢ ⎥⎡ ⎢−0.5 ⎤ 0 −0.5 ⎥ 252 84 ⎢ 0 ⎥ ⎢ −0.5 −0.5⎥ ⎣ ⎢ 0 =⎢ ⎥ 84 252 0 ⎦ 0 −0.5⎥ ⎢ 0.5 ⎥ 0 ⎢ 0 84 ⎢ 0 −0.5 0.5 ⎥ ⎥ ⎢ ⎣ 0.5 0 0.5 ⎦ 0 0.5 0.5 ⎡ −0.5 0 −0.5 0 0.5 0 ×⎣ 0 0.5 0 −0.5 0 −0.5 0.5 −0.5 −0.5 −0.5 −0.5 0.5 ⎡ 84 −42 42 0 −84 42 −42 ⎢−42 84 0 −42 42 −84 0 ⎢ ⎢ 42 0 84 42 −42 0 −84 ⎢ ⎢ 42 84 0 42 −42 ⎢ 0 −42 =⎢ 42 −42 0 84 −42 42 ⎢−84 ⎢ ⎢ 42 −84 0 42 −42 84 0 ⎢ ⎣−42 0 −84 −42 42 0 84 0 42 −42 −84 0 −42 42 ⎡ 84 −42 42 0 −84 42 −42 ⎢−42 84 0 −42 42 −84 0 ⎢ ⎢ 42 0 84 42 −42 0 −84 ⎢ ⎢ 42 84 0 42 −42 ⎢ 0 −42 =⎢ 42 −42 0 84 −42 42 ⎢−84 ⎢ ⎢ 42 −84 0 42 −42 84 0 ⎢ ⎣−42 0 −84 −42 42 0 84 0 42 −42 −84 0 −42 42 -------

1

B T CB det[J ] dξ dη

⎤ 0.5 0 1 0 0.5⎦ 4 4 0.5 0.5 ⎤ 0 42 ⎥ ⎥ −42 ⎥ ⎥ ⎥ −84 ⎥ 1 ⎥ 4 0 ⎥4 ⎥ −42 ⎥ ⎥ 42 ⎦ 84 ⎤ 0 42 ⎥ ⎥ −42 ⎥ ⎥ ⎥ −84 ⎥ ⎥. 0 ⎥ ⎥ −42 ⎥ ⎥ 42 ⎦ 84

-------

The equilibrium equation for this quasi-static problem is ku = f ,

(4.98)

130

Finite element method

⎡

84 ⎢−42 ⎢ ⎢ 42 ⎢ ⎢ ⎢ 0 ⎢ ⎢−84 ⎢ ⎢ 42 ⎢ ⎣−42 0

−42 84 0 −42 42 −84 0 42

42 0 84 42 −42 0 −84 −42

0 −42 42 84 0 42 −42 −84

−84 42 −42 0 84 −42 42 0

42 −84 0 42 −42 84 0 −42

−42 0 −84 −42 42 0 84 42

0 42 −42 −84 0 −42 42 84

⎡

⎤⎡

Rx1 Ry1 Rx2 Ry2

⎤

⎤ ⎢ ⎥ 0 ⎢ ⎥ ⎥⎢ 0 ⎥ ⎢ ⎥ ⎥⎢ ⎥ ⎢ ⎥ ⎥⎢ 0 ⎥ ⎢ ⎥ ⎥⎢ ⎥ ⎢ ⎥ ⎥⎢ ⎥ ⎢ ⎥ π ⎥⎢ 0 ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ = ⎢ F cos ⎥ ⎥ ⎢ux3 ⎥ ⎢ ⎥ 4 ⎥⎢ ⎥ ⎢ π⎥ ⎥ ⎢uy3 ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ ⎢−F cos ⎥ ⎦⎣ 0 ⎦ ⎢ 4⎥ ⎢ ⎥ ⎣ Rx4 ⎦ uy4 0

so that with the boundary conditions it simpliﬁes to ⎤ ⎡ ⎤⎡ ⎤ ⎡ √ 10 2/2 84 −42 0 ux3 ⎢ ⎥⎢ ⎥ ⎢ √ ⎥ ⎢−42 ⎥ ⎢uy3 ⎥ = ⎢−10 2/2⎥ . 84 −42 ⎦ ⎣ ⎦⎣ ⎦ ⎣ uy4 0 −42 84 0 The solution is obtained from u = k −1 f , ⎡ ⎤ ⎡ 0.017857 0.011905 ux3 ⎢ ⎥ ⎢ ⎢uy3 ⎥ = ⎢0.011905 0.023810 ⎣ ⎦ ⎣ uy4 0.005952 0.011905 ⎡ ⎤ ⎡ ⎤ ux3 0.04209 ⎢ ⎥ ⎢ ⎥ ⎢uy3 ⎥ = ⎢−0.08418⎥ mm. ⎣ ⎦ ⎣ ⎦ uy4 −0.04209

⎤ √ 10 2/2 ⎥⎢ √ ⎥ ⎢−10 2/2⎥ , 0.011905⎥ ⎦ ⎦⎣ 0.017857 0

0.005952

⎤⎡

The reactions can be obtained from ⎡

84 ⎢−42 ⎢ ⎢ 42 ⎢ ⎢ ⎢ 0 ⎢ ⎢−84 ⎢ ⎢ 42 ⎢ ⎣−42 0

−42 84 0 −42 42 −84 0 42

42 0 84 42 −42 0 −84 −42

0 −42 42 84 0 42 −42 −84

−84 42 −42 0 84 −42 42 0

42 −84 0 42 −42 84 0 −42

−42 0 −84 −42 42 0 84 42

0 42 −42 −84 0 −42 42 84

⎤⎡

⎤

⎡

Rx1 Ry1 Rx2 Ry2

⎤

⎢ ⎥ 0 ⎢ ⎥ ⎥⎢ 0 ⎥ ⎢ ⎥ ⎥⎢ ⎥ ⎢ ⎥ ⎥⎢ 0 ⎥ ⎢ ⎥ ⎥⎢ ⎥ ⎢ ⎥ ⎥⎢ ⎥ ⎢ ⎥ π 0 ⎥⎢ ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ = ⎢ F cos ⎥ , ⎥ ⎢ux3 ⎥ ⎢ ⎥ 4 ⎥⎢ ⎥ ⎢ π⎥ ⎥ ⎢uy3 ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ ⎢−F cos ⎥ ⎢ ⎦⎣ 0 ⎦ 4⎥ ⎢ ⎥ ⎣ Rx4 ⎦ uy4 0

Finite element equilibrium equations

131

√ Rx1 = −84ux3 + 42uy3 + 0uy4 = −10 2/2N, √ Ry1 = 42ux3 − 84uy3 + 42uy4 = 10 2/2N, Rx2 = −42ux3 + 0uy3 − 42uy4 = 0, Ry2 = 0ux3 + 42uy3 − 84uy4 = 0, Rx4 = 42ux3 + 0uy3 + 42uy4 = 0. We can carry out an equilibrium check as follows: √ √ √ 10 2 10 2 10 2 =− +0+0+ = 0, Fx = Rx1 + Rx2 + Rx4 + 2 2 2 √ √ √ F 2 10 2 10 2 = +0− = 0. Fy = Ry1 + Ry2 − 2 2 2 The element strains at the integration point may be determined as ε(ξ, η) = ε(0, 0) ≈

NNODE

B I (0, 0) · uI

I =1

⎤ 0.021045 = ⎣ 0.021045 ⎦ −0.08418 ⎡

0 −0.5 −0.5

-------

−0.5 0 −0.5

0.5 0 0 −0.5 −0.5 0.5

0.5 0 0.5

0.5 0 0 −0.5 −0.5 0.5

-------

−0.5 0 ⎣ = 0 0.5 0.5 −0.5

0 −0.5 −0.5

-------

⎡

−0.5 0 −0.5

-------

0 0.5 −0.5

-------

−0.5 =⎣ 0 0.5

-------

⎡

⎡

0.5 0 0.5

⎤ 0 ⎢ 0 ⎥ ⎢ ⎥ ⎤⎢ 0 ⎥ ⎥ 0 ⎢ ⎢ ⎥ 0 ⎢ ⎥ 0.5⎦ ⎢ ⎥ ⎢ux3 ⎥ 0.5 ⎢ ⎥ ⎢uy3 ⎥ ⎢ ⎥ ⎣ 0 ⎦ uy4 ⎤ ⎡ 0 ⎥ ⎢ 0 ⎥ ⎢ ⎥ ⎢ ⎤⎢ 0 ⎥ 0 ⎢ ⎥ 0 ⎥ ⎢ 0.5⎦ ⎢ ⎥ ⎢ 0.04209 ⎥ ⎥ 0.5 ⎢ ⎢−0.08418⎥ ⎥ ⎢ ⎦ ⎣ 0 −0.04209

132

Finite element method

and the stresses are given by ⎤ ⎤⎡ 0.021045 252 84 0 σ(ξ, η) = Cε(ξ, η) = ⎣ 84 252 0 ⎦ ⎣ 0.021045 ⎦ −0.08418 0 0 84 ⎤ ⎡ √ ⎡ ⎤ 10√2/2 7.071068 ⎦ ⎣ ⎣ = 7.071068 = 10 2/2 ⎦ N/mm2 . √ −7.071068 −10 2/2 ⎡

A further check is that the internal forces at nodal points must be equal to nodal external forces (note that the reactions are external forces too): ⎡ int ⎤ fx1 ⎢ ⎥ ⎢f int ⎥ ⎢ y1 ⎥ ⎢ ⎥ ⎢f int ⎥ ⎢ x2 ⎥ ⎢ ⎥ ⎢f int ⎥ 1 1 ⎢ y2 ⎥ T ⎥= B σ dV = B T σ dx dy f int = ⎢ ⎢ int ⎥ 0 0 V ⎢fx3 ⎥ ⎢ ⎥ ⎢ int ⎥ ⎢fy3 ⎥ ⎢ ⎥ ⎢ int ⎥ ⎢fx4 ⎥ ⎣ ⎦ int fy4 1 1 1 1 1 B T σ det[J ] dξ dη = B T σ dξ dη = 4 −1 −1 −1 −1 √ ⎤ ⎡ −10 2/2 ⎡ ⎤ −0.5 0 0.5 ⎢ √ ⎥ ⎢ 10 2/2 ⎥ ⎢ ⎥ ⎢ ⎥ 0.5 −0.5⎥ ⎢ 0 ⎢ ⎥ ⎢ ⎥ ⎥ 0 ⎢−0.5 0 −0.5⎥ ⎡ √ ⎤ ⎢ ⎢ ⎥ ⎢ ⎥ 10 2/2 ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ 0 ⎢ 0 −0.5 −0.5⎥ ⎢ √ ⎥ ⎢ ⎥ T 1 T ⎢ ⎥ ⎥ ⎢ =B σ 4=B σ=⎢ 10 2/2 ⎦ = ⎢ √ ⎥ N. ⎥ ⎣ ⎢ 4 0 −0.5⎥ ⎢ 0.5 10 2/2 ⎥ √ ⎢ ⎥ ⎢ ⎥ ⎢ √ ⎥ ⎢ 0 −0.5 0.5 ⎥ −10 2/2 ⎢ ⎥ ⎢ ⎥ ⎢−10 2/2⎥ ⎢ ⎥ ⎢ ⎥ 0 0.5 ⎦ ⎣ 0.5 ⎢ ⎥ 0 ⎣ ⎦ 0 0.5 0.5 0 We need to summarize a few important points before leaving this section. In all the examples considered, we have used only one or two ﬁnite elements. This is intended

Finite element equilibrium equations

133

to aid in the development of understanding of the ﬁnite element method rather than to suggest that practical problems can be solved in this way. Most engineering problems require very large numbers of ﬁnite elements in order to obtain an accurate representation and solution. Naturally, the calculations are then carried out on a computer. We should also note that we have gone on to determine solutions for only quasi-static problems. This required the solution of the Equation (4.98). However, we have set up the ﬁnite element equilibrium (also often known as momentum balance) equations for a number of dynamic problems which we have not attempted to solve. Solution of these problems requires in general the numerical integration of the momentum balance Equation (4.85), using, for example, the explicit central difference time integration scheme, which is introduced brieﬂy later on, or an implicit scheme. So far, in this chapter, we have been concerned with both geometrically linear and non-linear problems in which the material behaviour has always been assumed to be linear (elasticity). We shall continue by introducing incremental ﬁnite element techniques for non-linear material behaviour; that is, in particular, for plasticity.

4.4.4

Finite element formulation for plasticity

The equilibrium equations derived in (4.71)–(4.75) from virtual work are applicable in general to linear and non-linear material behaviour. In order to address a particular example, we return to the equilibrium Equation (4.69) but for simplicity, assume quasistatic conditions and so ignore inertia terms, and we consider small deformations. Using Voigt notation the equation of virtual work becomes δW = δD T σ dV − t · δv dA = 0.

∂

With the ﬁnite element discretization as before, the equation becomes δW =

NNODE

T B I dv I

I =1

σ dV −

∂

t·

NNODE

NI δv I dA.

I =1

For small strain elastic–plastic material behaviour, we σ = Cεe = C(ε − εp ) so δW =

NNODE

I =1

T B I δv I

C(ε − εp ) dV −

∂

t·

NNODE I =1

NI δv I dA

134

Finite element method

and with the ﬁnite element discretization for the strain presented in Section 4.4.3, this becomes ⎛ ⎞ NNODE δW I = δv TI ⎝ B TI CB J dV ⎠ uJ I,J =1

− δv TI

NNODE

I =1

B TI Cεp dV

− δv TI

NNODE I =1

∂

NI t dA.

As before, for an arbitrary virtual velocity, we may then write the element equilibrium equation as (4.99) ku − f p = f , where fp =

NNODE I =1

B TI Cεp dV .

In contrast to linear elastic problems in which there exists a unique relationship between stress and elastic strain, no such uniqueness holds for plasticity problems. An incremental approach to solving (4.99) is therefore almost always necessary, and to emphasize this, the displacement, plastic strain, and external force terms are written as increments so that ku − f p = f (4.100) and f p =

NNODE I =1

B TI Cεp dV .

(4.101)

Equation (4.100) may alternatively be written as ku = f ,

(4.102)

where f = f p + f . 4.4.4.1 Single truss element undergoing elastic–plastic deformation. We now return to the single truss element which we examined for the case of elastic material behaviour in Section 4.4.2.1. The problem is shown in Fig. 4.10(a) and the single element discretization in 4.10(b). For this problem, the B matrix, and the stiffness matrix, k, remain unchanged as 1 EA 1 −1 B = [−1 1], k= L L −1 1

Finite element equilibrium equations

135

and we write the incremental external force vector as F1 f = . P The plasticity ‘force’ is determined from (4.101) for this element as 1 1 −1 T p p p −1 p Eε A det(J ) dξ = EAε B Cε dV = f = 1 1 ξ =0 L so that from (4.100) the equilibrium equation becomes EA 1 −1 u1 −1 F1 . − EAεp = u2 P 1 L −1 1 With the boundary condition that u1 = 0, this reduces to EA u2 − EAεp = P . L Rearranging gives P L + Lε p . (4.103) u2 = EA In the absence of plasticity, this just gives us an incremental form of the expression we obtained before for elasticity in Section 4.4.2.1. For the case of plasticity, however, the increment in displacement now becomes that due to the elastic deformation together with that resulting from the plastic strain, which unsurprisingly in this small strain formulation has magnitude Lεp . To demonstrate further the need for an incremental approach, let us now assign elastic linear strain hardening plasticity properties to the rod material and determine the rod extension on application of a given force, P . In Section 2.4.2, we saw that for uniaxial linear isotropic hardening the relation between the increment in uniaxial stress and plastic strain was given by σ εp = h in which h is the strain hardening constant. Writing σ = P /A gives P ε p = Ah and substituting into (4.102) gives P L 1 1 P L LP + = + . (4.104) u2 = EA Ah A E h Therefore, the incremental displacement for elastic and elastic–plastic conditions becomes P L . Elastic : σ < σy , u2 = EA 1 P L 1 + . Elastic–plastic : σ ≥ σy , u2 = A E h

136

Finite element method

11 N L = 10 mm

E = 1000 MPa A = 1.0 mm2 sy = 10 MPa h = 100 MPa

Fig. 4.18 A uniform bar under axial loading with the properties shown.

Let us analyse incrementally the problem shown in Fig. 4.18. We will apply the load incrementally. The ﬁrst load increment, however, will be chosen to cause ﬁrst yield. That is, P1 = σy A = 10 N. The displacement increment is given by 10 × 10 P L = = 0.1 mm u(1) = EA 1000 × 1 so u(1) = u(0) + u(1) = 0 + 0.1 = 0.1 mm. Subsequent displacement increments must take account of the plasticity so that u(2) =

1 × 10 10 × 1 P L LP + = + = 0.11 mm EA Ah 1000 × 1 1 × 100

and u(2) = u(1) + u(2) = 0.1 + 0.11 = 0.21 mm. We see from Equation (4.104) that since the rate of hardening is constant (i.e. h is ﬁxed), the displacement—load relationship becomes independent of increment size, once the material has yielded. However, were we to introduce non-linear hardening where, for example, h depends on plastic strain, Equation (4.104) shows that the displacement—load relationship then becomes dependent on the increment size.

4.5 4.5.1

Integration of momentum balance and equilibrium equations Explicit integration using the central difference method

The ﬁnite element discretization of the momentum balance equation for a damped system can be expressed in matrix form as follows: Mu¨ + Cu˙ + Fint = Fext , where M is the mass matrix, Fint the internal force vector, and Fext the external force vector. The integration of the equations can be carried out by means of the explicit central difference time integration scheme. The scheme is derived from Taylor series

Integration of momentum balance and equilibrium equations

137

expansions of the displacements, u, as follows. t 2 + ··· 2 t 2 ˙ ¨ u(t − t) = u(t) − u(t)t + u(t) − ··· . 2 The central difference approximations are obtained taking the difference of the above expressions to give the velocity uN+1 − uN −1 u˙ N = 2t and by summing the expressions for the accelerations ˙ ¨ u(t + t) = u(t) + u(t)t + u(t)

u¨ N =

uN+1 − 2uN + uN −1 , (t)2

where uN = u(tN ). Assuming that the acceleration is constant between tN and tN +1 the central difference approximations can be rearranged to give the following second-order integration scheme 1 uN+1 = uN + u˙ N t + u¨ N (t)2 , 2 1 u˙ N+1 = u˙ N + (u¨ N + u¨ N +1 )t. 2 These are more commonly rewritten by deﬁning the intermediate velocities based on the assumption that the acceleration is constant between t0 and t0+1/2 as well as between tN−1/2 and tN+1/2 so that 1 u˙ 1/2 = u˙ 0 + u¨ 0 t 2 to give the leap frog explicit method u˙ N+1/2 = u˙ N−1/2 + u¨ N t, uN+1 = uN + u˙ N+1/2 t. The central difference method can be applied with a varying time increment (which is particularly important if the response of the continuum is non-linear), as illustrated in Fig. 4.19. Let tN+1 be the time increment between tN and tN +1 with uN = u(tN ) as illustrated in Fig. 4.19. The mid-step velocities are deﬁned by ˙ N−1/2 ), u˙ N−1/2 = u(t

˙ N +1/2 ), u˙ N +1/2 = u(t

138

Finite element method ∆tN

∆tN + 1

t N –1

tN

t N +1

t N + 1/2

t N –1/2

t

üN N –1/2

N +1/2

uN

uN +1

Fig. 4.19 Central difference integration scheme.

where 1 1 (tN−1 + tN ), tN +1/2 = (tN + tN +1 ). 2 2 The central difference formula for velocity is tN −1/2 =

u˙ N+1/2 =

uN+1 − uN , tN +1

while the central difference formula for acceleration is u¨ N =

u˙ N+1/2 − u˙ N −1/2 , tN+1/2

where 1 (tN + tN +1 ). 2 The discretization of the momentum balance equation for an undamped system can be obtained by substituting the acceleration term with its ﬁnite difference approximation as follows: u˙ N+1/2 − u˙ N−1/2 int ext M + FN = FN , tN+1/2 tN+1/2 =

which yields u˙ N+1/2 = M−1 (Fext − Fint )tN +1/2 + u˙ N −1/2 and uN+1 = uN + u˙ N+1/2 tN +1 . Subsequently, the internal and external force vectors can be calculated as int FN+1 = Fint (uN+1 ),

ext FN+1 = Fext (uN +1 ),

which completes the Nth time step. Furthermore, if the mass matrix is diagonalized the system of differential equations uncouples and can be solved independently for each degree of freedom (see, e.g. Newland).

Integration of momentum balance and equilibrium equations

139

4.5.1.1 Stability of the explicit time stepping scheme. The solution of a SDOF equilibrium equation u¨ + ω2 u = 0 can be obtained using the central difference time stepping scheme as follows u¨ N =

uN+1 − 2uN + uN −1 = −ω2 uN (t)2

giving the difference equation uN+1 − (2 − ω2 (t)2 )uN + uN −1 = 0. Trying solutions uN = An where A is the ampliﬁcation factor gives A2 − (2 − ω2 (t)2 )A + 1 = 0. The roots of this polynomial are

ω2 (t)2 A= 1− 2

%

±

ω2 (t)2 1− 2

2 − 1.

For stability |A| ≤ 1, which gives the stability condition as t ≤

2 . ω

For a general multidegree of freedom system, the stability condition becomes t ≤

2 , ωmax

where ωmax = max{ωi } i

is the element maximum eigenvalue. A conservative estimate of the stable time increment is given by the following minimum taken over all the elements t ≤ min

Lc , cd

where Lc is the characteristic element length and cd is the current effective dilatational wave speed of the material.

140

4.5.2

Finite element method

Introduction to implicit integration

Implicit integration schemes are often preferred to their explicit counterparts since they involve the determination of a residual force at each step and iteration within the step to minimize the residual force to within a speciﬁed tolerance. We brieﬂy introduce three techniques; the tangential stiffness method, the initial tangential stiffness method, and the Newton–Raphson method. We conﬁne ourselves here to quasi-static problems so assume inertia effects are negligible. 4.5.2.1 Tangential stiffness method. The discretized static equilibrium equation given in (4.102), for example, will not generally be satisﬁed unless a convergence occurs which can be expressed in terms of residual forces as follows k(u)u − f = Ψ = 0. The iteration starts from an initially guessed solution u0 and the corresponding tangential stiffness matrix k(u0 ). The residual forces are calculated from Ψ0 = k(u0 )u0 − f . The correction u is calculated as follows: un = [K(un )]−1 Ψn

(4.105)

and an improved solution is then obtained as follows: un+1 = un + un . The process continues until the residual forces Ψn are smaller than a speciﬁed tolerance. 4.5.2.2 Initial tangential stiffness method. The initial tangential stiffness method differs from the previous method only in that the correction to the displacement, given in Equation (4.105), is now calculated always based upon the initial tangential stiffness matrix so that un = [k(u0 )]−1 Ψn and as before, the improved solution is obtained as un+1 = un + un and the process continues until the residual forces Ψn are smaller than a speciﬁed tolerance.

Integration of momentum balance and equilibrium equations

141

4.5.2.3 Newton–Raphson method. As in the previous methods, the residual force is determined from = k(u)u − f = 0. (4.106) Using a Taylor expansion, may be approximated by ∂(u) (u) + (4.107) u + O(u2 ) = 0. ∂u The matrix J = ∂/∂u is called the Jacobian (which has nothing to do with the Jacobian introduced above for the mapping of spatial to local element conﬁgurations), or effective tangent stiffness, and from (4.106) it can be seen that this comprises a term corresponding to the internal forces, termed the tangent stiffness matrix, and a further term corresponding to the ‘external’ forces, called the load stiffness matrix. Equation (4.107) provides a linearization of (4.106) and may be written as + Ju = 0 so that J(un )un = −(un ) and the displacement is updated by un+1 = un + un . The iteration continues until the tolerance limit on residual force is achieved. The two schemes introduced above, namely explicit and implicit integration, may be used for the integration of the momentum balance, or equilibrium, ﬁnite element equations. In implementing plasticity models into ﬁnite element formulations, it is often necessary, in addition, to integrate a set of constitutive equations (e.g. to give the plastic strain increment). For this additional integration, it is also possible to employ either implicit or explicit integration methods. In the overall solution process, therefore, there are several possible combinations of implicit and explicit integration. Finite element methods which employ implicit schemes for the integration of the momentum balance, or equilibrium equations, regardless of whether the constitutive equations are integrated using implicit or explicit integration, are referred to as implicit ﬁnite element methods. Similarly, ﬁnite element methods which employ explicit schemes for the integration of the momentum balance, or equilibrium equations, are called explicit ﬁnite element methods. Both implicit and explicit formulations are available in ABAQUS. It can be seen that the implicit scheme offers the more robust overall approach, because of the iteration necessary in order to achieve convergence. Explicit schemes, however, can often produce more rapid solutions, and are more appropriate for dynamic analyses. Care has to be taken, however, in choosing time step size and ensuring the calculated solution does not drift away from the true solution. We shall examine this further in the context of integration of constitutive equations in Chapter 5.

142

Finite element method

Further reading Bathe, K.-J. (1996). Finite Element Procedures. Prentice Hall, New Jersey, revised edition. Belytschko, T., Liu, K.W., and Moran, B. (2000). Non-linear Finite Element Analysis for Continua and Structures. John Wiley & Sons, New York. Bonet, J. and Wood, R.D. (1997). Non-linear Continuum Mechanics for Finite Element Analysis. Cambridge University Press. Hinton, E. and Owen, D.R.J. (1979). An Introduction to Finite Element Computations. Pineridge Press, Swansea. Newland, D.E. (1989). Mechanical Vibration Analysis and Computation. Longman Scientiﬁc and Technical, John Wiley and Sons, New York. Owen, D.R.J. and Hinton, E. (1980). Finite Elements in Plasticity: Theory and Practice. Pineridge Press, Swansea. Timoshenko, S. and Goodier, J.N. (1983). Theory of Elasticity. McGraw-Hill, New York. Zienkiewicz, O.C. and Taylor, R.L. (1989). The Finite Element Method. McGraw-Hill, London, 4th edition.

5. Implicit and explicit integration of von Mises plasticity

5.1

Introduction

In this chapter, we shall return to the constitutive equations for plasticity introduced in Chapter 2 and see how they may be integrated and how the Jacobian or tangent stiffness may be obtained from them. We shall explore both implicit and explicit schemes for the integration of the constitutive equations. To start, we shall consider small strain, time-independent, linear isotropic hardening plasticity before looking at kinematic hardening and viscoplasticity. First, we return to the determination of the plastic multiplier.

5.2

Implicit and explicit integration of constitutive equations

We saw from Chapter 2 that the yield function for isotropic hardening can be written 1/2 3

f = σe − r − σy = σ :σ − r − σy = 0 (5.1) 2 and that the plastic multiplier, in principal stress space is given by dλ =

(∂f/∂σ) · C dε , (∂f/∂σ) · C(∂f/∂σ) − (∂f/∂p)[(2/3)(∂f/∂σ) · (∂f/∂σ)]1/2

(5.2)

where all terms are written in Voigt notation. Before proceeding, let us redetermine the plastic multiplier more generally, without the constraint of working in principal stress space. The consistency condition is written in terms of the stress tensor df (σ , p) =

∂f ∂f : dσ + dp = 0. ∂σ ∂p

If we write the tensor normal, n, for a von Mises material n=

∂f 3 σ

= , ∂σ 2 σe

144

Implicit and explicit integration

the consistency condition becomes df (σ , p) = n : dσ +

∂f dp = 0, ∂p

where without loss of generality, we assume out of plane shears are zero, so ⎡ ⎤ n11 n12 0 n = ⎣n12 n22 0 ⎦ . 0 0 n33 Let us also write, in Voigt notation, the vector normal, n, ⎡ ⎤ n11 ⎢ n22 ⎥ ⎥ n=⎢ ⎣ n33 ⎦ . 2n12 We can then see that ⎡ n11 n12 n : dσ = ⎣n12 n22 0 0

⎤ ⎡

dσ11 0 0 ⎦ : ⎣dσ12 n33 0

dσ12 dσ22 0

⎤ ⎡ ⎤ dσ11 n11 0 ⎢ n22 ⎥ ⎢dσ22 ⎥ ⎥ ⎢ ⎥ 0 ⎦=⎢ ⎣ n33 ⎦ · ⎣dσ33 ⎦ ≡ n · dσ dσ33 2n12 dσ12 ⎤

⎡

so that, provided the normal vector, n, in Voigt notation contains twice the tensorial normal shear terms, then n : dσ ≡ n · dσ and the consistency condition becomes df (σ , p) = n · dσ +

∂f dp = 0. ∂p

We may now determine the plastic multiplier with Hooke’s law written in Voigt notation, as before dσ = C(dε − dεp ). The increment in tensorial plastic strain is obtained from the normality hypothesis, dε p = dλ

∂f = dλn, ∂σ

which we may write in Voigt notation as dεp = dλn remembering that the shear strain terms in the Voigt strain vector are engineering shears; that is, twice the tensorial shears. Hooke’s law then becomes dσ = C(dε − dλn)

Implicit and explicit integration of constitutive equations

145

and combining with the consistency condition, in which, for a von Mises material, dp = dλ, we obtain ∂f n · C(dε − dλn) + dλ = 0 ∂p so that the plastic multiplier is given by dλ =

n · C dε . n · Cn − (∂f /∂p)

For linear isotropic hardening, r = hp so that ∂f /∂p = −∂r/∂p = −h and n · C dε . n · Cn + h Finally, the stress increment is given by dλ =

dσ = C dεe = C(dε − dεp ) = C(dε − dλn).

(5.3)

(5.4)

With knowledge of the total strain increment, dε, together with the stress, σ, Equation (5.3) allows the plastic multiplier to be determined so that the stress increment can be obtained from (5.4). The updated stress, σ + dσ may then be obtained. This is called an explicit integration process. If we denote all quantities at time t with subscript t, and those at the next increment forward in time, t + t, in a similar way, then we may write dλt =

nt · C dεt , nt · Cnt + h

dσt = C(dεt − dλnt ),

(5.5)

dr = h dp = h dλt . The integration to obtain all quantities at the end of the time step, t, may then be written as σt+t = σt + dσt , p

p

p

εt+t = εt + dεt ,

(5.6)

rt+t = rt + drt . This is called a ﬁrst-order forward Euler explicit integration scheme. Its advantage is its simplicity and it is straightforward to implement as we shall see later. However, there are a number of disadvantages which need to be considered. First, because it is an explicit scheme, it is conditionally stable; that is, it may become unstable. Second, the accuracy of the integration depends, of course, on the time step size, t, chosen. Great care is therefore required in ensuring that the time step does not become too large such that erroneous results are obtained. Third, and perhaps most importantly,

146

Implicit and explicit integration

the plastic multiplier given in Equation (5.5) was obtained to ensure that at time, t, the yield condition in (5.1) is satisﬁed. However, the forward integration process does not ensure that the yield condition is also satisﬁed at time t + t, and as a result, it is possible for the solution, over many time steps, to drift away from the yield surface. This is overcome by means of implicit integration of the equations which has the additional advantage of being unconditionally stable. The accuracy remains dependent, however, on the time step size. We introduce an implicit scheme, known as the radial return method for von Mises plasticity, in Section 5.2.1.

5.2.1

Implicit integration: the radial return method

Figure 5.1(a) shows a von Mises yield surface with a schematic representation of the explicit integration method described above. A step forward in time takes the updated stresses outside of the yield surface. Figure 5.1(b) shows a representation of an implicit scheme. A trial stress increment is chosen which again takes the updated stresses, σ trt+t , outside of the yield surface. The stress is then updated with a plastic correction to bring it back onto the yield surface at time t + t. In deviatoric stress space, the plane stress von Mises ellipse becomes a circle, and the plastic correction term is always directed towards the centre of the yield surface (because of the normality condition). The technique has therefore come to be known as the radial return method. In what follows, we shall take all quantities to be those at the end of a time step, t + t, unless speciﬁcally stated. So, the stress at t + t is just σ and that at the beginning of the time step, at time t, is σ t . We may write Hooke’s law in multiaxial form in terms of stress and strain tensors as σ = 2Gεe + λ Tr(εe )I . (a)

(b)

st + ∆t

s2 sy

s2 sy

st

st + ∆t

st

sy

sy sy

s1

sy

sy

s1

sy

Fig. 5.1 Schematic representations of (a) explicit integration and (b) implicit integration, using the radial return method, of von Mises plasticity equations.

Implicit and explicit integration of constitutive equations

147

The elastic strain at the end of the time step may be written as εe = εet + ε e = εet + ε − ε p so that σ = 2G(εet + ε − ε p ) + λ Tr(εet + ε − ε p )I and so p σ = 2G(εet + ε) + λ Tr(ε et + ε) I − 2Gε Elastic predictor Plastic corrector

(5.7)

since Tr(ε p ) = 0. The elastic predictor, or trial stress, is denoted by σ tr = 2G(εet + ε) + λ Tr(εet + ε)I

(5.8)

σ = σ tr − 2Gε p = σ tr − 2Gpn,

(5.9)

so that from (5.7), which we may write as

3 σ

. 2 σe The stress may be expressed in terms of its deviatoric and mean as σ = σ tr − 2Gp

(5.10)

1 σ = σ + (σ : I )I 3

(5.11)

1 σ

σ + (σ : I )I = σ tr − 3Gp 3 σe

(5.12)

so that with (5.10) we obtain

and rearranging gives

1 + 3G

1 p σ = σ tr − (σ : I )I . σe 3

(5.13)

With some algebra, using Equation (5.8), we show that σ tr − 13 (σ : I )I is just the

deviatoric of the trial stress, σ tr as follows, where K is the elastic bulk modulus. 1 σ tr − (σ : I )I = 2G(εet + ε) + λI (ε et + ε) : I − Kεe : II 3 = 2G(εet + ε) + λI (ε et + ε) : I − K(εet + ε − ε p ) : II = 2G(εet + ε) + λI (ε et + ε) : I − KI (ε et + ε) : I

= 2G(εet + ε) + (λ − K)I (ε et + ε) : I ≡ σ tr .

148

Implicit and explicit integration

p

1 + 3G σ = σ tr . (5.14) σe If we take the contracted tensor product of each side of this with itself, we obtain p 2

σ : σ = σ tr : σ tr 1 + 3G σe or 1/2 p 3 tr

tr

1 + 3G σ :σ ≡ σetr . (5.15) σe = σe 2 This gives, ﬁnally, σe + 3Gp = σetr . (5.16) We therefore obtain

The multiaxial yield condition is f = σe − r − σy = σetr − 3Gp − r − σy = 0.

(5.17)

This is generally a non-linear equation in p which may be solved using Newton’s method. We write ∂f dp + · · · = 0. (5.18) f+ ∂p For linear hardening, r = hp so that ∂r ∂r = = h. ∂p ∂p

(5.19)

Substituting (5.17) into (5.18), using (5.19) therefore gives σetr − 3Gp − r − σy + (−3G − h) dp = 0. Rearranging gives

σetr − 3Gp − r − σy . 3G + h We may write the integration in iterative form then, as dp =

r (k) = rt + hp (k) , dp =

σetr − 3Gp (k) − r (k) − σy , 3G + h

(5.20)

p (k+1) = p(k) + dp. The effective stress may then be determined from (5.16); the deviatoric stress tensor from (5.14), so that the plastic strain tensor increment is

ε p =

σ

σ tr 3 3 p ≡ p tr 2 σe 2 σe

Implicit and explicit integration of constitutive equations

149

and the elastic increment ε e = ε − εp and the stress increment is given by σ = 2Gεe + λI ε e : I . We have now introduced both explicit and implicit integration of the plasticity constitutive equations. It is important to note that in the implicit scheme, all quantities are written at the end of the time increment. This ensures that the yield condition, given in Equation (5.17), is satisﬁed at the end of the time increment, therefore avoiding ‘drift’ from the yield surface which can occur in the explicit scheme. The implicit scheme, because it enables signiﬁcantly larger time increments to be used, generally leads to much more rapid solutions. In an implementation within implicit ﬁnite element code, we saw in Section 4.5.2.3 that the implicit integration of the momentum balance or equilibrium equations requires the determination of the Jacobian that comprises both the tangent stiffness matrix and the load stiffness matrix. The tangent stiffness matrix depends very much on the material behaviour, and hence on the constitutive equations. In the implementation of a plasticity model into implicit ﬁnite element code, it is therefore necessary to provide the material tangent stiffness matrix in addition to the integration of the plasticity constitutive equations. In explicit ﬁnite element code, however, which does not depend upon knowledge of the Jacobian, the tangent stiffness matrix is not required. The determination of the material Jacobian for implicit ﬁnite element code is very much bound up with the integration of the constitutive equations used. Typically, in implementing a plasticity model into commercial codes such as ABAQUS explicit or LSDyna (which is an explicit code), for example, we need to provide a subroutine which contains the integration of the plasticity constitutive equations (whether implicit or explicit). For implementations into implicit code, such as ABAQUS standard, we need to provide a subroutine which contains both the integration of the plasticity constitutive equations (whether implicit or explicit) together with the material Jacobian or tangent stiffness matrix. It is useful to note from Section 4.5.2.3 that the Jacobian is required in the iterative procedure in minimizing the force residual. If convergence occurs after a given number of iterations, the Jacobian does not inﬂuence the accuracy of the solution, but the rate at which convergence is achieved. It is for this reason that often approximate Jacobians are used (e.g. in the initial tangent stiffness method in Section 4.5.2.2). A further reason is that depending on the complexity of the plasticity model, the material Jacobian may not be derivable in analytical terms so that a numerical, approximate implementation has to be developed. Perturbation methods can allow the accurate numerical determination of the Jacobian. In the following section, we shall address ﬁrst, the material Jacobian for an elastic material, and

150

Implicit and explicit integration

then that for the time-independent linear strain isotropic hardening plasticity model for which the implicit integration scheme was presented in this section.

5.3 5.3.1

Material Jacobian Isotropic elasticity

Hooke’s law may be written incrementally as σ = 2Gεe + λIε e : I ,

(5.21)

which may be written more succinctly as σ = (2GI + λII ) : εe in which I is the fourth-order identity tensor with the properties I : I = I : I = I and I : ε = ε : I = ε. We will deﬁne the material Jacobian here in the way it is required in the ABAQUS ﬁnite element code as ∂σ /∂ε where ∂σ dε ∂ε in which the shear strains are taken to be engineering shears. For example, dσ =

∂σ11 ∂ε12 1 ∂σ11 ∂σ11 = = , ∂γ12 ∂ε12 ∂γ12 2 ∂ε12 where ∂σ11 /∂ε12 is obtained from Equation (5.21). The material Jacobian becomes, therefore, for conditions of plane strain or axial symmetry (γ13 = γ23 = 0), ⎛ ⎞ ∂σ11 ∂σ11 ∂σ11 ∂σ11 ⎜ ∂ε11 ∂ε22 ∂ε33 ∂γ12 ⎟ ⎛ ⎞ ⎜ ⎟ 2G + λ λ λ 0 ⎜ ⎟ ⎜ ∂σ22 ∂σ22 ∂σ22 ∂σ22 ⎟ ⎜ ⎟ ⎜ ⎟ λ 2G + λ λ 0 ⎟ ⎜ ∂ε11 ∂ε22 ∂ε33 ∂γ12 ⎟ ⎜ ⎟ ⎜ ∂σ ⎜ ⎟ ⎟. = ⎜ ∂σ ∂σ ∂σ ∂σ ⎟ = ⎜ ⎜ 33 33 33 33 ⎟ λ λ 2G + λ 0 ⎟ ⎜ ∂ε ⎟ ⎜ ⎜ ⎟ ⎠ ⎜ ∂ε11 ∂ε22 ∂ε33 ∂γ12 ⎟ ⎝ 1 ⎜ ⎟ 2G 0 0 0 2 ⎜ ∂σ12 ∂σ12 ∂σ12 ∂σ12 ⎟ ⎝ ⎠ ∂ε11 ∂ε22 ∂ε33 ∂γ12 Note that in general, ∂σ /∂ε and ∂σ /∂ε are not the same thing; the former Jacobian quantity is required in ABAQUS, for example, for quadratic convergence. Unfortunately, the material Jacobian for plasticity is not quite so easy to obtain. It is derived in Section 5.3.2 for the plasticity model considered above; that is, for time-independent isotropic linear strain hardening plasticity.

Material Jacobian

5.3.2

151

Material Jacobian for time-independent isotropic linear strain hardening plasticity

We start from Equation (5.14) by applying the differential operator, δ (in a similar way as used to ﬁnd the ﬁrst variation of an integral in Chapter 4) so that we obtain 3Gp 3G p

(5.22) δσe σ = δσ tr . δσ + δpσ − 1 + 3G 2 σe σe σe Also, from (5.16), we may write δσe + 3Gδp = δσetr .

(5.23)

The yield condition is written as δf = δσe − δr = 0 so that for linear hardening, δσe = δr = hδp, where δp is not the plastic strain in the increment, but an inﬁnitesimal quantity, so that we may write δσe = δr = hδp. Combining with (5.23) gives hδp + 3Gδp = δσetr so δp = Combining with (5.23) gives

δσetr . h + 3G

δσe = δσetr 1 −

3G . h + 3G

(5.24)

(5.25)

We now use (5.25), (5.24), and (5.19) in Equation (5.22) to eliminate δσe , δp, and p respectively to give (after some algebra) σetr δσetr σetr

σ = δσ tr . σe − δσ + (5.26) σe σe σe 1 + (3G/ h) Consider the term, 1/2 −1/2 3 tr

3 tr

1 3 tr

3

= σ : σ tr σ : σ tr δσ : σ tr + σ tr : δσ tr δσetr = δ 2 2 2 2 2 3 1 tr

tr

σ : δσ . = 2 σetr

152

Implicit and explicit integration

Substituting this together with the expression for σ in Equation (5.14) into (5.26) gives

σe 3 1 σe σ tr σ tr

(5.27) δσ = : δσ tr + tr δσ tr . − tr σe 2 1 + (3G/ h) σe σetr σetr If we write 3 1 σe σe Q= − tr and R = tr 2 1 + (3G/ h) σe σe then (5.27) becomes

σ tr σ tr

δσ = Q tr tr + RI : δσ tr . (5.28) σe σe Remember that in deriving the Jacobian, we are trying to relate δσ to δε. We may write the deviatoric trial stress in terms of the deviatoric trial strain using Hooke’s law (because the trial stress is obtained assuming elasticity) as 1 tr

tr

tr tr δσ = 2Gδε = 2G δε − II : δε 3 and δεtr ≡ δε 1 δσ = 2G δε − II : δε . 3 Substituting into Equation (5.28) gives

1 σ tr σ tr

δσ = Q tr tr + RI : 2G δε − II : δε 3 σe σe

so

tr

σ tr σ tr 1 σ tr σ tr 2 = 2GQ tr tr : δε − Q tr tr : (II : δε) + 2GRδε − GRI : (II : δε). 3 σe σe 3 σe σe

The second term of the right-hand side is zero since σ tr is deviatoric so

σ tr σ tr σ tr σ tr : (II : δε) = : I Tr(δε) = 0 σetr σetr σetr σetr and therefore δσ = 2GQ

σ tr σ tr 2 : δε + 2GRδε − GRII : δε tr tr σe σe 3

since I : I = I . Finally, the stress is given in terms of its deviatoric by 1 δσ = δσ + II : δσ = δσ + KII : δε e = δσ + KII : (δε − δε p ) 3

= δσ + KII : δε.

(5.29)

Material Jacobian

153

Substituting into (5.29) gives

σ tr σ tr 2 δσ = 2GQ tr tr : δε + 2GRδε + K − GR II : δε. σe σe 3

We may write this in the shortened form as

σ tr σ tr 2 δσ = 2GQ tr tr + 2GRI + K − GR II σe σe 3

(5.30)

: δε.

(5.31)

Equation (5.30) provides the Jacobian or the material tangent stiffness matrix. In this case, because it has been derived from the implicit backward Euler integration scheme, which is used to integrate the plasticity constitutive equations, it is called the consistent tangent stiffness. Let us determine some of the terms using (5.30).

δσ11 = 2GQ

tr σ11 1 tr σe σetr

tr tr tr tr tr tr × (σ11 δε11 + σ22 δε22 + σ33 δε33 + 2σ12 δε12 + 2σ13 δε13 + 2σ23 δε23 ) 2 + 2GRδε11 + K − GR (δε11 + δε22 + δε33 ). 3 The ﬁrst term of the Jacobian is, therefore,

tr

σ tr σ11 ∂δσ11 2 D11 = GR = 2GQ 11 + 2GR + K − ∂δε11 3 σetr σetr

and the next is D12

tr σ tr

σ11 ∂δσ11 2 22 = = 2GQ tr tr + K − GR ∂δε22 σe σe 3

and so on. A shear term is given by tr 2σ tr

tr σ tr

σ12 σ12 ∂δσ12 1 ∂δσ12 1 12 D44 = 2GQ tr tr + 2GR = 2GQ tr 12 = = + GR ∂δγ12 2 ∂δε12 2 σe σe σe σetr and D14 is

tr σ tr σ12 ∂δσ11 1 ∂δσ11 = = 2GQ 11 . D14 = ∂δγ12 2 ∂δε12 σetr σetr For conditions of axial symmetry (so that the out of plane shears, σ13 , ε13 and σ23 , ε23 do not exist) therefore, the Jacobian is the symmetrical matrix ⎞ ⎛ D11 D12 D13 D14 ⎜ ∂δσ D22 D23 D24 ⎟ ⎟. =⎜ ⎝ D33 D34 ⎠ ∂δε D44

154

Implicit and explicit integration

5.4

Kinematic hardening

In this section, we shall use implicit (backward Euler) integration for the case of linear kinematic hardening, and obtain the consistent tangent stiffness. We will then go on to address combined linear kinematic hardening with non-linear isotropic hardening, and to introduce combined non-linear kinematic and isotropic hardening. We will ﬁnish by introducing semi-implicit integration schemes for plasticity. 5.4.1

Linear kinematic hardening

With the backward Euler scheme, as given in Section 5.2.1.2 for isotropic hardening, Hooke’s law may be written in its predictor–corrector form as σ = σ tr − 2Gpn

(5.32)

in which σ tr is the elastic trial stress. We employ linear kinematic hardening so that the back stress increment is given by 2 cεp 3 and as a result, if we write the back stress at time, t, as x t , then at the end of the time step, t + t, it becomes 2 x = x t + cεp (5.33) 3 and with the normality hypothesis for von Mises plasticity, x =

2 x = x t + cpn, 3

(5.34)

where

3 σ − x (5.35) 2 σe for kinematic hardening, in which x is, of course, itself deviatoric, and p is the increment in effective plastic strain. Combining (5.35) and (5.34) gives n=

2 2 σ = x t + pcn + σe n. 3 3 The deviatoric stress is

1 σ = σ − II : σ 3 so that with (5.32), we may write (5.36) as 1 2 2 σ tr − 2Gpn − II : σ = x t + pcn + σe n. 3 3 3

(5.36)

Kinematic hardening

155

We saw earlier that we may write 1

σ tr − II : σ ≡ σ tr 3 so that

2 2

σ tr − 2Gpn = x t + pcn + σe n. 3 3 Taking the contracted product of both sides of (5.37) with n gives 2 2 tr

(σ − x t ) : n = n : n 2Gp + pc + σe 3 3 and 3 σ − x 3 σ − x 3 3

n:n= (σ − x) : (σ − x) . : = 2 σe 2 σe 2σe2 2 But the effective stress, σe , is deﬁned by 1/2 3

σe = (σ − x) : (σ − x) 2 so that 3 n:n= . 2 Equation (5.38) therefore reduces to

(σ tr − x t ) : n = 3Gp + pc + σe . From (5.32) we may write

(5.37)

(5.38)

(5.39)

σ = σ tr − 2Gpn

so that from (5.35), we may write n as

3 σ tr − 2Gpn − x 3 σ tr − 2Gpn − x t − (2/3)cpn n= = . 2 σe 2 σe Rearranging this equation for n gives

3 σ tr − x t n= 2 σe + 3Gp + cp

(5.40)

and substituting into (5.39) gives 1/2 3 tr

tr

(σ − x t ) : (σ − x t ) ≡ σetr = 3Gp + pc + σe . (5.41) 2 Note that the effective trial stress is determined with respect to the back stress taken at time, t, rather than at the end of the time increment. Rearranging this equation gives p =

σetr − σe . 3G + c

(5.42)

156

Implicit and explicit integration

The yield function for the case of kinematic hardening is f = σe − σy = 0

(5.43)

so that σe = σy . In Equation (5.42), therefore, for the case of linear kinematic hardening, none of the terms depends upon the effective plastic strain. Equation (5.42) is therefore an exact, closed-form expression for p and in this instance, no iteration is required for its determination. Plastic and elastic strains and the stress may then be updated using (5.42) to give

3 σ tr − x t n= . 2 σetr εp = pn, p

εp = εt + ε p , ε e = εet + ε e = εet + ε − ε p , σ = 2Gεe + λII : εe . 5.4.1.1 Consistent tangent stiffness for linear kinematic Hardening. In implicit ﬁnite element code, in addition to the integration of the plasticity constitutive equations, it is also necessary to provide the material Jacobian—the tangent stiffness matrix. Here, we determine the consistent (i.e. with the implicit integration given above) tangent stiffness for linear kinematic hardening. Using (5.40) and (5.41), n may be written as

3 σ tr − x t n= . 2 σetr We have therefore

σ =σ

tr

− 2Gpn = σ

tr

3 − 2Gp 2

σ tr − x t σetr

and substituting for p from (5.42) gives

tr

tr 3 σ − σ − x σ

e t σ = σ tr − 2G e 3G + c 2 σetr and after a little algebra, we obtain 1 − σe /σetr c/3G + σe /σetr

+ xt . σ = σ tr 1 + c/3G 1 + c/3G

Kinematic hardening

157

Applying the differential operator, and rearranging, we obtain (1 + c/3G)

σetr

δσ = δσ tr (1 + (c/3G)(σetr /σe )) σe

+ σ tr (δσe /σe − δσetr /σetr ) − (δσe /σe − δσetr /σetr )x t . From the yield function in (5.43), δf = δσe = 0 so this reduces to (1 + c/3G)

σetr

δσ = δσ tr (1 + (c/3G)(σetr /σe )) − (σ tr − x t )(δσetr /σetr ). σe (5.44)

Now,

σetr so

1/2

3 tr

(σ − x t ) : (σ tr − x t ) = 2

−1/2 3 tr

1 3 tr

3 tr

tr

tr

tr

(σ −x t ) : (σ −x t ) (σ −x t ) : δσ + δσ : (σ −x t ) = 2 2 2 2 1 3

= tr (σ tr − x t ) : δσ tr . σe 2

δσetr

Substituting into (5.44), and writing Q=

σe /σetr + c/3G 1 + c/3G

gives

δσ = Qδσ

tr

δσ

1 3 σe tr 2 σe 1 + c/3G

(σ tr − x t ) (σ tr − x t )

+R : δσ tr . tr tr σe σe

As before, tr

R=−

1 = 2G δε − II : δε 3

so that

(σ tr − x t ) (σ tr − x t ) 2 : δε − GQII : δε δσ = 2GQδε + 2GR tr tr σe σe 3

and ﬁnally, δσ = 2GQδε + 2GR

2 (σ tr − x t ) (σ tr − x t ) GQ II : δε : δε − K − σetr σetr 3 (5.45)

which gives the consistent tangent stiffness.

158

5.4.2

Implicit and explicit integration

Combined isotropic and linear kinematic hardening

The isotropic hardening evolution equation is dr = h dp in which h can be a function of p so that r is not necessarily linear, and for the linear kinematic hardening, 2 dx = c dεp . 3 Because of the assumption of linearity, as before we may write 2 x = x t + cpn 3 and from Section 5.4, we have σe = σetr − (3G + c)p in which σetr and σe are given by 1/2 3 tr

tr

tr σe = , (σ − x t ) : (σ − x t ) 2

(5.46) 1/2

3

(σ − x) : (σ − x) σe = 2

.

The yield function is f = σe − r − σy = 0 which becomes, after substituting (5.46) f = σetr − (3G + c)p − r − σy = 0.

(5.47)

In this case, r depends on h which may, for non-linear hardening, depend on p and the equation can be non-linear. We use Newton’s method to solve it by writing f+

∂f dp = 0 ∂p

and substituting (5.47) gives dp =

σetr − (3G + c)p − r − σy . 3G + c + h

(5.48)

Let us simplify it for the cases of linear kinematic hardening and isotropic hardening only to compare with the previous equations. If there is no isotropic hardening, then r = h = 0 and (5.48) becomes dp =

σetr − (3G + c)p − σy 3G + c

(5.49)

Kinematic hardening

159

and for linear kinematic hardening, σe = σetr − (3G + c)p and σe = σy so (5.49) gives dp = 0. That is, there is no iteration required and p is given by σetr − σy 3G + c

p =

as before. If there is no kinematic hardening, x = 0 and c = 0 so (5.49) becomes dp = where

σetr − 3Gp − r − σy , 3G + h

1/2 3 tr

tr

= σ :σ 2 which is what we obtained before in Section 5.2.1.

σetr

5.4.3

Introduction to implicit integration of combined non-linear kinematic and isotropic hardening

In the previous sections in which we assumed linear kinematic hardening, we wrote the kinematic hardening variable in terms of its value at the start of the increment, x t , and the incremental value. As a result, subsequent equations were set up in terms of x t . Here, we will now introduce the more general case of non-linear kinematic hardening, and will ﬁnd the equations depending on quantities at the end of the time increment. As before, the deviatoric stress can be written in predictor–corrector form in terms of the trial stress and plastic return as

σ = σ tr − 2Gpn

(5.50)

and the normal, n, is given by

3 σ − x . 2 σe Combining these equations and after a little algebra, we obtain 2 tr

(σ − x) : n = σe + 2Gp n : n 3 n=

(5.51)

and we have shown before that n : n = 23 , so

(σ tr − x) : n = σe + 3Gp.

(5.52)

160

Implicit and explicit integration

We can also obtain from (5.50) and (5.51)

n=

3 σ tr − 2Gpn − x 2 σe

so that rearranging,

3 σ tr − x . n= 2 σe + 3Gp Combining with (5.52) gives σe = σetr − 3Gp, where

1/2

σetr

(5.53)

3 tr

(σ − x) : (σ tr − x) = 2

.

(5.54)

The yield function is f = σe − r − σy = σetr − 3Gp − r − σy = 0

(5.55)

with σetr given by (5.54). Note now that because x depends on p (non-linearly for the case of non-linear kinematic hardening) as may r, Equation (5.55) is a non-linear equation in p for which we will need to use Newton’s iterative solution method, for which we obtain dp = and

σetr

(k)

− 3Gp (k) − r (k) − σy (k)

3G + (∂r (k) /∂p) − (∂σetr /∂p)

(5.56)

p(k+1) = p(k) + dp.

Both σetr and r are the two derivatives with respect to p need to be updated at every iteration for a fully implicit integration. Often, with complex plasticity hardening laws, this may be challenging. A simpler approach is to integrate the effective plastic strain implicitly but to update the normal n and the internal variables—the isotropic and kinematic hardening—explicitly. Such an approach is called semi-implicit integration. 5.4.4

Semi-implicit integration of combined non-linear kinematic and isotropic hardening

In the semi-implicit scheme, Newton’s method is used to determine the effective plastic strain increment using Equation (5.56) and the yield function (5.55) written at the end of the time increment ensures that drift from the yield surface does not occur. However, the updates of all other quantities are carried out explicitly as follows: (k+1)

εp

= p(k+1) nt ,

Implicit integration in viscoplasticity

where nt = (k+1)

εp εe

(k+1)

161

3 σ t − x t , 2 σet (k+1)

p

= εt + ε p

(k+1)

= ε − εp

σ (k+1) = 2Gε

e(k+1)

,

,

+ λII : εe

(k+1)

,

r (k+1) = rt + r, x (k+1) = x t + x, where, for example, the non-linear kinematic hardening increment, x, is given by 2 (k+1) + γ x t p(k+1) x = cεp 3 and the isotropic hardening increment by r = b(Q − r)p(k+1) if the non-linear evolution equations given in Chapter 2 are adopted, and 1/2 3 tr

(k+1) tr

(k+1) tr (k+1) σe ) : (σ − x ) . (σ − x = 2 The semi-implicit scheme is not unconditionally stable and we need to be concerned, therefore, about both stability and accuracy when using it.

5.5

Implicit integration in viscoplasticity

We saw in Chapter 2 that the plastic strain rate can be written, for a viscoplastic von Mises material, as ∂f ε˙ p = p˙ ∂σ in which, for viscoplasticity, p˙ is now speciﬁed by a constitutive equation (as opposed to being determined by the consistency condition) which, for both isotropic and kinematic hardening, can be written as p˙ = φ(σ , x, r). We may write this incrementally as p = φ(σ , x, r)t = φt. For both kinematic and isotropic hardening, the yield function is f = J (σ − x ) − r − σy .

(5.57)

162

5.5.1

Implicit and explicit integration

Uniaxial viscoplasticity equations

We will present implicit backward Euler integration for the uniaxial form of the equations ﬁrst, for simplicity, and we start from the viscoplastic constitutive equation. Equation (5.57) may be written in uniaxial form, if we consider isotropic hardening only for now, as p = φ(σe , r)t (5.58) and we may write this in a form suitable for Newton’s iterative solution as ψ = p − φ(σe , r)t = 0.

(5.59)

In preparation for differentiation, we may write the stress in terms of p by remembering (5.16) σe + 3Gp = σetr (5.60) so that (5.59) becomes ψ(p, r) = p − φ(p, r)t = 0.

(5.61)

Using Newton’s method, we have ψ+

∂ψ ∂ψ dp + dr = 0 ∂p ∂r

and differentiating (5.61) and substituting into (5.62) gives ∂φ ∂φ t dp − t dr = 0. p − φt + 1 − ∂p ∂r

(5.62)

(5.63)

We will write, from here on, φp =

∂φ ∂p

and

φr =

∂φ ∂r

and similarly for other derivatives. If we assume for now linear isotropic hardening, then dr = h dp = h dp. Substituting into (5.63) and rearranging gives dp =

φ(p, r) − p/t . 1/t − φp − hφr

(5.64)

As an example, let us consider a particular viscoplasticity constitutive equation, given by p˙ = φ(σe , r) = α sinh β(σe − r − σy ) in which σy , α, and β are material constants. Using (5.59) this becomes p˙ = φ(p, r) = α sinh β(σ tr − 3Gp − r − σy )

Implicit integration in viscoplasticity

163

and the required derivatives are φp = −3Gαβ cosh β(σ tr − 3Gp − r − σy ) and φr = −αβ cosh β(σ tr − 3Gp − r − σy ) so that (5.64) gives dp =

α sinh β(σ tr − 3Gp − r − σy ) − p/t 1/t +3Gαβ cosh β(σ tr −3Gp−r −σy )+hαβ cosh β(σ tr −3Gp−r −σy )

with r = rt + hp. As before in rate-independent plasticity, an iterative procedure is used to determine p from p(k+1) = p(k) + dp. 5.5.2

Multiaxial viscoplasticity

For the case of isotropic hardening, Equation (5.64) still holds for the multiaxial case, and the plastic strain tensor increment can then be determined from

σ

σ tr 3 3 ε = pn = p ≡ p tr

2 σe 2 σe p

so that the elastic strain and hence stress increments can be determined in the usual way. We shall next consider combined multiaxial linear isotropic and kinematic hardening such that the constitutive equation is written as p˙ = φ(p, x, r) in which x is the tensorial kinematic hardening variable. The problem may be written, as before, ψ(p, x, r) = p − φ(p, x, r)t = 0 and

∂ψ ∂ψ ∂ψ dp + : dx + dr = 0. ∂p ∂x ∂r We may write the derivatives as ψ+

∂ψ = 1 − φp t, ∂p

∂ψ = −φ x t, ∂x

∂ψ = −φr t ∂r

(5.65)

164

Implicit and explicit integration

so that (5.65) becomes p − φt + (1 − φp t) dp − φ x : dxt − φr drt = 0.

(5.66)

Let us write the linear isotropic and kinematic hardening equations as dr = h dp = h dp, 2 2 c dεp = c dpn 3 3 so that substituting into (5.66) and rearranging gives dx =

dp =

φt − p . 1 − φp t − hφr t − (2/3)cφ x : nt

(5.67)

If we consider again a viscoplastic constitutive equation with kinematic and isotropic hardening of the form p˙ = φ(σ , x, r) = α sinh β(J (σ − x ) − r − σy ) = α sinh β(σe − r − σy ), then

3 σ − x

∂φ ∂σe = −φσe = −φσe n ∂σe ∂x 2 J (σ − x ) and the term φ x : n may be simpliﬁed to φx = −

3 φ x : n = −φσe n : n = − φσe . 2 Substituting into (5.67) gives dp =

φ − p/t 1/t − φp − hφr + cφσe

(5.68)

which is solved iteratively. The plastic strain increment is then determined from

σ − x

3 σ tr − x

3 ε = p ≡ p . 2 J (σ − x ) 2 σetr p

5.5.3

Consistent tangent stiffness for viscoplasticity with isotropic hardening

The predictor–corrector form of the stress is

σ = σ tr − 2Gpn or where

σ = σ tr − 2Gpn,

(5.69)

3 σ tr 3 σ

n= = 2 σetr 2 σe

(5.70)

Implicit integration in viscoplasticity

165

and σe = σetr − 3Gp. Rearranging (5.70) gives

σe tr

σ σetr

σ = and applying the differential operator σe

δσ = tr δσ tr + σe

δσe σe δσetr − σetr σetr σetr

σ tr .

(5.71)

Now, δσetr =

1 3 tr

σ : δσ tr tr σe 2

(5.72)

and

1 3

σ : δσ . (5.73) σe 2 Substituting (5.72) and (5.73) into (5.71) and eliminating σ using (5.70) gives δσe =

3 σ tr σ tr σe tr

σe 3 σ tr σ tr

: δσ + δσ − : δσ tr . δσ = tr tr tr tr tr tr 2 σe σe σe σe 2 σe σe

Because of the contracted product of δσ in the ﬁrst term on the right-hand side, we will substitute for this using the differential form of (5.50)

δσ = δσ tr − 2Gδpn to give

3 σ tr σ tr σe tr

σe 3 σ tr σ tr

tr

: (δσ − 2Gδpn) + δσ − : δσ tr tr tr tr tr tr tr 2 σe σe σe σe 2 σe σe

3 σ tr σ tr σe tr

σe 3 σ tr σ tr

=− : 2Gδpn + tr δσ + 1 − tr : δσ tr . tr tr tr tr 2 σe σe σe σe 2 σe σe

δσ =

Now,

3 σ tr 3 :n=n:n= tr 2 σe 2 so

σ tr σe tr

σe 3 σ tr σ tr

: δσ tr . δσ = − tr : 3Gδpn + tr δσ + 1 − tr tr tr σe σe σe 2 σe σe

(5.74)

The viscoplastic constitutive equation is written as, from (5.57), p = φ(σ , r) t

(5.75)

166

Implicit and explicit integration

so that δp = (φσ : δσ + φr δr) t.

(5.76)

Let us assume isotropic hardening of the form δr = q(r)δp. Because δp is again an inﬁnitesimal increment in p (as opposed to the plastic strain increment), this can be written as δr = q(r)δp.

(5.77)

Substituting this together with the second equation of (5.69) for δσ into (5.76) gives δp = (φσ : (δσ tr − 2Gδpn) + φr q(r)δp)t and rearranging δp =

φσ : δσ tr . 1/t + 2Gφσ : n + φr q(r)

(5.78)

Substituting into (5.74) gives δσ = −

σe tr

σe 3 σ tr σ tr σ tr φσ : δσ tr

n+ δσ + 1− : δσ tr . : 3G σetr 1/t +2Gφσ : n+φr q(r) σetr σetr 2 σetr σetr

Let us write 3G α=− , 1/t + 2Gφσ : n + φr q(r) then

σe 3 1 − tr , γ = 2 σe

σe β = tr , σe

σ tr σ tr σ tr

δσ = α tr φσ : δσ tr + βδσ tr + γ tr tr : δσ tr . σe σe σe

(5.79)

Now, 2

δσ tr = 2Gδε = 2Gδε − G(δε : I )I . 3 Because φ is a function of the effective stress, its derivatives with respect to the stress

components are deviatoric, and hence φσ : δσ tr = φσ : (δσ tr + (1/3)δσ tr : II ) =

φσ : δσ tr since φσ : I = 0. In addition, δσ = δσ + KII : δε so that (5.79) becomes

σ tr σ tr 2 σ tr δσ = 2Gα tr φσ + K − Gβ II + 2Gγ tr tr σe 3 σe σe which gives the consistent tangent stiffness.

: δε + 2Gβδε

(5.80)

Incrementally objective integration for large deformations

5.6

167

Incrementally objective integration for large deformations

So far, we have addressed the update of stress over a given time increment on the basis that there is no incremental rotation. In large deformation analyses, however, in which deformations and rigid body rotations can become large, we need to take account of the effect of incremental rotation on the determination of the updated stress. Figure 5.1 shows the representation of a body in its original conﬁguration and then in deformed conﬁgurations at times t and t + t. In the deformed conﬁgurations, the local material (or co-rotational) coordinate systems are shown indicating that an incremental rotation has occurred between the conﬁgurations at times t and t + t. We need to ensure that the stress update is carried out with respect to the same reference frame. For example, in using a userdeﬁned subroutine for plasticity in ABAQUS, the user is supplied with the strains at the beginning and end of the time increment, together with the stress at the beginning of the time increment, but all these quantities and other tensor quantities have usually already been incrementally rotated to account for the incremental rigid body rotation. We shall return to this in Chapter 6. For now, however, we shall look at an incrementally objective stress update. First, referring to Fig. 5.2, let us assume we know the stresses, σ t , at time t with respect to the material reference frame, that is, the undeformed conﬁguration at that time. Also, we have determined the spin, W , given by the antisymmetric part of the velocity gradient. The stress rate, σ˙ , with respect to the material reference frame, or undeformed conﬁguration, at time t, taking full account of the incremental rigid body rotation, is

Deformed configuration at t

Deformed configuration at t + ∆t

Undeformed (original) configuration y Ft y

y⬘ x

Y

x

X

x⬘

F t + ∆t

Fig. 5.2 A body in its original (undeformed) conﬁguration and in deformed conﬁgurations at times t and t + t.

168

Implicit and explicit integration

given by

∇

σ˙ = σ +W t σ t − σ t W t

(5.81)

so that the updated stress (written explicitly) with respect to the undeformed conﬁguration at time t is simply σ t+t = σ + σ˙ t. We can write Equation (5.81) in incremental form, if we wish, as ∇

σ = σ + (W t σ t − σ t W t )t

(5.82)

which we may also write as ∇

σ = σ + Rσ t R T

(5.83)

∇

in which σ is the increment in objective, or co-rotational, stress, and R is a rotation to be determined. We shall further consider these approaches in Chapter 6, concerned with the implementation of plasticity models into ﬁnite element code.

Further reading Bathe, K.-J. (1996). Finite Element Procedures. Prentice Hall, New Jersey, revised edition. Belytschko, T., Liu, K.W., and Moran, B. (2000). Nonlinear Finite Element Analysis for Continua and Structures. John Wiley & Sons, New York. Simo, J.C. and Hughes, T.J.R. (1998). Computational Inelasticity. Springer-Verlag, New York. Chaboche, J.-L. (1986). ‘Time-independent constitutive theories for cyclic plasticity’. International Journal of Plasticity, 2(2), 149–188. Hughes, T.J.R. (1984). ‘Numerical implementation of constitutive models: rateindependent deviatoric plasticity’. In Nemat Nasser S., Asaro R.J., and Hegemier G.A. (eds), Theoretical Foundation for Large-Scale Computations of Non-linear Material Behaviour, Martinus Nijhoff Publication, The Netherlands, 29–57. Krieg, R.D. and Key, S.W. (1976). ‘Implementation of a time dependent plasticity theory into structural computer programs’, In Constitutive Equations in Viscoplasticity: Computational and Engineering Aspects (eds) Stricklin J.A. and Saczalski K.J.), ASME.

6. Implementation of plasticity models into ﬁnite element code

6.1

Introduction

Several commercial ﬁnite element software packages (e.g. ABAQUS, LSDyna, and MARC) provide the facility for users to specify their own material models. In ABAQUS, the user is required to provide a Fortran subroutine called a ‘UMAT’. This chapter is concerned with the implementation of plasticity models into ﬁnite element code, which is carried out, by example, in using ABAQUS. In particular, we start by developing an ABAQUS UMAT for elasticity, and discuss the tests necessary to verify the model implementation into ABAQUS. We go on to consider isotropic hardening plasticity with explicit and implicit integration, with continuum and consistent tangent stiffnesses, large deformation formulations using rotated variables provided by ABAQUS, and from ﬁrst principles using the deformation gradient. We use the problem of simple shear with elasticity to verify the large deformation implementations. We then present an implicit implementation for elasto-viscoplasticity (and creep). All the Fortran coding, together with the necessary ABAQUS input ﬁles, are available through the OUP website. Finite element code is often modular in structure, whether it be commercial code or written in-house. An important module is that relating to material behaviour; in other words, the constitutive stress response of the material given prescribed conditions of deformation. In ABAQUS, but in a similar way for all codes, a range of information is passed into the material module relating to both the beginning and end of a time increment. In particular, stress, strain, and deformation gradient are provided at the beginning of the time increment. Strain and the deformation gradient are also provided at the end of the increment. Within the module, it is then necessary to execute three tasks. First, the stresses at the end of the time increment must be determined and, second, for the case of an implicit analysis (i.e. the ﬁnite element momentum balance or equilibrium equations are solved implicitly) using ABAQUS standard, for example, the material Jacobian, or tangent stiffness, must also be provided. Third, any state variables (such as the isotropic hardening variable or effective plastic strain) must

170

Implementation of plasticity models

be updated to the end of the time increment. In fact, in coding an ABAQUS UMAT, a large range of information is provided, some of which will be referred to later. However, the job of the UMAT is clear: to update the stresses and state variables to the end of the time increment and to provide the Jacobian. We start by addressing elasticity.

6.2

Elasticity implementation

We discuss elasticity and its implementation into a UMAT for two main reasons. First, it provides a good introduction to writing and testing a UMAT subroutine for those who are new to the process. Second, it provides a basis from which elastoplasticity models may be developed. For the latter reason, while is no way essential for elasticity, we use an incremental approach in implementing the linear elastic equations. In Chapter 5, Hooke’s law was given in an incremental form in Equation (5.21) together with the material Jacobian, for the case in which there are no out of plane shears (e.g. plane strain and axisymmetric problems). With knowledge of the increment in strains (provided to the UMAT), together with the speciﬁcation of elastic constants (we shall take E = 210 GPa and ν = 0.3 throughout), the stress increment is obtained either from Equation (5.21), or its equivalent written in Voigt notation, ⎛ ⎞⎛ ⎞ 2G + λ λ λ 0 ε11 ⎜ λ ⎜ ⎟ 2G + λ λ 0⎟ ⎟ ⎜ε22 ⎟ . σ = Cεe = ⎜ (6.1) ⎝ λ ⎠ ⎝ λ 2G + λ 0 ε33 ⎠ 0 0 0 G γ12 Because ABAQUS provides most tensor quantities in vector (Voigt) form, it may be more convenient to use Equation (6.1) than the tensor form given in (5.21). However, this is not always the case, and later we shall use the tensor form in preference, particularly where it is necessary to work from the deformation gradient. Note that the shear strain quantities provided by ABAQUS are always engineering shears, that is, twice the tensorial shear strains. It is also important to check the ordering of shear quantities, which can vary depending on element type used. Equation (6.1) is suitable for plane strain and axisymmetric problems, but not for problems of plane stress or three dimensions, for which different stiffness matrices are required. For linear elasticity, the material Jacobian is just the elastic stiffness matrix so that speciﬁcation of the Jacobian in the UMAT is easy. The coding required for the UMAT for linear elasticity for plane strain, axisymmetric, and three-dimensional problems, is available through the OUP website. A complete list of all the UMAT coding, together with ABAQUS input ﬁles, is given in Appendix B.

Veriﬁcation of implementations

6.3

171

Veriﬁcation of implementations

The veriﬁcation of the model implementation is vital. For complex material models, this requires the development of an independent solver (which will often be numerical) for uniaxial and pure shear problems so that direct comparison with the results obtained using the UMAT can be made. In addition, it is necessary to test the UMAT using a single, and where appropriate, multiple elements, for conditions of strain control and load control under uniaxial and pure shear conditions. If possible, perhaps by ‘switching off’ parts of the model implemented into the UMAT, make comparisons with a multiaxial problem with non-uniform strain and stress distributions for which the solution is known (either an independent solution or one obtained using an internal ABAQUS model). In this chapter, we shall not carry out all of the veriﬁcation tests described for all the model implementations, but it is certainly advisable to do so for new model implementations into UMATs. Because of their importance, we go through some of the possible veriﬁcation tests step by step. 1. Single and multiple element uniaxial tests. Figure 6.1 shows an axisymmetric single- and four-element unit square which is subjected to uniaxial displacement or force control in the z-direction producing uniform, uniaxial stress, σzz , and strain, εzz , with εrz = σrr = σθ θ = σrz = 0, which can be compared with independent closed-form solutions. The four-element problem is important since it introduces a ‘free’ node, which does not exist for the single four-noded axisymmetric element. The force controlled test is important for checking errors in the Jacobian. 2. Single element simple shear test. The uniaxial tests in (1) do not involve the shear terms at all, so it is important to include a problem which tests these terms, particularly because of the potential for errors with the use of engineering shear strains rather than their tensorial counterparts. Figure 6.2 shows a plane strain single-element unit square under simple shear loading. For small deformations, εxx = εyy = σxx = σyy = 0,

Displacement or force

Displacement or force z

z 1.0

1.0

ur = 0.0

ur = 0.0

0.0

0.0 0.0

1.0 r

uz = 0.0

0.0

1.0 r uz = 0.0

Fig. 6.1 Schematic diagram showing an axisymmetric single- and four-element unit square under uniaxial displacement or force controlled loading.

172

Implementation of plasticity models g y 1.0

0.0 0.0

1.0 x ux = uy = 0.0

Fig. 6.2 Schematic diagram showing a plane strain single-element unit square under simple shear loading.

and uniform shear strain, γxy , and stress, σxy , are produced which can be compared with independent closed-form solutions. 3. Non-uniform strain and stress ﬁeld. Often, a comparison test which generates non-uniform strain and stress ﬁelds will not be possible because a comparison may well not exist, and a closed-form solution is now no longer possible. However, it is sometimes possible to simplify the implemented plasticity model (e.g. by turning off the porosity in a Gurson-type porous plasticity model) such that a comparison with another solution (e.g. produced using one of the many built-in models contained within ABAQUS) is then possible. While this will not test all the features of the model implemented into the UMAT, it nonetheless may test a good number of them, and may therefore be worthwhile. Later in the chapter, both an implicit and explicit implementation of isotropic hardening plasticity are tested in this way by comparing the results obtained with those produced using the built-in ABAQUS model.

6.4

Isotropic hardening plasticity implementation

In Chapter 5, we presented both explicit and implicit integration of the equations for linear strain hardening isotropic plasticity, together with the consistent tangent stiffness for the implicit scheme. We will implement both integration schemes into ABAQUS UMATs and discuss the advantages and disadvantages of each. We start with the explicit scheme which was described at the beginning of Section 5.2, and introduce the continuum Jacobian.

6.4.1

Explicit integration for isotropic hardening plasticity with continuum Jacobian

We may summarize the implementation as follows. All quantities are assumed to be given at time, t, that is, at the start of the time increment, unless indicated

Isotropic hardening plasticity implementation

173

otherwise: (i) Determine the yield function

f = σe − r − σy =

3

σ : σ

2

1/2 − r − σy .

(6.2)

(ii) Determine if actively yielding Is

f > 0?

(iii) Determine the plastic multiplier n · C dε , n · Cn + h f < 0, dλ = 0.

f > 0,

dλ =

(6.3)

(iv) Determine stress and isotropic hardening increments dσ = C dεe = C(dε − dλn), dr = h dp = h dλ.

(6.4)

(v) Update all quantities to the end of the time increment, using explicit integration σt+t = σ + dσ, p

εt+t = εp + dεp ,

(6.5)

rt+t = r + dr. (vi) Determine Jacobian. (vii) End. We now address the determination of the Jacobian. In Chapter 5, we derived the consistent tangent stiffness for the implicit integration scheme. For the purposes of the explicit integration considered here, we introduce what is sometimes referred to as the continuum Jacobian. That is, it is not derived explicitly on the basis of the integration scheme, but directly from the constitutive equations. We start from the stress–strain relationship written in Voigt notation dσ = C dεe = C(dε − dλn),

(6.6)

which we may write out fully for conditions of axial symmetry or plane strain as ⎛ ⎞ ⎛ ⎞ ⎛ ⎞ ⎛⎛ ⎞ ⎛ ⎞⎞ dσ11 dσ1 C11 C12 C13 C14 dε1 n1 ⎜dσ22 ⎟ ⎜dσ2 ⎟ ⎜ ⎟ ⎜⎜dε2 ⎟ ⎜n2 ⎟⎟ C C C 22 23 24 ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜⎜ ⎟ − dλ ⎜ ⎟⎟ . ⎝dσ33 ⎠ = ⎝dσ3 ⎠ = ⎝ ⎝n3 ⎠⎠ C33 C34 ⎠ ⎝⎝dε3 ⎠ dσ12 dσ4 sym C44 dε4 n4 (6.7)

174

Implementation of plasticity models

We may write the Jacobian (here symmetric) as ⎛ J11 J12 ∂ dσ ⎜ J22 J = =⎜ ⎝ ∂ dε sym

J13 J23 J33

⎞ J14 J24 ⎟ ⎟ J34 ⎠ J44

(6.8)

so that, for example, the ﬁrst term is J11 =

∂ dσ1 ∂ dλ = C11 − (C11 n1 + C12 n2 + C13 n3 + C14 n4 ). ∂ dε1 ∂ dε1

With some algebra we may show, therefore, that ∂ dλ , (6.9) ∂ dε where ⊗ is the dyadic product of two vectors, details of which may be found in Appendix A. In a similar way, by considering the numerator of the plastic multiplier given in Equation (6.3), we may show that J = C − Cn ⊗

Cn ∂ dλ = ∂ dε n · Cn + h so that the continuum Jacobian is J =C−

Cn ⊗ Cn . n · Cn + h

(6.10)

The explicit integration and provision of Jacobian is then complete. An ABAQUS UMAT containing this formulation, together with various input ﬁles for uniaxial displacement and load control, together with a four-point beam bending problem, are available via the OUP website (full details are given in Appendix B). In addition, the very same problems are analysed using the built-in ABAQUS linear strain hardening plasticity model (chosen to represent a material with E = 210,000 GPa, ν = 0.3, σy = 240 MPa, and h = 1206 MPa). In all the analyses using the explicit UMAT, the maximum time increment allowed in the analysis is carefully chosen to ensure stability and accuracy. Despite this, at the elastic–plastic transition, the stress at ﬁrst yield is overestimated because the stress at the start of the increment was determined on the basis of elastic behaviour in the previous increment. With an explicit scheme, this is never corrected so that the stresses remain slightly overestimated throughout the analysis. The error in stress can be reduced by decreasing the time increment size, but at the cost of the computer CPU time and error accumulation. In any case, many more time increments are required using the explicit UMAT than are required using the built-in ABAQUS implicit plasticity integration. This is a further serious shortcoming of the explicit integration method, which needs to be weighed against the advantage

Isotropic hardening plasticity implementation

175

of simplicity, particularly for complex constitutive equations. However, despite considerably longer computer CPU times, the results obtained for the four-point bend simulation from the explicit UMAT and the built-in ABAQUS plasticity model are found to be near-identical. We consider an implicit implementation in Section 6.4.2. 6.4.2

Implicit integration for isotropic hardening plasticity with consistent Jacobian

We may summarize the implementation as follows. As opposed to the explicit case, all quantities are now assumed to be given at the end of the time increment, that is, at time t + t, unless otherwise indicated. (i) Determine the elastic trial stress σ tr = σt + 2Gε + λIε : I . (ii) Determine the trial yield function f =

σetr

− r − σy =

3 tr

σ : σ tr 2

(6.11)

1/2 − r − σy .

(6.12)

(iii) Determine if actively yielding Is f > 0? (iv) If yes, use Newton iteration to determine the effective plastic strain increment r (k) = rt + hp, dp =

σetr − 3Gp (k) − r (k) − σy , 3G + h

(6.13)

p (k+1) = p(k) + dp. Otherwise, p = 0. (v) Determine plastic and elastic strain and stress increments

σ tr 3 ε = p tr , 2 σe p

ε e = ε − εp ,

(6.14)

σ = 2Gε + λIε : I . e

e

(vi) Update all quantities to the end of the time increment σ = σt + σ , p = pt + p.

(6.15)

176

Implementation of plasticity models

(vii) Determine consistent Jacobian

σ tr σ tr 2 δσ = 2GQ tr tr : δε + 2GRδε + K − GR II : δε. σe σe 3

(6.16)

(viii) End. An ABAQUS UMAT containing this formulation, together with various input ﬁles for uniaxial displacement and load control, together with a four-point beam bending problem, are available through the OUP website (full details are given in Appendix B). In addition, as before, the very same problems are analysed using the built-in ABAQUS linear strain hardening plasticity model. Using implicit integration with the consistent tangent stiffness eliminates the problem which occurred at the elastic–plastic transition when using explicit integration. In addition, the use of implicit integration enables much larger time increments to be used, therefore signiﬁcantly reducing CPU times. The disadvantage of the implicit formulation is simply the difﬁculty in obtaining the consistent tangent stiffness for complex constitutive equations. Often, analytical forms are simply not obtainable, in which case a numerical procedure may be possible. The results obtained for the four-point bend simulation from the implicit UMAT and the built-in ABAQUS plasticity model are found to be identical.

6.5

Large deformation implementations

We have not yet differentiated between small and large deformation implementations in this chapter. In fact, the UMATs discussed above for both explicit and implicit schemes are suitable for both small and large deformation problems using ABAQUS. This is because the necessary rigid body rotations for the strains and stresses have already been carried out by ABAQUS before they are provided to the UMAT routine. That is, referring back to Section 5.6, the large deformation stress update necessary is ∇

∇

σ = σ + (W σt − σt W )t = σ + Rσt R T ∇

(6.17)

in which σ is the co-rotational stress increment. The stress, σt , at the start of the time increment (and the strain) has already been rotated by ABAQUS (i.e. the stress provided at the start of the time increment is effectively Rσt R T ) so that all we need to do within the UMAT is to carry out the stress update. Sometimes, depending on the plasticity model employed, it is necessary to use internal variables which are also tensor quantities. An example is the back stress in a kinematic hardening model. The components of the back stress will need to be updated within the UMAT ( just like the scalar isotropic hardening variable in the previous sections) and stored in what are called state variable arrays in ABAQUS. Because state variables are not modiﬁed

Large deformation implementations

177

by ABAQUS, it is necessary for the user to carry out the rigid body rotations on tensorial state variables. In fact, ABAQUS provides a utility subroutine to simplify this process. If, for example, the tensorial variable recovered from the state variable array at the start of the increment is, say, x t , then the user must carry out the rigid body rotation Rx t R T before updating x to the end of the time increment within the UMAT. The rotation is carried out by a single call of the utility subroutine rotsig detailed in the ABAQUS manuals. Sometimes, constitutive equations for elasticity and plasticity are formulated in terms of the deformation gradient, F. Examples include hyperelasticity—large strain non-linear elasticity and crystal plasticity. It may be, however, that the user simply wishes to work from the deformation gradient rather than use the strain and stress quantities provided by ABAQUS to the UMAT subroutine. In Section 6.5.1, we present a large deformation implementation based on an explicit scheme.

6.5.1

Implementation using the deformation gradient

We may summarize the implementation as follows. In this explicit approach, all quantities are assumed to be given at time, t, that is, at the start of the time increment, unless indicated otherwise. (i) Determine the velocity gradient L = F˙ F −1 .

(6.18)

(ii) Determine the rate of deformation and spin D=

1 (L + LT ), 2

W =

1 (L − LT ). 2

(6.19)

(iii) Determine the yield function f = σe − r − σy =

3

σ : σ

2

1/2 − r − σy .

(6.20)

(iv) Determine if actively yielding Is

f > 0?

(6.21)

(v) Determine rate of plastic deformation f > 0, f < 0,

D p = as speciﬁed by constitutive equation, D p = 0.

(6.22)

178

Implementation of plasticity models

(vi) Determine rate of elastic deformation and Jaumann stress rate and isotropic hardening rate De = D − Dp, ∇

σ = 2GD e + λID e : I ,

(6.23)

r˙ = h˙ p. (vii) Determine stresses with respect to material reference ∇

σ˙ = σ +W σ − σ W .

(6.24)

(viii) Update all quantities to the end of the time increment, using explicit integration σt+t = σ + σ˙ t,

(6.25)

rt+t = r + r˙ t. (ix) Determine Jacobian. (x) End.

We will next address the veriﬁcation of a large deformation implementation, which is valid for both the implicit and explicit implementations in Sections 6.4.1 and 6.4.2. Note that uniaxial displacement or force controlled loading will not test whether the rigid body rotations are being calculated correctly, since for these cases, the continuum spin, W , is zero. A good test, however, is provided in the form of simple shear if we allow the strains to become quite large. To simplify matters, we will ‘switch off’ the plasticity and allow elasticity only, since the test is being carried out to check the rigid body rotation calculation rather than the constitutive response. We obtained the deformation gradient for simple shear in Section 3.5.1 as 1 δ F = . 0 1 ˙ the velocity gradient is Considering a constant rate of shearing, δ, 0 δ˙ L= 0 0 so that the rate of deformation and spin are 1 0 δ˙ 1 0 D= , W = 2 δ˙ 0 2 −δ˙

δ˙ . 0

Large deformation implementations

179

Note that the spin is non-zero so that rigid body rotation, together with stretch, is occurring. The Jaumann stress rate is given by ∇ 0 δ˙ σ = 2GD + λID : I = G ˙ (6.26) δ 0 and the stress rate with respect to the material (undeformed) reference is σ˙ xx σ˙ xy σ˙ = , σ˙ xy σ˙ yy

(6.27)

which is given in terms of the Jaumann stress rate by ∇

σ˙ = σ +W σ − σ W so that substituting for the spin and (6.26) and (6.27) gives 1 1 −σxy σyy σ˙ xx σ˙ xy σxy 0 1 ˙ ˙ = Gδ + δ − δ 1 0 σ˙ xy σ˙ yy 2 −σxx −σxy 2 −σyy

σxx σxy

so that 1 ˙ yy − σxx ), σ˙ xy = Gδ˙ + δ(σ 2 ˙ xy , σ˙ xx = δσ ˙ xy . σ˙ yy = −δσ

(6.28) (6.29) (6.30)

Equations (6.29) and (6.30) give, with the initial condition that all stresses are zero, σyy = −σxx . Differentiating (6.28) and substituting for (6.29) and (6.30) gives σ¨ xy + δ˙2 σxy = 0, which has solution ˙ + B cos δt. ˙ σxy = A sin δt The initial conditions require that B = 0. Solving for σxx and σyy using Equations (6.29) and (6.30) and imposing the initial conditions gives the solution ˙ σxy = G sin δt,

˙ σxx = −σyy = G(1 − cos δt).

(6.31)

180

Implementation of plasticity models

Stress (GPa)

y

x

150 100 50 0 –50 0.00 –100 –150 –200

sxx sxy 0.20

0.40

0.60

0.80

1.00

Time (s)

syy

Fig. 6.3 Unit square under simple shear at a rate of 5.0 s−1 and the corresponding stresses.

For small strain, δ, at constant strain rate, these reduce to σxy = Gδ

and

σxx = −σyy = 0.

(6.32)

The harmonic variation in (6.31) results from the large deformation, and in particular, the rigid body rotation taking place. This non-physical result arises because we are using a small strain, linear elasticity model under conditions of large deformation. Despite its non-physicality, it provides a good test of the calculation of the rigid body rotations in the large deformation UMAT. In order to do this, a single plane strain element, as shown in Fig. 6.2, has been subjected to simple shear to large strain. This has been carried out using the UMAT with elasticity described in Section 6.2, which uses ABAQUS-provided stresses and strains, a further UMAT based on the deformation gradient, described in this section, and using the built-in elasticity model in ABAQUS. The results obtained are identical and are shown in Fig. 6.3. The various UMATs, together with the ABAQUS input ﬁles, are detailed in Appendix B and are available via the OUP website.

6.6

Elasto-viscoplasticity implementation

Viscoplasticity, meaning rate-dependent plasticity in which the plastic multiplier is determined through the use of a viscoplastic constitutive equation as opposed to the use of the consistency condition, was introduced in Chapter 4. The radial return, implicit backward Euler integration for viscoplasticity was discussed in Chapter 5. Here, we present an implicit implementation for linear isotropic strain hardening elasto-viscoplasticity. Such an implementation can readily be simpliﬁed for the implicit analysis of creep. We employ a sinh-type viscoplastic constitutive equation and for simplicity, use the initial tangent stiffness (i.e. the elastic stiffness) for the material Jacobian. The viscoplastic constitutive equation is taken to be p˙ = φ(σe , r) = α sinh β(σe − r − σy )

Elasto-viscoplasticity implementation

181

and the multiaxial plastic strain increments are given by εp = pn =

σ

3 p . 2 σe

We determine the increment in effective plastic strain as described in Chapter 5 as follows. Note that all quantities are now assumed to be given at the end of the time increment, that is, at time t + t, unless otherwise indicated. (i) Determine the elastic trial stress σ tr = σ t + 2Gε + λIε : I .

(6.33)

(ii) Determine the trial yield function f =

σetr

− r − σy =

3 tr

σ : σ tr 2

1/2 − r − σy .

(6.34)

(iii) Determine if actively yielding Is

f > 0?

(iv) If yes, use Newton iteration to determine the effective plastic strain increment φ(σe , r) = α sinh β(σetr − 3Gp − r − σy ), φp = −3Gαβ cosh β(σetr − 3Gp − r − σy ), φr = −αβ cosh β(σetr − 3Gp − r − σy ), (6.35)

r = rt + hp, dp =

φ(p, r) − (p/t) , (1/t) − φp − hφr

p(k+1) = p(k) + dp. (v) Determine plastic and elastic strain and stress increments

σ tr 3 ε = p tr , 2 σe p

ε e = ε − εp ,

(6.36)

σ = 2Gε + λIε : I . e

e

182

Implementation of plasticity models

(vi) Update all quantities to the end of the time increment σ = σ t + σ , p = pt + p.

(6.37)

(vii) Determine Jacobian. (viii) End. An ABAQUS UMAT containing this formulation, together with various input ﬁles for uniaxial displacement and load control, together with a four-point beam bending problem, are available via the OUP website (full details are given in Appendix B). In addition, uniaxial, closed form implicit and explicit solutions are provided in Fortran programs for veriﬁcation of the implementation.

Part II. Plasticity models

This page intentionally left blank

7. Superplasticity

7.1

Introduction

Superplasticity is the ability of some materials to undergo very large, irreversible, tensile elongations without necking and failing. Generally, a very ﬁne grain structure is required (a typical grain size will be of the order of 1 µm) and a deformation temperature of about 0.5 Tm is necessary to enable the appropriate superplastic deformation mechanisms to operate. Two common superplastically formed classes of material are aluminium and titanium alloys, which are used extensively in the aerospace and aeroengine industry. Superplastic forming exploits the ability of the material to undergo very large tensile elongations in metal sheet stretch forming and blow moulding processes, and has many advantages for the manufacture of complex shapes in sheet metal using simple low pressure pneumatic forming equipment. In this chapter, we shall introduce superplasticity and its characteristics, constitutive equations for superplastic deformation which are coupled with the accompanying microstructural evolution, the multiaxial form of the equations, and an industrial application.

7.2

Some properties of superplastic alloys

Superplasticity is very much a viscoplastic process in the sense that the stress response is highly strain-rate dependent. The uniaxial response to variable constant true strain-controlled loading is simpliﬁed and schematically shown in Fig. 7.1. There is often a very strong strain-rate sensitivity, and in addition, strain hardening is seen to occur. This results from a number of possible causes including the effect of grain growth which occurs in superplasticity, and from dislocation hardening processes. If we choose a particular strain in Fig. 7.1(b) and pick off the corresponding stress for each of the stress–strain curves at all the strain rates, we may then plot log(stress) versus log(strain rate), which often produces a curve of the form shown in Fig. 7.2. Region (i) corresponds to very low strain rates in which diffusion processes dominate when the temperature is higher than ∼0.5 Tm . Region (iii) corresponds to very high

186

Superplasticity «3 •

(a)

(b) «2 «1 •

Stress

Strain

•

s3

«3

s2

«2

s1

«1

•

•

•

sy

Time

Strain

Fig. 7.1 Schematic showing simpliﬁed superplastic stress response which is dependent on strain rate.

ln(stress)

Superplastic region

(i)

(ii)

(iii)

ln(strain rate)

Fig. 7.2 log(stress) versus log(strain) showing the region usually considered to be superplastic.

strain rate at which diffusion is largely inhibited so that deformation occurs through dislocation motion, some of which is perhaps thermally activated, but diminishing with increasing strain rate. Region (ii) is that in which superplasticity takes place; that is, large tensile strains (∼1–2) are achievable which are many times larger than those obtainable in regions (i) and (iii). Because of the approximate linearity in region (ii), the ln(stress)–ln(strain rate) relationship can be written as ln(σ ) = m ln(˙ε ) + k

(7.1)

in which m and k are constants. Rearranging (7.1) gives σ = K ε˙ m

(7.2)

in which K is a further constant. In Equation (7.2), m is called the strain-rate sensitivity and is, of course, the gradient of the ln(stress) versus ln(strain rate) curve. In fact, the higher the value of m, the better the superplastic deformation, and the larger the tensile elongations achievable in the absence of necking and failure. Generally, for what would be described as superplastic deformation, m > 0.35. If, from Fig. 7.2, we now plot the strain-rate sensitivity versus ln(strain rate), we will obtain the graph shown schematically in Fig. 7.3.

Some properties of superplastic alloys

187

Superplastic region m

0.35

ln(strain rate)

Fig. 7.3 Schematic representation of strain-rate sensitivity versus log(strain rate). L

L + dL

P

P

Uniform region with

Area Stress Strain rate

A s • «

Necked region with

Area Stress Strain rate

A + dA s + ds • « + ds

Fig. 7.4 Schematic diagram showing a uniform, circular test piece with cross-sectional area A under load P before and after the introduction of a neck.

We shall now examine further the signiﬁcance of the strain-rate sensitivity, m, in superplasticity, by considering a uniform, uniaxial circular test piece containing a single, idealized neck shown schematically in Fig. 7.4. We employ the incompressibility condition, apply constant load, P , to the test piece during necking and assume the stress–strain rate relationship given in (7.2). The incompressibility condition gives AL = (A + dA)(L + dL) ≈ AL + L dA + A dL

188

Superplasticity

so that

dL dA =− = −dε = −˙ε dt A L

and

dA = −˙ε A dt

(7.3)

or, in the neck,

d(A + dA) = −(˙ε + d˙ε )(A + dA), dt which, when combined with (7.3) gives d A d˙ε (dA) ≈ −(A d˙ε + ε˙ dA) = −dA˙ε +1 . dt dA ε˙

(7.4)

The constancy of load, P , gives σA = (σ + dσ )(A + dA) so that

dA dσ =− . (7.5) σ A The constitutive equation σ = K ε˙ m gives d˙ε d˙ε m m m m 1+ = K ε˙ 1 + m + · · · σ + dσ = K(˙ε + d˙ε) = K ε˙ ε˙ ε˙ so that

d˙ε dσ ≈m . σ ε˙

(7.6)

Combining (7.6) and (7.5) gives A d˙ε 1 =− dA ε˙ m and substituting into (7.4) gives

d 1 (dA) ≈ −dA˙ε 1 − . dt m

(7.7)

This equation tells us that the rate of development of the neck depends upon the quantity 1 − (1/m). As the strain-rate sensitivity increases, and approaches unity, the rate of necking decreases to zero. We therefore see the signiﬁcance of the strainrate sensitivity in superplasticity; the higher the value of m, the more necking can be inhibited therefore allowing greater elongations prior to the onset of necking and failure. A much more complete introduction to superplasticity can be found in Pilling and Ridley (1989).

Constitutive equations for superplasticity

7.3

189

Constitutive equations for superplasticity

The constitutive equation in (7.2) is simple, but is often inadequate for simulating superplasticity processes because the ln(stress)–ln(strain rate) relationship is not often linear, particularly over strain-rate regimes which occur in practical processing. In addition, it says nothing about the inﬂuence of changing microstructure during superplastic deformation, which is known to be important (Ghosh and Hamilton, 1979; Ghosh and Raj, 1981; Hamilton, 1984; Zhou and Dunne, 1996). We present here constitutive equations for superplasticity for the particular commercially important titanium alloy, Ti–6Al–4V. This alloy ﬁnds application in a range of aero-engine components, but for component manufacture using superplastic forming, the engine fan blades are perhaps the most important. Uniaxial stress–strain curves for the Ti–6Al–4V alloy undergoing superplastic deformation at 927◦ C are shown in Fig. 7.5. A strong strain-rate effect is seen together with signiﬁcant strain hardening. The stresses required to cause the deformation are, however, really quite small but the tensile strains achieved during the superplastic deformation are large. The hardening is due to several processes; perhaps the most important is the increasing average grain size. The average grain size at the start of all the tests shown in Fig. 7.5 is 6.4 µm. At the end of the deformation, it has increased to about 10 µm, and depends on the rate of deformation. The evolution of the average grain size for each of the stress–strain curves shown in Fig. 7.5 is shown in Fig. 7.6.

25 1.0 × 10–3 s–1

Stress (MPa)

20

15 2.0 × 10–4 s–1 10

5

5.0 × 10–5 s–1

0 0.0

0.2

0.4

0.6 Strain

0.8

1.0

Fig. 7.5 Superplastic stress–strain curves for Ti–6Al–4V at 927◦ C at the strain rates shown. The initial grain size is 6.4 µm.

190

Superplasticity

0.012 5.0 × 10–5 s–1

Grain size (mm)

1.0 × 10–3 s–1

0.0 s–1

2.0 × 10–4 s–1

0.01

0.008

0.006 0

100

200

300

400

Time (min)

Fig. 7.6 Grain size versus time curves for Ti–6Al–4V at 927◦ C at the strain rates shown. The initial grain size is 6.4 µm.

An important feature is that for a strain rate of 0.0 s−1 , that is, a static test in which no deformation takes place, grain growth still takes place; this is called static grain growth. As the strain rate is increased, so the rate of growth of grain size increases. That part of the grain growth resulting from the straining is often referred to as deformation-enhanced grain growth. Normal grain growth (Shewmon, 1969) gives rise to a kinetic equation for static grain growth of the form α1 l˙ = γ (7.8) l in which l is the average grain size, and α1 and γ are material constants. The deformation-enhanced grain growth is accounted for with an additional term so that the complete kinetic equation can be written as α1 l˙ = γ + β1 p˙ (7.9) l in which β1 is a further material constant and p˙ is, as before, the effective plastic strain rate. The symbols in Fig. 7.5 are, in fact, experimental data and the lines result from ﬁtting Equation (7.9) to the data. The material constants for this particular temperature of 927◦ C are given in Table 7.1 and assume grain size to be speciﬁed in millimetres. We now return to the microstructure–deformation coupling (Zhou and Dunne, 1996; Kim and Dunne, 1999) and employ the following elastic-viscoplastic constitutive equations α ε˙ p = µ sinh β(σ − r − σy ), (7.10) l ˙ (7.11) r˙ = (c1 − γ1 r)p, σ˙ = E(˙ε − ε˙ p ),

(7.12)

Constitutive equations for superplasticity

191

Table 7.1 Material constants for Ti–6Al–4V at 927◦ C. α 0.437 × 10−5

β 0.0919

µ 1.06

σy (MPa) 0.5

E (MPa) 1000

c1 8.397

γ1 0.666

α1 0.128 × 10−16

β1 0.9625 × 10−13

γ 5.0

Stress (MPa)

100

10 1.0 0.6 0.2

1 10–6

10–5

10–4 10–3 Strain rate (s–1)

10–2

10–1

Fig. 7.7 Experimental (symbols) and predicted (lines) stress versus strain rate curves for Ti–6Al–4V at 927◦ C with an initial grain size of 6.4 µm for the strain levels shown.

which are coupled with the grain growth equation in (7.9). Equation (7.10) is the viscoplastic constitutive equation in which, as before, α and β are material constants, l is the current grain size, and µ the deformation–microstructure coupling constant. The hardening seen in Fig. 7.4 does not all result from the grain growth, although a substantial part of it does. A further isotropic hardening term, r, has therefore been introduced with evolution equation given in (7.11) in which c1 and γ1 are material constants. Equation (7.12) is Hooke’s law. Equations (7.9)–(7.12) constitute the uniaxial material model for superplasticity. With the material constants for the grain growth kinetic equation having been already determined, the unknown constants in Equations (7.10) and (7.11) are obtained by ﬁtting the equations (Zhou and Dunne, 1996) to the experimental data in Fig. 7.5. The resulting computed stress–strain curves are given by the solid lines in the ﬁgure. Comparisons of predicted and experimental log(stress) versus log(strain rate) behaviour for the Ti-alloy with an initial grain size of 6.4 µm obtained at the strain levels shown are given in Fig. 7.7, and the corresponding predicted variation of strain-rate sensitivity with strain rate (at a strain of 1.0) is shown in Fig. 7.8.

192

Superplasticity 1.0

Strain-rate sensitivity

0.8

0.6

0.4

0.2

0.0 1E–06

Initial grain size 6.4 mm 9 mm 11.5 mm

1E–05

1E–04

1E–03

1E–02

1E–01

Strain rate (s–1)

Fig. 7.8 Predicted variation of strain-rate sensitivity with strain rate for the initial grain sizes shown for Ti–6Al–4V at 927◦ C.

7.4

Multiaxial constitutive equations and applications

We may write the multiaxial equations within the framework of viscoplasticity by assuming the normality hypothesis and von Mises material behaviour. The multiaxial viscoplastic strain rate, given these assumptions, is Dp =

3 σ

p˙ , 2 σe

(7.13)

where

α sinh β(σe − r − σy ) (7.14) lµ and Equations (7.9) and (7.11) remain unchanged. If considering large deformations (which is normally the case for superplasticity), the Jaumann stress rate is, as before, p˙ =

∇

σ = σ˙ + W σ − σ W .

(7.15)

These equations, together with (7.9) and (7.11), have been implemented into ABAQUS by means of the CREEP routine, which is described in Chapter 8. This facilitates an easier implicit implementation, but a UMAT implementation would be carried out as described for viscoplasticity in Chapters 5 and 6, although if a plane stress implementation is required, additional problems would need to be addressed. The application we consider is the superplastic blow-forming of a rectangular-section box made from 1.25 mm thick Ti–6Al–4V sheet and processed at 900◦ C (Lin and Dunne, 2001, with thanks to Dr. Lin). The model is shown in Fig. 7.9 in which just one quarter

Multiaxial constitutive equations and applications

193

Material mesh

Rigid die surface

Die surface normal

Fig. 7.9 Finite element model for the rectangular-section box die surface and the material blank.

is included, for reasons of symmetry, and both the initially ﬂat sheet and the die surface are included. The superplastic forming process consists of clamping the ﬂat Ti-alloy sheet (modelled using shell elements) against the die, the surface of which forms a cavity in the shape required. Gas pressure is applied to the top face of the sheet, forcing it to acquire the die shape. In these analyses, the maximum strain rate over the deforming sheet is controlled to be close to the optimum deforming rate of the material; that is, the strain rate required to give the highest strain-rate sensitivity obtained from the equivalent of Fig. 7.7, but for 900◦ C. This is achieved by varying the applied gas pressure. The process is considered completed at a forming time, tf , when all nodes on the deforming sheet are in contact with the die. Figure 7.10 shows the deformation of the superplastic metal sheet at three stages during the forming process at times t/tf = 0.1, t/tf = 0.6, and t/tf = 1.0. The contours show the magnitude of the effective plastic strain rate. The maximum target strain rate speciﬁed for the analysis is 1.0 × 10−5 s−1 which is achieved by application of uniformly distributed gas pressure. Figure 7.10 shows that the distribution of effective plastic strain rate is highly non-uniform. This is typical of many practical superplastic forming processes; while ideally it is necessary to deform superplastically all points in the material at the same optimum strain rate (to maximize strain-rate sensitivity and hence elongation), this is rarely achievable in practice. It is possible, however, to ensure that a target maximum strain rate is not exceeded, and in this analysis, the gas pressure is varied to ensure a nominal maximum strain rate of 1.0 × 10−5 s−1 . The variation of the maximum strain rate during the

194

Superplasticity

(a) Strain rate + 0.00E–00 + 2.00E–06 + 3.00E–06 + 4.00E–06 + 5.00E–06 + 6.00E–06 + 7.00E–06 + 8.00E–06

(b) Strain rate + 0.00E–00 + 2.00E–06 + 3.00E–06 + 4.00E–06 + 5.00E–06 + 6.00E–06 + 7.00E–06 + 8.00E–06

(c) Strain rate + 0.00E–00 + 2.00E–06 + 3.00E–06 + 4.00E–06 + 5.00E–06 + 6.00E–06 + 7.00E–06 + 8.00E–06

Fig. 7.10 The simulated superplastically deforming sheet showing the effective plastic strain rate at fractional processing times of t/tf = 0.1, t/tf = 0.6, and t/tf = 1.0. (See also Plate 1.)

forming process is shown in Fig. 7.11 for target strain rates of both 1.0 × 10−5 s−1 and 1.0 × 10−4 s−1 , and the corresponding variations in gas pressure to achieve these are given in Fig. 7.12. Higher gas pressure is needed for the higher target strain rate because of the higher ﬂow stresses required. The gas pressure increases during the

Multiaxial constitutive equations and applications

195

Maximum strain rate (s–1)

1E–03

1 × 10– 4 s–1 1E–04

1 × 10– 5 s–1 1E–05

1E–06 0.0

0.2

0.4

0.6

0.8

1.0

t /t f

Fig. 7.11 Variation of the maximum strain rate over the deforming material blank during the superplastic forming process for the two target strain rates ε˙ = 1 × 10−5 and ε˙ = 1 × 10−4 s−1 .

Gas pressure (KPa)

400

300

200 1 × 10– 4 s–1

100 1 × 10– 5 s–1

0 0.0

0.2

0.5 t /t f

0.8

1.0

Fig. 7.12 Variation of gas pressure to ensure a maximum strain rate in the deforming sheet of 1.0 × 10−5 and 1.0 × 10−4 s−1 .

superplastic forming because of increasing geometrical and frictional constraint and, in addition, because the material hardens during deformation which is due to the grain growth taking place. High gas pressure is required to ﬁll the corner part of the die, which is the last stage of the forming process. In Fig. 7.10, it is apparent that the last part of the sheet to be formed is the corner, which is also the area of maximum thinning and where tearing is most likely to occur. This is made clear by looking at the through-thickness strain ﬁelds which are shown for the two target strain rates of 1.0 × 10−5 and 1.0 × 10−4 s−1 in Fig. 7.13(a) and (b), respectively.

196

Superplasticity

(a)

Thickness strain – 1.20E+00 – 1.07E+00 – 9.15E–01 – 7.60E–01 – 6.05E–01 – 4.50E–01 – 2.95E–01 – 1.40E–01

(b) Thickness strain – 1.20E+00 – 1.07E+00 – 9.15E–01 – 7.60E–01 – 6.05E–01 – 4.50E–01 – 2.95E–01 – 1.40E–01

Fig. 7.13 Through-thickness strain ﬁelds at the end of the superplastic forming carried out with target maximum strain rates of (a) 1.0 × 10−5 and (b) 1.0 × 10−4 s−1 . (See also Plate 2.)

The lower strain rate is seen to lead to a higher spatial variation in throughthickness strain; that is, thinning, which is often not desirable in practical processing. In fact, the ranges of out-of-plane strain for the low and high strain rates are 1.06 and 0.84, respectively. The reason for this becomes clear on looking at the grain size distributions, shown in Fig. 7.14. At the lower target strain rate, the average grain size increase is larger than that at the higher strain rate because of static grain growth, which is inhibited in the latter. In addition, at the lower strain rate, the range of ﬁnal grain size is less than that at the higher rate. For the case of the higher strain rate, therefore, the larger grain size in the deforming material in the corner (relative to that at the boundaries) leads to a higher stress in the corner region to generate the same strains seen for the lower strain rate. This inhibits straining in the corner region producing larger strains in the boundary regions. The net result is a more uniform strain distribution for the high strain rate, and a correspondingly more uniform thinning. This is generally preferable

References

197

(a) Grain sizes + 1.14E–02 + 1.15E–02 + 1.16E–02 + 1.16E–02 + 1.17E–02 + 1.18E–02 + 1.18E–02 + 1.19E–02

(b)

Grain sizes +7.93E – 03 +8.06E – 03 +8.20E – 03 +8.33E – 03 +8.60E – 03 +8.74E – 03 +8.88E – 03 +9.01E – 03

Fig. 7.14 Average grain size ﬁelds at the end of the superplastic forming carried out with target maximum strain rates of (a) 1.0 × 10−5 and (b) 1.0 × 10−4 s−1 . (See also Plate 3.)

in practice, and results directly from the interactions of the superplastic deformation and microstructural evolution. These industrially important effects could not have been obtained without microstructurally based constitutive equations. An additional important effect is the distribution of grain size in commercial Ti–6Al–4V, which has not been addressed here. However, modelling techniques to incorporate it, its effects on strain-rate sensitivity and hence on necking and failure have been addressed by Kim and Dunne (1999), where further information may be found.

References Ghosh, A.K. and Hamilton, C.H. (1979). ‘Mechanical behaviour and hardening characteristics of a superplastic Ti–6Al–4V alloy’. Metallurgical Transactions, 10, 699–706. Ghosh, A.K. and Raj, R. (1981). ‘Grain size distribution effect in superplasticity’. Acta Metallurgica, 29, 607–616.

198

Superplasticity

Hamilton, C.H. (1984). ‘Superplasticity in titanium alloys’. In Agrawal, S.P. (ed.), Superplastic Forming, Proceedings of the Symposium, California, March 13–22, American Society for Metals. Kim, T.-W. and Dunne, F.P.E. (1999). ‘Modelling heterogeneous microstructures in superplasticity’. Proceedings of the Royal Society, 455, 701–718. Lin, J. and Dunne, F.P.E. (2001). ‘Modelling grain growth evolution and necking in superplastic blow-forming’. International Journal of Mechanical Science, 43, 595–609. Pilling, J. and Ridley, N. (1989). Superplasticity in Crystalline Solids. The Institute of Metals, London. Shewmon, P.G. (1969). Transformations in Metals. McGraw-Hill, New York. Zhou, M. and Dunne, F.P.E. (1996). ‘Mechanisms-based constitutive equations for the superplastic behaviour of a titanium alloy’. Journal of Strain Analysis, 31, 65–73.

8. Porous plasticity

8.1

Introduction

We have so far considered plasticity and viscoplasticity processes in which it has been assumed that the deforming material has been incompressible. There are some materials, however, for which this is not the case. An important example is in the processing of metal powders in which, generally at elevated temperature, the powder is consolidated by plastic deformation and the elimination of the porosity. During the process, signiﬁcant volume changes occur because of the removal of the porosity. A further example of compressible or porous plasticity is that in which signiﬁcant voiding develops in a material undergoing plastic deformation resulting from a damage process (e.g. creep cavitation). Again, while possibly small, volume changes occur during the deformation and the incompressibility condition no longer holds. A feature of the constitutive equations in porous plasticity is that there becomes a dependence on mean stress as we shall see shortly. In this chapter, we introduce the porous plasticity model of Duva and Crow and outline its implementation into ABAQUS using both a UMAT material subroutine and the simpler ABAQUS CREEP routine. For simplicity, within the UMAT, we use explicit integration of the constitutive equations and employ the initial stiffness as the material Jacobian. A number of constitutive relations for the consolidation of metal powders have been developed. They have been used to predict the dependence of densiﬁcation rate on consolidation pressure and temperature as well as volume fraction of voids. One of the ﬁrst constitutive models for consolidation of metal powder was developed by Wilkinson and Ashby (1975). They analysed the creep collapse of a thick-walled spherical shell subjected to externally applied hydrostatic loading. In general, consolidation occurs under the action of a range of stress states that are not purely hydrostatic, for which the Wilkinson and Ashby model is therefore inappropriate. Subsequent research has therefore broadened the Wilkinson and Ashby model to more general loading conditions. The models have taken into account the effects of deviatoric and hydrostatic components of stress state by introducing potentials which make possible the

200

Porous plasticity

development of relationships between macroscopic strain rate and stress state (Cocks, 1989; Ponte Castaneda, 1991; Duva and Crow, 1992; Sofronis and McMeeking, 1992). The strain rate potential (φ) for a porous material can be written as a function of both deviatoric and hydrostatic stresses ε˙ 0 σ0 φ= n+1

S σ0

n+1 ,

(8.1)

where S 2 = aσe2 + bσm2 , 3

σ : σ , 2 1 σm = II : σ . 3 σe2 =

(8.2) (8.3) (8.4)

S is an effective effective stress (Duva and Crow, 1994) given in terms of the effective, σe , and hydrostatic, σm , stresses, n is the creep exponent, and the coefﬁcients a and b are functions of current relative density, D, which is equivalent to the solid volume fraction of the porous material, a is associated with the deviatoric component and b with the hydrostatic component. The coefﬁcients a and b are chosen such that, at the fully dense stage, that is, D = 1, the coefﬁcient b becomes 0 and a becomes 1. The effective effective stress, S, is then reduced to σe . The various densiﬁcation models for monolithic materials in the literature use different approaches to obtain the strain rate potential. This leads to different expressions for the coefﬁcients a and b (Duva and Crow, 1994). Duva and Crow (1994) proposed a strain rate potential for computing densiﬁcation rates. Based on the strain rate potentials of Cocks (1989) and Ponte Castaneda (1991), the coefﬁcients a and b were chosen to ensure that the potential gives densiﬁcation rates identical to those of Wilkinson and Ashby (1975) in the hydrostatic load limit, and agree with both Cocks (1989) and Ponte Castaneda (1991) in the limit when the hydrostatic stress vanishes. The densiﬁcation rates predicted by Duva and Crow’s strain rate potential are consistent with their cell model calculations which were derived based on Hill’s minimum principle for velocity. Duva and Crow predict densiﬁcation rates which compare favourably with the prediction from the Wilkinson and Ashby model in the hydrostatic limit. The Duva and Crow potential also satisﬁes the lower bounds derived by both Cocks and Ponte Castaneda in the limit that the hydrostatic stress vanishes. The densiﬁcation rate predicted from the Duva and Crow model, in the presence of a large deviatoric stress component, is closer to the experimental results than the predictions of Sofronis and McMeeking (1992).

Implementation of porous material constitutive equations

8.2

201

Finite element implementation of the porous material constitutive equations

Strain rates are determined by differentiating the strain rate potential, φ, to give ∂φ 1 n−1 3

ε˙ = = AS aσ + bI σm (8.5) ∂σ 2 3 in which 2/(n+1) 2 1 + (2/3)(1 − D) 3 n(1 − D) a= and b = 1/n n 2n/(n+1) 2n (1 − (1 − D) ) D and where A is a material parameter given by ε˙ 0 A = n. (8.6) σ0 The dilatation rate can be obtained from ε˙ kk = ε˙ xx + ε˙ yy + ε˙ zz and hence, the densiﬁcation rate is given as D˙ = −D ε˙ kk ,

(8.7) (8.8)

where D is the relative density. 8.2.1

Implementation into ABAQUS UMAT

The constitutive equations for porous metals developed by Duva and Crow (1992) are implemented into the ﬁnite element software ABAQUS within a large deformation formulation using a UMAT subroutine. A simple, explicit, forward Euler integration is adopted. ABAQUS supplies to the UMAT subroutine the deformation gradient at the beginning and the end of each time step, F t and F t+δt . The user is required to supply the Cauchy stress at the end of the time step. The algorithms, ﬁrst, need to deﬁne the rate of deformation gradient, F˙ , which can be calculated, for small time steps, as 1 F˙ = (F t+δt − F t ). (8.9) δt Then, the velocity gradient, L, is L = FF −1 . The total rate of deformation, D, and the spin tensor, W , are given by 1 D = (L + LT ), 2 1 W = (L − LT ). 2

(8.10)

(8.11) (8.12)

202

Porous plasticity

The strain components are calculated independently from 1 ε = − ln(FF T )−1 . 2

(8.13)

˙ can be calculated from The dilatation rate, ε˙ kk , and the densiﬁcation rate, D, Equations (8.7) and (8.8), respectively. The relative density at the end of each time step is determined using the ﬁrst-order Euler integration scheme ˙ D t+δt = D t + Dδt.

(8.14)

∇

The co-rotational stress rate σ is given by ∇

σ =

Eν E De + II : D e , (1 + ν) (1 + ν)(1 − 2ν)

(8.15)

where E is Young’s modulus, ν is Poisson’s ratio, and D e is the rate of elastic deformation given by (8.16) De = D − Dp. D p is the rate of plastic deformation as given in Equation (8.5). The stress increment, with respect to the material reference frame, is calculated as ∇

∇

σ = σ +Rσ t R t .

(8.17)

This, therefore, provides for an objective update of the stress with respect to a ﬁxed ∇

coordinate system during the time step. The stress increment, σ , for each time step can be determined by utilizing the ﬁrst-order Euler integration scheme ∇

σ = σ t.

(8.18)

The updated stress is returned to ABAQUS through the UMAT subroutine. Because here, we adopt an explicit ﬁrst-order forward Euler integration, great care is necessary in choosing an appropriate time step, and in ensuring meaningful results are obtained. 8.2.2

Implementation into ABAQUS CREEP subroutine

The implementation of the Duva and Crow constitutive equations for consolidation is also carried out using the ABAQUS CREEP facility. This subroutine is suitable for constitutive equations in which the increments of inelastic strain are functions of the hydrostatic stress and the equivalent deviatoric stress described by Mises’ or Hill’s deﬁnitions, while the UMAT subroutine allows more general forms of constitutive laws to be implemented, and easier handling of internal state variables.

Implementation of porous material constitutive equations

203

ABAQUS computes the incremental creep strain components as 1 εcr = ¯εcr n + ¯εsw I , 3 where n is the direction normal to the yield surface, given by

(8.19)

∂σe . (8.20) ∂σ ¯ε cr and ¯ε sw are the equivalent creep strains conjugate to the deviatoric stress and the mean stress, respectively. Therefore, ¯εcr corresponds to the conventional deviatoric creep strain and ¯εsw to the volumetric strain occurring because of void closure. In order to implement the porous material constitutive equations using the CREEP subroutine, the plastic strain rate equation deﬁned in Equation (8.5) has to be decomposed into two parts as follows n=

3 1 ε˙ p = AS n−1 aσ + AS n−1 bσm I . (8.21) 2 3 The ﬁrst part is associated with the deviatoric stress and the second with the mean stress. The user is required to provide ¯ε cr , ∂¯εcr /∂σe , ∂¯εcr /∂p, ¯εsw , ∂¯εsw /∂σe , and ∂¯εsw /∂p, in which σe is the equivalent stress and p is the equivalent pressure stress given as 1 p = − (σxx + σyy + σzz ). (8.22) 3 The variables are obtained as follows: ¯ε cr = AS n−1 aσe t, 1 (n − 1)aσe ∂¯ε cr cr , + = ¯ε ∂σe σe S2 ∂¯ε cr cr (n − 1)bσm = −¯ε , ∂p S2 ¯εsw = Abσm S n−1 t, ∂¯εsw sw (n − 1)aσe , = ¯ε ∂σe S2 1 (n − 1)bσm ∂¯εsw sw = −¯ε . + ∂p σm S2

(8.23) (8.24) (8.25) (8.26) (8.27) (8.28)

In order to calculate σe and σm , the stress components are required. The CREEP subroutine does not provide these quantities, and therefore the USDFLD subroutine has to be utilized to access material point data and assign stress components to state variables, which are then passed into the CREEP subroutine. The densiﬁcation rate

204

Porous plasticity Table 8.1 Material parameters.

A0 n

T < 750◦ C

T ≥ 750◦ C

8.49 2.18

95.67 1.53

0.98

Relative density

0.93

0.88

0.83

Predicted using UMAT subroutine Predicted using CREEP subroutine

0.78 0

10

20

30

40

50

Time (min)

Fig. 8.1 Graph showing comparisons of relative density–time curves obtained from the porous plasticity material model utilizing both an ABAQUS UMAT subroutine and a CREEP subroutine.

can therefore be obtained from Equation (8.8). The relative density for each time increment can be determined by utilizing the ﬁrst-order Euler integration as given in Equation (8.14). The porous plasticity material model implemented using the CREEP subroutine was veriﬁed against that using the UMAT subroutine by simulating a simple compression process using a single plane strain element subjected to in-plane compressive load of 20 MPa at 925◦ C. The material constants, A0 and n, used are given in Table 8.1, and A is calculated from −Q (8.29) A = A0 exp RT in which T is the temperature, R the gas constant, and Q activation energy. Figure 8.1 shows comparisons of the relative density evolution over time calculated by the porous material model using the CREEP and the UMAT subroutines. The results can be seen to be identical. The Duva and Crow porous plasticity model has been used (empirically) to approximate the behaviour in consolidation of continuous (SiC) ﬁbre, (Ti) metal matrix

Application to consolidation of Ti–MMCs

205

300 mm

Reinforced area

Fig. 8.2 Schematic diagram of an aero-engine bling showing region of reinforcement with Ti–MMC and a demonstrator disc (from King, 1998).

composite materials (Ti–MMCs) being developed for potential application to aeroengine components together with shafts, discs, brakes, and aircraft landing gear. Application to an aero-engine ‘bling’—a bladed ring—is shown in Fig. 8.2. The Ti–MMC material in the unconsolidated and fully consolidated state is shown in Fig. 8.3(a) and (b), respectively.

8.3

Application to consolidation of Ti–MMCs

The simple consolidation model, which was implemented using the CREEP subroutine as described above, was set up to simulate (empirically) the consolidation of Ti–MMCs under a range of processing conditions. The consolidation process is

206

Porous plasticity

(a)

(b)

Fig. 8.3 Micrographs showing Ti–6Al–4V matrix, SiC continuous ﬁbre composite material (a) unconsolidated and (b) consolidated at 925◦ C for 30 min at 15 MPa.

Ti–MMC

Die

Fig. 8.4 Schematic diagram showing arrays of Ti–MMCs undergoing consolidation.

1 Model prediction Experimental data

Relative density

0.95

0.9

0.85

0.8

0.75 0

40

80

120

160

200

Time (min)

Fig. 8.5 Predicted and measured relative density evolution with time for Ti–6Al–4V/SiC composite consolidated at a constant temperature of 925◦ C with a pressure of 20 MPa.

References

207

1 Model prediction Experimental data

Relative density

0.95

0.9

0.85

0.8

0.75 0

40

80

120 Time (min)

160

200

Fig. 8.6 Predicted and measured relative density evolution with time for Ti–6Al–4V/SiC composite consolidated at a constant temperature of 700◦ C with a pressure of 20 MPa.

shown schematically in Fig. 8.4. Generally, there are many more layers of ﬁbres and the pressure is applied by means of a mechanical punch. The mechanical die ensures that the Ti–MMCs undergo plane strain compression. Some of the results of the simulations, which were carried out at a constant temperature of 925◦ C under a pressure of 20 MPa, and at a temperature of 700◦ C under a constant pressure of 20 MPa, are shown in Figs 8.5 and 8.6, respectively, showing the important effect of temperature.

References Cocks, A.C.F. (1989). ‘Inelastic deformation of porous materials’. Journal of the Mechanics and Physics of Solids, 37(6), 693. Duva, J.M. and Crow, P.D. (1992). ‘The densiﬁcation of powders by power-law creep during hot isostatic pressing’. Acta Metallurgica, 40(1), 31. Duva, J.M. and Crow, P.D. (1994). ‘Analysis of consolidation of reinforced materials by power-law creep’. Mechanics of Materials, 17, 25. King, J. (1998). ‘Composites take off without a parachute’. Materials World, 5(6), 324. Ponte Castaneda, P. (1991). ‘The effective mechanical properties of nonlinear isotropic composites’. Journal of the Mechanics and Physics of Solids, 39(1), 45. Sofronis, P. and McMeeking, R.M. (1992). ‘Creep of power-law material containing spherical voids’. Journal of Applied Mechanics, Transactions of ASME, 59(2), 88. Wilkinson, D.S. and Ashby, M.F. (1975). ‘Pressure sintering by power law creep’. Acta Metallurgica, 23, 1277.

This page intentionally left blank

9. Creep in an aero-engine combustor material

9.1

Introduction

Aero-engine components operating under in-service conditions are often subjected to a range of complex cyclic mechanical and thermal loading, leading to combined creep and cyclic plasticity. The polycrystalline nickel-base superalloy (C263) is a commercial alloy used for stationary components in aero-engines such as combustion chambers, casings, liners, exhaust ducting, and bearing housings. It is a ﬁne-precipitate strengthened alloy at 800◦ C, with a precipitate solvus temperature of 925◦ C (Betteridge and Heslop, 1974). Combustion chamber applications require the material to undergo temperature ﬂuctuations between 20◦ C and 950◦ C, and the temperature range is therefore such that the precipitate solvus can be exceeded during in-service operation. Signiﬁcant microstructural change is therefore likely to occur during ordinary operation, leading to quite profound changes in the creep mechanisms in the material, controlling both deformation and component life. In this chapter, we shall introduce a physically based creep model which explicitly accounts for microstructural change, and its inﬂuence on creep deformation and failure, in polycrystalline nickel-base alloy C263 for temperatures both above and below the γ solvus. The implementation into ABAQUS is carried out using a forward Euler integration scheme and we again use the initial stiffness as the material Jacobian for simplicity.

9.2

Physically based constitutive equations

Creep in nickel alloy C263 occurs through diffusion-activated dislocation climb and precipitate ‘cutting’, depending on the precipitate spacing, λp (or equivalently, size, rs , for a given precipitate volume fraction, φp , which in turn depends on temperature, T ). Above a critical particle spacing, λpc , dislocation climb dominates, whereas below the critical spacing, precipitate ‘cutting’ dominates. The material also undergoes coarsening at temperature such that the particle spacing increases with time.

210

Creep in aero-engine components

All of these microstructural processes are embodied within creep constitutive equations. The creep strain rate, p˙ c , also depends upon the density, ρn , of mobile dislocations which in turn depends on the accumulated creep strain. The constitutive equation set embodying all the mechanisms discussed above is given below. The activation volume, V , depends on the active obstruction mechanism. In the case of dislocation pinning by precipitates, V is dependent on the pinning distance, which in turn depends on the precipitate spacing. For precipitate cutting, the activation volume is Vc . In the creep strain rate equation, the uniaxial strain rate, ε˙ c , in response to a uniaxial stress, σ , is determined from the corresponding shear values ¯ , in which M¯ using the usual relationships (Dieter, 1988): ε˙ = γ˙ /M¯ and σ = Mτ is the Taylor factor. F is the Helmholtz free energy, b the Burger’s vector, ν the frequency of dislocation jumping energy barriers, kb the Boltzman constant, and ρi the initial density of mobile dislocations. ρn ρi ([4π/3φp ]1/3 − 2) 2 σe V −F p˙ c = b , (9.1) sinh ν exp ¯ − ω) kb T [4π/3φp ]1/3 M¯ kb T M(1 where V = Vc , if φp > 0 and λp < λpc V = λp b2 , if φp > 0, λp > λpc and λp < λd V = λd b2 , if φp = 0 and

λp = rs

4π 3φp

1/3

(cutting), (climbing), (dislocation network)

−2 ,

ρ˙n = ψ ε˙ c . In Equation (9.1), ω is a scalar damage variable which has evolution equation χ σ1 ω˙ = H (σ1 )p˙ c (9.2) σe in which σ1 is the maximum principal stress, H the Heaviside function, and and χ are material constants (χ being the sensitivity of stress state parameter). The equations contain just two unknown ﬁtting constants, namely ψ and associated with the multiplication of mobile dislocations and cavitation, occurring largely within the tertiary creep regime. All the other material constants are physical properties or measurable physical quantities. Creep tests have been carried out by Rolls-Royce over the temperature range 700–750◦ C, and by Zhang and Knowles (2001) on C263 over the temperature range 800–950◦ C. Prior to creep testing, the material had been subjected to the standard

Physically based constitutive equations

(a)

(b)

2.0

10

450 MPa

380 MPa

350 MPa 8

1.5

200 MPa

1.0

Strain (%)

Strain (%)

250 MPa 320 MPa

0.5

270 MPa

0.0 0.0

6

4

2

0 1.0

2.0

3.0 4.0 Time (s)

5.0

0

6.0 [× 106]

(c)

2

4

6 Time (s)

8

10 [× 106]

(d)

4.5

30 40 MPa

4.0 25

200 MPa

3.5

160 MPa

20 Strain (%)

3.0 Strain (%)

211

250 MPa

2.5 2.0 1.5

15 10 50 MPa

1.0 5 0.5 0.0 0

1

2 Time (s)

3 [× 106]

Experimental results

0 0.0

0.1

0.2

0.3 0.4 Time (s)

0.5

0.6 [× 106]

Computed results

Fig. 9.1 Comparison of experimental and computed isothermal creep results at (a) 700◦ C, (b) 750◦ C,

(c) 800◦ C, and (d) 950◦ C.

heat treatment. This involves solutioning at 1150◦ C for 2 h, quenching and ageing at 800◦ C for 8 h followed by air cooling. The results of the tests are shown in Fig. 9.1 by the broken lines. The constants and constant groups appearing in the equations have been determined by standard optimization techniques. The volume fraction of γ precipitate is known at each test temperature, Burger’s vector for this material is taken as 2.5 × 10−10 m (Frost and Ashby, 1982), and the initial density of dislocations can be estimated to

212

Creep in aero-engine components Table 9.1 Physical constants determined from creep data by optimization. F (J/atom)

λpc (nm)

Vc (m3 )

ν (s−1 )

M¯

7.4 × 10−19

64.9

4.05 × 10−27

15.1 × 1021

3.57

be 1010 m−2 (Hull, 1975). The remaining temperature-independent physical properties can then be determined using the results of the optimization and the model equations. The results of this process are shown in Table 9.1, which includes the Helmholtz free energy, F , the critical particle spacing, λpc , above which dislocation bowing dominates over particle cutting, the activation volume for cutting, Vc , the frequency of dislocations jumping energy barriers, ν, and the Taylor factor. The temperature dependence of the two empirical constants for the evolution of multiplication of mobile dislocation density and cavitation is shown in Appendix 9.1. The computed creep curves resulting from the determination of the creep parameters are also shown in Fig. 9.1.

9.3

Multiaxial implementation into ABAQUS

We assume multiaxial creep deformation in nickel alloy C263 to obey von Mises behaviour; that is, the relationship between uniaxial creep strain rate and stress is identical to that between the effective creep strain rate and effective stress. Under multiaxial conditions, the creep strain rate ‘direction’ is taken to be normal to the dissipative surface, in an analogous way to that in plasticity, giving the multiaxial creep strain rate as 3 σ

ε˙ c = p˙ c 2 σe

in which σ is the deviatoric stress tensor, and σe the effective stress, given by 1/2 3

σe = σ :σ 2 and the effective creep strain rate, p˙ c , is given in Equation (9.1). The equations have been implemented into an ABAQUS UMAT using a simple forward Euler explicit integration scheme with the initial stiffness method; that is, the material Jacobian is speciﬁed simply as the elasticity matrix. 9.3.1

Finite element modelling of biaxial creep tests

A range of tests have been carried out on nickel alloy C263 in order to investigate its stress state sensitivity of creep failure. The tests have been carried out on thin-walled

Multiaxial implementation into ABAQUS

213

Table 9.2 Summary of tests and loading conditions, and corresponding stress state. Shear stress (MPa) Tension Tension–torsion Torsion Compression–torsion

0 160 184 160

Axial stress (MPa) 320 160 0 −160

σ1 /σe 1.0 0.81 0.58 0.31

tubular specimens which have been subjected to uniaxial tension, tension–torsion, torsion, and compression–torsion. The material was subjected to the standard heat treatment such that its uniaxial creep behaviour, through to failure, is correctly modelled using the above constitutive equations with the material properties given in Manonukul et al. (2002). The test specimen gauge section has length 16 mm, with internal and external radii of 3.12 and 4.12 mm, respectively. The tests were carried out at 800◦ C such that the von Mises effective stress for each test was the same, namely 320 MPa. The loading conditions applied are summarized in Table 9.2. The loads were increased linearly from zero to the maximum (to give the desired stresses) over 14 s, and were then held at the maximum value. The experimental test results are shown in Fig. 9.2(a). The quality of the creep data obtained for the torsion test is, unfortunately, not as good as desired because of problems with temperature control. However, the results do demonstrate the strong dependence of creep life on stress state. The stress state, given by σ1 /σe , for each test, is shown in Table 9.2. The test specimens were modelled by developing three-dimensional meshes of the gauge sections (i.e. uniform-section tubes). Because of the need to carry out compression tests, the wall thickness was constrained by buckling problems. As a result, the specimen wall thickness was such that an assumption of uniform shear strain and stress through the wall thickness would not have been appropriate. A two-dimensional ﬁnite element model was therefore necessitated. However, because of the ease of speciﬁcation of torsional loading conditions using three-dimensional elements (as opposed to axisymmetric elements with ‘twist’ in ABAQUS), 240 eight-noded, three-dimensional solid elements were used so that the specimen thickness contained two elements. Geometrical non-linearity was accounted for using the standard ABAQUS large strain formulation. Under torsional loading, because of the radial variation of stress, the loads applied were chosen to ensure that the average effective stress through the thickness was that desired, that is, 320 MPa. The creep behaviour of the material was described by the constitutive equations given above. The only unknown parameter in the equations is the stress state sensitivity, χ. The four tests described above were simulated using the ﬁnite element model. Parametric studies were carried out in order

214

Creep in aero-engine components

(a)

0.3 Tension–torsion

Torsion

Equivalent creep strain

0.25 Compression–torsion

0.2 0.15

Tension

0.1 0.05 0 0

100000

200000

300000

400000

500000

600000

700000

800000

Time (s) (b)

0.3

Equivalent creep strain

0.25

Compression–torsion

0.2 Torsion 0.15 Tension–torsion

0.1

Compression

0.05

Tension

0 0

100000

200000

300000

400000

500000

600000

700000

800000

Time (s)

Fig. 9.2 (a) Experimental and (b) computed equivalent creep strain versus time for isothermal creep tests carried out at 800◦ C with effective stress 320 MPa for the loading conditions shown.

to determine χ. This was done by choosing that value of χ which provided computed results closest to those seen in the experiments. The computed results obtained using a value for χ of 0.38 are shown in Fig. 9.2(b). This value lies within the range for nickel alloys discussed by Dyson and Loveday (1981). Considerably different creep lives are seen to occur depending on the stress state, and this is captured well by the model. The computed creep curve for uniaxial compression shown in Fig. 9.2(b) can be seen to have a slowly increasing gradient, even though there is no creep cavitation

Multiaxial implementation into ABAQUS

215

Displacement of the top boundary (mm)

2 1.8

Indicates predicted failure on the basis of a damage level of 0.3 through the specimen section

1.6 194 MPa

1.4 1.2 1

161 MPa

0.8

104 MPa

0.6 0.4 0.2 0 0

500

1000

1500

2000

2500

Time (h)

Fig. 9.3 Predicted displacement of the top boundary versus time (solid lines) for the double notch specimen subjected to the stresses shown. Broken straight lines indicate experimentally determined times to failure.

occurring. This results from both the precipitate coarsening and the multiplication of mobile dislocations, both of which are included in the model.

9.3.2

Prediction of notched bar creep behaviour

Three experimental tests have been carried out on double notched bar test specimens. The specimens have gauge length 25.4 mm and diameter 5.62 mm. The circular notches have diameter 1.12 mm and they are separated by 7 mm along the length of the specimen. The effect of the notches is to introduce multiaxial stress states local to the notches, which inﬂuence creep damage evolution, as discussed above. Uniaxial loading was applied to generate nominal section stresses of 104, 161, and 194 MPa, respectively. The test specimens were modelled using axisymmetric elements. Because of symmetry, just one quarter of the specimen section was modelled explicitly. The specimen lifetimes have been predicted and the lives compared with those obtained in the experiments. The predicted displacements of the top boundary of the test specimen are shown for the three applied, nominal stresses of 104, 161, and 194 MPa in Fig. 9.3. The creep damage evolution for the case of the 161 MPa nominal stress is shown in Fig. 9.4(a). At this stress level, creep damage is predicted to initiate at the notch root after creeping for about 13 h. By the time creep has continued for 166 h, the damage has evolved right across the test specimen, in which the damage level is 0.26 or higher. This is

216

Creep in aero-engine components

Cavitation damage parameter

(a)

+0.00E+00 +2.00E–02 +4.36E–02 +6.73E–02 +9.09E–02 +1.15E–01 +1.38E–01 +1.62E–01 +1.85E–01 +2.09E–01 +2.33E–01 +2.56E–01 +2.80E–01 +3.00E–01 (b)

(c)

2

7

2

0

2

6

8

2

5

0

0

Number of creep voids

3

7

12

7

2

4

4

4

15

6

3

0

2

9

9

5

2

0

0 1–3 4–6 7–9 10–12 13

1

3

4

22

8

2

5

1

17

30

2

1

Fig. 9.4 Creep damage ﬁelds (a) predicted by the model, (b) observed in the microstructure, and (c) from a surface void count using the micrograph. (See also Plate 4.)

References

217

Table 9.3 Predicted and experimentally determined top boundary displacement at failure (deﬁned as experimental specimen separation). Stress (MPa) 104 161

Predicted displacement at failure (mm)

Experimental displacement at failure (mm)

1.9 0.1

1.97 0.11

shown in Fig. 9.4(a), together with a micrograph of the corresponding region of the test specimen in Fig. 9.4(b). Microcracking can be seen to initiate at the notch root at an angle of about 22◦ from the horizontal. A surface void count has been carried out and the results are shown in Fig. 9.4(c). The damage ﬁelds in Fig. 9.4(a) can be seen to predict reasonably well both the site of major cracking and the distribution of experimentally observed creep cavitation. Dyson and McLean (1990) have argued that creep rupture occurs typically when the creep cavity damage achieves a value of about 0.3. This results from the coalescence of creep cavitation and the propagation of macroscopic creep cracking. The experimentally determined failure times are shown in Fig. 9.3 by the dashed lines. The measured and calculated displacements of the top boundary at failure, which show good agreement, are shown in Table 9.3. The predicted displacement at failure was determined as the predicted displacement when a damage level of about 0.3 had been achieved through the specimen section. However, the analyses were not stopped once a creep damage level of 0.3 had been achieved across the specimen section, and hence Fig. 9.3 shows the calculated top boundary displacement continuing to increase as the damage level exceeds 0.3. A further reason for continuing the analysis is the difﬁculty of deﬁning creep failure in the calculations. In the experiments, this is easier; it is simply the measured time until the specimen breaks. An alternative way to deﬁne calculated specimen rupture time is simply to examine the top boundary displacement rate, and to assume that rupture occurs once the rate becomes large. On this basis, the comparison of predicted and experimental time to rupture results shown in Fig. 9.3 is reasonable.

References Betteridge, W. and Heslop, J. (1974). The Nimonic Alloys. Edward Arnold, London, UK. Dyson, B.F. and Loveday, M.S. (1981). In Ponter, A.R.S. and Hayhurst, D.R. (eds), Proceedings of the Creep in Structures IUTAM Symposium, Springer, Berlin, 406–421.

218

Creep in aero-engine components

Dyson, B.F. and McLean, M. (1990). ‘Creep deformation of engineering alloys— development from physical modelling’. Iron and Steel Institute of Japan International (ISIJ), 30, 802–811. Dieter, G.E. (1988). Mechanical Metallurgy. McGraw-Hill Book Co., London, UK. Frost, H.J. and Ashby, M.F. (1982). Deformation-Mechanism Maps: The Plasticity and Creep of Metals and Ceramics. Pergamon Press, Oxford, UK. Hull, D. (1975). Introduction to Dislocations, 2nd edition. Pergamon Press, Oxford, UK. Manonukul, A., Dunne, F.P.E., and Knowles, D. (2002). ‘Physically-based model for creep in nickel-base superalloy C263 both above and below the γ solvus’. Acta Materialia, 50(11), 2917–2931. Zhang, Y.-H. and Knowles, D. (2001). ‘Deformation behaviour and development of microstructure during creep of a nickel-base superalloy’. In Parker, J.D. (ed.), Proceedings of the 9th International Conference on Creep and Fracture of Engineering Materials and Stuctures, April 2001, Gomer Press, UK.

Appendix 9.1 The dependence of precipitate volume fraction, φ, on temperature, T , in C263 φ = −4.537 × 10−9 T 3 + 1.261 × 10−5 T 2 − 1.187 × 10−2 T + 3.915. The dependence of constants and on temperature.

ψ

700◦ C

750◦ C

800◦ C

950◦ C

496.1 1.58×10−2

435.2 3.01×10−2

10.0 18.62

1.1×10−19 19.84

10. Cyclic plasticity, creep, and TMF

10.1

Introduction

In Chapter 9, we examined creep in the aero-engine combustor material nickel-base superalloy C263. In this chapter, we address combined anisothermal cyclic plasticity and creep. We use time-independent cyclic plasticity with both isotropic and kinematic hardening which we combine with the physically based creep model described in Chapter 9. The plasticity model is implemented into ABAQUS Implicit by means of a UMAT subroutine which employs a simple ﬁrst-order forward (explicit) integration scheme and the initial stiffness method. We then address isothermal cyclic plasticity and creep, followed by an examination of thermo-mechanical fatigue in nickel alloy C263.

10.2

Constitutive equations for cyclic plasticity

C263 is largely rate-independent and shows very limited creep response at temperatures below ∼600◦ C. During zero-mean, strain-controlled reversed plasticity below this temperature, the material exhibits both kinematic hardening within individual cycles, and isotropic strain softening/hardening over many cycles, depending on the temperature. The resulting stress–strain hysteresis loops show considerable change as plastic strain accumulates. Above ∼600◦ C, under similar loading, the material starts to exhibit strain-rate dependence. Viscoplastic constitutive equations for a polycrystalline nickel-base alloy have been presented by Yaguchi et al. (2002a,b), who considered uniaxial creep, isothermal, and anisothermal cyclic plasticity between 450◦ C and 950◦ C. Because of the wide temperature range considered here (20–950◦ C), a uniﬁed viscoplasticity-creep model is not adopted because of the numerical problems that can arise when using such a model for time-independent plasticity. In any case, it would, in addition, prevent the retention of the physical basis of the creep model to be used here, presented by Manonukul et al. (2002). A non-uniﬁed approach has therefore been adopted in which conventional time-independent reversed plasticity

220

Cyclic plasticity, creep, and TMF

theory for low-temperature deformation has been combined with the physically based creep model for elevated temperature deformation. The further justiﬁcation for the separation of creep and time-independent plasticity terms is that at 20◦ C, for example, (thermally activated) creep simply does not occur. Deformation takes place by plastic slip which is not aided by thermally activated dislocation climb. Conversely, at 950◦ C, deformation is dominated by diffusion-controlled processes, and plastic slip, aided by thermal activation or otherwise, is negligible. At about 800◦ C, both sets of mechanisms operate, and a uniﬁed viscoplasticity theory would be appropriate. However, for the main application considered here—thermo-mechanical fatigue with considerable temperature variations, 20–950◦ C, our approach can be justiﬁed. It is therefore assumed that the elastic, dε e , time-independent plastic, dεp , creep, dεc , and thermal, dεθ , strain increments may be additively decomposed such that the total strain, dε, is given by dε = dεe + dε p + dε c + dε θ .

(10.1)

There have been many developments in the modelling of kinematic hardening that take account, for example, of non-proportional loadings (Voyiadjis and Abu Al-Rub, 2003). However, for simplicity here, the Chaboche combined isotropic and kinematic hardening model (Lemaitre and Chaboche, 1990) is employed for time-independent plasticity. The increment in non-linear kinematic hardening dx and the increment in isotropic hardening dr are given, respectively, by dx =

2 c dεp − γ x dp 3

(10.2)

and dr = b(Q − r) dp, where

dp =

2 p dε : dεp 3

(10.3)

1/2 .

(10.4)

Here, x is the kinematic hardening stress tensor, r the isotropic hardening stress, and b and Q are temperature dependent material parameters associated with isotropic hardening. Temperature and accumulated plastic strain dependent material parameters associated with kinematic hardening are c and γ , respectively. A large number of fully reversed cyclic plasticity tests have been carried out in order to determine the temperature-dependent material parameters arising in the kinematic hardening equations. dp is the effective time-independent plastic strain increment. The increment in plastic strain is determined in the conventional way assuming a von

Constitutive equations for cyclic plasticity

221

Mises yield function, f , given by 1/2 3

f = − r − σy = 0 (σ − x ) : (σ − x ) 2 so that

∂f 3 σ − x

(10.5) = dλ 2 σe ∂σ in which dλ is the plastic multiplier which, for combined isotropic and kinematic hardening, is given, using Voigt notation, by dεp = dλ

dλ =

(∂f /∂σ) · C dε (∂f /∂σ) · {(2/3)c(∂f /∂σ) − γ x} + b(Q − R) + (∂f /∂σ) · C(∂f /∂σ)

=

( 23 )(σ /σe ) · C dε

( 23 )(σ /σe )·{( 23 )c( 23 )(σ /σe ) − γ x} + b(Q − R) + ( 23 )(σ /σe )· C( 23 )(σ /σe )

.

(10.6) The effective stress is, of course, given by 1/2 3

σe = . (σ − x ) : (σ − x ) 2 The increment in thermal strain is calculated in the usual way as dε θ = α dθI

(10.7)

in which α is the coefﬁcient of thermal expansivity, dθ the increment in temperature, and I the identity matrix. The multiaxial constitutive equations presented above for creep and plasticity have been implemented into a UMAT user subroutine using the simple ﬁrst-order explicit Euler forward integration scheme as follows 3 σ

c θ dσt = C dεt − dλ − dε − dε 2 σe in which the increment in creep strain is obtained from Equation (9.33) and those in Table 9.1, and σt+t = σt + dσt , x t+t = x t + dx t , p

p

p

εt+t = εt + dεt , rt+t = rt + drt .

222

10.3

Cyclic plasticity, creep, and TMF

Constitutive equations for C263 undergoing TMF

The thermo-mechanical loading cycles to which the nickel-base superalloy C263 is subjected in-service are such that the γ solvus is exceeded so that the material is, in effect, solution treated. This has a profound effect on the behaviour of the material; under conditions of both creep and reversed plasticity. The rate-controlling mechanisms for creep deformation change from precipitate cutting and dislocation pinning at precipitates, and climb, to that of the pinning of dislocations through the establishment of a dislocation network. The physically based creep model employed here is able to capture these changes and to represent the micro- and macro-scale creep deformation. For a given temperature, the precipitate volume fraction is known, and because the precipitate coarsening kinetics has been quantiﬁed, both size and hence spacing of the precipitate is known. These quantities appear explicitly in the physically based creep model. The effect of solution treating on cyclic plastic response is also very signiﬁcant and has been addressed. Cyclic plasticity tests between 20◦ C and 950◦ C have been carried out. With the combined creep–cyclic plasticity model described above, the temperature dependence of the isotropic and kinematic hardening constants have been determined (Manonukul et al., 2001). The effect of precipitate volume fraction on cyclic plasticity behaviour is introduced into the model, therefore, through the temperature dependence of the material parameters for cyclic plasticity. At temperatures of about 800◦ C and above, C263 creeps quite signiﬁcantly. This appears in the cyclic plasticity response as a reduction in the overall stress level, occurring through relaxation. LCF tests have been carried out on C263 at 800◦ C and 950◦ C under fully reversed (R = −1), strain-controlled loading through to failure. The experimentally determined and calculated stress–strain hysteresis loops for the ﬁrst and second cycles of the standard heat treated material are shown in Fig. 10.1. At 800◦ C, two strain rates have been used such that ramping times (the time over which the strain is applied linearly with time) of 1 and 10 s have been imposed resulting in the hysteresis loops shown in Fig. 10.1(a) and (b), respectively. Figure 10.1(c) shows the results for 950◦ C. In these cycles, a 1-s strain hold has been imposed at the tensile and compressive peak strains. At 800◦ C, this does not result in a distinctive stress relaxation, but this can be seen at 950◦ C in the computed result. However, the experiments show a much more progressive stress relaxation at the peak strains suggesting that the rate of relaxation is not well represented by the creep model. This occurs for a number of reasons. First, the creep model at 950◦ C was developed from experimental data obtained for a much lower stress level (a maximum of 50 MPa) whereas here, stresses of over 200 MPa are developed in the hysteresis loop. In addition, our cyclic plasticity model does not contain an explicit static recovery term,

Constitutive equations for C263 undergoing TMF

223

600

(a)

400 200 0 – 0.6

– 0.4

– 0.2

0

0.2

0.4

0.6

0

0.2

0.4

0.6

0

0.2

0.4

0.6

– 200 – 400 – 600 600

(b)

400 200 0 – 0.6

– 0.4

– 0.2 – 200 – 400 – 600 300

(c)

100

– 0.6

– 0.4

– 0.2

– 100

– 300 Experimental

Computed

Fig. 10.1 Experimental and computed LCF stress–strain curves for the ﬁrst and second cycles at (a) 800◦ C, 1 s ramping time, strain range 0.9%, (b) 800◦ C, 10 s ramping time, strain range 1%, and (c) 950◦ C, strain range 0.75%.

and further, the creep and plastic strain increments have, of course, been decoupled in the present work. Note that the microstructure of the material being loaded at 950◦ C is considerably different to that at 800◦ C because of the dissolution of the precipitate at the higher temperature. However, for both temperatures considered here, the peak stress levels are reasonably well predicted.

224

Cyclic plasticity, creep, and TMF

600

400 (b) (a)

200 (c) 0 0

200

400

600

800

1000

1200

1400

(c) – 200 (b)

(a)

– 400

– 600 Experimental

Computed

Fig. 10.2 Experimental and computed LCF peak stresses versus cycles at (a) 800◦ C, 1 s ramping time,

strain range 0.9%, (b) 800◦ C, 10 s ramping time, strain range 1%, and (c) 950◦ C, strain range 0.75%.

Figure 10.2 shows the comparisons of computed and experimental peak stresses versus cycles for each of the cases (a), (b), and (c) in Fig. 10.1, through to failure. Good predictions of life can be seen to be achieved for (b) and (c) for which intergranular creep cavitation dominates. Intergranular creep damage typically observed under these conditions is shown in Fig. 10.2. The life is overpredicted for (a) since creep damage accumulation has ceased to be the dominant failure process. A micrograph for these conditions shows that transgranular fracture is now occurring. Microstructural examination of specimens tested at 800◦ C and 950◦ C has been carried out after specimen failure. LCF tests carried out at 800◦ C, with 1-s ramp times, led to sample fracture surfaces showing transgranular cracking, as shown in Fig. 10.2, indicating that lifetime under these conditions is dominated by fatigue

Constitutive equations for C263 undergoing TMF

225

processes. However, microstructural examination of specimens also tested at 800◦ C but with a considerably longer ramp time of 10 s showed the development of intergranular damage, which dominated in some regions of the material. The lifetime of the material under these conditions may well be inﬂuenced quite strongly by creep damage processes. Examination of microstructures of specimens tested at 950◦ C showed that intergranular cracking dominated at these temperatures, even for a ramp time of 1 s. The dominant failure process for these conditions is intergranular creep fracture. The results of the tests carried out at 800◦ C shown in Fig. 10.2(a) and (b) show the development of macrocracking towards the end of the test which inﬂuences the observed stress–strain response which becomes different in tension and compression because of crack closure effects. The isotropic creep damage model used in the present work is not capable of predicting crack closure effects. The result at 950◦ C, however, which is dominated by creep softening and cavitation, does not show this effect. 10.3.1

TMF in C263 both above and below the γ solvus

TMF tests have been carried out on C263 under conditions of both in and out of phase loading. Strain controlled tests have been carried out between strains of zero and a peak of 0.6%, in which the temperature is also varied between 300◦ C and 950◦ C. The strain and temperature loading imposed, together with the results obtained, are shown in Fig. 10.3. First, considering the in-phase loading shown in Fig. 10.3(a), the experimental results obtained for the initial loading, below the γ solvus temperature, give stress levels that lie a little below that expected from both the solution treated and the standard treated material. After a time of 45 s, the temperature has exceeded 925◦ C, and in fact, the experimental results give stress levels that would be anticipated for such a material. It should be noted that prior to the imposition of the strain, the test specimen has undergone a prior temperature loading cycle. This is necessary to enable temperature compensation to be carried out on the TMF test rig. The consequence is that the material is, therefore, in effect in the solution treated state. The modelling of the behaviour has therefore been carried out with this assumption. For the cyclic plasticity modelling, two sets of material parameters were determined; one for the solution treated material (with the appropriate temperature dependence), and a further one for the standard treated material (i.e. for the material containing the precipitate volume fraction, which is dependent on temperature). The model for the solution treated plasticity and creep behaviour give the computed behaviour also shown in Fig. 10.3(a). As the temperature increases, a number of processes are taking place. The volume fraction of precipitate is decreasing, and at 925◦ C, becomes zero. The creep rate becomes determined by dislocation network

(a)

Strain (%)

Cyclic plasticity, creep, and TMF

300

0

0.1

0.3

0.5

0.7

– 300

(b)

Strain (%)

Strain (%)

300 200

Stress (MPa)

Temperature (8C)

0 – 0.1 – 100 – 200

100 – 0.7

– 0.5

0 – 0.1 – 100

– 0.3

0.1

– 200 – 300 Strain (%)

(c)

Strain (%)

800 600 400

Stress (MPa)

0.6 0.4 0.2 0 50 100 Time (s)

100

200 – 0.2

0 – 200 0

Temperature (8C)

Stress (MPa)

200

0.2

0.4

– 400 – 600 – 800 Strain (%) Experimental

Predicted

0.6

Temperature (8C)

226

1000 500 0

0

50 100 Time (s) Time (s) 50 100

0 0 – 0.2 – 0.4 – 0.6 1000 500 0 0

0

50 100 Time (s) Time (s) 50 100

0.4 – 0.1

1000 500 0 0

50 100 Time (s)

Fig. 10.3 Experimental and predicted stress–strain curves for (a) in-phase TMF at temperature range 300–950◦ C and (b) out-of-phase TMF at temperature range 300–950◦ C, and (c) in-phase TMF at temperature range 300–800◦ C .

pinning (Manonukul et al., 2002) and increases as the temperature increases. The combined effects of these processes result in the predicted decreasing stress level. At a time of 45 s, both the strain and temperature loading are reversed, and a comparatively small elastic region (though creep deformation is still occurring) can be seen, which

References

227

is followed by a conventional plasticity region in which creep deformation becomes negligibly small as the temperature decreases towards 300◦ C. Note that the material continues to harden during this phase, with no stress relaxation occurring at the higher compressive stresses because of the elimination of creep. The stress levels measured and predicted by the model are those that would be anticipated from the solution treated material. The standard heat treated material would show considerably higher stresses. With the reversal of the loading again, a rather larger elastic region is observed because of the increased yield stress at lower temperature, and because of the existing hardening that has already taken place. The measured and predicted stresses developed with increasing plastic deformation show good agreement and, unlike the ﬁrst quarter-cycle, are those that would be expected for the solution treated material. The loading conditions and results obtained for out-of-phase TMF are shown in Fig. 10.3(b). In this case, the high tensile stresses occur during the low temperature parts of the loading cycle, and conventional plastic behaviour is observed. At the higher temperatures, the material is in compression, but again, stress relaxation can be seen to occur, and the features of the experimentally obtained results can be seen to be reasonably reproduced. For in-phase TMF with the same strain range, but with the temperature varying between 300◦ C and 800◦ C, the experimental and predicted results obtained are shown in Fig. 10.3(c). Good comparisons are achieved for these conditions.

References Lemaitre, J. and Chaboche, J.-L. (1990). Mechanics of Solid Materials. Cambridge University Press, Cambridge. Manonukul, A., Dunne, F.P.E., and Knowles, D. (2001). ‘Thermo-mechanical fatigue in nickel-base superalloy C263’. Internal Report, Department of Engineering Science, Oxford University, England. Manonukul, A., Dunne, F.P.E., and Knowles, D. (2002). ‘Physically-based model for creep in nickel-base superalloy C263 both above and below the γ solvus’. Acta Materialia, 50, 2917–2931. Voyiadjis, G.Z. and Abu Al-Rub R.K. (2003). ‘Thermodynamic based model for the evolution equation of the backstress in cyclic plasticity’. International Journal of Plasticity, 19(12), 2121–2147. Yaguchi, M., Yamamoto, M., and Ogata, T. (2002a). ‘A viscoplastic constitutive model for nickel-base superalloy Part I: kinematic hardening rule of anisotropic dynamic recovery’. International Journal of Plasticity, 18(8), 1083–1109. Yaguchi, M., Yamamoto, M., and Ogata, T. (2002b). ‘A viscoplastic constitutive model for nickel-base superalloy Part II: modelling under anisothermal conditions’. International Journal of Plasticity, 18(8), 1111–1131.

This page intentionally left blank

Appendix A: Elements of tensor algebra

The dot (scalar) product of two ﬁrst-order tensors (vectors) gives a scalar

n NB. Einstein summation convention: ui vi = ui vi i=1

u · v = ui vi = v · u = vi ui =

n i=1 n

ui vi ,

(A1)

vi ui ,

(A2)

i=1

v · u = u · v.

(A3)

Double contraction (double dot product) of two second-order tensors gives a scalar σ : ε = σij εij =

n n

σij εij ,

(A4)

εij σij ,

(A5)

i=1 j =1

ε : σ = εij σij =

n n i=1 j =1

ε : σ = σ : ε.

(A6)

The dot product of a ﬁrst-order tensor with a second-order tensor gives a ﬁrst-order tensor n σij nj , (A7) σ · n ⇒ (σij nj )i = j =1

n · σ ⇒ (nj σji )i =

n j =1

nj σji ,

(A8)

230

Appendix A: Elements of tensor algebra

hence the expression n·σ =σ ·n

(A9)

is valid only if σ is symmetric (i.e. if σij = σji for any i, j ). The dyadic (direct) product of two ﬁrst-order tensors gives a second-order tensor u ⊗ v ⇒ (u ⊗ v)ij = ui vj . For example, if

⎡ ⎤ u1 ⎣ u = u2 ⎦ u3

then

⎡ ⎤ v1 ⎣ v = v2 ⎦ , v3

and

⎛

u1 v1 u ⊗ v = ⎝u2 v1 u3 v1

(A10)

⎞ u1 v3 u 2 v3 ⎠ . u3 v3

u1 v2 u2 v2 u3 v2

The product of two second-order tensors gives a second-order tensor a · b ⇒ (a · b)ij = aik bkj =

n

aik bkj .

(A11)

k=1

Double contraction (double dot product) of a third-order tensor with a second-order tensor gives a ﬁrst-order tensor ξ :σ =

3

ξijk σjk ei .

(A12)

i,j,k=1

Double contraction (double dot product) of a fourth-order tensor with a second-order tensor gives a second-order tensor c : ε ⇒ (c : ε)ij = cijkl εkl =

n n

cijkl εkl

(A13)

k=1 l=1

hence the expression c:ε=ε:c

(A14)

is valid only if c exhibits major symmetry (i.e. if cijkl = cklij for any i,j ,k,l). The dyadic (direct) product of two second-order tensors gives a fourth-order tensor f ⊗ g ⇒ (f ⊗ g)ijkl = fij gkl . Kronecker delta—a special second-order tensor / δij = 1, if i = j, δ ⇒ δij δij = 0, if i = j.

(A15)

(A16)

Appendix A: Elements of tensor algebra

231

The unit fourth-order tensor (exhibits major but not minor symmetry) I ⇒ Iijkl = δik δjl

(A17)

has the following important property I : ε = ε : I,

(A18)

which is valid for any second-order tensor ε. A symmetrized unit fourth-order tensor (exhibits both major and minor symmetry) s I s ⇒ Iijkl =

1 (δik δjl + δil δjk ) 2

(A19)

ensures the following identity I s : ε = ε : I s,

(A20)

which is valid only if the second-order tensor ε is symmetric.

Differentiation Differentiation of a tensor valued function (e.g. u, σ ) with respect to its tensorial argument (e.g. x, ε). Example: Differentiation of the ﬁrst-order tensor u with respect to the ﬁrst-order tensor x gives the second-order tensor ∂u ∂u ∂ui ⇒ = . (A21) ∂x ∂x ij ∂xj Special case: ∂u ⇒ ∂u

∂u ∂u

=δ= ij

∂ui = δij . ∂xj

(A22)

Example: Differentiation of the second-order tensor σ with respect to the secondorder tensor ε gives the fourth-order tensor ∂σij ∂σ ∂σ ⇒ = . (A23) ∂εkl ∂ε ∂ε ijkl Special case: ∂σ ⇒ ∂σ

∂σ ∂σ

=I= ijkl

∂σij = Iijkl . ∂σkl

(A24)

232

Appendix A: Elements of tensor algebra

The chain rule Example: Second-order tensor f depends on a second-order tensor u and a scalar v ∂fij ∂fij ∂umn ∂fij ∂v ∂f ∂u ∂f ∂v ∂f ∂f = : + ⊗ ⇒ = = + . ∂x ∂u ∂x ∂v ∂x ∂x ijkl ∂xkl ∂umn ∂xkl ∂v ∂xkl (A25) The gradient of a scalar ﬁeld gives a ﬁrst-order tensor ∇f ⇒

∂f . ∂xi

(A26)

The gradient of a ﬁrst-order tensor ﬁeld gives a second-order tensor ∇v ⇒

∂vj . ∂xi

(A27)

The gradient of a second-order tensor ﬁeld gives a ﬁrst-order tensor with its components being second-order tensors ∇σ ⇒ (∇σ )j = Hence,

⎡⎡ ∂σ

xx

⎢⎢ ∂x ⎢⎢ ⎢⎢ ∂σxx ⎢⎢ ⎢⎢ ∂y ⎢⎢ ⎢⎣ ∂σxx ⎢ ⎢ ⎢ ∂z ⎢ ⎢⎡ ∂σ yx ⎢ ⎢⎢ ⎢⎢ ∂x ⎢⎢ ⎢⎢ ∂σyx ∇σ = ⎢ ⎢⎢ ∂y ⎢⎢ ⎢⎢ ∂σyx ⎢⎣ ⎢ ∂z ⎢ ⎢ ⎢⎡ ⎢ ∂σzx ⎢ ⎢ ⎢ ∂x ⎢⎢ ⎢ ⎢ ∂σzx ⎢⎢ ⎢ ⎢ ∂y ⎢⎢ ⎣ ⎣ ∂σ zx ∂z

∂σij ∂σji = . ∂xi ∂xi

∂σxy ∂x ∂σxy ∂y ∂σxy ∂z ∂σyy ∂x ∂σyy ∂y ∂σyy ∂z ∂σzy ∂x ∂σzy ∂y ∂σzy ∂z

⎤ ∂σxz ⎤ ⎥ ∂x ⎥ ⎥⎥ ⎥ ∂σxz ⎥ ⎥⎥ ⎥ ∂y ⎥⎥ ⎥ ∂σxz ⎦⎥ ⎥ ⎥ ∂z ⎥ ⎥ ⎤ ∂σyz ⎥ ⎥ ⎥ ∂x ⎥ ⎥⎥ ⎥ ∂σyz ⎥ ⎥⎥ ⎥. ∂y ⎥ ⎥⎥ ⎥ ⎥ ∂σyz ⎥ ⎦⎥ ∂z ⎥ ⎥ ⎥ ⎤⎥ ∂σzz ⎥ ⎥ ⎥ ∂x ⎥ ⎥⎥ ⎥ ∂σzz ⎥ ⎥ ⎥ ⎥ ∂y ⎥ ⎥⎥ ∂σzz ⎦ ⎦ ∂z

(A28)

(A29)

Appendix A: Elements of tensor algebra

233

The divergence of a second-order tensor gives a ﬁrst-order tensor div σ = Tr[(∇σ )i ]. Hence,

⎡

⎡

∂σxx ⎢ ⎢ ∂x ⎢ ⎢ ⎢ ⎢ ∂σ xx ⎢Tr ⎢ ⎢ ⎢ ∂y ⎢ ⎢ ⎢ ⎢ ⎢ ⎣ ∂σxx ⎢ ⎢ ∂z ⎡ ⎤ ⎢ ⎢ ⎡ ∂σij ⎢ ∂σyx ⎢Tr ∂x ⎥ ⎢ ⎢ ⎢ i ⎥ ⎢ ⎢ ∂x ⎢ ⎥ ⎢ ⎢ ⎢ ⎥ ∂σij ⎥ ⎢ ⎢ ⎢ ∂σyx ⎢ div σ = ⎢Tr = ⎢Tr ⎢ ⎥ ∂xi ⎥ ⎢ ⎢ ∂y ⎢ ⎥ ⎢ ⎢ ⎢ ⎣ ∂σyx ⎣ ∂σij ⎦ ⎢ ⎢ Tr ⎢ ∂z ⎢ ∂xi ⎢ ⎡ ⎢ ∂σzx ⎢ ⎢ ⎢ ∂x ⎢ ⎢ ⎢ ⎢ ⎢ ⎢ ∂σzx ⎢ Tr ⎢ ⎢ ⎢ ∂y ⎢ ⎢ ⎣ ⎣ ∂σzx ∂z

(A30)

⎤⎤ ∂σxy ∂σxz ∂x ∂x ⎥ ⎥⎥ ⎥ ∂σxy ∂σxz ⎥ ⎥⎥ ⎥⎥ ∂y ∂y ⎥⎥ ⎥⎥ ⎥ ∂σxy ∂σxz ⎦⎥ ⎥ ∂z ∂z ⎥ ⎥ ⎤⎥ ⎡ ⎤ ∂σxy ∂σxz ∂σxx ∂σyy ∂σyz ⎥ ⎥ + + ⎥ ⎢ ∂y ∂z ⎥ ∂x ∂x ⎥ ⎥⎥ ⎢ ∂x ⎥ ⎥ ⎥ ⎢ ∂σyy ∂σyz ⎥⎥ ⎢ ∂σyx ∂σyy ∂σyz ⎥ ⎥ + + ⎥⎥ = ⎢ ⎥. ∂y ∂y ⎥⎥ ⎢ ∂x ∂y ∂y ⎥ ⎥⎥ ⎢ ⎥ ⎣ ∂σzx ∂σyy ∂σyz ⎦⎥ ∂σzy ∂σzz ⎦ ⎥ + + ∂z ∂y ⎥ ∂x ∂y ∂z ⎥ ⎤⎥ ∂σzy ∂σzz ⎥ ⎥ ⎥ ∂x ∂x ⎥ ⎥⎥ ⎥ ∂σzy ∂σzz ⎥ ⎥⎥ ⎥⎥ ∂y ∂y ⎥ ⎥ ⎥⎥ ∂σzy ∂σzz ⎦ ⎦ ∂z ∂z (A31)

Rotation Finite rotation is mathematically described by the orthogonal second-order tensor R −1 = R T ,

(A32)

which transforms a ﬁrst-order tensor as follows x = R · x

(A33)

σ = R · σ · RT .

(A34)

and a second-order tensor as follows

Successive ﬁnite rotations do not commute, that is, R 1 · R 2 = R 2 · R 1 .

(A35)

234

Appendix A: Elements of tensor algebra

r

z

r y

x

r0 =

r r

Fig. A.1 Finite rotation vector.

r1 If the axis r = r2 and the magnitude r = |r| of a ﬁnite rotation are known the r3 orthogonal second-order tensor which describes such rotation can be expressed in the form of an exponential function as follows: R = exp[ˆr ] = I + rˆ +

1 2 rˆ + · · ·, 2!

(A36)

where rˆ is the associated skew-symmetric tensor ⎤ ⎡ 0 −r3 r2 rˆ = ⎣ r3 0 −r1 ⎦ , −r2 r1 0

(A37)

which satisﬁes rˆ · r = 0,

(A38)

rˆ · x = r × x as illustrated in Fig. A.1. Small rotations can be approximated by

⎡

1 1 2 ⎣ R = exp[ˆr ] = I + rˆ + rˆ + · · · ≈ I + rˆ = 0 2! 0

0 1 0

⎤ ⎡ 0 0 ⎦ ⎣ 0 + r3 1 −r2

−r3 0 r1

⎤ r2 −r1 ⎦ , 0 (A39)

which do commute (I + rˆ 1 ) · (I + rˆ 2 ) = (I + rˆ 2 ) · (I + rˆ 1 ) = I + rˆ 1 + rˆ 2 + rˆ 1 · rˆ 2 ≈ I + rˆ 1 + rˆ 2 . (A40)

Appendix B: Fortran coding available via the OUP website∗

Directory/ﬁle

Description

elasticity elastic.f

UMAT for plane strain and axial symmetry for elastic behaviour using ABAQUS stress and strain quantities

elas_axidisp.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial displacement controlled loading, requiring UMAT elastic.f

elas_axiforce.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial force controlled loading, requiring UMAT elastic.f

plasticity_exp code_exp.f

UMAT for plane strain and axial symmetry for elastic, linear strain hardening plastic behaviour using explicit integration with continuum Jacobian, using ABAQUS stress and strain quantities. Suitable for large deformations

plas_exp_axidisp_aba.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial displacement controlled loading, using ABAQUS *PLASTIC

plas_exp_axiforce_aba_inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial force controlled loading, using ABAQUS *PLASTIC

∗ www.oup.co.uk/isbn/0–19–856826–6

236

Appendix B: Fortran coding

plas_exp_axidisp.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial displacement controlled loading, requiring UMAT code_exp.f

plas_exp_axiforce.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial force controlled loading, requiring UMAT code_exp.f

plas_exp_beam_aba.inp

Four point bend loading using ABAQUS*PLASTIC, requiring mesh ﬁle beam_mesh.inp

plas_exp_beam.inp

Four point bend loading requiring UMAT code_exp.f, requiring mesh ﬁle beam_mesh.inp

plasticity_imp code_imp.f

UMAT for plane strain and axial symmetry for elastic, linear strain hardening plastic behaviour using implicit integration with consistent Jacobian, using ABAQUS stress and strain quantities. Suitable for large deformations

plas_imp_axidisp_aba.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial displacement controlled loading, using ABAQUS *PLASTIC

plas_imp_axiforce_aba_inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial force controlled loading, using ABAQUS *PLASTIC

plas_imp_axidisp.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial displacement controlled loading, requiring UMAT code_imp.f

plas_imp_axiforce.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial force controlled loading, requiring UMAT code_imp.f

plas_imp_beam_aba.inp

Four point bend loading using ABAQUS*PLASTIC, requiring mesh ﬁle beam_mesh.inp

plas_imp_beam.inp

Four point bend loading requiring UMAT code_imp.f, requiring mesh ﬁle beam_mesh.inp

Appendix B: Fortran coding

237

spin spin_elastic.f

UMAT for three-dimensional, plane strain, and axial symmetry for elastic behaviour using ABAQUS stress and strain quantities

spin_elas_def.f

UMAT for three-dimensional, plane strain, and axial symmetry for elastic behaviour using the deformation gradient

spin_axidisp.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial displacement controlled loading, requiring UMAT spin_elas_def.f

spin_axiforce.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial force controlled loading, requiring UMAT spin_elas_def.f

spin_shear.inp

ABAQUS input ﬁle for a single plane strain element under simple shear, requiring UMAT spin_elas_def.f

spin_shear_aba.inp

ABAQUS input ﬁle for a single plane strain element under simple shear, using ABAQUS*ELASTIC

visco uni_visco_imp.f

Closed form Fortran implicit solution for uniaxial elasto-viscoplasticity

uni_visco_exp.f

Closed form Fortran explicit solution for uniaxial elasto-viscoplasticity

visco_imp.f

UMAT for plane strain and axial symmetry for elastic, linear strain hardening viscoplastic behaviour using implicit integration using the initial tangent stiffness, using ABAQUS stress and strain quantities. Suitable for large deformations

visco_imp_axidisp.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial displacement controlled loading, requiring UMAT visco_imp.f

238

Appendix B: Fortran coding

visco_imp_axiforce.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial force controlled loading, requiring UMAT visco_imp.f

visco_imp_beam.inp

Four point bend loading requiring UMAT visco_beam.f, requiring mesh ﬁle beam_mesh.inp

Index

ABAQUS 141, 149, 150, 167, 169, 235 ABAQUS input ﬁles 169 accumulated plastic strain 23 Almansi strain 50 angular velocity tensor 63 anisothermal cyclic plasticity 220 antisymmetric 51 Armstrong–Frederick 21 associated ﬂow 18 axial vibration 106, 115 B matrix 99 back stress 29 backward Euler integration 146, 161 Bauschinger effect 28 bcc 6 biaxial creep tests 213 bowing 212 Burger’s vector 8

calculus of variations 85 cantilever beam 118 Cauchy stress 72 Cauchy–Green tensor 49, 50 cavitation 210 central difference method 136 Chaboche 31 coarsening 209 combustion chambers 209 conservation of energy 84 consistency condition 20 consistent Jacobian 153 consistent tangent stiffness 153 consolidation 199 constant strain element 99 constitutive equations 40 continuum tangent stiffness 172 continuum damage 210 continuum Jacobian 172 continuum plasticity 10 continuum spin 61 contracted tensor product 15

convergence 140 co-rotational 73 creep 209 CREEP subroutine 202 critical resolved shear stress 7 crystal plasticity 5, 9 crystallographic orientation 3 crystallographic slip 5 cyclic hardening 37 cyclic plasticity 219

deformation-enhanced grain growth 190 deformation gradient 48 deformed conﬁguration 48 densiﬁcation rate 201 deviatoric stress 14 diagonalization 56 differentiation of a tensor 231 dilatation 201 direction of plastic ﬂow 19 dislocation bowing 212 dislocation density 210 displacement-based ﬁnite element method 98 divergence of a second-order tensor 233 double contracted product 15 Duva and Crow 200 dyadic product 230 dynamical path 84

effective plastic strain rate 14 effective stress 13 elastic predictor 147 elastic stiffness matrix 22, 100 elastic–plastic deformation 11 engineering shears 100 equations of motion 90 equilibrium 83 equivalent stress 13 Euler–Lagrange equation 86 explicit ﬁnite element methods 1, 141 explicit integration 136, 143

240

Index

fcc 6 ﬁnite element formulation for plasticity 133 ﬁnite element method 83 ﬁnite rotations 57 ﬁrst variation 87 forward integration 145 Gauss quadrature 126 geometric non-linearity 108 gradient of a ﬁrst-order tensor 232 gradient of a scalar 232 gradient of a second-order tensor 232 grain boundaries 3 grain growth 190 grain size 190 Hamilton’s principle 84 hardening 23 Helmholtz free energy 210 Hooke’s law 22, 170 hydrostatic stress 14 hysteresis 222 identity tensor 42 implicit 140, 143 implicit ﬁnite element methods 143 implicit implementation for elasto-viscoplasticity 161 implicit integration 146 implicit scheme 146 incompressibility 3, 12 incremental nature of plasticity 35 incremental rotation 176 initial tangential stiffness method 140 integration point 126 intergranular cracking 224 intergranular creep fracture 217 intermediate conﬁguration 66 internal variables 40 isoparametric 109 isotropic hardening 150 J2 plasticity 17 Jacobian 150 Jaumann stress rate 76 J-integral 84 Kinematic hardening 27 kinematics 47 kinetic energy 84 Lagrangian 84 Lame constant 42 large deformation(s) 47 leap frog explicit method 137

mass and spring system 90 mass matrix 105 material objectivity 69 material reference frame 48 material stress rate 78 mean stress 14 microstructural evolution 190 Mohr’s circle 69 momentum balance equations 106 multiaxial creep strain rate 212 multiaxial stress state 20, 212 multiplicative decomposition 67 necking 187 Newton iteration 148 Newton’s method 148 Newton–Raphson method 141 nickel alloy C263 209 nickel-base superalloy 209 nodal force vector 112 nodal forces 107 non-conservative 84 non-linear kinematic hardening 32 norm 30 normal grain growth 190 normality hypothesis 18 notched bar test 215 objective stress 72 objectivity 69 one-dimensional rod element 99 original conﬁguration 48 orthogonality 58 out of phase loading 225 over-stress 38 particle cutting 209 perfect plasticity 11 plane stress 18 plastic correction 146 plastic deformation gradient 66 plastic multiplier 19 plastic strain rate tensor 14 polar decomposition theorem 57 polycrystal 3 polycrystalline 3 porosity 199 porous plasticity 199 potential energy 84 potential function 45 power-law creep 44 Prager 29 precipitate coarsening 209 precipitate cutting 209 precipitate spacing 210 predictor–corrector 146 principal coordinates 56

Index

principal stresses 13 principle of virtual work 90 quasi-static problems 105 radial return method 146 rate-dependent plasticity 38 rate of deformation 60 reaction 130 reversed plasticity 28, 219 rigid body rotation 57 rotation 233 rotation matrix 58 Schmid’s law 7 second-order tensors 229 second stress invariant 17 semi-implicit integration 160 shape functions 97 shearing 3 simple shear 58 single and multiple element uniaxial tests 171 single element simple shear test 178 skew 51 slip system 5 solvus temperature 209 spin 61 stability of the explicit time stepping 139 static grain growth 190 stationary value 87 stiffness matrix 105 strain decomposition 11 strain measure 49 strain-rate sensitivity 39, 186 strain tensor 100 stress space 17 stress tensor 14 stress transformation 72 stress vector 70 stretch 48 stretch ratios 54 superplastic forming 192 Superplasticity 185

tangent stiffness 140, 150 tangential stiffness matrix 150 tension–torsion 213 tensorial notation 229 tensors 229 thermo-mechanical fatigue 219 thinning 195 time-dependent plasticity 38 time-independent plasticity 11 Ti–MMCs 205 titanium alloy, Ti–6Al–4V 189 traction 70 transformation of stress 72 transverse vibration 118, 122 Tresca 17 trial stress 147 true strain 53 truss element 99

UMAT 169 undeformed conﬁguration 48 uniaxial loading 14, 42 update of stress 143 upsetting 42

velocity gradient 60 veriﬁcation of the model implementation 171 virtual work 90 viscoplasticity 38 viscous stress 39 Voigt notation 19, 100 volume changes 199 von Mises 17

weak formulation 83 work conjugacy 111

yield criteria 17 yield function 17 yielding 3

241

This page intentionally left blank

(a)

(b) Strain rate

Strain rate

+ 0.00E – 00 + 2.00E – 06 + 3.00E – 06 + 4.00E – 06 + 5.00E – 06 + 6.00E – 06 + 7.00E – 06 + 8.00E – 06

+ 0.00E – 00 + 2.00E – 06 + 3.00E – 06 + 4.00E – 06 + 5.00E – 06 + 6.00E – 06 + 7.00E – 06 + 8.00E – 06

(c)

Strain rate + 0.00E – 00 + 2.00E – 06 + 3.00E – 06 + 4.00E – 06 + 5.00E – 06 + 6.00E – 06 + 7.00E – 06 + 8.00E – 06

Plate 1 The simulated superplastically deforming sheet showing the effective plastic strain rate at fractional processing times of t/tf = 0.1, t/tf = 0.6, and t/tf = 1.0.

(b)

(a) Thickness strain – 1.20E + 00 – 1.07E + 00 – 9.15E – 01 – 7.60E – 01 – 6.05E – 01 – 4.50E – 01 – 2.95E – 01 – 1.40E – 01

Thickness strain – 1.20E + 00 – 1.07E + 00 – 9.15E – 01 – 7.60E – 01 – 6.05E – 01 – 4.50E – 01 – 2.95E – 01 – 1.40E – 01

Plate 2 Through-thickness strain ﬁelds at the end of the superplastic forming carried out with target maximum strain rates of (a) 1.0 × 10−5 and (b) 1.0 × 10−4 s−1 .

(a)

(b) Grain sizes

Grain sizes

+7.93E – 03 +8.06E – 03 +8.20E – 03 +8.33E – 03 +8.60E – 03 +8.74E – 03 +8.88E – 03 +9.01E – 03

+ 1.14E – 02 + 1.15E – 02 + 1.16E – 02 + 1.16E – 02 + 1.17E – 02 + 1.18E – 02 + 1.18E – 02 + 1.19E – 02

Plate 3 Average grain size ﬁelds at the end of the superplastic forming carried out with target maximum strain rates of (a) 1.0 × 10−5 and (b) 1.0 × 10−4 s−1 .

Cavitation damage parameter

(a)

+0.00E+00 +2.00E–02 +4.36E–02 +6.73E–02 +9.09E–02 +1.15E–01 +1.38E–01 +1.62E–01 +1.85E–01 +2.09E–01 +2.33E–01 +2.56E–01 +2.80E–01 +3.00E–01

(b) (c) 2

7

6

8

3

2

2

0

2

2

5

0

0

Number of creep voids

7

12

7

2

4

4

4

15

6

3

0

2

9

9

5

2

0

0 1–3 4–6 7–9 10–12 13

1

3

4

22

8

2

5

1

17

30

1

Plate 4 Creep damage ﬁelds (a) predicted by the model, (b) observed in the microstructure, and (c) from a surface void count using the micrograph.

This page intentionally left blank

Introduction to Computational Plasticity FIONN DUNNE AND NIK PETRINIC Department of Engineering Science Oxford University, UK

1

3

Great Clarendon Street, Oxford ox2 6dp Oxford University Press is a department of the University of Oxford. It furthers the University’s objective of excellence in research, scholarship, and education by publishing worldwide in Oxford New York Auckland Cape Town Dar es Salaam Hong Kong Karachi Kuala Lumpur Madrid Melbourne Mexico City Nairobi New Delhi Shanghai Taipei Toronto With ofﬁces in Argentina Austria Brazil Chile Czech Republic France Greece Guatemala Hungary Italy Japan Poland Portugal Singapore South Korea Switzerland Thailand Turkey Ukraine Vietnam Oxford is a registered trade mark of Oxford University Press in the UK and in certain other countries Published in the United States by Oxford University Press Inc., New York © Oxford University Press, 2005 The moral rights of the authors have been asserted Database right Oxford University Press (maker) First published 2005 Reprinted 2006 (with corrections) All rights reserved. No part of this publication may be reproduced, stored in a retrieval system, or transmitted, in any form or by any means, without the prior permission in writing of Oxford University Press, or as expressly permitted by law, or under terms agreed with the appropriate reprographics rights organization. Enquiries concerning reproduction outside the scope of the above should be sent to the Rights Department, Oxford University Press, at the address above You must not circulate this book in any other binding or cover and you must impose the same condition on any acquirer British Library Cataloguing in Publication Data (Data available) Library of Congress Cataloging in Publication Data (Data available) Typeset by Newgen Imaging Systems (P) Ltd., Chennai, India Printed in Great Britain on acid-free paper by Biddles Ltd, King’s Lynn ISBN 0-19-856826-6 (Hbk)

978-0-19-856826-1

3 5 7 9 10 8 6 4 2

To Hannah and Roberta, with love

This page intentionally left blank

Preface

The intention of this book is to bridge the gap between undergraduate texts in engineering plasticity and the many excellent books in computational plasticity aimed at more senior graduate students, researchers, and practising engineers working in solid mechanics. The book is in two parts. The ﬁrst introduces microplasticity and covers continuum plasticity, the kinematics of large deformations and continuum mechanics, the ﬁnite element method, implicit and explicit integration of plasticity constitutive equations, and the implementation of the constitutive equations, and the associated material Jacobian, into ﬁnite element software. In particular, the implementation into the commercial code ABAQUS is addressed (and to help, we provide a range of ABAQUS material model UMATs), together, importantly, with the tests necessary to verify the implementation. Our intention, wherever possible, is to develop a good physical feel for the plasticity models and equations described by considering, at every stage, the simpliﬁcation of the equations to uniaxial conditions. In addition, we hope to provide a reasonably physical understanding of some of the large deformation quantities (such as the continuum spin) and concepts (such as objectivity) which are often unfamiliar to many undergraduate engineering students who demand more than just a mathematical description. The second part of the book introduces a range of plasticity models including those for superplasticity, porous plasticity, creep, cyclic plasticity, and thermo-mechanical fatigue (TMF). We also describe a number of practical applications of the plasticity models introduced to demonstrate the reasonable maturity of continuum plasticity in engineering practice. We hope, above all, that this book will help all those—undergraduates, graduates, researchers, and practising engineers—who need to move on from knowledge of undergraduate plasticity to modern practice in computational plasticity. Our aims have been to encourage development of understanding, and ease of passage to the more advanced texts on computational plasticity. September 2004

F. P. E. D. and N. P.

This page intentionally left blank

Contents Acknowledgements

xii

Notation

xiii

Part I. Microplasticity and continuum plasticity 1. 1.1 1.2 1.3 1.4

2. 2.1 2.2 2.3 2.4 2.5 2.6 2.7

3. 3.1 3.2 3.3 3.4 3.5

Microplasticity Introduction Crystal slip Critical resolved shear stress Dislocations Further reading Continuum plasticity Introduction Some preliminaries Yield criterion Isotropic hardening Kinematic hardening Combined isotropic and kinematic hardening Viscoplasticity and creep Further reading Kinematics of large deformations and continuum mechanics Introduction The deformation gradient Measures of strain Interpretation of strain measures Polar decomposition

3 3 5 7 8 10 11 11 11 17 23 27 36 38 45 47 47 48 49 52 57

x

Contents

3.6 3.7 3.8 3.9

Velocity gradient, rate of deformation, and continuum spin Elastic–plastic coupling Objective stress rates Summary Further reading

60 66 69 81 82

4.

The ﬁnite element method for static and dynamic plasticity

83

Introduction Hamilton’s principle Introduction to the ﬁnite element method Finite element equilibrium equations Integration of momentum balance and equilibrium equations Further reading

83 84 96 100 136 142

4.1 4.2 4.3 4.4 4.5

5. 5.1 5.2 5.3 5.4 5.5 5.6

6. 6.1 6.2 6.3 6.4 6.5 6.6

Implicit and explicit integration of von Mises plasticity Introduction Implicit and explicit integration of constitutive equations Material Jacobian Kinematic hardening Implicit integration in viscoplasticity Incrementally objective integration for large deformations Further reading Implementation of plasticity models into ﬁnite element code Introduction Elasticity implementation Veriﬁcation of implementations Isotropic hardening plasticity implementation Large deformation implementations Elasto-viscoplasticity implementation

143 143 143 150 154 161 167 168 169 169 170 171 172 176 180

Part II. Plasticity models 7. 7.1 7.2

Superplasticity Introduction Some properties of superplastic alloys

185 185 185

Contents

7.3 7.4

8.

Constitutive equations for superplasticity Multiaxial constitutive equations and applications References Porous plasticity

8.1 8.2

Introduction Finite element implementation of the porous material constitutive equations Application to consolidation of Ti–MMCs References

8.3

9.

Creep in an aero-engine combustor material

9.1 9.2 9.3

Introduction Physically based constitutive equations Multiaxial implementation into ABAQUS References Appendix 9.1

xi

189 192 197 199 199 201 205 207 209 209 209 212 217 218

10. Cyclic plasticity, creep, and TMF

219

10.1 Introduction 10.2 Constitutive equations for cyclic plasticity 10.3 Constitutive equations for C263 undergoing TMF References

219 219 222 227

Appendix A: Elements of tensor algebra

229

Differentiation The chain rule Rotation

231 232 233

Appendix B: Fortran coding available via the OUP website

235

Index

239

Acknowledgements

The authors would like to express their sincere gratitude to Esteban Busso for reading a draft and providing many helpful comments and suggestions, to Paul Buckley for the provision of the ﬁgures in Chapter 1, and to Jinguo Lin for permission to use Figures 7.9–7.14. The authors acknowledge, with gratitude, permission granted to reproduce the following ﬁgures: Figures 7.9–7.14: Elsevier Ltd, Oxford, UK. Figures 8.1–8.6: Institute of Materials Communications Ltd, London, UK. Figures 9.1–9.4, 10.1–10.3: Elsevier Ltd, Oxford, UK.

Notation

• Regular italic typeface (v, σ, . . .): scalars, scalar functions. • Bold italic typeface (P , v, A, σ , . . .): points, vectors, tensors, vector and tensor functions. • Helvetica bold italic typeface (C, c, I, . . .): fourth order tensors.

Operations f (·) det[·] Tr[·] ln(·) [·] ∂ [·] ∂x ∇(·) = grad[·] div[·] = tr[∇(·)] x·y x⊗y σ :ε √ |u| = √u · u |A| = A : A

function of (·) determinant of [·] trace of [·] logarithm of (·) increment of [·] partial derivative of [·] with respect to x gradient of [·] divergence of [·] scalar product of vectors dyadic product of vectors double contraction of tensors norm of vector norm of tensor

Some commonly used notation C D E E ε

fourth-order tensor of material constants rate of deformation tensor Lagrangian strain tensor Young’s modulus strain tensor

xiv

F f ρ I J K M ν P P R R σ t t u u˙ u¨ W

Notation

deformation gradient force vector ﬁeld density second-order identity tensor Jacobian stiffness matrix mass matrix Poisson’s ratio material particle material point ∈ Rn rotation tensor real set Cauchy stress tensor time surface traction vector displacement vector ﬁeld velocity vector ﬁeld acceleration vector ﬁeld work

Part I. Microplasticity and continuum plasticity

This page intentionally left blank

1. Microplasticity

1.1

Introduction

This chapter brieﬂy introduces the origins of yield and plastic ﬂow, and in particular, attempts to explain the usual assumptions in simple continuum plasticity of isotropy, incompressibility, and independence of hydrostatic stress. While short, we introduce grains, crystal slip, slip systems, resolved shear stress, and dislocations; the minimum knowledge of microplasticity for users of continuum plasticity. The origin of plasticity in crystalline materials is crystal slip. Metals are usually polycrystalline; that is, made up of many crystals in which atoms are stacked in a regular array. A typical micrograph for a polycrystalline nickel-base superalloy is shown in Fig. 1.1 in which the ‘crystal’ or grain boundaries can be seen. The grain size is about 100 µm. The grain boundaries demarcate regions of different crystallographic orientation. If we represent the crystallographic structure of a tiny region of a single grain by planes of atoms, as shown in Fig. 1.2(a), we can then visualize plastic deformation taking place as shown in Fig. 1.2(a) and (b); this is crystallographic slip. Unlike elastic deformation, involving only the stretching of interatomic bonds, slip requires the breaking and re-forming of interatomic bonds and the motion of one plane of atoms relative to another. After shearing the crystal from conﬁguration 1.2(a) to conﬁguration 1.2(b), the structure is unchanged except at the extremities of the crystal. A number of very important phenomena in macroscopic plasticity become apparent from just two Figs 1.1 and 1.2: (1) plastic slip does not lead to volume change; this is the incompressibility condition of plasticity; (2) plastic slip is a shearing process; hydrostatic stress, at the macrolevel, can often be assumed not to inﬂuence slip; (3) in a polycrystal, plastic yielding is often an isotropic process. As we will see later, the incompressibility condition is very important in macroscale plasticity and manifests itself at the heart of constitutive equations for plasticity.

4

Microplasticity

100 mm

Fig. 1.1 Micrograph of polycrystal nickel-base alloy C263. (a)

τ

τ

(b)

τ

τ

Fig. 1.2 Schematic representation of the crystallographic structure within a single grain undergoing slip.

However, not all plastic deformation processes are incompressible. A porous metal, for example, under compressive load may undergo plastic deformation during which the pores reduce in size. Consequently, there is a change of volume and a dependence on hydrostatic stress. However, the volume change does not originate from the plastic slip process itself, but from the pore closure. The fact that plastic slip is a shearing process gives more information about the nature of yielding; in principle, it tells us that plastic deformation is independent of hydrostatic stress (pressure). For non-porous metals, this is one of the cornerstones of yield criteria. The von Mises criterion, for example, is one in which the initiation of macroscale yield is quite independent of hydrostatic stress. If we take a sample of the theoretical material shown schematically in Fig. 1.2(a) and submerge it to an ever deeper depth in an imaginary sea of water, the hydrostatic stress becomes ever larger but causes no more than the atoms in the theoretical material to come closer together. It will never in itself be able to generate the shearing necessary for crystallographic slip. Figure 1.1 shows a micrograph of a polycrystal. If we assume that there is no preferred crystallographic orientation, but that the orientation changes randomly from one

Crystal slip

(a)

5

(b)

Fig. 1.3 (a) Photograph of a single zinc crystal and (b) a schematic diagram representing single slip in a single crystal.

grain to the next, and if our sample of material contains a sufﬁciently large number of grains, we can get a reasonable physical feel that macroscale yielding of the material will be isotropic. This is a further cornerstone of the von Mises yield criterion.

1.2

Crystal slip

The evidence for crystal slip being the origin of plasticity comes from mechanical tests carried out on single crystals of metals. The single crystal of zinc shown in Fig. 1.3(a) is a few millimetres in width and has been loaded beyond yield in tension. The planes that can be seen are those on which slip has occurred resulting from many hundreds of dislocations running through the crystal and emerging at the edge. Each dislocation contributes just one Burger’s vector of relative displacement, but with many such dislocations, the displacements become large. Figure 1.3(b) shows schematically what is happening in Fig. 1.3(a). The ends of the test sample have not been constrained in the lateral directions. It can be seen that single slip in this case leads to the horizontal displacement of one end relative to the other. Had this test been carried out in a conventional uniaxial testing machine, the lateral motion would have been prevented. In order to retain compatibility, then, with the imposed axial displacement, the slip planes would have to rotate towards the loading direction. The uniaxial loading therefore leads not only to crystallographic slip, but also to rotation of the crystallographic lattice.

1.2.1

Slip systems: slip directions and slip normals

Observations on single crystals show that slip tends to occur preferentially on certain crystal planes and in certain speciﬁc crystal directions. The combination of a slip

6

Microplasticity

(111)

–

[110]

¯ in an fcc lattice. Fig. 1.4 The particular slip system (111)[110] (112)

(101)

(123)

–

(111)

Fig. 1.5 Slip systems in bcc materials.

plane and a slip direction is called a slip system. These tend to be the most densely packed planes and the directions in which the atoms are packed closest together. This is explained in terms of dislocations. In face centred cubic (fcc) materials, the most densely packed planes are the diagonal planes of the unit cell. In fact the crystal is ‘close-packed’ in these planes; the observed slip systems are shown in Fig. 1.4. ¯ The full family of slip systems in such crystals may be written as 110{111}. There are 12 such systems in an fcc crystal (four planes each with three directions). In body centre cubic (bcc) crystals, there are several planes that are of similar density of packing, and hence there are several families of planes on which slip occurs. However, there is no ambiguity about the slip direction, since the atoms are closest ¯ direction and those equivalent to it. The slip systems observed in bcc along the [111] crystals are shown in Fig. 1.5. Thus, there are three families of slip systems operative: ¯ 111{101};

¯ 111{112};

¯ 111{123}.

Table 1.1 shows the slip systems found in single crystals of some of the important fcc and bcc pure metals together with the resolved shear stress required to cause slip—the critical resolved shear stress (CRSS).

Critical resolved shear stress

7

Table 1.1 Slip systems and CRSS for some pure metals. Metal

Structure

Slip systems

CRSS (MPa)

Cu Al Ni

fcc fcc fcc

¯ 110{111} ¯ 110{111} ¯ 110{111}

0.64 0.40 5.8

α-Fe Mo Ta

bcc bcc bcc

¯ ¯ ¯ 111{101}, 111{112}, 111{123} ¯ 111{101} ¯ ¯ ¯ 111{101}, 111{112}, 111{123}

32 50 50

t Slip plane normal

n s f

l

s Slip direction

Fig. 1.6 A single crystal containing slip plane with normal n, slip direction s, and loaded in direction t.

1.3

Critical resolved shear stress

Suppose a single crystal in the shape of a rod is tested in tension. The axis of the rod is parallel to unit vector t. The crystal has an active slip plane, normal in direction of unit vector n. It has an active slip direction parallel to unit vector s, as shown in Fig. 1.6. When the applied tensile stress is σ , the shear stress acting on the slip plane and in the slip direction is τ which may be found as follows: if the cross-sectional area of the rod is A, the force in the slip direction is Aσ cos λ and it acts on an area A/cos φ of the slip plane. Hence the resolved shear stress is τ = σ cos φ cos λ = σ (t · n)(t · s).

(1.1)

Slip will take place on the slip system, that is, the crystal will yield, when τ reaches the CRSS. This is known as Schmid’s law. The data shown in Fig. 1.7 were obtained from tensile tests on cadmium single crystals which are hexagonal close packed (hcp). The measured yield stress depends upon the angle between the tensile loading direction and the basal plane. The minimum stress to cause yield occurs when the tensile axis is 45◦ to this plane, that is, when the shear stress is maximized. Schmid’s law provides a good explanation for the observed behaviour.

8

Microplasticity 7 Data Schmid’s law

Yield stress (MPa)

6 5 4 3 2 1 0 0

30 60 90 Angle between tensile axis and basal plane

Fig. 1.7 The dependence of yield stress on the angle between the tensile axis and basal plane in an hcp cadmium single crystal.

b

Fig. 1.8 An edge dislocation.

1.4

Dislocations

The theoretical shear strength of a crystal, calculated assuming that the shear is homogeneous (the entire crystal shears simultaneously on one plane), is given by G . τth = 2π The expected shear strength is therefore very large; many orders of magnitude greater than the CRSS values are shown in Table 1.1. The assumption of homogeneous shear is, of course, wrong and plastic deformation in crystals normally occurs by the movement of the line defects known as dislocations, that are usually present in large numbers. The glide of a dislocation involves only very local rearrangements of atoms close to it, and requires a stress much lower than τth , thereby explaining the low observed values of CRSS. Each dislocation is associated with a unit of slip displacement given by the Burgers vector b. Since the dislocation is a line defect, there are two extreme cases. Figure 1.8 shows a schematic representation of an edge dislocation. In this case the Burgers vector b is perpendicular to the line of the dislocation, and the dislocation corresponds to the edge of a missing half-plane of atoms. Thus b and

Dislocations

9

b

Fig. 1.9 A screw dislocation.

the dislocation line deﬁne a plane: a speciﬁc slip plane. If l is a unit vector parallel to the dislocation line, then s=

b |b|

and

n=

b×l . |b|

(1.2)

Figure 1.9 shows a schematic representation of a screw dislocation. This is the other extreme case where the Burger’s vector is parallel to the dislocation line. The dislocation itself corresponds to a line of scissors-like shearing of the crystal. It follows from the fact that b is parallel to l, that, although the slip direction s is deﬁned, the slip plane n is not. Hence, a screw dislocation can cause slip on any slip plane containing l. Dislocations are therefore vital in understanding yield and plastic ﬂow. We have said nothing about the important role of dislocations in strain hardening and softening. Nor have we discussed the effect of temperature on diffusivity which inﬂuences or controls many plastic deformation mechanisms including thermally activated dislocation climb leading to recovery, vacancy core and boundary diffusion, and grain boundary sliding. All of these subjects can be found in existing materials text books, some of which are listed below. Our aim has been to include sufﬁcient material on microplasticity to ensure that the physical bases of at least some of the assumptions made in macrolevel continuum plasticity are understood. There have been many developments over the last 25 years in physically based microplasticity modelling, including the development of time-independent and ratedependent crystal plasticity. Here, for a given crystallographic lattice (e.g. fcc), using ﬁnite element techniques, the resolved shear stresses on all slip systems can be determined to ﬁnd the active slip systems. Within either a time-independent or rate-dependent formulation, the slip on each active system can be determined from which the overall total deformation can be found. Such models are being used successfully for the plastic and creep deformation of single crystal materials which ﬁnd application in aero-engines. The modelling of single crystal components has become

10

Microplasticity

possible with the development of high-performance computing. More recently, using ﬁnite element techniques, polycrystal plasticity models have been developed. Here, the understanding of microplasticity discussed above is also employed and again, as in single crystal plasticity, the active slip systems can be identiﬁed and the corresponding slips determined to give the overall deformation within a given grain. This is now done for all the grains in the polycrystal, which all have their own measured or speciﬁed crystallographic orientations, subject to the requirements of equilibrium and compatibility which are imposed within the ﬁnite element method. In order to do this, it is necessary to generate many ﬁnite elements within each grain. It is clear that for large numbers of grains, such polycrystal plasticity modelling becomes untenable. The consequence is that while desirable, it is not (for the foreseeable future) going to be feasible to carry out polycrystal plasticity modelling at the engineering component level. Currently, and for many years to come, the plastic deformation occurring in both the processing to produce engineering components, and occurring under in-service conditions at localized regions of a component, will continue to be modelled using continuum-level plasticity. This is particularly so in engineering industry where pressures of time and cost demand rapid analyses. We will now, therefore, leave microplasticity and address, in the remainder of the book, continuum-level plasticity.

Further reading Dieter, G.E. (1988). Mechanical Metallurgy. McGraw-Hill Book Co., London. Meyers, M.A., Armstrong, R.W., and Kirchner, H.O.K. (1999). Mechanics and Materials. Fundamentals and Linkages. John Wiley & Sons Inc., New York.

2. Continuum plasticity

2.1

Introduction

This chapter introduces the fundamentals of time-independent and rate-dependent continuum, or phenomenological plasticity: multiaxial yield, normality hypothesis, consistency condition, isotropic and kinematic hardening, and simple constitutive equations for viscoplasticity and creep. We assume throughout the chapter that we are dealing with small strain problems in the absence of large rigid body rotations. The kinematics of large deformations are left until the following chapter.

2.2 2.2.1

Some preliminaries Strain decomposition

Figure 2.1 shows the idealized stress–strain behaviour which might be obtained from a purely uniaxial tensile test. Plasticity commences at a uniaxial stress of σy , after which the material strain hardens. It is called hardening because the stress is increasing relative to perfect plastic behaviour, also shown in the ﬁgure. If, at a strain of ε, the loading were to be reversed, the material would cease to deform plastically (at least in the absence of time-dependent effects) and would show a linearly decreasing stress with strain such that the gradient of this part of the stress–strain curve would Linear strain hardening

s

sy s

E E

«p

Perfect plasticity

«e

«

Fig. 2.1 The classical decomposition of strain into elastic and plastic parts.

12

Continuum plasticity

again be the Young’s modulus, E, shown in Fig. 2.1. Once a stress of zero is achieved (provided the material remains elastic on full reversal of the load), the strain remaining in the test specimen is the plastic strain, εp . The recovered strain, εe , is the elastic strain and it can be seen that the total strain, ε, is the sum of the two ε = εe + εp .

(2.1)

This is called the classical additive decomposition of strain. It is also apparent from Fig. 2.1 that the stress achieved at a strain of ε is given by σ = Eε e = E(ε − εp ).

(2.2)

In many practical situations, particularly in materials processing operations such as forging or superplastic forming, for example, the strains achieved can be very large indeed, and of order 1–4. Compare the magnitude of this strain with that of typical elastic strains of order 0.001 (the 0.1% proof strain) which are generated in metals, even in forming processes (you can estimate this from the measured forces to give a stress, and the elastic strains are of order σ/E). In such circumstances, it is entirely reasonable to make the assumption that ε e ≈ 0 so that εp ≈ ε. 2.2.2

Incompressibility condition

We saw in Chapter 1 that plastic deformation satisﬁes the incompressibility condition; that is, the deformation takes place without volume change. The consequence of this is that the sum of the plastic strain rate components is zero: p

p

p

ε˙ X + ε˙ Y + ε˙ Z = 0.

(2.3)

This is easily veriﬁed by considering a cube of material, with dimensions shown in Fig. 2.2, which undergoes purely plastic, uniform deformation (or simply argue that the strains are very large so that the elastic components are negligibly small). Constancy of volume requires xyz = x0 y0 z0 . Differentiating both sides with respect to time, and dividing by xyz gives y˙ z˙ x˙ + + = 0. (2.4) x y z The strains are deﬁned by x εX = ln x0 and similarly for εY and εZ , and the strain rate in the Y -direction is therefore 1 ˙ ε˙ Y = y. y Equation (2.4) is therefore the incompressibility condition given in Equation (2.3).

Some preliminaries

y

13

y0 z0

Y Z

z

x x0 X

Fig. 2.2 An element of material undergoing plastic, incompressible, elongation in the Y -direction.

2.2.3

Effective stress and plastic strain rate

Identifying the yield condition for uniaxial, monotonically increasing load is straightforward: If σ < σy then the material is elastic, If σ ≥ σy then the material has yielded. It is not quite so straightforward for a multiaxial stress state; that is, one in which more than one direct stress exists. A whole range of multiaxial yield criteria exist. The most commonly used in engineering practice, particularly for computational analysis, is that of von Mises (to which we will return later), which relies on the knowledge of an effective stress, sometimes called (von Mises) equivalent stress. In terms of principal stresses, the effective stress is deﬁned as 1 σe = √ [(σ1 − σ2 )2 + (σ2 − σ3 )2 + (σ3 − σ1 )2 ]1/2 , (2.5) 2 or in terms of direct and shear stresses, 1/2 3 2 2 2 2 2 2 (σ + σ22 + σ33 + 2σ12 + 2σ23 + 2σ31 ) , (2.6) σe = 2 11 where we use the numerical subscripts 1, 2, and 3 in an equivalent way to X, Y , and Z to indicate direction. σe is, of course, a scalar quantity and its origin lies in the postulate that yielding occurs when a critical elastic shear energy is achieved. Mohr’s circle tells us that in a given plane, the maximum shear stress is τ = (σ1 − σ2 )/2 so that with γ = τ/G, the elastic shear energy per unit volume is τ γ /2 = τ 2 /2G = (σ1 − σ2 )2 /8G. The origin of the terms in Equation (2.5) then becomes apparent. An effective plastic strain rate, p, ˙ is deﬁned, similarly, as √ 2 p p p p p p p˙ = (2.7) [(˙ε1 − ε˙ 2 )2 + (˙ε2 − ε˙ 3 )2 + (˙ε3 − ε˙ 1 )2 ]1/2 . 3

14

Continuum plasticity

Writing the stress and plastic strain rate tensors (dropping the plastic strain rate components) as ⎛ ⎞ ⎛ σ11 σ12 σ13 ε˙ 11 ε˙ 12 σ = ⎝σ21 σ22 σ23 ⎠ and ε˙ = ⎝ε˙ 21 ε˙ 22 ε˙ 31 ε˙ 32 σ31 σ32 σ33 then the effective stress and plastic strain rate may be written as 1/2 3

σe = σ :σ 2 1/2 2 p p 1/2 2 ε˙ : ε˙ ε˙ : ε˙ p˙ = ≈ 3 3

superscript p on the ⎞ ε˙ 13 ε˙ 23 ⎠ ε˙ 33

(2.8)

(2.9)

in which σ is the deviatoric stress given by σ = σ −

1 Tr(σ )I , 3

(2.10)

for example 1

σ11 = σ11 − (σ11 + σ22 + σ33 ) 3 1 2 = σ11 − (σ22 + σ33 ) 3 3 and

= σ12 − 0 ≡ σ12 . σ12

The deviatoric stress can be seen to be the difference between the stress and the mean stress, σm = 13 (σ11 + σ22 + σ33 ); the latter is often called the hydrostatic stress. The symbol ‘:’ in Equations (2.9) is called the double contracted product, or double dot product, of two second-order tensors, which will be deﬁned a little later in the chapter. The equations in (2.9) for the effective stress and plastic strain rates are a useful and compact way of writing the equations given in (2.5) and (2.7), respectively. The coefﬁcients in Equations (2.5) and (2.7) (and equivalently in Equations (2.9)) are chosen to ensure that under purely uniaxial loading, the effective stress σe is identical to the uniaxial stress and the effective plastic strain rate, p, ˙ is identical to the uniaxial plastic strain rate. Let us look at this in detail for the case in which a test specimen is loaded uniaxially upto large plastic strain (so that ε e ε p , and ε ≈ ε p ) under an applied stress σ11 , shown schematically in Fig. 2.3. We will now use Equation (2.9) to determine the effective stress and plastic strain rate.

Some preliminaries

15

s

1 2 s 3

Fig. 2.3 Uniaxial loading of a schematic test piece.

In these circumstances, σ11 = σ, σ22 = σ33 = 0, and all the shear components are zero. The incompressibility condition leads to the requirement that ε˙ 11 + ε˙ 22 + ε˙ 33 = 0.

(2.11)

Because of symmetry, ε˙ 22 = ε˙ 33 so that incompressibility gives ε˙ 22 = ε˙ 33 = − 21 ε˙ 11 = − 21 ε˙ . The deviatoric stress components can be determined using Equation (2.10) as 1

σ11 = σ11 − (σ11 + σ22 + σ33 ) 3 2 = σ11 3 1

σ22 = σ22 − (σ11 + σ22 + σ33 ) 3 1 = − σ11 . 3 Similarly, 1

σ33 = − σ11 3 and

σ12 = σ23 = σ33 =0

so that the deviatoric stress tensor becomes, for uniaxial loading, ⎞ ⎛2 0 0 3 σ11 σ = ⎝ 0 0 ⎠. − 13 σ11 1 0 0 − 3 σ11

(2.12)

We can now use Equation (2.9) to determine the effective stress for this trivial case, but we ﬁrst need to ﬁnd the contracted tensor product, σ : σ . This is deﬁned, for two

16

Continuum plasticity

second-order tensors, A and B, by A:B=

n n

Aij Bij .

(2.13)

i=1 j =1

That is, multiply component by component and sum the terms to give a scalar quantity. σ : σ is therefore given by 4 2 1 2 1 2 6 2 2 + σ11 + σ11 = σ11 ≡ σ2 σ : σ = σ11 9 9 9 9 3 and so

σe =

3

σ : σ

2

1/2

=

32 2 σ 23

1/2 ≡ σ.

For a uniaxial stress state, therefore, σe ≡ σ . Let us follow the same procedure for the effective plastic strain rate. With the incompressibility condition and symmetry conditions discussed above the plastic strain rate tensor becomes ⎛ ⎞ ⎛ ⎞ ε˙ 11 ε˙ 0 0 0 0 ε˙ = ⎝ 0 − 21 ε˙ 11 0 ⎠ = ⎝0 − 21 ε˙ 0 ⎠ 1 0 0 − 2 ε˙ 11 0 0 − 21 ε˙ so that 1/2 2 2 1 2 1 2 1/2 2 ε˙ : ε˙ ε˙ + ε˙ + ε˙ = p˙ = 3 3 4 4 1/2 23 2 ε˙ = = ε˙ . 32

For uniaxial loading, therefore, p˙ = ε˙ . Note that the plastic strain rates appearing in Equation (2.9) are not given as deviatoric quantities, that is, ε . This is because the plastic strain rate components are, in themselves, deviatoric due to the incom of plastic pressibility condition. For example, consider the deviatoric component ε˙ 11 strain rate. 1

ε˙ 11 = ε˙ 11 − (˙ε11 + ε˙ 22 + ε˙ 33 ). 3 Because of the incompressibility condition, therefore,

ε˙ 11 ≡ ε˙ 11 .

Yield criterion

2.3

17

Yield criterion

Only the von Mises yield criterion is considered here. There are many others including that of Tresca and the Gurson model for porous materials. In Chapter 1, we saw that there were several general requirements for yield in isotropic, non-porous materials. Let f be a yield function such that f = 0 is our yield criterion. Then: 1. Yield is independent of the hydrostatic stress. Since f is independent of σm , it must be expressible in terms of the deviatoric stresses σi (i = 1, . . . , 3) alone. 2. Yield in polycrystalline metals can be taken to be isotropic (provided we are concerned with yield in a volume of material containing many grains) and must therefore be independent of the labelling of the axes. Thus f must be a symmetric function of σi (i = 1, . . . , 3). 3. Yield stresses measured in compression have the same magnitude as yield stresses measured in tension. Thus f must be an even function of σi (i = 1, . . . , 3). The von Mises yield function is deﬁned by f = σe − σy =

3

σ : σ

2

1/2 − σy

(2.14)

and, with reference to Equation (2.5), it can be seen that it satisﬁes the three requirements given above. The yield criterion is given by f < 0: Elastic deformation f = 0: Plastic deformation.

(2.15)

The second stress invariant, J2 , is deﬁned as J2 = ( 21 σ : σ )1/2 and it is for this reason that plastic ﬂow based on the von Mises yield criterion is often referred to as J2 plasticity. Geometrically, Equation (2.14) corresponds to a cylinder in threedimensional principal stress space with axis lying along the line σ1 = σ2 = σ3 . It is apparent from this that hydrostatic stress has no effect on yield according to the von Mises criterion. Even inﬁnite, but equal, principal stresses σ1 , σ2 , and σ3 will never cause yield, since σe remains zero (see Equation (2.5)) and f < 0. Let us consider the yield function in two-dimensional principal stress space by putting σ3 = 0 and so imposing conditions of plane stress. Geometrically, this corresponds to ﬁnding the intersection between the von Mises cylinder and the plane σ3 = 0.

18

Continuum plasticity

d«p2 Load point

d«p

s2 sy

d«p1 Tangent to yield surface

Yield surface ( f = 0)

sy

sy

sy

s1

Elastic region

Fig. 2.4 The von Mises yield surface for conditions of plane stress, showing the increment in plastic strain, dε p , in a direction normal to the tangent to the surface.

From Equations (2.14) and (2.5), 1/2 3 f = σe − σy = σ :σ − σy 2 1 = √ [(σ1 − σ2 )2 + (σ2 − σ3 )2 + (σ3 − σ1 )2 ]1/2 − σy , 2 which for plane stress, at yield, becomes 1 f = √ [(σ1 − σ2 )2 + σ22 + σ12 ]1/2 − σy = 0 2

(2.16)

so σ12 − σ1 σ2 + σ22 = σy2 , which is the equation of an ellipse. The yield criterion is shown, for plane stress, in Fig. 2.4. Naturally, when σ1 = 0, σ2 = σy at yield and similarly for the other points where the ellipse intersects the lines σ1 = 0 and σ2 = 0. 2.3.1

The normality hypothesis of plasticity

We have now looked at the conditions necessary to initiate yielding. The question then is what happens after that if loading continues? After yield comes plastic ﬂow and the normality hypothesis of plasticity enables us to determine the ‘direction’ of ﬂow. For what is termed associated ﬂow, the hypothesis states that the increment in the plastic strain tensor is in a direction (i.e. relative to the principal stress directions) which is normal to the tangent to the yield surface at the load point. This is shown schematically in Fig. 2.4, but may be written in terms of the yield function, f , as dεp = dλ

∂f ∂σ

or

ε˙ p = λ˙

∂f . ∂σ

(2.17)

Yield criterion

19

In these expressions, the direction of the plastic strain increment (or equivalently, plastic strain rate) is given by ∂f /∂σ while the magnitude is determined, for the plastic strain rate, by λ˙ . This is called the plastic multiplier which we shall return to later. In order to look at this in more detail, and to make understanding easier, let us write the plastic strain rate and stress tensors in vector form (using what is known as Voigt notation, which we shall address in greater depth in Chapter 4). We will continue to consider principal components only, for the time being. Then for plane stress, σ σ= 1 . σ2 Note that the vector representation of the stress, σ, is not italicized. This is the convention to be adopted throughout the book for stress and strain: an italicized bold σ and ε indicates a tensor, a non-italicized bold symbol a vector, or Voigt notation. The yield function f , written in terms of principal stresses is, from Equation (2.16) 1 f = √ [(σ1 − σ2 )2 + σ22 + σ12 ]1/2 − σy = 0, 2 and we can then determine the direction of plastic ﬂow from Equation (2.17) as ⎞ ⎛ ∂f

1 2 (σ1 − σ1 σ2 + σ22 )−1/2 (2σ1 − σ2 ) ⎜ ∂σ1 ⎟ ∂f 2 ⎟ , = grad(f ) = ⎜ ⎝ ∂f ⎠ = 1 2 2 −1/2 (2σ − σ ) ∂σ 2 1 2 (σ1 − σ1 σ2 + σ2 ) ∂σ2 − σ 2σ 1 2 which has direction −σ + 2σ . This is normal to the yield surface at all points 1

2

(e.g. choose σ1 = σ2 = α, say, and the direction of the normal is clearly along the line σ1 = σ2 ). Let us now derive the plastic strain increment using the normality hypothesis with the von Mises yield criterion given in Equation (2.14), but using the other expression for effective stress for three-dimensions given in Equation (2.5). We p will look at just one component, namely dε1 , to see the general pattern emerge. From Equation (2.17), the ﬁrst component of direction of plastic ﬂow is given by ∂f 1 1 = √ [(σ1 − σ2 )2 + (σ2 − σ3 )2 + (σ3 − σ1 )2 ]−1/2 [2(σ1 − σ2 ) − 2(σ3 − σ1 )] ∂σ1 2 2 (3/2)[σ1 − (1/3)(σ1 + σ2 + σ3 )] = σe so ∂f 3 σ1

= ∂σ1 2 σe

20

Continuum plasticity

remembering the deﬁnition of deviatoric stress given in Equation (2.10). Similar results are obtained for the other components so that Equation (2.17) may be rewritten, for the von Mises yield criterion, as dεp = dλ

3 σ

∂f = dλ ∂σ 2 σe

(2.18)

in which the stress and strain are now written as tensor quantities. Let us now look at the meaning of the plastic multiplier (at least, that is, for a von Mises material). We can use the expression for effective plastic strain rate in Equation (2.9) to write a similar expression for the increment in effective plastic strain as 1/2 2 p p dp = dε : dε . (2.19) 3 If we substitute Equation (2.18) into (2.19) we obtain 2 3 σ 3 σ 1/2 ((3/2)σ : σ )1/2 dp = dλ : dλ = dλ 3 2 σe 2 σe σe so that with Equation (2.9) we obtain

and similarly,

dp = dλ

(2.20)

p˙ = λ˙ .

(2.21)

So, for a von Mises material, the plastic multiplier, dλ, turns out simply to be the increment in effective plastic strain. We can then rewrite the ﬂow rule in Equation (2.18) as σ

3 dε p = dp . (2.22) 2 σe In order for Equation (2.22) to be useful to us, we need to be able to calculate the increment in effective plastic strain, dp, or equivalently, the plastic multiplier, so that with prescribed loading, we can then calculate the increment in plastic strain components. We will address this next. 2.3.2

Consistency condition

Let us consider the case of uniaxial, tensile loading, for which the stress path taken relative to the yield surface is shown in Fig. 2.5. Starting from zero stress, σ2 then increases while the material deforms elastically until the load point (i.e. the point in stress space corresponding to the current loading) meets the yield surface at σ2 = σy . At this point, the material behaves plastically,

Yield criterion

Load point

21

s2 s2 sy

sy

sy

sy

«2

s1

sy Yield surface ( f = 0)

Fig. 2.5 The von Mises yield surface for plane stress and the corresponding stress–strain curve obtained for uniaxial straining in the 2-direction.

with no hardening, as shown in the resulting stress–strain curve in Fig. 2.5. With further plastic deformation, the load point remains on the yield surface and the stress remains constant and equal to σ y . The requirement for the load point to remain on the yield surface during plastic deformation (at least, that is, for time-independent plasticity—we will look at viscoplasticity later) is called the consistency condition, and it is this that enables us to determine the plastic multiplier, or equivalently for a von Mises material, the increment in effective plastic strain. The yield function given in Equation (2.14) includes a dependence on the stress components and the yield stress, σy . We will see later, when considering hardening, that the yield stress can increase (and sometimes decrease), and does so often as a function of effective plastic strain, p. It is therefore convenient to write the yield function as f (σ, p) = σe − σy = σe (σ ) − σy (p) = 0. (2.23) The consistency condition is written, for an incremental change in stress and effective plastic strain f (σ + dσ, p + dp) = 0. (2.24) We can expand this as f (σ + dσ, p + dp) = f (σ, p) +

∂f ∂f : dσ + dp. ∂σ ∂p

(2.25)

Note that all terms in the equation are scalar. Let us work in principal stress space only. The advantage of this is simplicity; the disadvantage is that we ignore the complicating features of dealing with tensor versus engineering strain components. However, this will be dealt with in Chapters 4–6. We will therefore store stress and strain principal components as vectors, in Voigt notation, as discussed above. The product

22

Continuum plasticity

∂f /∂σ : dσ then becomes the scalar (dot) product, (∂f/∂σ)·dσ of two vectors (this is only true in principal stress space, as we shall see later) which gives a scalar. Combining Equations (2.23)–(2.25) gives ∂f ∂f dp = 0. · dσ + ∂p ∂σ

(2.26)

We can use Hooke’s law in incremental form to relate the stress and elastic strains, written as column vectors, by dσ = C dεe = C(dε − dεp )

(2.27)

in which C is the elastic stiffness matrix. We will use the most general form for the plastic strain increment, given in Equation (2.17), for now, but simplify for the case of the von Mises yield criterion later. Substituting (2.17) into (2.27) gives ∂f dσ = C dε − dλ (2.28) ∂σ and (2.28) into (2.26)

∂f ∂f ∂f + dp = 0. · C dε − dλ ∂σ ∂p ∂σ

(2.29)

We can obtain the most general form for dp, that is, without assuming a von Mises material for the time being, by using Equations (2.17) and (2.19) to give 1/2 2 p 2 2 ∂f ∂f ∂f 1/2 ∂f 1/2 p dp = = = dε : dε dλ : dλ dλ · dλ 3 3 ∂σ ∂σ 3 ∂σ ∂σ (2.30) for principal stress space, in which the contracted tensor product simpliﬁes to the scalar product. Substituting (2.30) into (2.29) and rearranging gives the plastic multiplier dλ dλ =

(∂f /∂σ) · C dε (∂f /∂σ) · C(∂f /∂σ) − (∂f /∂p)((2/3)(∂f /∂σ) · (∂f /∂σ))1/2

.

(2.31)

The stress increment can then be determined by substituting (2.31) into (2.28) to give ∂f (∂f /∂σ) · C dε dσ = C dε − ∂σ (∂f/∂σ) · C(∂f/∂σ) − (∂f/∂p)((2/3)(∂f/∂σ) · (∂f/∂σ))1/2 (∂f/∂σ) · C ∂f dε = C−C ∂σ (∂f/∂σ) · C(∂f/∂σ) − (∂f/∂p)((2/3)(∂f/∂σ) · (∂f/∂σ))1/2 (2.32)

Isotropic hardening

23

or dσ = C ep dε.

(2.33)

C ep is called the tangential stiffness matrix. In the absence of plastic deformation, dλ = 0, and in this case, C ep ≡ C, the elastic stiffness matrix. In the case of plastic deformation, with knowledge of the total strain increment, the stress increment can be obtained from Equation (2.32). Before looking at the plastic multiplier in more detail, to gain better physical insight, we will ﬁrst introduce isotropic hardening.

2.4

Isotropic hardening

Many metals, when deformed plastically, harden; that is, the stress required to cause further plastic deformation increases, often as a function of accumulated plastic strain, p, which can be written as p = dp = p˙ dt, (2.34) where p˙ and dp are given in (2.9) and (2.19), respectively. A uniaxial stress–strain curve with non-linear hardening is shown in Fig. 2.6 together with schematic representations of the initial and subsequent yield surfaces. In this instance, the subsequent yield surface is shown expanded compared with the original. When the expansion is uniform in all directions in stress space, the hardening is referred to as isotropic. Let us just consider what happens in going from elastic behaviour to plastic, hardening behaviour in Fig. 2.6. Loading is in the 2-direction, so the load point moves in the σ2 direction from zero until it meets the initial yield surface at σ2 = σy . Yield occurs at this point. In order s2

s2

sy

sy

sy

sy sy

Saturation Hardening «2

s1 sy

Initial yield surface

r

Yield Subsequent, expanded yield surfaces after plastic deformation

Fig. 2.6 Isotropic hardening, in which the yield surface expands with plastic deformation, and the corresponding uniaxial stress–strain curve.

24

Continuum plasticity

for hardening to take place, and for the load point to stay on the yield surface (the consistency condition requires this), the yield surface must expand as σ2 increases, shown in Fig. 2.6. The amount of expansion is often taken to be a function of accumulated plastic strain, p, and for this case, the yield function becomes that given in (2.23), f (σ, p) = σe − σy (p) = 0,

(2.35)

where σy (p) might be of the form σy (p) = σy0 + r(p)

(2.36)

in which σy0 is the initial yield stress and r(p) is called the isotropic hardening function. There are many forms used for r(p) but a common one is r˙ (p) = b(Q − r)p˙

or

dr(p) = b(Q − r) dp

(2.37)

in which b and Q are material constants, which gives an exponential shape to the uniaxial stress–strain curve which saturates with increasing plastic strain, since integrating (2.37) with initial condition r(0) = 0, gives r(p) = Q(1 − e−bp ).

(2.38)

Q is the saturated value of r so that the peak stress achieved with this kind of hardening, from Equation (2.36), is therefore (σy0 +Q). The constant b determines the rate at which saturation is achieved. Figure 2.6 shows an example of the uniaxial stress–strain behaviour predicted using this kind of isotropic hardening function. Let us now consider a slightly simpler form of isotropic hardening and determine the plastic multiplier in Equation (2.31) and hence the stress increments in (2.32). 2.4.1

Linear isotropic hardening

We write the linear isotropic hardening function as dr(p) = h dp

(2.39)

in which h is a constant. With this hardening, we expect the uniaxial stress–strain curve to look like that shown in Fig. 2.7. For uniaxial conditions, dp = dεp , and referring to Figs 2.6 and 2.7, the stress increase due to isotropic hardening is just dr, so using Equation (2.39) we may write dσ h and, of course, the increment in elastic strain is just dεp =

dεe =

dσ E

Isotropic hardening

Gradient = E s

(

1–

E E+h

25

)

r sy «p

sy «

Fig. 2.7 Stress–strain curve for linear strain hardening with dr = h dεp .

so that the total strain is dσ dσ + = dσ dε = E h giving

E+h , Eh

E dσ = E 1 − E+h

dε.

The plastic multiplier has been derived, in Equation (2.31), in terms of the total strain increment. This is the most appropriate form when considering the development of computational techniques, including the ﬁnite element method in which, often, the total strain increments are provided, step by step, and it is then necessary to calculate the corresponding stress increments. However, in order to obtain better physical insight into the process, it is more appropriate (and simpler) to write the plastic multiplier in terms of a known stress increment. In this section, we will obtain the plastic multiplier in terms of the stress increment so that we can then examine the equations for a simple uniaxial problem using the von Mises yield criterion in Section 2.4.2. Now, returning to the plastic multiplier and combining Equations (2.26) and (2.30), we obtain ∂f ∂f ∂f 2 ∂f ∂f ∂f dp = · dσ + dλ · = 0. (2.40) · dσ + ∂p ∂σ ∂p 3 ∂σ ∂σ ∂σ Rearranging (2.40) gives the plastic multiplier, but now in terms of the stress increment, dσ , as −(∂f/∂σ) · dσ . (2.41) dλ = (∂f/∂p)((2/3)(∂f/∂σ) · (∂f/∂σ)) 2.4.2

Uniaxial loading with linear isotropic hardening

Let us consider purely uniaxial loading, in the 1-direction, for a material that yields according to the von Mises criterion. In other words, we will apply a stress σ1 in the

26

Continuum plasticity

1-direction, and all other stresses are zero. For simplicity, we will continue to work in principal stress space and represent the stresses in Voigt notation; that is, the stress is written in vector form as ⎡ ⎤ σ1 σ = ⎣σ2 ⎦ . σ3 We will now determine the plastic multiplier using Equation (2.41). We will consider the denominator ﬁrst. With the hardening function given in (2.39), the yield function becomes f (σ, p) = σe (σ ) − σy (p) = σe (σ ) − σy0 − r(p) = 0 (2.42) from which we can obtain

∂r ∂f =− = −h. (2.43) ∂p ∂p For the von Mises yield criterion, ∂f/∂σ can be obtained using Equation (2.18), with the deviatoric stress components taken from (2.12), as ⎡ 2 ⎤ ⎡ ⎤ σ1 1 ∂f 3 σ

3 1 ⎢ 31 ⎥ ⎢ 1 ⎥ − = = ⎣− 3 σ1 ⎦ = ⎣ 2 ⎦ ∂σ 2 σe 2 σ1 − 21 − 1 σ1 3

so that ∂f ∂p

2 ∂f ∂f · 3 ∂σ ∂σ

⎤ ⎡ ⎤⎞1/2 1 1 ⎜ 2 ⎢− 1 ⎥ ⎢− 1 ⎥⎟ = −h ⎝ ⎣ 2 ⎦ · ⎣ 2 ⎦⎠ = −h. 3 − 21 − 21 ⎛ ⎡

The numerator can be determined as follows: ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ 1 1 dσ1 dσ1 ∂f ⎢− 1 ⎥ ⎣ ⎦ ⎢− 1 ⎥ ⎣ ⎦ = dσ1 · dσ = − ⎣ 2 ⎦ · dσ2 = − ⎣ 2 ⎦ · 0 − ∂σ 1 1 0 dσ 3 −2 −2

(2.44)

(2.45)

and substituting (2.44) and (2.45) into (2.41) gives the plastic multiplier as dλ =

dσ1 . h

(2.46)

For a von Mises material, under uniaxial loading, therefore, p

dλ = dp = dε1 =

dσ1 . h

(2.47)

This is telling us that the increment in stress for unit increase in plastic strain is h. This arises because we chose linear hardening with gradient h. We know, of course,

Kinematic hardening

27

that because we are considering uniaxial loading and the incompressibility condition applies, the other plastic strain increments must be 1 p 1 dσ1 p p dε2 = dε3 = − dε1 = − . (2.48) 2 2 h We can, of course, obtain the other plastic strain components formally from Equation (2.17) as ⎡ ⎤ 1 dσ1 ⎢ 1 ⎥ ∂f p dε = dλ (2.49) = ⎣− 2 ⎦ ∂σ h 1 −2 in agreement with (2.48). The total strain increment in the loading direction is given by dσ1 dσ1 + . (2.50) E h Rearranging (2.50), and omitting the subscript 1 to indicate the uniaxial loading direction, gives E dσ = E 1 − dε, (2.51) E+h which is what we obtained earlier for linear strain hardening shown in Fig. 2.7. Equation (2.51) shows the linear hardening obtained, under uniaxial loading, for the isotropic hardening model chosen in Equation (2.39). If we choose perfect plasticity, that is, with no hardening (h = 0), Equation (2.51) gives a stress increment of zero. The plastic multiplier can, using (2.51) and (2.46), be rewritten as p

dε1 = dε1e + dε1 =

dλ =

2.5

E dε1 . E+h

(2.52)

Kinematic hardening

In the case of monotonically increasing loading, it is often reasonable to assume that any hardening that occurs is isotropic. For the case of reversed loading, however, this is often not appropriate. Consider a material which hardens isotropically, shown schematically in Fig. 2.8. At a strain of εi , corresponding to load point (1) shown in the ﬁgure, the load is reversed so that the material behaves elastically (the stress is now lower than the yield stress) and linear stress–strain behaviour results up until load point (2). At this point, the load point is again on the expanded yield surface, and any further increase in load results in plastic deformation. Figure 2.8(b) shows that isotropic hardening leads to a very large elastic region, on reversed loading, which is often not what would be seen in experiments. In fact, a much smaller elastic region

28

Continuum plasticity (a)

(b) s2

Load point (1)

s2

sy

sy E

sy

sy

«i

s1

«2

E sy

Initial yield surface

Subsequent, expanded yield surface

Load point (2)

Fig. 2.8 Reversed loading with isotropic hardening showing (a) the yield surface and (b) the resulting stress–strain curve. (b)

(a) Load point (1)

s2

s2

sy

sy

E E

|x| sy

sy

s1

«2

sy Initial yield surface

Subsequent, translated yield surface

Load point (2)

Fig. 2.9 Kinematic hardening showing (a) the translation, |x| of the yield surface with plastic strain, and (b) the resulting stress–strain curve with shifted yield stress in compression—the Bauschinger effect.

is expected and this results from what is often called the Bauschinger effect, and kinematic hardening. In kinematic hardening, the yield surface translates in stress space, rather than expanding. This is shown in Fig. 2.9. In Fig. 2.9(a), the stress increases until the yield stress, σy , is achieved. With continued loading, the material deforms plastically and the yield surface translates. When load point (1) is achieved, the load is reversed so that the material deforms elastically until point (2) is achieved when the load point is again in contact with the yield surface. The elastic region is much smaller than that for isotropic hardening shown in Fig. 2.8(b). In fact, for the kinematic hardening in Fig. 2.9, the elastic region

Kinematic hardening

29

is of size 2σy whereas for the isotropic hardening, it is 2(σy + r). In the case of plastic ﬂow with kinematic hardening, note that the consistency condition still holds; the load point must always lie on the yield surface during plastic ﬂow. In addition, normality still holds; the increment in plastic strain has direction normal to the tangent to the yield surface at the load point. The yield function describing the yield surface must now also depend on the location of the surface in stress space. Consider the initial yield surface shown in Fig. 2.9. Under applied loading and plastic deformation, the surface translates to the new location shown such that the initial centre point has been translated by |x|. We now need to determine the stresses relative to the new yield surface centre to check for yield. In the absence of kinematic hardening, the yield function written in terms of tensor stresses is 1/2 3

f = σe − σy = − σy . σ :σ 2 With kinematic hardening, however, it is 1/2 3

f = (σ − x ) : (σ − x ) − σy (2.53) 2 in which x is the kinematic hardening variable and is often called a back stress. Because it is a variable deﬁned in stress space, it has the same components as stress, and we can write it as a tensor, or, using Voigt notation, as a vector. In order to understand Equation (2.53), let us consider purely uniaxial loading with linear kinematic hardening. 2.5.1

Kinematic hardening under uniaxial loading

We will take the increment in kinematic hardening to be proportional to the increment in plastic strain, hence 2 2 dx = c dεp or equivalently, x˙ = cε˙ p (2.54) 3 3 in which c is a material constant, and the coefﬁcient of 23 will be discussed below. This is called Prager linear hardening. Equation (2.54) has the similarity with isotropic hardening, that the hardening variable depends linearly on the plastic strain. The major difference is that isotropic hardening is described by a scalar variable, r, whereas for kinematic hardening, the hardening variable (or back stress) is a tensor, just as for stress. Because of the incompressibility condition, we know that the plastic strain increment is a deviatoric quantity, that is 1 dε p = dεp − Tr(dεp ) ≡ dεp . (2.55) 3

30

Continuum plasticity

From Equation (2.54), dx is therefore also a deviatoric quantity so that for uniaxial loading in the 1-direction, we may write ⎞ ⎛ ⎞ ⎛ 0 0 x11 x11 0 0 ⎜ 1 0 ⎟ x = x = ⎝ 0 x22 0 ⎠ = ⎝ 0 − 2 x11 (2.56) ⎠. 1 0 0 x33 0 0 − 2 x11 The magnitude or norm of x is deﬁned by x = |x| = (x : x)1/2 ⎡⎛ 0 x11 ⎢⎜ 0 − 1 x = ⎣⎝ 2 11 0 0 1 2 2 = x11 + x11 + 4

(2.57) ⎞ ⎛

0 x11 ⎟ ⎜ 0 −1x ⎠:⎝ 2 11 − 21 x11 0 0 1/2 3 1 2 x = x11 4 11 2 0 0

0 0

⎞⎤1/2 ⎟⎥ ⎠⎦

− 21 x11 (2.58)

so the uniaxial component of x, that is x11 , is 23 times the magnitude of x. Bear in mind that under uniaxial loading, the effective stress is identical to the uniaxial applied stress, and the effective plastic strain increment is identical to the uniaxial plastic strain increment. Note also that like the plastic strain, uniaxial loading leads to the development of not only the uniaxial component of x, but also the other direct components as well. This is because x depends directly on the plastic strain, given in its evolution equation in (2.54). Consider now the components of dx, for uniaxial loading, in Equation (2.54). ⎛ ⎛ p ⎞ ⎞ 0 0 dε11 dx11 0 0 2 ⎜ ⎜ p − 21 dε11 0 ⎟ 0 ⎟ − 21 dx11 dx = ⎝ 0 ⎠ = c⎝ 0 ⎠ 3 1 1 p 0 0 − 2 dx11 0 0 − 2 dε11 so that 2 2 p c dε11 ≡ c dp. (2.59) 3 3 It is often simpler, and in particular, for uniaxial loading, to write the equations in terms of the magnitude of x rather than the loading direction component. Combining Equations (2.59) and (2.58), therefore, gives dx11 =

p

dx = c dε11 ≡ c dp, which is why the coefﬁcient of

2 3

appears in Equation (2.55).

(2.60)

Kinematic hardening

31

We may now determine the terms necessary for the yield function in Equation (2.53) for uniaxial loading as ⎛2 ⎞ 0 0 3 σ11 − x11 ⎜ ⎟ σ − x = ⎝ (2.61) 0 − 21 23 σ11 − x11 0 ⎠ 1 2 0 0 − 2 3 σ11 − x11 which can be written in terms of the magnitude, x, of the back stress as ⎞ ⎛ 0 0 σ11 − x 2⎜ ⎟ 0 − 21 (σ11 − x) σ − x = ⎝ 0 ⎠ 3 1 0 0 − 2 (σ11 − x) so that

⎛

0 (σ11 − x) 4⎜ 1

0 − 2 (σ11 − x) (σ − x ) : (σ − x ) = ⎝ 9 0 0 ⎛ 0 (σ11 − x) ⎜ 1 0 − 2 (σ11 − x) :⎝ 0

0

0 0

⎟ ⎠

− 21 (σ11 − x) ⎞ 0 ⎟ 0 ⎠ − 21 (σ11 − x)

4 1 1 = (σ11 − x)2 + (σ11 − x)2 + (σ11 − x)2 9 9 9 2 = (σ11 − x)2 3 so that

⎞

1/2 3

f = (σ − x ) : (σ − x ) − σy = |σ11 − x| − σy = 0. (2.62) 2 Because we are considering here only uniaxial loading, σ 11 is just the uniaxial stress, σ , so Equation (2.62) can be written f = |σ − x| − σy = 0.

(2.63)

The physical interpretation of Equation (2.63) can be seen in Fig. 2.9. Plastic deformation leads to the translation of the yield surface in stress space. Under uniaxial conditions, therefore, further yield occurs if |σ − x| is equal to the yield stress, σy . There are many forms of kinematic hardening available. What often distinguishes them is how the direction of translation of the yield surface is chosen, and the rate of its evolution as a function of the plastic strain. We shall now look at what is often called Armstrong–Frederick, or Chaboche non-linear kinematic hardening.

32

Continuum plasticity

2.5.2

Non-linear kinematic hardening

In its multiaxial form, the increment, dx, in the back stress is given by dx =

2 c dεp − γ x dp 3

(2.64)

2 p cε˙ − γ xp˙ 3

(2.65)

or equivalently, x˙ =

in which γ is a further material constant. In its uniaxial form, for monotonically increasing plastic strain, Equation (2.64) may be written in terms of the magnitude, x, as dx = c dεp − γ x dεp , which can be integrated, taking x to be 0 at εp = 0, to give x=

c p (1 − e−γ ε ). γ

(2.66)

The resulting form of the stress–strain curve, for this non-linear kinematic hardening, is shown together with the translated yield surface, in Fig. 2.10. As the plastic strain increases, so the back stress, x, in Equation (2.66) saturates to the value c/γ giving a maximum saturated stress of σy + c/γ . The constant γ is the time constant and determines the rate of saturation of stress. c/γ determines the magnitude. We will now examine the ﬂow rule for kinematic hardening. Saturated stress

s2

s2 x

sy

E sy

c/g

sy

sy

s1

sy «2

sy Initial yield surface

Subsequent, translated yield surface

Fig. 2.10 Non-linear kinematic hardening and the resulting non-linear hardening stress–strain curve which saturates at stress c/γ .

Kinematic hardening

2.5.3

33

Flow rule with kinematic hardening

We will use the normality hypothesis in Equation (2.17) together with the yield function in (2.53) to determine the ﬂow rule for plastic deformation with kinematic hardening. First, let us write the yield function, f , as 1/2 3

f = − σy (σ − x ) : (σ − x ) 2 = J (σ − x ) − σy .

(2.67)

The normality hypothesis then gives dεp = dλ

3 σ − x

∂f . = dλ ∂σ 2 J (σ − x )

(2.68)

We now need to use the consistency condition to determine the plastic multiplier. First, let us use Equation (2.68) just to show that 1/2 2 p [(3/2)(σ − x ) : (σ − x )]1/2 dp = dε : dεp = dλ (2.69) = dλ 3 J (σ − x ) for the case of kinematic hardening with a von Mises yield criterion. The yield function depends upon the stress, σ , and the back stress, x, which are both tensor quantities. However, for simplicity, we shall now work in principal stress space again, and use Voigt notation. The consistency condition becomes ∂f ∂f · dσ + · dx = 0, (2.70) ∂σ ∂x which, when combined with Hooke’s law in (2.27), the normality hypothesis in (2.17), and Equation (2.69) gives ∂f ∂f ∂f 2 p · C dε − dλ + · c dε − γ x dλ ∂σ ∂σ ∂x 3 ∂f ∂f 2 ∂f ∂f · C dε − dλ + · c dλ − γ x dλ = 0 = ∂σ ∂σ ∂x 3 ∂σ so that dλ =

(∂f/∂σ) · C dε (∂f/∂σ) · C(∂f/∂σ) + γ (∂f/∂x) · x − (2/3)c(∂f /∂x) · (∂f /∂σ )

(2.71)

and the plastic strain increment is dεp =

∂f (∂f/∂σ) · C dε (∂f/∂σ) · C(∂f/∂σ) + γ (∂f/∂x) · x − (2/3)c(∂f/∂x) · (∂f/∂σ) ∂σ (2.72)

34

Continuum plasticity

and so the stress increment can be obtained from Equation (2.27). We will simplify this to the case of uniaxial loading to interpret the terms in Section 2.5.4, but ﬁrst, we will start by obtaining the plastic multiplier in terms of stress rather than strain increments. Starting from the consistency condition in (2.70) gives ∂f ∂f ∂f ∂f 2 (2.73) · dσ + · dx = · dσ + · c dεp − γ x dp = 0. ∂σ ∂x ∂σ ∂x 3 From the yield function in (2.67), ∂f/∂x = −(∂f /∂σ ) and dp = dλ and with (2.68), (2.73) becomes ∂f ∂f 2 ∂f · dσ − · c dλ − γ x dλ = 0 ∂σ ∂σ 3 ∂σ so that −(∂f/∂σ) · dσ dλ = . (2.74) γ (∂f/∂σ) · x − (2/3)c(∂f/∂σ) · (∂f/∂σ) We will examine this for uniaxial loading in a von Mises material in the following section. 2.5.4

Simple uniaxial loading

For uniaxial loading, we can determine the terms in the denominator of Equation (2.74) as follows: ⎡

⎡ ⎤ ⎡ ⎤ ⎤ ⎡ ⎤ 1 1 1 x1 ∂f 2 ∂f ∂f ⎢− 1 ⎥ ⎣ ⎦ 2 ⎢− 1 ⎥ ⎢− 1 ⎥ γ · = γ ⎣ 2 ⎦ · x2 − c ⎣ 2 ⎦ · ⎣ 2 ⎦ . ·x− c 3 ∂σ ∂σ 3 ∂σ x3 − 21 − 21 − 21

(2.75)

We know that x is a deviatoric quantity so that for uniaxial loading in the 1-direction, 1 x2 = x3 = − x1 2 so that Equation (2.75) becomes just 23 γ x1 − c. Now, we can write x1 = 23 x so that this becomes γ x − c. The numerator in (2.74) is, as before, just −dσ1 so that the plastic multiplier for uniaxial loading is just dσ1 dλ = . (2.76) c − γx In a similar manner to that for the isotropic hardening example, we can obtain the uniaxial stress increment as E dσ = E 1 − dε. (2.77) E + c − γx

Kinematic hardening

35

Let us look at this in a little more detail. If the material behaviour is purely elastic, then the plastic multiplier is zero and the right-hand term in the bracket is zero so that (2.77) simply reduces to dσ = E dε. If we have elastic, perfectly plastic behaviour, that is, no strain hardening, then c = γ = 0 and then (2.77) tells us that during plastic deformation, the increment in stress is zero. If the material undergoes linear kinematic hardening, that is, γ = 0, the stress–strain relation during plasticity becomes E dσ = E 1 − dε (2.78) E+c which is linear during plastic deformation since c is constant. This equation for linear kinematic hardening and that for linear isotropic hardening in Equation (2.51) can be seen to be near identical. The two types of hardening are in fact the same for monotonically increasing loading (provided c = h) and only differ under uniaxial conditions on a load reversal when the Bauschinger effect becomes important. If, ﬁnally, the material undergoes non-linear kinematic hardening, the back stress, x, increases according to its evolution equation, (2.64), so that the stress increment progressively decreases until saturation is achieved at which point, no further stress increase occurs. This can be seen by substituting the equation for x, given in (2.66), into (2.77) to give E dσ = E 1 − dε E + c − γx E E =E 1− dε = E 1 − dε. p p E + c − γ [(c/γ )(1 − e−γ ε )] E + ce−γ ε As the plastic strain increases, so the exponential term diminishes until ultimately, the material becomes perfectly plastic with dσ = 0. Before ﬁnishing this section, Equation (2.77) demonstrates quite nicely the incremental nature of plasticity. Let us consider ﬁrst the case of elasticity only. Equation (2.77) gives dσ = E dε, e where dε = dε . Integrating this equation is clearly possible such that at any particular value of elastic strain, the stress can be calculated. This is simply not possible for the case of plasticity, for which all we can do (normally) is consider increments in stress resulting from an increment in strain. This follows from Equation (2.77) since x itself depends upon strain, so that the increment in stress varies from step to step. The increment in stress, and indeed plastic strain, often depend then, in plasticity, on the history of prior deformation. Plasticity must, in general, therefore, be considered to be an incremental process.

36

Continuum plasticity Expanded yield surface (isotropic hardening) after many cycles s2

s2 B

sy

sy

A

«2

sy s1

sy

C sy

D

Plasticity recommences

Initial yield surface Translated yield surface (kinematic hardening)

Expanded hysteresis loop resulting from isotropic hardening

Strain

Fig. 2.11 Combined kinematic and isotropic hardening.

Time

Fig. 2.12 Strain imposed resulting in cyclic plasticity shown in Fig. 2.11.

2.6

Combined isotropic and kinematic hardening

We will consider, ﬁnally, materials which harden both kinematically and isotropically. This is particularly appropriate for applications to cyclic plasticity where within an individual cycle, kinematic hardening is the dominant hardening process such that the Bauschinger effect can be represented, but over (normally) quite large numbers of cycles, the material also hardens isotropically such that the peak tension and compression stresses in a given cycle increase from one cycle to the next until saturation is achieved. Such a process is represented schematically in Fig. 2.11. Starting from the point of zero stress and strain, the material is subjected to the strain shown in Fig. 2.12. The stress increases until yield is achieved at point A, and the material kinematically hardens leading to the translation of the yield surface, as shown in Fig. 2.11. Once the peak strain is achieved, the strain reversal occurs so that the material becomes elastic

Combined isotropic and kinematic hardening

37

at point B. Elastic deformation continues until the load point reaches the yield surface again at point C where plasticity recommences until the next strain reversal at point D. The yield surface is translated again because of the kinematic hardening. The stress– strain loop BCDB produced in this way is called a hysteresis loop. If, in addition to the kinematic hardening, the material also isotropically hardens, then superimposed upon the translation of the yield surface is a progressive expansion, shown by the broken line hysteresis loop in Fig. 2.11. This process, by which the peak stress and strain in a hysteresis loop increase, due to isotropic hardening, is often called cyclic hardening, as it often occurs from cycle to cycle over many cycles. Kinematic hardening, on the other hand, occurs within each cycle. We will consider the case of non-linear kinematic and isotropic hardening, given by Equations (2.64) and (2.37), respectively. In order to determine the plastic multiplier, we will use the consistency condition as before. The yield function, for combined kinematic and isotropic hardening, depends on the stress, back stress, and accumulated plastic strain as follows f = J (σ − x ) − r(p) − σy

(2.79)

so that the consistency condition becomes ∂f ∂f ∂f · dx + dp = 0. · dσ + ∂x ∂p ∂σ

(2.80)

Substituting for dσ and dx from Equations (2.27) and (2.64) and writing ∂f /∂p = −(∂r/∂p) from (2.79), together with (2.37) gives ∂f ∂f 2 p p (2.81) · C(dε − dε ) + · c dε − γ x dp − b(Q − r(p)) dp = 0. ∂σ ∂x 3 Following the procedure for isotropic and kinematic hardening, (2.81) can be rearranged to give the plastic multiplier. Assuming von Mises behaviour, dp = dλ, and substituting for dε p from (2.17), gives the plastic multiplier as dλ =

(∂f/∂σ)· C dε . (∂f/∂σ)· C(∂f/∂σ)− γ (∂f/∂σ)· x +(2/3)c(∂f/∂σ)· (∂f/∂σ)+b(Q − r(p)) (2.82)

In a similar manner as before, we can determine the plastic multiplier in terms of the increment of stress, rather than strain, as follows. Equation (2.80) is written as 2 ∂f ∂f · c dεp − γ x dp − b(Q − r(p)) dp = 0 · dσ + ∂x 3 ∂σ

38

Continuum plasticity

so that the plastic multiplier becomes dλ =

(∂f/∂σ) · dσ . (2/3)c(∂f/∂σ) · (∂f/∂σ) − γ (∂f/∂σ) · x + b(Q − r(p))

(2.83)

As in previous examples, we can reduce this to the form for uniaxial loading of a von Mises material and obtain for the uniaxial stress increment E dε. (2.84) dσ = E 1 − E + c − γ x + b(Q − r(p))

2.7

Viscoplasticity and creep

So far, we have considered time-independent plasticity only; that is, the stress–strain behaviour has been assumed to be independent of the rate of loading, whether strain or stress controlled. The plasticity of materials which do exhibit rate effects is called viscoplasticity. We shall see that the same formalism for viscoplasticity is also appropriate for creep—the time dependent, irreversible deformation of a material under load. The usual convention for terminology is that viscoplasticity describes rate-dependent plasticity in which crystallographic slip is the dominant deformation process, though likely enhanced by thermally-activated processes such as diffusion-activated dislocation climb. Creep is normally used to describe low strain rate, time-dependent irreversible deformation which is either diffusion controlled, or inﬂuenced by diffusion, though there may well be crystallographic slip still occurring. In viscoplasticity, the elastic–plastic strain decomposition still holds, and yield is determined as for time-independent plasticity with a yield function. In addition, the plastic ﬂow rule is obtained as before using the normality hypothesis of plasticity, and once yielding has occurred, the material may harden isotropically or kinematically. An important difference occurs, however, in that the consistency condition is no longer formally applied so that the load point may now lie outside of the yield surface. As a result, some viscoplasticity models are referred to as over-stress models. We shall start by addressing uniaxial loading in the 1-direction, as before, for conditions of plane stress. Figure 2.13 shows schematically the material’s stress–strain response and the corresponding yield surface which we assume to expand due to linear isotropic hardening. At load point (1) shown on the yield surface in Fig. 2.13(a) and at the corresponding point on the uniaxial stress–strain curve in Fig. 2.13(b), for the case of time-independent plasticity, the stress achieved is the yield stress, σy , together with the contribution from the linear isotropic hardening, r(p) so that σ = σy + r(p).

Viscoplasticity and creep

39

(b)

(a) Load point (1)

s2

s2

sy

sy

sv r (p)

E sy

sy

s1

sy «2

sy Initial yield surface

Subsequent, expanded yield surface

Fig. 2.13 (a) The von Mises yield surface in plane stress for viscoplasticity with linear isotropic hardening, with viscous (over-stress) stress σv , and (b), the corresponding stress strain curve.

The resulting stress–strain curve is that shown by the broken line in Fig. 2.13(b). However, for the case of viscoplasticity, the stress is augmented by the viscous stress, σ v , also shown schematically in Fig. 2.13(b) by the solid line. There are many types of equations used to represent the viscous stress, but they often contain a dependence on the effective plastic strain rate (which for uniaxial conditions is identical to the uniaxial plastic strain rate), p. ˙ This, of course, is how the strain rate dependence of the plasticity is introduced. Let us consider the commonly used power law function σv = Kp˙ m

(2.85)

in which K and m are material constants. The constant m is called the material’s strain rate sensitivity. From Fig. 2.13(b), the stress–strain curve which includes the rate-dependence of stress is therefore σ = σy + r(p) + σv = σy + r(p) + Kp˙ m .

(2.86)

In viscoplasticity, the uniaxial stress depends on the yield stress, the hardening of the yield stress, and the plastic strain rate. The stress response is, therefore, strain rate dependent. For this reason, viscoplasticity is sometimes referred to as time-dependent plasticity or rate-dependent plasticity. Let us consider the uniaxial behaviour described by Equation (2.86) in a little more detail, but to simplify, let us assume perfect plasticity so that there is no isotropic hardening and r(p) = 0. In this case, the equation becomes σ = σy + Kp˙ m .

(2.87)

40

Continuum plasticity

(b)

(a)

s3 Stress

Strain

«• 3 «2

s2 s1

•

«1

sy

•

Plastic strain, p

Time

Fig. 2.14 (a) Applied strain and (b) the resulting rate-dependent stress response.

If we apply strain controlled loading to the uniaxial sample, as shown in Fig. 2.14(a), at a range of different strain rates as shown, the stress response (for given σy , K, and m) as a function of the plastic strain is shown in Fig. 2.14(b). The strain rate dependence of stress is clear and for the three strain rates applied, the corresponding stresses are given by Equation (2.87). Once yield is achieved, for uniaxial perfect plasticity, since dσ = 0, dp = dε, or equivalently, p˙ = ε˙ so that the stresses are σ1 = σy + K ε˙ 1m , σ2 = σy + K ε˙ 2m , σ3 =

(2.88)

σy + K ε˙ 3m .

Many materials exhibit strain rate-dependent plasticity, but unlike the stress–strain curves in Fig. 2.14, would also show isotropic or kinematic hardening. Let us return to the case of isotropic hardening given in Equation (2.86). We can rearrange the equation to give σ − r − σy 1/m p˙ = . (2.89) K If in addition to isotropic hardening, kinematic hardening also occurs, Equation (2.89) becomes σ − x − r − σy 1/m p˙ = . (2.90) K Equations (2.89) and (2.90) are constitutive equations relating uniaxial plastic strain rate to uniaxial stress, and which depend upon internal variables; the isotropic hardening, r, and the kinematic hardening, x. For a von Mises material, the uniaxial stress is identical to the effective stress and similarly for the effective plastic strain rate. Equation (2.90) can therefore be written J (σ − x ) − r − σy 1/m p˙ = . (2.91) K

Viscoplasticity and creep

41

In viscoplasticity, we need a constitutive equation, such as (2.91), which relates the effective plastic strain rate to the stress and internal hardening variables. This replaces the consistency condition in time-independent plasticity, which forces the load point to stay on the yield surface during plastic deformation. In viscoplasticity, the load point may lie outside the yield surface because of the viscous or over-stress. In addition to the viscoplastic constitutive equation, as before, we make use of the normality hypothesis and the elastic constitutive equation; namely Hooke’s law. For viscoplasticity, we write the normality hypothesis, from Equation (2.17), as ε˙ p = λ˙

∂f . ∂σ

(2.92)

The yield function is, from Section 2.6, f = J (σ − x ) − r(p) − σy so that

(2.93)

∂f 3 σ − x

= ∂σ 2 J (σ − x )

and

3 σ − x

λ˙ . (2.94) 2 J (σ − x ) We showed in Section 2.5.3 that for a von Mises material, dp = dλ, or equivalently p˙ = λ˙ so that (2.94) becomes ε˙ p =

ε˙ p =

σ − x

3 p˙ . 2 J (σ − x )

(2.95)

We may now combine the constitutive equation given in (2.91) with (2.95) to give the plastic ﬂow rule for viscoplasticity with isotropic and kinematic hardening as 1/m 3 J (σ − x ) − r − σy σ − x

p ε˙ = . (2.96) K 2 J (σ − x ) To complete the model, we need the evolution equations for the isotropic and kinematic hardening variables r and x, and the rate form of Hooke’s law. From Section 2.4, Equation (2.37) and Section 2.5.2, Equation (2.65), the hardening rates are given by r˙ (p) = b(Q − r)p, ˙

(2.97)

2 p cε˙ − γ x p˙ (2.98) 3 and we will now write Hooke’s law in terms of tensor rather than vector strain terms as x˙ =

σ˙ = 2G˙εe + λ Tr(˙εe )I ,

(2.99)

42

Continuum plasticity

where ε˙ e = ε˙ − ε˙ p

(2.100)

and in which G is the shear modulus, λ the Lame constant given by λ=

Eν (1 − 2ν)(1 + ν)

and I is the identity tensor given by ⎛

1 I = ⎝0 0

⎞ 0 0⎠ . 1

0 1 0

Equations (2.96)–(2.100) form the complete elastic–viscoplastic model. At a given time, t, with knowledge of the current total strain rate, ε˙ and the hardening variables r and x, together with the stress, σ , these equations enable the stresses at the end of a given step forward in time to be determined. We will address this in a later chapter, but for now, let us examine the equations for a simple problem of uniform, uniaxial, and axisymmetric upsetting. 2.7.1

Uniform, uniaxial, and axisymmetric compression

Upsetting is the name given to the open-die forging of cylindrical billets of material. We will consider the uniaxial compression of a cylinder between two platens such that the frictional effects on the contacting surfaces are negligible so that the cylinder remains under uniform, uniaxial compression. The process is shown schematically in Fig. 2.15.

z Undeformed material Platens Deformed material

u r

Fig. 2.15 Frictionless, uniaxial compression representing open-die forging.

Viscoplasticity and creep

43

We will consider constant strain rate-controlled loading and write the plastic strain rates as ⎞ ⎛ p p ε˙ rr ε˙ rz 0 ⎟ ⎜ p p ⎟. ε˙ p = ⎜ (2.101) ε ˙ 0 ε ˙ zz rz ⎠ ⎝ p 0 0 ε˙ θ θ Because we are assuming friction to be negligible, the shear terms are zero. The boundary conditions give us that σrr = σθ θ = σrz = 0 so that the stress and deviatoric stress tensors for the problem become ⎛ 1 ⎞ ⎞ ⎛ 0 0 − 3 σzz 0 0 0 ⎜ ⎟ 2 σ = ⎝ 0 σ = ⎝0 σzz 0⎠ , 0 ⎠. 3 σzz 0 0 0 0 0 − 13 σzz

(2.102)

We will now use Equation (2.96) to determine the plastic strain rate components for the problem. Under this loading, J (σ − x ) = σzz − x (2.103) and from Section 2.5.1,

⎛

− 21 (σzz − x) 0 2

⎝ σ −x = 0 σzz − x 3 0 0

⎞

0 0 − 21 (σzz

⎠ − x)

so that (2.96) becomes ⎞ ⎛ p p ε˙ rr ε˙ rz 0 ⎟ 3 |σzz − x| − r − σy 1/m ⎜ p p ⎟= ⎜ε˙ rz ε˙ zz 0 ⎠ 2 ⎝ K p 0 0 ε˙ θθ ⎛ 1 0 − (σzz − x) 2⎜ 2 1 × 0 σzz − x ⎝ |σzz − x| 3 0 0 which reduces to ⎛ p ⎞ p ⎛ ε˙ rr ε˙ rz 0 1/m − 21 ⎜ p ⎟ |σzz − x| − r − σy ⎜ p ⎜ε˙ rz ε˙ zz 0 ⎟ ⎝ 0 ⎝ ⎠= K p 0 0 0 ε˙ θ θ

(2.104)

0 1 0

⎞

0

⎟ ⎠

0 − 21 (σzz − x)

0

⎞

⎟ 0 ⎠. − 21

(2.105)

44

Continuum plasticity

We may now look at individual components of the plastic strain rate. We see that |σzz − x| − r − σy 1/m p ε˙ zz = (2.106) K which is, of course, just what we would get for purely uniaxial loading, and Equation (2.105) also shows that 1 p 1 |σzz − x| − r − σy 1/m p p ε˙ rr = ε˙ θ θ = − ε˙ zz = − 2 K 2 demonstrating that the incompressibility condition of plasticity is satisﬁed. 2.7.2

Power-law creep

Let us look at one further case in which we assume there to be neither isotropic nor kinematic hardening. Equation (2.96) then becomes, for the plastic strain rate, 1/m σ

3 J (σ ) − σy p (2.107) ε˙ = K J (σ ) 2 and J (σ ) = σe so the equation reduces further to 3 σe − σy 1/m σ

p ε˙ = . 2 K σe

(2.108)

Often in creep problems, where the time-dependent deformation is not dependent upon yield, creep deformation is assumed to occur with the application of a non-zero stress. For creep problems, therefore, Equation (2.108) is often written σ

3 σe 1/m σ

3 3 ε˙ c = = A(σe )n = Aσen−1 σ

(2.109) 2 K σe 2 σe 2 which is the multiaxial form of Norton’s creep law, where A and n are material constants. For uniaxial loading, it reduces to 2 3 Aσen−1 σ = Aσ n . 2 3 For completeness, we can write out Equation (2.109) in full component form as ⎛

⎛ c c c ⎞

⎞ σxx σxy ε˙ xx ε˙ xy ε˙ xz σxz ⎜ c c c ⎟ = 3 Aσ n−1 ⎜σ

⎟ ε˙ yz σyz (2.110) ⎠ ⎝ yx σyy ⎠ ⎝ε˙ yx ε˙ yy e 2 c c c

ε˙ zx ε˙ zy ε˙ zz σzx σzy σzz ε˙ c =

in which the stress and strain rate tensors are symmetric.

Further reading

2.7.3

45

Potential and yield function equivalence

In the last example, we saw how the plastic strain rate, based on the normality hypothesis together with an appropriate constitutive equation for plastic strain rate, was determined for viscoplasticity, but then reduced to Norton’s law for creep deformation. Because creep processes may occur independently of plastic yielding, it is not appropriate to use a yield surface, in the conventional sense discussed earlier. Instead, a potential function is deﬁned from which creep strain rates are determined. We will deﬁne a potential, φ, such that ε˙ 0 σ0 σe n+1 φ= (2.111) n + 1 σ0 in which ε˙ 0 and σ˙ 0 are material constants with units of strain rate and stress, respectively. The potential function, φ, therefore has units of Joules per second per unit volume. It therefore represents an energy per second per unit volume. The plastic (creep) strain rate is determined from ∂φ ∂σ

(2.112)

3 ε˙ 0 σ0 n−1 3 σ σ = Aσen−1 σ , 2 σ0n+1 e 2

(2.113)

ε˙ c = giving ε˙ c =

which is identical to Equation (2.109). The potential function, φ, in creep plays a similar role to the yield function in plasticity. In fact, often the yield function is considered to be a potential function. The surfaces in stress space represented by φ are often called equipotential surfaces; the energy per second per unit volume is the same at each point on the potential surface, just as the value of σe takes the same value on every point of a yield surface in plasticity.

Further reading Dieter, G.E. (1988). Mechanical Metallurgy. McGraw-Hill Book Co., London. Hill, R. (1998). The Mathematical Theory of Plasticity. OUP (Oxford Classics Series). (ﬁrst published in 1950). Khan, A.S. and Huang, S. (1995). Continuum Theory of Plasticity. John Wiley & Sons Inc, New York. Lemaitre, J. and Chaboche, J.-L. (1990). Mechanics of Solid Materials. CUP, Cambridge, UK. Lubarda, V.A. (2002). Elastoplasticity Theory. CRC Press, Florida, USA.

This page intentionally left blank

3. Kinematics of large deformations and continuum mechanics

3.1

Introduction

The strains, be they elastic or plastic, which most engineering components undergo in service are usually small, that is, 200%). This is three orders of magnitude larger than the strain needed to cause yield. In manufacturing processes, another very important feature is material rotation. Deformation processing leading to large plastic strains often also leads to large rigid body rotations. The bending of a circular plate, to large deformation, is an example which shows the rigid body rotation. Figure 3.1 shows the result of applying a large downward displacement at the centre of an initially horizontal, simply supported circular disc. Only one half of the disc section is shown. While the displacements and rigid body rotations can be very large, the strains remain quite small.

×

×

Fig. 3.1 Simulated large elastic–plastic deformation of an initially horizontal, simply supported circular plate. Only one half of the plate section is shown.

48

Large deformations and continuum mechanics

Towards the outer edge of the disc, where it is supported, the ﬁnite element simulation shows that the strains generated are quite small, but that because of the disc bending, the rigid body rotations are very large. Generally, deformation comprises of stretch, rigid body rotation, and translation. The stretch provides the shape change. The rigid body rotation neither contributes to shape change nor to internal stress. Because a translation does not lead to a change in stress state, we will not address it in detail here. In this chapter, we will give an introduction to measures of large deformation, rigid body rotation, elastic–plastic coupling in large deformation, stress rates, and what is called material objectivity, or frame indifference. Later chapters dealing with the implementation of plasticity models into ﬁnite element code will rely on the material covered here and in Chapter 2.

3.2

The deformation gradient

In order to look at deformation, let us consider a small lump of imaginary material which is yet to be loaded so that it is in the undeformed (or initial ) conﬁguration (or state). This is shown schematically as state A in Fig. 3.2. We will now apply a load to the material in state A so that it deforms to that shown in state B, the deformed or current conﬁguration. We will assume that the material undergoes combined stretch (i.e. relative elongations with respect to the three orthogonal axes), rigid body rotation, and translation. We will measure all quantities relative to the global XYZ axes, often known as the material coordinate system. Consider an inﬁnitesimal line, PQ, or vector, dX, embedded in the material in the undeformed conﬁguration. The position of point P is given by vector X, relative to the material reference frame. The line PQ undergoes deformation from state A to the deformed

Deformed (current) configuration, state B

Z Q9 dx O

x Q dX X

P9 u

X

P Y

Undeformed (original) configuration, state A

Fig. 3.2 An element of material in the reference or undeformed conﬁguration undergoing deformation to the deformed or current conﬁguration.

Measures of strain

49

conﬁguration in state B. In doing so, point P has been translated by u to point P . Relative to the material reference frame, point P is given by vector x where x = X + u.

(3.1)

The inﬁnitesimal vector dX is transformed to its deformed state, dx, by the deformation gradient, F , where dx = F dX. We can write this in component form as ⎛ ⎞ ⎛ Fxx dx ⎝dy ⎠ = ⎝Fyx dz Fzx

Fxy Fyy Fzy

⎛ ∂x

⎞ ⎛ ⎞ ⎜ ∂X dX Fxz ⎜ ⎜ ∂y ⎠ ⎝ dY ⎠ = ⎜ Fyz ⎜ ∂X dZ Fzz ⎝ ∂z ∂X

(3.2) ∂x ∂Y ∂y ∂Y ∂z ∂Y

∂x ⎞ ∂Z ⎟ ⎛dX ⎞ ⎟ ∂y ⎟ ⎝ ⎠ ⎟ dY ∂Z ⎟ dZ ⎠ ∂z ∂Z

(3.3)

or F =

∂x . ∂X

(3.4)

The deformation gradient, F , provides a complete description of deformation (excluding translations) which includes stretch as well as rigid body rotation. Rigid body rotation does not contribute to shape or size change, or internal stress. In solving problems, it is necessary to separate out the stretch from the rigid body rotation contained within F . In the following sections, we will see examples of stretch, rigid body rotation, and their combination, and how they are described by the deformation gradient.

3.3

Measures of strain

Let us consider the length, ds, of the line dx in the deformed conﬁguration. We may write ds 2 = dx · dx = (F dX) · (F dX) = dXT F TF dX T ∂x T ∂x = dX dX = dXT C dX ∂X ∂X so that C = F TF .

(3.5)

C is called the (left) Cauchy–Green tensor. Consider also the length, dS, of the element, dX, in the undeformed state: dS 2 = dXT dX.

(3.6)

50

Large deformations and continuum mechanics

Now dx = F dX so

dX = F −1 dx.

Substituting into Equation (3.6) gives dS 2 = (F −1 dx)T F −1 dx = dx T (F −1 )TF −1 dx = dx T B −1 dx, where

B −1 = (F −1 )TF −1

(3.7)

and B is called the (right) Cauchy–Green tensor. Both B and C are in fact measures of stretch as we will now see. A measure of the stretch is given by the difference in lengths of the lines PQ and

P Q in Fig. 3.2 in the undeformed and deformed conﬁgurations, respectively. We can write (3.8) ds 2 − dS 2 = dx · dx − dx · B −1 dx = dx · (I − B −1 ) dx in which I is the identity tensor. It can be seen, therefore, that B is related to the change in length of the line; in other words, a measure of stretch. It is independent of rigid body rotation because the orientations of the lines in the undeformed and deformed conﬁgurations are irrelevant. If ds and dS are the same length, then there is no stretch and ds 2 − dS 2 = 0. From Equation (3.8), this means that B=I

(3.9)

and there is no stretch, so that in this instance, the deformation gradient contains only rigid body rotation. The Cauchy–Green tensor, B, could itself be used as a measure of strain, since it is independent of rigid body rotation, but depends upon the stretch. This is an important criterion for any strain measure in large deformation analysis in which rigid body rotation occurs. A strain which depends upon rigid body rotation would not be appropriate since it would give a different measure of the strain depending upon orientation. However, the Cauchy–Green tensor given in (3.9) contains nonzero components even though the stretch is zero. An alternative and more appropriate strain measure called the Almansi strain was introduced: 1 e = (I − B −1 ) (3.10) 2 so that for zero stretch, e = 0.

Measures of strain

51

This strain measure behaves more like familiar strains, such as engineering strain, since for zero stretch, it gives us strain components of zero. A further measure of strain is the logarithmic, or true strain deﬁned as 1 ε = − ln B −1 , (3.11) 2 which we shall consider in more detail later. In determining the change of length of the line OP, we could have chosen the original conﬁguration to work in as follows: ds 2 − dS 2 = dx T dx − dX T dX = (F dX)T F dX − dXT dX = dXF TF dX − dXT dX = dXT (F TF − I ) dX = dXT (C − I ) dX = dXT (2E) dX, where

1 1 (C − I ) = (F TF − I ). (3.12) 2 2 E is called the large strain or the Green–Lagrange strain tensor. We can make this look a little more familiar, perhaps, by combining Equations (3.4) for F and (3.1) for x ∂x ∂(u + X) ∂u F = = = +I ∂X ∂X ∂X and then substituting into (3.12) to give

T 1 T ∂u 1 ∂u E = (F F − I ) = +I +I −I 2 2 ∂X ∂X

∂u T ∂u T ∂u 1 ∂u + . (3.13) + = 2 ∂X ∂X ∂X ∂X E=

If we ignore the second-order term, this reduces to 1 ∂u ∂u T E= . + 2 ∂X ∂X

(3.14)

We will examine this and other strains for simple uniaxial loading in Section 3.4. Before doing so, let us examine the symmetry of the strain quantities presented above. The symmetric part of a tensor, A, is given by 1 (A + AT ) (3.15) 2 and the antisymmetric or skew symmetric (or sometimes simply skew) part of A by sym(A) =

asym(A) =

1 (A − AT ). 2

(3.16)

52

Large deformations and continuum mechanics

To be pedantic, let us write out the symmetric and antisymmetric parts of the 2 × 2 matrix A given by a11 a12 A= a21 a22 in which a12 = a21 . ⎛ a12 + a21 ⎞ a11 2 ⎠ sym(A) = ⎝ a12 + a21 a22 2 and ⎛ a12 − a21 ⎞ 0 2 ⎠. asym(A) = ⎝ a12 − a21 − 0 2 Clearly, sym(A) is symmetric and the leading diagonal of an antisymmetric tensor always contains zeros. Let us now consider the quantity F TF which appears above in a number of strain quantities: 1 sym(F TF ) = [F TF + (F TF )T ] = F TF 2 and 1 asym(F TF ) = [F TF − (F TF )T ] = 0. 2 We see, therefore, that F TF is a symmetric tensor so that, in fact, the quantities B −1 , C, ε, and E are all themselves symmetric. In general, F will not necessarily be symmetric. If it is, the deformation it represents is made only up of stretch.

3.4

Interpretation of strain measures

Let us determine the deformation gradient for the simple case of a uniaxial rod which is subjected, ﬁrst to purely rigid body rotation and then to uniaxial stretch and then consider some of the measures of deformation and strain introduced in Section 3.3. 3.4.1

Rigid body rotation only

Figure 3.3 shows a rod lying along the Y -axis which undergoes a clockwise rotation about the Z-axis of angle θ . There is no stretch imposed, so the deformation gradient is simply the rotation matrix, R, given by ⎞ ⎛ cos θ − sin θ 0 (3.17) F = R = ⎝ sin θ cos θ 0⎠ . 0 0 1

Interpretation of strain measures

Y, y

y

53

u Y x

X, x

X

Fig. 3.3 A rod undergoing rigid body rotation through angle θ.

The uppercase letters in Fig. 3.3, XY, refer to the material reference frame directions. Also shown in the ﬁgure is a coordinate system which rotates with the deforming material (in this case, the rotating rod). We will generally use lowercase letters, xy, to indicate the reference frame which rotates with the material. This is called the co-rotational reference frame. We can now determine the Cauchy–Green tensor, B −1 , and the strain quantities. From Equation (3.7), ⎞ ⎞⎛ ⎛ cos θ sin θ 0 cos θ − sin θ 0 B −1 = (F −1 )TF −1 = ⎝ sin θ cos θ 0⎠ ⎝− sin θ cos θ 0⎠ 0 0 1 0 0 1 ⎞ ⎛ 1 0 0 ⎝ = 0 1 0⎠ . 0 0 1 The tensor B −1 is found to be the identity tensor for rigid body rotation because there is no stretch. Measures of deformation that are appropriate for large deformations with rigid body rotation must have this property: that they depend upon the stretch but are independent of the rigid body rotation. The Almansi strain, from (3.10), is 1 e = (I − B −1 ) = 0 2 and the true strain, (3.11), is given by 1 ε = ln B −1 = 0. 2 Similarly, the Green strain is 1 E = (F TF − I ) = 0. 2 We see that the three strain measures give zero for the case of rigid body rotation. Before moving away from rotation, it is important to note that a rotation tensor, such as R, is always orthogonal, that is, RR T = I

(3.18)

54

Large deformations and continuum mechanics

Deformed rod after stretch

Undeformed rod

Y, y

l

l0

Z, z

X, x

r r0

Fig. 3.4 A rod undergoing pure stretch in the absence of rigid body rotation.

so that

R T = R −1 .

We will make much use of this property in the subsequent sections. 3.4.2

Uniaxial stretch

Let us now consider uniaxial stretch of the circular rod in the Y -direction. This is shown schematically in Fig. 3.4. Note that because there is no rotation in this case, the co-rotational reference frame is directionally coincident with the material reference frame. For the uniaxial stretch shown, the stretch ratios, λ, are λx =

r , r0

λy =

l , l0

λz =

r . r0

(3.19)

Let us consider the case of large strain such that the elastic strains can be ignored. For large plastic deformation, the incompressibility condition written in terms of stretches is λx λy λz = 1 (3.20) so that

and therefore

1 λx = λz ≡ λy

−1/2 l λx = λz = . (3.21) l0 Considering the stretch along the Y -axis, any point, Y , lying on the undeformed rod becomes the point y = λy Y on the deformed rod. The deformation can therefore be represented by x = λx X, y = λy Y, z = λz Z

Interpretation of strain measures

so that

∂x = λx , ∂X

∂y = λy , ∂Y

55

∂z = λz ∂Z

and

∂x ∂x = = 0 etc. ∂Y ∂Z The deformation gradient can then be determined using Equation (3.3), ⎛ ⎞ ∂x ∂x ∂x ⎜ ∂X ∂Y ∂Z ⎟ ⎛ ⎞ ⎜ ⎟ λx 0 0 ⎜ ⎟ ∂x ∂y ∂y ∂y ⎟ ⎝ =⎜ = 0 λy 0 ⎠ F = ⎜ ∂X ⎜ ∂X ∂Y ∂Z ⎟ ⎟ 0 0 λz ⎝ ∂z ∂z ∂z ⎠ ∂X ∂Y ∂Z and with (3.19) and (3.21) ⎞ ⎛ −1/2 l 0 0 ⎟ ⎜ l ⎟ ⎜ 0 ⎟ ⎜ l ⎟. 0 0 F =⎜ ⎟ ⎜ l0 ⎟ ⎜ −1/2 ⎠ ⎝ l 0 0 l0 We ﬁrst notice that F is symmetric so that FT = F and therefore represents stretch only. Let us examine the various deformation and strain tensors. The inverse of F is ⎛ 1/2 ⎞ l 0 0 ⎟ ⎜ ⎜ l0 ⎟ ⎜ ⎟ −1 l ⎜ ⎟ F −1 = ⎜ 0 0 ⎟ ⎜ ⎟ l0 ⎜ 1/2 ⎟ ⎝ ⎠ l 0 0 l0 so the Cauchy–Green tensor is given by ⎛ ⎞ l 0 0⎟ ⎜ l0 ⎜ ⎟ −2 ⎜ ⎟ l −1 −1 T −1 −1 −1 B = (F ) F = F F = ⎜ 0⎟ ⎜0 ⎟. l0 ⎜ ⎟ ⎝ l⎠ 0 0 l0

56

Large deformations and continuum mechanics

The true plastic strain is, therefore, ⎞ ⎛ ⎛ ⎞ l 1 l 0 0 − ln 0 0 ⎟ ⎜ l0 ⎟ 2 l0 ⎜ −2 ⎟ ⎜ ⎟ ⎜ ⎟ ⎜ 1 1 l l ⎟ ⎜ ⎟=⎜ ε = − ln B −1 = − ln ⎜ 0 ln 0 ⎟. 0 0 ⎟ ⎜ ⎟ 2 2 ⎜ l0 l0 ⎟ ⎜ ⎝ 1 l⎠ ⎝ l⎠ 0 0 − ln 0 0 2 l0 l0 (3.22) We see that the true strain components are εxx = εzz = − 21 ln(l/l0 ) = − 21 εyy and εyy = ln(l/l0 ), as we would expect for uniaxial plasticity conditions. Before leaving the true strain, note that we needed to take the logarithm of the Cauchy–Green tensor which we did by operating on the leading diagonal alone. We were able to do this in this case because the leading diagonal terms happen, in this simple case, to be the principal parts of the tensor (i.e. the eigenvalues). In general, in order to carry out an operation, p, on tensor A having a linearly independent set of eigenvectors, we need to diagonalize the tensor and operate on the principal values. In practice, this means transforming the tensor into its principal coordinates, by ﬁnding the eigenvalues and eigenvectors of A, operating on it and transforming it back. If the modal matrix (i.e. the matrix containing the eigenvectors of A) is written as M, and the diagonal matrix (i.e. the matrix containing the ˆ then A can be written eigenvalues of A along the leading diagonal) as A, ˆ −1 A = M AM so that we operate on A to give p(A) as follows −1 ˆ p(A) = Mp(A)M ,

(3.23)

where the operation p is carried out only on the leading diagonal terms. For example, −1 ˆ ln(A) = M ln(A)M .

In Equation (3.22), the modal matrix of B −1 in this case is just the identity matrix and −1 its diagonal matrix Bˆ is the same as B −1 so that ln(B −1 ) = M ln(Bˆ

−1

)M −1 = I ln(B −1 )I −1 = ln(B −1 ).

Let us ﬁnally determine the Green strain ﬁrst from (3.12) and second directly from the displacements using (3.14).

Polar decomposition

Using (3.12), we need ⎛ 2 r 0 ⎜ ⎜ r0 2 ⎜ l ⎜ F TF = ⎜ 0 ⎜ l0 ⎜ ⎝ 0 0

⎞

⎛ 2r ⎟ 1 + ⎟ ⎜ r0 ⎟ ⎜ ⎟ ⎜ 0 0 ⎟≈⎜ ⎟ ⎜ 2 ⎟ ⎝ r ⎠ 0 r0 0

57

⎞ 0

0

2l 1+ l0 1+

0

⎟ ⎟ ⎟ 0 ⎟ ⎟ 2r ⎠ r0

if we write r = r0 + r and assume that the strains are small, so that ⎤ ⎛ ⎡⎛ ⎞ ⎞ 2r r 1 + 0 0 0 0 ⎢⎜ ⎟ ⎛1 0 0⎞⎥ ⎜ r0 ⎟ r0 ⎥ ⎜ ⎢ ⎜ ⎟ ⎟ 1 ⎢⎜ l 2l ⎥ ⎜ ⎟ ⎝ ⎟ ⎠ = − E = ⎢⎜ 0 0 0 1+ 0 0 1 0 ⎥ ⎜ ⎟ ⎟. ⎥ ⎜ ⎟ ⎟ 2 ⎢⎜ l0 l0 0 0 1 ⎦ ⎝ ⎣⎝ r ⎠ 2r ⎠ 0 0 0 0 1+ r0 r0 We see that the components of the Green strain are therefore approximately the engineering strain components. If we now start from (3.14) in which we have also neglected second-order terms, we need the displacements, u, which are given by ux = (r − r0 ) so that

⎛

r ⎜ r0 ⎜ ∂u ⎜ =⎜ 0 ∂X ⎜ ⎝ 0

Y uy = (l − l0 ) , l0

X , r0

l l0 0

0 ⎟ ⎟ ⎟ 0 ⎟ ⎟ r ⎠ r0

Z r0

⎛

⎞ 0

uz = (r − r0 )

and

r ⎜

⎜ r0 ∂u T 1 ∂u ⎜ =⎜ 0 + E= ⎜ 2 ∂X ∂X ⎝ 0

⎞ 0 l l0 0

0 ⎟ ⎟ ⎟ 0 ⎟ ⎟ r ⎠ r0

as before. We have looked at a number of examples in which stretch and rigid body rotation have taken place exclusively. We will now look at how to separate them in cases where they occur simultaneously, using the polar decomposition theorem.

3.5

Polar decomposition

Recall that the deformation at any material point can be considered to comprise three parts: (1) rigid body translation (which we do not need to consider here); (2) rigid body rotation; (3) stretch.

58

Large deformations and continuum mechanics

The polar decomposition theorem states that any non-singular, second-order tensor can be decomposed uniquely into the product of an orthogonal tensor (a rotation), and a symmetric tensor (stretch). The deformation gradient is a non-singular, second-order tensor and can therefore be written as F = RU = VR, (3.24) where R is an orthogonal (R TR = I ) rotation tensor, and U and V are symmetric (U = U T ) stretch tensors. Using the polar decomposition theorem, we can now examine in more detail the right and left Cauchy–Green deformation tensors. From Equation (3.7), B −1 = (F −1 )TF −1 = [(VR)−1 ]T (VR)−1 = (R −1 V −1 )T R −1 V −1 = (V −1 )T (R −1 )T R −1 V −1 = (V −1 )T V −1 since R is orthogonal

B −1 = V −1 V −1 = (V −1 )2 ,

where the squaring operation is carried out on the diagonalized form of V −1 . This conﬁrms, therefore, that B is a measure of deformation that depends on stretch only, and is independent of the rigid body rotation, R. Similarly, for C, C = F TF = (RU )TRU = U T R TRU = U TU = U2

since R is orthogonal since U is symmetric.

The true strain rate can now be written in terms of V since 1 1 (3.25) ε = − ln B −1 = − ln(V −1 )2 = ln V , 2 2 which is also independent of the rigid body rotation and dependent on the stretch alone. Let us have a look at a problem in which both stretch and rigid body rotation occur together: the problem of simple shear. 3.5.1

Simple shear

Figure 3.5 shows schematically the simple shear by δ, in two dimensions, of a unit square. We can represent the deformation, which transforms a point (X, Y ) in the undeformed conﬁguration to (x, y) in the deformed conﬁguration, by x = X + δY,

y=Y

Polar decomposition

Y, y

59

Deformed square

d 1 Undeformed square 1

X, x

Fig. 3.5 A unit square undergoing simple shear.

so that

∂x ∂x = 1, = δ, ∂X ∂Y The deformation gradient is, therefore, 1 F = 0

∂y = 0, ∂X

∂y = 1. ∂Y

δ . 1

We can then determine the Cauchy–Green tensor, C, from 1 0 1 δ 1 δ T C=F F = . = δ 1 0 1 δ 1 + δ2

(3.26)

Note the symmetry of this deformation tensor. We can use the polar decomposition theorem to separate out the stretch and rigid body rotation contained in the deformation gradient. Let us set cos ϕ sin ϕ Uxx Uxy R= (3.27) U= − sin ϕ cos ϕ Uyx Uyy so that

F = RU

gives

1 0

δ cos ϕ = 1 − sin ϕ

sin ϕ cos ϕ

Uxx Uyx

Uxy . Uyy

(3.28)

Solving for the stretches in terms of δ and ϕ gives cos ϕ sin ϕ U= sin ϕ cos ϕ + δ sin ϕ and substituting back into (3.28) gives δ sin ϕ = √ 2 2 + δ2

and

so that R=√

1 22 + δ 2

2 cos ϕ = √ 2 2 + δ2

2 −δ

δ 2

(3.29)

60

Large deformations and continuum mechanics

and U=√

1

2 δ

δ . 2 + δ2

(3.30) 22 + δ 2 Comparing Equations (3.30) and (3.26), and with a little algebra conﬁrms that C = U 2 . U is the symmetric stretch and Equation (3.29) shows that the rigid body rotation is non-zero. It is useful to examine why this is. It may not be obvious that the deformation corresponding to simple shear shown in Fig. 3.5 leads to a rigid body rotation. Let us ﬁrst determine the Green–Lagrange strain for this deformation. Using Equation (3.12), 1 T 1 1 1 0 δ 1 δ 1 0 E = (F F − I ) = (C − I ) = − = . δ 1 + δ2 0 1 2 2 2 δ δ2 2 (3.31) From Equation (3.29), or from the components of strain in Equation (3.31), we see that the principal stretch directions rotate as the simple shear proceeds. That is, the ‘material axes’ rotate relative to the direction of the applied deformation. The polar decomposition theorem is fundamental to large deformation kinematics and we shall return to it in subsequent sections.

3.6

Velocity gradient, rate of deformation, and continuum spin

We have so far considered stretch, rigid body rotation, measures of strain, and the polar decomposition theorem which enables us to separate out stretch and rotation. All the quantities considered have been independent of time. However, many plasticity formulations (viscoplasticity is an obvious case) are developed in terms of rate quantities and it is necessary, therefore, to consider how the quantities already discussed can be put in rate form. Often, in fact, even rate-independent plasticity models are written in rate form for implementation into ﬁnite element code. This is easy to understand given that plasticity is an incremental process; rather than deal with increments in plastic strain, it is often more convenient to work with the equivalent quantity, plastic strain rate. Consider a spatially varying velocity ﬁeld, that is, one for which the material point velocities vary spatially. The increment in velocity, dv, occurring over an incremental change in position, dx, in the deformed conﬁguration, may be written as ∂v dx. ∂x The velocity gradient describes the spatial rate of change of the velocity and is given by dv =

L=

∂v . ∂x

(3.32)

Velocity gradient, rate of deformation, and continuum spin

61

Consider the time rate of change of the deformation gradient: ∂ ∂x ∂v ∂v ∂x ˙ F = = = = LF ∂t ∂X ∂X ∂x ∂X or ˙ −1 . L = FF

(3.33)

The velocity gradient, therefore, maps the deformation gradient onto the rate of change of the deformation gradient. The velocity gradient can be decomposed into symmetric (stretch related) and antisymmetric (rotation related) parts: L = sym(L) + asym(L), where sym(L) =

1 (L + LT ) 2

(3.34)

and 1 (L − LT ). (3.35) 2 The symmetric part is called the rate of deformation, D, and the antisymmetric part the continuum spin, W , so that asym(L) =

L = D + W,

(3.36)

where the rate of deformation D=

1 (L + LT ) 2

(3.37)

1 (L − LT ). 2

(3.38)

and the continuum spin is given by W =

We shall now examine both quantities, the rate of deformation and the continuum spin, for some simple examples, including uniaxial stretch and purely rigid body rotation in order to gain a physical feel for these quantities. 3.6.1

Rigid body rotation and continuum spin

We have previously looked at the rigid body rotation of a uniaxial rod. Figure 3.3 shows this schematically. We will now look not only at the rigid body rotation, but also the rate at which it occurs. Consider the rotation of the rod shown in Fig. 3.3,

62

Large deformations and continuum mechanics

at time t making an angle θ with the Y -axis, with no stretch, rotating at constant rate ˙ The deformation gradient at any instant is given by θ. ⎞ ⎛ cos θ − sin θ 0 (3.39) F = ⎝ sin θ cos θ 0⎠ 0 0 1 so that the rate of change of deformation gradient is ⎛ − sin θ − cos θ F˙ = θ˙ ⎝ cos θ − sin θ 0 0

⎞ 0 0⎠ . 0

(3.40)

In order to determine the velocity gradient, we need the inverse of F which we can obtain from (3.39) as ⎞ ⎛ cos θ sin θ 0 F −1 (= F T in this case) = ⎝− sin θ cos θ 0⎠ . 0 0 1 We may then determine the velocity gradient using Equation (3.33) as ⎞ ⎛ ⎞⎛ ⎛ 0 cos θ sin θ 0 − sin θ − cos θ 0 ˙ −1 = θ˙ ⎝ cos θ L = FF − sin θ 0⎠ ⎝− sin θ cos θ 0⎠ = θ˙ ⎝1 0 0 0 1 0 0 0 The transpose of L is

⎛

0 LT = θ˙ ⎝−1 0 so that the deformation gradient is given by

1 0 0 ⎛

0 1 D = (L + LT ) = θ˙ ⎝0 2 0

⎞ 0 0⎠ . 0

⎞ 0 0⎠ 0 0 0 0

⎞ 0 0⎠ = 0 0

and the continuum spin is

⎛ 0 1 W = (L − LT ) = θ˙ ⎝1 2 0

−1 0 0

−1 0 0

⎞ 0 0⎠ . 0

(3.41)

That is, there is no stretch rate contributing to the velocity gradient so that the rate of deformation is zero, but rigid body rotation occurs so that the continuum spin is non-zero. Let us now examine the signiﬁcance of the continuum spin for the case of rigid body rotation of the uniaxial rod without stretch.

Velocity gradient, rate of deformation, and continuum spin

˙ given by Consider the rate of rotation, R, ⎛ − sin θ − cos θ ˙ ⎝ ˙ R = θ cos θ − sin θ 0 0 Next, consider the product of W and R ⎞⎛ ⎛ cos θ − sin θ 0 −1 0 ⎠ ⎝ ⎝ ˙ WR = θ 1 0 0 sin θ cos θ 0 0 0 0 0

⎞ 0 0⎠ . 0

⎞ ⎛ − sin θ 0 ⎠ ⎝ ˙ 0 = θ cos θ 0 1

63

(3.42)

− cos θ − sin θ 0

⎞ 0 0⎠ . 0

That is, for this particular case of rigid body rotation only, we see that ˙ = WR R

(3.43)

˙ Remembering that R is orthogonal so so that W is the tensor that maps R onto R. T −1 that R = R , W can be written for this simple case as ˙ T. W = RR

(3.44)

The spin is not itself, therefore, a rate of rotation, but it is closely related to it. Let us use the polar decomposition theorem to examine the continuum spin in a little more detail and more generally, and introduce the angular velocity tensor. 3.6.2

Angular velocity tensor

From Equation (3.38), the continuum spin is given by 1 (L − LT ) 2 so substituting for the velocity gradient from (3.33) gives W =

1 ˙ −1 ˙ −1 − (F −1 )TF˙ T ). ˙ −1 )T ) = 1 (FF (FF − (FF 2 2 If we now substitute for F using the polar decomposition theorem in (3.24), after a little algebra we obtain W =

1 ˙ T ˙ T + R(U˙ U −1 − (U˙ U −1 )T )R T ]. [RR − R R 2 We will simplify this further by considering the product W =

RR T = I , which we can differentiate with respect to time to give ˙ T + RR ˙T =0 RR

(3.45)

64

Large deformations and continuum mechanics

so that

˙ T = −R R ˙ T = −(RR ˙ T )T . RR

(3.46)

˙ T is antisymmetric, since any tensor Z for which Z = −Z T We see, therefore, that RR is antisymmetric because 1 1 (Z + Z T ) = (Z − Z) = 0. 2 2 Substituting (3.46) into (3.45) gives sym(Z) =

˙ T + 1 R(U˙ U −1 − (U˙ U −1 )T )R T W = RR 2

(3.47)

or 1 (3.48) W = Ω + R(U˙ U −1 − (U˙ U −1 )T )R T = + R asym(U˙ U −1 )R T 2 ˙ T is called the angular velocity tensor which depends only on the in which Ω = RR rigid body rotation and its rate of change and is independent of the stretch. If we consider a deformation comprising of rigid body rotation only, as we did in Section 3.6.1, or if the stretch is negligibly small, then Equation (3.48) simply reduces to ˙ T W = Ω = RR

(3.49)

as we saw in Equation (3.44). In general, the angular velocity tensor and continuum spin are not the same; Equation (3.48) shows that they differ depending on the stretch, U . Both W and Ω are important when considering objective stress rates, as we shall see in Section 3.8. We will look at one further simple example in which we examine in particular the rate of deformation and the continuum spin; that of uniaxial stretch with no rigid body rotation. 3.6.3

Uniaxial stretch

We considered the uniaxial elongation of a rod lying along the Y -direction earlier (see Fig. 3.4) for which we obtained the deformation gradient, assuming purely plastic deformation and the incompressibility condition, in terms of the current, l, and original, l0 , rod lengths as ⎛ −1/2 ⎞ l 0 0 ⎜ l ⎟ ⎜ 0 ⎟ ⎜ ⎟ l ⎜ ⎟. F =⎜ 0 0 ⎟ l0 ⎜ ⎟ −1/2 ⎠ ⎝ l 0 0 l0

Velocity gradient, rate of deformation, and continuum spin

65

We will now determine the rate of deformation and continuum spin for the case of uniaxial stretch. Differentiating the deformation gradient gives ⎛ ⎞ 1 l −3/2 1 ˙ l 0 0 ⎜− ⎟ ⎜ 2 l0 ⎟ l0 ⎜ ⎟ ˙ l ⎜ ⎟ F˙ = ⎜ ⎟ 0 0 ⎜ ⎟ l0 −3/2 ˙ ⎟ ⎜ ⎝ l⎠ 1 l 0 0 − 2 l0 l0 and

F −1

⎛ 1/2 l ⎜ ⎜ l0 ⎜ ⎜ =⎜ 0 ⎜ ⎜ ⎝ 0

⎞ 0 −1 l l0 0

⎟ ⎟ ⎟ ⎟ 0 ⎟ ⎟ 1/2 ⎟ ⎠ l 0

l0

so that the velocity gradient is ⎛ ⎞ 1 l −1 l˙ 0 0 ⎜− ⎟ l0 ⎜ 2 l0 ⎟ ⎜ ⎟ ˙ l −1 l ⎜ ⎟ −1 ˙ L = FF = ⎜ ⎟= 0 0 ⎜ ⎟ l0 l0 ⎜ −1 ˙ ⎟ ⎝ 1 l l⎠ 0 0 − 2 l0 l0

⎛ 1 ⎜− 2 l˙ ⎜ ⎜0 l⎜ ⎝ 0

0 1 0

⎞ 0 ⎟ ⎟ 0 ⎟ ⎟. 1⎠ − 2

This is a symmetric quantity and therefore equal to the rate of deformation. In addition, its antisymmetric part is zero so that the continuum spin is zero. Formally, ⎞ ⎛ 1 −2 0 0 ˙ 1 l D = (L + LT ) = ⎝ 0 1 0 ⎠ , 2 l (3.50) 0 0 − 21 1 W = (L − LT ) = 0. 2 There is, therefore, no rigid body rotation occurring; just stretch. Let us look at the rate of deformation for this case of uniaxial stretch. For uniaxial stretch in the Y -direction, the true plastic strain components are given by εyy = ln

l , l0

1 εxx = εzz = − εyy 2

66

Large deformations and continuum mechanics

so that the strain rates are l˙ 1 l˙ ε˙ xx = ε˙ zz = − and ε˙ xy = ε˙ yz = ε˙ zx = 0. ε˙ yy = , l 2l Examination of the components of the deformation gradient in (3.50) shows, therefore, that D, for this case, can be rewritten ⎛ ⎞ ε˙ xx 0 0 D = ⎝ 0 ε˙ yy 0 ⎠ . (3.51) 0 0 ε˙ zz For uniaxial stretch, therefore, in the absence of a rigid body rotation, it can be seen that the rate of deformation is identical to the true strain rate. This is not generally the case; it happens to be so for this example because there is no rigid body rotation. However, the example gives us a reasonable feel for what kind of measure the rate of deformation is. We now return to the consideration of elastic–plastic material behaviour under large deformation conditions. We will consider cases in which the elastic strains, while not negligible, can always be assumed to be small compared with the plastic strains.

3.7

Elastic–plastic coupling

Consider now an imaginary lump of material in the undeformed conﬁguration, shown in Fig. 3.6. The material contains a line vector, dX. As before, after deformation F

Initial configuration

Current configuration

Z dX

dx x

X x

O

Fe Fp X dp Y

Intermediate, stress-free, configuration

Fig. 3.6 Schematic diagram showing an element of a material in the initial and current conﬁgurations and in the intermediate, stress-free, conﬁguration.

Elastic–plastic coupling

67

to the deformed or current conﬁguration, the line vector is transformed to dx. The transformation mapping of dX to dx is, of course, the deformation gradient, F . We now introduce what is called the intermediate conﬁguration. In transforming from the initial to deformed conﬁguration, the line vector dX has undergone elastic and plastic deformation. The intermediate conﬁguration is that in which line vector dx has been unloaded to a stress-free state; this is an imaginary state corresponding to one in which dX in the undeformed conﬁguration has undergone purely plastic deformation to become dp in the intermediate conﬁguration. The transformation mapping of dX to dp is the plastic deformation gradient so that dp = F p dX and the plastic deformation gradient is deﬁned as ∂p . (3.52) ∂X In the current conﬁguration dp is deformed into dx by the elastic deformation so that Fp =

dx = F e dp and the elastic deformation gradient is deﬁned as Fe =

∂x . ∂p

(3.53)

We may then write dx = F e dp = F eF p dX so that F = F eF p .

(3.54)

This is the classical multiplicative decomposition of the deformation gradient into elastic and plastic parts, due to Erastus Lee. Note that for general inhomogeneous plastic deformation, unloading a body will not generally lead to uniform zero stress; rather a residual stress ﬁeld exists. Considering a ﬁnite number of material points within a continuum, at each point an unstressed conﬁguration can be obtained, but F p and F e are, strictly, no longer pointwise continuous. Within the context of a ﬁnite element analysis, however, in which a discretization is necessary and the discontinuity of stress and strain resulting from the discretization is the norm, this is not a problem. In addition, note that the intermediate conﬁguration described by p is, in general, not uniquely determined since an arbitrary rigid body rotation can be superimposed on it, still leaving it unstressed. In Equation (3.54), both the elastic and plastic deformation gradients may contain both stretch and rigid body rotation.

68

Large deformations and continuum mechanics

However, in order to overcome the uniqueness problem, often, by convention, all the rigid body rotation is lumped into the plastic deformation gradient, F p , such that the elastic deformation gradient, F e , includes stretch only (no rigid body rotation). As a result, F e is written Fe = Ve

(symmetric stretch)

and so F p = V pR in which R is the equivalent total rigid body rotation. With this convention, let us now look at the velocity gradient and address the decomposition of the elastic and plastic rates of deformation. 3.7.1

Velocity gradient and elastic and plastic rates of deformation

We will now determine the velocity gradient in terms of the elastic and plastic deformation gradient decomposition given in (3.54). The velocity gradient is given by ∂ p e (F eF p )(F eF p )−1 = (F eF˙ + F˙ F p )F p−1F e−1 ∂t e p e p = F˙ F e−1 + F eF˙ F p−1F e−1 = V˙ V e−1 + V e F˙ F p−1 V e−1 .

˙ −1 = L = FF

Now, e Le = V˙ V e−1 = D e + W e p Lp = F˙ F p−1 = D p + W p

so L = Le + V e Lp V e−1 = D e + W e + V e D p V e−1 + V e W p V e−1 .

(3.55)

Now, D = sym(L)

W = asym(L).

Therefore, using Equation (3.55), D = D e + sym(V e D p V e−1 ) + sym(V e W p V e−1 )

(3.56)

W = W e + asym(V e D p V e−1 ) + asym(V e W p V e−1 ).

(3.57)

and In general, therefore, we see from (3.56) the result that the elastic and plastic rates of deformation are not additively decomposed, that is, D = D e + D p .

Objective stress rates

69

This is unlike the additive decomposition of elastic and plastic strain rates for the case of small deformation theory, given in Equation (2.1). However, if the elastic strains are small, then V e = V e−1 ≈ I . Also, sym(D P ) = D P , sym(W P ) = 0, since rate of deformation and spin are symmetric and antisymmetric, respectively. Hence, for small elastic stretches (V e ≈ I ), from Equations (3.56) and (3.57), D = De + DP

(3.58)

W = W e + W P.

(3.59)

and

This is an important and well-known result and we will shortly see that Equation (3.58) is often used in the implementation of plasticity models into ﬁnite element code. The plastic rate of deformation, D p , like the plastic strain rate in small strain theory, is speciﬁed by a constitutive equation. Often, in ﬁnite element implementations, the total rate of deformation, D, is known such that if D p is speciﬁed by a constitutive equation, then D e can be determined using (3.58) so that the stress rate may be determined using Hooke’s law. Once we know the stress rate, we can integrate over time to determine stress. This brings us to the ﬁnal step in our brief examination of continuum mechanics. We need to address stress rate and how to determine it in a material undergoing rigid body rotation with respect to a ﬁxed coordinate system. We will do this in Section 3.8, and then summarize the most important steps required in going from knowledge of deformation to determination of stress, before introducing ﬁnite element methods in Chapter 4.

3.8

Objective stress rates

The primary focus of this section is stress rate, but before looking at this, we need to look at what is called material objectivity. We will start not by considering stress rate, but by something more familiar; transformation of stress.

3.8.1

Principle of material objectivity or frame indifference

Consider the transformation of the stress tensor, σ , which undergoes a rotation through θ relative to the (XYZ) coordinate system. The stress transformation equations, or Mohr’s circle, tell us that the transformed stresses, σ , with respect to the

70

Large deformations and continuum mechanics

Reference plane ∆F n ∆A

u

s∆ A τ∆ A

Body

Fig. 3.7 Schematic diagram showing a body cut by a plane with normal n generating an area of intersection of A, subjected to resultant force F .

(XYZ) coordinate system become

σXX = σXX cos2 θ + 2σXY sin θ cos θ + σY Y sin2 θ

σY Y = σXX sin2 θ − 2σXY sin θ cos θ + σY Y cos2 θ

σXY

= (σY Y − σXX ) sin θ cos θ + σXY

(cos2 θ

(3.60)

− sin θ). 2

The last of the three equations enables us to determine the direction of the principal axes, relative to the applied stress direction, and of course, the principal stresses.

= 0 so that It does this because along the principal directions, σXY tan 2θ =

σXY . σXX − σY Y

(3.61)

We will look at an alternative way of dealing with stress (and indeed, other tensor quantities such as strain) transformation. In order to do this, we need to introduce the stress vector or surface traction. 3.8.1.1 The stress vector or traction. Figure 3.7 shows a lump of material, making up a body which has been cut by a plane with normal direction n, with an inﬁnitesimal area of intersection, A. Under uniform stress state, the resultant force acting on the area A is F . The stress vector acting on the area A is deﬁned by F t= . (3.62) A A→0 By deﬁnition, t is a vector quantity with normal, σ , and shear, τ , components, as shown in Fig. 3.7. We will now look at how the stress vector, t, on a particular plane with normal n is related to the stress tensor, σ . Consider the three orthogonal planes shown in Fig. 3.8(a) and the resulting plane ABC, reproduced in Fig. 3.8(b).

Objective stress rates (a)

y B sxy

tx sxz

szz

szy

tz

(b) s

szx

B

t

sxx n

z

71

A syy syz

syx

C

x

τ

A C

ty

Fig. 3.8 Schematic diagram showing (a) the stress vectors acting on three orthogonal planes with components in the x-, y-, and z-directions shown and (b) the resultant stress vector acting on plane ABC which has normal n, with components n = [nx ny nz ]T .

On each of the orthogonal planes in Fig. 3.8(a), a stress vector acts. For example, on plane ‘x’, that is, the plane orthogonal to the x-direction, the stress vector is t x . The stress vectors acting on the three orthogonal planes have components given by ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ σzx σxx σyx ⎣ ⎦ ⎣ ⎣ ⎦ t x = σxy , t x = σzy ⎦ . (3.63) t y = σyy , σzz σyz σxz The convention is that on plane ‘x’, the stress components are labelled σxx in the x-direction, σxy in the y-direction, and so on. If the area of plane ABC is A, then the areas of the three orthogonal planes are given by ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ 0 0 1 Ax = ⎣0⎦ · An = Anx , Ay = ⎣1⎦ · An = Any , Az = ⎣0⎦ · An = Anz . 0 1 0 (3.64a) By consideration of equilibrium, the resultant force on plane ABC must be balanced by the forces on the three orthogonal planes so that ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ σxx σyx σzx ⎦ ⎦ ⎣ ⎣ ⎣ tA = t x Ax + t y Ay + t z Az = σxy Anx + σyy Any + σzy ⎦ Anz . (3.64b) σxz σyz σzz Therefore ⎡

⎤ ⎡ ⎤ ⎡ ⎤ ⎛ σxx σyx σzx σxx ⎣ ⎦ ⎦ ⎦ ⎣ ⎣ ⎝ t = σxy nx + σyy ny + σzy nz = σyx σxz σyz σzz σzx

σxy σyy σzy

⎞⎡ ⎤ nx σxz ⎠ ⎣ σyz ny ⎦ σzz nz

(3.65)

72

Large deformations and continuum mechanics

remembering that for reasons of moment, or rotational equilibrium, the stress tensor is symmetric so that σxy = σyx etc. Equation (3.65) can be written in a simple way as t = σ n.

(3.66)

3.8.1.2 Transformation of stress. Let us now return to the problem of transformation of stress. Consider the stress vector, t, acting on a surface with normal n. At the point of interest, the stress is fully described by the tensor σ . Under some rotation, R, the stress vector t is transformed to t acting on a plane with normal n , and similarly, the stress σ is transformed to σ such that t = σn

and

t = σ n .

Under rotation, R, the vectors t and n transform according to t = Rt which give Combining these gives but

and

t = Rσ n and

n = Rn n = R T n .

t = RσR T n

t = σ n

so that ﬁnally

σ = RσR T . (3.67) We see, therefore, that unlike a vector, the stress tensor, σ , transforms according to Equation (3.67). To see what this means in detail, let us consider the two-dimensional transformation giving Equations (3.60). The rotation matrix, R, corresponding to the rotation of θ is cos θ − sin θ R= sin θ cos θ so that cos θ sin θ cos θ − sin θ σxx σxy

σ = . − sin θ cos θ sin θ cos θ σxy σyy Multiplying these equations will give Equation (3.60). The stress transformation equations, or Mohr’s circle representation, are beautifully and succinctly summarized, therefore, in Equation (3.67). This equation also tells us how other tensor quantities (such as strain, for example) transform. More formally, a tensor, A, is said to be frame indifferent or objective if it rotates according to the following: A = QAQT .

(3.68)

Comparing Equation (3.67) with (3.68) shows that the Cauchy stress tensor is objective. Let us consider a simple example to understand what is meant by objective.

Objective stress rates

3.8.2

73

Stressed rod under rotation: co-rotational stress

Consider a rod initially lying parallel to the Y -axis, of cross-sectional area A, under constant, axial, force P , shown schematically in Fig. 3.9(a). In this conﬁguration, with respect to the XY coordinate system, the stresses in the rod are: P , σXY = 0. A A co-rotational (xy) coordinate system has been introduced which rotates with the rod. The stresses in the rod relative to the co-rotational (xy) coordinate system initially are, similarly, P σxx = 0, σyy = , σxy = 0. A The rod undergoes a rotation of θ as shown in Fig. 3.9(b), relative to the (XY ) coordinate system. With respect to the co-rotational system, the rod is subjected to an unchanging stress in the y-direction of P/A; all other stress components remain zero. The stresses σXX = 0,

(a) Y P/A

σY Y =

s XX = 0 s Y Y = P/A s XY = 0

s XX ≠ 0 s YY ≠ 0 s XY ≠ 0

(b) Y u P/A

y

x y x

P/A

P/A

X

X

(c) Y

s X X = P/A s YY = 0 s XY = 0 x P/A

y

P/A

X

Fig. 3.9 A rod of cross-sectional area A undergoing rigid body rotation while subjected to axial force P (a) in the initial conﬁguration, (b) having rotated through angle θ, and (c) after rotating through 90◦ showing the changing stresses with respect to the material (XY) reference frame.

74

Large deformations and continuum mechanics

in the rod, however, when measured with respect to the material (XY) reference frame can be seen to change. For example, when the rod has rotated through 90◦ as shown in Fig. 3.9(c), it lies parallel to the X-axis so that now, the stresses with respect to the material (XY) reference frame are P σXY = 0. , σY Y = 0, A They are, therefore, completely different to what they were in the initial state shown in Fig. 3.9(a). However, the stresses relative to the co-rotational system are as before; that is, P σxx = 0, σxy = 0. σyy = , A The stresses relative to the co-rotational coordinate system, which we shall designate by σ , are related to those relative to the material (XY ) coordinate system, which we shall designate by σ , by σ = RσR T (3.69) σXX =

in which R is just the rotation matrix. σ is called an objective or co-rotational stress because with respect to the co-rotational reference frame (and indeed, the material undergoing the rotation), its stress state has not changed; it has simply rotated. Note that the co-rotational stress, given in Equation (3.69) follows the requirement of objectivity given in Equations (3.67) and (3.68). The objective stress, therefore, results from the constitutive response of the material; it is independent of orientation and derives from the material response rather than the rigid body rotation. Before addressing stress rate and its objectivity, we will ﬁrst look at the objectivity, or otherwise, of a number of other important quantities in large deformation kinematics. 3.8.3

Objectivity of deformation gradient, velocity gradient, and rate of deformation

Consider the deformation gradient F . dx = F dX.

(3.70)

After a transformation, Q, the quantities in Equation (3.70) become dx , F , and dX

so that dx = F dX . (3.71) Now,

dx = Q dx = QF dX

and dX remains unchanged under deformation, by deﬁnition, so that dX = dX.

Objective stress rates

75

Therefore, from Equation (3.71), F = QF .

(3.72)

F is, therefore, in fact objective and behaves like a vector because it is what is called a two point tensor, that is, only one of its two indices is in the spatial coordinate, x. We will now look at the objectivity of the velocity gradient, the rate of deformation, and the continuum spin. Differentiating Equation (3.72) gives

˙ + QF˙ F˙ = QF

so that

˙ + QF˙ )F −1 Q−1 = QQ ˙ T + QFF ˙ −1 QT L = F˙ F −1 = (QF

and

˙ T + QLQT . L = QQ

(3.73)

Comparing with the requirement for objectivity in Equation (3.68), therefore, shows that the velocity gradient is not objective. The transformed velocity gradient, L , from Equation (3.73) can be written L =

1 1 ˙ −1 . Q(L + LT )QT + Q(L − LT )QT +QQ 2 2 Symmetric

(3.74)

Antisymmetric

˙ T is antisymmetric. Therefore, from (3.74), From Equation (3.46) we see that QQ D = sym(L ) = and

1 Q(L + LT )QT = QDQT 2

˙ −1 . W = asym(L ) = QWQT + QQ

(3.75)

Therefore, the deformation rate, D, is objective, but the continuum spin, W , is not. It is useful to ask whether this is important or not. In Sections 3.8.1 and 3.8.2, we examined the objectivity of the Cauchy stress and found that it is indeed objective. The Cauchy stress is, therefore, a quantity for which the properties are independent of the reference frame. This is very important in the development of constitutive equations. An equation which relates elastic strain to stress, for example, must be independent of the reference frame in which the relationship is used; in other words, the constitutive equation must provide information about the material response which is independent of rigid body rotation. The same holds for constitutive equations relating rate of plastic deformation (which we have just shown to be objective) to Cauchy stress (also objective), or the constitutive equation relating stress rate to elastic rate of deformation. In fact, plasticity

76

Large deformations and continuum mechanics

problems, especially within the context of ﬁnite element implementations, are often formulated in rate form. It is therefore necessary for us to address stress rate and, in particular, to examine whether stress rate is objective or otherwise. It turns out that there are many measures of objective stress rate, and we will focus on one in particular; the Jaumann stress rate.

3.8.4

Jaumann stress rate

We will examine, ﬁrst, a rather contrived problem in order to get a physical feel for the meaning of the Jaumann stress rate. We will then look more generally at the objectivity of this stress rate, and ﬁnish by looking at a simple example. Consider again a rod under axial stress σ , shown in Fig. 3.10(a). The stress tensor, with respect to the material axes is σt . During a time increment of t, the rod undergoes a rigid body rotation such that at time t + t, the rod lies as shown in Fig. 3.10(b) in which the co-rotational reference axes (xy) now coincide with the material reference axes (XY ).

(a) Y

(b) Y

∆u

0 0 0 sRt+ ∆t = 0 s 0 0 0 0

s

s y

x y

x s s

Time = t Time = t + ∆t

X

X s + ∆s

(c) Y

y

0 st + ∆t = 0 0

0 s + ∆s 0

0 0 0

x s + ∆s Time = t + ∆t X

Fig. 3.10 A rod under axial stress, σ , undergoing rigid body rotation (a) at a time t, (b) at a time t + t having gone through incremental rotation R (corresponding to angle θ about the Z-direction) and (c) at the same time t + t but having also undergone stress increment σ .

Objective stress rates

77

The stress tensor σ with respect to the co-rotational reference frame is ⎞ ⎛ 0 0 0 σ t = ⎝0 σ 0⎠ , 0 0 0 which is obtained from

σt = Rσt R T ,

(3.76)

where R is the incremental rigid body rotation. Following the rigid body rotation, the rod is subjected to an additional axial stress, σ , shown in Fig. 3.10(c), so that the ﬁnal stress tensor, with respect to the co-rotational frame (and the material frame since they are coincident at time t + t) is ⎞ ⎛ 0 0 0

σt+t = ⎝0 σ + σ 0⎠ . 0 0 0 The Cauchy stress increment with respect to the co-rotational frame may be written approximately, using Equation (2.99), as σ = [2GD e + λTr(D e )I ]t,

(3.77)

where we have used the rate of elastic deformation in place of the elastic strain rate. The stress increment results, therefore, purely from the material’s constitutive response and is co-rotational. We may then write the co-rotational stress tensor at time t + t as the sum of (3.76) and (3.77) to give

σt+t ≡ σt+t = Rσt R T + [2GD e + λTr(D e )I ]t.

(3.78)

In order to investigate this further, let us consider the case in which the incremental rigid body rotation, R, is small. We may then approximate the rotation matrix as R = exp[ˆr ] ≈ I + ˆr in which ˆr is the associated antisymmetric tensor which is approximately given by Wt (a full explanation for this can be found, e.g., in Belytschko et al., 2000). Substituting into (3.78) then gives σt+t = (I + Wt)σt (I + Wt)T + [2GD e + λTr(D e )I ]t = σt + σt W Tt + W σt t + W σt W Tt 2 + [2GD e + λTr(D e )I ]t so that σt+t − σt = σt W T + W σt + σt W σt t + [2GD e + λTr(D e )I ]. t

78

Large deformations and continuum mechanics

Now, both σt and σt+t are given with respect to the material reference frame so that taking the limit, and letting t → 0, gives us the material stress rate, σ˙ as σ˙ = σt W T + W σt + 2GD e + λTr(D e )I and as W is antisymmetric (we saw earlier that this means W T = −W ), we obtain σ˙ = W σt − σt W + 2GD e + λTr(D e )I . We can rewrite this as

∇

σ˙ = σ +W σt − σt W , where

∇

σ = 2GD e + λTr(D e )I .

(3.79) (3.80) (3.81)

∇

σ in Equations (3.80) and (3.81) is called the Jaumann stress rate and it is the stress rate that results purely from the constitutive response of the material and not from rigid body rotation. It is, therefore, as we shall see in Section 3.8.4.1, an objective stress rate. We may therefore use it in constitutive equations such as (3.81) in which both the Jaumann stress rate and the elastic rate of deformation are objective quantities. The material stress rate, σ˙ however, does depend upon rigid body rotation. σ˙ is the Cauchy stress rate with respect to the material reference frame; that is, in Figs 3.9 and 3.10, σ˙ gives the stress rate with respect to the material (XY ) axes. In ﬁnite element simulations, we are ordinarily interested in the stresses with respect to the material axes. Equation (3.80) is therefore important in that it enables us to determine the required stresses from knowledge of the material’s constitutive response given by the Jaumann stress rate in (3.81). It is useful to remember that the stresses, σt , in Equation (3.80), are also given with respect to the material reference frame. 3.8.4.1 Objectivity of Jaumann stress rate. Let us now show that the Jaumann stress rate is objective. We saw earlier that a quantity A is said to be objective if it transforms according to (3.68), that is A = QAQT and that the Cauchy stress transforms in this way (σ = QσQT ). Differentiating the stress with respect to time gives T T ˙ ˙ T ) = QσQ ˙ ˙ T. ˙ T + σQ ˙ T + QσQ σ˙ = QσQ + Q(σQ + QσQ

(3.82)

We see from Equation (3.82) that the material rate of Cauchy stress is not objective (even though the stress itself is) since it does not transform according to (3.68). We saw in Section 3.8.3, Equation (3.75) that ˙ −1 . W = QWQT + QQ

Objective stress rates

79

Rearranging and remembering that Q is orthogonal gives

so that since both W and gives

W

˙ = W Q − QW Q

(3.83)

˙ T = −QT W + WQT Q

(3.84)

are antisymmetric. Substituting (3.83) and (3.84) into (3.82)

˙ T + Qσ WQT − QσQT W σ˙ = W QσQT − QW σQT + QσQ so that

σ˙ = Q(σ W − W σ + σ˙ )QT + W QσQT − QσQT W .

(3.85)

Substituting for QσQT = σ into (3.85) gives σ W − W σ + σ˙ = Q(σ W − W σ + σ˙ )QT .

(3.86) ∇

Equation (3.86) therefore shows that the Jaumann stress rate, σ , satisﬁes the requirement for objectivity in Equation (3.68), where ∇

σ = σ˙ + σ W − W σ .

(3.87)

There are objective stress rates other than that of Jaumann. Details of these may be found in many of the more advanced text books on continuum mechanics, and in particular, that of Belytschko et al. (2000). 3.8.4.2 Example of Jaumann stress rate for a rotating rod. We will conclude Section 3.8.4 with a simple example of a rotating rod under constant, uniaxial stress. We refer back to Fig. 3.9(b) which shows the rotating bar at an instant at which it makes an angle θ with the vertical. It is subject to a constant, uniaxial stress of P/A at all times. This, of course, gives a constant co-rotational stress (with respect to co-rotational xy-axes) of ⎞ ⎛ 0 0 σ = ⎝ (3.88) P ⎠. 0 A The stresses with respect to the material (XY ) axes, however, change with the rotation, as shown in Fig. 3.9(a)–(c). This means that there is a rate associated with each stress component which also changes with the rotation. We will now determine the stresses in the rod with respect to the material axes as it rotates. We will do this in two ways; ﬁrst, we will set up the problem in rate form and integrate to obtain the stresses and second, use the standard method for transformation of stress using Equation (3.67) (or equivalently, Mohr’s circle).

80

Large deformations and continuum mechanics ∇

We may obtain the objective, or co-rotational stress rate, σ , simply by differentiating (3.88) with respect to time. As the co-rotational stress is always constant, its derivative is zero, so ⎞ ⎛ 0 0 ∂ ⎝ ∇ σ = P ⎠ = 0. ∂t 0 A The stress rate with respect to the original conﬁguration, σ˙ , is given by rearranging (3.87) ∇

σ˙ = σ − σ W + W σ = W σ − σ W .

(3.89)

If there is no rotation, then W = 0 and (3.89) tells us that the stress rates with respect to the material axes are also zero. However, the rod is rotating, with constant angular speed θ˙ . We showed for this case, Equation (3.41), that this results in a continuum spin given by 0 −1 W = θ˙ . (3.90) 1 0 The stresses with respect to the material axes may be written σXX σXY σ = . σXY σY Y

(3.91)

Substituting (3.90) and (3.91) into (3.89) gives σ − σ −2σ XY XX Y Y σ˙ = θ˙ . σXX − σY Y 2σXY That is

dσXX dσY Y = −2θ˙ σXY ≡ − dt dt

and

(3.92)

dσXY = θ˙ (σXX − σY Y ). (3.93) dt Equation (3.92) gives σXX = −σY Y +k where k is just a constant. The initial conditions are σXX (0) = 0, σY Y (0) = P/A, σXY (0) = 0 so that k = P/A. Differentiating (3.93) and substituting into (3.92) and using k = P/A gives d2 σXX P = +4θ˙ 2 σXX = 2θ˙ 2 . A dt 2 This has general solution σXX = A sin 2θ + B cos 2θ +

P , 2A

Summary

81

˙ so that with the initial conditions, the full solution is where θ = θt, P P P σXX = sin2 θ, (3.94) σY Y = cos2 θ, σXY = sin θ cos θ. A A A We see, therefore, that the stresses with respect to the material reference frame change correctly with angle θ . For example, when θ = 0, σXX = 0, σY Y = P/A, σXY = 0, and when θ = π/2, σXX = P/A, σY Y = 0, σXY = 0. Finally, we will determine the same stresses using the stress transformation equation in (3.67). That is, σ = RσR T ↑ ↑ (x, y) (X, Y ) reference reference so that the stresses in the material (XY ) reference are given by ⎛ ⎞ 0 0 P cos θ sin θ ⎝ cos θ − sin θ sin2 θ σ = = P⎠ − sin θ cos θ sin θ cos θ A sin θ cos θ 0 A which just gives the expressions in Equation (3.94).

3.9

sin θ cos θ , cos2 θ

Summary

Before leaving the kinematics of large deformations, we will summarize some of the important steps required in going from knowledge of deformation through to the determination of stresses for an elastic–plastic material undergoing large deformations. This is often required in the implementation of plasticity models into ﬁnite element code so it is something we shall return to later. We assume that any deformation taking place is such that the stretches due to elasticity are small compared with those for plasticity so that the additive decomposition of rate of deformation given in Equation (3.58) holds. We also assume full knowledge of the deformation gradient, F and its rate, F˙ . The steps required in determining stresses are then as follows. 1. Determine the velocity gradient ˙ −1 . L = FF 2. Determine the rates of deformation and continuum spin 1 D = sym(L) = (L + LT ), 2 1 W = asym(L) = (L − LT ). 2

82

Large deformations and continuum mechanics

3. The rate of plastic deformation is speciﬁed by a constitutive equation. For example, from Chapter 2, for combined isotropic and kinematic hardening with power law dependence of effective plastic strain rate on stress, we have in the current conﬁguration 1/m σ − x

3 J (σ − x ) − r − σy p D = . 2 K J (σ − x ) 4. Determine the rate of elastic deformation De = D − Dp. 5. Determine the Jaumann stress rate using the tensor form of Hooke’s law, Equation (3.81), from the rate of elastic deformation ∇

σ = 2GD e + λTr(D e )I . 6. Determine the material rate of stress using (3.80) ∇

σ˙ = σ +W σ − σ W . 7. Use a numerical technique to obtain the stresses with respect to the material reference frame by integrating σ˙ . We will address all of these steps in some detail in later chapters.

Further reading Belytschko, T., Liu, W.L., and Moran, B. (2000). Non-linear Finite Elements for Continua and Structures. John Wiley & Sons Inc, New York. Khan, A.S. and Huang, S. (1995). Continuum Theory of Plasticity. John Wiley & Sons Inc, New York. Lubarda, V.A. (2002). Elastoplasticity Theory. CRC Press, Florida, USA. Simo, J.C. and Hughes, T.J.R. (1997). Computational Inelasticity. Springer-Verlag, Berlin.

4. The ﬁnite element method for static and dynamic plasticity

4.1

Introduction

There are few practical problems in plasticity which can be solved analytically. This is usually because of irregular geometry and/or complicated boundary and loading conditions. Computational mechanics, and in particular, the ﬁnite element method, enables the approximate solution of these types of problems. The important requirements of equilibrium, and compatibility, together with a material’s constitutive response, enable solutions to be obtained subject to the satisfaction of initial and boundary conditions. Satisfying the requirements of equilibrium, compatibility, constitutive equations, and boundary conditions is essential for the solution of any solid mechanics problem. Within the ﬁnite element method, the body under consideration is discretized into a ﬁnite number of elements and nodes, with the latter each having a speciﬁed number of degrees of freedom. The ﬁnite element model representing the body therefore contains a ﬁnite number of degrees of freedom and the implication is that the requirement for equilibrium cannot be satisﬁed exactly at every point in the continuum (in what is called the strong sense). Instead, within the ﬁnite element technique, a weak formulation of equilibrium is used in which global equilibrium for the body as a whole is imposed even though this does not necessarily ensure pointwise equilibrium. Further details of strong and weak formulations are available in texts that are more specialized. A weak formulation can be obtained by consideration of the principle of virtual work, which appears in many text books, but here, we shall use Hamilton’s principle. The advantage, as we shall see, is that the equilibrium equations of motion can be obtained in a fully uniﬁed manner, for both quasi-static and dynamic problems, and that the boundary conditions for the problem are also obtained. We shall use Hamilton’s principle to obtain the equations of motion (and boundary conditions) for a number of well known discrete and continuous systems. In this way, we aim to develop a good physical feel for what the principle is doing before addressing more complicated ﬁnite element applications.

84

Finite element method

We introduce Hamilton’s principle in Section 4.2. A reasonable knowledge of vector calculus is useful, but the important results are not impenetrable without it! Unfamiliar readers may like to skip on to the introduction to the ﬁnite element method in Section 4.3. Here, in keeping with the aims of this book, we address ﬁrst a simple one-dimensional rod element subjected to elastic deformation alone and then very brieﬂy look at element assemblage and some other ﬁnite element types. We then return to elastic–plastic problems and address plasticity in a one-dimensional rod element.

4.2

Hamilton’s principle

Hamilton’s principle, which results from conservation of energy, is one of the most general principles of mechanics. It provides a means for ﬁnding the equilibrium equations (equations of motion) of a dynamical system by determining the stationary value of a scalar integral. The principle states that the variation of the kinetic and potential energy plus the variation of the work done by non-conservative (external) forces acting during any time interval t1 to t2 must be zero. We will shortly see what is meant by variation, and of course, non-conservative implies forces that cannot be described by the change in a potential energy function (as can strain energy, for example), which are not already included in the potential energy term. Let the total kinetic energy of the system be T , the potential energy of the system be U , and the work done by non-conservative forces be W . The Lagrangian, L, is deﬁned as L=T −U +W (4.1) and the J-integral is deﬁned as t2 J = L dt = t1

t2

t1

(T − U + W ) dt.

(4.2)

Hamilton’s principle states that the ﬁrst variation (denoted by δ) of J is zero thus t2 t2 δL dt = δ(T − U + Wnc ) dt = 0. (4.3) δJ = t1

t1

In other words, the motion of a system between speciﬁed, realizable initial, and ﬁnal conditions at times t1 to t2 is such that the average value of L relative to any dynamical path compatible with the physical constraints has a stationary value. An illustration of such a motion is given in Fig. 4.1 for a single degree of freedom system (SDOF). Generally, the kinetic energy, potential energy, and work of non-conservative forces depend on some function (e.g. displacement, temperature, etc.) of time y(t) which

Hamilton’s principle

x

85

Two dynamical paths compatible with constraints (the difference between trajectories is dx)

dx

x(t ) x(t ) t1

t2

t

Fig. 4.1 Two dynamical paths subjected to having the same state at times t1 and t2 .

can be expressed as follows J =

t2

t1

L dt =

t2

t1

L(y, y , t) dt

(4.4)

in which y is just y˙ = dy/dt. Hamilton’s principle tells us that the dynamical path, y(t), is that which leads to a stationary value of J . Let us now look at how Equation (4.4), called a functional, may be minimized by use of the calculus of variations. Let y = y(t) be the actual minimizing curve (as distinct from any admissible curve) and let Y (t) = y(t) + εη(t) (4.5) be the family of comparison curves, where η(t) is an arbitrary function subjected to the constraint that η(t1 ) = η(t2 ) = 0 (4.6) and ε is an arbitrary parameter. The corresponding J integral is t2 L(Y, Y , t) dt J¯(ε) = t1

and its variation with respect to ε is t2 ∂L ∂Y

∂L ∂Y ∂ ¯ J (ε) = + dt. ∂ε ∂Y ∂ε ∂Y ∂ε t1

(4.7)

(4.8)

For ε = 0, and using (4.5), this variation yields by integrating by parts, as t2 t2 t2 ∂L

∂L t2 ∂L ∂L d ∂L ∂ ¯ J (0) = η + η dt = η dt + η − η dt

∂ε ∂y ∂y ∂y dt ∂y

t1 t1 ∂y t1 t1 t2 d ∂L ∂L ∂L t2 − η dt + η , = ∂y dt ∂y

∂y t1 t1

86

Finite element method

which for η(t1 ) = η(t2 ) = 0 yields t2 ∂ ¯ d ∂L ∂L J (0) = − η dt. ∂ε ∂y dt ∂y

t1

(4.9)

Therefore, the necessary condition for minimization of J is ∂ ¯ ∂ ¯ J (0) = J (ε) = 0. ∂ε ∂ε Hence,

t2

t1

(4.10)

∂L d ∂L η dt = 0. − ∂y dt ∂y

Since η is arbitrary, it follows that ∂L d ∂L − = 0, ∂y dt ∂y

(4.11)

which is known as Euler–Lagrange equation and which must be satisﬁed for J to have a minimum. If the function y(t) is replaced by y + δy where δy is the variation of y such that δy(t1 ) = δy(t2 ) = 0,

(4.12)

then it follows using Taylor’s theorem that t2 ∂L ∂L

J (y + δy) = J (y) + δy + (δy) dt ∂y ∂y t1 t2 2 ∂ L 2 ∂ 2L ∂ 2 L 2 1

δy + 2 δy(δy) + 2 (δy ) dt + 2! t1 ∂y∂y

∂y 2 ∂y 3 t2 ∂ 1 ∂ δy + δy L(y, y , t) dt + · · · + (4.13) 3! t1 ∂y ∂y since ∂F ∂F ∂F +s +t ∂x ∂y ∂z 2 ∂ ∂ ∂ 1 r +s +t F (x, y, z) + · · · . + 2! ∂x ∂y ∂z

F (x + r, y + s, z + t) ≈ F (x, y, z) + r

The quantity

δJ =

t2

t1

∂L ∂L

δy + (δy) dt ∂y ∂y

(4.14)

Hamilton’s principle

87

is called the ﬁrst variation while ∂ 2L ∂ 2 L 2 1 t2 ∂ 2 L 2

2 δy + 2 δy(δy) + 2 (δy ) dt δ J = ∂y∂y

2! t1 ∂y 2 ∂y is the second variation of J . If the ﬁrst variation is equal to zero for a particular function y(t) of the admissible class, the functional J (y) is said to have a stationary value for that particular function y. Before returning to equilibrium equations, let us look at one simple example to help understand the process of ﬁnding a stationary value. 4.2.1

Stationary value: minimizing the distance between two points

Figure 4.2 shows two points (x1 , y1 ) and (x2 , y2 ) which are joined by an inﬁnite number of possible paths, y(x). Only one is shown in the ﬁgure! Here note that y(x) is a function only of position, x, and not time. Our aim is to use the above approach to determine that path which minimizes the distance between the two points. An element of length dl lies on the path shown, and its length can be written as 2 dy 2 2 2 2 dl = dx + dy = dx 1 + dx such that

dl = (1 + y 2 )1/2 dx

and ﬁnally, we obtain the functional, or J integral as x2 J =l= (1 + y 2 )1/2 dx.

(4.15)

x1

Equation (4.15) is the functional which we wish to minimize to obtain the shortest path. We will use two approaches to do this. The ﬁrst is by obtaining directly the y

(x2, y2)

y (x) dl

dy dx

(x1, y1)

x1

x2

x

Fig. 4.2 A particular path, y(x), between two points, (x1 , y1 ) and (x2 , y2 ), and an element, dl, lying on the path.

88

Finite element method

stationary value of (4.15) and the second is to do the same by using the Euler–Lagrange Equation (4.11). The ﬁrst variation of (4.15) is given by x2 x2 1

2 1/2 (1 + y ) dx = (1 + y 2 )−1/2 δ(y 2 ) dx δJ = δ x1 x1 2 x2 = (1 + y 2 )−1/2 y δy dx. x1

Now,

dy d = (δy) δy = δ dx dx so x2 d δJ = (1 + y 2 )−1/2 y (δy) dx. dx x1 Integrating by parts gives x2 d ((1 + y 2 )−1/2 y ) δy dx δJ = [y (1 + y 2 )−1/2 δy]xx21 − dx x1 and since δy(x1 ) = δy(x2 ) = 0, and for a stationary value, we obtain x2 d ((1 + y 2 )−1/2 y ) δy dx = 0. δJ = − x1 dx Since δy is arbitrary, we obtain the differential equation d ((1 + y 2 )−1/2 y ) = 0, (4.16) dx which (unsurprisingly) has the solution y = Ax + B in which A and B are constants of integration. We see, therefore, that the process of ﬁnding the ﬁrst variation (or equivalently, the stationary value) of J , results in ﬁnding the function y(x) which minimizes the functional, J . To ﬁnish off, let us do the same thing but now using the Euler–Lagrange Equation (4.11). The functional, J , is a function of y, y , and x and from Equation (4.15) may be written as x2 J = L(y, y , x) dx,

where

L(y, y , x)

=

(1 + y 2 )1/2

x1

so the Euler–Lagrange equation becomes ∂L d ∂L − = 0. ∂y dx ∂y

(4.17)

Now, ∂L ∂L 1 = 0 and = (1 + y 2 )−1/2 2y

∂y ∂y 2 and substituting into (4.17) just gives us the differential Equation (4.16) which has the solution as before.

Hamilton’s principle

4.2.2

89

Equilibrium equations

Let us now return to Hamilton’s principle to see how it can be used to obtain equilibrium equations. For a solid elastic body, in the absence of body forces, the components of the Lagrangian can be expressed as follows: 1 T = ρ u˙ · u˙ dV , 2 1 σ : ε dV , (4.18) U= 2 t · u dA W = ∂

in which u and u˙ are the displacement and velocity vectors, ρ the density, t the stress vector, or traction, σ and ε the stress and strain tensors respectively, and ∂ and are domains of area, A and volume, V , respectively. Substituting for the stress vector, t, from Equation (3.66), and making use of the divergence theorem gives W = σ n · u dA = div [σ u] dV . (4.19) ∂

The J integral is, therefore t2 (T − U + W ) dt J = t1 t2

=

t1

1 1 ρ u˙ · u˙ dV − σ : ε dV + div [σ u] dV dt. 2 2

Taking the ﬁrst variation of J gives t2 δJ = δ(T − U + W ) dt t1 t2

1 1 2ρ u˙ · δ u˙ dV − (σ : δε + δσ : ε) dV + div [σ δu] dV dt = 2 2 t1 t2 ∂ ρ u˙ · δu dV − σ : δε dV + div [σ δu] dV dt = 0 = ∂t t1

and noting that div [σ δu] = div [σ ] · δu + σ : ∇δu and ∇δu = δε and integrating by parts gives t2 δJ = − ρ u¨ · δu dV + div σ δu dV dt t1 t2

=

t1

− ρ u¨ dV + div σ dV · δu dt = 0

90

Finite element method

so that

(−ρ u¨ + div σ ) · δu dV = 0

(4.20)

and since δu is arbitrary, −ρ u¨ + div σ = 0. These are the well-known equilibrium equations of stress analysis. If we consider quasi-static conditions, ρ u¨ = 0, and expand div σ , we obtain the more familiar expressions ⎡ ⎤ ∂σxy ∂σxx ∂σxz + + ⎢ ∂x ∂y ∂z ⎥ ⎢ ⎥ ⎢ ∂σ ∂σyy ∂σyz ⎥ ⎢ yx ⎥ + + div σ = ⎢ ⎥ = 0. ⎢ ∂x ∂y ∂y ⎥ ⎢ ⎥ ⎣ ∂σzx ∂σzy ∂σzz ⎦ + + ∂x ∂y ∂z Hamilton’s principle has therefore given us the very general form of the equilibrium equations of stress analysis. In addition, Equation (4.20) can be seen to be a statement ! of the principle of virtual work. The term (−ρ u¨ + div σ ) dV is just the residual force, r, so that the expression in (4.20) is simply δW = r · δu = 0. That is, in the course of an arbitrary, inﬁnitesimal virtual displacement, δu, from a position of equilibrium, the work done is zero. Hamilton’s principle has therefore provided us with the condition for equilibrium and, in doing so, a statement of the principle of virtual work. Before moving on to its application to ﬁnite elements, let us consider a few more examples, one for a discrete system, and two further continuous systems, in which we shall employ Hamilton’s principle to obtain the momentum balance equations for a number of simple problems. 4.2.3

Further examples of Hamilton’s principle

4.2.3.1 Discrete spring–mass problem. Consider the SDOF spring–mass system shown in Fig. 4.3. We will use Hamilton’s principle to derive the equation of motion for the mass, m. k

m

x(t )

Fig. 4.3 Simple SDOF mass and spring system.

Hamilton’s principle

91

We may write expressions for the kinetic and potential energies of the system as 1 1 T = mx˙ 2 . U = kx 2 , 2 2 The J integral may then be written, in the absence of external forces, as t2 t2 1 2 1 2 J = mx˙ − kx dt. (T − U ) dt = 2 2 t1 t1 Taking the ﬁrst variation gives t2 d 1 t2 mx˙ (δx) − kx δx dt (2mx˙ δ x˙ − 2kx δx) dt = δJ = 2 t1 dt t1 and integrating by parts, we get δJ =

[mx˙ δx]tt21

−

t2 t1

(mx¨ δx + kx δx) dt

and since δx(t1 ) = δx(t2 ) = 0, and δx is arbitrary, t2 δJ = − (mx¨ + kx) δx dt = 0 so mx¨ + kx = 0. t1

Hamilton’s principle has given us the governing equation of motion, or equilibrium equation, for the well known mass–spring problem. 4.2.3.2 Transverse vibration of a continuous beam. We shall next consider a continuous system and use Hamilton’s principle to obtain the equations of motion for it. Figure 4.4(a) shows an elastic beam undergoing bending with deﬂection, y. The bending moment variation with angle, φ, is shown in Fig. 4.4(b) assuming elastic behaviour. (b) M

(a) y

y

f+

−f −x dU =

f x

df

1 M df 2 f

Fig. 4.4 (a) An elastic beam in bending undergoing deﬂection y and rotation φ and (b) the linear variation of bending moment M with rotation φ leading to stored elastic strain energy U .

92

Finite element method

The elastic strain energy stored in an element of length dx of the beam is 1 1 ∂φ dU = M dφ ≈ M dx 2 2 ∂x and ∂y φ= ∂x so that 1 ∂ 2y dU = M 2 dx. 2 ∂x For an elastic beam, the bending moment is related to the deﬂection, y, by ∂ 2y , ∂x 2 where E is Young’s modulus and I is the second moment of area. Thus, 2 2 1 ∂ y dU = EI dx 2 ∂x 2 and ﬁnally, the potential energy for a beam of length L is 2 2 1 L ∂ y U= EI dx. 2 0 ∂x 2 The kinetic energy, in an element of length dx, of the beam, is 2 1 ∂y dT = ρA dx 2 ∂t in which A is the beam’s cross-sectional area. Hence the total system energy is 2 1 L ∂y T = ρA dx. ∂t 2 0 The work done by external forces, F (x, t) per unit length, is given by L F (x, t)y dx. W = M = EI

(4.21)

kinetic (4.22)

(4.23)

0

Consider the simply supported beam undergoing transverse vibration shown in Fig. 4.5. We apply Hamilton’s principle in the usual way. The J integral is t2 L dt J = t1

1 = 2

t2

t1

"

L 0

∂y ρA ∂t

2

L

dx − 0

EI

∂ 2y ∂x 2

2

L

dx + 0

# F (x, t)y dx dt.

Hamilton’s principle

93

F (x, t)

dx

Fig. 4.5 A simply supported beam with distributed load F (x, t) in transverse vibration.

We take the ﬁrst variation of J to give the stationary value and equate to zero t2 δJ = δL dt = 0. t1

Let us take the variation term by term. The contribution from the work done by external forces is obtained by substituting from (4.23) to give t2 L t2 δW dt = F (x, t) δy dx dt. t1

t1

0

The kinetic energy term, substituting for (4.22), is L 2 t2 ∂y 1 t2 δT dt = ρAδ dx dt 2 t1 ∂t 0 t1 L 1 t2 ∂y ∂y = δ dx dt ρA 2 2 t1 ∂t ∂t 0 t2 L ∂y ∂y = δ dx dt ρA ∂t ∂t 0 t1 t2 L ∂y ∂ = ρA δy dx dt 0 ∂t ∂t t1 # t2 t2 L " ∂y ∂ 2y δy − δy 2 dt dx = ρA ∂t ∂t 0 t1 t1 but δy(t1 ) = δy(t2 ) = 0 thus

t2

t1

δT dt = −ρA 0

L t2 t1

δy

∂ 2y dt dx. ∂t 2

94

Finite element method

The elastic strain energy term is, using (4.21),

t2 t1

1 δU dt = 2

= EI

t2

δ

t1

t2

t1

L

EI

∂ 2y ∂x 2

∂ 2y

∂2

0 L 0

∂x 2 ∂x 2

2

dx dt =

t2

t1

L 0

2 EI ∂ 2 y ∂ y 2 2δ dx dt 2 ∂x ∂x 2

δy dx dt

# ∂ 3y ∂ δy dx dt = EI − 3 0 ∂x ∂x t1 0 # L L 4 L 3 t2 " 2 ∂ y ∂ y ∂ ∂ y δy + δy dx dt. δy − = EI 4 ∂x 2 ∂x ∂x 3 0 ∂x t1 0 0

t2

"

∂ 2y ∂ δy ∂x 2 ∂x

L

L

Finally, summing the terms,

∂ 4y ∂ 2y δJ = − EI 4 + ρA 2 δy dx dt ∂x ∂t 0 t1 L # L 3 t2 L t2 " 2 ∂ y ∂ y ∂ δy F (x, t) δy dx dt dt + δy + − EI ∂x 2 ∂x ∂x 3 0 t1 t1 0 0 t2 L ∂ 4y ∂ 2y = − EI 4 + ρA 2 − F δy dx dt ∂x ∂t 0 t1 " L # L 3 t2 2 ∂ y ∂ y ∂ δy dt = 0. (4.24) δy − + EI ∂x 2 ∂x ∂x 3 t1 0 0

t2

L

For δJ to be zero the integrands between 0 and L must be zero and since δy is arbitrary it follows that the individual terms in (4.24) must also vanish so that (assuming uniform, constant transverse loading, F ), EI

∂ 4y ∂ 2y + ρA =F ∂x 4 ∂t 2

and in addition, the boundary conditions are ∂ 2y ∂ δy = 0 for x = 0 and x = L, ∂x 2 ∂x ∂ 3y δy = 0 for x = 0 and x = L, ∂x 3

(4.25)

Hamilton’s principle

95

which means either

∂ 2y =0 ∂x 2

∂ δy = 0 ∂x

or

for x = 0 and x = L

and

(4.26)

either

∂ 3y =0 ∂x 3

δy = 0

or

for x = 0 and x = L.

Equation (4.25) is the equilibrium equation for the vibrating beam problem. However, note that Hamilton’s principle has also given us the boundary conditions for the problem in Equations (4.26). We shall ﬁnish by looking at one further example. 4.2.3.3 Transverse vibration of a beam with axial loading. We shall now consider the previous problem but with the addition of an externally applied axial force, P , as shown in Fig. 4.6. The axial force does work as the beam shortens due to transverse displacement (here, we are ignoring axial displacement which results from the axial strain due to the force, P ). An element of the beam, ds, shortens by $ ds − dx = dx 2 + dy 2 − dx = =

⎧% ⎨ ⎩

1+

dy dx

2

%

1+

⎫ ⎬

dy dx

1 − 1 dx ≈ ⎭ 2

2 dx − dx ∂y ∂x

2 dx.

The work done by the axial force per differential length 1 dWP = P 2

∂y ∂x

2 dx.

F (x, t ) P

P

dy

ds

dx

dx

Fig. 4.6 Simply supported beam subjected to axial force P while undergoing transverse vibration.

96

Finite element method

The ﬁrst variation of the work done by external forces then becomes 2 t2 L t2 ∂y 1 F (x, t) δy + δP dx dt δW dt = 2 ∂x 0 t1 t1 t2 L ∂y ∂ δy dx dt F (x, t) δy + P = ∂x ∂x 0 t1 L # t2 L " ∂y ∂ 2y δy F (x, t) δy − P 2 δy dx + P dt. = ∂x ∂x 0 t1 0 Thus, for uniform transverse loading F (x, t) = F , the equilibrium equation becomes ∂ 2y ∂ 2y ∂ 4y + P + ρA =F ∂x 4 ∂x 2 ∂t 2 and the boundary conditions are EI

∂ 2y ∂ δy = 0 for x = 0 and x = L, ∂x 2 ∂x ∂ 3y ∂ 2y EI 3 + P 2 = 0 for x = 0 and x = L, ∂x ∂x which means either

∂ 2y =0 ∂x 2

either

EI

or

∂ δy = 0 ∂x

for x = 0 and x = L

and

4.3

∂ 2y ∂ 3y + P =0 ∂x 3 ∂x 2

or

δy = 0

for x = 0 and x = L.

Introduction to the ﬁnite element method

In this section, we will make use of Hamilton’s principle to obtain ﬁnite element equilibrium equations which we shall then apply to some simple, uniaxial problems, before considering some further ﬁnite elements, and their application in statics and dynamics. We shall start with an introduction to the ﬁnite element method. Figure 4.7 shows a representation of an undeformed body when the value of time is zero, which has been discretized into a ﬁnite number of tetrahedral ﬁnite elements which approximate the initial geometry of the body. A particular, single ﬁnite element is shown which has nodes at points P1 , P2 , P3 , and P4 in the undeformed conﬁguration. On the application of a load (which may be mechanical or thermal, for example), the body deforms (and undergoes

Introduction to the ﬁnite element method

97

Z, z F

Time = t Y, y p3 Time = 0

F

P3

X, x

P2

P4

p2

p4 p1

P1

Fig. 4.7 Schematic diagram showing the ﬁnite element discretization of a body with three-dimensional tetrahedral elements.

transformation ) to that shown in the current conﬁguration at time t. The nodes of the single element, after deformation, are now located at p1 , p2 , p3 , and p4 . For simplicity, let us suppose that the quantity we are interested in determining is temperature, chosen because it is a scalar variable. The basis of the ﬁnite element method is to assign nodes to the elements and to assume that we can determine shape functions to enable interpolation to give the value of the temperature at any point within the element in terms of the nodal values of temperature. The tetrahedral element shown in the ﬁgure has four nodes. If the temperatures at the four nodes are θ1 , θ2 , θ3 , and θ4 respectively, then the temperature anywhere within the element is given by n Ni θi , (4.27) θ = N1 θ1 + N2 θ2 + N3 θ3 + N4 θ4 = i=1

where Ni are called shape (or interpolation) functions. Let us consider in isolation the element shown in Fig. 4.7 in the deformed conﬁguration. The element is shown in Fig. 4.8(a) with respect to the current conﬁguration, and in (b) with respect to a local element reference frame (ξ1 , ξ2 , ξ3 ). A transformation is clearly needed to map the element from the local reference frame to the current conﬁguration, and similarly, from the local reference frame to the original conﬁguration, and we shall address this later. The shape functions for this element, in terms of the local variables, are N1 (ξ1 , ξ2 , ξ3 ) = 1 − ξ1 − ξ2 − ξ3 , N2 (ξ1 , ξ2 , ξ3 ) = ξ1 , N3 (ξ1 , ξ2 , ξ3 ) = ξ2 , N4 (ξ1 , ξ2 , ξ3 ) = ξ3 .

98

Finite element method (a)

(b)

j3

x3

4 4 1 1 2

2

3 x2

x1

3 j2

j1

Fig. 4.8 Four-noded tetrahedral element shown with respect to (a) the current conﬁguration and (b) the local element reference frame.

An important feature of the shape functions in the ﬁnite element method is that they generally take a value of unity at their own node and are zero at all others; at node 1, for example, ξ1 = ξ2 = ξ3 = 0, so N1 = 1. They generally sum to unity: N1 + N2 + N3 + N4 = 1; there are however, some special elements for which this is not the case. With knowledge of position (ξ1 , ξ2 , ξ3 ) within an element, the shape functions can be used together with Equation (4.27) to determine the value of the temperature at any point within the element, given the nodal temperatures. The shape functions may be used in a similar way for any variable of interest, but often, the ﬁnite element equilibrium equations are set up with displacement as the basic quantity for which solutions are obtained. Such an approach is often referred to, therefore, as the displacementbased ﬁnite element method. We will look at a further, very simple ﬁnite element in order to examine the displacement-based approach. Figure 4.9 shows a uniform bar under axial force P which has been discretized with a number of uniaxial truss elements. Each element has two nodes and is of length L. Each node has just one degree of freedom; namely axial displacement, u. The bar lies along the x-direction in the current conﬁguration. The shape functions are N1 (ξ ) = 1 − ξ,

N2 (ξ ) = ξ,

(4.28)

where ξ = x/L and 0 ≤ ξ ≤ 1, and the element displacements are given by u(ξ ) = N1 u1 + N2 u2 . This is often written in vector form as u(ξ ) = N uI = [N1

u1 . N2 ] u2

(4.29)

Introduction to the ﬁnite element method

99

P x

P

u2

L

x u1 N2 1

N1 1

N1(j) = 1– j

1

j N2(j) = j

1

j

Fig. 4.9 A uniform bar discretized using uniaxial truss elements with shape functions shown.

Because we know the displacement everywhere within the element, we can determine the small strain, which, for this simple, uniaxial displacement is just ∂N1 ∂ξ ∂u ∂N1 ∂N2 u1 ε= = = ∂ξ ∂x ∂x ∂x ∂x u2 u1 1 . = [−1 1] L u2

∂N2 ∂ξ ∂ξ ∂x

u

1

u2 (4.30)

The derivatives of the type ∂ξ /∂x relate the current conﬁguration to the local element reference frame and, in effect, provide the mapping of the element from the current conﬁguration to the local element reference frame. In this case, because ξ = x/L, the mapping is trivial and the derivatives ∂ξ /∂x are easily obtained. We will see how to do this for more general cases a little later. The matrix of spatial derivatives of the shape functions, given in Equation (4.30), is often referred to as the B matrix where for this particular element, B=

1 [−1 L

1].

(4.31)

It can be seen from (4.30) that the strain is constant everywhere within the element; it is an example (as is the four-noded tetrahedran above) of a constant strain element. In order to progress with the analysis of the loaded bar, we need to obtain the equations of motion or equilibrium. We shall do this in a general way using Hamilton’s principle, and then return to the loaded bar and to uniaxial truss elements.

100

Finite element method

4.4

Finite element equilibrium equations

4.4.1

Some preliminaries: tensor and Voigt notation, tensorial versus engineering strain

Tensorial notation is very elegant when it comes to theoretical derivations. However, for the purposes of developing numerical algorithms for implementation into computer programs, it is often more practical to work with arrays thus representing second-order tensor (strain, stress) as one-dimensional arrays and constitutive tensors (the elasticity tensor) as two-dimensional arrays. Symmetry of stress and strain tensors is used to obtain the following (memory saving) notation (Voigt notation): ⎡ ⎤ σxx ⎢ ⎥ ⎢σyy ⎥ ⎡ ⎤ ⎢ ⎥ σxx σxy σxz ⎢σ ⎥ ⎢ ⎥ ⎢ zz ⎥ σ = ⎣σxy σyy σyz ⎦ → σ = ⎢ ⎥ , (4.32) ⎢σxy ⎥ ⎢ ⎥ σxz σyz σzz ⎢σ ⎥ ⎣ yz ⎦ σxz ⎡ ⎤ ⎡ ⎤ εxx εxx ⎢ε ⎥ ⎢ ⎥ ⎢ yy ⎥ ⎢ εyy ⎥ ⎡ ⎤ ⎢ ⎥ ⎢ ⎥ εxx εxy εxz ⎢ εzz ⎥ ⎢ ε ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ zz ⎥ ε = ⎣εxy εyy εyz ⎦ → ε = ⎢ ⎥ = ⎢ (4.33) ⎥. ⎢γxy ⎥ ⎢2εxy ⎥ ⎢ ⎥ ⎢ ⎥ εxz εyz εzz ⎢γyz ⎥ ⎢2ε ⎥ ⎣ ⎦ ⎣ yz ⎦ γzx 2εzx Note that in vector, or Voigt notation, the shear strain components are stored as engineering shears, that is, twice the tensor shears. This sometimes causes confusion, so let us clarify by recalling Hooke’s law. Writing stress and elastic strain as column vectors, Hooke’s law in three dimensions becomes ⎤ ⎡ ⎤⎡ ⎡ ⎤ λ + 2µ λ λ 0 0 0 εxx σxx ⎥ ⎢ ⎥⎢ ⎢ ⎥ ⎢ λ ⎢ εyy ⎥ λ + 2µ λ 0 0 0⎥ ⎢σyy ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎥⎢ ⎢ ⎥ ⎢ ⎥ ⎢ λ λ λ + 2µ 0 0 0 ⎥ ⎢ εzz ⎥ ⎢ σzz ⎥ ⎥ ⎢ ⎢ ⎥ ⎥, ⎥⎢ σ = ⎢ ⎥ = Cε = ⎢ (4.34) ⎥ ⎢ ⎥ ⎢ γ 0 0 0 µ 0 0 ⎢σxy ⎥ xy ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎥⎢ ⎢ ⎥ ⎢ 0 ⎥ ⎢ γyz ⎥ ⎢ σyz ⎥ 0 0 0 µ 0 ⎥ ⎢ ⎥⎢ ⎣ ⎦ ⎦ ⎣ ⎦⎣ γ 0 0 0 0 0 µ xz σxz

Finite element equilibrium equations

101

where λ = Eν/(1 + ν)(1 − 2ν) and µ = G = E/2(1 + ν) are the Lame constants. Let us take one of the shear terms, for example, σxy = µγxy ≡

E γxy . 2(1 + ν)

We will now obtain the same shear stress, this time using the relation, given in Equation (2.99), that is, ⎛ ⎞ σxx σxy σxz ⎜ ⎟ ⎟ σ =⎜ ⎝σxy σyy σyz ⎠ = 2Gε + λTr(ε)I σxz σyz σzz ⎞ ⎛ ⎛ 1 εxx εxy εxz ⎟ ⎜ ⎜ ⎟ ⎜ = 2G ⎜ ⎝εxy εyy εyz ⎠ + λ(εxx + εyy + εzz ) ⎝0 εxz εyz εzz 0

(4.35) stress–strain tensor

0

0

⎞

1

⎟ 0⎟ ⎠.

0

1

The shear stress is, therefore, σxy = 2Gεxy ≡

E εxy . (1 + ν)

(4.36)

Comparison of (4.35) and (4.36) shows that we must have γxy = 2εxy and similarly for the other shear strains. A more elegant explanation of this is as follows. Let us consider the case of pure elastic shear, as described by the stress and strain tensors ⎛ ⎞ ⎛ ⎞ 0 σxy σxz 0 εxy εxz ⎜ ⎟ ⎜ ⎟ ⎟ σ =⎜ ε=⎜ 0 σyz ⎟ ⎝σxy ⎠, ⎝εxy 0 εyz ⎠ . σxz σyz 0 εxz εyz 0 The elastic strain energy per unit volume is given by the tensor product ⎛ ⎞ ⎛ ⎞ 0 σxy σxz 0 εxy εxz ⎟ ⎜ ⎟ 1⎜ 1 σ :ε= ⎜ :⎜ σxy 0 σyz ⎟ εxy 0 εyz ⎟ ⎝ ⎠ ⎝ ⎠ = (σxy εxy + σyz εyz + σxz εxz ) 2 2 σxz σyz 0 εxz εyz 0 and substituting for the shear stresses using (4.36) and similar expressions gives E 1 2 2 (ε 2 + εyz + εxz ). σ :ε= 1 + ν xy 2

(4.37)

102

Finite element method

We can also calculate the strain energy using engineering shear strain as 1 (τxy γxy + τyz γyz + τxz γxz ) 2 E 1 2 2 2 2 2 (γ 2 + γyz + γyz + γxz )= + γxz ). = G(γxy 4(1 + ν) xy 2

(4.38)

Comparison of (4.37) and (4.38), given that the three shear strains are independent, gives γxy = 2εxy as before, and similarly for the other shear strains. The strain tensor is, of course, an objective quantity; that is, one that satisﬁes the criteria for objectivity discussed in Chapter 3, and this means a quantity whose properties remain unchanged under rotation. We must therefore use the tensorial shear strain components (as opposed to the engineering shear) when rotating a strain. It might be of interest to note that it is for this reason that Mohr’s circle for strain is drawn in terms of γxy /2(= εxy ) rather than γxy . We write the dot product of two ﬁrst-order tensors, or vectors, as uT · v = ui vi = v T · u = vi ui =

n i=1 n

ui vi , vi ui

i=1

so that v T · u = uT · v. If, therefore, we calculate the product of the stress vector, for example, then from (4.32), σT · σ = (σxx

σyy

σzz

σxy

σyz

σxz ) · (σxx

σyy

σzz

σxy

σyz

σxz )T

2 2 2 2 2 2 = σxx + σyy + σzz + σxy + σyz + σxz .

It is important to note that this does not give the same result as the equivalent product of the stress tensor, which is 2 2 2 2 2 2 + σyy + σzz + 2(σxy + σyz + σxz ). σ : σ = σxx

It is therefore necessary to take care when using the vector (Voigt) notation for stress and strain in carrying out calculations. So, for example, the norm of σ , written |σ | is 2 2 2 2 2 2 1/2 + σyy + σzz + 2(σxy + σyz + σxz )] |σ | = (σ : σ )1/2 = [σxx

Finite element equilibrium equations

but if we work from the stress written as a column vector, then |σ | = σT Sσ, which includes the following scaling matrix ⎡ 1 0 0 ⎢ ⎢0 1 0 ⎢ ⎢ ⎢0 0 1 S=⎢ ⎢0 0 0 ⎢ ⎢ ⎢0 0 0 ⎣ 0 0 0

0

0

0

0

0

0

2

0

0

2

0

0

0

⎤

⎥ 0⎥ ⎥ ⎥ 0⎥ ⎥. 0⎥ ⎥ ⎥ 0⎥ ⎦ 2

The following are further examples of possible dangers in using Voigt notation: 1. Second invariant of deviatoric stress in tensorial notation 1 J2 = σ : σ

2 and its correct expression in Voigt notation 1 J2 = σ T Sσ . 2 2. Gradient of J2 invariant in tensorial notation ∂J2 = σ

∂σ

and its correct expression in Voigt notation ∂J2 = Sσ . ∂σ

3. Strain norm in tensorial notation √ |ε| = ε : ε and its correct expression in Voigt notation |ε| = εT S −1 ε, ⎡

where

S −1

1

⎢ ⎢0 ⎢ ⎢ ⎢0 =⎢ ⎢0 ⎢ ⎢ ⎢0 ⎣ 0

0

⎤

0

0

0

0

1

0

0

0

0

1

0

0

0

0

1 2

0

0

0

0

1 2

⎥ 0⎥ ⎥ ⎥ 0⎥ ⎥. 0⎥ ⎥ ⎥ 0⎥ ⎦

0

0

0

0

1 2

103

104

4.4.2

Finite element method

Finite element equations using Hamilton’s principle

For the purposes of obtaining the ﬁnite element equilibrium equations, we shall conﬁne ourselves initially to small elastic deformation problems so that we will not need to worry about the kinematics of large deformations. We will address large deformations later. The components of the Lagrangian for a general body subject to tractions t are given in Equations (4.18) using tensorial notation. We shall write them, here, using Voigt notation for a particular (the ‘m’th) ﬁnite element as follows 1 Tm = ρ u˙ T u˙ dV , 2 1 εT σ dV , (4.39) Um = 2 uT t dA, Wm = ∂

in which all non-scalar quantities are represented as column vectors and in particular, the stress and strain vectors are given by Equations (4.32) and (4.33), respectively ˙ and similarly for and the engineering shear strains are used. Note that u˙ T u˙ ≡ u˙ · u, other vector quantities. For completeness, the displacement and traction vectors are given by ⎡ ⎤ ⎡ ⎤ ux tx ⎢ ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ u=⎢ ⎣uy ⎦ and t = ⎣ty ⎦ . uz tz Hooke’s law, from Equation (4.34), is written as σ = Cεe .

(4.40)

The displacement within the particular ﬁnite element may be written in terms of the nodal displacements, uI , as we did in (4.29) so that u = N uI

(4.41)

and the strains can be written, in general, in terms of the nodal displacements and the B matrix, as we did for the truss element in Equation (4.30), ε = BuI .

(4.42)

For the uniaxial truss element, ε becomes just the unaxial, scalar, strain ε, but for other element types (in two and three dimensions), the other strain components are needed. We shall see an example of this later.

Finite element equilibrium equations

105

In applying Hamilton’s principle, we shall start from the Lagrangian, Lm , for the single element 1 1 Lm = Tm − Um + Wm = Tm = ρ u˙ T u˙ dV − εT σ dV + uT t dA 2 2 ∂ and substituting Equations (4.40)–(4.42) gives 1 T 1 T T T T Lm = u˙ I ρN N dV u˙ I − uI B CB dV uI + uI N T t dA. 2 2 ∂ If we deﬁne element mass and stiffness matrices as ρN T N dV m=

(4.43)

and k=

and the vector of nodal forces as

B T CB dV

(4.44)

N T t dA,

(4.45)

f =

∂

then the Lagrangian becomes Lm =

1 T 1 u˙ I mu˙ I − uTI kuI + uTI f . 2 2

The J integral is, therefore t2 J = Lm dt = t1

t2

t1

1 T 1 T T u˙ mu˙ I − uI kuI + uI f dt 2 I 2

and applying Hamilton’s principle gives t2 1 1 T T T δJ = δ(u˙ I mu˙ I ) − δ(uI kuI ) + δ(uI f ) dt 2 2 t1 t2 δuTI (−mu¨ I − kuI + f ) dt = 0. = t1

Since δuI is an arbitrary displacement, this gives for the equilibrium equation, for a single ﬁnite element mu¨ I + kuI = f . (4.46) Equation (4.46) is the ﬁnite element equilibrium equation, or equation of motion, written in terms of nodal displacements, uI . In the absence of inertia forces, it reduces to the standard, quasi-static equation kuI = f .

(4.47)

106

Finite element method

Some authors differentiate between momentum balance equations and equilibrium equations; those that are derived which include inertia (dynamic) effects—for example, that given in (4.46)—are often referred to as momentum balance equations, and those which do not include inertia effects (for quasi-static problems), are simply called equilibrium equations. In most cases in what follows, we shall simply refer to both types as equilibrium equations. In Section 4.4.2.1, we shall determine the mass and stiffness matrices for a truss element and examine a single-element problem. 4.4.2.1 Single truss element problem. Consider the uniform bar with crosssectional area A, made of material with density ρ, and Young’s modulus E, shown in Fig. 4.10(a). This is discretized with a single, uniaxial truss element shown in Fig. 4.10(b). The shape functions are those given in (4.28), N1 (ξ ) = 1 − ξ,

N2 (ξ ) = ξ

so that N = [1 − ξ

ξ ].

From above, (4.31), the B matrix is B=

1 [−1 L

1].

The mass matrix can then be determined from (4.43) as L 1−ξ T m= ρN N dV = ρ [1 − ξ x=0 ξ

ξ ]A dx.

This integral is currently given with respect to the deformed conﬁguration, x, so it needs to be transformed to the local element reference frame, ξ . While trivial in this case, since ξ = x/L, in general we would need to obtain the Jacobian, mapping dV (or equivalently, dx) in the current conﬁguration to dV (or, dξ ) in the element reference

r, E, A P

r, E, A

1 L

x2 u2

x1 u1

(b)

(a)

2

L

Fig. 4.10 (a) A uniform bar under axial force, P , and (b) its discretization using a single truss element.

Finite element equilibrium equations

frame, as we shall see later. For now, however, 1 L 1 − ξ 1−ξ ρ [1 − ξ ξ ]A dx = ρ [1 − ξ m= x=0 ξ =0 ξ ξ 1 (1 − ξ )2 ξ(1 − ξ ) dξ = ρAL 0 ξ(1 − ξ ) ξ2 so

m = ρAL The stiffness matrix is, using (4.44) B T CB dV = k=

=

1

ξ =0

E L2

L

x=0

1 −1

−1 1

1 3 1 6

1 6 1 3

.

1 1 −1 E [−1 L 1 L

107

ξ ]AL dξ

(4.48)

1]A dx

AL dξ,

where in this simple uniaxial case, the elasticity matrix C is simply Young’s modulus, E, so

EA 1 −1 (4.49) k= L −1 1 and the nodal force vector, (4.45), for this problem is simply F1 f = P

(4.50)

in which P is just the prescribed force at node 2 and F1 the currently unknown reaction at node 1, and no integration over ξ is necessary. Note that because t is a traction (stress vector), t dA is the force acting on the area dA at nodes 1 and 2. The integration of dA at the two ends therefore just gives A and is independent of ξ , so that tA at node 2 is P and that at node 1 is F1 , both of which act in a direction parallel to t; that is, the x-direction. The equilibrium Equation (4.46) therefore gives 1 1

u¨ 1 F1 EA 1 −1 u1 6 3 + = ρAL . (4.51) 1 1 L −1 1 u ¨ u P 2 2 6 3 Let us assume inertia forces are negligible and that this is, therefore, a quasi-static problem so that we may eliminate the inertia term from (4.51) to give

F1 EA 1 −1 u1 = . L −1 1 u2 P

108

Finite element method

With the boundary condition that u1 = 0, these equations can be solved to give the expected result that PL u2 = , F1 = −P EA and using u = N uI , that 0 PL =ξ . u2 = [1 − ξ ξ ] EA u2 where 0 ≤ ξ ≤ 1. Despite using just a single element, these results are exact. This is only because, in this particular problem, we have been using a constant strain element to discretize what is, in any case, a constant strain problem. In the following section, we shall give a more general description of the ﬁnite element method which includes the kinematics of large deformations and recognizes that the displacement of the nodes can become large; the problem then becomes geometrically non-linear. In addition, we need to give a fuller description of the mapping process between the current (and original) conﬁguration and the local element reference frame. We will then look at several further examples. 4.4.3

General ﬁnite element approach

We will now return to the body in the initial and current conﬁgurations shown in Fig. 4.7. We will formulate the ﬁnite element equations with respect to the current, or deformed, conﬁguration. When carried out incrementally, this is usually called an updated Lagrangian formulation. An alternative is to set up the equations with respect to the original conﬁguration, in which case, it is called a total Lagrangian formulation. The initial position of the material particle P within the element shown can be speciﬁed as follows X(ξ , t) ≈

NNODE

NI (ξ )XI (t),

(4.52)

I =1

where NNODE denotes the number of ﬁnite element nodes, NI (ξ ) represents, as before, the element shape functions and X I indicates the initial positions of the ﬁnite element nodal points P I , which are given in terms of the local element reference, (ξ1 , ξ2 , ξ3 ) shown in Fig. 4.8. Assuming that the material particle P remains attached to the same ﬁnite elements during the motion, the current positions of the material particles at the time t are speciﬁed by x(ξ , t) ≈

NNODE I =1

NI (ξ )x I (t)

(4.53)

Finite element equilibrium equations

109

where x I (t) denotes the current positions of the ﬁnite element nodal points pI . In the example in Section 4.4.2.1, the displacements were assumed to be small and there were no rigid body rotations. X(ξ , t) and x(ξ , t) were therefore identical and in addition, because the element considered was one-dimensional, ξ in Equations (4.52) and (4.53) was simply the scalar ξ . For two-dimensional elements, for example, two local reference frame independent variables are needed, (ξ1 , ξ2 ), to specify position. For the previous truss element example, x(ξ , t) becomes x(ξ, t) ≈

2

NI (ξ )xI (t) = (1 − ξ )x1 (t) + ξ x2 (t).

(4.54)

I =1

Equation (4.54), and for the general case (4.53), therefore, maps any point within an element, speciﬁed by ξ with respect to the local element reference system, onto the corresponding position in the current conﬁguration. The displacement and the velocity ﬁelds within each ﬁnite element are approximated as follows u(ξ , t) ≈

NNODE

NI (ξ )uI (t),

(4.55)

NI (ξ )v I (t).

(4.56)

I =1

v(ξ , t) ≈

NNODE I =1

In Equations (4.52)–(4.55), the same shape functions are used for interpolating position and displacement. Elements for which this holds true are called isoparametric. The deformation gradient tensor is obtained by differentiating Equation (4.53) with respect to the initial conﬁguration as follows F (ξ , t) ≈

NNODE

x I (t) ⊗ ∇X NI (ξ , t),

(4.57)

I =1

∂NI (ξ ) ∂NI ∂NI ∂NI = (4.58) ∇ X NI (ξ , t) = ∂X(t) ∂X ∂Y ∂Z are the derivatives of the shape functions NI . The gradient term, ∇, and the dyadic product, ⊗, are explained in Appendix A. The derivative can be rewritten as follows ∂NI (ξ ) ∂NI (ξ ) ∂ξ ∂NI (ξ ) ∂X(t) −1 ∇X NI (ξ , t) = . (4.59) = = ∂X(t) ∂ξ ∂X(t) ∂ξ ∂ξ where

It is normally not possible to determine ∂ξ /∂X in Equation (4.59) directly since Equation (4.52) speciﬁes X in terms of ξ . It is therefore necessary to determine ∂X/∂ξ instead and obtain the inverse. The derivative ∂X/∂ξ is called the Jacobian and relates

110

Finite element method

inﬁnitesimal quantities in the material conﬁguration to those in the local element coordinate system. We shall see this in several examples later. Using Equation (4.52), ∂X ∂NI (ξ ) = XI (t), ∂ξ ∂ξ

(4.60)

where the members of ∂X/∂ξ are given by NNODE ∂NI ∂Xi . = XiI ∂ξj ∂ξj

(4.61)

I =1

The small strain tensor can be approximated NNODE 1 1 [∇u + (∇u)T ] ≈ [uI (t) ⊗ ∇X NI (ξ ) + ∇X NI (ξ ) ⊗ uI (t)]. 2 2 I =1 (4.62) The velocity gradient is obtained as the spatial derivative of the velocity in Equation (4.56) as NNODE L(ξ , t) ≈ v I (t) ⊗ ∇x NI (ξ , t)

ε(ξ , t) =

I =1

and the rate of deformation tensor is obtained by using D = (1/2)(L + LT ) as follows D(ξ , t) ≈

NNODE 1 (v I (t) ⊗ ∇x NI (ξ , t) + ∇x NI (ξ , t) ⊗ v I (t)), 2

(4.63)

I =1

where

∂NI (ξ ) (4.64) ∂x(t) are the spatial derivatives with respect to the current conﬁguration, and are obtained from the shape functions as ∂NI (ξ ) ∂NI (ξ ) ∂ξ ∂NI (ξ ) ∂x(t) −1 , (4.65) = = ∇x NI (ξ , t) = ∂x(t) ∂ξ ∂x(t) ∂ξ ∂ξ ∇x NI (ξ , t) =

where members of the Jacobian, ∂x/∂ξ , are given by NNODE ∂NI ∂xi = xiI . ∂ξj ∂ξj

(4.66)

I =1

We return now to the equilibrium Equation (4.20), obtained from Hamilton’s principle, but write the increment in virtual work per unit volume and per unit time as ¨ · δv dV = 0, (div[σ ] − ρ u) (4.67) δW =

Finite element equilibrium equations

111

where δv is an arbitrary virtual velocity in the current conﬁguration. By noting that div[σ · δv] = div[σ ] · δv + σ : ∇δv,

(4.68)

n · σ δv = δv · t

that ∇δv = δL and that because σ is symmetric, it can be shown (with a little algebra) that σ : δL = σ : δD, substituting into (4.67) with the application of the divergence theorem gives δW = ρ u¨ · δv dV + σ : δD dV − t · δv dA = 0. (4.69)

∂

The second term in the right-hand side of (4.69) is the internal work per unit volume per second. A stress quantity is called work conjugate to the strain if their double contracted tensor product yields work. The co-rotational Cauchy, or true, stress is work conjugate to the rate of deformation. The spatial virtual work equation, (4.69), which describes the dynamic equilibrium of the element can be rewritten in terms of the ﬁnite element discretization as follows

NNODE

NNODE δW ≈ NI u¨ I NI δv I dV ρ

I =1

+

−

1 (δv I ⊗ ∇ x NI + ∇ x NI ⊗ δv I ) dV 2 I =1 NNODE

t· NI δv I dA.

σ :

∂

I =1

NNODE

(4.70)

I =1

As σ is a symmetric tensor, this reduces to

NNODE

NNODE ρ NI u¨ I NI δv I dV δW ≈

I =1

+

σ :

I =1

NNODE

δv I ⊗ ∇x NI dV −

I =1

∂

t·

NNODE

NI δv I dA

I =1

and as the nodal virtual velocities are independent of the integration, this may be rewritten to give NNODE δW ≈ δv I · NIT ρ u¨ I [N1 , N2 , . . . , NNNODE ] dV I =1

+

NNODE I =1

δv I ·

σ ∇x NI dV −

NNODE I =1

δv I ·

NI t dA.

(4.71)

112

Finite element method

The virtual work equation can ﬁnally be written in vector form as dW ≈

NNODE

dv I · (f Iinert + f Iint − f Iext )

(4.72)

I =1

by introducing expressions for the equivalent element nodal force vectors as follows f Iinert = NIT ρ u¨I [N1 , N2 , . . . , NNNODE ] dV , (4.73) int σ ∇ x NI dV , (4.74) fI = ext NI t dA, (4.75) fI = ∂

where f Iinert , f Iint , and f Iext represent the inertial, the internal, and the external element nodal forces, respectively. Since the discretized rate of virtual work, Equation (4.72) must be satisﬁed for all cases of the arbitrary virtual velocities, the element equation can be rewritten f Iinert + f Iint − f Iext = 0.

(4.76)

The nodal forces can be further assembled into global vectors (column matrices) by summing over all elements to give ⎡ ⎡ ⎤ ⎤ ⎡ ext ⎤ f 1inert f 1int f1 ⎢ inert ⎥ ⎢ int ⎥ ⎢ ext ⎥ ⎢f 2 ⎥ ⎢f 2 ⎥ ⎢f 2 ⎥ ⎢ ⎢ ⎥ ⎥ inert int ext ⎢ F = ⎢ . ⎥, (4.77) F = ⎢ . ⎥, F =⎢ . ⎥ ⎥, ⎢ .. ⎥ ⎢ .. ⎥ ⎣ .. ⎦ ⎣ ⎣ ⎦ ⎦ f ninert

f nint

f next

where n is the total number of points used in the discretization. Finally, the ﬁnite element discretization can be expressed by the set of non-linear equilibrium equations as follows: Finert (u) + Fint (u) − Fext (u) = 0 (4.78) for the set (column matrix) of nodal displacements ⎡ ⎤ u1 (t) ⎢u (t)⎥ ⎢ 2 ⎥ ⎥ u=⎢ ⎢ .. ⎥ ⎣ . ⎦ un (t) at time t.

(4.79)

Finite element equilibrium equations

113

We can rewrite Equation (4.76) in a more familiar way by considering the internal work term and writing it in terms of Voigt notation. We will assume small strain elasticity for simplicity. Returning to Equation (4.69), the internal work term originates from I δW = σ : δD dV

and may be written using Voigt notation as σ : δD dV = δDT σ dV , δW I =

(4.80)

where DT = (Dxx

Dyy

Dzz

2Dxy

2Dyz

2Dzx )

in which the off-diagonal terms (shear terms) are doubled to satisfy work conjugacy as speciﬁed in (4.80). The rate of deformation is given in terms of nodal velocities in (4.63) by D=

NNODE 1 (v I ⊗ ∇x NI + ∇x NI ⊗ v I ). 2 I =1

After some algebra, this can be written in Voigt notation as ⎡ ∂N

⎤

I

0

⎢ ∂x ⎢ ⎡ ⎤ ⎢ Dxx ⎢ 0 ⎢ ⎢ ⎥ ⎢ ⎢ Dyy ⎥ ⎢ ⎢ ⎥ ⎢ ⎢ ⎥ NNODE ⎢ 0 NNODE ⎢ Dzz ⎥ ⎢ ⎢ ⎥ ⎢ D=⎢ B I · vI = ⎥= ⎢ ∂NI ⎢2Dxy ⎥ I =1 I =1 ⎢ ⎢ ⎥ ⎢ ∂y ⎢ ⎥ ⎢ ⎢2Dyz ⎥ ⎢ ⎣ ⎦ ⎢ ⎢ 0 2Dzx ⎢ ⎢ ⎣ ∂N

∂NI ∂y 0 ∂NI ∂x ∂NI ∂z

I

0

∂z

0

⎥ ⎥ ⎥ 0 ⎥ ⎥ ⎥ ⎥ ∂NI ⎥ ⎡vxI ⎤ ⎥ ⎢ ⎥ ∂z ⎥ ⎥ ⎢vyI ⎥ ⎥⎣ ⎦ 0 ⎥ ⎥ vzI ⎥ ⎥ ∂NI ⎥ ⎥ ∂y ⎥ ⎥ ∂NI ⎦ ∂x

(4.81)

so that from (4.80) the internal energy term becomes δW I =

δDT σ dV =

NNODE

I =1

T B I dv I

σ dV .

(4.82)

114

Finite element method

If we assume purely elastic small deformation, then from (4.34), we may write

T NNODE I B I dv I Cε dV δW =

=

I =1

NNODE

T B I δv I

C

NNODE

I =1

B J uJ

dV

J =1

⎞

⎛

so that

NNODE

δW I = δv TI ⎝

I,J =1

B TI CB J dV ⎠ uJ

(4.83)

since we may also write the small strains in terms of the nodal displacements as ⎡ ∂N ⎤ I 0 0 ⎢ ∂x ⎥ ⎢ ⎥ ⎤ ⎡ ⎢ ⎥ ∂N I εxx ⎢ 0 0 ⎥ ⎢ ⎥ ⎥ ⎢ ∂y ⎢ ⎥ ⎢ εyy ⎥ ⎢ ⎥⎡ ⎤ ⎥ ⎢ ∂N ⎢ ⎥ uxI I ⎥ NNODE ⎢ ⎢ ⎥ 0 0 NNODE ⎢ εzz ⎥ ⎢ ⎢ ⎥ ∂z ⎥ ⎥ ⎢ ⎢ ⎥ ⎢uyI ⎥. B I · uI = ε=⎢ ⎥= ⎢ ⎥ ⎣ ⎦ ∂N ∂N ⎢2εxy ⎥ I I I =1 I =1 ⎢ ⎥ ⎢ 0 ⎥ ⎢ ⎥ ⎥ ⎢ ∂x ⎢ ∂y ⎥ uzI ⎢2εyz ⎥ ⎢ ⎥ ⎦ ⎣ ⎢ ∂NI ∂NI ⎥ ⎢ 0 ⎥ 2εzx ⎢ ∂z ∂y ⎥ ⎢ ⎥ ⎣ ∂N ∂NI ⎦ I 0 ∂z ∂x Equation (4.83) can be written as δW I = δv TI kuI , where k=

NNODE I,J =1

B TI CB J dV .

(4.84)

When combined with (4.71) and considering an arbitrary virtual velocity, δv, gives mu¨ + ku = f

(4.85)

ku = f .

(4.86)

and for quasi-static problems, This equation, in general, is non-linear if the problem considered is geometrically non-linear. This is because the stiffness matrix, k, depends upon the B matrix which

Finite element equilibrium equations

115

contains the derivatives of the shape functions with respect to the spatial coordinates. In a geometrically non-linear problem, the spatial coordinates change so that the stiffness matrix also changes. For geometrically non-linear problems, Equation (4.86) therefore has to be solved incrementally, and at each increment, the stiffness matrix must be updated. In the following sections, we look at a number of small deformation (geometrically linear) examples including a two-element axial vibration problem in which element assembly is addressed, a single-element and two-element bending problem in which beam elements are introduced, and a single square element static elastic problem in which linear four-noded (quad) elements are introduced. 4.4.3.1 Axial vibration of a beam using two truss elements. The uniform bar shown in Fig. 4.11(a) undergoes axial vibration. It is discretized using two truss elements shown in Fig. 4.11(b). The truss element formulation, relative to the local element reference frame, is shown in Fig. 4.12. (a)

2 A ∂ u2 dx ∂t

, E, A

dx

P

P + ∂P dx ∂x

L

(b)

x1 u1

1

1 , E, A

x2

x3

u2

u3

2 , E, A

2

L/2

3

L/2

Fig. 4.11 A uniform bar undergoing axial vibration (a) shown schematically and (b) its discretization using two truss elements.

l=1 1

2

0

1

j

Fig. 4.12 Linear truss element formulation shown relative to the local element reference frame, ξ .

116

Finite element method

The shape functions are N1 = 1 − ξ,

N2 = ξ

and in this problem, the two elements are identical so that their mass and stiffness matrices, respectively, are the same. Also, because this is a problem in which the displacements are inﬁnitesimal, the current and original conﬁgurations are taken to be the same. We shall determine the mass and stiffness matrices for a single element, and then consider their assemblage. The mass matrix given by (4.43) with respect to the spatial (which in this case coincides with the material) coordinate system is m=

ρN N dV = T

L/2

X=0

ρN T NA dX

but of course, the shape functions are given with respect to the local element reference frame. Therefore, we write m=

L/2

X=0

= ρA

ρN N A dX = T

1

ξ =0

1

ξ =0

1−ξ [1 − ξ ξ

ρN T NA det(J ) dξ

ξ ] det(J ) dξ

(4.87)

in which J is the Jacobian, mapping the spatial coordinate system onto the local element reference frame. In this one-dimensional problem, the determinant of the Jacobian is just ∂X ∂ X1 ∂N1 ∂N2 X1 det(J ) = = , = [N1 N2 ] X2 ∂ξ X2 ∂ξ ∂ξ ∂ξ which is of the general form given in Equation (4.60). Using the shape functions, we obtain L L L X1 det(J ) = [−1 1] = = = |[−X1 + X2 ]| = 0 + X2 2 2 2 so that the element mass matrix becomes

1 2 ξ − ξ2 ρAL 1 1 − 2ξ + ξ ρAL 3 m= dξ = 1 2 2 ξ =0 ξ − ξ2 ξ2 6

1 6 1 3

.

(4.88)

Finite element equilibrium equations

Let us write the mass matrix for elements 1 and 2 as 2 1 1 m11 m111 m112 ρAL 3 6 = = , m m1 = 2 1 1 2 m121 m122 m221 6 3 then the global mass matrix is given by ⎤ ⎡1 ⎡ 1 m112 0 m11 3 L ⎢1 ⎥ ⎢ 1 1 2 2 M = ⎣m21 m22 + m11 m12 ⎦ = ρA ⎣ 6 2 0 m221 m222 0

1 6 2 3 1 6

0

m212 m222

⎤

1⎥ 6⎦ 1 3

ρAL = 2 ⎡

=

1 6 ⎢1 ρAL ⎣ 12

0

1

1 12 1 3 1 12

117

1 6 1 3

3 1 6

0

,

⎤

1⎥ 12 ⎦ . 1 6

(4.89) The element stiffness matrix is given by (4.44) in terms of the spatial coordinates by L T B CB dV = B T CBA dX. k=

X=0

Introducing again the Jacobian in (4.87), the integral can be written with respect to the local element reference frame by 1 1 L T k= B CBA det(J ) dξ = B T CBA dξ . 2 ξ =0 ξ =0 Because the truss elements are one-dimensional, the elasticity matrix, C, becomes just the scalar Young’s modulus, E, so EAL 1 k= B T B dξ . 2 ξ =0 The B matrix contains the derivatives of the shape functions with respect to the spatial coordinates. We are assuming small displacements, however, and that the problem remains geometrically linear so that the spatial and material coordinates remain the same. Hence, ∂N1 ∂ξ ∂N2 ∂ξ ∂N1 ∂N2 ∂N1 ∂N2 B= ≡ = . ∂ξ ∂X ∂ξ ∂X ∂x ∂x ∂X ∂X In general, ∂ξ /∂X cannot be determined directly, since we ordinarily know X in terms of ξ . In its most general form, the relationship is given by (4.52), and for the truss element in this problem, this is X X = [N1 N2 ] 1 . X2 We have already determined the Jacobian derivative, in (4.87), and note that this is the inverse of ∂ξ /∂X. That is, therefore, −1 ∂ξ ∂X −1 L 2 −1 = =J = = . ∂ξ 2 L ∂X

118

Finite element method

In general, therefore, the derivatives needed for the B matrix are obtained from the inverse of the Jacobian. The B matrix is, therefore, ∂N1 ∂ξ ∂N2 ∂ξ 2 2 2 B= = [−1 1] = −1 × 1× ∂ξ ∂X ∂ξ ∂X L L L so that the element stiffness matrix becomes 2 EAL 1 2 2EA 1 −1 k= [−1 1] dξ = 1 2 L −1 ξ =0 L

−1 . 1

(4.90)

As for the mass matrices, we write the stiffness matrices for the two elements as 1 2 2 1 k11 k12 k11 k12 2EA 1 −1 2EA 1 −1 = = , k2 = k1 = 1 1 2 2 L −1 1 L −1 1 k21 k22 k21 k22 so that the global stiffness matrix become ⎡ ⎤ 1 1 ⎡ k11 k12 0 1 ⎢ 1 ⎥ 2EA 1 + k2 2 ⎥= ⎣−1 K=⎢ k k k 22 11 12 ⎦ ⎣ 21 L 0 2 2 0 k21 k22

−1 2 −1

⎤ ⎡ 0 2 EA ⎣−2 −1⎦ = L 1 0

−2 4 −2

⎤ 0 −2⎦ . 2

(4.91) The ﬁnite element equilibrium equation, given in (4.46) and (4.85) then becomes Mu¨ + Ku = 0 so

⎡

1 6 ⎢1 ⎢ ρAL ⎣ 12

0

⎤

⎡ ⎤ ⎡ u ¨ 2 1 ⎥ EA ⎣ 1 ⎥⎣ ⎦ −2 ¨2 + 12 ⎦ u L 0 u ¨ 3 1

1 12 1 3 1 12

0

−2 4 −2

⎤⎡ ⎤ ⎡ ⎤ u1 0 0 ⎦ ⎣ ⎦ ⎣ −2 u2 = 0⎦ . 0 2 u3

6

With the boundary condition u1 = 0, this reduces to 1 1 EA 4 −2 u2 u¨ 2 0 3 12 ρAL + = . 1 1 0 u¨ 3 u3 L −2 2 12

6

4.4.3.2 Cantilever beam in bending using a single element. The problem geometry and ﬁnite element discretization are shown in Figs 4.13 and 4.14. The Hermitian shape functions in the element local coordinate system (note that dx = L dξ ) are obtained as follows: N = a0 + a1 ξ + a2 ξ 2 + a3 ξ 3 .

Finite element equilibrium equations

119

r, E, A, I

L

Fig. 4.13 Cantilever beam of uniform section with second moment of area I .

v2

v1 u1

1

u1

r, E, A, I

1 x

2

L

Fig. 4.14 Single beam element discretization of a cantilever. The element has four degrees of freedom; two translational and two rotational.

First degree of freedom (y1 ) ⎫ dN1 ⎪ = 0⎪ ⎬ 1 dξ ⇒ N1 = 1−3ξ 2 +2ξ 3 . ⎪ dN1 ⎭ = 0⎪ ξ = 1, N1 = 0, 0 dξ

ξ = 0, N1 = 1,

1

j

1

j

Second degree of freedom (θ1 ) ⎫ dN2 ⎪ = 1⎪ ξ = 0, N2 = 0, ⎬ dξ ⇒ N2 = ξ −2ξ 2 +ξ 3 . ⎪ dN2 ⎭ = 0⎪ ξ = 1, N2 = 0, dξ

1 0

Third degree of freedom (y2 ) ξ = 0,

N3 = 0,

ξ = 1,

N3 = 1,

⎫ dN3 ⎪ = 0⎪ ⎬ dξ ⇒ N3 = 3ξ 2 −2ξ 3 . ⎪ dN3 ⎭ = 0⎪ dξ

1 0

1

j

120

Finite element method

Fourth degree of freedom (θ2 ) ξ = 0,

N4 = 0,

ξ = 1,

N4 = 0,

⎫ dN4 ⎪ = 0⎪ ⎬ dξ ⇒ N4 = −ξ 2 +ξ 3 . ⎪ dN4 ⎭ = 1⎪ dξ

1 0

1

j

We shall now apply Hamilton’s principle in order to obtain the ﬁnite element equilibrium equations. For a beam in bending, we may write the kinetic, T , and potential (strain), U , energies as 2 2 2 1 L 1 L ∂v ∂ v T = ρA dx, U= EI dx. 2 0 ∂t 2 0 ∂x 2 The ﬁnite element discretization is given by v(x, t) = N1 (ξ )v1 (t) + N2 (ξ )θ1 (t) + N3 (ξ )v2 (t) + N4 (ξ )θ2 (t) ∂v2 ∂v1 + N3 (ξ )v2 (t) + N4 (ξ ) ∂ξ ∂ξ ∂v1 ∂v2 + N3 (ξ )v2 (t) + N4 (ξ )L , = N1 (ξ )v1 (t) + N2 (ξ )L ∂x ∂x = N1 (ξ )v1 (t) + N2 (ξ )

which we shall write as v = Nu = [N1 (ξ )

N2 (ξ )

N3 (ξ )

N4 (ξ )] v1

∂v1 ∂x

v2

∂v2 ∂x

T .

The derivatives in the strain energy term are given by 1 ∂ 2v 1 ∂ 2 N1 ∂ 2 N2 ∂v1 ∂ 2 N3 ∂ 2 N4 ∂v2 ∂ 2v + = 2 2 = 2 v1 + L v2 + L ∂x 2 L ∂ξ L ∂ξ 2 ∂ξ 2 ∂x ∂ξ 2 ∂ξ 2 ∂x ⎤ ⎡ v1 ⎥ ⎢ ⎢ ∂v1 ⎥ ⎥ ⎢ ⎢ ∂x ⎥ 1 ∂ 2 N1 ∂ 2 N2 ∂ 2 N3 ∂ 2 N4 ⎥ = Bu. = 2 L L ⎢ ⎥ ⎢ L ∂ξ 2 ∂ξ 2 ∂ξ 2 ∂ξ 2 ⎢ v2 ⎥ ⎥ ⎢ ⎣ ∂v2 ⎦ ∂x The element kinetic and strain energies are given by L 1 L 1 T T T ˙ (N u) ˙ dx = u˙ T = ρA(N u) ρAN N dx u˙ 2 2 0 0

Finite element equilibrium equations

and

121

T 2 ∂ N ∂ 2N u u dx EI ∂ξ 2 ∂ξ 2 0 2 T 2 L ∂ N ∂ N 1 T dx u EI = u 2 2 ∂ξ ∂ξ 2 0 L 1 T T = u EI B B dx u. 2 0

1 U= 2

L

The element Lagrangian, L, is L=T −U = where

1 T 1 u˙ mu˙ − uT ku, 2 2

L

m=

(4.92)

ρAN T N dx

(4.93)

EI B T B dx.

(4.94)

0

and

k=

L

0

Integrating the Lagrangian with respect to time, and taking the ﬁrst variation gives mu¨ + ku = 0. The element mass matrix is ⎡ e ⎤ m11 me12 me13 me14 ⎢ e ⎥ e e e ⎥ ⎢m L m m m 22 23 24 ⎥ ⎢ 21 m=⎢ ρAN T N dx = ⎥ ⎢me me me me ⎥ 0 32 33 34 ⎦ ⎣ 31 me41 me42 me43 me44 ⎡ ⎤ 1 − 3ξ 2 + 2ξ 3 ⎥ 1⎢ ⎢(ξ − 2ξ 2 + ξ 3 )L⎥ ⎢ ⎥ = ρA ⎢ ⎥ 2 3 ⎢ ⎥ 0 − 2ξ 3ξ ⎣ ⎦ 2 3 (−ξ + ξ )L × 1 − 3ξ 2 + 2ξ 3 (ξ − 2ξ 2 + ξ 3 )L 3ξ 2 − 2ξ 3 ⎤ ⎡ 156 22L 54 −13L ρAL ⎢ 13L −3L2 ⎥ 4L2 ⎥. ⎢ 22L = 13L 156 −22L⎦ 420 ⎣ 54 −13L −3L2 −22L 4L2

. (−ξ 2 + ξ 3 )L L dξ

122

Finite element method

The element stiffness matrix is given by ⎡ e ⎤ e e e k13 k14 k11 k12 ⎢ e ⎥ e e e ⎥ ⎢k L ⎢ 21 k22 k23 k24 ⎥ k=⎢ = EI B T B dx ⎥ ⎢k e k e k e k e ⎥ 0 34 ⎦ 32 33 ⎣ 31 e e e e k41 k42 k43 k44 ⎡ ⎤ −6 + 12ξ ⎢ ⎥ 1 ⎥ 1 ⎢ 1 ⎢(−4 + 6ξ )L⎥ = ⎢ ⎥ EI 2 2 L 0 L ⎢ 6 − 12ξ ⎥ ⎣ ⎦ (−2 + 6ξ )L × [−6 + 12ξ (−4 + 6ξ )L 6 − 12ξ ⎤ ⎡ 12 6L −12 6L EI ⎢ 6L 4L2 −6L 2L2 ⎥ ⎥. = 3 ⎢ L ⎣−12 −6L 12 −6L⎦ 6L 2L2 −6L 4L2

(−2 + 6ξ )L]L dξ

The ﬁnite element equilibrium equation becomes ⎡ ⎤ ⎤ y¨1 156 22L 54 −13L ⎢ ⎥ 2 ⎢ θ¨ ⎥ ρAL ⎢ 13L −3L2 ⎥ 22L 4L ⎥ ⎢ 1⎥ ⎢ ⎥ 13L 156 −22L⎦ ⎢ 420 ⎣ 54 ⎣y¨2 ⎦ 2 2 −13L −3L −22L 4L θ¨2 ⎡ ⎤⎡ ⎤ ⎡ ⎤ 12 6L −12 6L y1 0 2 2 ⎢ ⎥ ⎢ ⎥ ⎢ EI 6L 4L −6L 2L ⎥ ⎢ θ1 ⎥ ⎢0⎥ ⎥. = + 3 ⎢ L ⎣−12 −6L 12 −6L⎦ ⎣y2 ⎦ ⎣0⎦ 0 6L 2L2 −6L 4L2 θ2 ⎡

With the boundary conditions v1 = 0 and θ1 = 0 at x = 0, the problem reduces to one with two degrees of freedom ρAL 156 −22L x¨2 EI 12 −6L x2 0 + 3 = . 2 2 ¨ −22L 4L −6L 4L 0 θ θ 420 L 3 3 4.4.3.3 Free transverse vibration of a propped cantilever using two beam elements. A uniform, propped cantilever beam is shown in Fig. 4.15 and its ﬁnite element discretization using two beam elements in Fig. 4.16.

Finite element equilibrium equations

123

r, E, A, I

L

Fig. 4.15 A uniform propped cantilever beam.

u1

1

y3

y2

y1 1 r, E, A, I

u2

2

u3

2 r, E, A, I

3

L /2

L /2

Fig. 4.16 Finite element discretization of a propped cantilever beam. The two beam elements are identical.

The element mass matrix (valid for both elements) is ⎡ 156

⎢ ⎢ ⎢ L ⎢ ⎢ 22 2 ρA(L/2) ⎢ ⎢ me = ⎢ 420 ⎢ ⎢ 54 ⎢ ⎢ ⎣ L −13 2

L 2 2 L 4 2 L 13 2 2 L −3 2

⎤ L 2 ⎥ 2 ⎥ L ⎥ ⎥ −3 ⎥ 2 ⎥ ⎥ L ⎥ ⎥ −22 ⎥ 2 ⎥ 2 ⎥ ⎦ L 4 2 −13

54

22

13

L 2

156 −22

L 2

and the stiffness matrix (valid for both elements) is ⎡ 12

⎢ ⎢ ⎢ ⎢ ⎢ 6L EI ⎢ ⎢ ke = (L/2)3 ⎢ ⎢−12 ⎢ ⎢ ⎢ ⎣ L 6 2

L 2 2 L 4 2 L −6 2 2 L 2 2 6

−12 −6

L 2

12 −6

L 2

⎤ L 2 ⎥ 2 ⎥ L ⎥ ⎥ 2 ⎥ 2 ⎥ ⎥. L ⎥ −6 ⎥ ⎥ 2 ⎥ 2 ⎥ L ⎦ 4 2 6

124

Finite element method

With the boundary conditions, we may write for the ﬁrst element ⎡

X

⎢ ⎡ ⎤ ⎡ ⎤ ⎢X y1 0 ⎢ ⎢ ⎢ θ1 ⎥ ⎢ 0 ⎥ EI ⎢ ⎥ = ⎢ ⎥ → k1 = u=⎢ ⎢ ⎣y2 ⎦ ⎣y2 ⎦ (L/2)3 ⎢X ⎢ ⎢ θ2 θ2 ⎣ X

X

X

X

X

X

12 −6

X

X

⎤

⎥ ⎥ ⎥ ⎥ L ⎥ −6 ⎥ 2 ⎥ ⎥ 2 ⎥ L ⎦ 4 2 X

L 2

and for element 2 that ⎡ ⎢ 12 ⎢ ⎡ ⎤ ⎡ ⎤ ⎢ y2 y2 ⎢ L ⎢6 ⎢θ2 ⎥ ⎢θ2 ⎥ EI ⎢ 2 ⎥ = ⎢ ⎥ → k2 = u=⎢ ⎢ ⎣y3 ⎦ ⎣ 0 ⎦ (L/2)3 ⎢ ⎢X ⎢ θ3 θ3 ⎢ ⎣ L 6 2

L 2 2 L 4 2 6

X 2 L 2 2

X X X X

⎤ L 2 ⎥ 2 ⎥ ⎥ L ⎥ ⎥ 2 2 ⎥ ⎥. ⎥ X ⎥ ⎥ 2 ⎥ L ⎦ 4 2 6

We proceed in a similar way for the mass matrix and obtain the ﬁnite element equilibrium equation Mu¨ + Ku = 0 to be ⎤ 13 ⎡ 156 0 − L ⎡ ⎤ ⎢ 4 ⎥ 172 ⎥ y¨2 ⎢ ⎥ ⎢ ⎥ EI ⎢ ρAL ⎢ 3 ⎢θ¨2 ⎥ + ⎢ ⎢ 0 L2 − L2 ⎥ ⎣ ⎦ L3 ⎣ 0 420 ⎢ 8 ⎥ ⎥ ⎢ ⎣ 13 24L 1 2 ⎦ θ¨3 3 L − L − L2 2 4 8 ⎡

0 16L2 4L2

⎤⎡ ⎤ ⎡ ⎤ y2 0 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢θ2 ⎥ = ⎢0⎥ . 4L2 ⎥ ⎦⎣ ⎦ ⎣ ⎦ 2 8L θ3 0

24L

4.4.3.4 Static analysis of a single square element. We will examine one further example before moving on; a single, two-dimensional, four-noded, isoparametric element subjected to a static force. We take the material behaviour to be elastic, and assume conditions of plane strain. The problem is shown schematically in Fig. 4.17, together with the elastic constants.

Finite element equilibrium equations

125

Geometry a = 1 mm 1

4

2

3

Material data E = 210 N / mm2 n = 0.25

a

Loading F = 10 N F

a

Discretization data (nodal coordinates) n1(0, 1), n2(0, 0), n3(1, 0), n4(1, 1)

45°

Fig. 4.17 Schematic diagram of a single, four-noded element subjected to force F directed at 45◦ to the vertical.

The shape functions for this element are as follows: Element local coordinate system 1 N1 (ξ, η) = (1 − ξ )(1 − η), h 4 1 4 3 N2 (ξ, η) = (1 + ξ )(1 − η), 1 4 1 N3 (ξ, η) = (1 + ξ )(1 + η), –1 1 4 j –1 1 N4 (ξ, η) = (1 − ξ )(1 + η). 1 2 4 We will ﬁnd that we need to carry out integrations (in order to obtain the stiffness matrix) of the shape functions. Previously, we have been able to do the integrations analytically. Here, we will need to use a numerical technique. Often, in order to simplify the process, the integration is carried out with respect to a particular point in the element; this point is known as an integration point. The integration will be performed numerically using a single integration point at P (ξ, η) = P (0, 0). Integrals over the element domain of the type I= f (ξ, η) dV

are expressed in the element local coordinate system by use of the Jacobian, J , as 1 1 I= f (ξ, η) det[J ] dξ dη, (4.95) −1 −1

where the Jacobian for a two-dimensional problem is given by ⎡ ∂X ∂X ⎤ ⎢ ∂ξ ∂η ⎥ ⎥ J =⎢ ⎣ ∂Y ∂Y ⎦ . ∂ξ

∂η

(4.96)

126

Finite element method

The integral in (4.95) will be approximated using Gauss quadrature (details may be found in any of the more specialized books on ﬁnite elements) by I≈

1

1

−1 −1

det[J ] dξ dη f (ξ, η).

The shape function derivatives at the integration point P (ξ, η) = P (0, 0) are obtained from ∂N ∂N ∂ξ ∂N ∂X −1 (4.97) = = ∂X ∂ξ ∂X ∂ξ ∂ξ and the shape function derivatives with respect to element local coordinates are given by ⎤ ∂N1 (0, 0) ∂N1 (0, 0) ⎥ ⎢ ∂ξ ∂η ⎥ ⎢ ⎡ ⎥ ⎢ (−1)(1 − η)|(0,0) ⎢ ∂N2 (0, 0) ∂N2 (0, 0) ⎥ ⎥ ⎢ ⎢ ⎥ 1 ⎢ (1)(1 − η)|(0,0) ∂ξ ∂η ∂N (0, 0) ⎢ ⎥= ⎢ =⎢ ⎥ 4 ⎢ (1)(1 + η)| ⎢ ∂N (0, 0) (0, 0) ∂N ∂ξ 3 3 (0,0) ⎥ ⎢ ⎣ ⎥ ⎢ ∂ξ ∂η ⎥ ⎢ (−1)(1 + η)|(0,0) ⎥ ⎢ ⎣ ∂N4 (0, 0) ∂N4 (0, 0) ⎦ ∂ξ ∂η ⎡ ⎤ −1 −1 ⎢ ⎥ 1 −1⎥ 1⎢ ⎥. = ⎢ 4⎢ 1⎥ ⎣1 ⎦ −1 1 ⎡

(1 − ξ )(−1)|(0,0)

⎤

⎥ (1 + ξ )(−1)|(0,0) ⎥ ⎥ (1 + ξ )(1)|(0,0) ⎥ ⎦ (1 − ξ )(1)|(0,0)

In order to determine the Jacobian matrix ∂X/∂ξ , let us ﬁrst write down the relationship between element and nodal positions; that is, X = N1 X1 + N2 X2 + N3 X3 + N4 X4 , Y = N1 Y1 + N2 Y2 + N3 Y3 + N4 Y4 . We see, therefore, that ∂N1 ∂NI ∂N2 ∂N3 ∂N4 ∂X = X1 + X2 + X3 + X4 = XI ∂ξ ∂ξ ∂ξ ∂ξ ∂ξ ∂ξ

Finite element equilibrium equations

127

and similarly for other terms. The Jacobian matrix, therefore, from (4.96) is ⎡ ∂X ∂X ⎤ ⎡ ∂N ∂NI ⎤ I XI XI ⎢ ∂ξ ⎢ ∂η ⎥ ∂η ⎥ ∂ξ ⎥=⎢ ⎥ J =⎢ ⎣ ∂Y ∂Y ⎦ ⎣ ∂NI ∂NI ⎦ YI YI ∂ξ ∂η ∂ξ ∂η ⎤ ⎡ ∂N1 ∂N1 ⎢ ∂ξ ∂η ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ ∂N2 ∂N2 ⎥ ⎥ ⎢ ∂ξ ∂η ⎥ X1 X2 X3 X4 ⎢ ⎥. ⎢ = ⎥ Y1 Y2 Y3 Y4 ⎢ ∂N ∂N 3 3 ⎥ ⎢ ⎥ ⎢ ∂η ⎥ ⎢ ∂ξ ⎥ ⎢ ⎣ ∂N4 ∂N4 ⎦ ∂η ∂ξ This can be written in the general form given in Equation (4.61) as J =X

∂N . ∂ξ

With the shape functions given above, evaluated at the integration point, and the nodal coordinates, the Jacobian becomes ⎡ ⎤ −1 −1 ⎥ ∂X ∂N X1 X2 X3 X4 1 ⎢ ⎢ 1 −1⎥ =X = ⎣ 1⎦ Y1 Y2 Y3 Y4 4 1 ∂ξ ∂ξ −1 1 1 −X1 + X2 + X3 − X4 −X1 − X2 + X3 + X4 = −Y1 − Y2 + Y3 + Y4 4 −Y1 + Y2 + Y3 − Y4 1 −0 + 0 + 1 − 1 −0 − 0 + 1 + 1 = 4 −1 + 0 + 0 − 1 −1 − 0 + 0 + 1 1 0 2 0 0.5 = . = −0.5 0 4 −2 0 The determinant of the Jacobian is ∂X 0 det[J ] = det = det −0.5 ∂ξ and its inverse is

∂X ∂ξ

−1

0 = 2

0.5 = 0.25 0

−2 . 0

128

Finite element method

Finally, the shape function derivatives with respect to the spatial (here, equivalent to the material) coordinates are ⎡ ⎤ −1 −1 −1 ∂N 1⎢ ∂N ∂X 1 −1⎥ 0 −2 ⎢ ⎥ = ⎣ = 1⎦ 2 0 ∂X ∂ξ ∂ξ 4 1 −1 1 ⎡ ⎤ ⎡ ⎤ −1 −1 −1 −1 ⎢ 1 −1⎥ 0 −0.5 1⎢ 1 −1⎥ 0 −2 ⎢ ⎥ ⎢ ⎥ =⎣ = ⎣ 1⎦ 2 0 1 1 ⎦ 0.5 0 4 1 −1 1 −1 1 ⎡ ⎤ −0.5 0.5 ⎢−0.5 −0.5⎥ ⎥ =⎢ ⎣ 0.5 −0.5⎦ . 0.5

0.5

The B matrix can now be obtained (for plane strain) from (4.81) ⎡ ⎤ ∂NI (0, 0) 0 ⎢ ⎥ ∂x ⎢ ⎥ ⎢ ∂NI (0, 0) ⎥ ⎢ ⎥ 0 BI = ⎢ ⎥, ∂y ⎢ ⎥ ⎢ ⎥ ⎣ ∂NI (0, 0) ∂NI (0, 0) ⎦ 0 0.5 −0.5

−0.5 0 −0.5

0 −0.5 −0.5

The elasticity matrix for plane strain is ⎡ λ + 2µ λ C=⎣ λ λ + 2µ 0 0

0.5 0 0 −0.5 −0.5 0.5 ⎤ 0 0⎦ , µ

νE = 84 N/mm2 , (1 + ν)(1 − 2ν) E = 84 N/mm2 , µ=G= 2(1 + ν) ⎤ ⎡ 252 84 0 C = ⎣ 84 252 0 ⎦ N/mm2 . 0 0 84 λ=

-------

−0.5 B=⎣ 0 0.5

∂x -------

∂y -------

⎡

0.5 0 0.5

⎤ 0 0.5⎦ . 0.5

Finite element equilibrium equations

129

The stiffness matrix can then be determined by using the approximate integration formula given above as k=

B CB dV = T

V

0

1 1

B CB dx dy = T

0

1

−1 −1

-------

≈ [B(0, 0)]T CB(0, 0) det[J (0, 0)].2.2 ⎤ ⎡ −0.5 0 0.5 ⎢ 0 0.5 −0.5⎥ ⎥ ⎢ ⎥⎡ ⎢−0.5 ⎤ 0 −0.5 ⎥ 252 84 ⎢ 0 ⎥ ⎢ −0.5 −0.5⎥ ⎣ ⎢ 0 =⎢ ⎥ 84 252 0 ⎦ 0 −0.5⎥ ⎢ 0.5 ⎥ 0 ⎢ 0 84 ⎢ 0 −0.5 0.5 ⎥ ⎥ ⎢ ⎣ 0.5 0 0.5 ⎦ 0 0.5 0.5 ⎡ −0.5 0 −0.5 0 0.5 0 ×⎣ 0 0.5 0 −0.5 0 −0.5 0.5 −0.5 −0.5 −0.5 −0.5 0.5 ⎡ 84 −42 42 0 −84 42 −42 ⎢−42 84 0 −42 42 −84 0 ⎢ ⎢ 42 0 84 42 −42 0 −84 ⎢ ⎢ 42 84 0 42 −42 ⎢ 0 −42 =⎢ 42 −42 0 84 −42 42 ⎢−84 ⎢ ⎢ 42 −84 0 42 −42 84 0 ⎢ ⎣−42 0 −84 −42 42 0 84 0 42 −42 −84 0 −42 42 ⎡ 84 −42 42 0 −84 42 −42 ⎢−42 84 0 −42 42 −84 0 ⎢ ⎢ 42 0 84 42 −42 0 −84 ⎢ ⎢ 42 84 0 42 −42 ⎢ 0 −42 =⎢ 42 −42 0 84 −42 42 ⎢−84 ⎢ ⎢ 42 −84 0 42 −42 84 0 ⎢ ⎣−42 0 −84 −42 42 0 84 0 42 −42 −84 0 −42 42 -------

1

B T CB det[J ] dξ dη

⎤ 0.5 0 1 0 0.5⎦ 4 4 0.5 0.5 ⎤ 0 42 ⎥ ⎥ −42 ⎥ ⎥ ⎥ −84 ⎥ 1 ⎥ 4 0 ⎥4 ⎥ −42 ⎥ ⎥ 42 ⎦ 84 ⎤ 0 42 ⎥ ⎥ −42 ⎥ ⎥ ⎥ −84 ⎥ ⎥. 0 ⎥ ⎥ −42 ⎥ ⎥ 42 ⎦ 84

-------

The equilibrium equation for this quasi-static problem is ku = f ,

(4.98)

130

Finite element method

⎡

84 ⎢−42 ⎢ ⎢ 42 ⎢ ⎢ ⎢ 0 ⎢ ⎢−84 ⎢ ⎢ 42 ⎢ ⎣−42 0

−42 84 0 −42 42 −84 0 42

42 0 84 42 −42 0 −84 −42

0 −42 42 84 0 42 −42 −84

−84 42 −42 0 84 −42 42 0

42 −84 0 42 −42 84 0 −42

−42 0 −84 −42 42 0 84 42

0 42 −42 −84 0 −42 42 84

⎡

⎤⎡

Rx1 Ry1 Rx2 Ry2

⎤

⎤ ⎢ ⎥ 0 ⎢ ⎥ ⎥⎢ 0 ⎥ ⎢ ⎥ ⎥⎢ ⎥ ⎢ ⎥ ⎥⎢ 0 ⎥ ⎢ ⎥ ⎥⎢ ⎥ ⎢ ⎥ ⎥⎢ ⎥ ⎢ ⎥ π ⎥⎢ 0 ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ = ⎢ F cos ⎥ ⎥ ⎢ux3 ⎥ ⎢ ⎥ 4 ⎥⎢ ⎥ ⎢ π⎥ ⎥ ⎢uy3 ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ ⎢−F cos ⎥ ⎦⎣ 0 ⎦ ⎢ 4⎥ ⎢ ⎥ ⎣ Rx4 ⎦ uy4 0

so that with the boundary conditions it simpliﬁes to ⎤ ⎡ ⎤⎡ ⎤ ⎡ √ 10 2/2 84 −42 0 ux3 ⎢ ⎥⎢ ⎥ ⎢ √ ⎥ ⎢−42 ⎥ ⎢uy3 ⎥ = ⎢−10 2/2⎥ . 84 −42 ⎦ ⎣ ⎦⎣ ⎦ ⎣ uy4 0 −42 84 0 The solution is obtained from u = k −1 f , ⎡ ⎤ ⎡ 0.017857 0.011905 ux3 ⎢ ⎥ ⎢ ⎢uy3 ⎥ = ⎢0.011905 0.023810 ⎣ ⎦ ⎣ uy4 0.005952 0.011905 ⎡ ⎤ ⎡ ⎤ ux3 0.04209 ⎢ ⎥ ⎢ ⎥ ⎢uy3 ⎥ = ⎢−0.08418⎥ mm. ⎣ ⎦ ⎣ ⎦ uy4 −0.04209

⎤ √ 10 2/2 ⎥⎢ √ ⎥ ⎢−10 2/2⎥ , 0.011905⎥ ⎦ ⎦⎣ 0.017857 0

0.005952

⎤⎡

The reactions can be obtained from ⎡

84 ⎢−42 ⎢ ⎢ 42 ⎢ ⎢ ⎢ 0 ⎢ ⎢−84 ⎢ ⎢ 42 ⎢ ⎣−42 0

−42 84 0 −42 42 −84 0 42

42 0 84 42 −42 0 −84 −42

0 −42 42 84 0 42 −42 −84

−84 42 −42 0 84 −42 42 0

42 −84 0 42 −42 84 0 −42

−42 0 −84 −42 42 0 84 42

0 42 −42 −84 0 −42 42 84

⎤⎡

⎤

⎡

Rx1 Ry1 Rx2 Ry2

⎤

⎢ ⎥ 0 ⎢ ⎥ ⎥⎢ 0 ⎥ ⎢ ⎥ ⎥⎢ ⎥ ⎢ ⎥ ⎥⎢ 0 ⎥ ⎢ ⎥ ⎥⎢ ⎥ ⎢ ⎥ ⎥⎢ ⎥ ⎢ ⎥ π 0 ⎥⎢ ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ = ⎢ F cos ⎥ , ⎥ ⎢ux3 ⎥ ⎢ ⎥ 4 ⎥⎢ ⎥ ⎢ π⎥ ⎥ ⎢uy3 ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ ⎢−F cos ⎥ ⎢ ⎦⎣ 0 ⎦ 4⎥ ⎢ ⎥ ⎣ Rx4 ⎦ uy4 0

Finite element equilibrium equations

131

√ Rx1 = −84ux3 + 42uy3 + 0uy4 = −10 2/2N, √ Ry1 = 42ux3 − 84uy3 + 42uy4 = 10 2/2N, Rx2 = −42ux3 + 0uy3 − 42uy4 = 0, Ry2 = 0ux3 + 42uy3 − 84uy4 = 0, Rx4 = 42ux3 + 0uy3 + 42uy4 = 0. We can carry out an equilibrium check as follows: √ √ √ 10 2 10 2 10 2 =− +0+0+ = 0, Fx = Rx1 + Rx2 + Rx4 + 2 2 2 √ √ √ F 2 10 2 10 2 = +0− = 0. Fy = Ry1 + Ry2 − 2 2 2 The element strains at the integration point may be determined as ε(ξ, η) = ε(0, 0) ≈

NNODE

B I (0, 0) · uI

I =1

⎤ 0.021045 = ⎣ 0.021045 ⎦ −0.08418 ⎡

0 −0.5 −0.5

-------

−0.5 0 −0.5

0.5 0 0 −0.5 −0.5 0.5

0.5 0 0.5

0.5 0 0 −0.5 −0.5 0.5

-------

−0.5 0 ⎣ = 0 0.5 0.5 −0.5

0 −0.5 −0.5

-------

⎡

−0.5 0 −0.5

-------

0 0.5 −0.5

-------

−0.5 =⎣ 0 0.5

-------

⎡

⎡

0.5 0 0.5

⎤ 0 ⎢ 0 ⎥ ⎢ ⎥ ⎤⎢ 0 ⎥ ⎥ 0 ⎢ ⎢ ⎥ 0 ⎢ ⎥ 0.5⎦ ⎢ ⎥ ⎢ux3 ⎥ 0.5 ⎢ ⎥ ⎢uy3 ⎥ ⎢ ⎥ ⎣ 0 ⎦ uy4 ⎤ ⎡ 0 ⎥ ⎢ 0 ⎥ ⎢ ⎥ ⎢ ⎤⎢ 0 ⎥ 0 ⎢ ⎥ 0 ⎥ ⎢ 0.5⎦ ⎢ ⎥ ⎢ 0.04209 ⎥ ⎥ 0.5 ⎢ ⎢−0.08418⎥ ⎥ ⎢ ⎦ ⎣ 0 −0.04209

132

Finite element method

and the stresses are given by ⎤ ⎤⎡ 0.021045 252 84 0 σ(ξ, η) = Cε(ξ, η) = ⎣ 84 252 0 ⎦ ⎣ 0.021045 ⎦ −0.08418 0 0 84 ⎤ ⎡ √ ⎡ ⎤ 10√2/2 7.071068 ⎦ ⎣ ⎣ = 7.071068 = 10 2/2 ⎦ N/mm2 . √ −7.071068 −10 2/2 ⎡

A further check is that the internal forces at nodal points must be equal to nodal external forces (note that the reactions are external forces too): ⎡ int ⎤ fx1 ⎢ ⎥ ⎢f int ⎥ ⎢ y1 ⎥ ⎢ ⎥ ⎢f int ⎥ ⎢ x2 ⎥ ⎢ ⎥ ⎢f int ⎥ 1 1 ⎢ y2 ⎥ T ⎥= B σ dV = B T σ dx dy f int = ⎢ ⎢ int ⎥ 0 0 V ⎢fx3 ⎥ ⎢ ⎥ ⎢ int ⎥ ⎢fy3 ⎥ ⎢ ⎥ ⎢ int ⎥ ⎢fx4 ⎥ ⎣ ⎦ int fy4 1 1 1 1 1 B T σ det[J ] dξ dη = B T σ dξ dη = 4 −1 −1 −1 −1 √ ⎤ ⎡ −10 2/2 ⎡ ⎤ −0.5 0 0.5 ⎢ √ ⎥ ⎢ 10 2/2 ⎥ ⎢ ⎥ ⎢ ⎥ 0.5 −0.5⎥ ⎢ 0 ⎢ ⎥ ⎢ ⎥ ⎥ 0 ⎢−0.5 0 −0.5⎥ ⎡ √ ⎤ ⎢ ⎢ ⎥ ⎢ ⎥ 10 2/2 ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ 0 ⎢ 0 −0.5 −0.5⎥ ⎢ √ ⎥ ⎢ ⎥ T 1 T ⎢ ⎥ ⎥ ⎢ =B σ 4=B σ=⎢ 10 2/2 ⎦ = ⎢ √ ⎥ N. ⎥ ⎣ ⎢ 4 0 −0.5⎥ ⎢ 0.5 10 2/2 ⎥ √ ⎢ ⎥ ⎢ ⎥ ⎢ √ ⎥ ⎢ 0 −0.5 0.5 ⎥ −10 2/2 ⎢ ⎥ ⎢ ⎥ ⎢−10 2/2⎥ ⎢ ⎥ ⎢ ⎥ 0 0.5 ⎦ ⎣ 0.5 ⎢ ⎥ 0 ⎣ ⎦ 0 0.5 0.5 0 We need to summarize a few important points before leaving this section. In all the examples considered, we have used only one or two ﬁnite elements. This is intended

Finite element equilibrium equations

133

to aid in the development of understanding of the ﬁnite element method rather than to suggest that practical problems can be solved in this way. Most engineering problems require very large numbers of ﬁnite elements in order to obtain an accurate representation and solution. Naturally, the calculations are then carried out on a computer. We should also note that we have gone on to determine solutions for only quasi-static problems. This required the solution of the Equation (4.98). However, we have set up the ﬁnite element equilibrium (also often known as momentum balance) equations for a number of dynamic problems which we have not attempted to solve. Solution of these problems requires in general the numerical integration of the momentum balance Equation (4.85), using, for example, the explicit central difference time integration scheme, which is introduced brieﬂy later on, or an implicit scheme. So far, in this chapter, we have been concerned with both geometrically linear and non-linear problems in which the material behaviour has always been assumed to be linear (elasticity). We shall continue by introducing incremental ﬁnite element techniques for non-linear material behaviour; that is, in particular, for plasticity.

4.4.4

Finite element formulation for plasticity

The equilibrium equations derived in (4.71)–(4.75) from virtual work are applicable in general to linear and non-linear material behaviour. In order to address a particular example, we return to the equilibrium Equation (4.69) but for simplicity, assume quasistatic conditions and so ignore inertia terms, and we consider small deformations. Using Voigt notation the equation of virtual work becomes δW = δD T σ dV − t · δv dA = 0.

∂

With the ﬁnite element discretization as before, the equation becomes δW =

NNODE

T B I dv I

I =1

σ dV −

∂

t·

NNODE

NI δv I dA.

I =1

For small strain elastic–plastic material behaviour, we σ = Cεe = C(ε − εp ) so δW =

NNODE

I =1

T B I δv I

C(ε − εp ) dV −

∂

t·

NNODE I =1

NI δv I dA

134

Finite element method

and with the ﬁnite element discretization for the strain presented in Section 4.4.3, this becomes ⎛ ⎞ NNODE δW I = δv TI ⎝ B TI CB J dV ⎠ uJ I,J =1

− δv TI

NNODE

I =1

B TI Cεp dV

− δv TI

NNODE I =1

∂

NI t dA.

As before, for an arbitrary virtual velocity, we may then write the element equilibrium equation as (4.99) ku − f p = f , where fp =

NNODE I =1

B TI Cεp dV .

In contrast to linear elastic problems in which there exists a unique relationship between stress and elastic strain, no such uniqueness holds for plasticity problems. An incremental approach to solving (4.99) is therefore almost always necessary, and to emphasize this, the displacement, plastic strain, and external force terms are written as increments so that ku − f p = f (4.100) and f p =

NNODE I =1

B TI Cεp dV .

(4.101)

Equation (4.100) may alternatively be written as ku = f ,

(4.102)

where f = f p + f . 4.4.4.1 Single truss element undergoing elastic–plastic deformation. We now return to the single truss element which we examined for the case of elastic material behaviour in Section 4.4.2.1. The problem is shown in Fig. 4.10(a) and the single element discretization in 4.10(b). For this problem, the B matrix, and the stiffness matrix, k, remain unchanged as 1 EA 1 −1 B = [−1 1], k= L L −1 1

Finite element equilibrium equations

135

and we write the incremental external force vector as F1 f = . P The plasticity ‘force’ is determined from (4.101) for this element as 1 1 −1 T p p p −1 p Eε A det(J ) dξ = EAε B Cε dV = f = 1 1 ξ =0 L so that from (4.100) the equilibrium equation becomes EA 1 −1 u1 −1 F1 . − EAεp = u2 P 1 L −1 1 With the boundary condition that u1 = 0, this reduces to EA u2 − EAεp = P . L Rearranging gives P L + Lε p . (4.103) u2 = EA In the absence of plasticity, this just gives us an incremental form of the expression we obtained before for elasticity in Section 4.4.2.1. For the case of plasticity, however, the increment in displacement now becomes that due to the elastic deformation together with that resulting from the plastic strain, which unsurprisingly in this small strain formulation has magnitude Lεp . To demonstrate further the need for an incremental approach, let us now assign elastic linear strain hardening plasticity properties to the rod material and determine the rod extension on application of a given force, P . In Section 2.4.2, we saw that for uniaxial linear isotropic hardening the relation between the increment in uniaxial stress and plastic strain was given by σ εp = h in which h is the strain hardening constant. Writing σ = P /A gives P ε p = Ah and substituting into (4.102) gives P L 1 1 P L LP + = + . (4.104) u2 = EA Ah A E h Therefore, the incremental displacement for elastic and elastic–plastic conditions becomes P L . Elastic : σ < σy , u2 = EA 1 P L 1 + . Elastic–plastic : σ ≥ σy , u2 = A E h

136

Finite element method

11 N L = 10 mm

E = 1000 MPa A = 1.0 mm2 sy = 10 MPa h = 100 MPa

Fig. 4.18 A uniform bar under axial loading with the properties shown.

Let us analyse incrementally the problem shown in Fig. 4.18. We will apply the load incrementally. The ﬁrst load increment, however, will be chosen to cause ﬁrst yield. That is, P1 = σy A = 10 N. The displacement increment is given by 10 × 10 P L = = 0.1 mm u(1) = EA 1000 × 1 so u(1) = u(0) + u(1) = 0 + 0.1 = 0.1 mm. Subsequent displacement increments must take account of the plasticity so that u(2) =

1 × 10 10 × 1 P L LP + = + = 0.11 mm EA Ah 1000 × 1 1 × 100

and u(2) = u(1) + u(2) = 0.1 + 0.11 = 0.21 mm. We see from Equation (4.104) that since the rate of hardening is constant (i.e. h is ﬁxed), the displacement—load relationship becomes independent of increment size, once the material has yielded. However, were we to introduce non-linear hardening where, for example, h depends on plastic strain, Equation (4.104) shows that the displacement—load relationship then becomes dependent on the increment size.

4.5 4.5.1

Integration of momentum balance and equilibrium equations Explicit integration using the central difference method

The ﬁnite element discretization of the momentum balance equation for a damped system can be expressed in matrix form as follows: Mu¨ + Cu˙ + Fint = Fext , where M is the mass matrix, Fint the internal force vector, and Fext the external force vector. The integration of the equations can be carried out by means of the explicit central difference time integration scheme. The scheme is derived from Taylor series

Integration of momentum balance and equilibrium equations

137

expansions of the displacements, u, as follows. t 2 + ··· 2 t 2 ˙ ¨ u(t − t) = u(t) − u(t)t + u(t) − ··· . 2 The central difference approximations are obtained taking the difference of the above expressions to give the velocity uN+1 − uN −1 u˙ N = 2t and by summing the expressions for the accelerations ˙ ¨ u(t + t) = u(t) + u(t)t + u(t)

u¨ N =

uN+1 − 2uN + uN −1 , (t)2

where uN = u(tN ). Assuming that the acceleration is constant between tN and tN +1 the central difference approximations can be rearranged to give the following second-order integration scheme 1 uN+1 = uN + u˙ N t + u¨ N (t)2 , 2 1 u˙ N+1 = u˙ N + (u¨ N + u¨ N +1 )t. 2 These are more commonly rewritten by deﬁning the intermediate velocities based on the assumption that the acceleration is constant between t0 and t0+1/2 as well as between tN−1/2 and tN+1/2 so that 1 u˙ 1/2 = u˙ 0 + u¨ 0 t 2 to give the leap frog explicit method u˙ N+1/2 = u˙ N−1/2 + u¨ N t, uN+1 = uN + u˙ N+1/2 t. The central difference method can be applied with a varying time increment (which is particularly important if the response of the continuum is non-linear), as illustrated in Fig. 4.19. Let tN+1 be the time increment between tN and tN +1 with uN = u(tN ) as illustrated in Fig. 4.19. The mid-step velocities are deﬁned by ˙ N−1/2 ), u˙ N−1/2 = u(t

˙ N +1/2 ), u˙ N +1/2 = u(t

138

Finite element method ∆tN

∆tN + 1

t N –1

tN

t N +1

t N + 1/2

t N –1/2

t

üN N –1/2

N +1/2

uN

uN +1

Fig. 4.19 Central difference integration scheme.

where 1 1 (tN−1 + tN ), tN +1/2 = (tN + tN +1 ). 2 2 The central difference formula for velocity is tN −1/2 =

u˙ N+1/2 =

uN+1 − uN , tN +1

while the central difference formula for acceleration is u¨ N =

u˙ N+1/2 − u˙ N −1/2 , tN+1/2

where 1 (tN + tN +1 ). 2 The discretization of the momentum balance equation for an undamped system can be obtained by substituting the acceleration term with its ﬁnite difference approximation as follows: u˙ N+1/2 − u˙ N−1/2 int ext M + FN = FN , tN+1/2 tN+1/2 =

which yields u˙ N+1/2 = M−1 (Fext − Fint )tN +1/2 + u˙ N −1/2 and uN+1 = uN + u˙ N+1/2 tN +1 . Subsequently, the internal and external force vectors can be calculated as int FN+1 = Fint (uN+1 ),

ext FN+1 = Fext (uN +1 ),

which completes the Nth time step. Furthermore, if the mass matrix is diagonalized the system of differential equations uncouples and can be solved independently for each degree of freedom (see, e.g. Newland).

Integration of momentum balance and equilibrium equations

139

4.5.1.1 Stability of the explicit time stepping scheme. The solution of a SDOF equilibrium equation u¨ + ω2 u = 0 can be obtained using the central difference time stepping scheme as follows u¨ N =

uN+1 − 2uN + uN −1 = −ω2 uN (t)2

giving the difference equation uN+1 − (2 − ω2 (t)2 )uN + uN −1 = 0. Trying solutions uN = An where A is the ampliﬁcation factor gives A2 − (2 − ω2 (t)2 )A + 1 = 0. The roots of this polynomial are

ω2 (t)2 A= 1− 2

%

±

ω2 (t)2 1− 2

2 − 1.

For stability |A| ≤ 1, which gives the stability condition as t ≤

2 . ω

For a general multidegree of freedom system, the stability condition becomes t ≤

2 , ωmax

where ωmax = max{ωi } i

is the element maximum eigenvalue. A conservative estimate of the stable time increment is given by the following minimum taken over all the elements t ≤ min

Lc , cd

where Lc is the characteristic element length and cd is the current effective dilatational wave speed of the material.

140

4.5.2

Finite element method

Introduction to implicit integration

Implicit integration schemes are often preferred to their explicit counterparts since they involve the determination of a residual force at each step and iteration within the step to minimize the residual force to within a speciﬁed tolerance. We brieﬂy introduce three techniques; the tangential stiffness method, the initial tangential stiffness method, and the Newton–Raphson method. We conﬁne ourselves here to quasi-static problems so assume inertia effects are negligible. 4.5.2.1 Tangential stiffness method. The discretized static equilibrium equation given in (4.102), for example, will not generally be satisﬁed unless a convergence occurs which can be expressed in terms of residual forces as follows k(u)u − f = Ψ = 0. The iteration starts from an initially guessed solution u0 and the corresponding tangential stiffness matrix k(u0 ). The residual forces are calculated from Ψ0 = k(u0 )u0 − f . The correction u is calculated as follows: un = [K(un )]−1 Ψn

(4.105)

and an improved solution is then obtained as follows: un+1 = un + un . The process continues until the residual forces Ψn are smaller than a speciﬁed tolerance. 4.5.2.2 Initial tangential stiffness method. The initial tangential stiffness method differs from the previous method only in that the correction to the displacement, given in Equation (4.105), is now calculated always based upon the initial tangential stiffness matrix so that un = [k(u0 )]−1 Ψn and as before, the improved solution is obtained as un+1 = un + un and the process continues until the residual forces Ψn are smaller than a speciﬁed tolerance.

Integration of momentum balance and equilibrium equations

141

4.5.2.3 Newton–Raphson method. As in the previous methods, the residual force is determined from = k(u)u − f = 0. (4.106) Using a Taylor expansion, may be approximated by ∂(u) (u) + (4.107) u + O(u2 ) = 0. ∂u The matrix J = ∂/∂u is called the Jacobian (which has nothing to do with the Jacobian introduced above for the mapping of spatial to local element conﬁgurations), or effective tangent stiffness, and from (4.106) it can be seen that this comprises a term corresponding to the internal forces, termed the tangent stiffness matrix, and a further term corresponding to the ‘external’ forces, called the load stiffness matrix. Equation (4.107) provides a linearization of (4.106) and may be written as + Ju = 0 so that J(un )un = −(un ) and the displacement is updated by un+1 = un + un . The iteration continues until the tolerance limit on residual force is achieved. The two schemes introduced above, namely explicit and implicit integration, may be used for the integration of the momentum balance, or equilibrium, ﬁnite element equations. In implementing plasticity models into ﬁnite element formulations, it is often necessary, in addition, to integrate a set of constitutive equations (e.g. to give the plastic strain increment). For this additional integration, it is also possible to employ either implicit or explicit integration methods. In the overall solution process, therefore, there are several possible combinations of implicit and explicit integration. Finite element methods which employ implicit schemes for the integration of the momentum balance, or equilibrium equations, regardless of whether the constitutive equations are integrated using implicit or explicit integration, are referred to as implicit ﬁnite element methods. Similarly, ﬁnite element methods which employ explicit schemes for the integration of the momentum balance, or equilibrium equations, are called explicit ﬁnite element methods. Both implicit and explicit formulations are available in ABAQUS. It can be seen that the implicit scheme offers the more robust overall approach, because of the iteration necessary in order to achieve convergence. Explicit schemes, however, can often produce more rapid solutions, and are more appropriate for dynamic analyses. Care has to be taken, however, in choosing time step size and ensuring the calculated solution does not drift away from the true solution. We shall examine this further in the context of integration of constitutive equations in Chapter 5.

142

Finite element method

Further reading Bathe, K.-J. (1996). Finite Element Procedures. Prentice Hall, New Jersey, revised edition. Belytschko, T., Liu, K.W., and Moran, B. (2000). Non-linear Finite Element Analysis for Continua and Structures. John Wiley & Sons, New York. Bonet, J. and Wood, R.D. (1997). Non-linear Continuum Mechanics for Finite Element Analysis. Cambridge University Press. Hinton, E. and Owen, D.R.J. (1979). An Introduction to Finite Element Computations. Pineridge Press, Swansea. Newland, D.E. (1989). Mechanical Vibration Analysis and Computation. Longman Scientiﬁc and Technical, John Wiley and Sons, New York. Owen, D.R.J. and Hinton, E. (1980). Finite Elements in Plasticity: Theory and Practice. Pineridge Press, Swansea. Timoshenko, S. and Goodier, J.N. (1983). Theory of Elasticity. McGraw-Hill, New York. Zienkiewicz, O.C. and Taylor, R.L. (1989). The Finite Element Method. McGraw-Hill, London, 4th edition.

5. Implicit and explicit integration of von Mises plasticity

5.1

Introduction

In this chapter, we shall return to the constitutive equations for plasticity introduced in Chapter 2 and see how they may be integrated and how the Jacobian or tangent stiffness may be obtained from them. We shall explore both implicit and explicit schemes for the integration of the constitutive equations. To start, we shall consider small strain, time-independent, linear isotropic hardening plasticity before looking at kinematic hardening and viscoplasticity. First, we return to the determination of the plastic multiplier.

5.2

Implicit and explicit integration of constitutive equations

We saw from Chapter 2 that the yield function for isotropic hardening can be written 1/2 3

f = σe − r − σy = σ :σ − r − σy = 0 (5.1) 2 and that the plastic multiplier, in principal stress space is given by dλ =

(∂f/∂σ) · C dε , (∂f/∂σ) · C(∂f/∂σ) − (∂f/∂p)[(2/3)(∂f/∂σ) · (∂f/∂σ)]1/2

(5.2)

where all terms are written in Voigt notation. Before proceeding, let us redetermine the plastic multiplier more generally, without the constraint of working in principal stress space. The consistency condition is written in terms of the stress tensor df (σ , p) =

∂f ∂f : dσ + dp = 0. ∂σ ∂p

If we write the tensor normal, n, for a von Mises material n=

∂f 3 σ

= , ∂σ 2 σe

144

Implicit and explicit integration

the consistency condition becomes df (σ , p) = n : dσ +

∂f dp = 0, ∂p

where without loss of generality, we assume out of plane shears are zero, so ⎡ ⎤ n11 n12 0 n = ⎣n12 n22 0 ⎦ . 0 0 n33 Let us also write, in Voigt notation, the vector normal, n, ⎡ ⎤ n11 ⎢ n22 ⎥ ⎥ n=⎢ ⎣ n33 ⎦ . 2n12 We can then see that ⎡ n11 n12 n : dσ = ⎣n12 n22 0 0

⎤ ⎡

dσ11 0 0 ⎦ : ⎣dσ12 n33 0

dσ12 dσ22 0

⎤ ⎡ ⎤ dσ11 n11 0 ⎢ n22 ⎥ ⎢dσ22 ⎥ ⎥ ⎢ ⎥ 0 ⎦=⎢ ⎣ n33 ⎦ · ⎣dσ33 ⎦ ≡ n · dσ dσ33 2n12 dσ12 ⎤

⎡

so that, provided the normal vector, n, in Voigt notation contains twice the tensorial normal shear terms, then n : dσ ≡ n · dσ and the consistency condition becomes df (σ , p) = n · dσ +

∂f dp = 0. ∂p

We may now determine the plastic multiplier with Hooke’s law written in Voigt notation, as before dσ = C(dε − dεp ). The increment in tensorial plastic strain is obtained from the normality hypothesis, dε p = dλ

∂f = dλn, ∂σ

which we may write in Voigt notation as dεp = dλn remembering that the shear strain terms in the Voigt strain vector are engineering shears; that is, twice the tensorial shears. Hooke’s law then becomes dσ = C(dε − dλn)

Implicit and explicit integration of constitutive equations

145

and combining with the consistency condition, in which, for a von Mises material, dp = dλ, we obtain ∂f n · C(dε − dλn) + dλ = 0 ∂p so that the plastic multiplier is given by dλ =

n · C dε . n · Cn − (∂f /∂p)

For linear isotropic hardening, r = hp so that ∂f /∂p = −∂r/∂p = −h and n · C dε . n · Cn + h Finally, the stress increment is given by dλ =

dσ = C dεe = C(dε − dεp ) = C(dε − dλn).

(5.3)

(5.4)

With knowledge of the total strain increment, dε, together with the stress, σ, Equation (5.3) allows the plastic multiplier to be determined so that the stress increment can be obtained from (5.4). The updated stress, σ + dσ may then be obtained. This is called an explicit integration process. If we denote all quantities at time t with subscript t, and those at the next increment forward in time, t + t, in a similar way, then we may write dλt =

nt · C dεt , nt · Cnt + h

dσt = C(dεt − dλnt ),

(5.5)

dr = h dp = h dλt . The integration to obtain all quantities at the end of the time step, t, may then be written as σt+t = σt + dσt , p

p

p

εt+t = εt + dεt ,

(5.6)

rt+t = rt + drt . This is called a ﬁrst-order forward Euler explicit integration scheme. Its advantage is its simplicity and it is straightforward to implement as we shall see later. However, there are a number of disadvantages which need to be considered. First, because it is an explicit scheme, it is conditionally stable; that is, it may become unstable. Second, the accuracy of the integration depends, of course, on the time step size, t, chosen. Great care is therefore required in ensuring that the time step does not become too large such that erroneous results are obtained. Third, and perhaps most importantly,

146

Implicit and explicit integration

the plastic multiplier given in Equation (5.5) was obtained to ensure that at time, t, the yield condition in (5.1) is satisﬁed. However, the forward integration process does not ensure that the yield condition is also satisﬁed at time t + t, and as a result, it is possible for the solution, over many time steps, to drift away from the yield surface. This is overcome by means of implicit integration of the equations which has the additional advantage of being unconditionally stable. The accuracy remains dependent, however, on the time step size. We introduce an implicit scheme, known as the radial return method for von Mises plasticity, in Section 5.2.1.

5.2.1

Implicit integration: the radial return method

Figure 5.1(a) shows a von Mises yield surface with a schematic representation of the explicit integration method described above. A step forward in time takes the updated stresses outside of the yield surface. Figure 5.1(b) shows a representation of an implicit scheme. A trial stress increment is chosen which again takes the updated stresses, σ trt+t , outside of the yield surface. The stress is then updated with a plastic correction to bring it back onto the yield surface at time t + t. In deviatoric stress space, the plane stress von Mises ellipse becomes a circle, and the plastic correction term is always directed towards the centre of the yield surface (because of the normality condition). The technique has therefore come to be known as the radial return method. In what follows, we shall take all quantities to be those at the end of a time step, t + t, unless speciﬁcally stated. So, the stress at t + t is just σ and that at the beginning of the time step, at time t, is σ t . We may write Hooke’s law in multiaxial form in terms of stress and strain tensors as σ = 2Gεe + λ Tr(εe )I . (a)

(b)

st + ∆t

s2 sy

s2 sy

st

st + ∆t

st

sy

sy sy

s1

sy

sy

s1

sy

Fig. 5.1 Schematic representations of (a) explicit integration and (b) implicit integration, using the radial return method, of von Mises plasticity equations.

Implicit and explicit integration of constitutive equations

147

The elastic strain at the end of the time step may be written as εe = εet + ε e = εet + ε − ε p so that σ = 2G(εet + ε − ε p ) + λ Tr(εet + ε − ε p )I and so p σ = 2G(εet + ε) + λ Tr(ε et + ε) I − 2Gε Elastic predictor Plastic corrector

(5.7)

since Tr(ε p ) = 0. The elastic predictor, or trial stress, is denoted by σ tr = 2G(εet + ε) + λ Tr(εet + ε)I

(5.8)

σ = σ tr − 2Gε p = σ tr − 2Gpn,

(5.9)

so that from (5.7), which we may write as

3 σ

. 2 σe The stress may be expressed in terms of its deviatoric and mean as σ = σ tr − 2Gp

(5.10)

1 σ = σ + (σ : I )I 3

(5.11)

1 σ

σ + (σ : I )I = σ tr − 3Gp 3 σe

(5.12)

so that with (5.10) we obtain

and rearranging gives

1 + 3G

1 p σ = σ tr − (σ : I )I . σe 3

(5.13)

With some algebra, using Equation (5.8), we show that σ tr − 13 (σ : I )I is just the

deviatoric of the trial stress, σ tr as follows, where K is the elastic bulk modulus. 1 σ tr − (σ : I )I = 2G(εet + ε) + λI (ε et + ε) : I − Kεe : II 3 = 2G(εet + ε) + λI (ε et + ε) : I − K(εet + ε − ε p ) : II = 2G(εet + ε) + λI (ε et + ε) : I − KI (ε et + ε) : I

= 2G(εet + ε) + (λ − K)I (ε et + ε) : I ≡ σ tr .

148

Implicit and explicit integration

p

1 + 3G σ = σ tr . (5.14) σe If we take the contracted tensor product of each side of this with itself, we obtain p 2

σ : σ = σ tr : σ tr 1 + 3G σe or 1/2 p 3 tr

tr

1 + 3G σ :σ ≡ σetr . (5.15) σe = σe 2 This gives, ﬁnally, σe + 3Gp = σetr . (5.16) We therefore obtain

The multiaxial yield condition is f = σe − r − σy = σetr − 3Gp − r − σy = 0.

(5.17)

This is generally a non-linear equation in p which may be solved using Newton’s method. We write ∂f dp + · · · = 0. (5.18) f+ ∂p For linear hardening, r = hp so that ∂r ∂r = = h. ∂p ∂p

(5.19)

Substituting (5.17) into (5.18), using (5.19) therefore gives σetr − 3Gp − r − σy + (−3G − h) dp = 0. Rearranging gives

σetr − 3Gp − r − σy . 3G + h We may write the integration in iterative form then, as dp =

r (k) = rt + hp (k) , dp =

σetr − 3Gp (k) − r (k) − σy , 3G + h

(5.20)

p (k+1) = p(k) + dp. The effective stress may then be determined from (5.16); the deviatoric stress tensor from (5.14), so that the plastic strain tensor increment is

ε p =

σ

σ tr 3 3 p ≡ p tr 2 σe 2 σe

Implicit and explicit integration of constitutive equations

149

and the elastic increment ε e = ε − εp and the stress increment is given by σ = 2Gεe + λI ε e : I . We have now introduced both explicit and implicit integration of the plasticity constitutive equations. It is important to note that in the implicit scheme, all quantities are written at the end of the time increment. This ensures that the yield condition, given in Equation (5.17), is satisﬁed at the end of the time increment, therefore avoiding ‘drift’ from the yield surface which can occur in the explicit scheme. The implicit scheme, because it enables signiﬁcantly larger time increments to be used, generally leads to much more rapid solutions. In an implementation within implicit ﬁnite element code, we saw in Section 4.5.2.3 that the implicit integration of the momentum balance or equilibrium equations requires the determination of the Jacobian that comprises both the tangent stiffness matrix and the load stiffness matrix. The tangent stiffness matrix depends very much on the material behaviour, and hence on the constitutive equations. In the implementation of a plasticity model into implicit ﬁnite element code, it is therefore necessary to provide the material tangent stiffness matrix in addition to the integration of the plasticity constitutive equations. In explicit ﬁnite element code, however, which does not depend upon knowledge of the Jacobian, the tangent stiffness matrix is not required. The determination of the material Jacobian for implicit ﬁnite element code is very much bound up with the integration of the constitutive equations used. Typically, in implementing a plasticity model into commercial codes such as ABAQUS explicit or LSDyna (which is an explicit code), for example, we need to provide a subroutine which contains the integration of the plasticity constitutive equations (whether implicit or explicit). For implementations into implicit code, such as ABAQUS standard, we need to provide a subroutine which contains both the integration of the plasticity constitutive equations (whether implicit or explicit) together with the material Jacobian or tangent stiffness matrix. It is useful to note from Section 4.5.2.3 that the Jacobian is required in the iterative procedure in minimizing the force residual. If convergence occurs after a given number of iterations, the Jacobian does not inﬂuence the accuracy of the solution, but the rate at which convergence is achieved. It is for this reason that often approximate Jacobians are used (e.g. in the initial tangent stiffness method in Section 4.5.2.2). A further reason is that depending on the complexity of the plasticity model, the material Jacobian may not be derivable in analytical terms so that a numerical, approximate implementation has to be developed. Perturbation methods can allow the accurate numerical determination of the Jacobian. In the following section, we shall address ﬁrst, the material Jacobian for an elastic material, and

150

Implicit and explicit integration

then that for the time-independent linear strain isotropic hardening plasticity model for which the implicit integration scheme was presented in this section.

5.3 5.3.1

Material Jacobian Isotropic elasticity

Hooke’s law may be written incrementally as σ = 2Gεe + λIε e : I ,

(5.21)

which may be written more succinctly as σ = (2GI + λII ) : εe in which I is the fourth-order identity tensor with the properties I : I = I : I = I and I : ε = ε : I = ε. We will deﬁne the material Jacobian here in the way it is required in the ABAQUS ﬁnite element code as ∂σ /∂ε where ∂σ dε ∂ε in which the shear strains are taken to be engineering shears. For example, dσ =

∂σ11 ∂ε12 1 ∂σ11 ∂σ11 = = , ∂γ12 ∂ε12 ∂γ12 2 ∂ε12 where ∂σ11 /∂ε12 is obtained from Equation (5.21). The material Jacobian becomes, therefore, for conditions of plane strain or axial symmetry (γ13 = γ23 = 0), ⎛ ⎞ ∂σ11 ∂σ11 ∂σ11 ∂σ11 ⎜ ∂ε11 ∂ε22 ∂ε33 ∂γ12 ⎟ ⎛ ⎞ ⎜ ⎟ 2G + λ λ λ 0 ⎜ ⎟ ⎜ ∂σ22 ∂σ22 ∂σ22 ∂σ22 ⎟ ⎜ ⎟ ⎜ ⎟ λ 2G + λ λ 0 ⎟ ⎜ ∂ε11 ∂ε22 ∂ε33 ∂γ12 ⎟ ⎜ ⎟ ⎜ ∂σ ⎜ ⎟ ⎟. = ⎜ ∂σ ∂σ ∂σ ∂σ ⎟ = ⎜ ⎜ 33 33 33 33 ⎟ λ λ 2G + λ 0 ⎟ ⎜ ∂ε ⎟ ⎜ ⎜ ⎟ ⎠ ⎜ ∂ε11 ∂ε22 ∂ε33 ∂γ12 ⎟ ⎝ 1 ⎜ ⎟ 2G 0 0 0 2 ⎜ ∂σ12 ∂σ12 ∂σ12 ∂σ12 ⎟ ⎝ ⎠ ∂ε11 ∂ε22 ∂ε33 ∂γ12 Note that in general, ∂σ /∂ε and ∂σ /∂ε are not the same thing; the former Jacobian quantity is required in ABAQUS, for example, for quadratic convergence. Unfortunately, the material Jacobian for plasticity is not quite so easy to obtain. It is derived in Section 5.3.2 for the plasticity model considered above; that is, for time-independent isotropic linear strain hardening plasticity.

Material Jacobian

5.3.2

151

Material Jacobian for time-independent isotropic linear strain hardening plasticity

We start from Equation (5.14) by applying the differential operator, δ (in a similar way as used to ﬁnd the ﬁrst variation of an integral in Chapter 4) so that we obtain 3Gp 3G p

(5.22) δσe σ = δσ tr . δσ + δpσ − 1 + 3G 2 σe σe σe Also, from (5.16), we may write δσe + 3Gδp = δσetr .

(5.23)

The yield condition is written as δf = δσe − δr = 0 so that for linear hardening, δσe = δr = hδp, where δp is not the plastic strain in the increment, but an inﬁnitesimal quantity, so that we may write δσe = δr = hδp. Combining with (5.23) gives hδp + 3Gδp = δσetr so δp = Combining with (5.23) gives

δσetr . h + 3G

δσe = δσetr 1 −

3G . h + 3G

(5.24)

(5.25)

We now use (5.25), (5.24), and (5.19) in Equation (5.22) to eliminate δσe , δp, and p respectively to give (after some algebra) σetr δσetr σetr

σ = δσ tr . σe − δσ + (5.26) σe σe σe 1 + (3G/ h) Consider the term, 1/2 −1/2 3 tr

3 tr

1 3 tr

3

= σ : σ tr σ : σ tr δσ : σ tr + σ tr : δσ tr δσetr = δ 2 2 2 2 2 3 1 tr

tr

σ : δσ . = 2 σetr

152

Implicit and explicit integration

Substituting this together with the expression for σ in Equation (5.14) into (5.26) gives

σe 3 1 σe σ tr σ tr

(5.27) δσ = : δσ tr + tr δσ tr . − tr σe 2 1 + (3G/ h) σe σetr σetr If we write 3 1 σe σe Q= − tr and R = tr 2 1 + (3G/ h) σe σe then (5.27) becomes

σ tr σ tr

δσ = Q tr tr + RI : δσ tr . (5.28) σe σe Remember that in deriving the Jacobian, we are trying to relate δσ to δε. We may write the deviatoric trial stress in terms of the deviatoric trial strain using Hooke’s law (because the trial stress is obtained assuming elasticity) as 1 tr

tr

tr tr δσ = 2Gδε = 2G δε − II : δε 3 and δεtr ≡ δε 1 δσ = 2G δε − II : δε . 3 Substituting into Equation (5.28) gives

1 σ tr σ tr

δσ = Q tr tr + RI : 2G δε − II : δε 3 σe σe

so

tr

σ tr σ tr 1 σ tr σ tr 2 = 2GQ tr tr : δε − Q tr tr : (II : δε) + 2GRδε − GRI : (II : δε). 3 σe σe 3 σe σe

The second term of the right-hand side is zero since σ tr is deviatoric so

σ tr σ tr σ tr σ tr : (II : δε) = : I Tr(δε) = 0 σetr σetr σetr σetr and therefore δσ = 2GQ

σ tr σ tr 2 : δε + 2GRδε − GRII : δε tr tr σe σe 3

since I : I = I . Finally, the stress is given in terms of its deviatoric by 1 δσ = δσ + II : δσ = δσ + KII : δε e = δσ + KII : (δε − δε p ) 3

= δσ + KII : δε.

(5.29)

Material Jacobian

153

Substituting into (5.29) gives

σ tr σ tr 2 δσ = 2GQ tr tr : δε + 2GRδε + K − GR II : δε. σe σe 3

We may write this in the shortened form as

σ tr σ tr 2 δσ = 2GQ tr tr + 2GRI + K − GR II σe σe 3

(5.30)

: δε.

(5.31)

Equation (5.30) provides the Jacobian or the material tangent stiffness matrix. In this case, because it has been derived from the implicit backward Euler integration scheme, which is used to integrate the plasticity constitutive equations, it is called the consistent tangent stiffness. Let us determine some of the terms using (5.30).

δσ11 = 2GQ

tr σ11 1 tr σe σetr

tr tr tr tr tr tr × (σ11 δε11 + σ22 δε22 + σ33 δε33 + 2σ12 δε12 + 2σ13 δε13 + 2σ23 δε23 ) 2 + 2GRδε11 + K − GR (δε11 + δε22 + δε33 ). 3 The ﬁrst term of the Jacobian is, therefore,

tr

σ tr σ11 ∂δσ11 2 D11 = GR = 2GQ 11 + 2GR + K − ∂δε11 3 σetr σetr

and the next is D12

tr σ tr

σ11 ∂δσ11 2 22 = = 2GQ tr tr + K − GR ∂δε22 σe σe 3

and so on. A shear term is given by tr 2σ tr

tr σ tr

σ12 σ12 ∂δσ12 1 ∂δσ12 1 12 D44 = 2GQ tr tr + 2GR = 2GQ tr 12 = = + GR ∂δγ12 2 ∂δε12 2 σe σe σe σetr and D14 is

tr σ tr σ12 ∂δσ11 1 ∂δσ11 = = 2GQ 11 . D14 = ∂δγ12 2 ∂δε12 σetr σetr For conditions of axial symmetry (so that the out of plane shears, σ13 , ε13 and σ23 , ε23 do not exist) therefore, the Jacobian is the symmetrical matrix ⎞ ⎛ D11 D12 D13 D14 ⎜ ∂δσ D22 D23 D24 ⎟ ⎟. =⎜ ⎝ D33 D34 ⎠ ∂δε D44

154

Implicit and explicit integration

5.4

Kinematic hardening

In this section, we shall use implicit (backward Euler) integration for the case of linear kinematic hardening, and obtain the consistent tangent stiffness. We will then go on to address combined linear kinematic hardening with non-linear isotropic hardening, and to introduce combined non-linear kinematic and isotropic hardening. We will ﬁnish by introducing semi-implicit integration schemes for plasticity. 5.4.1

Linear kinematic hardening

With the backward Euler scheme, as given in Section 5.2.1.2 for isotropic hardening, Hooke’s law may be written in its predictor–corrector form as σ = σ tr − 2Gpn

(5.32)

in which σ tr is the elastic trial stress. We employ linear kinematic hardening so that the back stress increment is given by 2 cεp 3 and as a result, if we write the back stress at time, t, as x t , then at the end of the time step, t + t, it becomes 2 x = x t + cεp (5.33) 3 and with the normality hypothesis for von Mises plasticity, x =

2 x = x t + cpn, 3

(5.34)

where

3 σ − x (5.35) 2 σe for kinematic hardening, in which x is, of course, itself deviatoric, and p is the increment in effective plastic strain. Combining (5.35) and (5.34) gives n=

2 2 σ = x t + pcn + σe n. 3 3 The deviatoric stress is

1 σ = σ − II : σ 3 so that with (5.32), we may write (5.36) as 1 2 2 σ tr − 2Gpn − II : σ = x t + pcn + σe n. 3 3 3

(5.36)

Kinematic hardening

155

We saw earlier that we may write 1

σ tr − II : σ ≡ σ tr 3 so that

2 2

σ tr − 2Gpn = x t + pcn + σe n. 3 3 Taking the contracted product of both sides of (5.37) with n gives 2 2 tr

(σ − x t ) : n = n : n 2Gp + pc + σe 3 3 and 3 σ − x 3 σ − x 3 3

n:n= (σ − x) : (σ − x) . : = 2 σe 2 σe 2σe2 2 But the effective stress, σe , is deﬁned by 1/2 3

σe = (σ − x) : (σ − x) 2 so that 3 n:n= . 2 Equation (5.38) therefore reduces to

(σ tr − x t ) : n = 3Gp + pc + σe . From (5.32) we may write

(5.37)

(5.38)

(5.39)

σ = σ tr − 2Gpn

so that from (5.35), we may write n as

3 σ tr − 2Gpn − x 3 σ tr − 2Gpn − x t − (2/3)cpn n= = . 2 σe 2 σe Rearranging this equation for n gives

3 σ tr − x t n= 2 σe + 3Gp + cp

(5.40)

and substituting into (5.39) gives 1/2 3 tr

tr

(σ − x t ) : (σ − x t ) ≡ σetr = 3Gp + pc + σe . (5.41) 2 Note that the effective trial stress is determined with respect to the back stress taken at time, t, rather than at the end of the time increment. Rearranging this equation gives p =

σetr − σe . 3G + c

(5.42)

156

Implicit and explicit integration

The yield function for the case of kinematic hardening is f = σe − σy = 0

(5.43)

so that σe = σy . In Equation (5.42), therefore, for the case of linear kinematic hardening, none of the terms depends upon the effective plastic strain. Equation (5.42) is therefore an exact, closed-form expression for p and in this instance, no iteration is required for its determination. Plastic and elastic strains and the stress may then be updated using (5.42) to give

3 σ tr − x t n= . 2 σetr εp = pn, p

εp = εt + ε p , ε e = εet + ε e = εet + ε − ε p , σ = 2Gεe + λII : εe . 5.4.1.1 Consistent tangent stiffness for linear kinematic Hardening. In implicit ﬁnite element code, in addition to the integration of the plasticity constitutive equations, it is also necessary to provide the material Jacobian—the tangent stiffness matrix. Here, we determine the consistent (i.e. with the implicit integration given above) tangent stiffness for linear kinematic hardening. Using (5.40) and (5.41), n may be written as

3 σ tr − x t n= . 2 σetr We have therefore

σ =σ

tr

− 2Gpn = σ

tr

3 − 2Gp 2

σ tr − x t σetr

and substituting for p from (5.42) gives

tr

tr 3 σ − σ − x σ

e t σ = σ tr − 2G e 3G + c 2 σetr and after a little algebra, we obtain 1 − σe /σetr c/3G + σe /σetr

+ xt . σ = σ tr 1 + c/3G 1 + c/3G

Kinematic hardening

157

Applying the differential operator, and rearranging, we obtain (1 + c/3G)

σetr

δσ = δσ tr (1 + (c/3G)(σetr /σe )) σe

+ σ tr (δσe /σe − δσetr /σetr ) − (δσe /σe − δσetr /σetr )x t . From the yield function in (5.43), δf = δσe = 0 so this reduces to (1 + c/3G)

σetr

δσ = δσ tr (1 + (c/3G)(σetr /σe )) − (σ tr − x t )(δσetr /σetr ). σe (5.44)

Now,

σetr so

1/2

3 tr

(σ − x t ) : (σ tr − x t ) = 2

−1/2 3 tr

1 3 tr

3 tr

tr

tr

tr

(σ −x t ) : (σ −x t ) (σ −x t ) : δσ + δσ : (σ −x t ) = 2 2 2 2 1 3

= tr (σ tr − x t ) : δσ tr . σe 2

δσetr

Substituting into (5.44), and writing Q=

σe /σetr + c/3G 1 + c/3G

gives

δσ = Qδσ

tr

δσ

1 3 σe tr 2 σe 1 + c/3G

(σ tr − x t ) (σ tr − x t )

+R : δσ tr . tr tr σe σe

As before, tr

R=−

1 = 2G δε − II : δε 3

so that

(σ tr − x t ) (σ tr − x t ) 2 : δε − GQII : δε δσ = 2GQδε + 2GR tr tr σe σe 3

and ﬁnally, δσ = 2GQδε + 2GR

2 (σ tr − x t ) (σ tr − x t ) GQ II : δε : δε − K − σetr σetr 3 (5.45)

which gives the consistent tangent stiffness.

158

5.4.2

Implicit and explicit integration

Combined isotropic and linear kinematic hardening

The isotropic hardening evolution equation is dr = h dp in which h can be a function of p so that r is not necessarily linear, and for the linear kinematic hardening, 2 dx = c dεp . 3 Because of the assumption of linearity, as before we may write 2 x = x t + cpn 3 and from Section 5.4, we have σe = σetr − (3G + c)p in which σetr and σe are given by 1/2 3 tr

tr

tr σe = , (σ − x t ) : (σ − x t ) 2

(5.46) 1/2

3

(σ − x) : (σ − x) σe = 2

.

The yield function is f = σe − r − σy = 0 which becomes, after substituting (5.46) f = σetr − (3G + c)p − r − σy = 0.

(5.47)

In this case, r depends on h which may, for non-linear hardening, depend on p and the equation can be non-linear. We use Newton’s method to solve it by writing f+

∂f dp = 0 ∂p

and substituting (5.47) gives dp =

σetr − (3G + c)p − r − σy . 3G + c + h

(5.48)

Let us simplify it for the cases of linear kinematic hardening and isotropic hardening only to compare with the previous equations. If there is no isotropic hardening, then r = h = 0 and (5.48) becomes dp =

σetr − (3G + c)p − σy 3G + c

(5.49)

Kinematic hardening

159

and for linear kinematic hardening, σe = σetr − (3G + c)p and σe = σy so (5.49) gives dp = 0. That is, there is no iteration required and p is given by σetr − σy 3G + c

p =

as before. If there is no kinematic hardening, x = 0 and c = 0 so (5.49) becomes dp = where

σetr − 3Gp − r − σy , 3G + h

1/2 3 tr

tr

= σ :σ 2 which is what we obtained before in Section 5.2.1.

σetr

5.4.3

Introduction to implicit integration of combined non-linear kinematic and isotropic hardening

In the previous sections in which we assumed linear kinematic hardening, we wrote the kinematic hardening variable in terms of its value at the start of the increment, x t , and the incremental value. As a result, subsequent equations were set up in terms of x t . Here, we will now introduce the more general case of non-linear kinematic hardening, and will ﬁnd the equations depending on quantities at the end of the time increment. As before, the deviatoric stress can be written in predictor–corrector form in terms of the trial stress and plastic return as

σ = σ tr − 2Gpn

(5.50)

and the normal, n, is given by

3 σ − x . 2 σe Combining these equations and after a little algebra, we obtain 2 tr

(σ − x) : n = σe + 2Gp n : n 3 n=

(5.51)

and we have shown before that n : n = 23 , so

(σ tr − x) : n = σe + 3Gp.

(5.52)

160

Implicit and explicit integration

We can also obtain from (5.50) and (5.51)

n=

3 σ tr − 2Gpn − x 2 σe

so that rearranging,

3 σ tr − x . n= 2 σe + 3Gp Combining with (5.52) gives σe = σetr − 3Gp, where

1/2

σetr

(5.53)

3 tr

(σ − x) : (σ tr − x) = 2

.

(5.54)

The yield function is f = σe − r − σy = σetr − 3Gp − r − σy = 0

(5.55)

with σetr given by (5.54). Note now that because x depends on p (non-linearly for the case of non-linear kinematic hardening) as may r, Equation (5.55) is a non-linear equation in p for which we will need to use Newton’s iterative solution method, for which we obtain dp = and

σetr

(k)

− 3Gp (k) − r (k) − σy (k)

3G + (∂r (k) /∂p) − (∂σetr /∂p)

(5.56)

p(k+1) = p(k) + dp.

Both σetr and r are the two derivatives with respect to p need to be updated at every iteration for a fully implicit integration. Often, with complex plasticity hardening laws, this may be challenging. A simpler approach is to integrate the effective plastic strain implicitly but to update the normal n and the internal variables—the isotropic and kinematic hardening—explicitly. Such an approach is called semi-implicit integration. 5.4.4

Semi-implicit integration of combined non-linear kinematic and isotropic hardening

In the semi-implicit scheme, Newton’s method is used to determine the effective plastic strain increment using Equation (5.56) and the yield function (5.55) written at the end of the time increment ensures that drift from the yield surface does not occur. However, the updates of all other quantities are carried out explicitly as follows: (k+1)

εp

= p(k+1) nt ,

Implicit integration in viscoplasticity

where nt = (k+1)

εp εe

(k+1)

161

3 σ t − x t , 2 σet (k+1)

p

= εt + ε p

(k+1)

= ε − εp

σ (k+1) = 2Gε

e(k+1)

,

,

+ λII : εe

(k+1)

,

r (k+1) = rt + r, x (k+1) = x t + x, where, for example, the non-linear kinematic hardening increment, x, is given by 2 (k+1) + γ x t p(k+1) x = cεp 3 and the isotropic hardening increment by r = b(Q − r)p(k+1) if the non-linear evolution equations given in Chapter 2 are adopted, and 1/2 3 tr

(k+1) tr

(k+1) tr (k+1) σe ) : (σ − x ) . (σ − x = 2 The semi-implicit scheme is not unconditionally stable and we need to be concerned, therefore, about both stability and accuracy when using it.

5.5

Implicit integration in viscoplasticity

We saw in Chapter 2 that the plastic strain rate can be written, for a viscoplastic von Mises material, as ∂f ε˙ p = p˙ ∂σ in which, for viscoplasticity, p˙ is now speciﬁed by a constitutive equation (as opposed to being determined by the consistency condition) which, for both isotropic and kinematic hardening, can be written as p˙ = φ(σ , x, r). We may write this incrementally as p = φ(σ , x, r)t = φt. For both kinematic and isotropic hardening, the yield function is f = J (σ − x ) − r − σy .

(5.57)

162

5.5.1

Implicit and explicit integration

Uniaxial viscoplasticity equations

We will present implicit backward Euler integration for the uniaxial form of the equations ﬁrst, for simplicity, and we start from the viscoplastic constitutive equation. Equation (5.57) may be written in uniaxial form, if we consider isotropic hardening only for now, as p = φ(σe , r)t (5.58) and we may write this in a form suitable for Newton’s iterative solution as ψ = p − φ(σe , r)t = 0.

(5.59)

In preparation for differentiation, we may write the stress in terms of p by remembering (5.16) σe + 3Gp = σetr (5.60) so that (5.59) becomes ψ(p, r) = p − φ(p, r)t = 0.

(5.61)

Using Newton’s method, we have ψ+

∂ψ ∂ψ dp + dr = 0 ∂p ∂r

and differentiating (5.61) and substituting into (5.62) gives ∂φ ∂φ t dp − t dr = 0. p − φt + 1 − ∂p ∂r

(5.62)

(5.63)

We will write, from here on, φp =

∂φ ∂p

and

φr =

∂φ ∂r

and similarly for other derivatives. If we assume for now linear isotropic hardening, then dr = h dp = h dp. Substituting into (5.63) and rearranging gives dp =

φ(p, r) − p/t . 1/t − φp − hφr

(5.64)

As an example, let us consider a particular viscoplasticity constitutive equation, given by p˙ = φ(σe , r) = α sinh β(σe − r − σy ) in which σy , α, and β are material constants. Using (5.59) this becomes p˙ = φ(p, r) = α sinh β(σ tr − 3Gp − r − σy )

Implicit integration in viscoplasticity

163

and the required derivatives are φp = −3Gαβ cosh β(σ tr − 3Gp − r − σy ) and φr = −αβ cosh β(σ tr − 3Gp − r − σy ) so that (5.64) gives dp =

α sinh β(σ tr − 3Gp − r − σy ) − p/t 1/t +3Gαβ cosh β(σ tr −3Gp−r −σy )+hαβ cosh β(σ tr −3Gp−r −σy )

with r = rt + hp. As before in rate-independent plasticity, an iterative procedure is used to determine p from p(k+1) = p(k) + dp. 5.5.2

Multiaxial viscoplasticity

For the case of isotropic hardening, Equation (5.64) still holds for the multiaxial case, and the plastic strain tensor increment can then be determined from

σ

σ tr 3 3 ε = pn = p ≡ p tr

2 σe 2 σe p

so that the elastic strain and hence stress increments can be determined in the usual way. We shall next consider combined multiaxial linear isotropic and kinematic hardening such that the constitutive equation is written as p˙ = φ(p, x, r) in which x is the tensorial kinematic hardening variable. The problem may be written, as before, ψ(p, x, r) = p − φ(p, x, r)t = 0 and

∂ψ ∂ψ ∂ψ dp + : dx + dr = 0. ∂p ∂x ∂r We may write the derivatives as ψ+

∂ψ = 1 − φp t, ∂p

∂ψ = −φ x t, ∂x

∂ψ = −φr t ∂r

(5.65)

164

Implicit and explicit integration

so that (5.65) becomes p − φt + (1 − φp t) dp − φ x : dxt − φr drt = 0.

(5.66)

Let us write the linear isotropic and kinematic hardening equations as dr = h dp = h dp, 2 2 c dεp = c dpn 3 3 so that substituting into (5.66) and rearranging gives dx =

dp =

φt − p . 1 − φp t − hφr t − (2/3)cφ x : nt

(5.67)

If we consider again a viscoplastic constitutive equation with kinematic and isotropic hardening of the form p˙ = φ(σ , x, r) = α sinh β(J (σ − x ) − r − σy ) = α sinh β(σe − r − σy ), then

3 σ − x

∂φ ∂σe = −φσe = −φσe n ∂σe ∂x 2 J (σ − x ) and the term φ x : n may be simpliﬁed to φx = −

3 φ x : n = −φσe n : n = − φσe . 2 Substituting into (5.67) gives dp =

φ − p/t 1/t − φp − hφr + cφσe

(5.68)

which is solved iteratively. The plastic strain increment is then determined from

σ − x

3 σ tr − x

3 ε = p ≡ p . 2 J (σ − x ) 2 σetr p

5.5.3

Consistent tangent stiffness for viscoplasticity with isotropic hardening

The predictor–corrector form of the stress is

σ = σ tr − 2Gpn or where

σ = σ tr − 2Gpn,

(5.69)

3 σ tr 3 σ

n= = 2 σetr 2 σe

(5.70)

Implicit integration in viscoplasticity

165

and σe = σetr − 3Gp. Rearranging (5.70) gives

σe tr

σ σetr

σ = and applying the differential operator σe

δσ = tr δσ tr + σe

δσe σe δσetr − σetr σetr σetr

σ tr .

(5.71)

Now, δσetr =

1 3 tr

σ : δσ tr tr σe 2

(5.72)

and

1 3

σ : δσ . (5.73) σe 2 Substituting (5.72) and (5.73) into (5.71) and eliminating σ using (5.70) gives δσe =

3 σ tr σ tr σe tr

σe 3 σ tr σ tr

: δσ + δσ − : δσ tr . δσ = tr tr tr tr tr tr 2 σe σe σe σe 2 σe σe

Because of the contracted product of δσ in the ﬁrst term on the right-hand side, we will substitute for this using the differential form of (5.50)

δσ = δσ tr − 2Gδpn to give

3 σ tr σ tr σe tr

σe 3 σ tr σ tr

tr

: (δσ − 2Gδpn) + δσ − : δσ tr tr tr tr tr tr tr 2 σe σe σe σe 2 σe σe

3 σ tr σ tr σe tr

σe 3 σ tr σ tr

=− : 2Gδpn + tr δσ + 1 − tr : δσ tr . tr tr tr tr 2 σe σe σe σe 2 σe σe

δσ =

Now,

3 σ tr 3 :n=n:n= tr 2 σe 2 so

σ tr σe tr

σe 3 σ tr σ tr

: δσ tr . δσ = − tr : 3Gδpn + tr δσ + 1 − tr tr tr σe σe σe 2 σe σe

(5.74)

The viscoplastic constitutive equation is written as, from (5.57), p = φ(σ , r) t

(5.75)

166

Implicit and explicit integration

so that δp = (φσ : δσ + φr δr) t.

(5.76)

Let us assume isotropic hardening of the form δr = q(r)δp. Because δp is again an inﬁnitesimal increment in p (as opposed to the plastic strain increment), this can be written as δr = q(r)δp.

(5.77)

Substituting this together with the second equation of (5.69) for δσ into (5.76) gives δp = (φσ : (δσ tr − 2Gδpn) + φr q(r)δp)t and rearranging δp =

φσ : δσ tr . 1/t + 2Gφσ : n + φr q(r)

(5.78)

Substituting into (5.74) gives δσ = −

σe tr

σe 3 σ tr σ tr σ tr φσ : δσ tr

n+ δσ + 1− : δσ tr . : 3G σetr 1/t +2Gφσ : n+φr q(r) σetr σetr 2 σetr σetr

Let us write 3G α=− , 1/t + 2Gφσ : n + φr q(r) then

σe 3 1 − tr , γ = 2 σe

σe β = tr , σe

σ tr σ tr σ tr

δσ = α tr φσ : δσ tr + βδσ tr + γ tr tr : δσ tr . σe σe σe

(5.79)

Now, 2

δσ tr = 2Gδε = 2Gδε − G(δε : I )I . 3 Because φ is a function of the effective stress, its derivatives with respect to the stress

components are deviatoric, and hence φσ : δσ tr = φσ : (δσ tr + (1/3)δσ tr : II ) =

φσ : δσ tr since φσ : I = 0. In addition, δσ = δσ + KII : δε so that (5.79) becomes

σ tr σ tr 2 σ tr δσ = 2Gα tr φσ + K − Gβ II + 2Gγ tr tr σe 3 σe σe which gives the consistent tangent stiffness.

: δε + 2Gβδε

(5.80)

Incrementally objective integration for large deformations

5.6

167

Incrementally objective integration for large deformations

So far, we have addressed the update of stress over a given time increment on the basis that there is no incremental rotation. In large deformation analyses, however, in which deformations and rigid body rotations can become large, we need to take account of the effect of incremental rotation on the determination of the updated stress. Figure 5.1 shows the representation of a body in its original conﬁguration and then in deformed conﬁgurations at times t and t + t. In the deformed conﬁgurations, the local material (or co-rotational) coordinate systems are shown indicating that an incremental rotation has occurred between the conﬁgurations at times t and t + t. We need to ensure that the stress update is carried out with respect to the same reference frame. For example, in using a userdeﬁned subroutine for plasticity in ABAQUS, the user is supplied with the strains at the beginning and end of the time increment, together with the stress at the beginning of the time increment, but all these quantities and other tensor quantities have usually already been incrementally rotated to account for the incremental rigid body rotation. We shall return to this in Chapter 6. For now, however, we shall look at an incrementally objective stress update. First, referring to Fig. 5.2, let us assume we know the stresses, σ t , at time t with respect to the material reference frame, that is, the undeformed conﬁguration at that time. Also, we have determined the spin, W , given by the antisymmetric part of the velocity gradient. The stress rate, σ˙ , with respect to the material reference frame, or undeformed conﬁguration, at time t, taking full account of the incremental rigid body rotation, is

Deformed configuration at t

Deformed configuration at t + ∆t

Undeformed (original) configuration y Ft y

y⬘ x

Y

x

X

x⬘

F t + ∆t

Fig. 5.2 A body in its original (undeformed) conﬁguration and in deformed conﬁgurations at times t and t + t.

168

Implicit and explicit integration

given by

∇

σ˙ = σ +W t σ t − σ t W t

(5.81)

so that the updated stress (written explicitly) with respect to the undeformed conﬁguration at time t is simply σ t+t = σ + σ˙ t. We can write Equation (5.81) in incremental form, if we wish, as ∇

σ = σ + (W t σ t − σ t W t )t

(5.82)

which we may also write as ∇

σ = σ + Rσ t R T

(5.83)

∇

in which σ is the increment in objective, or co-rotational, stress, and R is a rotation to be determined. We shall further consider these approaches in Chapter 6, concerned with the implementation of plasticity models into ﬁnite element code.

Further reading Bathe, K.-J. (1996). Finite Element Procedures. Prentice Hall, New Jersey, revised edition. Belytschko, T., Liu, K.W., and Moran, B. (2000). Nonlinear Finite Element Analysis for Continua and Structures. John Wiley & Sons, New York. Simo, J.C. and Hughes, T.J.R. (1998). Computational Inelasticity. Springer-Verlag, New York. Chaboche, J.-L. (1986). ‘Time-independent constitutive theories for cyclic plasticity’. International Journal of Plasticity, 2(2), 149–188. Hughes, T.J.R. (1984). ‘Numerical implementation of constitutive models: rateindependent deviatoric plasticity’. In Nemat Nasser S., Asaro R.J., and Hegemier G.A. (eds), Theoretical Foundation for Large-Scale Computations of Non-linear Material Behaviour, Martinus Nijhoff Publication, The Netherlands, 29–57. Krieg, R.D. and Key, S.W. (1976). ‘Implementation of a time dependent plasticity theory into structural computer programs’, In Constitutive Equations in Viscoplasticity: Computational and Engineering Aspects (eds) Stricklin J.A. and Saczalski K.J.), ASME.

6. Implementation of plasticity models into ﬁnite element code

6.1

Introduction

Several commercial ﬁnite element software packages (e.g. ABAQUS, LSDyna, and MARC) provide the facility for users to specify their own material models. In ABAQUS, the user is required to provide a Fortran subroutine called a ‘UMAT’. This chapter is concerned with the implementation of plasticity models into ﬁnite element code, which is carried out, by example, in using ABAQUS. In particular, we start by developing an ABAQUS UMAT for elasticity, and discuss the tests necessary to verify the model implementation into ABAQUS. We go on to consider isotropic hardening plasticity with explicit and implicit integration, with continuum and consistent tangent stiffnesses, large deformation formulations using rotated variables provided by ABAQUS, and from ﬁrst principles using the deformation gradient. We use the problem of simple shear with elasticity to verify the large deformation implementations. We then present an implicit implementation for elasto-viscoplasticity (and creep). All the Fortran coding, together with the necessary ABAQUS input ﬁles, are available through the OUP website. Finite element code is often modular in structure, whether it be commercial code or written in-house. An important module is that relating to material behaviour; in other words, the constitutive stress response of the material given prescribed conditions of deformation. In ABAQUS, but in a similar way for all codes, a range of information is passed into the material module relating to both the beginning and end of a time increment. In particular, stress, strain, and deformation gradient are provided at the beginning of the time increment. Strain and the deformation gradient are also provided at the end of the increment. Within the module, it is then necessary to execute three tasks. First, the stresses at the end of the time increment must be determined and, second, for the case of an implicit analysis (i.e. the ﬁnite element momentum balance or equilibrium equations are solved implicitly) using ABAQUS standard, for example, the material Jacobian, or tangent stiffness, must also be provided. Third, any state variables (such as the isotropic hardening variable or effective plastic strain) must

170

Implementation of plasticity models

be updated to the end of the time increment. In fact, in coding an ABAQUS UMAT, a large range of information is provided, some of which will be referred to later. However, the job of the UMAT is clear: to update the stresses and state variables to the end of the time increment and to provide the Jacobian. We start by addressing elasticity.

6.2

Elasticity implementation

We discuss elasticity and its implementation into a UMAT for two main reasons. First, it provides a good introduction to writing and testing a UMAT subroutine for those who are new to the process. Second, it provides a basis from which elastoplasticity models may be developed. For the latter reason, while is no way essential for elasticity, we use an incremental approach in implementing the linear elastic equations. In Chapter 5, Hooke’s law was given in an incremental form in Equation (5.21) together with the material Jacobian, for the case in which there are no out of plane shears (e.g. plane strain and axisymmetric problems). With knowledge of the increment in strains (provided to the UMAT), together with the speciﬁcation of elastic constants (we shall take E = 210 GPa and ν = 0.3 throughout), the stress increment is obtained either from Equation (5.21), or its equivalent written in Voigt notation, ⎛ ⎞⎛ ⎞ 2G + λ λ λ 0 ε11 ⎜ λ ⎜ ⎟ 2G + λ λ 0⎟ ⎟ ⎜ε22 ⎟ . σ = Cεe = ⎜ (6.1) ⎝ λ ⎠ ⎝ λ 2G + λ 0 ε33 ⎠ 0 0 0 G γ12 Because ABAQUS provides most tensor quantities in vector (Voigt) form, it may be more convenient to use Equation (6.1) than the tensor form given in (5.21). However, this is not always the case, and later we shall use the tensor form in preference, particularly where it is necessary to work from the deformation gradient. Note that the shear strain quantities provided by ABAQUS are always engineering shears, that is, twice the tensorial shear strains. It is also important to check the ordering of shear quantities, which can vary depending on element type used. Equation (6.1) is suitable for plane strain and axisymmetric problems, but not for problems of plane stress or three dimensions, for which different stiffness matrices are required. For linear elasticity, the material Jacobian is just the elastic stiffness matrix so that speciﬁcation of the Jacobian in the UMAT is easy. The coding required for the UMAT for linear elasticity for plane strain, axisymmetric, and three-dimensional problems, is available through the OUP website. A complete list of all the UMAT coding, together with ABAQUS input ﬁles, is given in Appendix B.

Veriﬁcation of implementations

6.3

171

Veriﬁcation of implementations

The veriﬁcation of the model implementation is vital. For complex material models, this requires the development of an independent solver (which will often be numerical) for uniaxial and pure shear problems so that direct comparison with the results obtained using the UMAT can be made. In addition, it is necessary to test the UMAT using a single, and where appropriate, multiple elements, for conditions of strain control and load control under uniaxial and pure shear conditions. If possible, perhaps by ‘switching off’ parts of the model implemented into the UMAT, make comparisons with a multiaxial problem with non-uniform strain and stress distributions for which the solution is known (either an independent solution or one obtained using an internal ABAQUS model). In this chapter, we shall not carry out all of the veriﬁcation tests described for all the model implementations, but it is certainly advisable to do so for new model implementations into UMATs. Because of their importance, we go through some of the possible veriﬁcation tests step by step. 1. Single and multiple element uniaxial tests. Figure 6.1 shows an axisymmetric single- and four-element unit square which is subjected to uniaxial displacement or force control in the z-direction producing uniform, uniaxial stress, σzz , and strain, εzz , with εrz = σrr = σθ θ = σrz = 0, which can be compared with independent closed-form solutions. The four-element problem is important since it introduces a ‘free’ node, which does not exist for the single four-noded axisymmetric element. The force controlled test is important for checking errors in the Jacobian. 2. Single element simple shear test. The uniaxial tests in (1) do not involve the shear terms at all, so it is important to include a problem which tests these terms, particularly because of the potential for errors with the use of engineering shear strains rather than their tensorial counterparts. Figure 6.2 shows a plane strain single-element unit square under simple shear loading. For small deformations, εxx = εyy = σxx = σyy = 0,

Displacement or force

Displacement or force z

z 1.0

1.0

ur = 0.0

ur = 0.0

0.0

0.0 0.0

1.0 r

uz = 0.0

0.0

1.0 r uz = 0.0

Fig. 6.1 Schematic diagram showing an axisymmetric single- and four-element unit square under uniaxial displacement or force controlled loading.

172

Implementation of plasticity models g y 1.0

0.0 0.0

1.0 x ux = uy = 0.0

Fig. 6.2 Schematic diagram showing a plane strain single-element unit square under simple shear loading.

and uniform shear strain, γxy , and stress, σxy , are produced which can be compared with independent closed-form solutions. 3. Non-uniform strain and stress ﬁeld. Often, a comparison test which generates non-uniform strain and stress ﬁelds will not be possible because a comparison may well not exist, and a closed-form solution is now no longer possible. However, it is sometimes possible to simplify the implemented plasticity model (e.g. by turning off the porosity in a Gurson-type porous plasticity model) such that a comparison with another solution (e.g. produced using one of the many built-in models contained within ABAQUS) is then possible. While this will not test all the features of the model implemented into the UMAT, it nonetheless may test a good number of them, and may therefore be worthwhile. Later in the chapter, both an implicit and explicit implementation of isotropic hardening plasticity are tested in this way by comparing the results obtained with those produced using the built-in ABAQUS model.

6.4

Isotropic hardening plasticity implementation

In Chapter 5, we presented both explicit and implicit integration of the equations for linear strain hardening isotropic plasticity, together with the consistent tangent stiffness for the implicit scheme. We will implement both integration schemes into ABAQUS UMATs and discuss the advantages and disadvantages of each. We start with the explicit scheme which was described at the beginning of Section 5.2, and introduce the continuum Jacobian.

6.4.1

Explicit integration for isotropic hardening plasticity with continuum Jacobian

We may summarize the implementation as follows. All quantities are assumed to be given at time, t, that is, at the start of the time increment, unless indicated

Isotropic hardening plasticity implementation

173

otherwise: (i) Determine the yield function

f = σe − r − σy =

3

σ : σ

2

1/2 − r − σy .

(6.2)

(ii) Determine if actively yielding Is

f > 0?

(iii) Determine the plastic multiplier n · C dε , n · Cn + h f < 0, dλ = 0.

f > 0,

dλ =

(6.3)

(iv) Determine stress and isotropic hardening increments dσ = C dεe = C(dε − dλn), dr = h dp = h dλ.

(6.4)

(v) Update all quantities to the end of the time increment, using explicit integration σt+t = σ + dσ, p

εt+t = εp + dεp ,

(6.5)

rt+t = r + dr. (vi) Determine Jacobian. (vii) End. We now address the determination of the Jacobian. In Chapter 5, we derived the consistent tangent stiffness for the implicit integration scheme. For the purposes of the explicit integration considered here, we introduce what is sometimes referred to as the continuum Jacobian. That is, it is not derived explicitly on the basis of the integration scheme, but directly from the constitutive equations. We start from the stress–strain relationship written in Voigt notation dσ = C dεe = C(dε − dλn),

(6.6)

which we may write out fully for conditions of axial symmetry or plane strain as ⎛ ⎞ ⎛ ⎞ ⎛ ⎞ ⎛⎛ ⎞ ⎛ ⎞⎞ dσ11 dσ1 C11 C12 C13 C14 dε1 n1 ⎜dσ22 ⎟ ⎜dσ2 ⎟ ⎜ ⎟ ⎜⎜dε2 ⎟ ⎜n2 ⎟⎟ C C C 22 23 24 ⎜ ⎟ ⎜ ⎟ ⎜ ⎟ ⎜⎜ ⎟ − dλ ⎜ ⎟⎟ . ⎝dσ33 ⎠ = ⎝dσ3 ⎠ = ⎝ ⎝n3 ⎠⎠ C33 C34 ⎠ ⎝⎝dε3 ⎠ dσ12 dσ4 sym C44 dε4 n4 (6.7)

174

Implementation of plasticity models

We may write the Jacobian (here symmetric) as ⎛ J11 J12 ∂ dσ ⎜ J22 J = =⎜ ⎝ ∂ dε sym

J13 J23 J33

⎞ J14 J24 ⎟ ⎟ J34 ⎠ J44

(6.8)

so that, for example, the ﬁrst term is J11 =

∂ dσ1 ∂ dλ = C11 − (C11 n1 + C12 n2 + C13 n3 + C14 n4 ). ∂ dε1 ∂ dε1

With some algebra we may show, therefore, that ∂ dλ , (6.9) ∂ dε where ⊗ is the dyadic product of two vectors, details of which may be found in Appendix A. In a similar way, by considering the numerator of the plastic multiplier given in Equation (6.3), we may show that J = C − Cn ⊗

Cn ∂ dλ = ∂ dε n · Cn + h so that the continuum Jacobian is J =C−

Cn ⊗ Cn . n · Cn + h

(6.10)

The explicit integration and provision of Jacobian is then complete. An ABAQUS UMAT containing this formulation, together with various input ﬁles for uniaxial displacement and load control, together with a four-point beam bending problem, are available via the OUP website (full details are given in Appendix B). In addition, the very same problems are analysed using the built-in ABAQUS linear strain hardening plasticity model (chosen to represent a material with E = 210,000 GPa, ν = 0.3, σy = 240 MPa, and h = 1206 MPa). In all the analyses using the explicit UMAT, the maximum time increment allowed in the analysis is carefully chosen to ensure stability and accuracy. Despite this, at the elastic–plastic transition, the stress at ﬁrst yield is overestimated because the stress at the start of the increment was determined on the basis of elastic behaviour in the previous increment. With an explicit scheme, this is never corrected so that the stresses remain slightly overestimated throughout the analysis. The error in stress can be reduced by decreasing the time increment size, but at the cost of the computer CPU time and error accumulation. In any case, many more time increments are required using the explicit UMAT than are required using the built-in ABAQUS implicit plasticity integration. This is a further serious shortcoming of the explicit integration method, which needs to be weighed against the advantage

Isotropic hardening plasticity implementation

175

of simplicity, particularly for complex constitutive equations. However, despite considerably longer computer CPU times, the results obtained for the four-point bend simulation from the explicit UMAT and the built-in ABAQUS plasticity model are found to be near-identical. We consider an implicit implementation in Section 6.4.2. 6.4.2

Implicit integration for isotropic hardening plasticity with consistent Jacobian

We may summarize the implementation as follows. As opposed to the explicit case, all quantities are now assumed to be given at the end of the time increment, that is, at time t + t, unless otherwise indicated. (i) Determine the elastic trial stress σ tr = σt + 2Gε + λIε : I . (ii) Determine the trial yield function f =

σetr

− r − σy =

3 tr

σ : σ tr 2

(6.11)

1/2 − r − σy .

(6.12)

(iii) Determine if actively yielding Is f > 0? (iv) If yes, use Newton iteration to determine the effective plastic strain increment r (k) = rt + hp, dp =

σetr − 3Gp (k) − r (k) − σy , 3G + h

(6.13)

p (k+1) = p(k) + dp. Otherwise, p = 0. (v) Determine plastic and elastic strain and stress increments

σ tr 3 ε = p tr , 2 σe p

ε e = ε − εp ,

(6.14)

σ = 2Gε + λIε : I . e

e

(vi) Update all quantities to the end of the time increment σ = σt + σ , p = pt + p.

(6.15)

176

Implementation of plasticity models

(vii) Determine consistent Jacobian

σ tr σ tr 2 δσ = 2GQ tr tr : δε + 2GRδε + K − GR II : δε. σe σe 3

(6.16)

(viii) End. An ABAQUS UMAT containing this formulation, together with various input ﬁles for uniaxial displacement and load control, together with a four-point beam bending problem, are available through the OUP website (full details are given in Appendix B). In addition, as before, the very same problems are analysed using the built-in ABAQUS linear strain hardening plasticity model. Using implicit integration with the consistent tangent stiffness eliminates the problem which occurred at the elastic–plastic transition when using explicit integration. In addition, the use of implicit integration enables much larger time increments to be used, therefore signiﬁcantly reducing CPU times. The disadvantage of the implicit formulation is simply the difﬁculty in obtaining the consistent tangent stiffness for complex constitutive equations. Often, analytical forms are simply not obtainable, in which case a numerical procedure may be possible. The results obtained for the four-point bend simulation from the implicit UMAT and the built-in ABAQUS plasticity model are found to be identical.

6.5

Large deformation implementations

We have not yet differentiated between small and large deformation implementations in this chapter. In fact, the UMATs discussed above for both explicit and implicit schemes are suitable for both small and large deformation problems using ABAQUS. This is because the necessary rigid body rotations for the strains and stresses have already been carried out by ABAQUS before they are provided to the UMAT routine. That is, referring back to Section 5.6, the large deformation stress update necessary is ∇

∇

σ = σ + (W σt − σt W )t = σ + Rσt R T ∇

(6.17)

in which σ is the co-rotational stress increment. The stress, σt , at the start of the time increment (and the strain) has already been rotated by ABAQUS (i.e. the stress provided at the start of the time increment is effectively Rσt R T ) so that all we need to do within the UMAT is to carry out the stress update. Sometimes, depending on the plasticity model employed, it is necessary to use internal variables which are also tensor quantities. An example is the back stress in a kinematic hardening model. The components of the back stress will need to be updated within the UMAT ( just like the scalar isotropic hardening variable in the previous sections) and stored in what are called state variable arrays in ABAQUS. Because state variables are not modiﬁed

Large deformation implementations

177

by ABAQUS, it is necessary for the user to carry out the rigid body rotations on tensorial state variables. In fact, ABAQUS provides a utility subroutine to simplify this process. If, for example, the tensorial variable recovered from the state variable array at the start of the increment is, say, x t , then the user must carry out the rigid body rotation Rx t R T before updating x to the end of the time increment within the UMAT. The rotation is carried out by a single call of the utility subroutine rotsig detailed in the ABAQUS manuals. Sometimes, constitutive equations for elasticity and plasticity are formulated in terms of the deformation gradient, F. Examples include hyperelasticity—large strain non-linear elasticity and crystal plasticity. It may be, however, that the user simply wishes to work from the deformation gradient rather than use the strain and stress quantities provided by ABAQUS to the UMAT subroutine. In Section 6.5.1, we present a large deformation implementation based on an explicit scheme.

6.5.1

Implementation using the deformation gradient

We may summarize the implementation as follows. In this explicit approach, all quantities are assumed to be given at time, t, that is, at the start of the time increment, unless indicated otherwise. (i) Determine the velocity gradient L = F˙ F −1 .

(6.18)

(ii) Determine the rate of deformation and spin D=

1 (L + LT ), 2

W =

1 (L − LT ). 2

(6.19)

(iii) Determine the yield function f = σe − r − σy =

3

σ : σ

2

1/2 − r − σy .

(6.20)

(iv) Determine if actively yielding Is

f > 0?

(6.21)

(v) Determine rate of plastic deformation f > 0, f < 0,

D p = as speciﬁed by constitutive equation, D p = 0.

(6.22)

178

Implementation of plasticity models

(vi) Determine rate of elastic deformation and Jaumann stress rate and isotropic hardening rate De = D − Dp, ∇

σ = 2GD e + λID e : I ,

(6.23)

r˙ = h˙ p. (vii) Determine stresses with respect to material reference ∇

σ˙ = σ +W σ − σ W .

(6.24)

(viii) Update all quantities to the end of the time increment, using explicit integration σt+t = σ + σ˙ t,

(6.25)

rt+t = r + r˙ t. (ix) Determine Jacobian. (x) End.

We will next address the veriﬁcation of a large deformation implementation, which is valid for both the implicit and explicit implementations in Sections 6.4.1 and 6.4.2. Note that uniaxial displacement or force controlled loading will not test whether the rigid body rotations are being calculated correctly, since for these cases, the continuum spin, W , is zero. A good test, however, is provided in the form of simple shear if we allow the strains to become quite large. To simplify matters, we will ‘switch off’ the plasticity and allow elasticity only, since the test is being carried out to check the rigid body rotation calculation rather than the constitutive response. We obtained the deformation gradient for simple shear in Section 3.5.1 as 1 δ F = . 0 1 ˙ the velocity gradient is Considering a constant rate of shearing, δ, 0 δ˙ L= 0 0 so that the rate of deformation and spin are 1 0 δ˙ 1 0 D= , W = 2 δ˙ 0 2 −δ˙

δ˙ . 0

Large deformation implementations

179

Note that the spin is non-zero so that rigid body rotation, together with stretch, is occurring. The Jaumann stress rate is given by ∇ 0 δ˙ σ = 2GD + λID : I = G ˙ (6.26) δ 0 and the stress rate with respect to the material (undeformed) reference is σ˙ xx σ˙ xy σ˙ = , σ˙ xy σ˙ yy

(6.27)

which is given in terms of the Jaumann stress rate by ∇

σ˙ = σ +W σ − σ W so that substituting for the spin and (6.26) and (6.27) gives 1 1 −σxy σyy σ˙ xx σ˙ xy σxy 0 1 ˙ ˙ = Gδ + δ − δ 1 0 σ˙ xy σ˙ yy 2 −σxx −σxy 2 −σyy

σxx σxy

so that 1 ˙ yy − σxx ), σ˙ xy = Gδ˙ + δ(σ 2 ˙ xy , σ˙ xx = δσ ˙ xy . σ˙ yy = −δσ

(6.28) (6.29) (6.30)

Equations (6.29) and (6.30) give, with the initial condition that all stresses are zero, σyy = −σxx . Differentiating (6.28) and substituting for (6.29) and (6.30) gives σ¨ xy + δ˙2 σxy = 0, which has solution ˙ + B cos δt. ˙ σxy = A sin δt The initial conditions require that B = 0. Solving for σxx and σyy using Equations (6.29) and (6.30) and imposing the initial conditions gives the solution ˙ σxy = G sin δt,

˙ σxx = −σyy = G(1 − cos δt).

(6.31)

180

Implementation of plasticity models

Stress (GPa)

y

x

150 100 50 0 –50 0.00 –100 –150 –200

sxx sxy 0.20

0.40

0.60

0.80

1.00

Time (s)

syy

Fig. 6.3 Unit square under simple shear at a rate of 5.0 s−1 and the corresponding stresses.

For small strain, δ, at constant strain rate, these reduce to σxy = Gδ

and

σxx = −σyy = 0.

(6.32)

The harmonic variation in (6.31) results from the large deformation, and in particular, the rigid body rotation taking place. This non-physical result arises because we are using a small strain, linear elasticity model under conditions of large deformation. Despite its non-physicality, it provides a good test of the calculation of the rigid body rotations in the large deformation UMAT. In order to do this, a single plane strain element, as shown in Fig. 6.2, has been subjected to simple shear to large strain. This has been carried out using the UMAT with elasticity described in Section 6.2, which uses ABAQUS-provided stresses and strains, a further UMAT based on the deformation gradient, described in this section, and using the built-in elasticity model in ABAQUS. The results obtained are identical and are shown in Fig. 6.3. The various UMATs, together with the ABAQUS input ﬁles, are detailed in Appendix B and are available via the OUP website.

6.6

Elasto-viscoplasticity implementation

Viscoplasticity, meaning rate-dependent plasticity in which the plastic multiplier is determined through the use of a viscoplastic constitutive equation as opposed to the use of the consistency condition, was introduced in Chapter 4. The radial return, implicit backward Euler integration for viscoplasticity was discussed in Chapter 5. Here, we present an implicit implementation for linear isotropic strain hardening elasto-viscoplasticity. Such an implementation can readily be simpliﬁed for the implicit analysis of creep. We employ a sinh-type viscoplastic constitutive equation and for simplicity, use the initial tangent stiffness (i.e. the elastic stiffness) for the material Jacobian. The viscoplastic constitutive equation is taken to be p˙ = φ(σe , r) = α sinh β(σe − r − σy )

Elasto-viscoplasticity implementation

181

and the multiaxial plastic strain increments are given by εp = pn =

σ

3 p . 2 σe

We determine the increment in effective plastic strain as described in Chapter 5 as follows. Note that all quantities are now assumed to be given at the end of the time increment, that is, at time t + t, unless otherwise indicated. (i) Determine the elastic trial stress σ tr = σ t + 2Gε + λIε : I .

(6.33)

(ii) Determine the trial yield function f =

σetr

− r − σy =

3 tr

σ : σ tr 2

1/2 − r − σy .

(6.34)

(iii) Determine if actively yielding Is

f > 0?

(iv) If yes, use Newton iteration to determine the effective plastic strain increment φ(σe , r) = α sinh β(σetr − 3Gp − r − σy ), φp = −3Gαβ cosh β(σetr − 3Gp − r − σy ), φr = −αβ cosh β(σetr − 3Gp − r − σy ), (6.35)

r = rt + hp, dp =

φ(p, r) − (p/t) , (1/t) − φp − hφr

p(k+1) = p(k) + dp. (v) Determine plastic and elastic strain and stress increments

σ tr 3 ε = p tr , 2 σe p

ε e = ε − εp ,

(6.36)

σ = 2Gε + λIε : I . e

e

182

Implementation of plasticity models

(vi) Update all quantities to the end of the time increment σ = σ t + σ , p = pt + p.

(6.37)

(vii) Determine Jacobian. (viii) End. An ABAQUS UMAT containing this formulation, together with various input ﬁles for uniaxial displacement and load control, together with a four-point beam bending problem, are available via the OUP website (full details are given in Appendix B). In addition, uniaxial, closed form implicit and explicit solutions are provided in Fortran programs for veriﬁcation of the implementation.

Part II. Plasticity models

This page intentionally left blank

7. Superplasticity

7.1

Introduction

Superplasticity is the ability of some materials to undergo very large, irreversible, tensile elongations without necking and failing. Generally, a very ﬁne grain structure is required (a typical grain size will be of the order of 1 µm) and a deformation temperature of about 0.5 Tm is necessary to enable the appropriate superplastic deformation mechanisms to operate. Two common superplastically formed classes of material are aluminium and titanium alloys, which are used extensively in the aerospace and aeroengine industry. Superplastic forming exploits the ability of the material to undergo very large tensile elongations in metal sheet stretch forming and blow moulding processes, and has many advantages for the manufacture of complex shapes in sheet metal using simple low pressure pneumatic forming equipment. In this chapter, we shall introduce superplasticity and its characteristics, constitutive equations for superplastic deformation which are coupled with the accompanying microstructural evolution, the multiaxial form of the equations, and an industrial application.

7.2

Some properties of superplastic alloys

Superplasticity is very much a viscoplastic process in the sense that the stress response is highly strain-rate dependent. The uniaxial response to variable constant true strain-controlled loading is simpliﬁed and schematically shown in Fig. 7.1. There is often a very strong strain-rate sensitivity, and in addition, strain hardening is seen to occur. This results from a number of possible causes including the effect of grain growth which occurs in superplasticity, and from dislocation hardening processes. If we choose a particular strain in Fig. 7.1(b) and pick off the corresponding stress for each of the stress–strain curves at all the strain rates, we may then plot log(stress) versus log(strain rate), which often produces a curve of the form shown in Fig. 7.2. Region (i) corresponds to very low strain rates in which diffusion processes dominate when the temperature is higher than ∼0.5 Tm . Region (iii) corresponds to very high

186

Superplasticity «3 •

(a)

(b) «2 «1 •

Stress

Strain

•

s3

«3

s2

«2

s1

«1

•

•

•

sy

Time

Strain

Fig. 7.1 Schematic showing simpliﬁed superplastic stress response which is dependent on strain rate.

ln(stress)

Superplastic region

(i)

(ii)

(iii)

ln(strain rate)

Fig. 7.2 log(stress) versus log(strain) showing the region usually considered to be superplastic.

strain rate at which diffusion is largely inhibited so that deformation occurs through dislocation motion, some of which is perhaps thermally activated, but diminishing with increasing strain rate. Region (ii) is that in which superplasticity takes place; that is, large tensile strains (∼1–2) are achievable which are many times larger than those obtainable in regions (i) and (iii). Because of the approximate linearity in region (ii), the ln(stress)–ln(strain rate) relationship can be written as ln(σ ) = m ln(˙ε ) + k

(7.1)

in which m and k are constants. Rearranging (7.1) gives σ = K ε˙ m

(7.2)

in which K is a further constant. In Equation (7.2), m is called the strain-rate sensitivity and is, of course, the gradient of the ln(stress) versus ln(strain rate) curve. In fact, the higher the value of m, the better the superplastic deformation, and the larger the tensile elongations achievable in the absence of necking and failure. Generally, for what would be described as superplastic deformation, m > 0.35. If, from Fig. 7.2, we now plot the strain-rate sensitivity versus ln(strain rate), we will obtain the graph shown schematically in Fig. 7.3.

Some properties of superplastic alloys

187

Superplastic region m

0.35

ln(strain rate)

Fig. 7.3 Schematic representation of strain-rate sensitivity versus log(strain rate). L

L + dL

P

P

Uniform region with

Area Stress Strain rate

A s • «

Necked region with

Area Stress Strain rate

A + dA s + ds • « + ds

Fig. 7.4 Schematic diagram showing a uniform, circular test piece with cross-sectional area A under load P before and after the introduction of a neck.

We shall now examine further the signiﬁcance of the strain-rate sensitivity, m, in superplasticity, by considering a uniform, uniaxial circular test piece containing a single, idealized neck shown schematically in Fig. 7.4. We employ the incompressibility condition, apply constant load, P , to the test piece during necking and assume the stress–strain rate relationship given in (7.2). The incompressibility condition gives AL = (A + dA)(L + dL) ≈ AL + L dA + A dL

188

Superplasticity

so that

dL dA =− = −dε = −˙ε dt A L

and

dA = −˙ε A dt

(7.3)

or, in the neck,

d(A + dA) = −(˙ε + d˙ε )(A + dA), dt which, when combined with (7.3) gives d A d˙ε (dA) ≈ −(A d˙ε + ε˙ dA) = −dA˙ε +1 . dt dA ε˙

(7.4)

The constancy of load, P , gives σA = (σ + dσ )(A + dA) so that

dA dσ =− . (7.5) σ A The constitutive equation σ = K ε˙ m gives d˙ε d˙ε m m m m 1+ = K ε˙ 1 + m + · · · σ + dσ = K(˙ε + d˙ε) = K ε˙ ε˙ ε˙ so that

d˙ε dσ ≈m . σ ε˙

(7.6)

Combining (7.6) and (7.5) gives A d˙ε 1 =− dA ε˙ m and substituting into (7.4) gives

d 1 (dA) ≈ −dA˙ε 1 − . dt m

(7.7)

This equation tells us that the rate of development of the neck depends upon the quantity 1 − (1/m). As the strain-rate sensitivity increases, and approaches unity, the rate of necking decreases to zero. We therefore see the signiﬁcance of the strainrate sensitivity in superplasticity; the higher the value of m, the more necking can be inhibited therefore allowing greater elongations prior to the onset of necking and failure. A much more complete introduction to superplasticity can be found in Pilling and Ridley (1989).

Constitutive equations for superplasticity

7.3

189

Constitutive equations for superplasticity

The constitutive equation in (7.2) is simple, but is often inadequate for simulating superplasticity processes because the ln(stress)–ln(strain rate) relationship is not often linear, particularly over strain-rate regimes which occur in practical processing. In addition, it says nothing about the inﬂuence of changing microstructure during superplastic deformation, which is known to be important (Ghosh and Hamilton, 1979; Ghosh and Raj, 1981; Hamilton, 1984; Zhou and Dunne, 1996). We present here constitutive equations for superplasticity for the particular commercially important titanium alloy, Ti–6Al–4V. This alloy ﬁnds application in a range of aero-engine components, but for component manufacture using superplastic forming, the engine fan blades are perhaps the most important. Uniaxial stress–strain curves for the Ti–6Al–4V alloy undergoing superplastic deformation at 927◦ C are shown in Fig. 7.5. A strong strain-rate effect is seen together with signiﬁcant strain hardening. The stresses required to cause the deformation are, however, really quite small but the tensile strains achieved during the superplastic deformation are large. The hardening is due to several processes; perhaps the most important is the increasing average grain size. The average grain size at the start of all the tests shown in Fig. 7.5 is 6.4 µm. At the end of the deformation, it has increased to about 10 µm, and depends on the rate of deformation. The evolution of the average grain size for each of the stress–strain curves shown in Fig. 7.5 is shown in Fig. 7.6.

25 1.0 × 10–3 s–1

Stress (MPa)

20

15 2.0 × 10–4 s–1 10

5

5.0 × 10–5 s–1

0 0.0

0.2

0.4

0.6 Strain

0.8

1.0

Fig. 7.5 Superplastic stress–strain curves for Ti–6Al–4V at 927◦ C at the strain rates shown. The initial grain size is 6.4 µm.

190

Superplasticity

0.012 5.0 × 10–5 s–1

Grain size (mm)

1.0 × 10–3 s–1

0.0 s–1

2.0 × 10–4 s–1

0.01

0.008

0.006 0

100

200

300

400

Time (min)

Fig. 7.6 Grain size versus time curves for Ti–6Al–4V at 927◦ C at the strain rates shown. The initial grain size is 6.4 µm.

An important feature is that for a strain rate of 0.0 s−1 , that is, a static test in which no deformation takes place, grain growth still takes place; this is called static grain growth. As the strain rate is increased, so the rate of growth of grain size increases. That part of the grain growth resulting from the straining is often referred to as deformation-enhanced grain growth. Normal grain growth (Shewmon, 1969) gives rise to a kinetic equation for static grain growth of the form α1 l˙ = γ (7.8) l in which l is the average grain size, and α1 and γ are material constants. The deformation-enhanced grain growth is accounted for with an additional term so that the complete kinetic equation can be written as α1 l˙ = γ + β1 p˙ (7.9) l in which β1 is a further material constant and p˙ is, as before, the effective plastic strain rate. The symbols in Fig. 7.5 are, in fact, experimental data and the lines result from ﬁtting Equation (7.9) to the data. The material constants for this particular temperature of 927◦ C are given in Table 7.1 and assume grain size to be speciﬁed in millimetres. We now return to the microstructure–deformation coupling (Zhou and Dunne, 1996; Kim and Dunne, 1999) and employ the following elastic-viscoplastic constitutive equations α ε˙ p = µ sinh β(σ − r − σy ), (7.10) l ˙ (7.11) r˙ = (c1 − γ1 r)p, σ˙ = E(˙ε − ε˙ p ),

(7.12)

Constitutive equations for superplasticity

191

Table 7.1 Material constants for Ti–6Al–4V at 927◦ C. α 0.437 × 10−5

β 0.0919

µ 1.06

σy (MPa) 0.5

E (MPa) 1000

c1 8.397

γ1 0.666

α1 0.128 × 10−16

β1 0.9625 × 10−13

γ 5.0

Stress (MPa)

100

10 1.0 0.6 0.2

1 10–6

10–5

10–4 10–3 Strain rate (s–1)

10–2

10–1

Fig. 7.7 Experimental (symbols) and predicted (lines) stress versus strain rate curves for Ti–6Al–4V at 927◦ C with an initial grain size of 6.4 µm for the strain levels shown.

which are coupled with the grain growth equation in (7.9). Equation (7.10) is the viscoplastic constitutive equation in which, as before, α and β are material constants, l is the current grain size, and µ the deformation–microstructure coupling constant. The hardening seen in Fig. 7.4 does not all result from the grain growth, although a substantial part of it does. A further isotropic hardening term, r, has therefore been introduced with evolution equation given in (7.11) in which c1 and γ1 are material constants. Equation (7.12) is Hooke’s law. Equations (7.9)–(7.12) constitute the uniaxial material model for superplasticity. With the material constants for the grain growth kinetic equation having been already determined, the unknown constants in Equations (7.10) and (7.11) are obtained by ﬁtting the equations (Zhou and Dunne, 1996) to the experimental data in Fig. 7.5. The resulting computed stress–strain curves are given by the solid lines in the ﬁgure. Comparisons of predicted and experimental log(stress) versus log(strain rate) behaviour for the Ti-alloy with an initial grain size of 6.4 µm obtained at the strain levels shown are given in Fig. 7.7, and the corresponding predicted variation of strain-rate sensitivity with strain rate (at a strain of 1.0) is shown in Fig. 7.8.

192

Superplasticity 1.0

Strain-rate sensitivity

0.8

0.6

0.4

0.2

0.0 1E–06

Initial grain size 6.4 mm 9 mm 11.5 mm

1E–05

1E–04

1E–03

1E–02

1E–01

Strain rate (s–1)

Fig. 7.8 Predicted variation of strain-rate sensitivity with strain rate for the initial grain sizes shown for Ti–6Al–4V at 927◦ C.

7.4

Multiaxial constitutive equations and applications

We may write the multiaxial equations within the framework of viscoplasticity by assuming the normality hypothesis and von Mises material behaviour. The multiaxial viscoplastic strain rate, given these assumptions, is Dp =

3 σ

p˙ , 2 σe

(7.13)

where

α sinh β(σe − r − σy ) (7.14) lµ and Equations (7.9) and (7.11) remain unchanged. If considering large deformations (which is normally the case for superplasticity), the Jaumann stress rate is, as before, p˙ =

∇

σ = σ˙ + W σ − σ W .

(7.15)

These equations, together with (7.9) and (7.11), have been implemented into ABAQUS by means of the CREEP routine, which is described in Chapter 8. This facilitates an easier implicit implementation, but a UMAT implementation would be carried out as described for viscoplasticity in Chapters 5 and 6, although if a plane stress implementation is required, additional problems would need to be addressed. The application we consider is the superplastic blow-forming of a rectangular-section box made from 1.25 mm thick Ti–6Al–4V sheet and processed at 900◦ C (Lin and Dunne, 2001, with thanks to Dr. Lin). The model is shown in Fig. 7.9 in which just one quarter

Multiaxial constitutive equations and applications

193

Material mesh

Rigid die surface

Die surface normal

Fig. 7.9 Finite element model for the rectangular-section box die surface and the material blank.

is included, for reasons of symmetry, and both the initially ﬂat sheet and the die surface are included. The superplastic forming process consists of clamping the ﬂat Ti-alloy sheet (modelled using shell elements) against the die, the surface of which forms a cavity in the shape required. Gas pressure is applied to the top face of the sheet, forcing it to acquire the die shape. In these analyses, the maximum strain rate over the deforming sheet is controlled to be close to the optimum deforming rate of the material; that is, the strain rate required to give the highest strain-rate sensitivity obtained from the equivalent of Fig. 7.7, but for 900◦ C. This is achieved by varying the applied gas pressure. The process is considered completed at a forming time, tf , when all nodes on the deforming sheet are in contact with the die. Figure 7.10 shows the deformation of the superplastic metal sheet at three stages during the forming process at times t/tf = 0.1, t/tf = 0.6, and t/tf = 1.0. The contours show the magnitude of the effective plastic strain rate. The maximum target strain rate speciﬁed for the analysis is 1.0 × 10−5 s−1 which is achieved by application of uniformly distributed gas pressure. Figure 7.10 shows that the distribution of effective plastic strain rate is highly non-uniform. This is typical of many practical superplastic forming processes; while ideally it is necessary to deform superplastically all points in the material at the same optimum strain rate (to maximize strain-rate sensitivity and hence elongation), this is rarely achievable in practice. It is possible, however, to ensure that a target maximum strain rate is not exceeded, and in this analysis, the gas pressure is varied to ensure a nominal maximum strain rate of 1.0 × 10−5 s−1 . The variation of the maximum strain rate during the

194

Superplasticity

(a) Strain rate + 0.00E–00 + 2.00E–06 + 3.00E–06 + 4.00E–06 + 5.00E–06 + 6.00E–06 + 7.00E–06 + 8.00E–06

(b) Strain rate + 0.00E–00 + 2.00E–06 + 3.00E–06 + 4.00E–06 + 5.00E–06 + 6.00E–06 + 7.00E–06 + 8.00E–06

(c) Strain rate + 0.00E–00 + 2.00E–06 + 3.00E–06 + 4.00E–06 + 5.00E–06 + 6.00E–06 + 7.00E–06 + 8.00E–06

Fig. 7.10 The simulated superplastically deforming sheet showing the effective plastic strain rate at fractional processing times of t/tf = 0.1, t/tf = 0.6, and t/tf = 1.0. (See also Plate 1.)

forming process is shown in Fig. 7.11 for target strain rates of both 1.0 × 10−5 s−1 and 1.0 × 10−4 s−1 , and the corresponding variations in gas pressure to achieve these are given in Fig. 7.12. Higher gas pressure is needed for the higher target strain rate because of the higher ﬂow stresses required. The gas pressure increases during the

Multiaxial constitutive equations and applications

195

Maximum strain rate (s–1)

1E–03

1 × 10– 4 s–1 1E–04

1 × 10– 5 s–1 1E–05

1E–06 0.0

0.2

0.4

0.6

0.8

1.0

t /t f

Fig. 7.11 Variation of the maximum strain rate over the deforming material blank during the superplastic forming process for the two target strain rates ε˙ = 1 × 10−5 and ε˙ = 1 × 10−4 s−1 .

Gas pressure (KPa)

400

300

200 1 × 10– 4 s–1

100 1 × 10– 5 s–1

0 0.0

0.2

0.5 t /t f

0.8

1.0

Fig. 7.12 Variation of gas pressure to ensure a maximum strain rate in the deforming sheet of 1.0 × 10−5 and 1.0 × 10−4 s−1 .

superplastic forming because of increasing geometrical and frictional constraint and, in addition, because the material hardens during deformation which is due to the grain growth taking place. High gas pressure is required to ﬁll the corner part of the die, which is the last stage of the forming process. In Fig. 7.10, it is apparent that the last part of the sheet to be formed is the corner, which is also the area of maximum thinning and where tearing is most likely to occur. This is made clear by looking at the through-thickness strain ﬁelds which are shown for the two target strain rates of 1.0 × 10−5 and 1.0 × 10−4 s−1 in Fig. 7.13(a) and (b), respectively.

196

Superplasticity

(a)

Thickness strain – 1.20E+00 – 1.07E+00 – 9.15E–01 – 7.60E–01 – 6.05E–01 – 4.50E–01 – 2.95E–01 – 1.40E–01

(b) Thickness strain – 1.20E+00 – 1.07E+00 – 9.15E–01 – 7.60E–01 – 6.05E–01 – 4.50E–01 – 2.95E–01 – 1.40E–01

Fig. 7.13 Through-thickness strain ﬁelds at the end of the superplastic forming carried out with target maximum strain rates of (a) 1.0 × 10−5 and (b) 1.0 × 10−4 s−1 . (See also Plate 2.)

The lower strain rate is seen to lead to a higher spatial variation in throughthickness strain; that is, thinning, which is often not desirable in practical processing. In fact, the ranges of out-of-plane strain for the low and high strain rates are 1.06 and 0.84, respectively. The reason for this becomes clear on looking at the grain size distributions, shown in Fig. 7.14. At the lower target strain rate, the average grain size increase is larger than that at the higher strain rate because of static grain growth, which is inhibited in the latter. In addition, at the lower strain rate, the range of ﬁnal grain size is less than that at the higher rate. For the case of the higher strain rate, therefore, the larger grain size in the deforming material in the corner (relative to that at the boundaries) leads to a higher stress in the corner region to generate the same strains seen for the lower strain rate. This inhibits straining in the corner region producing larger strains in the boundary regions. The net result is a more uniform strain distribution for the high strain rate, and a correspondingly more uniform thinning. This is generally preferable

References

197

(a) Grain sizes + 1.14E–02 + 1.15E–02 + 1.16E–02 + 1.16E–02 + 1.17E–02 + 1.18E–02 + 1.18E–02 + 1.19E–02

(b)

Grain sizes +7.93E – 03 +8.06E – 03 +8.20E – 03 +8.33E – 03 +8.60E – 03 +8.74E – 03 +8.88E – 03 +9.01E – 03

Fig. 7.14 Average grain size ﬁelds at the end of the superplastic forming carried out with target maximum strain rates of (a) 1.0 × 10−5 and (b) 1.0 × 10−4 s−1 . (See also Plate 3.)

in practice, and results directly from the interactions of the superplastic deformation and microstructural evolution. These industrially important effects could not have been obtained without microstructurally based constitutive equations. An additional important effect is the distribution of grain size in commercial Ti–6Al–4V, which has not been addressed here. However, modelling techniques to incorporate it, its effects on strain-rate sensitivity and hence on necking and failure have been addressed by Kim and Dunne (1999), where further information may be found.

References Ghosh, A.K. and Hamilton, C.H. (1979). ‘Mechanical behaviour and hardening characteristics of a superplastic Ti–6Al–4V alloy’. Metallurgical Transactions, 10, 699–706. Ghosh, A.K. and Raj, R. (1981). ‘Grain size distribution effect in superplasticity’. Acta Metallurgica, 29, 607–616.

198

Superplasticity

Hamilton, C.H. (1984). ‘Superplasticity in titanium alloys’. In Agrawal, S.P. (ed.), Superplastic Forming, Proceedings of the Symposium, California, March 13–22, American Society for Metals. Kim, T.-W. and Dunne, F.P.E. (1999). ‘Modelling heterogeneous microstructures in superplasticity’. Proceedings of the Royal Society, 455, 701–718. Lin, J. and Dunne, F.P.E. (2001). ‘Modelling grain growth evolution and necking in superplastic blow-forming’. International Journal of Mechanical Science, 43, 595–609. Pilling, J. and Ridley, N. (1989). Superplasticity in Crystalline Solids. The Institute of Metals, London. Shewmon, P.G. (1969). Transformations in Metals. McGraw-Hill, New York. Zhou, M. and Dunne, F.P.E. (1996). ‘Mechanisms-based constitutive equations for the superplastic behaviour of a titanium alloy’. Journal of Strain Analysis, 31, 65–73.

8. Porous plasticity

8.1

Introduction

We have so far considered plasticity and viscoplasticity processes in which it has been assumed that the deforming material has been incompressible. There are some materials, however, for which this is not the case. An important example is in the processing of metal powders in which, generally at elevated temperature, the powder is consolidated by plastic deformation and the elimination of the porosity. During the process, signiﬁcant volume changes occur because of the removal of the porosity. A further example of compressible or porous plasticity is that in which signiﬁcant voiding develops in a material undergoing plastic deformation resulting from a damage process (e.g. creep cavitation). Again, while possibly small, volume changes occur during the deformation and the incompressibility condition no longer holds. A feature of the constitutive equations in porous plasticity is that there becomes a dependence on mean stress as we shall see shortly. In this chapter, we introduce the porous plasticity model of Duva and Crow and outline its implementation into ABAQUS using both a UMAT material subroutine and the simpler ABAQUS CREEP routine. For simplicity, within the UMAT, we use explicit integration of the constitutive equations and employ the initial stiffness as the material Jacobian. A number of constitutive relations for the consolidation of metal powders have been developed. They have been used to predict the dependence of densiﬁcation rate on consolidation pressure and temperature as well as volume fraction of voids. One of the ﬁrst constitutive models for consolidation of metal powder was developed by Wilkinson and Ashby (1975). They analysed the creep collapse of a thick-walled spherical shell subjected to externally applied hydrostatic loading. In general, consolidation occurs under the action of a range of stress states that are not purely hydrostatic, for which the Wilkinson and Ashby model is therefore inappropriate. Subsequent research has therefore broadened the Wilkinson and Ashby model to more general loading conditions. The models have taken into account the effects of deviatoric and hydrostatic components of stress state by introducing potentials which make possible the

200

Porous plasticity

development of relationships between macroscopic strain rate and stress state (Cocks, 1989; Ponte Castaneda, 1991; Duva and Crow, 1992; Sofronis and McMeeking, 1992). The strain rate potential (φ) for a porous material can be written as a function of both deviatoric and hydrostatic stresses ε˙ 0 σ0 φ= n+1

S σ0

n+1 ,

(8.1)

where S 2 = aσe2 + bσm2 , 3

σ : σ , 2 1 σm = II : σ . 3 σe2 =

(8.2) (8.3) (8.4)

S is an effective effective stress (Duva and Crow, 1994) given in terms of the effective, σe , and hydrostatic, σm , stresses, n is the creep exponent, and the coefﬁcients a and b are functions of current relative density, D, which is equivalent to the solid volume fraction of the porous material, a is associated with the deviatoric component and b with the hydrostatic component. The coefﬁcients a and b are chosen such that, at the fully dense stage, that is, D = 1, the coefﬁcient b becomes 0 and a becomes 1. The effective effective stress, S, is then reduced to σe . The various densiﬁcation models for monolithic materials in the literature use different approaches to obtain the strain rate potential. This leads to different expressions for the coefﬁcients a and b (Duva and Crow, 1994). Duva and Crow (1994) proposed a strain rate potential for computing densiﬁcation rates. Based on the strain rate potentials of Cocks (1989) and Ponte Castaneda (1991), the coefﬁcients a and b were chosen to ensure that the potential gives densiﬁcation rates identical to those of Wilkinson and Ashby (1975) in the hydrostatic load limit, and agree with both Cocks (1989) and Ponte Castaneda (1991) in the limit when the hydrostatic stress vanishes. The densiﬁcation rates predicted by Duva and Crow’s strain rate potential are consistent with their cell model calculations which were derived based on Hill’s minimum principle for velocity. Duva and Crow predict densiﬁcation rates which compare favourably with the prediction from the Wilkinson and Ashby model in the hydrostatic limit. The Duva and Crow potential also satisﬁes the lower bounds derived by both Cocks and Ponte Castaneda in the limit that the hydrostatic stress vanishes. The densiﬁcation rate predicted from the Duva and Crow model, in the presence of a large deviatoric stress component, is closer to the experimental results than the predictions of Sofronis and McMeeking (1992).

Implementation of porous material constitutive equations

8.2

201

Finite element implementation of the porous material constitutive equations

Strain rates are determined by differentiating the strain rate potential, φ, to give ∂φ 1 n−1 3

ε˙ = = AS aσ + bI σm (8.5) ∂σ 2 3 in which 2/(n+1) 2 1 + (2/3)(1 − D) 3 n(1 − D) a= and b = 1/n n 2n/(n+1) 2n (1 − (1 − D) ) D and where A is a material parameter given by ε˙ 0 A = n. (8.6) σ0 The dilatation rate can be obtained from ε˙ kk = ε˙ xx + ε˙ yy + ε˙ zz and hence, the densiﬁcation rate is given as D˙ = −D ε˙ kk ,

(8.7) (8.8)

where D is the relative density. 8.2.1

Implementation into ABAQUS UMAT

The constitutive equations for porous metals developed by Duva and Crow (1992) are implemented into the ﬁnite element software ABAQUS within a large deformation formulation using a UMAT subroutine. A simple, explicit, forward Euler integration is adopted. ABAQUS supplies to the UMAT subroutine the deformation gradient at the beginning and the end of each time step, F t and F t+δt . The user is required to supply the Cauchy stress at the end of the time step. The algorithms, ﬁrst, need to deﬁne the rate of deformation gradient, F˙ , which can be calculated, for small time steps, as 1 F˙ = (F t+δt − F t ). (8.9) δt Then, the velocity gradient, L, is L = FF −1 . The total rate of deformation, D, and the spin tensor, W , are given by 1 D = (L + LT ), 2 1 W = (L − LT ). 2

(8.10)

(8.11) (8.12)

202

Porous plasticity

The strain components are calculated independently from 1 ε = − ln(FF T )−1 . 2

(8.13)

˙ can be calculated from The dilatation rate, ε˙ kk , and the densiﬁcation rate, D, Equations (8.7) and (8.8), respectively. The relative density at the end of each time step is determined using the ﬁrst-order Euler integration scheme ˙ D t+δt = D t + Dδt.

(8.14)

∇

The co-rotational stress rate σ is given by ∇

σ =

Eν E De + II : D e , (1 + ν) (1 + ν)(1 − 2ν)

(8.15)

where E is Young’s modulus, ν is Poisson’s ratio, and D e is the rate of elastic deformation given by (8.16) De = D − Dp. D p is the rate of plastic deformation as given in Equation (8.5). The stress increment, with respect to the material reference frame, is calculated as ∇

∇

σ = σ +Rσ t R t .

(8.17)

This, therefore, provides for an objective update of the stress with respect to a ﬁxed ∇

coordinate system during the time step. The stress increment, σ , for each time step can be determined by utilizing the ﬁrst-order Euler integration scheme ∇

σ = σ t.

(8.18)

The updated stress is returned to ABAQUS through the UMAT subroutine. Because here, we adopt an explicit ﬁrst-order forward Euler integration, great care is necessary in choosing an appropriate time step, and in ensuring meaningful results are obtained. 8.2.2

Implementation into ABAQUS CREEP subroutine

The implementation of the Duva and Crow constitutive equations for consolidation is also carried out using the ABAQUS CREEP facility. This subroutine is suitable for constitutive equations in which the increments of inelastic strain are functions of the hydrostatic stress and the equivalent deviatoric stress described by Mises’ or Hill’s deﬁnitions, while the UMAT subroutine allows more general forms of constitutive laws to be implemented, and easier handling of internal state variables.

Implementation of porous material constitutive equations

203

ABAQUS computes the incremental creep strain components as 1 εcr = ¯εcr n + ¯εsw I , 3 where n is the direction normal to the yield surface, given by

(8.19)

∂σe . (8.20) ∂σ ¯ε cr and ¯ε sw are the equivalent creep strains conjugate to the deviatoric stress and the mean stress, respectively. Therefore, ¯εcr corresponds to the conventional deviatoric creep strain and ¯εsw to the volumetric strain occurring because of void closure. In order to implement the porous material constitutive equations using the CREEP subroutine, the plastic strain rate equation deﬁned in Equation (8.5) has to be decomposed into two parts as follows n=

3 1 ε˙ p = AS n−1 aσ + AS n−1 bσm I . (8.21) 2 3 The ﬁrst part is associated with the deviatoric stress and the second with the mean stress. The user is required to provide ¯ε cr , ∂¯εcr /∂σe , ∂¯εcr /∂p, ¯εsw , ∂¯εsw /∂σe , and ∂¯εsw /∂p, in which σe is the equivalent stress and p is the equivalent pressure stress given as 1 p = − (σxx + σyy + σzz ). (8.22) 3 The variables are obtained as follows: ¯ε cr = AS n−1 aσe t, 1 (n − 1)aσe ∂¯ε cr cr , + = ¯ε ∂σe σe S2 ∂¯ε cr cr (n − 1)bσm = −¯ε , ∂p S2 ¯εsw = Abσm S n−1 t, ∂¯εsw sw (n − 1)aσe , = ¯ε ∂σe S2 1 (n − 1)bσm ∂¯εsw sw = −¯ε . + ∂p σm S2

(8.23) (8.24) (8.25) (8.26) (8.27) (8.28)

In order to calculate σe and σm , the stress components are required. The CREEP subroutine does not provide these quantities, and therefore the USDFLD subroutine has to be utilized to access material point data and assign stress components to state variables, which are then passed into the CREEP subroutine. The densiﬁcation rate

204

Porous plasticity Table 8.1 Material parameters.

A0 n

T < 750◦ C

T ≥ 750◦ C

8.49 2.18

95.67 1.53

0.98

Relative density

0.93

0.88

0.83

Predicted using UMAT subroutine Predicted using CREEP subroutine

0.78 0

10

20

30

40

50

Time (min)

Fig. 8.1 Graph showing comparisons of relative density–time curves obtained from the porous plasticity material model utilizing both an ABAQUS UMAT subroutine and a CREEP subroutine.

can therefore be obtained from Equation (8.8). The relative density for each time increment can be determined by utilizing the ﬁrst-order Euler integration as given in Equation (8.14). The porous plasticity material model implemented using the CREEP subroutine was veriﬁed against that using the UMAT subroutine by simulating a simple compression process using a single plane strain element subjected to in-plane compressive load of 20 MPa at 925◦ C. The material constants, A0 and n, used are given in Table 8.1, and A is calculated from −Q (8.29) A = A0 exp RT in which T is the temperature, R the gas constant, and Q activation energy. Figure 8.1 shows comparisons of the relative density evolution over time calculated by the porous material model using the CREEP and the UMAT subroutines. The results can be seen to be identical. The Duva and Crow porous plasticity model has been used (empirically) to approximate the behaviour in consolidation of continuous (SiC) ﬁbre, (Ti) metal matrix

Application to consolidation of Ti–MMCs

205

300 mm

Reinforced area

Fig. 8.2 Schematic diagram of an aero-engine bling showing region of reinforcement with Ti–MMC and a demonstrator disc (from King, 1998).

composite materials (Ti–MMCs) being developed for potential application to aeroengine components together with shafts, discs, brakes, and aircraft landing gear. Application to an aero-engine ‘bling’—a bladed ring—is shown in Fig. 8.2. The Ti–MMC material in the unconsolidated and fully consolidated state is shown in Fig. 8.3(a) and (b), respectively.

8.3

Application to consolidation of Ti–MMCs

The simple consolidation model, which was implemented using the CREEP subroutine as described above, was set up to simulate (empirically) the consolidation of Ti–MMCs under a range of processing conditions. The consolidation process is

206

Porous plasticity

(a)

(b)

Fig. 8.3 Micrographs showing Ti–6Al–4V matrix, SiC continuous ﬁbre composite material (a) unconsolidated and (b) consolidated at 925◦ C for 30 min at 15 MPa.

Ti–MMC

Die

Fig. 8.4 Schematic diagram showing arrays of Ti–MMCs undergoing consolidation.

1 Model prediction Experimental data

Relative density

0.95

0.9

0.85

0.8

0.75 0

40

80

120

160

200

Time (min)

Fig. 8.5 Predicted and measured relative density evolution with time for Ti–6Al–4V/SiC composite consolidated at a constant temperature of 925◦ C with a pressure of 20 MPa.

References

207

1 Model prediction Experimental data

Relative density

0.95

0.9

0.85

0.8

0.75 0

40

80

120 Time (min)

160

200

Fig. 8.6 Predicted and measured relative density evolution with time for Ti–6Al–4V/SiC composite consolidated at a constant temperature of 700◦ C with a pressure of 20 MPa.

shown schematically in Fig. 8.4. Generally, there are many more layers of ﬁbres and the pressure is applied by means of a mechanical punch. The mechanical die ensures that the Ti–MMCs undergo plane strain compression. Some of the results of the simulations, which were carried out at a constant temperature of 925◦ C under a pressure of 20 MPa, and at a temperature of 700◦ C under a constant pressure of 20 MPa, are shown in Figs 8.5 and 8.6, respectively, showing the important effect of temperature.

References Cocks, A.C.F. (1989). ‘Inelastic deformation of porous materials’. Journal of the Mechanics and Physics of Solids, 37(6), 693. Duva, J.M. and Crow, P.D. (1992). ‘The densiﬁcation of powders by power-law creep during hot isostatic pressing’. Acta Metallurgica, 40(1), 31. Duva, J.M. and Crow, P.D. (1994). ‘Analysis of consolidation of reinforced materials by power-law creep’. Mechanics of Materials, 17, 25. King, J. (1998). ‘Composites take off without a parachute’. Materials World, 5(6), 324. Ponte Castaneda, P. (1991). ‘The effective mechanical properties of nonlinear isotropic composites’. Journal of the Mechanics and Physics of Solids, 39(1), 45. Sofronis, P. and McMeeking, R.M. (1992). ‘Creep of power-law material containing spherical voids’. Journal of Applied Mechanics, Transactions of ASME, 59(2), 88. Wilkinson, D.S. and Ashby, M.F. (1975). ‘Pressure sintering by power law creep’. Acta Metallurgica, 23, 1277.

This page intentionally left blank

9. Creep in an aero-engine combustor material

9.1

Introduction

Aero-engine components operating under in-service conditions are often subjected to a range of complex cyclic mechanical and thermal loading, leading to combined creep and cyclic plasticity. The polycrystalline nickel-base superalloy (C263) is a commercial alloy used for stationary components in aero-engines such as combustion chambers, casings, liners, exhaust ducting, and bearing housings. It is a ﬁne-precipitate strengthened alloy at 800◦ C, with a precipitate solvus temperature of 925◦ C (Betteridge and Heslop, 1974). Combustion chamber applications require the material to undergo temperature ﬂuctuations between 20◦ C and 950◦ C, and the temperature range is therefore such that the precipitate solvus can be exceeded during in-service operation. Signiﬁcant microstructural change is therefore likely to occur during ordinary operation, leading to quite profound changes in the creep mechanisms in the material, controlling both deformation and component life. In this chapter, we shall introduce a physically based creep model which explicitly accounts for microstructural change, and its inﬂuence on creep deformation and failure, in polycrystalline nickel-base alloy C263 for temperatures both above and below the γ solvus. The implementation into ABAQUS is carried out using a forward Euler integration scheme and we again use the initial stiffness as the material Jacobian for simplicity.

9.2

Physically based constitutive equations

Creep in nickel alloy C263 occurs through diffusion-activated dislocation climb and precipitate ‘cutting’, depending on the precipitate spacing, λp (or equivalently, size, rs , for a given precipitate volume fraction, φp , which in turn depends on temperature, T ). Above a critical particle spacing, λpc , dislocation climb dominates, whereas below the critical spacing, precipitate ‘cutting’ dominates. The material also undergoes coarsening at temperature such that the particle spacing increases with time.

210

Creep in aero-engine components

All of these microstructural processes are embodied within creep constitutive equations. The creep strain rate, p˙ c , also depends upon the density, ρn , of mobile dislocations which in turn depends on the accumulated creep strain. The constitutive equation set embodying all the mechanisms discussed above is given below. The activation volume, V , depends on the active obstruction mechanism. In the case of dislocation pinning by precipitates, V is dependent on the pinning distance, which in turn depends on the precipitate spacing. For precipitate cutting, the activation volume is Vc . In the creep strain rate equation, the uniaxial strain rate, ε˙ c , in response to a uniaxial stress, σ , is determined from the corresponding shear values ¯ , in which M¯ using the usual relationships (Dieter, 1988): ε˙ = γ˙ /M¯ and σ = Mτ is the Taylor factor. F is the Helmholtz free energy, b the Burger’s vector, ν the frequency of dislocation jumping energy barriers, kb the Boltzman constant, and ρi the initial density of mobile dislocations. ρn ρi ([4π/3φp ]1/3 − 2) 2 σe V −F p˙ c = b , (9.1) sinh ν exp ¯ − ω) kb T [4π/3φp ]1/3 M¯ kb T M(1 where V = Vc , if φp > 0 and λp < λpc V = λp b2 , if φp > 0, λp > λpc and λp < λd V = λd b2 , if φp = 0 and

λp = rs

4π 3φp

1/3

(cutting), (climbing), (dislocation network)

−2 ,

ρ˙n = ψ ε˙ c . In Equation (9.1), ω is a scalar damage variable which has evolution equation χ σ1 ω˙ = H (σ1 )p˙ c (9.2) σe in which σ1 is the maximum principal stress, H the Heaviside function, and and χ are material constants (χ being the sensitivity of stress state parameter). The equations contain just two unknown ﬁtting constants, namely ψ and associated with the multiplication of mobile dislocations and cavitation, occurring largely within the tertiary creep regime. All the other material constants are physical properties or measurable physical quantities. Creep tests have been carried out by Rolls-Royce over the temperature range 700–750◦ C, and by Zhang and Knowles (2001) on C263 over the temperature range 800–950◦ C. Prior to creep testing, the material had been subjected to the standard

Physically based constitutive equations

(a)

(b)

2.0

10

450 MPa

380 MPa

350 MPa 8

1.5

200 MPa

1.0

Strain (%)

Strain (%)

250 MPa 320 MPa

0.5

270 MPa

0.0 0.0

6

4

2

0 1.0

2.0

3.0 4.0 Time (s)

5.0

0

6.0 [× 106]

(c)

2

4

6 Time (s)

8

10 [× 106]

(d)

4.5

30 40 MPa

4.0 25

200 MPa

3.5

160 MPa

20 Strain (%)

3.0 Strain (%)

211

250 MPa

2.5 2.0 1.5

15 10 50 MPa

1.0 5 0.5 0.0 0

1

2 Time (s)

3 [× 106]

Experimental results

0 0.0

0.1

0.2

0.3 0.4 Time (s)

0.5

0.6 [× 106]

Computed results

Fig. 9.1 Comparison of experimental and computed isothermal creep results at (a) 700◦ C, (b) 750◦ C,

(c) 800◦ C, and (d) 950◦ C.

heat treatment. This involves solutioning at 1150◦ C for 2 h, quenching and ageing at 800◦ C for 8 h followed by air cooling. The results of the tests are shown in Fig. 9.1 by the broken lines. The constants and constant groups appearing in the equations have been determined by standard optimization techniques. The volume fraction of γ precipitate is known at each test temperature, Burger’s vector for this material is taken as 2.5 × 10−10 m (Frost and Ashby, 1982), and the initial density of dislocations can be estimated to

212

Creep in aero-engine components Table 9.1 Physical constants determined from creep data by optimization. F (J/atom)

λpc (nm)

Vc (m3 )

ν (s−1 )

M¯

7.4 × 10−19

64.9

4.05 × 10−27

15.1 × 1021

3.57

be 1010 m−2 (Hull, 1975). The remaining temperature-independent physical properties can then be determined using the results of the optimization and the model equations. The results of this process are shown in Table 9.1, which includes the Helmholtz free energy, F , the critical particle spacing, λpc , above which dislocation bowing dominates over particle cutting, the activation volume for cutting, Vc , the frequency of dislocations jumping energy barriers, ν, and the Taylor factor. The temperature dependence of the two empirical constants for the evolution of multiplication of mobile dislocation density and cavitation is shown in Appendix 9.1. The computed creep curves resulting from the determination of the creep parameters are also shown in Fig. 9.1.

9.3

Multiaxial implementation into ABAQUS

We assume multiaxial creep deformation in nickel alloy C263 to obey von Mises behaviour; that is, the relationship between uniaxial creep strain rate and stress is identical to that between the effective creep strain rate and effective stress. Under multiaxial conditions, the creep strain rate ‘direction’ is taken to be normal to the dissipative surface, in an analogous way to that in plasticity, giving the multiaxial creep strain rate as 3 σ

ε˙ c = p˙ c 2 σe

in which σ is the deviatoric stress tensor, and σe the effective stress, given by 1/2 3

σe = σ :σ 2 and the effective creep strain rate, p˙ c , is given in Equation (9.1). The equations have been implemented into an ABAQUS UMAT using a simple forward Euler explicit integration scheme with the initial stiffness method; that is, the material Jacobian is speciﬁed simply as the elasticity matrix. 9.3.1

Finite element modelling of biaxial creep tests

A range of tests have been carried out on nickel alloy C263 in order to investigate its stress state sensitivity of creep failure. The tests have been carried out on thin-walled

Multiaxial implementation into ABAQUS

213

Table 9.2 Summary of tests and loading conditions, and corresponding stress state. Shear stress (MPa) Tension Tension–torsion Torsion Compression–torsion

0 160 184 160

Axial stress (MPa) 320 160 0 −160

σ1 /σe 1.0 0.81 0.58 0.31

tubular specimens which have been subjected to uniaxial tension, tension–torsion, torsion, and compression–torsion. The material was subjected to the standard heat treatment such that its uniaxial creep behaviour, through to failure, is correctly modelled using the above constitutive equations with the material properties given in Manonukul et al. (2002). The test specimen gauge section has length 16 mm, with internal and external radii of 3.12 and 4.12 mm, respectively. The tests were carried out at 800◦ C such that the von Mises effective stress for each test was the same, namely 320 MPa. The loading conditions applied are summarized in Table 9.2. The loads were increased linearly from zero to the maximum (to give the desired stresses) over 14 s, and were then held at the maximum value. The experimental test results are shown in Fig. 9.2(a). The quality of the creep data obtained for the torsion test is, unfortunately, not as good as desired because of problems with temperature control. However, the results do demonstrate the strong dependence of creep life on stress state. The stress state, given by σ1 /σe , for each test, is shown in Table 9.2. The test specimens were modelled by developing three-dimensional meshes of the gauge sections (i.e. uniform-section tubes). Because of the need to carry out compression tests, the wall thickness was constrained by buckling problems. As a result, the specimen wall thickness was such that an assumption of uniform shear strain and stress through the wall thickness would not have been appropriate. A two-dimensional ﬁnite element model was therefore necessitated. However, because of the ease of speciﬁcation of torsional loading conditions using three-dimensional elements (as opposed to axisymmetric elements with ‘twist’ in ABAQUS), 240 eight-noded, three-dimensional solid elements were used so that the specimen thickness contained two elements. Geometrical non-linearity was accounted for using the standard ABAQUS large strain formulation. Under torsional loading, because of the radial variation of stress, the loads applied were chosen to ensure that the average effective stress through the thickness was that desired, that is, 320 MPa. The creep behaviour of the material was described by the constitutive equations given above. The only unknown parameter in the equations is the stress state sensitivity, χ. The four tests described above were simulated using the ﬁnite element model. Parametric studies were carried out in order

214

Creep in aero-engine components

(a)

0.3 Tension–torsion

Torsion

Equivalent creep strain

0.25 Compression–torsion

0.2 0.15

Tension

0.1 0.05 0 0

100000

200000

300000

400000

500000

600000

700000

800000

Time (s) (b)

0.3

Equivalent creep strain

0.25

Compression–torsion

0.2 Torsion 0.15 Tension–torsion

0.1

Compression

0.05

Tension

0 0

100000

200000

300000

400000

500000

600000

700000

800000

Time (s)

Fig. 9.2 (a) Experimental and (b) computed equivalent creep strain versus time for isothermal creep tests carried out at 800◦ C with effective stress 320 MPa for the loading conditions shown.

to determine χ. This was done by choosing that value of χ which provided computed results closest to those seen in the experiments. The computed results obtained using a value for χ of 0.38 are shown in Fig. 9.2(b). This value lies within the range for nickel alloys discussed by Dyson and Loveday (1981). Considerably different creep lives are seen to occur depending on the stress state, and this is captured well by the model. The computed creep curve for uniaxial compression shown in Fig. 9.2(b) can be seen to have a slowly increasing gradient, even though there is no creep cavitation

Multiaxial implementation into ABAQUS

215

Displacement of the top boundary (mm)

2 1.8

Indicates predicted failure on the basis of a damage level of 0.3 through the specimen section

1.6 194 MPa

1.4 1.2 1

161 MPa

0.8

104 MPa

0.6 0.4 0.2 0 0

500

1000

1500

2000

2500

Time (h)

Fig. 9.3 Predicted displacement of the top boundary versus time (solid lines) for the double notch specimen subjected to the stresses shown. Broken straight lines indicate experimentally determined times to failure.

occurring. This results from both the precipitate coarsening and the multiplication of mobile dislocations, both of which are included in the model.

9.3.2

Prediction of notched bar creep behaviour

Three experimental tests have been carried out on double notched bar test specimens. The specimens have gauge length 25.4 mm and diameter 5.62 mm. The circular notches have diameter 1.12 mm and they are separated by 7 mm along the length of the specimen. The effect of the notches is to introduce multiaxial stress states local to the notches, which inﬂuence creep damage evolution, as discussed above. Uniaxial loading was applied to generate nominal section stresses of 104, 161, and 194 MPa, respectively. The test specimens were modelled using axisymmetric elements. Because of symmetry, just one quarter of the specimen section was modelled explicitly. The specimen lifetimes have been predicted and the lives compared with those obtained in the experiments. The predicted displacements of the top boundary of the test specimen are shown for the three applied, nominal stresses of 104, 161, and 194 MPa in Fig. 9.3. The creep damage evolution for the case of the 161 MPa nominal stress is shown in Fig. 9.4(a). At this stress level, creep damage is predicted to initiate at the notch root after creeping for about 13 h. By the time creep has continued for 166 h, the damage has evolved right across the test specimen, in which the damage level is 0.26 or higher. This is

216

Creep in aero-engine components

Cavitation damage parameter

(a)

+0.00E+00 +2.00E–02 +4.36E–02 +6.73E–02 +9.09E–02 +1.15E–01 +1.38E–01 +1.62E–01 +1.85E–01 +2.09E–01 +2.33E–01 +2.56E–01 +2.80E–01 +3.00E–01 (b)

(c)

2

7

2

0

2

6

8

2

5

0

0

Number of creep voids

3

7

12

7

2

4

4

4

15

6

3

0

2

9

9

5

2

0

0 1–3 4–6 7–9 10–12 13

1

3

4

22

8

2

5

1

17

30

2

1

Fig. 9.4 Creep damage ﬁelds (a) predicted by the model, (b) observed in the microstructure, and (c) from a surface void count using the micrograph. (See also Plate 4.)

References

217

Table 9.3 Predicted and experimentally determined top boundary displacement at failure (deﬁned as experimental specimen separation). Stress (MPa) 104 161

Predicted displacement at failure (mm)

Experimental displacement at failure (mm)

1.9 0.1

1.97 0.11

shown in Fig. 9.4(a), together with a micrograph of the corresponding region of the test specimen in Fig. 9.4(b). Microcracking can be seen to initiate at the notch root at an angle of about 22◦ from the horizontal. A surface void count has been carried out and the results are shown in Fig. 9.4(c). The damage ﬁelds in Fig. 9.4(a) can be seen to predict reasonably well both the site of major cracking and the distribution of experimentally observed creep cavitation. Dyson and McLean (1990) have argued that creep rupture occurs typically when the creep cavity damage achieves a value of about 0.3. This results from the coalescence of creep cavitation and the propagation of macroscopic creep cracking. The experimentally determined failure times are shown in Fig. 9.3 by the dashed lines. The measured and calculated displacements of the top boundary at failure, which show good agreement, are shown in Table 9.3. The predicted displacement at failure was determined as the predicted displacement when a damage level of about 0.3 had been achieved through the specimen section. However, the analyses were not stopped once a creep damage level of 0.3 had been achieved across the specimen section, and hence Fig. 9.3 shows the calculated top boundary displacement continuing to increase as the damage level exceeds 0.3. A further reason for continuing the analysis is the difﬁculty of deﬁning creep failure in the calculations. In the experiments, this is easier; it is simply the measured time until the specimen breaks. An alternative way to deﬁne calculated specimen rupture time is simply to examine the top boundary displacement rate, and to assume that rupture occurs once the rate becomes large. On this basis, the comparison of predicted and experimental time to rupture results shown in Fig. 9.3 is reasonable.

References Betteridge, W. and Heslop, J. (1974). The Nimonic Alloys. Edward Arnold, London, UK. Dyson, B.F. and Loveday, M.S. (1981). In Ponter, A.R.S. and Hayhurst, D.R. (eds), Proceedings of the Creep in Structures IUTAM Symposium, Springer, Berlin, 406–421.

218

Creep in aero-engine components

Dyson, B.F. and McLean, M. (1990). ‘Creep deformation of engineering alloys— development from physical modelling’. Iron and Steel Institute of Japan International (ISIJ), 30, 802–811. Dieter, G.E. (1988). Mechanical Metallurgy. McGraw-Hill Book Co., London, UK. Frost, H.J. and Ashby, M.F. (1982). Deformation-Mechanism Maps: The Plasticity and Creep of Metals and Ceramics. Pergamon Press, Oxford, UK. Hull, D. (1975). Introduction to Dislocations, 2nd edition. Pergamon Press, Oxford, UK. Manonukul, A., Dunne, F.P.E., and Knowles, D. (2002). ‘Physically-based model for creep in nickel-base superalloy C263 both above and below the γ solvus’. Acta Materialia, 50(11), 2917–2931. Zhang, Y.-H. and Knowles, D. (2001). ‘Deformation behaviour and development of microstructure during creep of a nickel-base superalloy’. In Parker, J.D. (ed.), Proceedings of the 9th International Conference on Creep and Fracture of Engineering Materials and Stuctures, April 2001, Gomer Press, UK.

Appendix 9.1 The dependence of precipitate volume fraction, φ, on temperature, T , in C263 φ = −4.537 × 10−9 T 3 + 1.261 × 10−5 T 2 − 1.187 × 10−2 T + 3.915. The dependence of constants and on temperature.

ψ

700◦ C

750◦ C

800◦ C

950◦ C

496.1 1.58×10−2

435.2 3.01×10−2

10.0 18.62

1.1×10−19 19.84

10. Cyclic plasticity, creep, and TMF

10.1

Introduction

In Chapter 9, we examined creep in the aero-engine combustor material nickel-base superalloy C263. In this chapter, we address combined anisothermal cyclic plasticity and creep. We use time-independent cyclic plasticity with both isotropic and kinematic hardening which we combine with the physically based creep model described in Chapter 9. The plasticity model is implemented into ABAQUS Implicit by means of a UMAT subroutine which employs a simple ﬁrst-order forward (explicit) integration scheme and the initial stiffness method. We then address isothermal cyclic plasticity and creep, followed by an examination of thermo-mechanical fatigue in nickel alloy C263.

10.2

Constitutive equations for cyclic plasticity

C263 is largely rate-independent and shows very limited creep response at temperatures below ∼600◦ C. During zero-mean, strain-controlled reversed plasticity below this temperature, the material exhibits both kinematic hardening within individual cycles, and isotropic strain softening/hardening over many cycles, depending on the temperature. The resulting stress–strain hysteresis loops show considerable change as plastic strain accumulates. Above ∼600◦ C, under similar loading, the material starts to exhibit strain-rate dependence. Viscoplastic constitutive equations for a polycrystalline nickel-base alloy have been presented by Yaguchi et al. (2002a,b), who considered uniaxial creep, isothermal, and anisothermal cyclic plasticity between 450◦ C and 950◦ C. Because of the wide temperature range considered here (20–950◦ C), a uniﬁed viscoplasticity-creep model is not adopted because of the numerical problems that can arise when using such a model for time-independent plasticity. In any case, it would, in addition, prevent the retention of the physical basis of the creep model to be used here, presented by Manonukul et al. (2002). A non-uniﬁed approach has therefore been adopted in which conventional time-independent reversed plasticity

220

Cyclic plasticity, creep, and TMF

theory for low-temperature deformation has been combined with the physically based creep model for elevated temperature deformation. The further justiﬁcation for the separation of creep and time-independent plasticity terms is that at 20◦ C, for example, (thermally activated) creep simply does not occur. Deformation takes place by plastic slip which is not aided by thermally activated dislocation climb. Conversely, at 950◦ C, deformation is dominated by diffusion-controlled processes, and plastic slip, aided by thermal activation or otherwise, is negligible. At about 800◦ C, both sets of mechanisms operate, and a uniﬁed viscoplasticity theory would be appropriate. However, for the main application considered here—thermo-mechanical fatigue with considerable temperature variations, 20–950◦ C, our approach can be justiﬁed. It is therefore assumed that the elastic, dε e , time-independent plastic, dεp , creep, dεc , and thermal, dεθ , strain increments may be additively decomposed such that the total strain, dε, is given by dε = dεe + dε p + dε c + dε θ .

(10.1)

There have been many developments in the modelling of kinematic hardening that take account, for example, of non-proportional loadings (Voyiadjis and Abu Al-Rub, 2003). However, for simplicity here, the Chaboche combined isotropic and kinematic hardening model (Lemaitre and Chaboche, 1990) is employed for time-independent plasticity. The increment in non-linear kinematic hardening dx and the increment in isotropic hardening dr are given, respectively, by dx =

2 c dεp − γ x dp 3

(10.2)

and dr = b(Q − r) dp, where

dp =

2 p dε : dεp 3

(10.3)

1/2 .

(10.4)

Here, x is the kinematic hardening stress tensor, r the isotropic hardening stress, and b and Q are temperature dependent material parameters associated with isotropic hardening. Temperature and accumulated plastic strain dependent material parameters associated with kinematic hardening are c and γ , respectively. A large number of fully reversed cyclic plasticity tests have been carried out in order to determine the temperature-dependent material parameters arising in the kinematic hardening equations. dp is the effective time-independent plastic strain increment. The increment in plastic strain is determined in the conventional way assuming a von

Constitutive equations for cyclic plasticity

221

Mises yield function, f , given by 1/2 3

f = − r − σy = 0 (σ − x ) : (σ − x ) 2 so that

∂f 3 σ − x

(10.5) = dλ 2 σe ∂σ in which dλ is the plastic multiplier which, for combined isotropic and kinematic hardening, is given, using Voigt notation, by dεp = dλ

dλ =

(∂f /∂σ) · C dε (∂f /∂σ) · {(2/3)c(∂f /∂σ) − γ x} + b(Q − R) + (∂f /∂σ) · C(∂f /∂σ)

=

( 23 )(σ /σe ) · C dε

( 23 )(σ /σe )·{( 23 )c( 23 )(σ /σe ) − γ x} + b(Q − R) + ( 23 )(σ /σe )· C( 23 )(σ /σe )

.

(10.6) The effective stress is, of course, given by 1/2 3

σe = . (σ − x ) : (σ − x ) 2 The increment in thermal strain is calculated in the usual way as dε θ = α dθI

(10.7)

in which α is the coefﬁcient of thermal expansivity, dθ the increment in temperature, and I the identity matrix. The multiaxial constitutive equations presented above for creep and plasticity have been implemented into a UMAT user subroutine using the simple ﬁrst-order explicit Euler forward integration scheme as follows 3 σ

c θ dσt = C dεt − dλ − dε − dε 2 σe in which the increment in creep strain is obtained from Equation (9.33) and those in Table 9.1, and σt+t = σt + dσt , x t+t = x t + dx t , p

p

p

εt+t = εt + dεt , rt+t = rt + drt .

222

10.3

Cyclic plasticity, creep, and TMF

Constitutive equations for C263 undergoing TMF

The thermo-mechanical loading cycles to which the nickel-base superalloy C263 is subjected in-service are such that the γ solvus is exceeded so that the material is, in effect, solution treated. This has a profound effect on the behaviour of the material; under conditions of both creep and reversed plasticity. The rate-controlling mechanisms for creep deformation change from precipitate cutting and dislocation pinning at precipitates, and climb, to that of the pinning of dislocations through the establishment of a dislocation network. The physically based creep model employed here is able to capture these changes and to represent the micro- and macro-scale creep deformation. For a given temperature, the precipitate volume fraction is known, and because the precipitate coarsening kinetics has been quantiﬁed, both size and hence spacing of the precipitate is known. These quantities appear explicitly in the physically based creep model. The effect of solution treating on cyclic plastic response is also very signiﬁcant and has been addressed. Cyclic plasticity tests between 20◦ C and 950◦ C have been carried out. With the combined creep–cyclic plasticity model described above, the temperature dependence of the isotropic and kinematic hardening constants have been determined (Manonukul et al., 2001). The effect of precipitate volume fraction on cyclic plasticity behaviour is introduced into the model, therefore, through the temperature dependence of the material parameters for cyclic plasticity. At temperatures of about 800◦ C and above, C263 creeps quite signiﬁcantly. This appears in the cyclic plasticity response as a reduction in the overall stress level, occurring through relaxation. LCF tests have been carried out on C263 at 800◦ C and 950◦ C under fully reversed (R = −1), strain-controlled loading through to failure. The experimentally determined and calculated stress–strain hysteresis loops for the ﬁrst and second cycles of the standard heat treated material are shown in Fig. 10.1. At 800◦ C, two strain rates have been used such that ramping times (the time over which the strain is applied linearly with time) of 1 and 10 s have been imposed resulting in the hysteresis loops shown in Fig. 10.1(a) and (b), respectively. Figure 10.1(c) shows the results for 950◦ C. In these cycles, a 1-s strain hold has been imposed at the tensile and compressive peak strains. At 800◦ C, this does not result in a distinctive stress relaxation, but this can be seen at 950◦ C in the computed result. However, the experiments show a much more progressive stress relaxation at the peak strains suggesting that the rate of relaxation is not well represented by the creep model. This occurs for a number of reasons. First, the creep model at 950◦ C was developed from experimental data obtained for a much lower stress level (a maximum of 50 MPa) whereas here, stresses of over 200 MPa are developed in the hysteresis loop. In addition, our cyclic plasticity model does not contain an explicit static recovery term,

Constitutive equations for C263 undergoing TMF

223

600

(a)

400 200 0 – 0.6

– 0.4

– 0.2

0

0.2

0.4

0.6

0

0.2

0.4

0.6

0

0.2

0.4

0.6

– 200 – 400 – 600 600

(b)

400 200 0 – 0.6

– 0.4

– 0.2 – 200 – 400 – 600 300

(c)

100

– 0.6

– 0.4

– 0.2

– 100

– 300 Experimental

Computed

Fig. 10.1 Experimental and computed LCF stress–strain curves for the ﬁrst and second cycles at (a) 800◦ C, 1 s ramping time, strain range 0.9%, (b) 800◦ C, 10 s ramping time, strain range 1%, and (c) 950◦ C, strain range 0.75%.

and further, the creep and plastic strain increments have, of course, been decoupled in the present work. Note that the microstructure of the material being loaded at 950◦ C is considerably different to that at 800◦ C because of the dissolution of the precipitate at the higher temperature. However, for both temperatures considered here, the peak stress levels are reasonably well predicted.

224

Cyclic plasticity, creep, and TMF

600

400 (b) (a)

200 (c) 0 0

200

400

600

800

1000

1200

1400

(c) – 200 (b)

(a)

– 400

– 600 Experimental

Computed

Fig. 10.2 Experimental and computed LCF peak stresses versus cycles at (a) 800◦ C, 1 s ramping time,

strain range 0.9%, (b) 800◦ C, 10 s ramping time, strain range 1%, and (c) 950◦ C, strain range 0.75%.

Figure 10.2 shows the comparisons of computed and experimental peak stresses versus cycles for each of the cases (a), (b), and (c) in Fig. 10.1, through to failure. Good predictions of life can be seen to be achieved for (b) and (c) for which intergranular creep cavitation dominates. Intergranular creep damage typically observed under these conditions is shown in Fig. 10.2. The life is overpredicted for (a) since creep damage accumulation has ceased to be the dominant failure process. A micrograph for these conditions shows that transgranular fracture is now occurring. Microstructural examination of specimens tested at 800◦ C and 950◦ C has been carried out after specimen failure. LCF tests carried out at 800◦ C, with 1-s ramp times, led to sample fracture surfaces showing transgranular cracking, as shown in Fig. 10.2, indicating that lifetime under these conditions is dominated by fatigue

Constitutive equations for C263 undergoing TMF

225

processes. However, microstructural examination of specimens also tested at 800◦ C but with a considerably longer ramp time of 10 s showed the development of intergranular damage, which dominated in some regions of the material. The lifetime of the material under these conditions may well be inﬂuenced quite strongly by creep damage processes. Examination of microstructures of specimens tested at 950◦ C showed that intergranular cracking dominated at these temperatures, even for a ramp time of 1 s. The dominant failure process for these conditions is intergranular creep fracture. The results of the tests carried out at 800◦ C shown in Fig. 10.2(a) and (b) show the development of macrocracking towards the end of the test which inﬂuences the observed stress–strain response which becomes different in tension and compression because of crack closure effects. The isotropic creep damage model used in the present work is not capable of predicting crack closure effects. The result at 950◦ C, however, which is dominated by creep softening and cavitation, does not show this effect. 10.3.1

TMF in C263 both above and below the γ solvus

TMF tests have been carried out on C263 under conditions of both in and out of phase loading. Strain controlled tests have been carried out between strains of zero and a peak of 0.6%, in which the temperature is also varied between 300◦ C and 950◦ C. The strain and temperature loading imposed, together with the results obtained, are shown in Fig. 10.3. First, considering the in-phase loading shown in Fig. 10.3(a), the experimental results obtained for the initial loading, below the γ solvus temperature, give stress levels that lie a little below that expected from both the solution treated and the standard treated material. After a time of 45 s, the temperature has exceeded 925◦ C, and in fact, the experimental results give stress levels that would be anticipated for such a material. It should be noted that prior to the imposition of the strain, the test specimen has undergone a prior temperature loading cycle. This is necessary to enable temperature compensation to be carried out on the TMF test rig. The consequence is that the material is, therefore, in effect in the solution treated state. The modelling of the behaviour has therefore been carried out with this assumption. For the cyclic plasticity modelling, two sets of material parameters were determined; one for the solution treated material (with the appropriate temperature dependence), and a further one for the standard treated material (i.e. for the material containing the precipitate volume fraction, which is dependent on temperature). The model for the solution treated plasticity and creep behaviour give the computed behaviour also shown in Fig. 10.3(a). As the temperature increases, a number of processes are taking place. The volume fraction of precipitate is decreasing, and at 925◦ C, becomes zero. The creep rate becomes determined by dislocation network

(a)

Strain (%)

Cyclic plasticity, creep, and TMF

300

0

0.1

0.3

0.5

0.7

– 300

(b)

Strain (%)

Strain (%)

300 200

Stress (MPa)

Temperature (8C)

0 – 0.1 – 100 – 200

100 – 0.7

– 0.5

0 – 0.1 – 100

– 0.3

0.1

– 200 – 300 Strain (%)

(c)

Strain (%)

800 600 400

Stress (MPa)

0.6 0.4 0.2 0 50 100 Time (s)

100

200 – 0.2

0 – 200 0

Temperature (8C)

Stress (MPa)

200

0.2

0.4

– 400 – 600 – 800 Strain (%) Experimental

Predicted

0.6

Temperature (8C)

226

1000 500 0

0

50 100 Time (s) Time (s) 50 100

0 0 – 0.2 – 0.4 – 0.6 1000 500 0 0

0

50 100 Time (s) Time (s) 50 100

0.4 – 0.1

1000 500 0 0

50 100 Time (s)

Fig. 10.3 Experimental and predicted stress–strain curves for (a) in-phase TMF at temperature range 300–950◦ C and (b) out-of-phase TMF at temperature range 300–950◦ C, and (c) in-phase TMF at temperature range 300–800◦ C .

pinning (Manonukul et al., 2002) and increases as the temperature increases. The combined effects of these processes result in the predicted decreasing stress level. At a time of 45 s, both the strain and temperature loading are reversed, and a comparatively small elastic region (though creep deformation is still occurring) can be seen, which

References

227

is followed by a conventional plasticity region in which creep deformation becomes negligibly small as the temperature decreases towards 300◦ C. Note that the material continues to harden during this phase, with no stress relaxation occurring at the higher compressive stresses because of the elimination of creep. The stress levels measured and predicted by the model are those that would be anticipated from the solution treated material. The standard heat treated material would show considerably higher stresses. With the reversal of the loading again, a rather larger elastic region is observed because of the increased yield stress at lower temperature, and because of the existing hardening that has already taken place. The measured and predicted stresses developed with increasing plastic deformation show good agreement and, unlike the ﬁrst quarter-cycle, are those that would be expected for the solution treated material. The loading conditions and results obtained for out-of-phase TMF are shown in Fig. 10.3(b). In this case, the high tensile stresses occur during the low temperature parts of the loading cycle, and conventional plastic behaviour is observed. At the higher temperatures, the material is in compression, but again, stress relaxation can be seen to occur, and the features of the experimentally obtained results can be seen to be reasonably reproduced. For in-phase TMF with the same strain range, but with the temperature varying between 300◦ C and 800◦ C, the experimental and predicted results obtained are shown in Fig. 10.3(c). Good comparisons are achieved for these conditions.

References Lemaitre, J. and Chaboche, J.-L. (1990). Mechanics of Solid Materials. Cambridge University Press, Cambridge. Manonukul, A., Dunne, F.P.E., and Knowles, D. (2001). ‘Thermo-mechanical fatigue in nickel-base superalloy C263’. Internal Report, Department of Engineering Science, Oxford University, England. Manonukul, A., Dunne, F.P.E., and Knowles, D. (2002). ‘Physically-based model for creep in nickel-base superalloy C263 both above and below the γ solvus’. Acta Materialia, 50, 2917–2931. Voyiadjis, G.Z. and Abu Al-Rub R.K. (2003). ‘Thermodynamic based model for the evolution equation of the backstress in cyclic plasticity’. International Journal of Plasticity, 19(12), 2121–2147. Yaguchi, M., Yamamoto, M., and Ogata, T. (2002a). ‘A viscoplastic constitutive model for nickel-base superalloy Part I: kinematic hardening rule of anisotropic dynamic recovery’. International Journal of Plasticity, 18(8), 1083–1109. Yaguchi, M., Yamamoto, M., and Ogata, T. (2002b). ‘A viscoplastic constitutive model for nickel-base superalloy Part II: modelling under anisothermal conditions’. International Journal of Plasticity, 18(8), 1111–1131.

This page intentionally left blank

Appendix A: Elements of tensor algebra

The dot (scalar) product of two ﬁrst-order tensors (vectors) gives a scalar

n NB. Einstein summation convention: ui vi = ui vi i=1

u · v = ui vi = v · u = vi ui =

n i=1 n

ui vi ,

(A1)

vi ui ,

(A2)

i=1

v · u = u · v.

(A3)

Double contraction (double dot product) of two second-order tensors gives a scalar σ : ε = σij εij =

n n

σij εij ,

(A4)

εij σij ,

(A5)

i=1 j =1

ε : σ = εij σij =

n n i=1 j =1

ε : σ = σ : ε.

(A6)

The dot product of a ﬁrst-order tensor with a second-order tensor gives a ﬁrst-order tensor n σij nj , (A7) σ · n ⇒ (σij nj )i = j =1

n · σ ⇒ (nj σji )i =

n j =1

nj σji ,

(A8)

230

Appendix A: Elements of tensor algebra

hence the expression n·σ =σ ·n

(A9)

is valid only if σ is symmetric (i.e. if σij = σji for any i, j ). The dyadic (direct) product of two ﬁrst-order tensors gives a second-order tensor u ⊗ v ⇒ (u ⊗ v)ij = ui vj . For example, if

⎡ ⎤ u1 ⎣ u = u2 ⎦ u3

then

⎡ ⎤ v1 ⎣ v = v2 ⎦ , v3

and

⎛

u1 v1 u ⊗ v = ⎝u2 v1 u3 v1

(A10)

⎞ u1 v3 u 2 v3 ⎠ . u3 v3

u1 v2 u2 v2 u3 v2

The product of two second-order tensors gives a second-order tensor a · b ⇒ (a · b)ij = aik bkj =

n

aik bkj .

(A11)

k=1

Double contraction (double dot product) of a third-order tensor with a second-order tensor gives a ﬁrst-order tensor ξ :σ =

3

ξijk σjk ei .

(A12)

i,j,k=1

Double contraction (double dot product) of a fourth-order tensor with a second-order tensor gives a second-order tensor c : ε ⇒ (c : ε)ij = cijkl εkl =

n n

cijkl εkl

(A13)

k=1 l=1

hence the expression c:ε=ε:c

(A14)

is valid only if c exhibits major symmetry (i.e. if cijkl = cklij for any i,j ,k,l). The dyadic (direct) product of two second-order tensors gives a fourth-order tensor f ⊗ g ⇒ (f ⊗ g)ijkl = fij gkl . Kronecker delta—a special second-order tensor / δij = 1, if i = j, δ ⇒ δij δij = 0, if i = j.

(A15)

(A16)

Appendix A: Elements of tensor algebra

231

The unit fourth-order tensor (exhibits major but not minor symmetry) I ⇒ Iijkl = δik δjl

(A17)

has the following important property I : ε = ε : I,

(A18)

which is valid for any second-order tensor ε. A symmetrized unit fourth-order tensor (exhibits both major and minor symmetry) s I s ⇒ Iijkl =

1 (δik δjl + δil δjk ) 2

(A19)

ensures the following identity I s : ε = ε : I s,

(A20)

which is valid only if the second-order tensor ε is symmetric.

Differentiation Differentiation of a tensor valued function (e.g. u, σ ) with respect to its tensorial argument (e.g. x, ε). Example: Differentiation of the ﬁrst-order tensor u with respect to the ﬁrst-order tensor x gives the second-order tensor ∂u ∂u ∂ui ⇒ = . (A21) ∂x ∂x ij ∂xj Special case: ∂u ⇒ ∂u

∂u ∂u

=δ= ij

∂ui = δij . ∂xj

(A22)

Example: Differentiation of the second-order tensor σ with respect to the secondorder tensor ε gives the fourth-order tensor ∂σij ∂σ ∂σ ⇒ = . (A23) ∂εkl ∂ε ∂ε ijkl Special case: ∂σ ⇒ ∂σ

∂σ ∂σ

=I= ijkl

∂σij = Iijkl . ∂σkl

(A24)

232

Appendix A: Elements of tensor algebra

The chain rule Example: Second-order tensor f depends on a second-order tensor u and a scalar v ∂fij ∂fij ∂umn ∂fij ∂v ∂f ∂u ∂f ∂v ∂f ∂f = : + ⊗ ⇒ = = + . ∂x ∂u ∂x ∂v ∂x ∂x ijkl ∂xkl ∂umn ∂xkl ∂v ∂xkl (A25) The gradient of a scalar ﬁeld gives a ﬁrst-order tensor ∇f ⇒

∂f . ∂xi

(A26)

The gradient of a ﬁrst-order tensor ﬁeld gives a second-order tensor ∇v ⇒

∂vj . ∂xi

(A27)

The gradient of a second-order tensor ﬁeld gives a ﬁrst-order tensor with its components being second-order tensors ∇σ ⇒ (∇σ )j = Hence,

⎡⎡ ∂σ

xx

⎢⎢ ∂x ⎢⎢ ⎢⎢ ∂σxx ⎢⎢ ⎢⎢ ∂y ⎢⎢ ⎢⎣ ∂σxx ⎢ ⎢ ⎢ ∂z ⎢ ⎢⎡ ∂σ yx ⎢ ⎢⎢ ⎢⎢ ∂x ⎢⎢ ⎢⎢ ∂σyx ∇σ = ⎢ ⎢⎢ ∂y ⎢⎢ ⎢⎢ ∂σyx ⎢⎣ ⎢ ∂z ⎢ ⎢ ⎢⎡ ⎢ ∂σzx ⎢ ⎢ ⎢ ∂x ⎢⎢ ⎢ ⎢ ∂σzx ⎢⎢ ⎢ ⎢ ∂y ⎢⎢ ⎣ ⎣ ∂σ zx ∂z

∂σij ∂σji = . ∂xi ∂xi

∂σxy ∂x ∂σxy ∂y ∂σxy ∂z ∂σyy ∂x ∂σyy ∂y ∂σyy ∂z ∂σzy ∂x ∂σzy ∂y ∂σzy ∂z

⎤ ∂σxz ⎤ ⎥ ∂x ⎥ ⎥⎥ ⎥ ∂σxz ⎥ ⎥⎥ ⎥ ∂y ⎥⎥ ⎥ ∂σxz ⎦⎥ ⎥ ⎥ ∂z ⎥ ⎥ ⎤ ∂σyz ⎥ ⎥ ⎥ ∂x ⎥ ⎥⎥ ⎥ ∂σyz ⎥ ⎥⎥ ⎥. ∂y ⎥ ⎥⎥ ⎥ ⎥ ∂σyz ⎥ ⎦⎥ ∂z ⎥ ⎥ ⎥ ⎤⎥ ∂σzz ⎥ ⎥ ⎥ ∂x ⎥ ⎥⎥ ⎥ ∂σzz ⎥ ⎥ ⎥ ⎥ ∂y ⎥ ⎥⎥ ∂σzz ⎦ ⎦ ∂z

(A28)

(A29)

Appendix A: Elements of tensor algebra

233

The divergence of a second-order tensor gives a ﬁrst-order tensor div σ = Tr[(∇σ )i ]. Hence,

⎡

⎡

∂σxx ⎢ ⎢ ∂x ⎢ ⎢ ⎢ ⎢ ∂σ xx ⎢Tr ⎢ ⎢ ⎢ ∂y ⎢ ⎢ ⎢ ⎢ ⎢ ⎣ ∂σxx ⎢ ⎢ ∂z ⎡ ⎤ ⎢ ⎢ ⎡ ∂σij ⎢ ∂σyx ⎢Tr ∂x ⎥ ⎢ ⎢ ⎢ i ⎥ ⎢ ⎢ ∂x ⎢ ⎥ ⎢ ⎢ ⎢ ⎥ ∂σij ⎥ ⎢ ⎢ ⎢ ∂σyx ⎢ div σ = ⎢Tr = ⎢Tr ⎢ ⎥ ∂xi ⎥ ⎢ ⎢ ∂y ⎢ ⎥ ⎢ ⎢ ⎢ ⎣ ∂σyx ⎣ ∂σij ⎦ ⎢ ⎢ Tr ⎢ ∂z ⎢ ∂xi ⎢ ⎡ ⎢ ∂σzx ⎢ ⎢ ⎢ ∂x ⎢ ⎢ ⎢ ⎢ ⎢ ⎢ ∂σzx ⎢ Tr ⎢ ⎢ ⎢ ∂y ⎢ ⎢ ⎣ ⎣ ∂σzx ∂z

(A30)

⎤⎤ ∂σxy ∂σxz ∂x ∂x ⎥ ⎥⎥ ⎥ ∂σxy ∂σxz ⎥ ⎥⎥ ⎥⎥ ∂y ∂y ⎥⎥ ⎥⎥ ⎥ ∂σxy ∂σxz ⎦⎥ ⎥ ∂z ∂z ⎥ ⎥ ⎤⎥ ⎡ ⎤ ∂σxy ∂σxz ∂σxx ∂σyy ∂σyz ⎥ ⎥ + + ⎥ ⎢ ∂y ∂z ⎥ ∂x ∂x ⎥ ⎥⎥ ⎢ ∂x ⎥ ⎥ ⎥ ⎢ ∂σyy ∂σyz ⎥⎥ ⎢ ∂σyx ∂σyy ∂σyz ⎥ ⎥ + + ⎥⎥ = ⎢ ⎥. ∂y ∂y ⎥⎥ ⎢ ∂x ∂y ∂y ⎥ ⎥⎥ ⎢ ⎥ ⎣ ∂σzx ∂σyy ∂σyz ⎦⎥ ∂σzy ∂σzz ⎦ ⎥ + + ∂z ∂y ⎥ ∂x ∂y ∂z ⎥ ⎤⎥ ∂σzy ∂σzz ⎥ ⎥ ⎥ ∂x ∂x ⎥ ⎥⎥ ⎥ ∂σzy ∂σzz ⎥ ⎥⎥ ⎥⎥ ∂y ∂y ⎥ ⎥ ⎥⎥ ∂σzy ∂σzz ⎦ ⎦ ∂z ∂z (A31)

Rotation Finite rotation is mathematically described by the orthogonal second-order tensor R −1 = R T ,

(A32)

which transforms a ﬁrst-order tensor as follows x = R · x

(A33)

σ = R · σ · RT .

(A34)

and a second-order tensor as follows

Successive ﬁnite rotations do not commute, that is, R 1 · R 2 = R 2 · R 1 .

(A35)

234

Appendix A: Elements of tensor algebra

r

z

r y

x

r0 =

r r

Fig. A.1 Finite rotation vector.

r1 If the axis r = r2 and the magnitude r = |r| of a ﬁnite rotation are known the r3 orthogonal second-order tensor which describes such rotation can be expressed in the form of an exponential function as follows: R = exp[ˆr ] = I + rˆ +

1 2 rˆ + · · ·, 2!

(A36)

where rˆ is the associated skew-symmetric tensor ⎤ ⎡ 0 −r3 r2 rˆ = ⎣ r3 0 −r1 ⎦ , −r2 r1 0

(A37)

which satisﬁes rˆ · r = 0,

(A38)

rˆ · x = r × x as illustrated in Fig. A.1. Small rotations can be approximated by

⎡

1 1 2 ⎣ R = exp[ˆr ] = I + rˆ + rˆ + · · · ≈ I + rˆ = 0 2! 0

0 1 0

⎤ ⎡ 0 0 ⎦ ⎣ 0 + r3 1 −r2

−r3 0 r1

⎤ r2 −r1 ⎦ , 0 (A39)

which do commute (I + rˆ 1 ) · (I + rˆ 2 ) = (I + rˆ 2 ) · (I + rˆ 1 ) = I + rˆ 1 + rˆ 2 + rˆ 1 · rˆ 2 ≈ I + rˆ 1 + rˆ 2 . (A40)

Appendix B: Fortran coding available via the OUP website∗

Directory/ﬁle

Description

elasticity elastic.f

UMAT for plane strain and axial symmetry for elastic behaviour using ABAQUS stress and strain quantities

elas_axidisp.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial displacement controlled loading, requiring UMAT elastic.f

elas_axiforce.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial force controlled loading, requiring UMAT elastic.f

plasticity_exp code_exp.f

UMAT for plane strain and axial symmetry for elastic, linear strain hardening plastic behaviour using explicit integration with continuum Jacobian, using ABAQUS stress and strain quantities. Suitable for large deformations

plas_exp_axidisp_aba.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial displacement controlled loading, using ABAQUS *PLASTIC

plas_exp_axiforce_aba_inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial force controlled loading, using ABAQUS *PLASTIC

∗ www.oup.co.uk/isbn/0–19–856826–6

236

Appendix B: Fortran coding

plas_exp_axidisp.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial displacement controlled loading, requiring UMAT code_exp.f

plas_exp_axiforce.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial force controlled loading, requiring UMAT code_exp.f

plas_exp_beam_aba.inp

Four point bend loading using ABAQUS*PLASTIC, requiring mesh ﬁle beam_mesh.inp

plas_exp_beam.inp

Four point bend loading requiring UMAT code_exp.f, requiring mesh ﬁle beam_mesh.inp

plasticity_imp code_imp.f

UMAT for plane strain and axial symmetry for elastic, linear strain hardening plastic behaviour using implicit integration with consistent Jacobian, using ABAQUS stress and strain quantities. Suitable for large deformations

plas_imp_axidisp_aba.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial displacement controlled loading, using ABAQUS *PLASTIC

plas_imp_axiforce_aba_inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial force controlled loading, using ABAQUS *PLASTIC

plas_imp_axidisp.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial displacement controlled loading, requiring UMAT code_imp.f

plas_imp_axiforce.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial force controlled loading, requiring UMAT code_imp.f

plas_imp_beam_aba.inp

Four point bend loading using ABAQUS*PLASTIC, requiring mesh ﬁle beam_mesh.inp

plas_imp_beam.inp

Four point bend loading requiring UMAT code_imp.f, requiring mesh ﬁle beam_mesh.inp

Appendix B: Fortran coding

237

spin spin_elastic.f

UMAT for three-dimensional, plane strain, and axial symmetry for elastic behaviour using ABAQUS stress and strain quantities

spin_elas_def.f

UMAT for three-dimensional, plane strain, and axial symmetry for elastic behaviour using the deformation gradient

spin_axidisp.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial displacement controlled loading, requiring UMAT spin_elas_def.f

spin_axiforce.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial force controlled loading, requiring UMAT spin_elas_def.f

spin_shear.inp

ABAQUS input ﬁle for a single plane strain element under simple shear, requiring UMAT spin_elas_def.f

spin_shear_aba.inp

ABAQUS input ﬁle for a single plane strain element under simple shear, using ABAQUS*ELASTIC

visco uni_visco_imp.f

Closed form Fortran implicit solution for uniaxial elasto-viscoplasticity

uni_visco_exp.f

Closed form Fortran explicit solution for uniaxial elasto-viscoplasticity

visco_imp.f

UMAT for plane strain and axial symmetry for elastic, linear strain hardening viscoplastic behaviour using implicit integration using the initial tangent stiffness, using ABAQUS stress and strain quantities. Suitable for large deformations

visco_imp_axidisp.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial displacement controlled loading, requiring UMAT visco_imp.f

238

Appendix B: Fortran coding

visco_imp_axiforce.inp

ABAQUS input ﬁle for single axisymmetric element under uniaxial force controlled loading, requiring UMAT visco_imp.f

visco_imp_beam.inp

Four point bend loading requiring UMAT visco_beam.f, requiring mesh ﬁle beam_mesh.inp

Index

ABAQUS 141, 149, 150, 167, 169, 235 ABAQUS input ﬁles 169 accumulated plastic strain 23 Almansi strain 50 angular velocity tensor 63 anisothermal cyclic plasticity 220 antisymmetric 51 Armstrong–Frederick 21 associated ﬂow 18 axial vibration 106, 115 B matrix 99 back stress 29 backward Euler integration 146, 161 Bauschinger effect 28 bcc 6 biaxial creep tests 213 bowing 212 Burger’s vector 8

calculus of variations 85 cantilever beam 118 Cauchy stress 72 Cauchy–Green tensor 49, 50 cavitation 210 central difference method 136 Chaboche 31 coarsening 209 combustion chambers 209 conservation of energy 84 consistency condition 20 consistent Jacobian 153 consistent tangent stiffness 153 consolidation 199 constant strain element 99 constitutive equations 40 continuum tangent stiffness 172 continuum damage 210 continuum Jacobian 172 continuum plasticity 10 continuum spin 61 contracted tensor product 15

convergence 140 co-rotational 73 creep 209 CREEP subroutine 202 critical resolved shear stress 7 crystal plasticity 5, 9 crystallographic orientation 3 crystallographic slip 5 cyclic hardening 37 cyclic plasticity 219

deformation-enhanced grain growth 190 deformation gradient 48 deformed conﬁguration 48 densiﬁcation rate 201 deviatoric stress 14 diagonalization 56 differentiation of a tensor 231 dilatation 201 direction of plastic ﬂow 19 dislocation bowing 212 dislocation density 210 displacement-based ﬁnite element method 98 divergence of a second-order tensor 233 double contracted product 15 Duva and Crow 200 dyadic product 230 dynamical path 84

effective plastic strain rate 14 effective stress 13 elastic predictor 147 elastic stiffness matrix 22, 100 elastic–plastic deformation 11 engineering shears 100 equations of motion 90 equilibrium 83 equivalent stress 13 Euler–Lagrange equation 86 explicit ﬁnite element methods 1, 141 explicit integration 136, 143

240

Index

fcc 6 ﬁnite element formulation for plasticity 133 ﬁnite element method 83 ﬁnite rotations 57 ﬁrst variation 87 forward integration 145 Gauss quadrature 126 geometric non-linearity 108 gradient of a ﬁrst-order tensor 232 gradient of a scalar 232 gradient of a second-order tensor 232 grain boundaries 3 grain growth 190 grain size 190 Hamilton’s principle 84 hardening 23 Helmholtz free energy 210 Hooke’s law 22, 170 hydrostatic stress 14 hysteresis 222 identity tensor 42 implicit 140, 143 implicit ﬁnite element methods 143 implicit implementation for elasto-viscoplasticity 161 implicit integration 146 implicit scheme 146 incompressibility 3, 12 incremental nature of plasticity 35 incremental rotation 176 initial tangential stiffness method 140 integration point 126 intergranular cracking 224 intergranular creep fracture 217 intermediate conﬁguration 66 internal variables 40 isoparametric 109 isotropic hardening 150 J2 plasticity 17 Jacobian 150 Jaumann stress rate 76 J-integral 84 Kinematic hardening 27 kinematics 47 kinetic energy 84 Lagrangian 84 Lame constant 42 large deformation(s) 47 leap frog explicit method 137

mass and spring system 90 mass matrix 105 material objectivity 69 material reference frame 48 material stress rate 78 mean stress 14 microstructural evolution 190 Mohr’s circle 69 momentum balance equations 106 multiaxial creep strain rate 212 multiaxial stress state 20, 212 multiplicative decomposition 67 necking 187 Newton iteration 148 Newton’s method 148 Newton–Raphson method 141 nickel alloy C263 209 nickel-base superalloy 209 nodal force vector 112 nodal forces 107 non-conservative 84 non-linear kinematic hardening 32 norm 30 normal grain growth 190 normality hypothesis 18 notched bar test 215 objective stress 72 objectivity 69 one-dimensional rod element 99 original conﬁguration 48 orthogonality 58 out of phase loading 225 over-stress 38 particle cutting 209 perfect plasticity 11 plane stress 18 plastic correction 146 plastic deformation gradient 66 plastic multiplier 19 plastic strain rate tensor 14 polar decomposition theorem 57 polycrystal 3 polycrystalline 3 porosity 199 porous plasticity 199 potential energy 84 potential function 45 power-law creep 44 Prager 29 precipitate coarsening 209 precipitate cutting 209 precipitate spacing 210 predictor–corrector 146 principal coordinates 56

Index

principal stresses 13 principle of virtual work 90 quasi-static problems 105 radial return method 146 rate-dependent plasticity 38 rate of deformation 60 reaction 130 reversed plasticity 28, 219 rigid body rotation 57 rotation 233 rotation matrix 58 Schmid’s law 7 second-order tensors 229 second stress invariant 17 semi-implicit integration 160 shape functions 97 shearing 3 simple shear 58 single and multiple element uniaxial tests 171 single element simple shear test 178 skew 51 slip system 5 solvus temperature 209 spin 61 stability of the explicit time stepping 139 static grain growth 190 stationary value 87 stiffness matrix 105 strain decomposition 11 strain measure 49 strain-rate sensitivity 39, 186 strain tensor 100 stress space 17 stress tensor 14 stress transformation 72 stress vector 70 stretch 48 stretch ratios 54 superplastic forming 192 Superplasticity 185

tangent stiffness 140, 150 tangential stiffness matrix 150 tension–torsion 213 tensorial notation 229 tensors 229 thermo-mechanical fatigue 219 thinning 195 time-dependent plasticity 38 time-independent plasticity 11 Ti–MMCs 205 titanium alloy, Ti–6Al–4V 189 traction 70 transformation of stress 72 transverse vibration 118, 122 Tresca 17 trial stress 147 true strain 53 truss element 99

UMAT 169 undeformed conﬁguration 48 uniaxial loading 14, 42 update of stress 143 upsetting 42

velocity gradient 60 veriﬁcation of the model implementation 171 virtual work 90 viscoplasticity 38 viscous stress 39 Voigt notation 19, 100 volume changes 199 von Mises 17

weak formulation 83 work conjugacy 111

yield criteria 17 yield function 17 yielding 3

241

This page intentionally left blank

(a)

(b) Strain rate

Strain rate

+ 0.00E – 00 + 2.00E – 06 + 3.00E – 06 + 4.00E – 06 + 5.00E – 06 + 6.00E – 06 + 7.00E – 06 + 8.00E – 06

+ 0.00E – 00 + 2.00E – 06 + 3.00E – 06 + 4.00E – 06 + 5.00E – 06 + 6.00E – 06 + 7.00E – 06 + 8.00E – 06

(c)

Strain rate + 0.00E – 00 + 2.00E – 06 + 3.00E – 06 + 4.00E – 06 + 5.00E – 06 + 6.00E – 06 + 7.00E – 06 + 8.00E – 06

Plate 1 The simulated superplastically deforming sheet showing the effective plastic strain rate at fractional processing times of t/tf = 0.1, t/tf = 0.6, and t/tf = 1.0.

(b)

(a) Thickness strain – 1.20E + 00 – 1.07E + 00 – 9.15E – 01 – 7.60E – 01 – 6.05E – 01 – 4.50E – 01 – 2.95E – 01 – 1.40E – 01

Thickness strain – 1.20E + 00 – 1.07E + 00 – 9.15E – 01 – 7.60E – 01 – 6.05E – 01 – 4.50E – 01 – 2.95E – 01 – 1.40E – 01

Plate 2 Through-thickness strain ﬁelds at the end of the superplastic forming carried out with target maximum strain rates of (a) 1.0 × 10−5 and (b) 1.0 × 10−4 s−1 .

(a)

(b) Grain sizes

Grain sizes

+7.93E – 03 +8.06E – 03 +8.20E – 03 +8.33E – 03 +8.60E – 03 +8.74E – 03 +8.88E – 03 +9.01E – 03

+ 1.14E – 02 + 1.15E – 02 + 1.16E – 02 + 1.16E – 02 + 1.17E – 02 + 1.18E – 02 + 1.18E – 02 + 1.19E – 02

Plate 3 Average grain size ﬁelds at the end of the superplastic forming carried out with target maximum strain rates of (a) 1.0 × 10−5 and (b) 1.0 × 10−4 s−1 .

Cavitation damage parameter

(a)

+0.00E+00 +2.00E–02 +4.36E–02 +6.73E–02 +9.09E–02 +1.15E–01 +1.38E–01 +1.62E–01 +1.85E–01 +2.09E–01 +2.33E–01 +2.56E–01 +2.80E–01 +3.00E–01

(b) (c) 2

7

6

8

3

2

2

0

2

2

5

0

0

Number of creep voids

7

12

7

2

4

4

4

15

6

3

0

2

9

9

5

2

0

0 1–3 4–6 7–9 10–12 13

1

3

4

22

8

2

5

1

17

30

1

Plate 4 Creep damage ﬁelds (a) predicted by the model, (b) observed in the microstructure, and (c) from a surface void count using the micrograph.

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close